Graphene demonstrates interesting electrical, optical, and optoelectronic properties. A number of other oneatomthick m
785 111 24MB
English Pages 1026 [1027] Year 2020
Table of contents :
Cover
Half Title
Title Page
Copyright Page
Table of Contents
Preface
Part 1: Electronic and Plasmonic Properties of Graphene and Graphene Structures
Chapter 1: Plasma Waves in TwoDimensional ElectronHole System in Gated Graphene Heterostructures
1.1: Introduction
1.2: Equations of the Model
1.3: Dispersion Equation for Plasma Waves
1.4: Limiting Cases
1.4.1: Low Temperatures or High Gate Voltages
1.4.2: Elevated Temperatures and Low Gate Voltages
1.5: General Results and Discussion
Chapter 2: Device Model for Graphene Bilayer FieldEffect Transistor
2.1: Introduction
2.2: GBLFET Energy Band Diagrams
2.3: Boltzmann Kinetic Equation and Its Solutions
2.3.1: Ballistic Electron Transport
2.3.2: Collisional Electron Transport
2.4: GBLFET DC Transconductance
2.5: GBLFET AC Transconductance
2.6: Analysis of the Results and Discussion
2.7: Conclusions
Chapter 3: ElectricallyInduced nip Junctions in Multiple Graphene Layer Structures
3.1: Introduction
3.2: Equations of the Model
3.3: Numerical Results
3.4: Analytical Model
3.5: The Reverse Current
3.6: MultipleGL Structures with Highly Conductive BGL
3.7: Conclusions
Chapter 4: Tunneling Recombination in Optically Pumped Graphene with ElectronHole Puddles
Chapter 5: Analytical Device Model for Graphene Bilayer FieldEffect Transistors Using Weak Nonlocality Approximation
5.1: Introduction
5.2: Device Model and Features of Operation
5.3: Main Equations of the Model
5.3.1: High TopGate Voltages
5.3.2: Near Threshold TopGate Voltages
5.3.3: Low TopGate Voltages
5.4: Potential Distributions, SourceDrain Current, and Transconductance
5.4.1: High TopGate Voltages: Subthreshold Voltage Range (Δm >> εF)
5.4.2: Near Threshold TopGate Voltages (Δm ≳ εF)
5.4.3: Low TopGate Voltages (Dm < ef)
5.5: Discussion
5.5.1: Role of Geometrical Parameters
5.5.2: Effect of Electron Scattering
5.5.3: Charge Inversion in the Gated Section
5.5.4: Interband Tunneling
5.6: Conclusions
Chapter 6: Hydrodynamic Model for ElectronHole Plasma in Graphene
6.1: Introduction
6.2: Derivation of Hydrodynamic Equations
6.3: Effect of ElectronHole Drag and DC Conductivity of Gated Graphene
6.4: Plasma and ElectronHole Sound Waves in Graphene
6.4.1: General Dispersion Relation for Collective Excitations
6.4.2: Analytical Solutions for Symmetric Bipolar and Monopolar Systems
6.4.3: Velocities and Damping Rates of the Waves
6.4.4: Comparison with Other Models
6.5: Discussion of the Results
Chapter 7: Interplay of Intra and Interband Absorption in a Disordered Graphene
7.1: Introduction
7.2: Basic Equations
7.2.1: Dynamic Conductivity
7.2.2: Partly Screened LongRange Disorder
7.3: Relative Absorption
7.3.1: Spectral Dependencies
7.3.2: Comparison with Experiment
7.4: Conclusions
Chapter 8: VoltageControlled Surface PlasmonPolaritons in Double Graphene Layer Structures
8.1: Introduction
8.2: Device Model
8.3: SPP Dispersion in Double Graphene Layer
8.4: Results and Discussion
8.5: Conclusions
Chapter 9: Hydrodynamic Electron Transport and Nonlinear Waves in Graphene
9.1: Introduction
9.2: Derivation of Hydrodynamic Equations
9.3: Nonlinear Effects in PlasmaWave Propagation
9.3.1: Formation of Solitons in Gated Graphene
9.3.2: ‘ShallowWater’ Plasma Waves in the Presence of Steady Electron Flow
9.3.3: Excitation of Electron PlasmaWaves by Direct Current
9.4: Discussion of the Results
9.5: Conclusions
Chapter 10: Effect of SelfConsistent Electric Field on Characteristics of Graphene pin Tunneling TransitTime Diodes
10.1: Introduction
10.2: Equations of the Model
10.3: Spatial Potential Distributions and CurrentVoltage Characteristics
10.4: GTUNNETT Admittance
10.5: Discussion
10.6: Conclusions
Chapter 11: Damping Mechanism of Terahertz Plasmons in Graphene on Heavily Doped Substrate
11.1: Introduction
11.2: Equations of the Model
11.3: Ungated Plasmons
11.4: Gated Plasmons
11.5: Conclusions
Chapter 12: Active Guiding of Dirac Plasmons in Graphene
Chapter 13: Vertical Electron Transport in van der Waals Heterostructures with Graphene Layers
13.1: Introduction
13.2: General Equations of the Model
13.3: The Peltier Cooling
13.4: Electric Fields versus Current and CurrentVoltage Characteristics
13.5: Potential Profiles
13.6: Discussions
13.6.1: Limiting Cases
13.6.2: Role of the pn–En Relation
13.6.3: Electron Heating in the Barrier Layers
13.6.4: Quantum Capacitance
13.6.5: Contact Effects
13.7: Conclusions
Chapter 14: Giant Plasmon Instability in DualGratingGate Graphene FieldEffect Transistor
14.1: Introduction
14.2: Mechanisms of Dyakonov–Shur and Ryzhii–Satou–Shur Instabilities
14.3: Simulation Model
14.4: Results and Discussion
14.5: Conclusion
Part 2: Detectors Based on Lateral Transport in Graphene and Graphene Structures
Chapter 15: Plasma Mechanisms of Resonant Terahertz Detection in a TwoDimensional Electron Channel with Split Gates
15.1: Introduction
15.2: Equations of the Model
15.3: Plasma Resonances
15.4: Resonant Electron Heating
15.5: Rectified Current and Detector Responsivity
15.6: Comparison of Dynamic and Heating Mechanisms
15.7: Temperature Dependences of the Detector Responsivity and Detectivity
15.8: Discussion
15.9: Conclusions
Chapter 16: Terahertz and Infrared Photodetection Using pin MultipleGrapheneLayer Structures
16.1: Introduction
16.2: Responsivity and Detectivity
16.3: Features of GLPD with Electrically Induced Junction
16.4: Dynamical Response
16.5: Comparison with QWIPs and QDIPs
16.6: Discussion and Conclusions
Chapter 17: Negative and Positive Terahertz and Infrared Photoconductivity in Uncooled Graphene
17.1: Introduction
17.2: GL Conductivity Dependence on the Carrier Temperature
17.3: GenerationRecombination and Energy Balance Equations
17.4: GL Photoconductivity
17.5: Clustered Impurities and Decorated GLs: LongRange Scattering
17.6: Responsivity of the GLBased Photodetectors
17.7: Heavily Doped GLs
17.8: Conclusions
Part 3: Population Inversion and Negative Conductivity in Graphene and Graphene Structures
Chapter 18: Negative Dynamic Conductivity of Graphene with Optical Pumping
18.1: Introduction
18.2: Equations of the Model
18.3: Weak Pumping
18.4: Strong Pumping
18.5: Conclusions
Chapter 19: Population Inversion of Photoexcited Electrons and Holes in Graphene and Its Negative Terahertz Conductivity
19.1: Introduction
19.2: Qualitative Pattern
19.3: Frequency Dependence of the Conductivity
19.4: Heating of Electrons and Holes
19.5: Discussion
Chapter 20: Negative Terahertz Dynamic Conductivity in Electrically Induced Lateral pin Junction in Graphene
20.1: Introduction
20.2: Device Model and Terminal AC Conductance
20.3: SelfExcitation of Plasma Oscillations
20.4: Conclusions
Chapter 21: Threshold of Terahertz Population Inversion and Negative Dynamic Conductivity in Graphene Under Pulse Photoexcitation
21.1: Introduction
21.2: Formulation of the Model
21.3: Results and Discussion
21.3.1: Time Evolution of QuasiFermi Level and Carrier Temperature
21.3.2: Time Evolution of Dynamic Conductivity for High and LowQuality Graphene
21.3.3: OpticalPhonon Emission versus Other Recombination Mechanisms
21.4: Conclusions
Chapter 22: Double Injection in Graphene pin Structures
22.1: Introduction
22.2: Model
22.2.1: The Structures Under Consideration
22.2.2: Equations of the Model
22.2.3: Boundary Conditions
22.2.4: Dimensionless Equations and Boundary Conditions
22.3: Injection Characteristics (Analytical Approach for a Special Case)
22.4: Numerical Results
22.5: CurrentVoltage Characteristics
22.6: Discussion
22.7: Conclusions
Chapter 23: CarrierCarrier Scattering and Negative Dynamic Conductivity in Pumped Graphene
23.1: Introduction
23.2: Intraband Dynamic Conductivity General Equations
23.3: Analysis of Intraband and Net Dynamic Conductivity
23.4: Discussion of the Results
23.5: Conclusions
Chapter 24: Negative Terahertz Conductivity in Disordered Graphene Bilayers with Population Inversion
Chapter 25: Negative Terahertz Conductivity in Remotely Doped Graphene Bilayer Heterostructures
25.1: Introduction
25.2: Device Model
25.3: Main Equations
25.4: Scattering Mechanisms
25.5: Net THz Conductivity
25.6: Results and Analysis
25.7: Discussion
25.8: Conclusions
Part 4: Stimulated Emission and Lasing in Graphene and Graphene Structures
Chapter 26: Feasibility of Terahertz Lasing in Optically Pumped Epitaxial Multiple Graphene Layer Structures
26.1: Introduction
26.2: Model
26.3: MGL Structure Net Dynamic Conductivity
26.4: Frequency Characteristics of Dynamic Conductivity
26.5: Role of the Bottom GL
26.6: Condition of Lasing
26.7: Conclusions
Chapter 27: Terahertz Lasers Based on Optically Pumped Multiple Graphene Structures with SlotLine and Dielectric Waveguides
27.1: Introduction
27.2: Device Model
27.3: Results and Discussion
27.4: Conclusions
Chapter 28: Observation of Amplified Stimulated Terahertz Emission from Optically Pumped Heteroepitaxial GrapheneonSilicon Materials
28.1: Introduction
28.2: Theoretical Model
28.3: Graphene on Silicon Sample for the Experiment
28.4: Experimental
28.5: Results and Discussion
28.6: Conclusion
Chapter 29: Toward the Creation of Terahertz Graphene Injection Laser
29.1: Introduction
29.2: Device Model
29.3: Equations of the Model
29.4: Effective Temperatures and CurrentVoltage Characteristics (Analytical Analysis)
29.4.1: Low Voltages
29.4.2: Special Cases
29.4.3: Long Optical Phonon Decay Time
29.5: Effective Temperatures and CurrentVoltage Characteristics (Numerical Results)
29.6: Dynamic Conductivity
29.7: Limitations of the Model and Discussion
29.8: Conclusions
Chapter 30: Ultrafast Carrier Dynamics and Terahertz Emission in Optically Pumped Graphene at Room Temperature
30.1: Introduction
30.2: Theory and Background
30.3: Sample and Characterization
30.4: Experiments
30.5: Results and Discussion
30.6: Conclusion
Chapter 31: Spectroscopic Study on Ultrafast Carrier Dynamics and Terahertz Amplified Stimulated Emission in Optically Pumped Graphene
31.1: Introduction
31.2: Carrier Relaxation and Recombination Dynamics in Optically Pumped Graphene
31.3: Experiments
31.3.1: Experimental Setup
31.3.2: Samples and Characterizations
31.3.2.1: Exfoliated graphene on SiO2/Si
31.3.2.2: Heteroepitaxial graphene on 3CSiC/Si
31.3.3: Results and Discussions
31.3.3.1: Exfoliated graphene on SiO2/Si
31.3.3.2: Heteroepitaxial graphene on 3CSiC/Si
31.4: Conclusion
Chapter 32: Gain Enhancement in Graphene Terahertz Amplifiers with Resonant Structures
32.1: Introduction
32.2: FDTD Model
32.3: Results and Discussion
32.4: Conclusions
Chapter 33: Plasmonic Terahertz Lasing in an Array of Graphene Nanocavities
Chapter 34: The Gain Enhancement Effect of Surface Plasmon Polaritons on Terahertz Stimulated Emission in Optically Pumped Monolayer Graphene
34.1: Introduction
34.2: Stimulated Terahertz (THz) Photon and Plasmon Emission in Optically Pumped Graphene
34.3: Experimental Observation of THz Stimulated Plasmon Emission in Optically Pumped Graphene
34.3.1: Experimental Setup and Sample Preparation
34.3.2: Temporal Profile and Fourier Spectrum of the PopulationInverted Graphene to the THz Pulse Irradiation
34.3.3: Spatial Field Distribution of the THz Probe Pulse Intensities
34.4: Conclusion
Chapter 35: Graphene Surface Emitting Terahertz Laser: Diffusion Pumping Concept
Chapter 36: Enhanced Terahertz Emission from Monolayer Graphene with Metal Mesh Structure
36.1: Introduction
36.2: Principle
36.3: Experimental
36.3.1: Basic Structure of THz Amplifier
36.3.2: Measurement Method
36.3.3: EM Simulation Model
36.4: Results and Discussion
36.4.1: GaAs + Graphene
36.4.2: GaAs + Metal
36.4.3: GaAs + Metal + Graphene
36.5: Conclusion
Chapter 37: Terahertz LightEmitting GrapheneChannel Transistor Toward SingleMode Lasing
37.1: Introduction
37.2: Device Design and Fabrication
37.2.1: Design and Fabrication Details
37.2.2: Principles of Operation
37.3: Results and Discussions
37.3.1: Broadband THz Light Emission
37.3.2: Towards SingleMode Lasing
37.4: Conclusions
Part 5: Detectors and Emitters Based on Photon/Plasmon Assisted Tunneling between Graphene Layers
Chapter 38: Injection Terahertz Laser Using the Resonant InterLayer Radiative Transitions in DoubleGrapheneLayer Structure
Chapter 39: DoubleGrapheneLayer Terahertz Laser: Concept, Characteristics, and Comparison
39.1: Introduction
39.2: Device Structures and Principles of Operation
39.3: InterGL and IntraGL Dynamic Conductivities
39.4: Terahertz Gain and GainOverlap Factors
39.5: Frequency and Voltage Dependences of the THz Gain
39.6: Discussion
39.7: Conclusion
Chapter 40: SurfacePlasmons Lasing in DoubleGrapheneLayer Structures
40.1: Introduction
40.2: Dynamic Conductivity Tensor
40.3: Electric Field Distributions, GainOverlap Factor, and Modal Gain
40.4: Conclusions
Chapter 41: Double Injection, ResonantTunneling Recombination, and CurrentVoltage Characteristics in DoubleGrapheneLayer Structures
41.1: Introduction
41.2: Model and the Pertinent Equations
41.3: Spatial and Voltage Dependences of Fermi Energy, Energy Gap, and Potential
41.4: Role of Scattering on Disorder
41.5: CurrentVoltage Characteristics
41.6: Conclusions
Chapter 42: VoltageTunable Terahertz and Infrared Photodetectors Based on DoubleGrapheneLayer Structures
Chapter 43: Plasmons in TunnelCoupled Graphene Layers: Backward Waves with Quantum Cascade Gain
43.1: Introduction
43.2: Dispersion Relation for Plasmons in TunnelCoupled Layers
43.3: HighFrequency Nonlocal Tunnel Current
43.4: Plasmons in the Presence of Tunneling
43.5: Effects of Interlayer Twist
43.6: Discussion and Conclusions
Chapter 44: Terahertz Wave Generation and Detection in DoubleGraphene Layered van der Waals Heterostructures
44.1: Introduction
44.2: Device Description and Principles of Operation
44.3: Experimental Methods
44.4: Results and Discussions
44.5: Conclusion
Chapter 45: UltraCompact Injection Terahertz Laser Using the Resonant InterLayer Radiative Transitions in MultiGrapheneLayer Structure
45.1: Introduction
45.2: Device Model
45.3: Results and Discussion
45.4: Conclusion
Part 6: Graphene Based van der Waals Heterostructures for THz Detectors and Emitters
Chapter 46: Graphene Vertical HotElectron Terahertz Detectors
46.1: Introduction
46.2: Device Structures and Principle of Operation
46.3: Vertical Electron Dark Current and Photocurrent
46.4: Electron Heating by Incoming THz Radiation
46.5: Responsivity
46.6: Dark Current Limited Detectivity
46.7: Role of the Electron Capture
46.8: Effect of Plasmonic Resonances
46.9: Limitations of the Model
46.10: Discussion
46.11: Conclusions
Chapter 47: Electron Capture in van der Waals GrapheneBased Heterostructures with WS2 Barrier Layers
47.1: Introduction
47.2: Model and Electron Wave Functions
47.3: Electron Capture Probability at Different Scattering Mechanisms
47.3.1: Capture due to the Emission of Barrier Optical Phonons
47.3.2: Capture due to the Emission of GL Optical Phonons
47.3.3: Capture Associated with the ElectronElectron Interaction
47.3.4: Results of Numerical Calculations
47.4: Capture Parameter and Capture Velocity
47.5: Conclusion
Chapter 48: Resonant Plasmonic Terahertz Detection in Vertical GrapheneBase HotElectron Transistors
48.1: Introduction
48.2: Device Model and Related Equations
48.3: Plasma Oscillations and Rectified Current
48.4: GBHET Detector Responsivity
48.4.1: Current Responsivity
48.4.2: Voltage Responsivity
48.5: Discussion
48.6: Conclusions
Chapter 49: Nonlinear Response of Infrared Photodetectors Based on van der Waals Heterostructures with Graphene Layers
49.1: Introduction
49.2: Device Structure and Model
49.3: Main Equations
49.4: Dark Characteristics
49.5: Photoresponse at Low IR Radiation Intensities
49.6: Nonlinear Response: High IR Radiation Intensities
49.7: Comments
49.8 Conclusions
Chapter 50: Effect of Doping on the Characteristics of Infrared Photodetectors Based on van der Waals Heterostructures with Multiple Graphene Layers
50.1: Introduction
50.2: Structure of GLIPs and Their Operation Principle
50.3: Equations of the Model
50.4: GLIP Responsivity
50.5: GLIP Detectivity
50.6: Discussion
50.7: Conclusions
Chapter 51: RealSpaceTransfer Mechanism of Negative Differential Conductivity in Gated GraphenePhosphorene Hybrid Structures: Phenomenological Heating Model
51.1: Introduction
51.2: Model
51.3: Main Equations of the Model
51.3.1: Conductivity of the GP Channel
51.3.2: Carrier Interband Balance
51.3.3: GenerationRecombination and Energy Balance Equations
51.3.4: General Set of the Equations
51.4: Numerical Results
51.5: Discussion
51.5.1: Screening in the GP Channel
51.5.2: Mutual Scattering of Electrons and Holes
51.5.3: Optical Phonon Heating
51.5.4: Relaxation of Substrate Optical Phonons
51.5.5: Possible Applications of the GP Devices
51.6: Conclusions
Chapter 52: Negative Photoconductivity and HotCarrier Bolometric Detection of Terahertz Radiation in GraphenePhosphorene Hybrid Structures
52.1: Introduction
52.2: Model
52.3: Conductivity of the GPChannel
52.4: Negative Photoconductivity in the GP Channels
52.5: Responsivity of the GPPhotodetectors
52.6: Bandwidth and GainBandwidth Product
52.7: Detectivity of the GPBolometers
52.8: Discussion
52.8.1: General Comments
52.8.2: Assumptions
52.9: Conclusions
Index
GrapheneBased Terahertz
Electronics and Plasmonics
GrapheneBased Terahertz
Electronics and Plasmonics
Detector and Emitter Concepts
edited by
Vladimir Mitin  Taiichi Otsuji  Victor Ryzhii
Published by Jenny Stanford Publishing Pte. Ltd. Level 34, Centennial Tower 3 Temasek Avenue Singapore 039190
Email: [email protected] Web: www.jennystanford.com British Library CataloguinginPublication Data A catalogue record for this book is available from the British Library.
GrapheneBased Terahertz Electronics and Plasmonics: Detector and Emitter Concepts Copyright © 2021 by Jenny Stanford Publishing Pte. Ltd. All rights reserved. This book, or parts thereof, may not be reproduced in any form or by any means, electronic or mechanical, including photocopying, recording or any information storage and retrieval system now known or to be invented, without written permission from the publisher.
For photocopying of material in this volume, please pay a copying fee through the Copyright Clearance Center, Inc., 222 Rosewood Drive, Danvers, MA 01923, USA. In this case permission to photocopy is not required from the publisher. ISBN 9789814800754 (Hardcover) ISBN 9780429328398 (eBook)
Contents
Preface
Part 1 Electronic and Plasmonic Properties of Graphene and Graphene Structures 1. Plasma Waves in TwoDimensional ElectronHole
System in Gated Graphene Heterostructures V. Ryzhii, A. Satou, and T. Otsuji 1.1 Introduction 1.2 Equations of the Model 1.3 Dispersion Equation for Plasma Waves 1.4 Limiting Cases 1.4.1 Low Temperatures or High Gate Voltages 1.4.2 Elevated Temperatures and
Low Gate Voltages 1.5 General Results and Discussion 2. Device Model for Graphene Bilayer FieldEffect Transistor V. Ryzhii, M. Ryzhii, A. Satou, T. Otsuji, and N. Kirova 2.1 Introduction 2.2 GBLFET Energy Band Diagrams 2.3 Boltzmann Kinetic Equation and Its Solutions 2.3.1 Ballistic Electron Transport 2.3.2 Collisional Electron Transport 2.4 GBLFET DC Transconductance 2.5 GBLFET AC Transconductance 2.6 Analysis of the Results and Discussion 2.7 Conclusions 3. ElectricallyInduced nip Junctions in
Multiple Graphene Layer Structures M. Ryzhii, V. Ryzhii, T. Otsuji, V. Mitin, and M. S. Shur 3.1 3.2
Introduction Equations of the Model
xxiii
3
4
5
7
9
9
10
12
17
18
19
24
25
26
29
30
32
35
41
42
43
vi
Contents
3.3 3.4 3.5 3.6 3.7
Numerical Results Analytical Model The Reverse Current MultipleGL Structures with Highly
Conductive BGL Conclusions
4. Tunneling Recombination in Optically Pumped
Graphene with ElectronHole Puddles V. Ryzhii, M. Ryzhii, and T. Otsuji 5. Analytical Device Model for Graphene Bilayer FieldEffect
Transistors Using Weak Nonlocality Approximation V. Ryzhii, M. Ryzhii, A. Satou, T. Otsuji, and V. Mitin 5.1 Introduction 5.2 Device Model and Features of Operation 5.3 Main Equations of the Model 5.3.1 High TopGate Voltages 5.3.2 Near Threshold TopGate Voltages 5.3.3 Low TopGate Voltages 5.4 Potential Distributions, SourceDrain Current,
and Transconductance 5.4.1 High TopGate Voltages: Subthreshold
Voltage Range (Δm >> εF) 5.4.2 Near Threshold TopGate
Voltages (Δm εF) 5.4.3 Low TopGate Voltages (Dm < ef) 5.5 Discussion 5.5.1 Role of Geometrical Parameters 5.5.2 Effect of Electron Scattering 5.5.3 Charge Inversion in the Gated Section 5.5.4 Interband Tunneling 5.6 Conclusions 6. Hydrodynamic Model for ElectronHole
Plasma in Graphene D. Svintsov, V. Vyurkov, S. Yurchenko, T. Otsuji,
and V. Ryzhii
6.1 Introduction 6.2 Derivation of Hydrodynamic Equations
46
49
51
54
55
59
69
70
72
73
77
77
78
79
79
81
85
88
88
89
91
92
92
97
98
99
Contents
6.3
6.4
6.5
Effect of ElectronHole Drag and DC
Conductivity of Gated Graphene Plasma and ElectronHole Sound Waves
in Graphene 6.4.1 General Dispersion Relation for
Collective Excitations 6.4.2 Analytical Solutions for Symmetric
Bipolar and Monopolar Systems 6.4.3 Velocities and Damping Rates of
the Waves 6.4.4 Comparison with Other Models Discussion of the Results
7. Interplay of Intra and Interband Absorption
in a Disordered Graphene F. T. Vasko, V. V. Mitin, V. Ryzhii, and T. Otsuji 7.1 Introduction 7.2 Basic Equations 7.2.1 Dynamic Conductivity 7.2.2 Partly Screened LongRange Disorder 7.3 Relative Absorption 7.3.1 Spectral Dependencies 7.3.2 Comparison with Experiment 7.4 Conclusions
8. VoltageControlled Surface PlasmonPolaritons
in Double Graphene Layer Structures D. Svintsov, V. Vyurkov, V. Ryzhii, and T. Otsuji 8.1 Introduction 8.2 Device Model 8.3 SPP Dispersion in Double Graphene Layer 8.4 Results and Discussion 8.5 Conclusions 9. Hydrodynamic Electron Transport and Nonlinear
Waves in Graphene D. Svintsov, V. Vyurkov, V. Ryzhii, and T. Otsuji 9.1 Introduction 9.2 Derivation of Hydrodynamic Equations
104
109
109
111
113
115
117
125
126
129
129
132
135
135
137
140
145
146
147
148
151
155
159
160
162
vii
viii
Contents
9.3
9.4 9.5
Nonlinear Effects in PlasmaWave Propagation 9.3.1 Formation of Solitons in Gated
Graphene 9.3.2 ‘ShallowWater’ Plasma Waves in
the Presence of Steady Electron Flow 9.3.3 Excitation of Electron PlasmaWaves
by Direct Current Discussion of the Results Conclusions
10. Effect of SelfConsistent Electric Field on Characteristics
of Graphene pin Tunneling TransitTime Diodes V. L. Semenenko, V. G. Leiman, A. V. Arsenin, V. Mitin, M. Ryzhii, T. Otsuji, and V. Ryzhii 10.1 Introduction 10.2 Equations of the Model 10.3 Spatial Potential Distributions and
CurrentVoltage Characteristics 10.4 GTUNNETT Admittance 10.5 Discussion 10.6 Conclusions 11. Damping Mechanism of Terahertz Plasmons in
Graphene on Heavily Doped Substrate A. Satou, Y. Koseki, V. Ryzhii, V. Vyurkov, and T. Otsuji 11.1 Introduction 11.2 Equations of the Model 11.3 Ungated Plasmons 11.4 Gated Plasmons 11.5 Conclusions 12. Active Guiding of Dirac Plasmons in Graphene M. Yu. Morozov, A. R. Davoyan, I. M. Moiseenko, A. Satou, T. Otsuji, and V. V. Popov 13. Vertical Electron Transport in van der Waals
Heterostructures with Graphene Layers V. Ryzhii, T. Otsuji, M. Ryzhii, V. Ya. Aleshkin, A. A. Dubinov, V. Mitin, and M. S. Shur 13.1 Introduction
166
166
169
171
173
175
181
182
184
188
192
195
197
201
202
204
207
211
215
219
231
232
Contents
13.2 13.3 13.4 13.5 13.6
13.7
General Equations of the Model The Peltier Cooling Electric Fields versus Current and
CurrentVoltage Characteristics Potential Profiles Discussions 13.6.1 Limiting Cases 13.6.2 Role of the pn–E n Relation 13.6.3 Electron Heating in the Barrier Layers 13.6.4 Quantum Capacitance 13.6.5 Contact Effects Conclusions
14. Giant Plasmon Instability in DualGratingGate
Graphene FieldEffect Transistor Y. Koseki, V. Ryzhii, T. Otsuji, V. V. Popov, and A. Satou 14.1 Introduction 14.2 Mechanisms of Dyakonov–Shur and
Ryzhii–Satou–Shur Instabilities 14.3 Simulation Model 14.4 Results and Discussion 14.5 Conclusion
Part 2 Detectors Based on Lateral Transport in Graphene and Graphene Structures
15. Plasma Mechanisms of Resonant Terahertz
Detection in a TwoDimensional Electron Channel
with Split Gates V. Ryzhii, A. Satou, T. Otsuji, and M. S. Shur 15.1 Introduction 15.2 Equations of the Model 15.3 Plasma Resonances 15.4 Resonant Electron Heating 15.5 Rectified Current and Detector Responsivity 15.6 Comparison of Dynamic and
Heating Mechanisms 15.7 Temperature Dependences of the Detector
Responsivity and Detectivity
233
238
239
241
243
243
245
246
247
248
249
255
256
258
259
262
265
271
272
274
276
277
278 279
282
ix
x
Contents
15.8 15.9
Discussion Conclusions
16. Terahertz and Infrared Photodetection Using
pin MultipleGrapheneLayer Structures V. Ryzhii, M. Ryzhii, V. Mitin, and T. Otsuji 16.1 Introduction 16.2 Responsivity and Detectivity 16.3 Features of GLPD with Electrically Induced
Junction 16.4 Dynamical Response 16.5 Comparison with QWIPs and QDIPs 16.6 Discussion and Conclusions
17. Negative and Positive Terahertz and Infrared
Photoconductivity in Uncooled Graphene V. Ryzhii, D. S. Ponomarev, M. Ryzhii, V. Mitin, M. S. Shur, and T. Otsuji 17.1 Introduction 17.2 GL Conductivity Dependence on the Carrier
Temperature 17.3 GenerationRecombination and Energy
Balance Equations 17.4 GL Photoconductivity 17.5 Clustered Impurities and Decorated
GLs: LongRange Scattering 17.6 Responsivity of the GLBased Photodetectors 17.7 Heavily Doped GLs 17.8 Conclusions
Part 3 Population Inversion and Negative Conductivity in Graphene and Graphene Structures 18. Negative Dynamic Conductivity of Graphene
with Optical Pumping V. Ryzhii, M. Ryzhii, and T. Otsuji 18.1 Introduction 18.2 Equations of the Model 18.3 Weak Pumping
284
285
289
290
292
296
297
299
302
307
308
310
312
314
318
320
321
323
331
332
332
335
Contents
18.4 18.5
Strong Pumping Conclusions
339
340
19. Population Inversion of Photoexcited Electrons
and Holes in Graphene and Its Negative Terahertz
Conductivity V. Ryzhii, M. Ryzhii, and T. Otsuji 19.1 Introduction 19.2 Qualitative Pattern 19.3 Frequency Dependence of the Conductivity 19.4 Heating of Electrons and Holes 19.5 Discussion
343
344
345
346
349
350
20. Negative Terahertz Dynamic Conductivity in
Electrically Induced Lateral pin Junction in Graphene V. Ryzhii, M. Ryzhii, M. S. Shur, and V. Mitin 20.1 Introduction 20.2 Device Model and Terminal AC Conductance 20.3 SelfExcitation of Plasma Oscillations 20.4 Conclusions
21. Threshold of Terahertz Population Inversion and
Negative Dynamic Conductivity in Graphene
Under Pulse Photoexcitation A. Satou, V. Ryzhii, Y. Kurita, and T. Otsuji 21.1 Introduction 21.2 Formulation of the Model 21.3 Results and Discussion 21.3.1 Time Evolution of QuasiFermi Level
and Carrier Temperature 21.3.2 Time Evolution of Dynamic Conductivity for High and LowQuality Graphene 21.3.3 OpticalPhonon Emission versus Other
Recombination Mechanisms 21.4 Conclusions
22. Double Injection in Graphene pin Structures V. Ryzhii, I. Semenikhin, M. Ryzhii, D. Svintsov, V. Vyurkov, A. Satou, and T. Otsuji 22.1 Introduction
353
354
354
358
360
363
364
365
369
369
372
375
377
381
382
xi
xii
Contents
22.2
22.3 22.4 22.5 22.6 22.7
Model 22.2.1 22.2.2 22.2.3 22.2.4
The Structures Under Consideration Equations of the Model Boundary Conditions Dimensionless Equations and
Boundary Conditions Injection Characteristics (Analytical
Approach for a Special Case) Numerical Results CurrentVoltage Characteristics Discussion Conclusions
23. CarrierCarrier Scattering and Negative Dynamic
Conductivity in Pumped Graphene D. Svintsov, V. Ryzhii, A. Satou, T. Otsuji, and V. Vyurkov 23.1 Introduction 23.2 Intraband Dynamic Conductivity General
Equations 23.3 Analysis of Intraband and Net Dynamic
Conductivity 23.4 Discussion of the Results 23.5 Conclusions 24. Negative Terahertz Conductivity in Disordered
Graphene Bilayers with Population Inversion D. Svintsov, T. Otsuji, V. Mitin, M. S. Shur, and V. Ryzhii
25. Negative Terahertz Conductivity in Remotely Doped
Graphene Bilayer Heterostructures V. Ryzhii, M. Ryzhii, V. Mitin, M. S. Shur, and T. Otsuji 25.1 Introduction 25.2 Device Model 25.3 Main Equations 25.4 Scattering Mechanisms 25.5 Net THz Conductivity 25.6 Results and Analysis 25.7 Discussion 25.8 Conclusions
384
384
386
387
388
390
392
397
399
402
407
408
411
416
420
423
429
441
442
445
446
448
449
450
457
458
Contents
Part 4 Stimulated Emission and Lasing in Graphene and Graphene Structures 26. Feasibility of Terahertz Lasing in Optically Pumped
Epitaxial Multiple Graphene Layer Structures
465
V. Ryzhii, M. Ryzhii, A. Satou, T. Otsuji, A. A. Dubinov,
and V. Ya. Aleshkin
26.1 26.2 26.3 26.4 26.5 26.6 26.7
Introduction Model MGL Structure Net Dynamic Conductivity Frequency Characteristics of Dynamic
Conductivity Role of the Bottom GL Condition of Lasing Conclusions
27. Terahertz Lasers Based on Optically Pumped
Multiple Graphene Structures with SlotLine
and Dielectric Waveguides
466
467
470
472
474
476
477
481
V. Ryzhii, A. A. Dubinov, T. Otsuji, V. Mitin, and M. S. Shur 27.1 27.2 27.3 27.4
Introduction Device Model Results and Discussion Conclusions
28. Observation of Amplified Stimulated Terahertz
Emission from Optically Pumped Heteroepitaxial
GrapheneonSilicon Materials
482
483
487
493
495
H. Karasawa, T. Komori, T. Watanabe, A. Satou, H. Fukidome, M. Suemitsu, V. Ryzhii, and T. Otsuji 28.1 28.2 28.3 28.4 28.5 28.6
Introduction Theoretical Model Graphene on Silicon Sample for the
Experiment Experimental Results and Discussion Conclusion
496
497
501
502
505
509
xiii
xiv
Contents
29. Toward the Creation of Terahertz Graphene
Injection Laser V. Ryzhii, M. Ryzhii, V. Mitin, and T. Otsuji 29.1 Introduction 29.2 Device Model 29.3 Equations of the Model 29.4 Effective Temperatures and CurrentVoltage
Characteristics (Analytical Analysis) 29.4.1 Low Voltages 29.4.2 Special Cases 29.4.3 Long Optical Phonon Decay Time 29.5 Effective Temperatures and CurrentVoltage
Characteristics (Numerical Results) 29.6 Dynamic Conductivity 29.7 Limitations of the Model and Discussion 29.8 Conclusions
30. Ultrafast Carrier Dynamics and Terahertz Emission in
Optically Pumped Graphene at Room Temperature S. BoubangaTombet, S. Chan, T. Watanabe, A. Satou, V. Ryzhii, and T. Otsuji 30.1 Introduction 30.2 Theory and Background 30.3 Sample and Characterization 30.4 Experiments 30.5 Results and Discussion 30.6 Conclusion 31. Spectroscopic Study on Ultrafast Carrier Dynamics
and Terahertz Amplified Stimulated Emission in
Optically Pumped Graphene T. Otsuji, S. BoubangaTombet, A. Satou, M. Suemitsu, and V. Ryzhii 31.1 Introduction 31.2 Carrier Relaxation and Recombination
Dynamics in Optically Pumped Graphene 31.3 Experiments 31.3.1 Experimental Setup
513
514
516
518
522
522
523
524
524
528
530
535
539
540
542
543
544
546
552
555
556
558
561
561
Contents
31.4
31.3.2 Samples and Characterizations 31.3.2.1 Exfoliated graphene on SiO2/Si 31.3.2.2 Heteroepitaxial graphene on 3CSiC/Si 31.3.3 Results and Discussions 31.3.3.1 Exfoliated graphene on SiO2/Si 31.3.3.2 Heteroepitaxial graphene on 3CSiC/Si Conclusion
32. Gain Enhancement in Graphene Terahertz Amplifiers with Resonant Structures Y. Takatsuka, K. Takahagi, E. Sano, V. Ryzhii, and T. Otsuji 32.1 Introduction 32.2 FDTD Model 32.3 Results and Discussion 32.4 Conclusions 33. Plasmonic Terahertz Lasing in an Array of Graphene Nanocavities
562 562 565 565 565 571 572 577
578 579 580 585 587
V. V. Popov, O. V. Polischuk, A. R. Davoyan, V. Ryzhii, T. Otsuji, and M. S. Shur 34. The Gain Enhancement Effect of Surface Plasmon Polaritons on Terahertz Stimulated Emission in Optically Pumped Monolayer Graphene T. Watanabe, T. Fukushima, Y. Yabe, S. A. Boubanga Tombet, A. Satou, A. A. Dubinov, V. Ya Aleshkin, V. Mitin, V. Ryzhii, and T. Otsuji 34.1 Introduction 34.2 Stimulated Terahertz (THz) Photon and Plasmon Emission in Optically Pumped Graphene 34.3 Experimental Observation of THz Stimulated Plasmon Emission in Optically Pumped Graphene
603
604 606 610
xv
xvi
Contents
34.4
34.3.1 Experimental Setup and Sample
Preparation 610
34.3.2 Temporal Profile and Fourier Spectrum
of the PopulationInverted Graphene
to the THz Pulse Irradiation 612
34.3.3 Spatial Field Distribution of the THz
Probe Pulse Intensities 614
Conclusion 615
35. Graphene Surface Emitting Terahertz Laser: Diffusion
Pumping Concept A. R. Davoyan, M. Yu. Morozov, V. V. Popov, A. Satou, and T. Otsuji 36. Enhanced Terahertz Emission from Monolayer
Graphene with Metal Mesh Structure T. Itatsu, E. Sano, Y. Yabe, V. Ryzhii, and T. Otsuji 36.1 Introduction 36.2 Principle 36.3 Experimental 36.3.1 Basic Structure of THz Amplifier 36.3.2 Measurement Method 36.3.3 EM Simulation Model 36.4 Results and Discussion 36.4.1 GaAs + Graphene 36.4.2 GaAs + Metal 36.4.3 GaAs + Metal + Graphene 36.5 Conclusion
37. Terahertz LightEmitting GrapheneChannel
Transistor Toward SingleMode Lasing D. Yadav, G. Tamamushi, T. Watanabe, J. Mitsushio, Y. Tobah, K. Sugawara, A. A. Dubinov, A. Satou, M. Ryzhii, V. Ryzhii, and T. Otsuji 37.1 Introduction 37.2 Device Design and Fabrication 37.2.1 Design and Fabrication Details 37.2.2 Principles of Operation
619
633
634
635
635
635
636
638
639
639
640
641
642
645
646
648
648
651
Contents
37.3 37.4
Results and Discussions 37.3.1 Broadband THz Light Emission 37.3.2 Towards SingleMode Lasing Conclusions
Part 5 Detectors and Emitters Based on Photon/Plasmon Assisted Tunneling between Graphene Layers
38. Injection Terahertz Laser Using the Resonant
InterLayer Radiative Transitions in
DoubleGrapheneLayer Structure
656
657
660
662
673
V. Ryzhii, A. A. Dubinov, V. Ya. Aleshkin, M. Ryzhii, and T. Otsuji 39. DoubleGrapheneLayer Terahertz Laser: Concept,
Characteristics, and Comparison
685
V. Ryzhii, A. A. Dubinov, T. Otsuji, V. Ya. Aleshkin, M. Ryzhii, and M. Shur 39.1 39.2 39.3 39.4 39.5 39.6 39.7
Introduction Device Structures and Principles of Operation InterGL and IntraGL Dynamic Conductivities Terahertz Gain and GainOverlap Factors Frequency and Voltage Dependences of
the THz Gain Discussion Conclusion
40. SurfacePlasmons Lasing in DoubleGrapheneLayer
Structures
686
687
689
691
694
696
697
703
A. A. Dubinov, V. Ya. Aleshkin, V. Ryzhii, M. S. Shur, and T. Otsuji 40.1 40.2 40.3 40.4
Introduction Dynamic Conductivity Tensor Electric Field Distributions, GainOverlap
Factor, and Modal Gain Conclusions
704
706
710
715
xvii
xviii
Contents
41 Double Injection, ResonantTunneling Recombination, and CurrentVoltage Characteristics in DoubleGrapheneLayer Structures M. Ryzhii, V. Ryzhii, T. Otsuji, P. P. Maltsev, V. G. Leiman, N. Ryabova, and V. Mitin 41.1 Introduction 41.2 Model and the Pertinent Equations 41.3 Spatial and Voltage Dependences of Fermi Energy, Energy Gap, and Potential 41.4 Role of Scattering on Disorder 41.5 CurrentVoltage Characteristics 41.6 Conclusions
42. VoltageTunable Terahertz and Infrared Photodetectors Based on DoubleGrapheneLayer Structures V. Ryzhii, T. Otsuji, V. Ya. Aleshkin, A. A. Dubinov, M. Ryzhii, V. Mitin, and M. S. Shur 43. Plasmons in TunnelCoupled Graphene Layers: Backward Waves with Quantum Cascade Gain D. Svintsov, Zh. Devizorova, T. Otsuji, and V. Ryzhii 43.1 43.2 43.3 43.4 43.5 43.6
Introduction Dispersion Relation for Plasmons in TunnelCoupled Layers HighFrequency Nonlocal Tunnel Current Plasmons in the Presence of Tunneling Effects of Interlayer Twist Discussion and Conclusions
44. Terahertz Wave Generation and Detection in DoubleGraphene Layered van der Waals Heterostructures D. Yadav, S. Boubanga Tombet, T. Watanabe, S. Arnold, V. Ryzhii, and T. Otsuji 44.1 44.2 44.3
Introduction Device Description and Principles of Operation Experimental Methods
719
720 722 728 730 731 735 739
751 752 753 755 764 767 768 783
784 785 789
Contents
44.4 44.5
Results and Discussions Conclusion
45. UltraCompact Injection Terahertz Laser Using the
Resonant InterLayer Radiative Transitions in
MultiGrapheneLayer Structure
790
795
801
A. A. Dubinov, A. Bylinkin, V. Ya. Aleshkin, V. Ryzhii, T. Otsuji, and D. Svintsov 45.1 45.2 45.3 45.4
Introduction Device Model Results and Discussion Conclusion
Part 6 Graphene Based van der Waals Heterostructures for THz Detectors and Emitters 46. Graphene Vertical HotElectron Terahertz Detectors
802
804
808
812
821
V. Ryzhii, A. Satou, T. Otsuji, M. Ryzhii, V. Mitin,
and M. S. Shur
46.1 46.2 46.3
Introduction Device Structures and Principle of Operation Vertical Electron Dark Current and
Photocurrent 46.4 Electron Heating by Incoming THz Radiation 46.5 Responsivity 46.6 Dark Current Limited Detectivity 46.7 Role of the Electron Capture 46.8 Effect of Plasmonic Resonances 46.9 Limitations of the Model 46.10 Discussion 46.11 Conclusions
47. Electron Capture in van der Waals GrapheneBased
Heterostructures with WS2 Barrier Layers
822
824
827
828
830
831
833
834
836
837
839
845
V. Ya. Aleshkin, A. A. Dubinov, M. Ryzhii, V. Ryzhii,
and T. Otsuji
47.1 47.2
Introduction Model and Electron Wave Functions
846
848
xix
xx
Contents
47.3
47.4 47.5
Electron Capture Probability at Different
Scattering Mechanisms 47.3.1 Capture due to the Emission of Barrier
Optical Phonons 47.3.2 Capture due to the Emission of GL
Optical Phonons 47.3.3 Capture Associated with the
ElectronElectron Interaction 47.3.4 Results of Numerical Calculations Capture Parameter and Capture Velocity Conclusion
48. Resonant Plasmonic Terahertz Detection in
Vertical GrapheneBase HotElectron Transistors V. Ryzhii, T. Otsuji, M. Ryzhii, V. Mitin, and M. S. Shur 48.1 Introduction 48.2 Device Model and Related Equations 48.3 Plasma Oscillations and Rectified Current 48.4 GBHET Detector Responsivity 48.4.1 Current Responsivity 48.4.2 Voltage Responsivity 48.5 Discussion 48.6 Conclusions
49. Nonlinear Response of Infrared Photodetectors
Based on van der Waals Heterostructures with
Graphene Layers V. Ryzhii, M. Ryzhii, D. Svintsov, V. Leiman, V. Mitin, M. S. Shur, and T. Otsuji 49.1 Introduction 49.2 Device Structure and Model 49.3 Main Equations 49.4 Dark Characteristics 49.5 Photoresponse at Low IR Radiation Intensities 49.6 Nonlinear Response: High IR Radiation
Intensities 49.7 Comments 49.8 Conclusions
850
850
851
853
855
858
860
865
866
869
873
877
877
880
882
884
889
890
891
893
895
896
898
902
903
Contents
50. Effect of Doping on the Characteristics of Infrared
Photodetectors Based on van der Waals
Heterostructures with Multiple Graphene Layers V. Ryzhii, M. Ryzhii, V. Leiman, V. Mitin, M. S. Shur, and T. Otsuji 50.1 50.2 50.3 50.4 50.5 50.6 50.7
Introduction Structure of GLIPs and Their Operation
Principle Equations of the Model GLIP Responsivity GLIP Detectivity Discussion Conclusions
51. RealSpaceTransfer Mechanism of Negative Differential
Conductivity in Gated GraphenePhosphorene
Hybrid Structures: Phenomenological Heating Model V. Ryzhii, M. Ryzhii, D. Svintsov, V. Leiman, P. P. Maltsev, D. S. Ponomarev, V. Mitin, M. S. Shur, and T. Otsuji 51.1 Introduction 51.2 Model 51.3 Main Equations of the Model 51.3.1 Conductivity of the GP Channel 51.3.2 Carrier Interband Balance 51.3.3 GenerationRecombination and
Energy Balance Equations 51.3.4 General Set of the Equations 51.4 Numerical Results 51.5 Discussion 51.5.1 Screening in the GP Channel 51.5.2 Mutual Scattering of Electrons and
Holes 51.5.3 Optical Phonon Heating 51.5.4 Relaxation of Substrate Optical
Phonons 51.5.5 Possible Applications of the GP
Devices 51.6 Conclusions
911
912
914
915
917
920
924
927
931
932
933
936
936
937
938
940
941
945
945
947
948
949
950
951
xxi
xxii
Contents
52. Negative Photoconductivity and HotCarrier
Bolometric Detection of Terahertz Radiation in
GraphenePhosphorene Hybrid Structures V. Ryzhii, M. Ryzhii, D. S. Ponomarev, V. G. Leiman, V. Mitin, M. S. Shur, and T. Otsuji 52.1 Introduction 52.2 Model 52.3 Conductivity of the GPChannel 52.4 Negative Photoconductivity in the GP
Channels 52.5 Responsivity of the GPPhotodetectors 52.6 Bandwidth and GainBandwidth Product 52.7 Detectivity of the GPBolometers 52.8 Discussion 52.8.1 General Comments 52.8.2 Assumptions 52.9 Conclusions
Index
957
958
959
962
965
967
971
972
973
973
975
976
985
Preface
Preface
The emergence and realization of new materials always strongly affected humankind. Iron and aluminum as well as their various compounds are the main materials used in almost all machines: ships, automobiles, trains, air and spacecraft, and others. Could we fly over oceans in liners taking hundreds of passengers from one point in the globe to another if Mother Nature did not supply us with aluminum. Humankind should be also happy that the Earth provided a huge amount of silicon and that its dioxide is a very stable substance. Would we have supercomputers, cell phones, personal computers, the internet, and many other things without siliconbased micro and nanoelectronics? The utilization of other semiconductor materials, such as gallium arsenide and its relatives, also greatly contributes to modern engineering. Some materials, known for decades, found their applications only in recent years. This is true for graphite and, particularly, its stack of a few monolayers. The unique electrical properties of the graphite monolayer have been known for a rather long time. The band structure of graphite and its monolayer and their consequences on electric characteristics were first described by P. R. Wallace in his paper published in Physical Review in 1947 [1]. The first graphite monolayers were produced in 1962 by H.P. Boehm and his colleagues (see, e.g., [2]). Such monolayers, which are allotropes of carbon consisting of a single layer of carbon atoms forming a hexagonal lattice, is now widely called graphene. The name graphene is a combination of graphite and the suffix ene [3]. However, thanks to pioneering works by A. Geim, K. Novoselov, W. de Heer, Ph. Kim, and their coworkers, only in the beginning of this century did it become understood that the unique properties of graphene can provide it wide application in different areas, in particular, in electronics and optoelectronics (see, e.g., [4]). This discovery caused a huge wave of theoretical, technological, and experimental works and, consequently, publications in the world scientific literature. There is also a large number of real
xxiii
xxiv
Preface
demonstrations of novel graphenebased devices: transistors, optical modulators, sources of electromagnetic radiation, and so forth. In 2010 A. Geim and K. Novoselov received the Nobel Prize for their pathbreaking work, which stressed the importance and prospects of graphene. The prize undoubtedly stimulated the pertinent research and application activities. Among the unique characteristics of graphene, one can indicate the virtually linear dispersion law (of the Dirac type) for electrons and holes accompanied with their gapless energy spectrum and very high electron and hole velocities (about 108 cm/s). Due to such features, graphene is fairly prospective for detectors and sources of electromagnetic radiation in the ranges of frequencies from terahertz to infrared and higher. The high electron and hole characteristic velocity promotes their very high mobilities, particularly at room temperature (much higher than in all other semiconductor materials). Therefore, it is possible to realize the socalled ballistic (collisionless) electron and hole transport across samples (and devices) with micrometer sizes and larger. The latter is very promising for highspeed electronic devices operating in the terahertz frequency range. Excellent dynamic properties of electrons and holes in graphene open prospects in realization of novel plasmonic terahertz devices. In spite of enormous research activity in the area of devices based on graphene, the amount of extensive review material on terahertz devices based on graphene is small. We hope that this review volume, which comprises journal articles by V. Mitin, T, Otsuji, V. Ryzhii, and their collaborators published from 2007 to present, would fill the gap and can be used by researchers and engineers working in the fields of electronics, plasmonics, and influence of plasmonics on device performance. Moreover, we think that the book can be used as a required text for advanced courses for PhD students and as a supplementary material for masterlevel courses. We used it successfully for term paper assignment as well as for projects of masterlevel students. For example, several teams of master’s students can be assigned to deliver consecutive chapters of a selected part for presentation in the class. We also assigned students to work on details of derivation, as in many sections the details are omitted. Moreover, the book will come handy while
Preface
writing small programs to plot results of the final equations first for the same set of parameters, as given in the sections, to be sure that the program is working properly and then to expand the calculation to a new set of parameters to better understand the limits of the results. Apart from the above introductory remarks, the collection comprises six parts separated into chapters. Each chapter presents an original journal article. Part 1 comprises papers devoted to the studies of general electronic and plasmonic phenomena in graphene and some graphenebased structures. It starts from the chapter in which the spectrum of plasmonic waves (the spatiotemporal variations of carrier density accompanied with the ac selfconsistent electric field) was calculated for graphene covered by a highly conducting electrode separated by an insulating layer (gated graphene). The main result of this chapter is that the wave velocity always exceeds the characteristic electron and hole velocity and, therefore, the Fermi velocity in graphene. This implies an important limitation on plasmon Landau damping and related processes. Several chapters in this part deal with the studies of the features of various diode and transistors using the graphene lateral channel, the graphene bilayer, lateral and vertical multiple graphene layer structures, and structures with two graphene layers separated by a tunneling barrier. In Part 2, results related to radiation detectors, in particular, terahertz detectors based on lateral graphenelayer structures, are presented. As demonstrated, graphenebased terahertz detectors can use interband transitions exploiting the absence of the energy gap as well the heating of the carriers by absorbing radiation (hot carrier bolometric detectors). The excitation of the plasmonic oscillations in such detectors can result in their resonant response. The latter can enable very high detector responsivity at resonant conditions. Part 3 demonstrates that optical and injection pumping creating interband population inversion leads to negative dynamic conductivity in different graphenelayer structures. The negative dynamic conductivity in the pumped graphene arises as a result of
xxv
xxvi
Preface
competition between the interband electron transitions from the conduction band to the valence band and the intraband processes of the photon absorption by the carriers (Drude absorption). Due to this, negative dynamic conductivity at the condition of population inversion appears in an intermediate spectral range corresponding to terahertz frequencies. In particular, it is shown that the generation of hot electrons and holes in graphene by optical pumping can result in elevated effective temperatures of the whole electron–hole plasma, adding complexity to the realization of interband population inversion. In Part 4, methods of forming interband population inversion in graphene structures are proposed and analyzed. Also, application for efficient terahertz sources of radiation, in particular, terahertzemitting diodes and lasers, are demonstrated. Different versions of graphenebased sources are considered, for example, with dielectric and slotline waveguides, including that with toothlike metal strips working for a distributed feedback cavity. Part 5 deals with detectors and emitters based on photon/ plasmonassisted tunneling between graphene layers separated with an atomically thin insulating/semiconducting layer. If an ndoped layer of graphene is separated from a pdoped layer of graphene by a thin dielectric, electron resonant tunneling would take place from the nlayer into the player if the Dirac points of both layers are aligned—that is, if energy and momentum are conserved during the tunneling. The shift of the alignment results in photonassisted tunneling. Depending on the direction of the shift, a photon is either absorbed or emitted during the tunneling. That allows to have wellcontrolled emitters or detectors of terahertz radiation. Part 6 expands the concepts of devices considered in Part 5 to a wider group of van der Waals heterostructures based on graphene. In the case of wider barriers, there is no tunneling between graphene layers, but there is a possibility for electrons from the filled valence band go to the widerbandgap material absorbing photons. In the case of transport perpendicular to the layers, the detector is analogous to the conventional quantum well photodetector, but its performance is superior to the latter as its operation is caused by interband absorption that has higher probability and does not depend on polarization. In the case of inplane transport, the conductivity depends on the difference in conductivity of graphene layers and
Preface
barrier layers. Graphene–phosphorene heterostructures are of special interest for inplane transport as mobility in phosphorene is strongly anisotropic and can be substantially lower than the mobility of graphene. This leads to a wellpronounced negative differential conductivity because with an increase in the electric field, electrons can transfer from graphene into phosphorene (real space transfer). As the result of real space transfer, the photoconductivity in graphenephosphorene heterostructures can be positive or negative. We would like to acknowledge our professional colleagues and collaborators with whom we published the papers included in this volume. Also, we wish to thank our loved ones for their support and for forgiving us for not devoting more time to them while working on this volume. Vladimir Mitin Taiichi Otsuji Victor Ryzhii
References 1. P. R. Wallace, The band theory of graphite. Phys. Rev., 71, 622–634 (1947). 2. H. P . Boehm, A. Clauss, G. O. Fischer, U. Hofmann, Das adsorptionsverhalten sehr dünner kohlenstofffolien. Z. Anorg. Allg. Chem., 316, 119–127 (1962), doi:10.1002/zaac.19623160303. 3. H. P. Boehm, R. Setton, and E. Stumpp, Nomenclature and terminology of graphite intercalation compounds. Pure Appl. Chem., 66(9), 1893– 1901 (1994). 4. K. S. Novoselov, A. K. Geim, S. V. Morozov, et. al., Electric field effect in atomically thin carbon films. Science, 306, 666–669 (2004).
xxvii
Part 1
Electronic and Plasmonic
Properties of Graphene and
Graphene Structures
Chapter 1
Plasma Waves in TwoDimensional ElectronHole System in Gated Graphene Heterostructures*
V. Ryzhii,a A. Satou,a and T. Otsujib aComputer
Solid State Physics Laboratory, University of Aizu,
AizuWakamatsu 9658580, Japan
bResearch Institute of Electrical Communication, Tohoku University,
Sendai 9808577, Japan
[email protected]
Plasma waves in the twodimensional electronhole system in a graphenebased heterostructure controlled by a highly conducting gate are studied theoretically. The energy spectra of twodimensional electrons and holes are assumed to be conical (neutrinolike), i.e., corresponding to their zero effective masses. Using the developed model, we calculate the spectrum of plasma waves (spatiotemporal variations of the electron and hole densities and the selfconsistent *Reprinted with permission from V. Ryzhii, A. Satou, and T. Otsuji (2007). Plasma waves in twodimensional electronhole system in gated graphene heterostructures, J. Appl. Phys., 101, 024509. Copyright © 2007 American Institute of Physics. GrapheneBased Terahertz Electronics and Plasmonics: Detector and Emitter Concepts Edited by Vladimir Mitin, Taiichi Otsuji, and Victor Ryzhii
Copyright © 2021 Jenny Stanford Publishing Pte. Ltd.
ISBN 9789814800754 (Hardcover), 9780429328398 (eBook)
www.jennystanford.com
4
Plasma Waves in TwoDimensional ElectronHole System
electric potential). We find that the sufficiently long plasma waves exhibit a linear (soundlike) dispersion, with the wave velocity determined by the gate layer thickness, the gate voltage, and the temperature. The plasma wave velocity in graphene heterostructures can significantly exceed the plasma wave velocity in the commonly employed semiconductor gated heterostructures. The gated graphene heterostructures can be used in different voltage tunable terahertz devices which utilize the plasma waves.
1.1 Introduction
Recent progress in fabrication of graphene, a monolayer of carbon atoms forming a dense honeycomb twodimensional (2D) crystal structure (which can also be considered as an unrolled singlewall carbon nanotube or as a giant flat fullerene molecule), and the demonstration of its exceptional electronic properties have attracted much interest [1]. The possibility of creating novel electronic devices on the basis of graphene heterostructures (see, for instance, Refs. [2] and [3]) has caused a surge of experimental and theoretical publications. The massless neutrinolike energy spectrum of electrons and holes in graphene can lead to specific features of the transport properties [4, 5], photonassisted transport [6], and quantum Hall effect [7–9], as well as the unusual highfrequency properties and collective behavior of the 2D electron or hole (2DEG or 2DHG) systems in graphenebased heterostructures [10–13]. The plasma waves in graphenebased heterostructures, in which the 2DEG or 2DHG system can serve as a resonant cavity or as a voltagecontrolled waveguide, can be used in different devices operating in the terahertz (THz) range of frequencies [14, 15]. Since the spectrum of plasma waves is sensitive to the electron (hole) mass, the plasma waves in graphene heterostructures can exhibit specific features associated with the zero electron and hole masses. The electron and hole sheet densities in graphene heterostructures with the conducting gate can be effectively varied by the gate voltage [1]. Thus, the massless electron and hole spectra and voltage tunability of the electron and hole densities open up new opportunities to create novel THz plasma wave devices based on graphene heterostructures on silicon substrates.
Equations of the Model
In this work, the spectrum of plasma waves (spatiotemporal variations of the electron and hole densities and selfconsistent electric potential) in a gated graphene heterostructure in wide ranges of the gate voltages and the temperatures is studied. A gated graphene heterostructure (with n+Si substrate serving as the gate and the gate layer made of SiO2) shown in Fig. 1.1 is considered. A limiting case of relatively large (positive) gate voltages at sufficiently low temperatures was considered recently by one of the present authors [13]. In this case, the plasma waves are associated with a degenerate 2DEG. Here, we generalize the study of plasma waves in gated graphene heterostructures for the situation when the gate voltage and temperature vary in wide ranges, so that the contribution of both electrons and holes and the features of their energy distributions can be essential.
1.2 Equations of the Model
We shall consider “classical” plasma waves with the wavelength l markedly exceeding the characteristic length of the electron de Broglie wave lF. In this case, we can use the following kinetic equations coupled with the equation governing the selfconsistent electric potential: ∂fe ∂f ∂f ∂j + vp e + e e ∂t ∂r ∂p ∂r
= Ie ,
z =0
(1.1)
Figure 1.1 Schematic view of a gated graphene heterostructure.
∂fh ∂f ∂f ∂j + vp h  e h ∂t ∂r ∂p ∂r
= Ih , z=0
(1.2)
5
6
Plasma Waves in TwoDimensional ElectronHole System
Here, fe = fe(p, r, t) and fh = fh(p, r, t) are the electron and hole distribution functions, respectively, j = j(r, z, t) is the electric potential, p = (px , py) is the electron (or hole) inplane momentum, r = (x, y) (x and y correspond to the directions in the graphene layer plane, while axis z is directed perpendicular to this plane), and e = e is the electron charge. The quantity vp is the velocity of an electron and a hole with momentum p: vp = ∂ep/∂p, where ep = uFp corresponds to the electron and hole massless spectra and uF is the characteristic (Fermi) velocity. As a result, vp = uFp/p, where p = p. The terms Ie and Ih on the righthand sides of Eqs. (1.1) and (1.2) govern the processes of electron and hole scattering and recombination. For the sake of simplicity, we disregard the electron and hole scattering processes and their recombination, and therefore set Ie = 0 and Ih = 0. This is justified when the characteristic frequency of plasma waves significantly exceeds the pertinent collision frequencies. The Poisson equation which supplements Eqs. (1.1) and (1.2) is presented as ∂2j ∂x
2
+
∂2j ∂y
2
+
∂2j ∂z
=
2
4pe ( S e  S h )d ( z ), æ
(1.3)
where æ is the dielectric constant of the surrounding space and d(z) is the Dirac delta function playing the role of the form factor of the 2DEG and 2DHG localization in the direction perpendicular to the graphene plane. Here, we have neglected the finiteness of the localization region thickness. The electron and hole sheet densities Se = Se(r, t) and Sh = Sh(r, t) and the distribution functions fe = fe(p, r, t) and fh = fh(p, r, t) are related by the following equations: Se =
2
Ú d pf , 2
(2p )
2
e
Sh =
2
Ú d pf 2
(2p )
2
h,
(1.4)
where is the reduced Planck constant. In equilibrium, the electron and hole distribution functions are given by È Ê v p  eF ˆ ˘ fe0 = Í1 + exp Á F ˙ Ë kBT ˜¯ ˚˙ ÍÎ
1
È Ê v p  eF ˆ ˘ = Í1 + exp Á F ˙ Ë kBT ˜¯ ˚˙ ÍÎ
1
fh0
,
,
(1.5)
Dispersion Equation for Plasma Waves
where eF is the Fermi energy, T is the temperature, and kB is the Boltzmann constant. The Fermi energy is determined by the condition of neutrality æVg/Wg = 4pe(Se0 – Sh0), where Vg is the gate voltage, Wg is the gate layer thickness, and Se0 and Sh0 are the equilibrium electron and hole densities, respectively. Considering Eq. (1.4) the latter condition can be presented as p æ2Vg 2eWg
Ú
= d 2p( fe0  f h0 ).
Taking into account Eq. (1.5), Eq. (1.6) can be rewritten as ÏÔ È Ê v p  eF ˆ ˘ = dp p Ì Í1 + exp Á F ˙ 0 4eWg Ë kBT ¯˜ ˚˙ ÔÓ ÎÍ 1 È Ê v p + e F ˆ ˘ ¸Ô  Í1 + exp Á F ˙ ˝, Ë kBT ¯˜ ˙˚ Ô ÎÍ ˛
æ2Vg
Ú
•
1
or, introducing the variable x = uFp/kBT, as æ2vF2Vg
Ê e ˆ =FÁ F ˜ , Ë kBT ¯ 4eWg (kBT ) 2
where
Ê e ˆ FÁ F ˜ = Ë kBT ¯
Ú
•
0

(1.6)
(1.7)
È 1 dx x Í Î 1 + exp(x  e F / kBT )
˘ 1 ˙. 1 + exp(x + e F / kBT ) ˚
(1.8)
At Vg = 0, Eqs. (1.7) and (1.8) naturally yield eF = 0 (which corresponds to Se0 = Sh0).
1.3 Dispersion Equation for Plasma Waves
Using the standard smallsignal analysis, i.e., assuming that fe,h(p, r, t) = fe0,h0(p) + dfe,h(p)exp[i(kx–wt)] and j(r, z, t) = dj(z)exp[i(kx–wt)], where dfe,h fe0,h0 are small perturbations, k and w are the wavenumber and frequency of the plasma wave, respectively, from Eqs. (1.1) and (1.2) we arrive at the following equations:
7
8
Plasma Waves in TwoDimensional ElectronHole System
(kvF px /p  w )d fe =  ek
∂fe0 df , ∂px z =0
(kvF px /p  w )d fh = ek
∂fh0 dj . ∂px z=0
(1.9) (1.10)
Assuming that the gate is equipotential (its potential is equal to Vg), Eq. (1.3) results in the following: dj z =0 = 
4p e(dS e  dS h )
æ  k  ÈÎcoth(kWg ) + 1˘˚ 2
Using Eqs. (1.4) and (1.11 ), we obtain dj z=0 = 
(1.11)
.
d p(d f p æ  k [coth(k  W ) + 1] Ú 2e
2
2
e
 d fh ).
g
(1.12)
Substituting dfe and dfh from Eqs. (1.9) and (1.10) into Eq. (1.12), we arrive at the dispersion equation relating the wavenumber and frequency of the plasma wave,
È ∂( fe0 + f h0 ) ˘ p æ2 [coth(k  Wg ) + 1] d 2p = Í˙. (1.13) 2 (k /k ) (w  kvF px /p) Î ∂px 2e ˚
Ú
Taking into account Eqs. (1.5) and (1.6), Eq. (1.13) can be transformed as p æ 2vF2 k [coth(k  Wg ) + 1] 4e2kBT = ¥
Ú
•
0
Ú
p
0
dQ cos Q (w/kvF  cos Q )
È ˘ 1 1 dx Í + ˙. Î 1 + exp(x  e F /kBT ) 1 + exp(x + e F /kBT ) ˚
(1.14)
Here, we have used the variables Q = cos1(px/p) and x = uFp/kBT. Integrating in Eq. (1.14) over dQ and dx, we arrive at the following dispersion equation for plasma waves: Ê æ2v2 ˆ =1+Á 2 F ˜ ÁË 4e Wg kBT ˜¯ (w/kvF )2  1 (w / kvF )
¥
 k  Wg [coth(k  Wg ) + 1] ln[2 + exp(e F /kBT ) + exp( e F /kBT )]
.
(1.15)
Limiting Cases
Equation (1.15) yields
w=
where
1  (aDK )2/(aDK + 1)2
a= D=
and
vF k
4e2Wg e F æ2vF2
,
,
Ê e ˆ Ê e ˆ˘ kBT È ln Í2 + exp Á F ˜ + exp Á  F ˜ ˙ , eF Ë kBT ¯ Ë kBT ¯ ˚˙ ÎÍ K−1 =  k Wg[coth(kWg) + 1].
(1.16) (1.17) (1.18) (1.19)
1.4 Limiting Cases 1.4.1 Low Temperatures or High Gate Voltages At sufficiently low temperatures or at sufficiently high (positive) gate voltages, the electron density substantially exceeds the density of holes and the electron Fermi energy is much larger than the thermal energy (eF = ħvF æVg /2eWg kBT), so that 2DEG is degenerate and D j 1. In this case, Eq. (1.14) and (1.15) yield w=
with
a=
vF k
1  (aK )2/(aK + 1)2
4e2Wg e F æ�2vF2
�
8e3WgVg æ�2vF2
,
(1.20)
.
(1.21)
At sufficiently high gate voltages, a 1. In this case, from Eq. (1.16) we obtain w vF k
a . 2k  Wg [coth(k  Wg ) + 1]
(1.22)
For long plasma waves (kWg 1), Eq. (1.22) yields (compare with Ref. [13])
9
10
Plasma Waves in TwoDimensional ElectronHole System
Ê k  Wg ˆ a w vF k Á 1 . 2 ¯˜ 2 Ë
(1.23)
One can see that relatively long plasma waves (longer than the gate layer thickness) in the gated graphene exhibit a linear (soundlike) spectrum with the wave phase and group velocities, which depend on the gate voltage (via the voltage dependence of parameter a). In this case, the wave phase and group velocities, w/k and dw/dk, are equal to s vF
2e2Wg e F a = µ Wg1/4Vg1/4 . 2 2 æ
(1.24)
These velocities depend on the gate voltage (via the voltage dependence of parameter a) as Vg1/4. If æ = 3.8, uF = 108 cm/s, Wg = 3 ¥ 105 cm (as in Ref. [1]), and Vg = 1 – 10 V, one obtains a j 48 – 152 and s j (4.9–8.7) ¥ 108 cm/s. In this case, the electron sheet density S0 j 7 ¥ (1010–1011) cm–2 corresponds to the Fermi energy eF j 40–126 meV. Since a 1 in a wide range of parameters, one can assume that s > uF (or even s uF). For short plasma waves (kWg > 1), Eq. (1.20) yields w � vF k 
e 2e F a . = vF k  4Wg æn2vF2
(1.25)
1.4.2 Elevated Temperatures and Low Gate Voltages At low gate voltages, the Fermi energy is small. In particular, when Vg = 0, one has eF = 0. Therefore, at low gate voltages one can assume that eF < kBT. In this case, D j (kBT/eF)ln 4. As a result, from Eq. (1.16) one can obtain w=
where
vF k
1  ( bK )2/( b K + 1)2
b=
8 ln 2e2Wg kBT æ2vF2
.
,
(1.26) (1.27)
At elevated temperatures T Tg = (æħ2u2F/4 ln 4kBe2Wg), parameter b 1, and
Limiting Cases
w vF k
b . 2 k  Wg [coth(k  Wg ) + 1]
(1.28)
If æ = 3.8, uF =108 cm/s, and Wg = 3 ¥ 10–5 cm, one obtains the following estimate: Tg j 7 K. For long plasma waves (kWg 1) one obtains Ê k  Wg ˆ 4 ln 2e2Wg kBT w " k Á1 , 2 ˜¯ æt2 Ë
so that the phase and group velocities can be presented as
(1.29)
Figure 1.2 Plasma wave frequency versus wavenumber calculated for a graphene heterostructure (Wg = 3 ¥ 10–5 cm and T = 10 K) at different gate voltages.
s
4 ln 2e2Wg kBT æn
2
µWg1/2T 1/2 .
(1.30)
As follows from Eq. (1.24), the frequency and the phase and group velocities of long plasma waves increase with the temperature as T1/2. This is due to the pertinent increase in the electron and hole densities. For relatively short plasma waves (kWg 1) we arrive at [11] w
k 
2 ln 2e2kBT æ
2
.
(1.31)
11
12
Plasma Waves in TwoDimensional ElectronHole System
1.5 General Results and Discussion The spectra of plasma waves in a graphene heterostructure with uF = 108 cm/s at T = 10 K calculated using Eq. (1.15) invoking Eq. (1.7) for different gate voltages are shown in Fig. 1.2. The plasma frequency versus wavenumber dependences are close to linear dependences at small wavenumbers (w µ k). At large wavenumbers (short plasma waves), the plasma frequency increases with the wavenumber as w µ k . As seen, the plasma frequency pronouncedly increases with increasing gate voltage. Figure 1.3 shows the dependence of the plasma wave phase velocity s (at small k) as a function of the gate voltage and the temperature. As follows from Fig. 1.3, the phase velocity is sensitive to the temperature only at low gate voltages when 2DEG and 2DHG systems are not degenerate. This is confirmed by the dependences shown in Fig. 1.4.
Figure 1.3 Dependences of the plasma wave phase velocity (long plasma waves) on the gate voltage and temperature.
Taking into account that for a degenerate 2DEG with massless electrons [as it follows from Eq. (1.4)] the dc electron density [16] is S e0 =
e F2
2p2vF2
,
and introducing the fictitious electron mass m=
eF
vF2
=
vF
æVg
2eWg
µWg1/2Vg1/2 ,
(1.32)
(1.33)
General Results and Discussion
the wave velocity s can be presented in the form
s=
4p e2Wg S e0 æm
=
eVg m
,
(1.34)
which formally coincides with that obtained for the “normal” 2DEG, s* =
4pe2Wg S e0 æ*m*
=
eVg
m*
,
(1.35)
where m* is the electron (hole) “normal” effective mass and æ* is the dielectric constant of the pertinent material (see, for instance, Refs. [14] and [15]). The fictitious mass m determines the relationship between the electron mobility and electron transport time [16]. However, the voltage dependences of s in the 2DEG of massless and normal electrons are different. The point is that in both cases Se µ Vg . But, the effective mass of the massless electrons increases with Vg as m µ eF µ Vg 1/2, whereas an increase in the effective mass of normal electrons is weak because it is associated with a modest nonparabolicity of their energy spectrum. One can see from Eqs. (1.34) and (1.35) s æ*m* = µWg1/4Vg1/4 . æm s*
(1.36)
Figure 1.4 Dependences of the plasma wave phase velocity (long plasma waves) on the gate voltage in graphene heterostructures at different temperatures.
13
14
Plasma Waves in TwoDimensional ElectronHole System
Since m < m* in certain ranges of thicknesses and voltages and usually æ < æ*, the plasma wave velocity in graphene heterostructures can pronouncedly exceed that in normal heterostructures. For example, assuming that uF = 108 cm/s, æ = 3.8, æ* = 12, Wg = (1–3) ¥ 10–5 cm, and Vg = 1–3 V, the ratio of the wave velocity in graphene heterostructures to that in AlGaAf/GaAs heterostructures with m* = 6 ¥ 10–29 g can be estimated as s/s* j 3–5. For a nondegenerate 2DEG2DHG system (Vg = 0 and eF = 0), Eq. (1.4) yields S e0 = S h0
1Êk Tˆ = Á B ˜ p Ë vF ¯
2
Ú
•
0
2
dx x p Ê kBT ˆ = . 1 + exp x 12 ÁË vF ¯˜
(1.37)
In this case, taking into account that the net carrier density is equal to Se0 + Sh0, the wave velocity can be presented in the form s=
4p e2Wg ( S e0 + S h0 ) æm
,
(1.38)
in which m = (p2kBT/12uF2). As follows from Eq. (1.16), the plasma wave phase velocity always exceeds the electron (hole) velocity, i.e., w/k > uF, disregarding the shape of the electron (hole) distribution. This implies that the Landau damping of the plasma waves in the system under consideration is absent. The plasma wave damping is associated with the electron (hole) scattering. The damping of the plasma waves associated with the scattering can be estimated as g = 1/2t, where t is the electron transport time. This time and the electron mobility m in the massless 2DEG are related by an equation which is different from that for the customary 2DEG. Taking into account that for the massless 2DEG the dc conductivity is proportional to eFt [16], one can express t via m: t = mm/e, where, in contrast to the semiconductors with the customary electron spectrum, m = eF/u2F, i.e., the fictitious mass introduced above.
Acknowledgment
This work was financially supported by the GrantinAid for Scientific Research (S) from the Japan Society for Promotion of Science, Japan.
References
References 1. K. S. Novoselov, A. K. Geim, S. V. Morozov, D. Jiang, M. I. Katsnelson, I. V. Grigorieva, S. V. Dubonos, and A. A. Firsov, Nature, 438, 197 (2005).
2. C. Berger, Z. Song, T. Li, X. Li, A. Y. Ogbazhi, R. Feng, Z. Dai, A. N. Marchenkov, E. H. Conrad, P. N. First, and W. A. de Heer, J. Phys. Chem., 108, 19912 (2004). 3. B. Obradovic, R. Kotlyar, F. Heinz, P. Matagne, T. Rakshit, M. S. Giles, M. A. Stettler, and D. E. Nikonov, Appl. Phys. Lett., 88, 142102 (2006).
4. K. Nomura and A. H. MacDonald, eprint condmat/0606589 (2006). 5. I. L. Aleiner and K. B. Efetov, Phys. Rev. Lett., 97, 236801 (2006).
6. B. Trauzettel, Ya. M. Blanter, and A. F. Morpurgo, eprint cond mat/0606505 (2006). 7. V. P. Gusynin and S. G. Sharapov, Phys. Rev. Lett., 95, 146801 (2005).
8. Y. Zhang, Y.W. Tan, H. Stormer, and P. Kim, Nature, 438, 201 (2005).
9. D. Abanin, P. A. Lee, and L. S. Levitov, Phys. Rev. Lett., 96, 176803 (2006).
10. V. P. Gusynin, S. G. Sharapov, and J. P. Carbotte, Phys. Rev. Lett., 96, 256802 (2006). 11. L. A. Falkovsky and A. A. Varlamov, eprint condmat/0606800 (2006). 12. O. Vafek, Phys. Rev. Lett., 97, 266406 (2006).
13. V. Ryzhii, Jpn. J. Appl. Phys., Part 2, 45, L923 (2006).
14. M. Dyakonov and M. Shur, IEEE Trans. Electron Devices, 43, 1640 (1996). 15. M. S. Shur and V. Ryzhii, Int. J. High Speed Electron. Syst., 13, 7 (2003). 16. V. P. Gusynin and S. G. Sharapov, Phys. Rev. B, 73, 245411 (2006).
15
Chapter 2
Device Model for Graphene Bilayer FieldEffect Transistor*
V. Ryzhii,a,b M. Ryzhii,a,b A. Satou,a,b T. Otsuji,b,c and N. Kirovad aComputational Nanoelectronics Laboratory, University of Aizu, AizuWakamatsu 9658580, Japan bJapan Science and Technology Agency, CREST, Tokyo 1070075, Japan cResearch Institute for Electrical Communication, Tohoku University, Sendai 9808577, Japan dLaboratoire de Physique des Solides, Univ. ParisSud, CNRS, UMR 8502, F91405 Orsay Cedex, France [email protected]
We present an analytical device model for a graphene bilayer fieldeffect transistor (GBLFET) with a graphene bilayer as a channel, and with back and top gates. The model accounts for the dependences of the electron and hole Fermi energies as well as energy gap in different sections of the channel on the bias backgate and topgate *Reprinted with permission from V. Ryzhii, M. Ryzhii, A. Satou, T. Otsuji, and N. Kirova (2009). Device model for graphene bilayer fieldeffect transistor, J. Appl. Phys., 105, 104510. Copyright © 2009 American Institute of Physics. GrapheneBased Terahertz Electronics and Plasmonics: Detector and Emitter Concepts Edited by Vladimir Mitin, Taiichi Otsuji, and Victor Ryzhii
Copyright © 2021 Jenny Stanford Publishing Pte. Ltd.
ISBN 9789814800754 (Hardcover), 9780429328398 (eBook)
www.jennystanford.com
18
Device Model for Graphene Bilayer FieldEffect Transistor
voltages. Using this model, we calculate the dc and ac sourcedrain currents and the transconductance of GBLFETs with both ballistic and collision dominated electron transport as functions of structural parameters, the bias backgate and topgate voltages, and the signal frequency. It is shown that there are two threshold voltages, Vth,1 and Vth,2, so that the dc current versus the topgate voltage relation markedly changes depending on whether the section of the channel beneath the top gate (gated section) is filled with electrons, depleted, or filled with holes. The electron scattering leads to a decrease in the dc and ac currents and transconductances, whereas it weakly affects the threshold frequency. As demonstrated, the transient recharging of the gated section by holes can pronouncedly influence the ac transconductance resulting in its nonmonotonic frequency dependence with a maximum at fairly high frequencies.
2.1 Introduction
The features of the electron and hole energy spectra in graphene provide the exceptional properties of graphenebased heterostructures and devices [1–6]. However, due to the gapless energy spectrum, the interband tunneling [7] can substantially deteriorate the performance of graphene fieldeffect transistors (GFETs) with realistic device structures [8–11]. To avoid drawbacks of the characteristics of GFETs based on graphene monolayer with zero energy gap, the patterned graphene (with an array of graphene nanoribbons) and the graphene bilayers can be used in graphene nanoribbon FETs (GNRFETs) and in graphene bilayer FETs (GBLFETs), respectively. The sourcedrain current in GNRFETs and GBLFETs, as in the standard FETs, depends on the gate voltages. The positively biased back gate provides the formation of the electron channels, whereas the negative bias voltage between the top gate and the channels results in forming a potential barrier for electrons which controls the current. By properly choosing the width of the nanoribbons, one can fabricate graphene structures with a relatively wide band gap [12] (see also Refs. [13–16]). Recently, the device dc and ac characteristics of GNRFETs were assessed using both numerical [14] and analytical [17–19] models. The effect of the transverse electric field (to the GBL plane) on the energy spectrum of GBLs [20–22] can also be used to manipulate and optimize the GBL
GBLFET Energy Band Diagrams
FET characteristics. A significant feature of GBLFETs is that under the effect of the transverse electric field not only the density of the twodimensional electron gas in the GBL varies, but the energy gap between the GBL valence and conduction bands appears. This effect can markedly influence the GBLFET characteristics. The structure of a GBLFET is shown in Fig. 2.1. In this chapter, we present a simple analytical device model for a GBLFET, obtain the device dc and ac characteristics, and compare these characteristics with those of GNRFETs. The chapter organized as follows. In Section 2.2, we consider the GBLFET band diagrams at different bias voltages and estimate the energy gaps and the Fermi energy in different sections of the device. Section 2.3 deals with the Boltzmann kinetic equation, which governs the electron transport at dc and ac voltages and the solutions of this equation. The cases of the ballistic and collision dominated electron transport are considered. In Sections 2.4 and 2.5, the dc transconductance and the ac frequencydependent transconductance are calculated using the results of Section 2.3. Section 2.6 deals with the demonstration and analysis of the main obtained results, numerical estimates, and comparison of the GBLFET properties with those of GNRFETs. In Section 2.7, we draw the main conclusions. In Appendix, some intermediate calculations related to the dynamic recharging of the gated section by holes due to the interband tunneling are singled out.
Figure 2.1 Schematic view of the GBLFET structure.
2.2 GBLFET Energy Band Diagrams We assume that the bias backgate voltage Vb > 0, while the bias topgate voltage Vt < 0. The electric potential of the channel at the source
19
20
Device Model for Graphene Bilayer FieldEffect Transistor
and drain contacts are j = 0 and j = Vd, respectively, where Vd is the bias drain voltage. The former results in the formation of a 2DEG in the GBL. The distribution of the electron density S along the GBL is generally nonuniform due to the negatively biased top gate forming the barrier region beneath this gate. Simultaneously, the energy gap Eg is also a function of the coordinate x (its axis is directed in the GBL plane from the source contact to the drain contact) being different in the source, topgate, and drain sections of the channel (see Fig. 2.2). Since the net topgate voltage apart from the bias component Vt comprises the ac signal component dV(t), the height of the barrier for electrons entering the section of the channel under the top gate (gated section) from the source side can be presented as D
(t) = D0 + dD(t).
(2.1)
Depending on the Fermi energy in the extreme sections of the channel, in particular, on its value, eF in the source section and on the height of the barrier in this section D0, there are three situations. The pertinent the GBLFET energy band diagrams are demonstrated in Fig. 2.2. The spatial distributions of electrons and holes in the GBL channel are different depending on the relationship between the topgate voltage Vt and two threshold voltages, Vth,1 and Vth,2. These threshold voltages are determined in the following. When Vth,2 < Vth,1 < Vt, the top of the conduction band in the gated section is below the Fermi level (Fig. 2.2a). In this case, an n+nn+ structure is formed in the GBL channel. At Vth,2 < Vt < Vth,1, the Fermi level is between the top of the conduction band and the bottom of the valence band in this section (Fig. 2.2b). This topgate voltage range corresponds to the formation of an n+in+ structure. If Vt < Vth,2 < Vth,1, both band edges are above the Fermi level (Fig. 2.2c), so that n+p and pn+ junctions are formed beneath the edges of the top gate. In the first and third ranges of the top gate voltage (a and b ranges), the electron and hole populations of the gated section are essential. In the second range (range b), the gated section is depleted. In the voltage range a, the sourcedrain current is associated with a hydrodynamical electron flow (due to effective electronelectron scattering) in the gated section. In this case, the sourcedrain current and GBLFET characteristics are determined by the conductivity of the gated section, which, in turn, is determined by the electron density and scattering mechanisms including the electron
GBLFET Energy Band Diagrams
electron scattering mechanism, and by the selfconsistent electric field directed in the channel plane. In such a situation, different hydrodynamical models of the electron transport (including the driftdiffusion model) can be applied (see, for instance, Refs. [23–27]). (a) ε F
Eg,s (b)
Eg
Eg,d = Eg,s
Δ(t)
(c)
(d) εF Eg,s
eVd Eg,d < Eg,s
Figure 2.2 Band diagrams at different top gate bias voltages (Vb > 0, Vd = 0): (a) Vth,2 < Vth,1 < Vt, (b) Vth,2 < Vt < Vth,1 (depleted gated section), and (c) Vt < Vth,2 < Vth,1 (gated section filled with holes), Panel (d) corresponds to Vth,2 < Vt < Vth,1 but with Vd > 0.
If Vth,2 < Vt < Vth,1, considering the potential distribution in the direction perpendicular to the GBL plane invoking the gradual channel approximation [28, 29] and assuming for simplicity that the thicknesses of the gate layers separating the channel and the pertinent gates, Wb and Wt, are equal to each other Wb = Wt = W, we obtain
(Vb + Vt ) 1 , dD(t ) =  edV (t ), (2.2) 2 2 where e = e is the electron charge. In the voltage range in question, the electron system in the gated section is not degenerate. This voltage range, as well as the range Vt < Vth,2 < Vth,1, correspond to the GBLFET “offstate.” Similar formulas take place for the barrier height from the drain side (with the replacement of D0 by D0 + eVd). In the cases when Vth,2 < Vth,1 < Vt or Vt < Vth,2 < Vth,1, D 0 = e
21
22
Device Model for Graphene Bilayer FieldEffect Transistor
(Vb + Vt ) 2peW ± Â0 , 2 k 1 2peW dD(t ) =  edV (t ) ± d Â (t ). 2 k D 0 = e
(2.3)
Here Â0 + d Â (t ) are the electron and hole densities in the gated section and κ is the dielectric constant of the gate layers. In the most interesting case when the electron densities in the source and drain sections are sufficiently large, so that the electron systems in these sections are degenerate. Considering this, the height of the barrier D0 is given by D 0 = e
D 0 = e
Vt (aB / 8W ) Ê a ˆ eVt Á B ˜ , Ë 8W ¯ [1 + (aB / 4W )]
Vt (aB / 8W ) + (Vt  Vb )(d / 2W ) , [1 + (aB / 4W )]
(2.4)
(2.5)
when Vth,2 < Vth,1 < Vt and Vt < Vth,2 < Vth,1, respectively. Here aB = κħ2/me2 is the Bohr radius, d is the effective spacing between the graphene layers in the GBL which accounts for the screening of the electric field between these layers [20, 21]. This quantity is smaller than the real spacing between the graphene layers in the GBL d0 j 0.36 nm. The Bohr radius aB can be rather different in different materials of the gate layers. In the cases of SiO2 and HfO2 (with k j 20 [30, 31]) gate gate layers, aB j 4 nm and aB j 20 nm, respectively. In deriving Eqs. (2.4) and (2.5), we have taken into account that in real GBLFETs, (aB/8W) 1. For the normal GBLFET operation, the electron densities, S s and S d , induced by the backgate voltage in the source and drain sections, respectively, should be sufficiently high markedly exceeding their thermal value ST = 2 ln 2mkBT/ph2, where kB is the Boltzmann constant and T is the temperature. This occurs when Vb > ln 2(8W/ aB) ¥ (kBT/e) + VT. In such a case, i.e., at sufficiently high backgate voltages, the Fermi energy in the source section is given by eF =
È Ê a eVb ˆ ˘ kBT ln Íexp Á B  1˙ . [1 + (aB / 8W )] ÍÎ Ë 8W kBT ¯˜ ˚˙
(2.6)
Here we considered that the electron density in the source section S s= kVb/4peW (the electron density in the drain section of the channel is approximately equal to S d = k(Vb – Vd)/4peW). If aB = 4 – 20 nm
GBLFET Energy Band Diagrams
at T = 300 K, VT j 0.035 – 0.173 V. As follows from Eq. (2.6), the Fermi energy in the source section at Vb VT is a linear function of Vb, practically independent of the temperature, and it can be presented as
e F � eVb
(aB / 8W ) Ê a ˆ � eVb Á B ˜ � kBT. Ë 8W ¯ [1 + (aB / 8W )]
(2.7)
Setting W = 5 nm, aB = 4 – 20 nm, and Vb = 1 V, we obtain eF = 48 – 91 meV. This case corresponds to the electron density in the source section is S s j 4 ¥ 1012 –2 ¥ 1013 cm–2. At Vd Vb, the electron density in the drain section is somewhat smaller but of the same order of magnitude. Comparing Eqs. (2.2), (2.4), and (2.5), one can see that the height of the barrier D0 increases with increasing absolute value of the topgate voltage rather slow in the voltage ranges a and “c” in contrast with its steep increase in the voltage range b. Since the energy gaps in GBLs Eg,s, Eg, and Eg,d depend on the local transverse electric field [20–22], they are different in different sections of the channel depending on the bias voltages,
E g ,s =
edVb ed (V  V ) ed(Vb  Vd ) , E g = 0 b t , E g ,d = . 2W 2W 2W
(2.8)
One can see that at Vt < 0 and Vd > 0, one obtains Eg > Eg,s ≥ Eg,d. Since d aB, the energy gap in the source section is much smaller than the Fermi energy in this section. Indeed, assuming d j d0 = 0.36 nm and W = 5 nm for Vb = 1 V from Eq. (2.8), we obtain Eg,s j 36 meV. However, the energy gap in the gated section at sufficiently high topgate voltages can be relatively large (see below). Naturally, an increase in the topgate voltage leads to an increase in the Fermi energy in the source (drain) section as well to an increase in the energy gaps in all sections. The threshold voltages Vth,1 and Vth,2 are determined by the conditions D0 = eF and D0 = eF + Eg, respectively. The latter implies that the Fermi energy of holes in the gated section e F( hole ) = D0 – eF – Eg = 0. As a result, the threshold voltages are given by d ˆ a ˆ a Ê Ê Vth ,1 Vb Á 1 + B ˜ , Vth ,2 Vb Á 1 + B + 0 ˜ . Ë Ë 4W ¯ 4W W ¯
(2.9)
23
24
Device Model for Graphene Bilayer FieldEffect Transistor
Since one can assume that d W, the threshold voltages are close to each other, Vth,1 Vth,2 with Vth,2 – Vth,1 j (2d0/W)Vb 4Eg,s/e. The values of the energy gap in the gated section at the threshold top gate voltages are given by
Eg
Vt =Vth , 1
E g
Vt =Vth,2
ed0Vb Êd ˆ 2E g ,s Á 0 ˜ . Ë d¯ W
(2.10)
Using the same parameters as in the above estimate of the energy gap in the source section, for the energy gap in the gated section at Vt j Vth,1 j –1 V, we obtain Eg j 72 meV. In the following we restrict our consideration by the situations when the height of the barrier for electrons in the gated section is sufficiently large (so that D0 > eF), which corresponds to the band diagrams shown in Figs. 2.2b and c.
2.3 Boltzmann Kinetic Equation and Its Solutions
The quasiclassical Boltzmann kinetic equation governing the electron distribution function fp = fp (x, t) in the section of the channel covered by the top gate (gated section) can be presented as
∂fp ∂t
+ vx
∂f p ∂x
Ú
= d 2qw(q)( fp + q  fp )d (e p +q  e p ).
(2.11)
Here, taking into account that the electron (and hole) dispersion relation at the energies close to the bottom of the conduction band is virtually parabolic with the effective mass m (m ~ 0.04 m0, where m0 is the bare electron mass), for the energy of electron with momentum p = (px, py) we put ep = p2/2m = e, ux = px/m = p cos q/m, where cos q = px/p (the xaxis and the yaxis are directed in the GBL plane) and w(q) is the probability of the electron scattering on disorder and acoustic phonons with the variation of the electron momentum by quantity q. The density of the electron (thermionic) current, J = J(x, t), in the gated section of the channel (per unit length in the ydirection) can be calculated using the following formula:
J=
4e
(2ph )2
Úd p v 2
x fp ,
(2.12)
Boltzmann Kinetic Equation and Its Solutions
where ħ is the reduced Planck constant. Disregarding the electronelectron collisions in the gated section of the channel (due a low electron density in this section in contrast to the source and drain sections where the electronelectron collisions are essential), we consider two limiting cases: ballistic transport of electrons across the gated section and strongly collisional electron transport.
2.3.1 Ballistic Electron Transport
If dV(t) = dVωe–iωt, where dVω Vt and ω are the amplitude and frequency of the ac signal, then the electron distribution function can be searched as fp = F0 + dFω (x) e–iωt and D = D0 + dDωe–iωt. Assuming that eVd kBT and solving Eq. (2.11) with the boundary conditions,
È e  D(t )  e ˘ = exp Í F ˙ , fp kBT ˚ Î where Lt is the top gate length, we obtain fp
px ≥0, x =0
px £0, x = Lt
Ê e  D0  e ˆ F0 exp Á F Q(px ), kBT Ë ¯˜
Ê e  D0  e m x ˆ dFw ( x ) = exp Á F + iw 2e cos Q ¯˜ kBT Ë Ê d Dw ˆ ¥ ÁQ( px ). Ë kBT ¯˜
0,
(2.13) (2.14)
(2.15)
Here, Q(px) is the unity step function. The first boundary condition given by Eq. (2.14) corresponds to quasi equilibrium electron distribution in the source section of the channel and the injection of electrons with the kinetic energy exceeding the barrier height D(t) from the source section to the gated section (at x = 0). The injection of electrons from the drain source to the gated section (at x = Lt) is negleted due to eVd kBT; this inequality leads to rather high barrier near the drain edge of the gated section. The presence of the unity step fuction Q(px) in Eqs. (2.16) and (2.17) reflects the fact that there are no electrons propagating backwards due to the absence of the electron scattering in the gated section.
25
26
Device Model for Graphene Bilayer FieldEffect Transistor
Using Eqs. (2.12), (2.14), and (2.15), we arrive at the following formulas for the dc and ac components, J0 and d Jω, of the current at the drain edge of the gated section (i.e., at x = Lt),
J0 = e
p
h
3/2 2
d Jw Ê dD w ˆ = ÁJ0 Ë kBT ˜¯
Here
w (x ) =
2
Ê e  D0 ˆ exp Á F = J0B , Ë kBT ˜¯
2m(kBT )3/2
Ú
•
0
(2.16)
dx xe x w (x ).
(2.17)
Ê ˆ wt ˜ dy exp Á i ÁË x 1  y2 ˜¯ p 0
2
Ú
1
Ê wt ˆ È Ê wt exp Á i ˜ ÍC Á wt Ë x ¯ ÍÎ ÁË 2 x
x 1/ 4
ˆ Ê wt ˜ + iS Á ˜¯ ÁË 2 x
ˆ˘ ˜˙, ˜¯ ˙ ˚
where t = Lt m / 2kBT is the effective ballistic transit time across the gated section of electrons with the thermal velocity uT =
2kBT/m and C(x) and S(x) are Frenel’s cosine and sine functions.
At ωt 1,
w (x )
Ê wt pˆ exp Á i +i ˜. 4¯ wt Ë x
2x 1/4
At ωt 1, Fw(x) tends to unity.
2.3.2 Collisional Electron Transport In the case of strongly collisional electron transport, the distribution function in the gated section is close to isotropic and it can be searched in the form fP = F + g cos q.
(2.18)
Here F = F(e, x, t) is the symmetrical part of the electron distribution function (which is generally not the equilibrium function). The second term in Eq. (2.18) presents the asymmetric part of the distribution
Boltzmann Kinetic Equation and Its Solutions
function with g = g(e, x, t). Similar approach was used for the calculation of characteristics of heterojunction bipolar transistors [32] (see also Refs. [19, 33]). As a result, after the averaging of Eq. (2.11) over the angle q, one can arrive at the following coupled equations:
e ∂g ∂gF 2e ∂F ∂F =, + vg = . ∂t 2m ∂x ∂t m ∂x
(2.19)
Here in the case of w(q) = w = const, which corresponds to the scattering of electrons on shortrange defects, v = mw/2. Equation (2.19) are reduced to the following equation for function F:
ˆ e ∂2F ∂ Ê ∂Fe + vF ˜ = . Á ¯ m ∂x 2 ∂t Ë ∂t
(2.20)
In the most interesting case when eVd kBT, the boundary conditions for Eq. (2.20) at x = 0 and x = Lt can be adopted in the following form: F
x =0
È e  D(t )  e ˘ = exp Í F ˙, F kBT Î ˚
x = Lt
0.
(2.21)
The boundary condition under consideration imply that at x = 0 there is the electron injection from the source section of the channel, whereas at x = Lt an effective extraction of the electrons into the drain section occurs due to a strong pulling dc electric field. Due to a strong electron scattering a significant portion of the injected electrons returns back to the source section. Setting as above dV(t) = dVωe–iωt and, hence, F = F0 + dFωe–iωt and g = F0 + dgω e–iωt, we obtain
d 2F0 dx 2
d 2d Fw dx and arrive at
2

= 0,
mw (w + iv p ) e
(2.22)
d Fw = 0,
È e  D 0  e ˘Ê xˆ F0 = exp Í F ˙Á1  ˜ , Lt ¯ kBT ˚Ë Î
(2.23) (2.24)
27
28
Device Model for Graphene Bilayer FieldEffect Transistor
È e  D 0  e ˘ sinh[a w (x  Lt )] Ê dDw ˆ dFw = exp Í F ˙ Á ˜, kBT Î ˚ sinh(a w Lt ) Ë kBT ¯
(2.25)
where aω = mw (w + iv)/ e . Considering Eqs. (2.19), (2.24), and (2.25), we obtain g0 = 
=
1 2e ∂F0 v m ∂x
È e  D0  e ˘ 2e exp Í F ˙, m kBT Î ˚
1 vLt
d gw = 
2e ∂dFw i (w + iv) m ∂x
(2.26)
È e  D0  e ˘ 2w = i exp Í F ˙ k T (w + iv) B Î ˚ ¥
cosh[a w (x  Lt )] Ê d Dw ˆ . sinh(a w Lt ) ËÁ kBT ¯˜
(2.27)
After that, using Eqs. (2.12), (2.26), and (2.27), we arrive at the following formulas for J0 and dJω (at x = Lt):
J0 = e
Ê e  D0 ˆ exp Á F = J0C , ˜ Ë kBT ¯ p h Lt v
2(kBT )2 2
d Jw Ê dD w ˆ = ÁJ0 Ë kBT ˜¯
Here
Hw (x ) =
Ú
•
0
dx xe x H w (x ).
(2.28)
(2.29)
it v
2w . sinh [2w (w + iv )t / x] w + iv 2
According to Eq. (2.28), J0C µ 1/Ltν. One needs to stress that the collisional case under consideration corresponds actually to νt 1. In the frequency range w ν/t2, Hw(x) j x . at w ν /t2, one obtains È (1 + i ) wt 2v ˘ ˙. Hw (x ) 2(1 + i) wt 2v exp ÍÍ ˙ x Î ˚
GBLFET DC Transconductance
2.4 GBLFET DC Transconductance Equations (2.16) and (2.28) provide the dependences of the sourcedrain dc current J0 as a function of the device structural parameters, temperature, and back and topgate voltages for GBLFETs with ballistic and collisional electron transport, respectively (in the limit eVd kBT). Using Eq. (2.16), one can find the dc transconductance G0 = (∂J0/∂Vt)Vb of a GBLFET with the ballistic electron transport:
G0B = e2
2mkBT
p 3/2 h2
when Vth,2 < Vt < Vth,1, and
G0B = e2
Ê e  D 0 ˆ eJ0B = , exp Á F Ë kBT ¯˜ 2kBT
Ê e  D0 ˆ eJ0B = exp Á F , 0 2kBT 0 Ë kBT ˜¯
2mkBT
p 3/2 h2
when Vt < Vth,2 < Vth,1. Here
Ê a ˆ 0 Á B ˜ . Ë 4W ¯
(2.30)
(2.31) (2.32)
Similarly, using Eq. (2.28), we obtain the following formulas for the GBLFET transconductance in the case of collisional electron transport:
G0C = e2
Ê e F  D0 ˆ eJ0C = exp , ËÁ kBT ¯˜ 2kBT p h2 Lt v kBT
when Vth,2 < Vt < Vth,1, and
G0C = e2
Ê e F  D0 ˆ eJ0C exp = ÁË k T ˜¯ 0 2k T 0 , ph2 Lt v B B kBT
(2.33)
(2.34)
when Vt < Vth,2 < Vth,1. As follows from the comparison of Eq. (2.30) with Eq. (2.31) and Eq. (2.33) with Eq. (2.34), the GBLFET dc transconductance in the top gate voltage range Vth,2 < Vt < Vth,1 (in the range b) might be much larger than that when Vt < Vth,2 < Vth,1 (in the range c) since aB 8W. This is due to relatively slow increase in D0 with increasing Vt  when the hole density in the gated section becomes essential. The voltage dependences of the dc transconductance can be obtained using Eqs. (2.30), (2.31), (2.33), and (2.34) and invoking Eqs. (2.2), (2.4), and (2.6). In particular, in a rather narrow voltage range Vth,2 < Vt < Vth,1, one obtains
29
30
Device Model for Graphene Bilayer FieldEffect Transistor
G0C =
È eV Ê a ˆ ˘ È e(V + V ) ˘
p B G0 µ exp Í b Á B ˜ ˙ exp Í b t ˙
˙ vt � ÍÎ kBT Ë 8 W ¯ ˙˚ Î 2kBT ˚
Èe(Vt  Vt h ,1 ) ˘
(2.35)
= exp Í ˙ .
Î 2kBT ˚
At sufficiently large absolute values of the topgate voltage when Vt < Vth,2 < Vth,1, the transconductance vs voltage dependence is given by
G0C =
È e(V  Vb ) Ê d0 ˆ ˘ p B Ê aB ˆ G0 µ Á
exp Í t ˜ Á
˜˙ Ë 4W ¯
vt � Î kBT Ë 2W ¯ ˚
Èe(Vt  Vth ,2 ) Ê aB ˆ ˘ ¥ exp Í ˙. ËÁ 8W ¯˜ ˚ kBT Î
2.5 GBLFET AC Transconductance
(2.36)
According to the Shockley–Ramo theorem [34, 35], the sourcedrain ac current is equal to the ac current induced in the highly conducting quasineutral portion of the drain section of the channel and in the drain contact by the electrons injected from the gated section. This current is determined by the injected ac current given by Eq. (2.16) or Eq. (2.28), as well as the electron transittime effects in the depleted portion of the drain section. However, if ωtd 1, where the td is the electron transit time in depleted region in question, the induced ac current is very close to the injected ac current [19, 36, 37]. Since, at moderate drain voltages, the length of depleted portion of the drain section Ld can usually be shorter than the top gate length Lt, in the most practical range of the signal frequencies ω t–1, one can assume that td t and, hence, ωtd 1. Considering this and using Eqs. (2.17) and (2.28), the GBLFET ac transconductance Gω = (∂d Jω/∂d Vω)Vb at different electron transport conditions can be presented as
GwB =
J 0B Ê ∂d � Dw Á 
Vw V kBT ÁË ∂d �
GwC =
J 0C Ê ∂d � Dw Á 
kBT ÁË ∂d � Vw V
respectively.
ˆ
˜ ˜ b ¯
•
Ú dx
ˆ
˜ ˜ b ¯
0
•
Ú dx
0
x e x w (x ),
(2.37)
x e x Hw (x ),
(2.38)
GBLFET AC Transconductance
In the range of gate voltages Vth,2 < Vt < Vth,1 (range b), Eq. (2.2) yields ∂dDw ∂dVw
Vd
e = . 2
(2.39)
In this case, Eqs. (2.37) and (2.38) result in
GwB =
eJ0B 2kBT
Ú
•
GwC =
eJ0C 2kBT
Ú
•
dx xe x w (x ),
(2.40)
dx x e x Hw (x ).
(2.41)
0
0
As follows from Eqs. (2.40) and (2.41), the characteristic frequencies of the ac transconductance rolloff are 1/t and ν/t2 in the case of the ballistic and collisional electron transport, respectively, i.e., the inverse times of the ballistic and diffusive transit across the gated section of the channel. Indeed, the quantity ν/t2 can be presented as D/ L2t , where D is the electron diffusion coefficient. The situation becomes more complex in the range of the top gate bias voltages Vt < Vth,2 < Vth,1 (range c). As follows from Eq. (2.4) in this voltage range, the quantity d Dω is determined not only by the ac voltage d Vω but also by the ac component of the hole density in the gated section dSw+ . Moreover, at sufficiently high signal frequencies, the hole system in the gated section can not manage to follow the variation of the ac voltage. Taking into account the dynamic response of the hole system (see Appendix), instead of Eq. (2.39) one can obtain ∂dDw ∂dVw
Vd
e =  w . 2
Here (see Appendix)
1 Ê a ˆ ÏÔÊ a ˆ w = Á B ˜ ÌÁ B ˜ + Ë 4W ¯ ÔÓË 4W ¯ 1  iwt r
Ê 1  iwt r ˆ , = 0 Á Ë 1  iwt r 0 ¯˜
(2.42)
¸Ô ˝ Ô˛
1
(2.43)
where tr is the time of the gated section recharging associated with changing of the hole density due to the tunneling or/and generation
31
32
Device Model for Graphene Bilayer FieldEffect Transistor
recombination processes. Generally, tr depends on the top gate length Lt. Accounting for Eq. (2.42), we arrive at the following formulas for the GBLFET ac transconductance when Vt < Vth,2 < Vth,1:
GwB =
eJ0B Rw 2kBT
Ú
•
GwC =
eJ0C Rw 2kBT
Ú
•
0
0
dx xe x Fw (x ),
(2.44)
dx xe x Hw (x ).
(2.45)
If ω tr–1, one obtains Rω j 1 and the ac transconductances in both b and c ranges of the top gate voltage are close to each other (compare Eqs. (2.40) and (2.41) with Eqs. (2.42) and (2.44)). However, at low signal frequencies (ω tr–1), the ac transconductance given by Eqs. (2.44) or (2.45) for the voltage range c are markedly smaller than those given by Eqs. (2.40) and (2.41) valid in the voltage range b.
2.6 Analysis of the Results and Discussion
Comparing G0B and G0C given by Eqs. (2.30) and (2.35), we obtain
G0C /G0B = p /vt . This implies that the above ratio markedly
decreases with increasing collision frequency (with decreasing electron mobility) and the top gate length, i.e., with the departure from the ballistic transport. As shown above, the dc current steeply drops in a narrow topgate voltage range Vth,2 < Vt < Vth,1. Indeed, the ratio J0B Vt = Vth,2/ J0B Vt = Vth,1 j exp[−(ed0Vb/WkBT)]. Setting W = 5 nm, T = 300 K, and Vb = 1–2 V, we find J0B Vt = Vth,2/ J0B Vt = Vth,1 j 3 ¥ 10–3 – 6 ¥ 10–2. The estimate of the dc current at Vt = Vth,2 j –Vb (which might be interesting for the GBLFET applications in digital large scale circuits) with W = 5 nm, T = 300 K, and Vb = 1 – 2 V yields J0B j 1 ¥ 10–3 – 2 ¥ 10–2 A/cm. At T = 77 K and Vb = 1 V, one obtains J0B j 7 ¥ 10–7 A/cm. In the case of a GBLFET with the width H = 1 mm, the latter corresponds to the characteristic value of the “offcurrent” J0B H j 70 pA. Similar values can be obtained at T = 300 K when –Vt = Vb j 4.6 V. As follows from Eq. (2.35), the GBL dc transconductance in the range of the top gate voltages Vth,2 < Vt < Vth,1 is particularly large
Analysis of the Results and Discussion
when Vt Vth,1. This is due to a sharp voltagesensitivity of the dc current and its relatively high values at such voltages. Indeed, using Eq. (2.28) at T = 300 K and Vt Vth,1, we obtain G0B 2500 mS/mm. In GBLFETs with Wt Wb, the dc transconductance can be even larger. The preexponential factor in the righthand side of Eq. (2.36) is proportional to a small parameter (aB/8W). The argument of the exponential function in this equation comprises small parameters (aB/8W) and (d0/2W). This implies that the dc transconductance in the voltage range Vt < Vth,2 < Vth,1 described by Eq. (2.36) is relatively small and is a faily weak function of the topgate voltage. As follows from Eqs. (2.35) and (2.36), the ratio of the dc transconductance at Vt Vth,2 to that at Vt Vth,1 is equal approximately to the following small value: (aB/4W) exp[ed0(Vth,2 – Vb)/2WkBT] = (aB/4W) exp (–2eEg,Sd0/dkBT); it is smaller then the ratio of the dc currents by parameter (aB/4W). Figure 2.3 shows the ac transconductance Gω normalized by the dc transconductance at the ballistic transport G0B as a function of the normalized signal frequency ωt calculated for GBLFETs with both ballistic and collisional electron transport. It is assumed that the top gate voltage is in the range Vth,2 < Vt < Vth,1. The inset in Fig. 2.3 shows the dependence of the normalized threshold frequency ωtt on νt µ νLt. The threshold frequency is defined as that at which Gω/G0 = l/ 2 . One can see that Gω pronouncedly decreases with increasing collision frequency. However, as seen from the inset in Fig. 2.3, the decrease in ωt with increasing ν is markedly slower: the ratio of ωt at νt = 2 and ωt at νt = 6 (i.e., three times larger) is approximately equal to 1.42. Setting Lt = 100 – 500 nm and T = 300 K, for the threshold frequency ft = ωt/2p at the ballistic transport, we obtain ftB j 0.485 – 0.97 THz. To realize the near ballistic regime of the electron transport (νt 1) in GBLFETs with such gate lengths, the electron mobility m > (1 – 5) ¥ 104 cm2/V s is required. The possibility of the latter mobilities at room temperatures was discussed recently (see, for instance, Ref. [6]). At a shorter top gate, Lt = 75 nm, one obtains ftB j 1.29 THz. In the case of a GBLFET with relatively long top gate and moderate mobility (Lt = 500 nm and m =2 ¥ 104 cm2/V s) when the effect of scattering is strong (ν j 2 ¥ 1012 s–1 and νt j 2.7), we obtain ftC j 94 GHz.
33
Device Model for Graphene Bilayer FieldEffect Transistor
1
1.5
ν = 0
1
B
ωtτ
0.8
Gω/G0
34
0.6
0.5
0.4
0 0
0.2
ντ = 2 ντ = 4
ντ = 6 0 0 2
4
ωτ
2
6
ντ
4
8
6
10
Figure 2.3 The ac transconductance (normalized by G B ) versus ωt calculated 0 for GBLFETs with ballistic (ν = 0) and collisional electron transport (νt = 2, 4, and 6) at the top gate voltage in range b, i.e., Vth,2 < Vt < Vth,1. For Lt = 100 nm and T = 300 K, wt = 10 corresponds to f = w/2p j 3.3 THz. The inset shows the normalized threshold frequency wtt as a function of parameter nt.
In Fig. 2.4, the similar dependences calculated for a GBLFET with collisional electron transport at Vth,2 < Vt < Vth,1 and at Vt < Vth,2 < Vth,1 are demonstrated. Since in the latter topgate voltage range the electron scattering on holes accumulated in the gated section can be strong, so that the realization of the ballistic transport at such topgate voltages might be problematic, only the dependences corresponding to the collisional electron transport are shown. As follows from Eqs. (2.44) and (2.45) and seen from Fig. 2.4, the ac transconductance at the top gate voltages Vt < Vth,2 < Vth,1 is fairly small at low frequencies w tr–1 being close to the dc transconductance (due to a smallness of parameter R j aB/4W), whereas it becomes much larger in the intermediate frequency range tr–1 w t 1 (or tr–1 w νt 2). This is due to the effect of holes in the gated section. Owing to this effect, the low frequency noises can be effectively suppressed. Using the above results for GBLFETs and those obtained previously [19] for GNRFETs, one can compare the GBL and GNR characteristics. In particular, considering the expressions for J0B found for GBLFETs and GNRFETs, we obtain J0B/J0B,GNR = 1/2. For the case of collisional transport, one obtains J0C/J0C,GNR ~ 1. As a result, the GBLFET and GNRFET dc transconductances are close to each other. The ratio of the GBLFET and GNRFET ac transconductances
Conclusions
at high signal frequencies is GωB/GωB,GNR µ 1/ wt , i.e., the GBLFET ac transconductance falls more steeply with increasing ω than the GNRFET ac transconductance. 1
Gω/G0
B
0.8 0.6
Vth,2 < Vt < Vth,1
ντ = 2 τr /τ = 50
0.4 Vt < Vth,2
0.2 0 2 10
10
1
0
ωτ
10
1
10
Figure 2.4 The ac transconductance (normalized by G B ) versus wt calculated 0 for GBLFETs with collisional electron transport (vt = 2) at the top voltage in range c ( Vt < Vth,2 < Vth,1 at tr/t = 50.
The GBLFET dc and ac characteristics obtained are valid if the interband tunneling sourcedrain current through the n+ – p and p – n+ junctions beneath the edges of the top gate are small in comparison with the thermionic current created by the electrons overcoming the potential barrier in the gated section. Such a tunneling current can be essential in the voltage range c (Vt < Vth,2 < Vth,1) depending on the energy gap near the top gates and the length of the n+ – p and p – n+ junctions in question. This implies that there is a limitation when the topgate voltage is not too high Vt in comparison with the threshold voltage Vth,2 (i.e., when Vt Vth,2), so that the calculated characteristics correspond to the most interesting voltage range where the ac transconductance can be rather large.
2.7 Conclusions
We have presented an analytical device model for a GBLFET. Using this model, we have calculated the GBLFET dc and ac characteristics and shown that:
35
36
Device Model for Graphene Bilayer FieldEffect Transistor
(1) The dependence of the dc current on the top gate voltage is characterized by the existence of three voltage ranges, corresponding to (a) the population of the gated section by electrons, (b) the depletion of this section, and (c) its essential filling with holes, and determined by the topgate threshold voltages Vth,1 and Vth,2. (2) The ac current is most sensitive to the topgate voltage Vt and the dc and ac transconductances are large when Vth,2 < Vt Vth,1. (3) The electron scattering in the gated section results in a marked reduction in the dc and ac transconductances. However, the threshold frequency corresponding to Gω/G0 = 1/ 2 decreases with increasing collision frequency relatively smoothly. (4) The transient recharging of the gated section by holes (at Vt < Vth,2) leads to a nonmonotonic frequency dependence of the ac transconductance with a pronounced maxima in the range of fairly high frequencies. This effect might be used for the optimization of GBLFETs with reduced sensitivity to low frequency noises. (5) The fabrication of GBLs with high electron mobility at elevated temperatures opens up the prospects of realization of terahertz GBLFETs with ballistic electron transport operating at room temperatures and surpassing FETs based on A3B5 compounds.
Acknowledgments
The authors are grateful to Professor S. Brazovskii (University ParisSud) and Professor E. Sano (Hokkaido University) for fruitful discussions and valuable information. The work was supported by the Japan Science and Technology Agency, CREST, Japan. One of the authors (N.K.) acknowledges the support by the INTAS grant 7972, and by the ANR program in France (the project BLAN073192276).
Appendix
Appendix: Dynamic Response of the Hole System in the Gated Section At sufficiently large values Vt, the gated section is essentially populated with the holes. As follows from Eq. (2.4),
1 2pe2W + dDw =  edVw dS w . 2 k
(2.A1)
The ac component of the hole density dSw+ obeys the continuity equation, which can be presented in the following form:
iwdSw+ = dGw +
d JwT
 d JwT
x =0
x = Lt
eLt
.
(2.A2)
Here dGw is the variation of the generation of holes in the gated section (associated, say, with the generation of holes by the
thermal radiation [38]) and d JwT
x =0
and d JwT
x = Lt
are the interband
tunneling ac currents near the source and drain edges of the top gate, respectively. For normal operation of GBLFETs, these tunneling current should relatively small. This is achieved in GNLFETs by proper choice of the energy gap in the different sections of the channel (Eg,s, Eg, and Eg,d, which should be not too small. The terms in the righthand side of Eq. (2.A2) can be presented as
dGw = K g (dDw  de F+ ),
d JwT
x =0
 d JwT
x = Lt
=
2(dDw  de F+ ) . eRt
(2.A3) (2.A4)
Here de F+ j (ph2/2m) dSw+ , Kg = 2m/ph2tg, where tg is the characteristic time of the generationrecombination processes in the gated section, Rt is the tunneling resistance of the pn junctions induced by the negative top gate voltage near the edges of the top gate: lnRt µ Eg3/2/e µ (Vb – Vt)3/2/Vt. From Eqs. (2.A1)–(2.A4), taking into account the limit ω Æ 0 (see Eqs. (2.5) and (2.30)), we find
e dDw =  dVw 2
37
38
Device Model for Graphene Bilayer FieldEffect Transistor
Ï ¸ 1 Ê aB ˆ 1 +Á Ô Ô ˜ Ë ¯ tg 4W t RC Ô Ê aB ˆ ÔÊ aB ˆ ¥Á + Ì ˝ Ë 4W ˜¯ ÔÁË 4W ˜¯ 1 Ê aB ˆ 1 Ô iw +Á ˜t Ô Ô Ë ¯ t 4 W g RC Ó ˛
e 1 Ê a ˆ ÏÔÊ a ˆ =  dVw Á B ˜ ÌÁ B ˜ + Ë 4W ¯ ÔÓË 4W ¯ 1  iwt r 2
1
1
Ô¸ ˝ , Ô˛
(2.A5)
where trc = RtCt is the time of the gated section recharging by the tunneling currents, Rt is the tunneling resistance of the pn junctions induced by the negative top gate voltage near the edges of the top gate, the quantity tr = trctg/[trc + (aB/4W)tg] is the characteristic time of the gated section recharging by holes, and Ct = κLt/2pW is the capacitance of the gated section. At ω Æ 0, Eq. (2.A5) leads to
1 dDw  edVw 0 , 2
where
0
∂dDw ∂dVw
Vd
e  0 , 2
(2.A6)
(aB / 4W ) (aB / 4W ), 1 + (aB / 4W )
i.e., coincides with the value given by Eq. (2.28). When w tr–1, Eq. (2.A5) yields
∂dDw 1 dDw  edVw , ∂dVw 2
Vd
e  . 2
(2.A7)
References 1. C. Berger, Z. Song, T. Li, X. Li, A.Y. Ogbazhi, R. Feng, Z. Dai, A. N. Marchenkov, E. H. Conrad, P. N. First, and W. A. de Heer, J. Phys. Chem., 108, 19912 (2004).
2. K. S. Novoselov, A. K. Geim, S. V. Morozov, D. Jiang, M. I. Katsnelson, I. V. Grigorieva, S. V. Dubonos, and A. A. Firsov, Nature, 438, 197 (2005).
3. B. Obradovic, R. Kotlyar, F. Heinz, P. Matagne, T. Rakshit, M. D. Giles, M. A. Stettler, and D. E. Nikonov, Appl. Phys. Lett., 88, 142102 (2006).
4. J. Hass, R. Feng, T. Li, X. Li, Z. Zong, W. A. de Heer, P. N. First, E. H. Conrad, C. A. Jeffrey, and C. Berger, Appl. Phys. Lett., 89, 143106 (2006).
References
5. A. K. Geim and K. S. Novoselov, Nat. Mater., 6, 183 (2007).
6. S. V.Morozov, K. S. Novoselov, M. I. Katsnelson, F. Schedin, D. C. Elias, J. A. Jaszczak, and A. K. Geim, Phys. Rev. Lett., 100, 016602 (2008) 7. V. V. Cheianov and V. I. Fal’ko, Phys. Rev. B, 74, 041403 (2006).
8. B. Huard, J. A. Sulpizio, N. Stander, K. Todd, B. Yang, and D. GoldhaberGordon, Phys. Rev. Lett., 98, 236803 (2007).
9. M. C. Lemme, T. J. Echtermeyer, M. Baus, and H. Kurz, IEEE Electron Device Lett., 28, 282 (2007).
10. V. Ryzhii, M. Ryzhii, and T. Otsuji, Appl. Phys. Express, 1, 013001 (2008),
11. V. Ryzhii, M. Ryzhii, and T. Otsuji, Phys. Stat. Sol. A, 205, 1527 (2008).
12. Z. Chen, Y.M. Lin, M. J. Rooks, and P. Avouris, Physica E, 40, 228 (2007). 13. K. Wakabayshi, Y. Takane, and M. Sigrist, Phys. Rev. Lett., 99, 036601 (2007).
14. Y. Quyang, Y. Yoon, J. K. Fodor, J. Guo, Appl. Phys. Lett., 89, 203107 (2006). 15. G. Liang, N. Neophytou, D. E. Nikonov, and M. S. Lundstrom, IEEE Tran. Electron Devices, 54, 677 (2007). 16. G. Fiori and G. Iannaccone, IEEE Electron Device Lett., 28, 760 (2007).
17. V. Ryzhii, M. Ryzhii, A. Satou, and T. Otsuji, J. Appl. Phys., 103, 094510 (2008). 18. V. Ryzhii, V. Mitin, M. Ryzhii, N. Ryabova, and T. Otsuji, Appl. Phys. Express, 1, 063002 (2008).
19. M. Ryzhii, A. Satou, V. Ryzhii, and T. Otsuji, J. Appl. Phys., 104, 114505 (2008).
20. T. Ohta, A. Bostwick, T. Seyel, K. Horn, E. Rotenberg, Science, 313, 951 (2006). 21. E. McCann, Phys. Rev. B, 74, 161403 (2006).
22. E. V. Castro, K. S. Novoselov, S. V. Morozov, N. M. R. Peres, J. M. L. dos Santos, J. Nilsson, F. Guinea, A. K. Geim, and A. H. Castro Neto, Phys. Rev. Lett., 99, 216802 (2007)
23. L. A. Falkovski, Phys. Rev. B, 75, 033409 (2007).
24. F. T. Vasko and V. Ryzhii, Phys. Rev. B, 76, 233404 (2007). 25. V. Vyurkov and V. Ryzhii, JETP Lett., 88, 322 (2008).
26. M. G. Ancona, 2008 International Conference on Semiconductor Processes and Devices (SISPAD 2008), Sept. 9–11, 2008, Hakone, Japan, p. 169.
39
40
Device Model for Graphene Bilayer FieldEffect Transistor
27. V. Vyurkov, I. Seminikhin, M.Ryzhii, T. Otsuji, and V. Ryzhii, Techn. Digest, International Symposium on Graphene Devices: Technology, Physics, and Modeling (ISGD2008), Nov. 17–19, 2008, AizuWakamatsu, Japan, p. 32. 28. M. Shur, Physics of Semiconductor Devices (Prentice Hall, New Jersey, 1990).
29. S. M. Sze, Physics of Semiconductor Devices (Wiley, New York, 1981).
30. E. P. Gusev, C. Carbal Jr., M. Copel, C. D’Emic, and M. Gribelenuk, Microelectron. Eng., 63, 145 (2003).
31. Y. Xuan, Y. Q. Wu, T. Shen, M. Qi, M. A. Capano, J. A. Cooper, and P. D. Ye, App. Phys. Lett., 92, 013101 (2008). 32. V. I. Ryzhii, A. A. Zakharova, and S. N. Panasov, Sov. Phys. Semicond., 19, 298 (1985). 33. E. Gnani, A. Gnudi, S. Reggiani, and G. Baccarani, IEEE Trans. Electron Devices, 55, 2918 (2008) 34. W. Shockley, J. Appl. Phys., 9, 635 (1938) 35. S. Ramo, Proc. IRE, 27, 584 (1939).
36. V. Ryzhii and G. Khrenov, IEEE Trans. Electron Devices, 42, 166 (1995).
37. V. Ryzhii, A. Satou, M. Ryzhii, T. Otsuji, and M. S. Shur, J. Phys.: Condens. Matter, 20, 384207 (2008). 38. F. T. Vasko and V. Ryzhii, Phys. Rev. B, 77, 195433 (2008).
Chapter 3
ElectricallyInduced nip Junctions in Multiple Graphene Layer Structures*
M. Ryzhii,a V. Ryzhii,a T. Otsuji,b V. Mitin,c and M. S. Shurd aComputational
Nanoelectronics Laboratory, University of Aizu,
AizuWakamatsu 9658580 and Japan Science and Technology Agency,
CREST, Tokyo 1070075, Japan
bResearch Institute of Electrical Communication, Tohoku University,
Sendai 9808577 and Japan Science and Technology Agency, CREST,
Tokyo 1070075, Japan
cDepartment of Electrical Engineering, University at Buffalo,
State University of New York, NY 14260, USA
dDepartment of Electrical, Computer, and Systems Engineering,
Rensselaer Polytechnic Institute, Troy, New York 12180, USA
[email protected]
The Fermi energies of electrons and holes and their densities in different graphene layers (GLs) in the n and p regions of the electrically induced nip junctions formed in multipleGL structures *Reprinted with permission from M. Ryzhii, V. Ryzhii, T. Otsuji, V. Mitin, and M. S. Shur (2010). Electricallyinduced nip junctions in multiple graphene layer structures, Phys. Rev. B, 82, 075419. Copyright © 2010 The American Physical Society. GrapheneBased Terahertz Electronics and Plasmonics: Detector and Emitter Concepts Edited by Vladimir Mitin, Taiichi Otsuji, and Victor Ryzhii
Copyright © 2021 Jenny Stanford Publishing Pte. Ltd.
ISBN 9789814800754 (Hardcover), 9780429328398 (eBook)
www.jennystanford.com
42
ElectricallyInduced nip Junctions in Multiple Graphene Layer Structures
are calculated both numerically and using a simplified analytical model. The reverse current associated with the injection of minority carriers through the n and p regions in the electricallyinduced nip junctions under the reverse bias is calculated as well. It is shown that in the electricallyinduced nip junctions with moderate numbers of GLs the reverse current can be substantially suppressed. Hence, multipleGL structures with such nip junctions can be used in different electron and optoelectron devices.
3.1 Introduction
The possibility to form electricallyinduced np and nip junctions [1–3] in gated graphene layers (GLs), as well as lateral arrays of graphene nanoribbons and graphene bilayer, opens up prospects of creation novel electronic and optoelectronic devices [4–8]. In contrast to GL structures with chemically doped n and pregion in the GL structures with electricallyinduced np and nip junctions, there is a possibility of their voltage control. Recent success in fabricating highquality multiple GLs Refs. [9–11] (see also the recent review article [12] and references therein) stimulates an interest in different prospective devices using multipleGL structures. These structures constitute the stacks of disoriented GLs (with the nonBernal stacking). Each GL exhibits linear dispersion relation for electrons and holes similar to that in a single GL. This is a wellestablished experimental fact (see, for instance, Refs. [11–14]. Using the multipleGL structures instead of singleGL structures can provide a significant improvement in device performance of terahertz tunneling transittime oscillators (similar to that considered in Ref. [4]), lasers with optical and electrical pumping, and high performance interband photodetectors [15–17]. Gated multipleGL structures can be also used in highfrequency fieldeffect transistors [18] and other devices (such as terahertz frequency multipliers, and plasmonic devices). However the penetration of the electric field (transverse to the GL plane) beyond the topmost GL as well as its sceening by electron or hole charges in GLs can substantially limit the influence of the gates (the effect of the quantum capacitance [19]). In this chapter, we study the influence of screening in gated multipleGL structures on the formation and characteristics of n or p regions and nip junctions in these structures. We calculate the
Equations of the Model
electron and hole Fermi energies and densities in GLs in the n and p regions as functions of the GL index, gate voltage, and temperature. Using these data, we find the voltage and temperature dependences of the reverse current in the nip junctions with different structural parameters. The multipleGL structures are often obtained by thermal decomposition from 4HSiC substrate (see, for instance, Refs. [9] and [10]) on the Cterminated surface. The majority of the top GLs is practically neutral, whereas a buffer bottom GL (BGL) or a few BGLs in the very close vicinity of the interface with SiC is highly conducting (doped) as a result of the charge transfer from SiC [9]. For the device applications akin those considered in Refs. [15–17], such a highly conducting BGL plays a negative role. Due to this, we focus on the multipleGL structures in which the BGL (or BGLs) and, hence, the effect of SiC substrate are eliminated. The multipleGL structures without the BGL (BGLs) can be fabricated using chemical/ mechanical reactions and transferred substrate techniques, which include chemically etching the substrate and the highly conducting GL (or GLs) and transferring the upper portion of the multipleGL structure on a Si or equivalent substrate. The mechanical peeling of the upper portion of GL with the subsequent placement on a substrate is another option. Possible modifications of the effects under consideration in the multipleGL structures with the highly conducting BGL are briefly discussed below. The structures with few nonBernal stacked GLs are also fabricated on 3CSiC(110) on Si(110) substrate [20].
3.2 Equations of the Model
Let us consider a multipleGL structure with the side Ohmic contacts to all GLs and two split gates (isolated from GLs) on the top of this structure as shown in Fig. 3.1a. Applying the positive (Vn = Vg > 0) or negative (Vp = –Vg < 0) voltage between the gate and the adjacent contact (gate voltage), one can obtain the electricallyinduced n or p region. In the single and multipleGL structures with two split top gates under the voltages of different polarity, one can create lateral np or nip junctions. Generally, the sourcedrain voltage V can be applied between the side Ohmic contacts to GLs. Depending on the polarity of this voltage, the np and nip junctions can be either direct or reverse biased. We assume that the potentials of the first
43
44
ElectricallyInduced nip Junctions in Multiple Graphene Layer Structures
(source) contact and the pertinent gate are js = 0 and jg = Vg > 0, respectively, and the potentials of another gate and contact (drain) are jg = –Vg < 0 and jd = V = 0 (or jd = V π 0. If the slot between the gates 2Lg is sufficiently wide (markedly exceeds the thickness of the gate layer Wg separating the gates and the topmost GL), there are intrinsic i regions in each GL under the slot. Thus the nip junction is formed. The pertinent band diagrams are shown in Figs. 3.1b and 3.1c. Since the side contacts are the Ohmic contacts, the electron Fermi energy in the kth GL sufficiently far from the contacts are given by mk = ±ejk. Here e is the electron charge and jk = jz = kd is the potential of the kth GL, k = 1, 2, ..., K, where K is the number of GLs in the structure, d is the spacing between GLs, and the axis z is directed perpendicular to the GL plane with z = 0 corresponding to the topmost GL and z = zK = Kd to the lowest one.
Figure 3.1 Schematic view of (a) a multipleGL structure and its band diagrams at (b) zero bias voltage (V = 0) and (c) at reverse bias (for GL with k = 1). Arrows indicate the directions of propagation of injected electrons and holes as well as those thermogenerated and generated due to interband tunneling.
Equations of the Model
Focusing on the n region (the p region can be considered in a similar way) and introducing the dimensionless potential y = 2j/Vg, one can arrive at the following onedimensional Poisson equation governing the potential distribution in the z direction (in the n region): d 2y dz 2
=
8pe æVg
Â(S K
k
)
 S k+ ◊ d ( z  kd + d ).
k =1
(3.1)
Here æ is the dielectric constant, d(z) and S k and S k+ are the equilibrium sheet densities in the kth GL of electrons and holes, respectively. These densities, taking into account the linear dispersion low for electrons and holes in graphene, are expressed via the electron Fermi energy as S k�
2Êk Tˆ = Á B ˜ p Ë �vF ¯
=
12S T p2
Ú
2
•
0
Ú
•
0
dxx 1 + exp(x � mk /kBT )
dxx , 1 + exp(x � mk /kBT )
(3.2)
where ST = (p/6)(kBT/hvF)2 is the electron anwd hole density in the intrinsic graphene at the temperature T, vF j 108 cm/s is the characteristic velocity of electrons and holes in graphene, and h and kB are the Planck and Boltzmann constants, respectively. Here it is assumed that the electron (hole) energy spectrum is e = vFp, where p is the absolute value of the electron momentum. The boundary conditions are assumed to be as follows: y z=0 = 2 + Wg
dy dz
,
z =0
dy dz
= 0.
z= zK +0
Equations (3.1)–(3.3) yield
2 y 1 = GF(y 1 )
for K = 1,
d d (2 y 1 ) y 1 +y 2 = GF(y 1 ), Wg Wg y 1 y 2 = GF(y 2 )
for K = 2, and
d d (2 y 1 )y 1 +y 2 = GF(y 1 ), Wg Wg
(3.3) (3.4)
(3.5)
45
46
ElectricallyInduced nip Junctions in Multiple Graphene Layer Structures
y k1  2y k +y k+1 =
d GF(y k ), (2 £ k £ K  1), Wg
y K1 y K = for K > 2. Here
F(y ) =
12 È Í p 2 ÎÍ

Ú
•
0
Ú
•
0
d GF(y K ) Wg
(3.6)
dxx 1 + exp(x U gy )
˘ dxx ˙, 1 + exp(x + U gy ) ˙˚
where G = (8p/æ)(eWgST/Vg) µ T2/Vg and Ug = eVg/2kBT.
(3.7)
3.3 Numerical Results
Equations (3.4)–(3.7) were solved numerically. The results of the calculations are shown in Figs. 3.2–3.5. In these calculations, we assumed that æ = 4, d = 0.35 nm, and Wg = 10 nm. Figure 3.2 shows the dependences of the electron Fermi energy mk =
eVg 2
yk
(3.8)
as a function of the GL index k calculated for multipleGL structures with different number of GLs K at different gate voltages and temperatures. One can see that the Fermi energy steeply decreases with increasing GL index. However, in GLs with not too large k, the Fermi energy is larger or about of the thermal energy. As one might expect, the electron Fermi energies in all GLs at T = 77 K are somewhat larger than at T = 300 K (see also Fig. 3.5). The obtained values of the electron Fermi energies in topmost GLs are m1 ⋍ 92 meV and m1 ⋍ 77 meV for Vg = 1000 mV at T = 77 K and T = 300 K, respectively. Figure 3.3 shows the voltage dependences of the electron Fermi energies in some GLs in multipleGL structure with K = 2, K = 10, and K = 50 at T = 300 K.
Numerical Results
Fermi energy, µk (meV)
80 T =300 K
60
Vg=1000 mV (K=10) 1000 mV (K=50) 500 mV (K=10) 500 mV (K=50)
40 20 0
0
2
4
6
Fermi energy, µk (meV)
100
8 10 12 14 16 18 20 GL index, k T =77 K
80
Vg=1000 mV (K=10)
60
1000 mV (K=50) 500 mV (K=10) 500 mV (K=50)
40 20 0
0
2
4
6
8 10 12 14 16 18 20 GL index, k
Figure 3.2 The electron Fermi energy mk as a function of the GL index k calculated for multipleGL structures with different number of GLs K for different gate voltages Vg at T = 300 K (upper panel) and T = 77 K (lower panel).
Figure 3.4 shows the electron densities S k in the structures with different number of GLs K at different temperatures. One can see that the calculated electron densities in GLs with sufficiently large indices (k > 15 at T = 77 K and T = 300 K) approach to their values in the intrinsic graphene (ST = 0.59 ¥ 1010 cm–2 and 8.97 ¥ 1010 cm–2). The electron densities in GLs in the structures with different K are rather close to each other, particularly, in GLs with small and moderate indices.
47
ElectricallyInduced nip Junctions in Multiple Graphene Layer Structures
k=1 (K=2) k=1 (K=50) k=10 (K=50) k=1 (K=10) k=10 (K=10)
Fermi energy, µk (meV)
100 80 60 40
T =300 K
20 0
0
200 400 800 600 Gate voltage, Vg (mV)
1000
Figure 3.3 Voltage dependences of electron Fermi energies in some GLs in multipleGL structure with different K at T = 300 K.
11
7×10 2
Electron density, Σk (cm )
48
11
Vg =1000 mV
6×10
11
5×10
T=300 K (K=10) 300 K (K=50) 77 K (K=10) 77 K (K=50)
11
4×10
11
3×10
11
2×10
11
1×10
0
0
2
4
6
8 10 12 14 16 18 20 GL index, k
Figure 3.4 Electron density vs GL index in multiple GLstructures with different number of GLs (K = 10 and K = 50) at different temperatures and Vg = 1000 mV.
Figure 3.5 presents the Fermi energies in GLs with different indices at different temperatures. One can see from Fig. 3.5 (as well as from Fig. 3.2) that the higher T corresponds to lower mk. This is due to an increasing dependence of the density of states on the energy and the thermal spread in the electron energies.
Analytical Model
Fermi energy, µk (meV)
120 T=10 K 77 K 300 K Analytical
100 80 60 40 K = 10 Vg = 1000 mV
20 0
0
2
4 6 GL index, k
8
10
Figure 3.5 Comparison of the mk vs k dependences calculated for different temperatures using numerical and simplified analytical (solid line) models.
3.4 Analytical Model At not too low gate voltages when Ug ≫ 1, one can assume that in a number of GLs the electrons under the gate are degenerate, i.e., mk ≫ kBT, and the contribution of holes (nondegenerate) can be disregarded, hence, from Eq. (3.7) we obtain F(y )
6
p2
U g2y 2 .
In this case, for a singleGL structure (K =1), Eq. (3.4) yields 2 y 1
6
(3.9)
U g2y 12 .
(3.10) p Solving Eq. (3.10) and considering Eq. (3.8), for the electron Fermi energy in a GL (in a singleGL structure), we obtain 2
m1 mg 1 
where mg = hvF
mg
eVg
,
(3.11)
æVg / 4eWg . For the same parameters as those
used in Figs. 3.2–3.4, m1 ⋍ 150 meV. Such a value is markedly larger
49
50
ElectricallyInduced nip Junctions in Multiple Graphene Layer Structures
than those calculated for the topmost GLs in multipleGL structures (although it is somewhat exaggerated because the temperature spread in the electron energies is disregarded). This can be attributed to the fact that in multipleGL structures the electron density is shared between the topmost GL and underlying GLs resulting in lower Fermi energies in all of them. Considering multipleGL structure with large K, one can neglect the discreteness of the structure and replace the summation in Eq. (3.1) by the integration. As a result, following Ref. [17], one can arrive at d 2y = 0 (Wg < z < 0, z > zK ), dz 2 G d 2y F(y ) (0 < z < zK ). = dz 2 dWg
In this case, considering Eq. (3.7), we arrive at d 2y y 2 = 2 dz 2 Ls
with the characteristic screening length Ls =
p dWg 6GU g
æd µ Vg1/2 . 2e3Vg
= hvF
(3.12)
(3.13) (3.14)
(3.15)
The boundary conditions for Eq. (3.14) are given by Eq. (3.3) In multipleGL structures with a large number of GLs (K ≫ 1), one can extend the coordinate of the lowest GL to infinity and set dy/ dzz = • = 0 with y• = 0. Solving Eq. (3.14) with the latter boundary conditions, we arrive at y=
1
,
(3.16)
C 3  C/2 = (Wg / 6Ls ).
(3.17)
(C + z / 6 Ls )2
where C satisfies the following equation: Since in reality Wg ≫
6Ls , one obtains C (Wg / 6 Ls )1/3 µ Vg1/6 .
Taking into account Eq. (3.8), Eq. (3.16) yields mk
eVg
2[C + (k  1)d/ 6Ls ]2
= m1ak .
(3.18)
The Reverse Current
Here
Ê Vg ˆ m1 = 2 µ Á ˜ 2C Ë Wg ¯ eVg
2/3
(3.19)
is the Fermi energy of electrons in the topmost GL in the n section (holes in the p section),
and
ak = [1 + (k – 1)g]–2,
g =
d 6LsC
µ
d Wg1/3L2s/3
Ê Vg ˆ µÁ ˜ Ë Wg ¯
(3.20)
1/3
.
(3.21)
Setting d = 0.35 nm, Wg = 10 nm, æ = 4, and Vg = 1 V, one can obtain Ls ⋍ 0.44 nm. C ⋍ 2.14, m1 ⋍ 109 meV, and g ⋍ 0.153. The mk versus k dependence obtained using our simplified analytical model, i.e., given by Eqs. (3.15) and (3.17) is shown by a solid line in Fig. 3.5. Equations (3.9)–(3.21) are valid when mK > kBT, i.e., at sufficiently large Vg or/and sufficiently small T. Since the Fermi energy (at fixed electron density) decreases with increasing temperature, the above formulas of our simplified (idealistic) model yield somewhat exaggerated values of this energy [compare the dependences in Fig. 3.5 obtained numerically using Eqs. (3.4)–(3.7) and that found analytically using Eqs. (3.18)–(3.21)].
3.5 The Reverse Current
The current across the nip junctions under their reverse bias (V < 0, see Fig. 3.2c) is an important characteristic of such junctions [21]. In particular, this current can substantially affect the performance of the terahertz tunneling transittime oscillators and interband photodetectors [5, 17]. This current is associated with the thermogeneration and tunneling generation of the electronhole pairs in the i region. A significant contribution to this current can be provided by the injection of minority carriers (holes in the n region and electrons in the p region). Such an injection current in the kth GL is determined by the height of the barrier for the minority carrier which, in turn, is determined by the Fermi energy mk of the majority
51
52
ElectricallyInduced nip Junctions in Multiple Graphene Layer Structures
carrier. The latter, as shown above, depends on the gate voltage and the GL index. As a result, the reverse current can be presented as J = Ji + Jth + Jtunn,
(3.22)
where the injection current (which is assumed to be of the thermionic origin) is given by Ji =
2evF Ê kBT ˆ p 2 ÁË hvF ˜¯ K
¥
ÂÚ
0
k=1
=
•
=
3
12 J T S T p
2
Ú
p /2
p /2
dq cosq
dxx 1 + exp(x + mk / kBT )
24evF S T p
2
K
ÂÚ
•
k =1
0
K
•
ÂÚ k =1
0
dxx , 1 + exp(x + mk /kBT ) dxx 1 + exp(x + mk /kBT )
(3.23)
with JT = 2evF ST/p. At T = 77 – 300 K, JT ⋍ 0.06 – 0.9 A/cm. Deriving Eq. (3.24), we have taken into account that the distribution function of holes which enter the n region overcoming the barrier in the kth GL with the height mk is fkpn ⋍ {1 + exp[(mk + vFp)/kBT]}–1. Similar formula is valid for electrons in the p region. The factor 2 appears in Eq. (3.24) due to the contribution of both holes and electrons. Equation (3.24) is valid when the bias voltage is not too small: eV > kBT. At V Æ 0 one has Ji Æ 0 (as well as Jth and Jtunn). Scattering of holes in the n region and electrons in the p region resulting in returning of portions of them back to the contacts leads to some decrease in Ji. The temperature dependences of the reverse current associated with the injection from the n and p region calculated using Eq. (3.23) (with the quantities mk shown in Fig. 3.5) are presented in Fig. 3.6. As one might expect, the reverse current sharply increases with the temperature and the number of GL. The latter is due to relatively low energy barriers for minority carriers in the n and p regions in GLs with large indices. For comparison, the injection current in a singleGL structure calculated using Eq. (3.23) with Eq. (3.8), is given by
The Reverse Current
J iS =
�
12 J T p
2
12 JT p2
Ú
•
0
dxx 1 + exp(x + m1/kBT )
Ê �vF æVg /8eWg exp Á k BT ÁË
ˆ ˜. ˜¯
(3.24)
At the same parameters as above and T = 300 K, Eq. (3.24) yields JiS ⋍ 0.01 A/cm. 1
Reverse current, Ji (A/cm)
10
0
10
Vg =1000 mV
1
10
2
10
3
10
K=10 5 2
4
10
5
10 50
100
200 150 250 Temperature, T (K)
300
Figure 3.6 Temperature dependence of reverse current (injection component, Ji) for multipleGL structures with different number of GLs.
When K g 1 m1 / kBT , the main contributions to the reverse current is associated with GLs with large indices (in which the barriers are very low), so that one obtains J i KJ T .
(3.25)
As follows from Eq. (3.25), the injection current (and, therefore, the net reverse current) can be fairly large due to the “shortcut” by GLs with large indices (placed deep below the gate). Since the thermogeneration is associated primarily with the absorption of optical phonons [21], the pertinent rate gth is independent of the electric field in the i region, but it is proportional to the i section length 2l (l ≲ Lg). The contribution of the thermogeneration to the reverse current can be presented as Jth = 4Kelgth.
(3.26)
53
54
ElectricallyInduced nip Junctions in Multiple Graphene Layer Structures
The quantity gth as a function of the temperature was calculated in Ref. [20]. Equations (3.23)–(3.26) are valid if 2l < lR, where lR is the recombination length. In the situations when the bias voltage between the side contacts is not too small (as it should be, for instance, in GLbased interband photodetectors), the recombination length is fairly long. Indeed, assuming that the recombination time (at T = 300 K) and the drift velocity are tr = 5 ¥ 10–10 s [22] and < v > ~ vF/2 = 5 ¥ 107 cm/s [18], respectively, one obtains lR ⋍ 250 mm. Assuming that 2l = 10 mm with gth = 1013 cm–2s–1 and gth = 1021 –2 cm s–1 at T = 77 K and T = 300 K, respectively [22], we obtain Jth ⋍ 3.2 ¥ (10–9–10–1) A/cm. One can see that the thermogeneration contribution to the reverse current is much smaller than the injection contribution at lower temperatures, while it can be substantial at T = 300 K in the nip structures with long i region. The tunneling generation can significantly contribute to the reverse current at elevated electric fields in the i region, i.e., in relatively short GL structures at elevated bias voltages [1, 5]. This current can be calculated using the following formula which follows from the expression for the tunneling probability in GLs [1, 2] (see, for instance [5]): J tunn =
evF Ê ev ˆ p 2l 2 ÁË 2lhvF ¯˜
3/2
µ
V 3/2 . l1/2
(3.27)
Depending on the nip junction applications, the quantities V and l should be chosen to provide either domination of tunneling current (as in tunneling transittime oscillators [4]) or its suppression (as in the interband photodetectors [17]).
3.6 MultipleGL Structures with Highly Conductive BGL
As it was mentioned in the introduction, the multipleGL structures obtained by the thermal decomposition from 4HSiC substrate, include a highly conductive BGL. Its presence can strongly affect the potential and electron density distributions across the multipleGL structure. However, the BGL influence depends on the connection between the BGL and the side contacts. The following options can be considered: (a) all the GLs are directly connected with the side contacts.
Conclusions
If the bias voltage between the side contacts V = 0, the potentials of GLs with different indices 1≤ k ≤ K (the BGL index is equal to K+1) can be found using the same equations as above, i.e., Eqs. (3.4)–(3.7) or Eq. (3.14) but with modified boundary conditions. Considering high conductivity of BGL, its potential can be assumed to be constant and equal to the side contact potential, the second condition in Eq. (3.6) should be replaced by yz=zK+1 = 0. In the case of multipleGL structures with sufficiently large K, both dy/dz and y steeply tend to zero with increasing z. This directly follows from Fig. 3.2 (see the curves calculated for K = 50), as well as from Eqs. (3.16)–(3.21). Thus, the difference between the potential distributions calculated using the boundary conditions dy/dzz=zK = 0 and yz=zK+1 = 0 is fairly small. Hence, the results obtained above are also applicable for the multipleGL structures with the highly conductive BGL if K 1. Since the highly conductive BGL effectively shorts out the side contacts, for the devices whose operation requires V ≠ 0 the GBL should be cut between the side contacts. (b) All the GLs, except the BGL, are connected with the side contacts and a bias voltage Vb is applied between the GBL and one of the side contacts. In this case, the GBL can be considered as the back gate so that the potential distribution is determined by both Vg and Vb. However, in the absence of the top gates, the obtained results can still be used if Wg and Vg in all equations substituted with d and Vb, respectively. (c) All the GLs, except the BGL, are connected with the side contacts, but the GBL is isolated from the side contacts. In such a case, the GBL plays the role of a floating gate. This case needs a separate analysis and will be considered elsewhere.
3.7 Conclusions
We calculated the Fermi energies and electron and hole densities in the electrically induced nip junctions formed in multipleGL structures as functions of the GL indices, gate voltage, temperature, and structural parameters. Using the obtained values of the Fermi energies and the heights of potential barriers for minority carriers in the n and p regions, we found the temperature dependences of the reverse injection current for multipleGL structures with different numbers of GLs. This analysis shows the possibility of
55
56
ElectricallyInduced nip Junctions in Multiple Graphene Layer Structures
the formation of effective electrically induced n and p regions and nip junctions, i.e., the nip junctions with suppressed reverse currents in multipleGL structures. These electrically induced nip junctions in multipleGL structures can be used in different devices, such as terahertz tunneling transittime oscillators, lasers, and highperformance interband photodetectors. They could enhance the device performance (increasing output power and responsivity) and expand their functions by allowing for the gatevoltage control.
Acknowledgments
This work was supported by the Japan Society for Promotion of Science and by the Japan Science and Technology Agency, CREST, Japan.
References
1. V. V. Cheianov and V. I. Fal’ko, Phys. Rev. B, 74, 041403(R) (2006).
2. L. M. Zhang and M. M. Fogler, Phys. Rev. Lett., 100, 116804 (2008).
3. B. Huard, J. A. Sulpizio, N. Stander, K. Todd, B. Yang, and D. GoldhaberGordon, Phys. Rev. Lett., 98, 236803 (2007). 4. B. Özyilmaz, P. JarilloHerrero, D. Efetov, D. Abanin, L. S. Levitov, and P. Kim, Phys. Rev. Lett., 99, 166804 (2007). 5. V. Ryzhii, M. Ryzhii, V. Mitin, and M. S. Shur, Appl. Phys. Express, 2, 034503 (2009).
6. M. Ryzhii and V. Ryzhii, Jpn. J. Appl. Phys. Part 2, 46, L151 (2007).
7. F. Xia, T. Murller, YM. Lin, A. ValdesGarsia, and F. Avouris, Nat. Nanotechnol., 4, 839 (2009). 8. M. Ryzhii and V. Ryzhii, Phys. Rev. B, 79, 245311 (2009).
9. F. Varchon, R. Feng, J. Hass, X. Li, B. Ngoc Nguyen, C. Naud, P. Mallet, J. Y. Veuillen, C. Berger, E. H. Conrad, and L. Magaud, Phys. Rev. Lett., 99, 126805 (2007).
10. M. Orlita, C. Faugeras, P. Plochocka, P. Neugebauer, G. Martinez, D. K. Maude, A.L. Barra, M. Sprinkle, C. Berger, W. A. de Heer, and M. Potemski, Phys. Rev. Lett., 101, 267601 (2008). 11. P. Neugebauer, M. Orlita, C. Faugeras, A.L. Barra, and M. Potemski, Phys. Rev. Lett., 103, 136403 (2009).
References
12. M. Orlita and M. Potemski, Semicond. Sci. Technol., 25, 063001 (2010).
13. D. L. Miller, K. D. Kubista, G. M. Rutter, M. Ruan, W. A. de Heer, P. N. First, and J. A. Stroscio, Science, 324, 924 (2009).
14. M. Sprinkle, D. Siegel, Y. Hu, J. Hicks, A. Tejeda, A. Taleb Ibrahimi, P. Le Fèvre, F. Bertran, S. Vizzini, H. Enriquez, S. Chiang, P. Soukiassian, C. Berger, W. A. de Heer, A. Lanzara, and E. H. Conrad, Phys. Rev. Lett., 103, 226803 (2009).
15. V. Ryzhii, M. Ryzhii, A. Satou, T. Otsuji, A. A. Dubinov, and V. Ya. Aleshkin, J. Appl. Phys., 106, 084507 (2009). 16. V. Ryzhii, A. A. Dubinov, T. Otsuji, V. Mitin, and M. S. Shur, J. Appl. Phys., 107, 054505 (2010).
17. V. Ryzhii, M. Ryzhii, V. Mitin, and T. Otsuji, J. Appl. Phys., 107, 054512 (2010).
18. V. Ryzhii, M. Ryzhii, and T. Otsuji, Phys. Status Solidi A, 205, 1527 (2008).
19. S. Luryi, Appl. Phys. Lett., 52, 501 (1988); see also S. Luryi, in HighSpeed Semiconductor Devices, by S. M. Sze (John Wiley, New York, 1990), p. 57. 20. H. Fukidome, Y. Miyamoto, H. Handa, E. Saito, and M. Suemitsu, Jpn. J. Appl. Phys., 49, 01AH03 (2010).
21. M. Shur, Physics of Semiconductor Devices (PrenticeHall, New Jersey, 1990). 22. F. Rana, P. A. George, J. H. Strait, S. Shivaraman, M. Chanrashekhar, and M. G. Spencer, Phys. Rev. B, 79, 115447 (2009).
23. R. S. Shishir, D. K. Ferry, and S. M. Goodnick, J. Phys.: Conf. Ser., 193, 012118 (2009).
57
Chapter 4
Tunneling Recombination in Optically Pumped Graphene with ElectronHole Puddles*
V. Ryzhii,a,c M. Ryzhii,a,c and T. Otsujib,c aComputational
Nanoelectronics Laboratory, University of Aizu, AizuWakamatsu 9658580, Japan bResearch Institute for Electrical Communication, Tohoku University, Sendai 9808577, Japan cJapan Science and Technology Agency, CREST, Tokyo 1070075, Japan [email protected]
We evaluate recombination of electrons and holes in optically pumped graphene associated with the interband tunneling between electronhole puddles and calculate the recombination rate and time. It is demonstrated that this mechanism can be dominant in a wide range of pumping intensities. We show that the tunneling recombination rate and time are nonmonotonic functions of the *Reprinted with permission from V. Ryzhii, M. Ryzhii, and T. Otsuji (2011). Tunneling recombination in optically pumped graphene with electronhole puddles, Appl. Phys. Lett., 99, 173504. Copyright © 2011 American Institute of Physics. GrapheneBased Terahertz Electronics and Plasmonics: Detector and Emitter Concepts Edited by Vladimir Mitin, Taiichi Otsuji, and Victor Ryzhii
Copyright © 2021 Jenny Stanford Publishing Pte. Ltd.
ISBN 9789814800754 (Hardcover), 9780429328398 (eBook)
www.jennystanford.com
60
Tunneling Recombination in Optically Pumped Graphene with ElectronHole Puddles
quasiFermi energies of electrons and holes and optical pumping intensity. This can result in hysteresis phenomena. The gapless energy spectrum of electrons and holes in graphene layers (GLs) and nonBernal stacked multiple graphene layers (MGLs) [1–3], which leads to specific features of its electrical and optical processes, opens up prospects of building of novel devices exploiting the interband absorption and emission of terahertz (THz) and infrared (IR) photons. Apart from an obvious possibility to use of graphene in THz and IR photodetectors [4–6], graphene layers (GLs) and multiple graphene layers (MGLs) can serve as active media in THz or IR lasers with optical [7–12] and injection [13] pumping. The achievement of sufficiently strong population inversion, which is necessary for negative dynamic conductivity in the THz or IR ranges of frequencies, can be complicated by the recombination processes. The recombination of electrons and holes in GLs at not too low temperatures is mainly determined by the emission of optical photons [14]. Due to a relatively high energy of optical phonons (hw0 0.2 eV), the recombination rate in GLs associated with this mechanism can be acceptable even at the room temperatures [10–12]. The radiative recombination in the practically interesting temperatures is weaker than that due to the optical phonon emission [15]. The acoustic phonon recombination mechanism as well as the Auger mechanism are forbidden due to the linearity of the electron and hole spectra even in the case their modifications associated with the intercarrier interaction [16, 17]. More complex processes involving the electron and hole scattering on impurities assisted by acoustic phonons also provide rather long recombination times which are longer than the radiative recombination time [18]. However in GLs with a disorder caused, for instance, by fluctuation of the surface charges resulting in the formation of the electron and hole puddles [19] (see also, for instance, Refs. [20–22]), the recombination can also be associated with the interband tunneling in the spots where the buildin fluctuation field is sufficiently strong. In this chapter, we find the dependences of the recombination rate and time in optically pumped graphene with electronhole puddles on the quasiFermi energy of electrons and holes (pumping intensity). The obtained results can be used for the interpretation of experimental observations and to promote the realization of graphenebased THz and IR lasers.
Tunneling Recombination in Optically Pumped Graphene with ElectronHole Puddles
The electric potential j = j (x, y, z), where x and y are the coordinates in the GL plane and the coordinate z is directed perpendicular to this plane, is governed by the Poisson equation presented in the following form: Dj =
Here,
Se =
2 p h2
Sh =
2 ph
2
4pe ( S e  S h  S i ) ◊d ( z ). æ
Ú
•
Ú
•
0
0
(4.1)
dp p , Ê vW p  me + ej ˆ 1 + exp Á ˜¯ kBT Ë dp p Ê v p + mh  ej ˆ 1 + exp Á W kBT ¯˜ Ë
,
and Si are the electron, hole, and charged impurity sheet densities, respectively, e = e, æ, h, and kB are the electron charge, dielectric constant, reduced Planck’s constant, and Boltzmann’s constant, vW 108 cm/s is the characteristic velocity, p is the electron and hole momentum, me and mh are the electron and hole quasiFermi energies counted from the Dirac point, T is the temperature, and D is the three dimensional Laplace operator. The delta function d(z) reflexes the localization of electrons, holes, and impurities in the GL plane z = 0. It is assumed that the electron spectra or electrons and holes are linear: ee = vWp and eh = –vWp. In the equilibrium, i.e., in the absence of pumping, me = mh = mi, where mi is determined by the spatially averaged impurity density ·Si(x, y)Ò or by the gate voltage (in gated GL structures). In the case of pumping of intrinsic GLs, me –mh = m π 0. In the latter case, T can differ from the lattice temperature Tl being both higher than Tl or lower [23]. Considering in the following the case ·Sd(x, y)Ò = 0 and assuming that the fluctuations are not too strong (ej < kBT), Eq. (4.1) can be linearized
(
)
Èj 4p e ˘ Dj = Í ln 1 + e m/kBT S ˙ ◊d ( z ), æ i˚ r Î s
(4.2)
2 where rs = (æh2vW /16e2kBT) is the screening length. Solving Eq. (4.2) with the boundary conditions jz=±• = 0 assuming that
61
62
Tunneling Recombination in Optically Pumped Graphene with ElectronHole Puddles
Si =
ÂS
qx ,qy
j( x , y , z ) =
ÂF
(i ) qx ,qy
qx ,qy
exp[i(qx x + qy y )],
exp( q  z ) exp[i(qx x + qy y)],
qx ,qy
where S(qi ),q x
y
and Fqx,qy are the pertinent amplitudes and q =
qx2 + qy2 , for the amplitude of the potential at the GL plane we
obtain
y qx ,qy =
2pe ˘ È 1 æ Íq + ln(1 + e m/kBT )˙ Î 2rs ˚
S(qi ),q . x
y
(4.3)
Setting q ~ π/ a , where a is the characteristic size of the puddles, and using Eq. (4.3), one can express y = maxyqx,qy via its value in the absence of screening y = 2eaS/æ y=
y . È a m/kBT ˘ )˙ ln(1 + e Í1 + Î 2p rs ˚
(4.4)
According to Eq. (4.4), the fluctuation electric field between positively and negatively charged puddles can be estimated as e ~ y/ a . Using the general formulas for the probability of the interband tunneling in GLs [24–26] and considering Eq. (4.4), the rate of the tunneling recombination can be presented as R~
R~
2 2e3/2
1/2 p 2 h3/2uW
y Ê mˆ R( m/ey ) , = a ËÁ ea ¯˜ 1 + hs ln(1 + e m/kBT )
2 2e3/2 Ê y ˆ 1/2 Á Ë a ˜¯ p 2h3/2uW
3/2
=
R [1 + hs ln(1 + e m/kBT )]3/2
(4.5) (4.6)
at relatively weak (m < ey) and strong (m > ey) optical pumping, respectively. Here, R~
2 2 Ê ey ˆ Á ah ¯˜ 1/2 Ë p 2vW
3/2
, hs =
8 e2akBT a . = 2 2p rs p æ h2vW
Tunneling Recombination in Optically Pumped Graphene with ElectronHole Puddles
Assuming that æ = 4, a = 30 nm, and S = 4 ¥ 1010 cm–2 [19], for the amplitude of the potential profile fluctuations e y and for the characteristic rate of the tunneling recombination R , we obtain the following estimates: e y = 8.5 meV and R 2.76 ¥ 1023 cm–2s–1, respectively. At T = 77 – 300 K, one obtains rs 0.67 – 2.62 nm and ηs = 0.47 – 1.82. These values are used in the following. In the case of strong pumping, the effective temperature of the electronhole plasma can be much higher than the lattice temperature [23]. As a result, the electronhole plasma can become nondegenerate, so that me = m < 0 while mh = –m > 0. This is possible when the plasma density increases with increasing pumping intensity slower that the effective temperature rises. In such a case, the screening vanishes (y y ), and R < 0. This implies that when m changes its sign, the tunneling recombination of electronhole pairs turns to their tunneling generation. This is because when the plasma density is lower than it would be in equilibrium but at the effective temperature T, the tunneling generation tends to establish an equilibrium density corresponding to T. The dependences of the tunneling recombination rate R versus the quasiFermi energy m for different temperatures T are shown in Fig. 4.1. For the calculations we used a formula for R which interpolates the dependences given by Eqs. (4.5) and (4.6). Figure 4.2 demonstrates also the dependences of the recombination rate R + R0 associated with both tunneling and optical phonon mechanisms (dashed lines). The contribution of the optical phonon mechanism R0 is taken into account using a simplified analytical formula [10, 23] derived from more rigorous one [14]: R0
˘ Ê w ˆÈ Ê 2m ˆ R0 exp Á  0 ˜ Íexp Á  1˙ . ˜ Ë kBT ¯ Ë kBT ¯ ÍÎ ˙˚
(4.7)
Here R0 3 ¥ 1024 cm–2s–1 [14] is the pertinent characteristic recombination rate. Disregarding the effects of electronhole heating or cooling and the effect of optical phonon heating [23], we have neglected the difference in the effective temperature T and the lattice temperature Tl. One can see that R is a nonmonotonic function
63
Tunneling Recombination in Optically Pumped Graphene with ElectronHole Puddles
of m with a maximum at a certain value of m. This is attributed to an increase in R at small m due to an increase in the electro and hole densities, i.e., in the number of carriers participating in the tunneling processes. However, at higher values of m, the screening of the potential fluctuations leads to a decrease in the electric field between the puddles and, consequently, in a decrease in the tunneling probability. When m increases further, the tunneling mechanism gives way to the optical phonon mechanism which becomes dominating. This results in a dramatic rise of R + R0 in the range of large m. The quantity m is governed by an equation equalizing the rate of recombination R + R0 and the rate of carrier photogeneration G = bI, where b = 0.023 is the GL absorption coefficient and I is the photon flux. Hence, the m – I dependence should exhibit the Sshape (see the dashed line in Fig. 4.1 corresponding to T = 200 K) leading to a hysteresis which might be pronounced at lowered temperatures. 10
24
2 1
Recombination rate, R (cm s )
64
23
10
T = 200 K
T = 300 K 22
10
0
20 40 60 QuasiFermi energy, µ (meV)
80
Figure 4.1 Recombination rate R vs quasiFermi energy m for tunneling mechanism (solid lines) and for combination of tunneling and optical phonon mechanism (dashed lines) in a GL at different temperatures T.
The recombination time is given by
tR =
(S e + S h ) 2(R + R0 )
Tunneling Recombination in Optically Pumped Graphene with ElectronHole Puddles
=
Ê kBT ˆ 2 Á p(R + R0 ) Ë hvW ˜¯
2
Ú
•
0
de e . 1 + exp(e  m / kBT )
(4.8)
The recombination time calculated without considering optical phonon mechanisms (solid lines) and with the latter (dashed lines) is shown in Fig. 4.2. As follows from Fig. 4.2, the tR – m dependence is also nonmonotonic with a minimum at moderate m (where tR ~ 2 ps) and a maximum at rather high m (where tR ~ 5 – 20 ps). Recombination time, τR (ps)
100
T = 200 K 10
T = 300 K
1 0
20 40 60 QuasiFermi energy, µ (meV)
80
Figure 4.2 Recombination time tR vs quasiFermi energy m at different temperatures T. Solid lines correspond to tunneling recombination, while dashed lines correspond to recombination associated with both tunneling and phonon mechanisms.
In optically pumped MGL structures, the electron and hole densities in each GL are close to each other provided the number of GLs K is not too large [27]. If the fluctuations are associated with the charges located near the lowermost GL, say, near the interface between this GL and the substrate, these fluctuations are screened by all GLs. In cases of such MGL structures, the first two terms in the righthand side of Eq. (4.1) can be multiplied by a factor K, so that the 2 / 16Ke2kBT ) . screening length becomes much shorter: rs(K ) = (æh2vW Consequently, parameter hs should be substituted by Khs. Naturally, this leads to a stronger suppression of the fluctuations (by a stronger
65
Tunneling Recombination in Optically Pumped Graphene with ElectronHole Puddles
screening) and hence to weakening of the tunneling recombination under consideration as shown in Fig. 4.3. If each GLs contains its own fluctuation charges, the averaging over a number of GL leads to a significant smoothening of the potential relief in all GL and, hence, to the suppression of the tunneling recombination is such MGL structures. 2 1
Tunneling recombination rate, R (cm s )
66
6×10
22
5×10
22
4×10
22
3×10
22
2×10
22
1×10
22
T = 200 K
T = 300 K
0 0
K=1 K = 10 20 40 80 60 QuasiFermi energy, µ (meV)
100
Figure 4.3 Tunneling recombination time tR vs quasiFermi energy m at different temperatures T in a GL (solid lines) and in MGL structure with ten GLs, i.e., K = 10 (dashed lines).
In conclusion, we calculated the recombination and time as functions of the quasiFermi energy in optically pumped graphene with electronhole puddles. It was shown that the tunneling recombination can be dominant recombination mechanism at low and moderate values of quasiFermi energy and, hence, at low and moderate pumping intensities. The dependences of the recombination and time on the quasiFermi energy and pumping intensity can be nonmonotonic resulting in hysteresis phenomena. The role of tunneling recombination can be diminished in MGL structures. The authors are grateful to N. Ryabova for comments on the manuscript and S. Boubanga Tombet for useful information. This
References
work was supported by the Japan Science and Technology Agency, CREST and by the Japan Society for Promotion of Science, Japan.
References
1. A. H. Castro Neto, F. Guinea, N. M. R. Peres, K. S. Novoselov, and A. K. Geim, Rev. Mod. Phys., 81, 109 (2009).
2. M. Sprinkle, D. Suegel, Y. Hu, J. Hicks, A. Tejeda, A. TalebIbrahimi, P. Le Fevre, F. Bertran, S. Vizzini, H. Enriquez, S. Chiang, P. Soukiassian, C. Berger, W. A. de Heer, A. Lanzara, and E. H. Conrad, Phys. Rev. Lett., 103, 226803 (2009). 3. M. Orlita and M. Potemski, Semicond. Sci. Technol., 25, 063001 (2010).
4. V. Ryzhii and M. Ryzhii, Phys. Rev. B, 79, 245311 (2009).
5. F. Xia, T. Murller, Y.M. Lin, A. ValdesGarsia, and F. Avouris, Nat. Nanotechnol., 4, 839 (2009).
6. V. Ryzhii, M. Ryzhii, V. Mitin, and T. Otsuji, J. Appl. Phys., 106, 084512 (2009). 7. V. Ryzhii, A. Satou, and T. Otsuji, J. Appl. Phys., 101, 024509 (2007).
8. F. Rana, IEEE Trans. Nanotechnol., 7, 91 (2008).
9. A. Dubinov, V. Ya. Aleskin, M. Ryzhii, and V. Ryzhii, Appl. Phys. Express, 2, 092301 (2009).
10. V. Ryzhii, M. Ryzhii, A. Satou, T. Otsuji, A. A. Dubinov, and V. Ya. Aleshkin, J. Appl. Phys., 106, 084507 (2009). 11. V. Ryzhii, A. A. Dubinov, T. Otsuji, V. Mitin, and M. S. Shur, J. Appl. Phys., 107, 054505 (2010).
12. A. A. Dubinov, V. Ya. Aleshkin, V. Mitin, T. Otsuji, and V. Ryzhii, J. Phys.: Condens. Matter, 23, 145302 (2011).
13. M. Ryzhii and V. Ryzhii, Jpn. J. Appl. Phys., 46, L151 (2007).
14. F. Rana, P. A. George, J. H. Strait, S. Shivaraman, M. Chanrashekhar, and M. G. Spencer, Phys. Rev. B, 79, 115447 (2009).
15. A. Satou, F. T. Vasko, and V. Ryzhii, Phys. Rev. B, 78, 115431 (2008).
16. M. S. Foster and I. L. Aleiner, Phys. Rev. B, 79, 085415 (2009).
17. D. M. Basko, S. Piscanec, and A. C. Ferrari, Phys. Rev. B, 80, 165413 (2009). 18. F. T. Vasko and V. V. Mitin, Phys. Rev. B, 84, 155445 (2011).
19. J. Martin, N. Akerman, G. Ulbricht, T. Lohmann, J. H. Smet, K. von Klitzing, and A. Yacoby, Nat. Phys., 4, 144 (2008).
67
68
Tunneling Recombination in Optically Pumped Graphene with ElectronHole Puddles
20. Y. Zhang, V. W. Brar, C. Girit, A. Zett, and M. F. Cromme, Nat. Phys., 5, 722 (2009).
21. J. M. Poumirol, W. Escoffer, A. Kumar, M. Goiran, R. Raquet, and J. M. Broto, New. J. Phys., 12, 083006 (2010).
22. P. ParoviAzar, N. Nafari, and M. Reza Rahimi Tabat, Phys. Rev. B, 83, 165434 (2011). 23. V. Ryzhii, M. Ryzhii, V. Mitin, A. Satou, and T. Otsuji, Jpn. J. Appl. Phys., 50, 9 (2011). 24. V. V. Cheianov and V. I. Fal’ko, Phys. Rev. B, 74, 041403(R) (2006).
25. A. Ossipov, M. Titov, and C. W. J. Beenakker, Phys. Rev. B, 75, 251401(R) (2007).
26. V. Ryzhii, M. Ryzhii, and T. Otsuji. Phys. Status Solidi A, 205, 1527 (2008). 27. M. Ryzhii, V. Ryzhii, T. Otsuji, V. Mitin, and M. S. Shur, Phys. Rev. B, 82, 075419 (2010).
Chapter 5
Analytical Device Model for Graphene Bilayer FieldEffect Transistors Using Weak Nonlocality Approximation*
V. Ryzhii,a,d M. Ryzhii,a,d A. Satou,b,d T. Otsuji,b,d and V. Mitinc aComputational
Nanoelectronics Laboratory, University of Aizu, AizuWakamatsu 9658580, Japan bResearch Institute for Electrical Communication, Tohoku University, Sendai 9808577, Japan cDepartment of Electrical Engineering, University at Buffalo, State University of New York, NY 14260, USA dJapan Science and Technology Agency, CREST, Tokyo 1070075, Japan [email protected]
We develop an analytical device model for graphene bilayer fieldeffect transistors (GBLFETs) with the back and top gates. The model is based on the Boltzmann equation for the electron transport and *Reprinted with permission from V. Ryzhii, M. Ryzhii, A. Satou, T. Otsuji, and V. Mitin (2011). Analytical device model for graphene bilayer fieldeffect transistors using weak nonlocality approximation, J. Appl. Phys., 109, 064508. Copyright © 2011 American Institute of Physics. GrapheneBased Terahertz Electronics and Plasmonics: Detector and Emitter Concepts Edited by Vladimir Mitin, Taiichi Otsuji, and Victor Ryzhii
Copyright © 2021 Jenny Stanford Publishing Pte. Ltd.
ISBN 9789814800754 (Hardcover), 9780429328398 (eBook)
www.jennystanford.com
70
Device Model for Graphene Bilayer FieldEffect Transistor
the Poisson equation in the weak nonlocality approximation for the potential in the GBLFET channel. The potential distributions in the GBLFET channel are found analytically. The sourcedrain current in GBLFETs and their transconductance are expressed in terms of the geometrical parameters and applied voltages by analytical formulas in the most important limiting cases. These formulas explicitly account for the shortgate effect and the effect of draininduced barrier lowering. The parameters characterizing the strength of these effects are derived. It is shown that the GBLFET transconductance exhibits a pronounced maximum as a function of the topgate voltage swing. The interplay of the shortgate effect and the electron collisions results in a nonmonotonic dependence of the transconductance on the topgate length.
5.1 Introduction
The unique properties of graphene layers, graphene nanoribbon arrays, and graphene bilayers [1–3] along with graphene nanomeshs [4] make them promising for different nanoelectronic device applications. The gapless energy spectrum of graphene layers allows to use them in terahertz and midinfrared detectors and lasers [5–9]. However, the gapless energy spectrum of graphene layers (GLs) is an obstacle for creating transistor digital circuits based on graphene fieldeffect transistors (GFETs) due to relatively strong interband tunneling in the FET offstate [10, 11]. The reinstatement of the energy gap in graphenebased structures like graphene nanoribbons, graphene nanomeshs, and graphene bilayers appears to be unavoidable to fabricate FETs with a sufficiently large on/ off ratio. Recently, the device dc and ac characteristics of graphene nanoribbon and graphene bilayer FETs (which are referred to as GNRFETs and GBLFETs, respectively) were both numerically and analytically assessed [12–19]. The device characteristics of GNRFETs operating in near ballistic and driftdiffusion regimes can be calculated analogously with those of nanowire and carbon nanotubeFETs (see, for instance [20–22] and references therein). The GBLFET characteristics can, in principle, be found using the same approaches as those realized previously for more customary FETs with a twodimensional electron system in the channel [23–31].
Introduction
However, some important features of GBLFETs, in particular, the dependence of both the electron density and the energy gap in different sections of the GBLFET channel on the gate and drain voltages should be considered [32–34], along with the “shortgate” effect and the draininduced barrier lowering [29]. In this chapter, we use a substantially generalized version of the GBLFET analytical device model [17, 18] to calculate the characteristics of GBLFETs (the threshold voltages, currentvoltage characteristics, and transconductance) in different regimes and analyze the possibility of a significant improvement of the ultimate performance of these FETs by shortening of the gate and decreasing of the gate layer thickness. The device model under consideration which presents the GBLFET characteristics in closed analytical form allows a simple and clear evaluation of the ultimate performance of GBLFETs and their comparison. The following effects are considered: (a) dependences of the electron density and energy gap in different sections of the channel on the applied voltages and the inversion of the gated section charge; (b) degeneracy of the electron system, particularly in the source and drain sections of the channel; (c) the shortgate effect and the effect of draininduced barrier lowering; (d) electron scattering in the channel. Our model is based on the Boltzmann kinetic equation for the electron system in the GBLFET and the Poisson equation in the weak nonlocality approximation [35, 36]. The use of the latter allows us to find the potential distributions along the channel in the most interesting cases and obtain the GBLFET characteristics analytically. The chapter is organized as follows. In Section 5.2, the GBLFET device model under consideration is presented and the features of GBLFET operation are discussed. In Section 5.3, the main equations of the model are cited. The general formulas for the sourcedrain current and the GBLFET transconductance simplified for the limiting cases (far below the threshold, near threshold, and at low topgate voltages corresponding to the onstate) are also presented. In this section, the sourcedrain current and the GBLFET transconductance are expressed in terms of the Fermi energy in the source and drain contacts and the height of the potential barrier in the channel. To find the barrier height, the Poisson equation is solved for different limiting cases in Section 5.4. The obtained potential
71
72
Device Model for Graphene Bilayer FieldEffect Transistor
distributions are used for the derivation of the explicit formulas for sourcedrain current and the transconductance as functions of the applied voltages and geometrical parameters. Section 5.5 deals with a brief discussion of some effects (role of the device geometry, electron scattering, charge inversion in the channel, and interband tunneling), which influence the GBLFET characteristics. In Section 5.6, we draw the main conclusions. Some reference data related to the voltage dependences of the Fermi energy and the energy gap in different sections of the GBLFET channel are contained in the Appendix.
5.2 Device Model and Features of Operation
We consider a GBLFET with the structure shown in Fig. 5.1. It is assumed that the back gate, which is positively biased by the pertinent voltage Vb > 0, provides the formation of the electron channel in the GBL between the Ohmic source and drain contacts. A relatively short top gate serves to control the sourcedrain current by forming the potential barrier (its height Dm depends on the top gate voltage Vt and other voltages) for the electrons propagating between the contacts.
Figure 5.1 Schematic view of the GBLFET structure.
We shall assume that the GBLFETs under the conditions when the electron systems in the source and drain sections are degenerate, i.e., eF kBT. This implies that the back gate voltage is sufficiently high to induce necessary electron density in the source and drain sections.
Main Equations of the Model
In the GBLFET the energy gap is electrically induced by the back gate voltage [32–34] (see also [18]). Thus in GBLFETs, the back gate plays the dual role: it provides the formation of the electron channel and the energy gap. Since the electric field component directed perpendicular to the GBL plane in the channel section below the top gate (gated section) is determined by both Vb and Vt, the energy gap can be different in different sections of the GBL channel: Eg,s (source section), Eg (gated section), and Eg,d (drain section) [17, 18]. At sufficiently strong topgate voltage (Vt < Vth < 0, where Vth is the threshold voltage), the gated section becomes depleted. Since the energy gaps in GBLs are in reality not particularly wide, at further moderate increase in Vt, the gated section of the channel becomes filled with holes (inversion of the charge in the gated section) if Vt < Vin < Vth, where Vin is the inversion voltage. As a result, the GBLFETs with moderate energy gap are characterized by the threshold and inversion voltages: Vth < 0 and Vin < 0. The explicit formulas for Vth and Vin shall be given in the following. The cases Vt = Vth and Vt = Vin correspond to the alignment of the Fermi level in the source section of the channel with the conduction band bottom and the valence band top, respectively, in the gated section.
5.3 Main Equations of the Model
Due to relatively high energy of optical phonons in graphene, the electron scattering in the GBLFET channel is primarily due to disorder and acoustic phonons. Considering such quasielastic scattering, the quasiclassical Boltzmann kinetic equation governing the steady state electron distribution function fp = fp(x) in the gated section of the channel can be presented as vx
∂f p ∂x
+e
∂j ∂fp = d 2qw(q)( fp+ q  fp )d (e p+q  e p ). ∂x ∂px
Ú
(5.1)
Here e = e is the electron charge, ep = p2/2m, m is the electron effective mass in GBL, p = (px,py) is the electron momentum in the GBL plane (z = 0), w(q) is the probability of the electron scattering on disorder and acoustic phonons with the variation of the electron momentum by quantity q = (qx,qy), vx = px, and axis x is directed in this plane (from the source contact to the drain contact, i.e., in the
73
74
Device Model for Graphene Bilayer FieldEffect Transistor
direction of the current). For simplicity, we disregard the effect of “Mexican hat” (see, for instance, Ref. [34]) and a deviation of the real energy spectrum in the GBL from the parabolic one (the latter can be marked in the source and drain sections with relatively high Fermi energies). The effective mass in GBLs m = γ1/2νW, where γ1 0.35 – 0.43 eV is the interlayer hopping integral and νW 108 cm/s is the characteristic velocity of electrons and holes in GLs [3, 34–36], so that m (0.03 – 0.04)m0, where m0 is the bare electron mass. One of the potential advantages of GBLFETs is the possibility of ballistic transport even if the topgate length Lt is not small. In such GBLFETs, one can neglect the righthand side term in Eq. (5.1). As in Refs. [10, 15, 37, 38], we use the following equation for the electric potential j = j (x) = y (x, z)z=0 in the GBL plane: (Wb + Wt ) ∂2j j  Vb j  Vt 4pe = (S   S + ). 3 Wb Wt k ∂x 2
(5.2)
Here, S– and S+ are the electron and hole sheet densities in the channel, respectively, k is the dielectric constant of the layers between the GBL and the gates and Wb and Wt are the thicknesses of these layers. In the following, we put Wb = Wt = W (except Section 5.5). Equation (5.2) is a consequence of the twodimensional Poisson equation for the electric potential y (x, z) in the GBLFET gated section (–Lt/2 £ x £ Lt/2 and –Wb £ z £ Wt, where Lt is the length of the top gate) in the weak nonlocality approximation [37]. This equation provides the potential distributions, which can be obtained from the twodimensional Poisson equation by expansion in powers of the parameter d = (Wb3 + Wt3)/15(Wb + Wt)/L2 = W2/15L2, where L is the characteristic scale of the lateral inhomogeneities (in the xdirection) assuming that d 1, i.e., L is not too small. The lowest approximation in such an expansion leads to the Shockley’s gradual channel approximation, in which the first term on the left side of Eq. (5.2) is neglected [39, 40]. The factor 1/3 appeared due to features of the Green function of the Laplace operator in the case of the geometry under consideration. The boundary conditions for Eqs. (5.1) and (5.2) are presented as fp
px ≥0,x =  Lt /2
= fs,p , fp
px £0,x = Lt /2
= fd,p ,,
(5.3)
Main Equations of the Model
j x =L /2 = 0, j x = L /2 = Vd + (e F,d  e F,s )/ e = Vd* , t
t
(5.4)
where fs,p and fd,p are the electron distribution functions in the source and drain sections of the channel. The functions fs,p and fd,p are the Fermi distribution functions with the Fermi energies eF,s and eF,d which are determined by the back gate and drain voltages, Vb and Vd [17, 18] (see also the Appendix): e F,s eVb
b b , e F,d e(Vb Vd ) , (1 + b) (1 + b)
(5.5)
where b = aB/8W, aB = kћ2/me2 is the Bohr radius, and ћ is the reduced Planck constant. In the following, we shall assume that b 1, so that eF,s beVb and eF,d be(Vb – Vd). In particular, if aB = 4 nm (GBL on SiO2) and W = 10 nm, one obtains b 0.05. Due to a smallness of b, we shall disregard a distinction between Vd* and Vd because Vd – Vd* bVd Vd (as shown in the Appendix). Restricting ourselves by the consideration of GBLFETs operation at not too high drain voltages, we also neglect the difference in the Fermi energies in the source and drain sections, i.e., put eF,d eF,s = eF. The sourcedrain dc current density (current per unit length in the direction perpendicular its flow) can be calculated using the following formulas: J= =
Ú d pv
4e
2
(2p )2 e p 2 2
Ú
•
•
dpy
x fp
Ú
•
0
dpx vx ( f p  f p ).
In this case, Eq. (5.1) with boundary conditions (5.3) yields fp  f p
Q( px2/ 2m + ej )  Q( px2/ 2m + ej  eVd ) , 1 + exp[( p2/ 2m + ej  e F )/ kBT ]
(5.6) (5.7)
where T is the temperature, kB is the Boltzmann constant, and Q(e) is the unity step function. Using Eqs. (5.6) and (5.7), we obtain ÏÔ 1 dx Ì 2 2 2 • D p m ÔÓ 1 + exp[( py / 2m + x  e F )/ kBT ¸Ô 1 ˝ 2 1 + exp[(p py / 2m + x  e F + eVd )/kBT ] Ô˛
J=
e
Ú
•
dpy
Ú
•
75
76
Device Model for Graphene Bilayer FieldEffect Transistor
=
ekBT p 2 2
Ï È ˘ Ê e F  py2 / 2m  D m ˆ Ô dpy Ìln Íexp Á ˜ + 1˙ ˜¯ ÁË • kBT ˙ Í ˚ ÓÔ Î
Ú
•
˘¸ È Ê e F  py2 / 2m  D m  eVd ˆ Ô ˙ 1  ln Íexp Á + ˜ ˝. ˜¯ ÁË kBT ˙Ô Í ˚˛ Î
(5.8)
Equation (5.8) can be presented in the following form: J = J0
•
Ú
0
{
dz ln ÈÎexp(d m  z 2 )+ 1˚˘
}
 ln ÈÎexp(d m  Ud  z 2 ) + 1˘˚ . Here (see, for instance, Ref. [23]) J0 =
2 2me(kBT )3/2 p 2 2
(5.9) (5.10)
,
is the characteristic current density, and dm = (eF – Dm)/kBT, and Ud = eVd/kBT are the normalized voltage swing and drain voltage, respectively. At m = 4 ¥ 10–29 g and T = 300 K, J0 2.443 A/cm. Figure 5.2 shows the dependences of the sourcedrain current J normalized by the value J0 as a function of the Ud calculated using Eq. (5.9) for different values of dm. The GBLFET transconductance g is defined as g=
∂J . ∂Vt
(5.11)
Equations (5.9) and (5.11) yield g = J0
Ú
•
0
{
dz ÈÎexp(z 2  d m ) + 1˚˘
 ÈÎexp( z 2  d m + Ud ) + 1˘˚
1
1
}
Ê ∂d m ˆ ÁË  ∂V ˜ . t ¯
(5.12)
The obtained formulas for the sourcedrain current and transconductance can be simplified in the following limiting cases.
Main Equations of the Model
2.5
δm = 2.0
J/J0
2 δm = 1.0
1.5 1
δm = 0.0
0.5
δm = 1.0 δm = 2.0
0 0
2
4
Ud
6
8
10
Figure 5.2 Normalized sourcedrain current J/J0 versus normalized drain voltage Ud at different values of normalized topgate voltage swing dm.
5.3.1 High TopGate Voltages At high topgate voltages, which correspond to the subthreshold voltage range, the barrier height exceeds the Fermi energy (Dm eF), so that dm 1. In this case (the electron system in the gated section is nondegenerate), using Eqs. (5.9) and (5.12), we obtain J=
g=
Ê e  Dm ˆ È Ê eVd ˆ ˘ p J0 exp Á F Í1  exp Á ˙, ˜ 2 Ë kBT ¯ ÎÍ Ë kBT ˜¯ ˙˚
Ê e  Dm ˆ È Ê eVd ˆ ˘ Ê ∂D m ˆ p J0 exp Á F . Í1  exp Á ˙ ˜ 2 kBT Ë kBT ¯˜ ˙˚ ËÁ ∂Vt ¯˜ Ë kBT ¯ ÎÍ
5.3.2 Near Threshold TopGate Voltages In this case, Dm eF,, i.e., dm 1, Eqs. (5.9) and (5.12) yield J J0
eVd kBT
È Ê eVd ˆ ˘ Ê e  Dm ˆ ˘ È Íz 1 +z 2 Á F ˙ Í1  exp Á ˙, ˜ Ë kBT ˜¯ ˙˚
Ë kBT ¯ ˙˚ ÎÍ ÍÎ g
Ê ∂D ˆ
z2 Á  m ˜ Ë ∂Vt ¯ (kBT ) J0eVd
2
(5.13)
(5.14)
(5.15) (5.16)
77
78
Device Model for Graphene Bilayer FieldEffect Transistor
at low drain voltages eVd kBT (Ud 1), and
È Ê e  Dm ˆ ˘ J J0 Íz 0 +z 1 Á F ˙, Ë kBT ¯˜ ˙˚ ÍÎ g
Ê ∂D ˆ J0 z1 Á  m ˜ kBT Ë ∂Vt ¯
at high drain voltages eVd kBT (Ud 1). Here, z0 = x2) + 1] 0.678, z1 =
Ú
•
0 2 1]
(5.17)
Ú
•
0
(5.18)
dx ln[exp(–
dx /[exp(x2) + 1] 0.536, and z2 =
Ú
•
0
dx
0.337. In the limit eF = Dm, Eqs. (5.13) and exp(x 2)/[exp(x 2) + (5.14) provide the values J and g close to those obtained from Eqs. (5.17) and (5.18), which are rigorous in such a limit.
5.3.3 Low TopGate Voltages
At low topgate voltages, Dm < eF, from Eqs. (5.9) 2 J I0[(e F  D m )3/2 Q(e F  D m ) 3
(e F  D m  eVd )3/2 Q(e F  D m  eVd )], g I0[(e F  D m )1/2 Q(e F  D m ) Ê ∂D ˆ (e F  D m  eVd )1/2 Q(e F  D m  eVd )]Á  m ˜ . Ë ∂Vt ¯ Here,
I0 =
2 2me , p 2 2
with J0 = I0 (kBT)3/2.
Using Eqs. (5.19) and (5.20), one obtains
Ê D ˆ J I0eVd (e F  D m ) I0eVd e F Á 1  m ˜ , 2e F ¯ Ë 1 eV Ê ∂D ˆ g I0 d Á  m ˜ 2 e F Ë ∂Vt ¯
at eVd eF – Dm, and
(5.19) (5.20) (5.21)
(5.22) (5.23)
Potential Distributions, SourceDrain Current, and Transconductance
Ê 3D ˆ 2 2 J = I0(e F  D m )3/2 I0e F3/2 Á 1  m ˜ , 3 3 2e F ¯ Ë Ê ∂D ˆ g I0 (e F  D m ) Á  m ˜ Ë ∂Vt ¯
(5.24) (5.25)
at eVd eF – Dm. The dependences shown in Fig. 5.2 describe implicitly the dependences of J calculated using the universal Eq. (5.9) on the backgate, topgate, and drain voltages as well as on the geometrical parameters. Equations (5.13)–(5.25) provide these dependences in most interesting limits. However, to obtain the explicit formulas for J as well as for g, one needs to determine the dependences of the barrier height Dm on all voltages and geometrical parameters. Since the electron densities in the gated section in the limiting cases under consideration are different, the screening abilities of the electron system in this section and the potential distributions are also different. The latter leads to different Dm vs Vt relations.
5.4 Potential Distributions, SourceDrain Current, and Transconductance
To obtain the explicit dependences of the sourcedrain current and the transconductance on the gate voltages Vb and Vt as well as on the drain voltage Vd, one needs to find the relationship between the barrier height Dm and these voltages. This necessitates the calculations of the potential distribution in the channel. The latter can be found from Eq. (5.2) in an analytical form in the following limiting cases.
5.4.1 High TopGate Voltages: Subthreshold Voltage Range (Δm >> εF)
When the barrier height Dm exceeds the Fermi energy eF, the electron density is low in the gated section and, hence, one can disregard the contribution of the electron charge in this section. In such a limit, we arrive at the following equation for the potential:
79
80
Device Model for Graphene Bilayer FieldEffect Transistor
F d 2j j = 0 ,
dx 2 L 20 L20
(5.26)
where L0 = 2 / 3W and F0 = –(Vb + Vt)/2. Solving Eq. (5.26) considering boundary conditions (5.4), for the case of high topgate voltages we obtain È cosh( x /L0 ) ˘ sinh[(2x + Lt )/ 2L0 ] j = F0 Í  1˙ +Vd . co sh( / ) sinh( Lt /L0) L 2L t 0 Î ˚
(5.27)
Limiting our consideration by the GBLFETs with not too short top gate (Lt W), Eq. (5.27) can be presented as È Ê L ˆ Ê x ˆ˘ j F0 Í1  2exp Á  t ˜ cosh Á ˜ ˙ Ë L ¯ ˙˚ Ë 2L0 ¯ ÍÎ Ê L ˆ Ê x ˆ . +Vd exp Á  t ˜ exp Á Ë L0 ¯˜ Ë 2L0 ¯ Equation (5.28) yields
(5.28)
Ê 1 ˆ eV D m eF0 Á 1  ˜  d h0 ¯ 2h0 Ë =
e(Vb + Vt ) Ê 1 ˆ eV 1 ˜  d , Á h0 ¯ 2h0 2 Ë
(5.29)
where h0 = exp(Lt/2L0)/2. Simultaneously, for the position of the barrier top one obtains xm = 
=
L0 Ê Vd ˆ ln 1 + ˜ 2 ÁË F0 ¯
L0 Ê 2Vd ˆ ln Á 1 . 2 Ë Vb + Vt ˜¯
(5.30)
The terms in the righthand side of Eq. (5.29) containing parameter h0 reflect the effect of the topgate geometry (finiteness of its length). This effect is weakened with increasing top barrier length Lt. The effect of draininduced barrier lowering in the case under consideration is described by the last term in the righthand side of Eq. (5.29). Equation (5.29) yields (∂Dm/∂Vt) = –(e/2)(1 – h0–1). Invoking Eqs. (5.13) and (5.14), we obtain
Potential Distributions, SourceDrain Current, and Transconductance
J=
È e(V V ) Ê p 1 ˆ˘ J0 exp Í t th Á 1  ˜ ˙ h0 ¯ ˙˚ 2 ÎÍ 2kBT Ë È Ê eVd ˆ Ê eV ˆ ˘ , ¥ Í1  exp Á  d ˜ ˙ exp Á Ë kBT ¯ ˚˙ Ë 2h0kBT ˜¯ ÎÍ
g
È e(V  V ) Ê 1 ˆ˘ p eJ0 exp Í t th Á 1  ˜ ˙ h0 ¯ ˙˚ 4 kBT ÎÍ 2kBT Ë È Ê eVd ˆ Ê eV ˆ ˘ ¥ Í1  exp Á  d ˜ ˙ exp Á . Ë kBT ¯ ˙˚ Ë 2h0kBT ¯˜ ÎÍ
(5.31)
(5.32)
Here, Vth = –[1 + 2b/(1 – h0–1 )]Vb –(1 + 2b)Vb. The rightmost factors in the righthand sides of Eqs. (5.31) and (5.32), associated with the effect of draininduced barrier lowering, lead to an increase in g with increasing Vd not only at eVd ~ kBT but at eVd kBT:g µ exp (eVd/2h0kBT). One can see that in the range of the topgate voltages under consideration, the GBLFET transconductance exponentially decreases with increasing  Vt + Vb and g�
Je p eJ0 , � g0 = 4 kBT 2kBT
(5.33)
where at T = 300 K the characteristic value of the transconductance g0 4330 mS/mm.
5.4.2 Near Threshold TopGate Voltages (Δm εF)
At eVd kBT ef, taking into account that the electron distribution is characterized by the equilibrium Fermi distribution function, the electron density in the gated section can be presented in the following form: S�
2m (e F + ej). p �2
Considering this, we reduce Eq. (5.2) to
d 2j j F  2 = 2. 2 L L dx
(5.34)
(5.35)
81
82
Device Model for Graphene Bilayer FieldEffect Transistor
Here,
L= F=
aW aBW 2 b, B =W 12 3 12(1 + 2b)
[e F /e  b(Vb +Vt )] b(bVb + Vt ) bVt , (1 + 2b)
so that L/L0 b < 1. The solution of Eq. (5.35) with boundary condition (5.4) is given by ˘ È cosh( x/L ) sinh[(2x + Lt )/ 2L] j =FÍ  1˙ +Vd sinh( Lt / 2L ) Î cosh( Lt / 2L ) ˚ È Ê L ˆ Ê x ˆ˘ F Í1  2exp Á  t ˜ cosh Á ˜ ˙ Ë L¯˚ Ë 2L ¯ Î Ê L ˆ Ê xˆ +Vd exp Á  t ˜ exp Á ˜ . Ë L¯ Ë 2L ¯ From Eq. (5.36) we obtain
(5.36)
Ê 1 ˆ eV D m eF Á 1  ˜  d h ¯ 2h Ë Ê 1 ˆ eV [e F  eb(Vb +Vt )]Á 1  ˜  d h ¯ 2h Ë Ê 1 ˆ eV ebVt Á 1  ˜  d , h Ë ¯ 2h
(5.37)
where h = exp (Lt/2L)/2, and the position of the barrier top is xm 
L Vd L Vd . 2 F 2b Vb
(5.38)
Since L < L0, one obtains h h0, and the terms in Eq. (5.37) containing parameter h can be disregarded. This implies that the effects of topgate geometry and draininduced barrier lowering are much weaker (negligible) in the case of the topgate voltages in question in comparison with the case of high topgate voltages. Substituting Dm from Eq. (5.37) into Eq. (5.16), for low drain voltages we arrive at g
J0e2Vdz 2 Ê 1ˆ 1  ˜ b. 2 Á h Ë ¯ (kBT )
(5.39)
Potential Distributions, SourceDrain Current, and Transconductance
At relatively high drain voltages (eVd > ef kBT), the electron charge in the source portion of the gated section (x £ xm, where xm is the coordinate of the barrier top) is primarily determined by the electrons injected from the source. The electron injection from the drain at high drain voltages is insignificant. Hence, the electron charge in the drain portion of the gated section can be disregarded. In this case, Eq. (5.2) can be presented as d 2j j F  2= 2 2 dx L L
at –Lt/2 £ x £ x0, and
(5.40)
F d 2j j  2 = 02 2 dx L0 L0
(5.41)
at x0 £ x £ Lt/2. At the point x = x0 corresponding to the condition ejx=x0 + eF = 0, the solutions of Eqs. (5.40) and (5.41) should be matched: j x=x dj dx
0 0
= j x=x =
x = x 0 0
0 +0
dj dx
=
eF , e
x = x 0 +0
.
(5.42)
Solving Eqs. (5.40) and (5.41) with conditions (5.4) and (5.42), we obtain the following formulas for the potential j at – Lt/2 £ x £ x0 and x0 £ x £ Lt/2 as well as an equation for x0: È cosh( x/L) ˘ Èe ˘ cosh( x0/L) j =FÍ  1˙  Í F + F F˙ cosh( Lt / 2L) ˚ Î cosh( Lt / 2L) ˚ Î e ¥
sinh[(x + Lt / 2)/L)] , sinh[(x0 + Lt / 2)/L)]
È cosh( x/L0) ˘ sinh[( x + Lt / 2)/L 0] j = F0 Í  1˙ +Vd L cosh( / 2 L ) sinh(( Lt /L0) t 0 ˚ Î
(5.43)
Èe sinh[( x0 + Lt / 2)/L 0] ˘ cosh( x0/L0)  F0 + Vd  Í F + F0 ˙ sinh((Lt /L0) cosh( Lt / 2L0) Îe ˚ ¥
sinh[(x  Lt / 2)/L 0] , sinh[(x0  Lt / 2) /L0 ]
(5.44)
83
Device Model for Graphene Bilayer FieldEffect Transistor
Vt = 7.0 V
1 0.5 Δ, eV
84
Vd = 0.0 V
Vd = 0.5 V
0
Vt = 5.5V
Lt = 100 nm 40 nm
0.5 1
0.25 0 0.25
0.25 0 0.25
x/Lt
Vd = 1.0 V
0.25 0 0.25
Figure 5.3 Barrier profile D = –ej at different topgate voltage Vt and drain voltage Vd for GBLFETs with different topgate length Lt. Upper and lower pairs of curves correspond to Vt – Vth = –1.5 V and Vt – Vth 0, respectively; W = 10 nm, b = 0.05, and Vb = 5.0 V.
˘ cosh( x0/L ) 1 ÏÔ sinh( x0/L) È e F Í +F F˙ ÌF L ÔÓ cosh( Lt / 2L) Î e cosh( Lt / 2L ) ˚ cosh[( x0 + Lt /2) / L )] ¸Ô ¥
˝ sinh[( x0 + Lt /2) / L )] Ô˛ =
cosh[( x 0 + Lt / 2) /L0 ] 1 ÏÔ sinh( x0/L0 )
+ Vd ÌF0 L 0 ÓÔ cosh( Lt / 2L0 )
sinh( Lt /L0 )
Èe cosh( x0/L0) sinh[( x0 + Lt / 2) /L0 ] ˘
 Í F + F0  F0 + Vd ˙ sinh(( Lt /L0 ) cosh( Lt /2L0)
Î e
˚
cosh[( x 0  Lt /2)/L0 ] Ô¸ ¥
˝ .
sinh[( x0  Lt /2) /L0 ] Ô˛
(5.45)
In the cases Vb + Vt 0 and –(Vb + Vt) Vb eF/e, Eq. (5.45) yields x0 = –Lt/2 + L In[4bVt/( b + 2b)(Vb + Vt)] and x0 –Lt/2 + 2L0eF/ [–e(Vb + Vt)] –Lt/2 + 2bL0Vb/[–(Vb + Vt)], respectively. When –(Vb + Vt) Æ +0, the matching point shifts toward the channel center. If –(Vb + Vt) increases, the matching point tends to the source edge of the channel. In this case, the role of the electron charge in the vicinity of the source edge diminishes, and the potential distribution tends to that given by Eq. (5.27). At the threshold, the matching point x0 coincides with the position of the barrier maximum xm. Considering that at x0 = xm, both
Potential Distributions, SourceDrain Current, and Transconductance
the lefthand and righthand sides of Eq. (5.45) are equal to zero, for the barrier top height near the threshold at relatively high drain voltages we obtain the following: Ê 1 ˆ eV D m eF0 Á 1  ˜  d h0 ¯ h0 Ë
=xm 
e(Vb + Vt ) Ê 1 ˆ eVd ÁË 1  h ¯˜  h , 2 0 0
Ê 2F ˆ Lt L 1 + L ln Á  t + L ln . ˜ 2 2 b Ë F  F0 ¯
(5.46) (5.47)
Both Eqs. (5.29) and (5.46) correspond to the situations when the electron density in a significant portion of the channel is fairly low. However there is a distinction in the dependence of Dm on Vd (the pertinent coefficients differ by factor of two). This is because in the first case the barrier top is located near the channel center, whereas in the second case it is shifted to the vicinity of the source edge [compare Eqs. (5.30) and (5.47)]. Using Eqs. (5.19) and (5.50), we obtain (∂ Dm/∂ Vt) = –(e/2)(1 – h0–1) and arrive at the following formula for the transconductance near the threshold, i.e., when Vt Vth È e(Vt Vth ) Ê 1 ˆ˘ J J0 Íz 0 +z 1 1 ˜˙, Á 2kBT Ë h0 ¯ ˙˚ ÍÎ g
J0e z 1 Ê 1ˆ 1  ˜ = gth . Á kBT 2 Ë h0 ¯
(5.48)
(5.49)
Here, as above, Vth –(1 + 2b)Vb. In particular, Eqs. (5.48) and (5.49) at Vt = Vth, yield Jth J0z0. For a GBLFET with Lt = 40 nm, W = 10 nm, at T = 300 K, one obtains Jth 1.656 A/cm and gth 2167 mS/mm.
5.4.3 Low TopGate Voltages (Dm < ef)
At relatively low topgate voltages when Dm < eF, the electron system is degenerate not only in the source and drain sections but in the gate section as well. In this topgate voltage range, the spatial variation of the potential is characterized by L W 2b/3. As a result, for Dm one obtains an equation similar to Eq. (5.37). Since L < L0 Lt, the
85
86
Device Model for Graphene Bilayer FieldEffect Transistor
parameter determining the effect of the topgate geometry and the effect of draininduced barrier lowering is h = exp(Lt/2L)/2 h0. As a consequence, one can neglect the effects in question in the topgate voltage range under consideration. As a result, one can arrive at 2 J I0e3/2[b(Vt  Vth )]3/2 [b(Vt Vth Vd ]3/2 3
when Vd £ b(Vt – Vth),
2 J I0e3/2[b(Vt  Vth )]3/2 , 3
when Vd > b(Vt – Vth), and
∂D m = be. ∂Vt
Considering Eq. (5.51), at low topgate voltages we obtain g
beI0 eVd be3/2I0 Vd 2 2 eF Vb
when eVd eF – Dm be(Vb + Vt), and
g beI0 e F b3/2e3/2I0 Vb = gon
(5.50)
(5.51) (5.52) (5.53) (5.54)
when eVd eF – Dm be(Vb + Vt). As follows from Eqs. (5.33) and (5.34), the transconductance is proportional to a small parameter b3/2. This is because the effect of the topgate potential is weakened due to a strong screening by the degenerate electron system in the gated section. As a result, the transconductance at low topgate voltages is smaller than that at the topgate voltage corresponding to the threshold. Assuming that b = 0.05 and Vb = 5 (eF 0.25 eV), we obtain gon 1467 mS/mm. Comparing Eqs. (5.49) and (5.54), we
find gon/gth µ b3/2 eVb/ kBT 0.158 and g/gth gon/gth 0.68. Since the sourcedrain current at high topgate voltages decreases exponentially when –Vt increases, the transconductance decreases as well. Figure 5.3 shows the barrier (conduction band) profile D = –ej in the GBLFETs calculated using Eqs. (5.27), (5.36), and (5.44) for different applied voltages and topgate lengths. As demonstrated, the barrier height naturally decreases with increasing Vt – Vth. At the threshold (Vt = Vth), the barrier height is equal to the Fermi energy (at b = 0.05 and Vb = 5 V, eF 0.25 eV). One can see that shortening
Potential Distributions, SourceDrain Current, and Transconductance
of the topgate leads to a marked decrease in the barrier height (the shortgate effect). The sourcedrain current as a function of the drain voltage for different topgate voltage swings is demonstrated in Fig. 5.4. The dependences corresponding to Vt – Vth < 0, Vt – Vth = 0, and Vt – Vth > 0 were calculated using formulas from subsections A, B, and C, respectively. Figure 5.5 shows that the transconductance as a function of the topgate voltage swing exhibits a pronounced maximum at Vt Vth. This maximum is attributed to the following. At high topgate voltages, the effect of screening is insignificant due to low electron density in the channel. As a result, the height of the barrier top is rather sensitive to the topgate voltage variations. The sourcedrain current in this case is exponentially small, so that the transconductance is small. In contrast, at low topgate voltages, the screening by the electrons in the channel is effective, leading to a much weaker control of the barrier height by the top voltage [pay attention to parameter b 1 in Eqs. (5.50)–(5.54)]. Despite, a strong sourcedrain current provides a moderate values of the transconductance. However, in the near threshold voltage range, both the sensitivity of the barrier height and the sourcedrain current to the topgate voltage are fairly large. Sourcedrain density, A/cm
100
W = 10 nm Vb = 5.0 V T = 300 K
Lt = 100 nm
b = 0.05
3.0 V 1.0 V
10
0.0 V
1
0.6 V 0.1 0
VtVth = 0.7 V 0.05
0.1 0.15 Drain voltage, V
0.2
0.25
Figure 5.4 Sourcedrain current J versus drain voltage Vd at different values of the topgate voltage swing Vt – Vth.
87
Device Model for Graphene Bilayer FieldEffect Transistor
Lt = 40 nm Vb = 5.0 V
3000 Transconductance, mS/mm
88
b = 0.05 Vd = 0.1 V
T = 300 K 2000
Wt = 5 nm Wt = 10 nm
1000
0 1
0 2 1 Topgate voltage swing, V
3
Figure 5.5 Transconductance g versus topgate voltage swing Vt – Vth.
5.5 Discussion 5.5.1 Role of Geometrical Parameters In the main part of the chapter, we assumed that the thicknesses of the gate layers are equal to each other: Wb = Wt = W. If Wb π Wt, the formulas obtained above should be slightly modified. In particular, near the threshold (∂Dm/∂Vt) = –(e/(1 + Wt/Wb)(1 – h0–1), so that the transconductance instead of Eq. (5.49) is given by g
Ê J0e z1 1ˆ 1 ˜ Á kBT (1 +Wt / Wb )z 0 Ë h0 ¯ J0e z1 . kBT (1 +Wt / Wb )z 0
(5.55)
As follows from the comparison of Eqs. (5.49) and (5.55), changing Wt, in particular, from Wt = Wb to Wt = Wb/2, leads to an increase in the transconductance at the topgate voltages near the threshold of 50% (compare the g versus Vt – Vth dependences in Fig. 5.5 for Wb = Wt =10 nm and Wb =10 nm and Wt = 5 nm).
Discussion
As demonstrated above, shortening of the top gate can result in deterioration of the GBLFET characteristics. This effect is characterized by parameters h and h0, which strongly depends on the topgate length Lt. This effect gives rise to a decrease in the transconductance if Lt becomes smaller. However, in the range of large Lt the electron collisions can play a substantial role. This leads to the transconductance rolloff with increasing Lt. The effect of draininduced barrier lowering is also characterized by parameters h and h0. As follows from Section 5.4, at subthreshold, the effect of draininduced barrier lowering results in the appearance of the factor exp(eVd/2h0kBT) [see Eqs. (5.31) and (5.32)]. This factor can provide a marked increase in J and g with increasing drain voltage in GBLFETs with relatively short top gates. For example, at W = 40 nm, Lt = 40 nm, T = 300 K, and Vd = 0.25 V, this factor is about 2.37. The obtained characteristics comprise parameter b, which is proportional to the Bohr radius aB. An increase in aB when a largek substrate, say, HfO2 (aB = 20 nm) is used instead of the SiO2 substrate (aB = 4 nm), and, consequently, an increase in b leads to higher sensitivity of the barrier height to the applied voltages and, hence, to higher transconductance.
5.5.2 Effect of Electron Scattering
As shown above, the potential distributions in the main part of the gated section are fairly flat. This implies that to determine the effect of electron scattering associated with disorder and acoustic phonons one can use Eq. (5.2) with the collisional term following the approach applied in Ref. [17]. The interaction of electrons with optical phonons, particularly with optical phonons in the substrate, can be effective in the gatedrain section at elevated drain voltages. However, even relatively strong scattering on optical phonons in this section should not markedly affect the dc characteristics under consideration, although it can be essential for the ac characteristics. Considering here the case when the elastic scattering mechanisms under consideration are strong, so that they lead to an effective isotropization of the electron distribution, one can find that the values of the sourcedrain current and the transconductance obtained in the previous section for the ballistic transport should be multiplied by a collision factor C. This factor is equals to C• = 2pkBT /m/Lt v ,
89
Device Model for Graphene Bilayer FieldEffect Transistor
where v = mw/2 is the collision frequency (we put w(q) = w = const. It characterizes the fraction of the electrons injected into the gated section and those reflected back due to the collisions. To obtain the GBLFET characteristics with the topgate lengths in a wide range (to follow the transition from the ballistic electron transport to the collisiondominated transport), we use for the collision factor the following interpolation formula: C=
1 , 1 + Lt /Lscat
(5.56)
where Lscat = 2p kBT /m/v is the characteristic scattering length. Figures 5.6 and 5.7 show the dependences of the transconductance maximum (approximately at Vt = Vth) on the topgate length calculated for GBLFETs with different Wt. The scattering length is assumed to be ∞ (ballistic transport), 500 nm, and 75 nm. At T = 300 K, this corresponds to the collision frequencies v = 0, v 1.14 ¥ 1012 s–1 (the electron mobilities m 1.75 ¥ 105 cm2/V s) and v 7.6 ¥ 1012 s–1 (m 2.63 ¥ 104 cm2/V s), respectively). One can see that in the case of essential electron collisions, g versus Lt dependences exhibit pronounced maxima. This is attributed to an interplay of two effects: the shortgate effect (weakening of the barrier controllability by the Maximum transconductance, mS/mm
90
Wt = 10 nm Wb = 10 nm b = 0.05 3000 Vb = 5.0 V Vd = 0.2 V
Lscat = ∞ Lscat = 500 nm Lscat = 75 nm
2000
1000 T = 300 K 0 0
100
200 300 Topgate length, nm
400
500
Figure 5.6 Maximum transconductance g versus topgate length Lt for Wt = 10 nm.
Discussion
Maximum transconductance, mS/mm
topgate voltage when Lt decreases) and the effect of collisions, which reinforces when Lt becomes larger (which decreases the current). As follows from Figs. 5.6 and 5.7, the electron collisions can lead to a dramatic decrease in the transconductance. Wt = 5 nm
3000
Lscat = ∞ Lscat = 500 nm Lscat = 75 nm
2000
1000
0
Wb = 10 nm b = 0.05 Vb = 5.0 V Vd = 0.2 V T = 300 K 0
100
200 300 Topgate length, nm
400
500
Figure 5.7 The same as in Fig. 5.6 but for Wt = 5 nm.
5.5.3 Charge Inversion in the Gated Section At sufficiently high topgate voltages Vt < Vin when Dm > eF + Eg,, the top of the valence band in the gated section of the channel can be markedly populated by holes (inversion of the gated section charge), so that the term in the righthand side of Eq. (5.2) becomes negative. The latter inequality corresponds to the following value of the inversion voltage [see Eqs. (5.A4) and (5.A5)]: d ˆ d ˆ Ê Ê Vin = Vb Á 1 + 2b + 0 ˜ Vth Á 1 + 0 ˜ . Ë Ë W¯ W¯
(5.57)
The hole charge provides an effective screening of the transverse electric field in the gated section. This leads to weakening of the sensitivity of the barrier height and the sourcedrain current on the top gate voltage Vt [15] and, hence, to a decrease in the transconductance. This pattern is valid at the dc voltages or when the characteristic time of their variation is long in comparison with the characteristic times of the thermogeneration of holes and the
91
92
Device Model for Graphene Bilayer FieldEffect Transistor
tunneling between the channel side regions and the gated section [15, 17]. In the situation when the hole recharging of the gated section of the channel is a relatively slow process, the ac transconductance at the frequencies higher than the characteristic recharging frequency can substantially exceed the dc transconductance.
5.5.4 Interband Tunneling
At elevated topgate voltages (Vt < Vin), the interband tunneling of electrons from the conduction band in the source to the valence band in the gated section as well as from the valence band in the gated section to the conduction band in the drain can be essential. At high drain voltages the latter tunneling processes can be particularly pronounced. This can result in elevated sourcedrain current despite rather high barrier. To limit the tunneling, the backgate voltage, which mainly determines the energy gap, should be high enough. A decrease in the gate layer thicknesses also promotes the tunneling suppression. For example, if W = (5 – 10) nm, Vb = – Vt = 5 V, the energy gap in the gated section of the channel Eg 0.17 – 0.34 eV [see Eq. (5.A4)]. Despite some attempts to calculate the tunneling currents in GFETs and GBLFETs (see, for instance, Refs. [11, 19], the problem for GBLFETs remains open. This is because the spatial nonuniformity of the energy gap in the channel and its nonlinear spatial dependence (particularly near the drain edge) associated with the features of the potential distribution under the applied voltages. Generalizing Eq. (5.A4), we obtain Eg = ed[Vb–j(x)]/2W, hence the energy gap varies from Eg = Eg,s edVb /W at x = –Lt/2 to Eg = Eg,s ed(Vb – Vd/2W at x = Lt/2. It reaches a maximum Eg = d(eVb + Dm)/2W at x = xm. One can see that Eg,d can be markedly smaller than Eg, especially at not too small drain voltages. Due to this, the deliberation of the tunneling in GBLFETs requires sufficiently rigorous device model (which could include the formulas for the potential distribution obtained above) and numerical approach.
5.6 Conclusions
We demonstrated that the developed device model of allows to derive the GBLFET characteristics: the potential distributions along
Appendix
the channel and the dependences of the sourcedrain current and the transconductance on the applied voltages and the geometrical parameters as closedform analytical expressions. The key element of the model, which provides an opportunity to solve the problem analytically, is the use of the Poisson equation in the weak nonlocality approximation. In particular, the model accounts for the effect of screening of the transverse electric field by the electron charge in the channel, the shortgate effect, and the effect of draininduced barrier lowering. The parameters h0 and h characterizing the strength of these effects in the cases of essentially depleted channel and strong screening were expressed via the geometrical parameters and the Bohr radius. As shown, the GBLFET transconductance exhibits a pronounced maximum as a function of the topgate voltage swing. The interplay of the shortgate effect and the electron collisions results in a nonmonotonic dependence of the transconductance on the topgate length. The obtained analytical formulas for the potential barrier height, the sourcedrain current, and the transconductance can be used for GBLFET optimization by proper choice of the thicknesses of gate layers, the topgate length, and the bias voltages.
Acknowledgments
The authors are grateful to H. Watanabe for stimulating comments and to V. V. V’yurkov for providing Ref. [31]. The work was supported by the Japan Science and Technology Agency, CREST, Japan.
Appendix: Voltage Dependences of the Fermi Energy and the Energy Gap
Disregarding the effect of “Mexicanhat” and the nonparabolicity of the electron energy spectrum, the density of states can be considered independent of the energy (in the energy range under consideration). Taking this into account, the electron Fermi energies and the energy gaps in the source and drain sections of the GBLFET channel are, respectively, given by Refs. [17, 18] (Wb = Wt = W), È Ê beV ˆ ˘
kT e F,s = B ln Íexp Á b ˜  1 ˙ ,
(1 + b ) ÍÎ Ë kBT ¯ ˙˚
(5.A1)
93
94
Device Model for Graphene Bilayer FieldEffect Transistor
e F,d =
È Ê be(Vb Vd ) ˆ ˘ kBT ln Íexp Á ˜¯  1˙ , (1 + b) ÍÎ kBT Ë ˚˙
E g,s =
edVb , 2W
E g,s =
ed(Vb Vd ) . 2W
(5.A2) (5.A3)
Here aB = kћ2/me2, b = aB/8W, and d d0, where d0 0.34 nm [32] is the spacing between the graphene layers in the GBL, while d stands for the effective spacing accounting for the screening of the transverse electric field by GBL (polarization effect). In portion of the gated section essentially occupied by electrons and its depleted portion, one obtains Eg =
ed(Vb  Vt ) ed (V  V ) , Eg = 0 b t , 2W 2W
(5.A4)
respectively. Due to aB d, from Eqs. (5.A1)–(5.A4) one obtains eF,s ≥ eF,d > Eg,s ≥ Eg,d. At Vt < 0, Eg can significantly exceed Eg,s and Eg,d. In the case of strong degeneracy of the electron system, Eqs. (5.A1) and (5.A2) yield e F,s eVb
aB/8W b . , e F,d e(Vb Vd ) (1 + b) (1 + b)
(5.A5)
The quantity eF,d is given by the same equations in which, however, Vb is substituted by Vb – Vd. As a result, e F,s  e F,d
beVd beVd , (1 + b)
eVd* = eVd + e F,d  e F,s
eVd . 1+ b
(5.A6)
(5.A7)
Since parameter b in reality is small, so that eF,s – eF,d beVd eVd and Vd* Vd we put eF,s = eF,d = eF and substitute Vd* by Vd.
References
1. C. Berger, Z. Song, T. Li, X. Li, A. Y. Ogbazhi, R. Feng, Z. Dai, A. N. Marchenkov, E. H. Conrad, P. N. First, and W. A. de Heer, J. Phys. Chem., 108, 19912 (2004). 2. K. S. Novoselov, A. K. Geim, S. V. Morozov, D. Jiang, M. I. Katsnelson, I. V. Grigorieva, S. V. Dubonos, and A. A. Firsov, Nature, 438, 197 (2005).
References
3. A. H. Castro Neto, F. Guinea, N. M. R. Peres, K. S. Novoselov, and A. K. Geim, Rev. Mod. Phys., 81, (2009). 4. J. Bai, X. Zhong, S. Jiang, Y. Huang, and X. Duan, Nat. Nanotechnol., 5, 190 (2010).
5. V. Ryzhii, M. Ryzhii, and T. Otsuji, J. Appl. Phys., 101, 083114 (2007).
6. F. Rana, IEEE Trans. Nanotechnol., 7, 91 (2008).
7. F. Xia, T. Murleer, Y.M. Lin, A. ValdesGarsia, and P. Avouris, Nat. Nanotechnol., 4, 839 (2009).
8. V. Ryzhii, M. Ryzhii, V. Mitin, and T. Otsuji, J. Appl. Phys., 107, 054512 (2010). 9. V. Ryzhii, A. A. Dubinov, T. Otsuji, V. Mitin, and M. S. Shur, J. Appl. Phys., 107, 054505 (2010).
10. V. Ryzhii, M. Ryzhii, and T. Otsuji, Appl. Phys. Express, 1, 013001 (2008).
11. V. Ryzhii, M. Ryzhii, and T. Otsuji, Phys. Status Solidi A, 205, 1527 (2008).
12. Y. Quyang, Y. Yoon, J. K. Fodor, and J. Guo, Appl. Phys. Lett., 89 203107 (2006). 13. G. Fiore and G. Iannaccone, IEEE Electron Device Lett., 28, 760 (2007).
14. G. Liang, N. Neophytou, D. E. Nikonov, and M. S. Lundstrom, IEEE Trans. Electron Devices, 54, 677 (2007).
15. V. Ryzhii, M. Ryzhii, A. Satou, and T. Otsuji, J. Appl. Phys., 103, 094510 (2008).
16. M. Ryzhii, A. Satou, V. Ryzhii, and T. Otsuji, J. Appl. Phys., 104, 114505 (2008). 17. V. Ryzhii, M. Ryzhii, A. Satou, T. Otsuji, and N. Kirova, J. Appl. Phys., 105, 104510 (2009). 18. M. Ryzhii and V. Ryzhii, Phys. Rev. B, 79, 245311 (2009).
19. M. Cheli, G. Fiori, and G. Iannaccone, IEEE Trans. Electron Devices, 56, 2979 (2009).
20. S. O. Koswatta, S. Hasan, M. S. Lundstrom, M. P. Anantram, and D. E. Nikonov, Appl. Phys. Lett., 89, 023125 (2006). 21. M. Lenzi, P. Palestri, E. Gnani, S. Reggiani, A. Gnudi, D. Esseni, L. Selmi, and G. Baccarani, IEEE Trans. Electron Devices, 55, 2087 (2008).
22. S. Fregonese, J. Gouet, C. Manex, and T. Zimmer, IEEE Trans. Electron Devices, 56, 1184 (2009). 23. K. Natori, J. Appl. Phys., 76, 4881 (1994).
95
96
Device Model for Graphene Bilayer FieldEffect Transistor
24. A. Rahman, J. Guo, S. Datta, and M. S. Lundstrom, IEEE Trans. Electron Devices, 50, 1853 (2003). 25. F. G. Pikus and K. K. Likharev, Appl. Phys. Lett., 71, 3661 (1997).
26. V. A. Sverdlov, T. J. Walls, and K. K. Likharev, IEEE Trans. Electron Devices, 50, 1926 (2003).
27. N. Sano, Phys. Rev. Lett., 93, 246803 (2004).
28. G. Mugnaini and G. Iannaccone, IEEE Trans. Electron Devices, 52, 1802 (2005). 29. R. Kim, P. A. Neophytou, G. Klimeck, and M. S. Lundstrom, J. Vac. Sci. Technol. B, 26, 1628 (2008).
30. R. Akis, N. Faralli, D. K. Ferry, S. M. Goodnick, K. A. Phatak, and M. Saratini, IEEE Trans. Electron Devices, 56, 2935 (2009).
31. A. N. Khomyakov and V. V. V’yurkov, Russian Microelectron., 38, 393 (2009). 32. T. Ohta, A. Q. Bostwick, T. Seyller, K. Horn, and E. Rotenberg, Science, 333, 951 (2006). 33. E. McCann, Phys. Rev. B, 74, 161403 (2006).
34. E. V. Castro, K. S. Novoselov, S. V. Morozov,N. M. R. Peres, J. M. B. Lopes dos Santos, L. Nilsson, F. Guinea, A. K. Geim, and A. H. Castro Neto, J. Phys.: Condens. Matter, 22, 175503 (2010).
35. E. A. Henriksen, Z. Jiang, L.C. Tung, M. E. Schwartz, M. Takita, Y. J. Wang, P. Kim, and H. Stormer, Phys. Rev. Lett., 100, 087403 (2008).
36. M. Orlita and M. Potemski, Semicond. Sci. Technol., 25, 063001 (2010). 37. A. A. Sukhanov and Y. Y. Tkach, Sov. Phys. Semicond., 18, 797 (1984).
38. A. O. Govorov, V. M. Kowalev, and A. V. Chaplik, JETP Lett., 70, 488 (1999).
39. S. M. Sze, Physics of Semiconductor Devices (Wiley, New York, 1981).
40. M. Shur, Physics of Semiconductor Devices (PrenticeHall, New Jersey, 1990).
Chapter 6
Hydrodynamic Model for ElectronHole Plasma in Graphene*
D. Svintsov,a V. Vyurkov,a S. Yurchenko,b T. Otsuji,c,d and V. Ryzhiib,d,e aInstitute
of Physics and Technology, Russian Academy of Sciences, Moscow 117218, Russia bScientific Educational Center “Photonics and Infrared Technics,” Bauman Moscow State Technical University, Moscow 105005, Russia cResearch Institute for Electrical Communication, Tohoku University, Sendai 9808577, Japan dJapan Science and Technology Agency, CREST, Tokyo 1070075, Japan eComputational Nanoelectronics Laboratory, University of Aizu, AizuWakamatsu 9658580, Japan [email protected]
We propose a hydrodynamic model describing steadystate and dynamic electron and hole transport properties of graphene structures which accounts for the features of the electron and hole spectra. It is intended for electronhole plasma in graphene *Reprinted with permission from D. Svintsov, V. Vyurkov, S. Yurchenko, T. Otsuji, and V. Ryzhii (2012). Hydrodynamic model for electronhole plasma in graphene, J. Appl. Phys., 111, 083715. Copyright © 2012 American Institute of Physics. GrapheneBased Terahertz Electronics and Plasmonics: Detector and Emitter Concepts Edited by Vladimir Mitin, Taiichi Otsuji, and Victor Ryzhii
Copyright © 2021 Jenny Stanford Publishing Pte. Ltd.
ISBN 9789814800754 (Hardcover), 9780429328398 (eBook)
www.jennystanford.com
98
Hydrodynamic Model for ElectronHole Plasma in Graphene
characterized by high rate of intercarrier scattering compared to external scattering (on phonons and impurities), i.e., for intrinsic or optically pumped (bipolar plasma), and gated graphene (virtually monopolar plasma). We demonstrate that the effect of strong interaction of electrons and holes on their transport can be treated as a viscous friction between the electron and hole components. We apply the developed model for the calculations of the graphene dc conductivity; in particular, the effect of mutual drag of electrons and holes is described. The spectra and damping of collective excitations in graphene in the bipolar and monopolar limits are found. It is shown that at high gate voltages and, hence, at high electron and low hole densities (or viceversa), the excitations are associated with the selfconsistent electric field and the hydrodynamic pressure (plasma waves). In intrinsic and optically pumped graphene, the waves constitute quasineutral perturbations of the electron and hole densities (electronhole sound waves) with the velocity being dependent only on the fundamental graphene constants.
6.1 Introduction
The hydrodynamic approach is quite reasonable for the description of dense electronhole plasma in semiconductor systems in which the electronelectron, electronhole, and holehole collisions dominate over the collisions of electrons and holes with disorder. In particular, such a situation can occur in intrinsic graphene at the room temperature, particularly, in the structures with low or moderate permittivity of the layers between which the graphene layer is clad, when the characteristic intercarrier collision frequency can reach high values. As a result, this frequency can be much greater than that of collisions with impurities or phonons. Similar situation occurs in the gated graphene at sufficiently high gate voltages when large electron or hole densities can be induced as well as at strong optical pumping of graphene. The hydrodynamic models of the electronhole systems in different structures and devices based on the standard semiconductors with parabolic and nearparabolic energy spectra of electrons and holes are widely used (see, for instance, Ref. [1]). However, in case of graphene, such models and the pertinent equations should be revised due to the linear energy spectra of
Derivation of Hydrodynamic Equations
electrons and holes. A hydrodynamic approach was recently used to describe the stationary transport processes in graphene [2]. However, the role of a strong electronhole scattering, which, as shown in our work, is crucial, was not addressed. In this chapter, we develop a strict hydrodynamic model for electronhole plasma in graphene and demonstrate its workability in some applications. The chapter is organized as follows. In Section 6.2, we derive the hydrodynamic equations (continuity equations, Euler equations, and energy transfer equations) for graphene from the Boltzmann–Vlasov kinetic equations for massless electrons and holes assuming high carriercarrier collision frequencies. Section 6.3 deals with the application of the derived equations for the calculations of graphene dc conductivity taking into account the effect of electronhole drag. In Section 6.4, the collective excitations in graphene at different conditions are considered using the obtained hydrodynamic equations. In particular, we show that two types of weakly damping excitations can exist in the electronhole plasma: (1) electron (or hole) plasma waves in gated graphene in the state with the Fermi level far from the Dirac point and (2) quasineutral electronhole sound waves in the bipolar electronhole plasma. The damping of both plasma waves (in virtually monopolar plasma) and electronhole sound waves (in bipolar plasma) is determined by the scattering on disorder, while the electronhole scattering almost does not affect the damping. In contrast, the plasma waves in bipolar electronhole systems exhibit a strong damping due to electronhole scattering processes. In Section 6.5, we draw the main conclusions. Some cumbersome formulas are singled out to the Appendix.
6.2 Derivation of Hydrodynamic Equations
For the massless electrons in holes in graphene the spectrum is linear e(p) = uFp. Hence, the kinetic equations governing the distribution functions fe = fe(p) and fh = fh(p) read, respectively, ∂f e p ∂f e ∂j ∂ f
+ u F + e
p ∂r ∂r ∂ p ∂t = St { fe , fe } + St { fe , f h } + St i { fe },
(6.1)
99
100
Hydrodynamic Model for ElectronHole Plasma in Graphene
∂fh p ∂fh ∂j ∂f + uF e ∂t p ∂r ∂r ∂p = St{ f h , f h } + St{ f h , fe } + St i { f h }.
(6.2)
Here uFp/p = ∂e(p)/∂p is the electron (hole) velocity, uF ≃ 108 cm/s is the characteristic velocity of electrons and holes in graphene (Fermi velocity), e = e is the absolute value of the electron charge, E = –∂j/∂r is the electric field, Sti{fe} and Sti{fh} are the collision integrals of electrons and holes, respectively, with disorder (impurities and phonons); St{fe, fe}, St{fh, fh}, and St{fe, fh} are the intercarrier collision integrals. In Eqs. (6.1) and (6.2) we have neglected the recombination terms assuming that the recombination rate is much smaller than that of collisions and the frequency of the plasma waves under consideration. As known [3], the Fermi distribution functions of electrons and holes È Ê e( p)  p ◊ Ve  me ˆ ˘ fe (p ) = Í1 + exp Á ˜¯ ˙ Ë T Î ˚
1
È Ê e( p)  p ◊ Vh  mh ˆ ˘ fh (p ) = Í1 + exp Á ˜¯ ˙ Ë T Î ˚
,
(6.3)
,
(6.4)
1
turn the electronelectron and holehole collision integrals to zero owing to the conservation of momentum and energy in the intercarrier collisions. In Eqs. (6.3) and (6.4) Ve and Vh are the average (drift) velocities of electrons and holes, respectively, me and mh are electron and hole chemical potentials, and the temperature T is measured in energy units. Hereafter we consider rather small drift velocities and perform an expansion of Eqs. (6.3) and (6.4) over Ve and Vh: fe (p ) = fe,0 
fe (p ) = fh,0 
∂fe,0 ∂e
∂fh,0 ∂e
p ◊ Ve ,
p ◊ Vh .
(6.5)
(6.6)
Here fe,0 and fh,0 stand for the functions, given by Eqs. (6.3) and (6.4), with Ve = Vh = 0. The distribution functions (6.5) and (6.6) still turn
Derivation of Hydrodynamic Equations
the electronelectron and holehole collision integrals to zero and, at the same moment, conserve the number of particles (the density is the same in moving and stationary frames). If the electric field is sufficiently weak and the inhomogenity of the electronhole plasma is small (as it will be assumed in the following), the electronhole collision integrals can be expanded over Ve and Vh and presented as St{fe, fh} = –St{fh, fe} ≃ (Vh – Ve) ◊ S{fe,0, fh,0} (for details see the Appendix). In this form, the electronhole collision terms describe the friction between the electron and hole plasma components. Similarly, the terms corresponding to the collisions of electrons and holes with disorder can be presented in the forms Sti{fe} = –Ve ◊ Si{fe,0} and Sti{fh} = –Vh ◊ Si{fh,0}. Here S and Si are the functionals of the distribution functions fe,0 and fh,0. At small values of electron and hole average velocities Ve and Vh, the friction terms can be considered as perturbations in comparison with the electronelectron and holehole collision terms. Thus the distribution functions given by Eqs. (6.3) and (6.4) are the approximate solutions of Eqs. (6.1) and (6.2). Then the quantities Ve, Vh, me, and mh (or the electron and hole sheet densities, Se and Sh) can be found considering the terms in the lefthand sides of Eqs. (6.1) and (6.2) and the friction terms as perturbations, using the standard procedure (akin to the Chapman–Enskog method [4] for the derivation of the hydrodynamic equations from the kinetic equations). On integrating Eqs. (6.1) and (6.2) over dGp = gd2p/(2pℏ)2 (where g = 4 is the electron degeneracy factor in graphene), we obtain the continuity equations for electrons and holes
∂S e ∂S e Ve + = 0, ∂t ∂r
∂S h ∂S h Vh + = 0. ∂t ∂r
(6.7)
To derive the Euler equations, one should integrate Eqs. (6.1) and (6.2) times p over dGp. In the case of parabolic dispersion, one could multiply the Boltzmann equation either by velocity or momentum as they are proportional to each other. For linear dispersion the choice of momentum is crucial. Just the momentum is conserved in particleparticle collisions unlike to the velocity which can be changed. After integration one obtains the system of Euler equations for electrons and holes:
101
102
Hydrodynamic Model for ElectronHole Plasma in Graphene
3 ∂ pe Ve ∂ uF pe ∂j +  eS e ∂r 2 ∂r 2 ∂t uF = be Ve  beh ( Ve  Vh ), 3 ∂ ph Vh ∂ uF ph ∂j + + eS h 2 ∂t uF ∂r 2 ∂r = bh Vh  beh ( Vh  Ve ).
(6.8) (6.9)
Here the angle brackets denote an integration over the equilibrium Fermi distribution functions, in particular, pe =
Ú
Ê uF p  me ˆ ˘ Í1 + exp Á ˙ ¯˜ ˚ Ë T Î
•È
0
1
2p gp2dp (2p)2
is the momentum modulus per unit area, the friction coefficients beh, be, and bh are the functions of the nonperturbed (steadystate) values of the chemical potentials me,0 and mh,0. One can rewrite Euler equations in a classical form on introducing the fictitious carrier masses Me =
pe
uF S e
, Mh =
ph
uF S h
,
which are estimated as 0.016 of the free electron mass at me = mh = 0 and T = 300 K. The detailed derivation of the friction coefficients can be found in the Appendix; here, we write down only the final expressions in several limits. The electronhole friction coefficient beh can be represented as beh = A
T 4e 4
5uF6 k 2
Êm m ˆ ◊IÁ e , h ˜ . ËT T ¯
(6.10)
where k is the effective permittivity of environment (the substrate and gate dielectric), the dimensionless constant A of the order of unity and the function I (me/T, mh/T) can be obtained after proper linearization of the electronhole collision integral (see the Appendix). For intrinsic graphene I (0, 0) = 1, while for monopolar plasma in gated graphene I (m/T, m/T) µ e–m/T due to the exponentially small number of holes. In the current chapter, we shall adopt the
Derivation of Hydrodynamic Equations
following interpolation for beh which is valid in the limiting cases of monopolar plasma and intrinsic graphene: beh =
veh pe ph S M S M = veh e e h h . uF pe + ph S e Me + S h M h
(6.11)
Here we have introduced the electronhole collision frequency neh to be estimated below in the Section 6.3. When the acoustic phonon scattering dominates, the coefficients be and bh can be presented as [5, 7] be =
D2T pe2
4r s2 3uF2
, bh =
D2T ph2
4rs2 3uF2
,
where D is the deformation potential constant, r is the sheet density of graphene, and s is the sound velocity. Due to the existence of several acoustic phonon branches and considerable discrepancy in experimental data of graphene constants [5–7], it is reasonable to use semiphenomenological formulas: be = lT pe2 , bh = lT ph2 ,
(6.12)
and extract the numerical value of λ from experimental data on dc conductivity (see Section 6.3). For scattering on charged impurities, the friction coefficients be and bh are reasonably proportional to the carrier densities and the density of charged impurities Si be µ SeSi,
bh µ ShSi.
(6.13)
In general, the density of charged impurities depends on the chemical potentials and temperature. At last, the system of hydrodynamic equations should be supplemented with the energy transfer equations. Introducing the energy density ·ee,hÒ = uF·pe,hÒ, the pertinent equations can be written down as ∂ ee ∂t
∂ eh ∂t
+
3 ∂ e e Ve ∂j = Qe ,  e Âe Ve 2 ∂r ∂r
+
∂j 3 ∂ e h Vh + e Â h Vh = Qh , 2 ∂r ∂r
(6.14)
(6.15)
103
104
Hydrodynamic Model for ElectronHole Plasma in Graphene
where the heat sink rates Qe and Qh are proportional to the difference between electron and phonon temperatures. However, in the present chapter we neglect the heating as we deal with lowfield dc conductivity and highfrequency plasma waves.
6.3 Effect of ElectronHole Drag and DC Conductivity of Gated Graphene
As one of the demonstrations of the hydrodynamic equations applications we calculate the dc conductivity of gated graphene. It is assumed that the electric potential and the charge density are related by the Poisson equation. In the gradual channel approximation [8] C(VG − j) = e(Se − Sh).
(6.16)
Here C = k/4pd is the specific capacitance per unit area, d and k are the thickness and permittivity of the gate dielectric, respectively, and VG is the gate voltage. To calculate the dc conductivity we rewrite the Euler equations for the steadystate situation in terms of electrochemical potentials: Se
∂( me  ej ) = be Ve  beh ( Ve  Vh ), ∂r
Sh
∂(ej  mh ) = bh Vh  beh ( Vh  Ve ), ∂r
(6.17)
(6.18)
where the derivative of electric potential is associated with drift current, as well as the derivative of chemical potential is associated with diffusion current. In the following we restrict our calculations by the consideration of the drift current only and, therefore, omit the terms ∂me,h/∂r in Eqs. (6.17) and (6.18). As a result, we arrive at the following expressions for the mean (drift) velocities of electrons and holes: È (S  S h )beh + bh S e ˘ ∂j , Ve =  Í e ˙ Î beh (be + bh ) + be bh ˚ ∂r È (S  S e )beh + be S h ˘ ∂j . Vh = Í h ˙ Î beh (be + bh ) + be bh ˚ ∂r
(6.19)
(6.20)
Effect of ElectronHole Drag and DC Conductivity of Gated Graphene
Substituting the quantities Ve and Vh from Eqs. (6.19) and (6.21) into the general expression for current density j = e(ShVh – SeVe) = G(–∂j/∂r), one obtains the following formula for the conductivity G: G=
e2 (S e  S h )2 e2 ( S 2e bh + S 2h be ) + . be + bh + be bh / beh beh (be + bh ) + be bh
(6.21)
The first term in the righthand side of Eq. (6.21) is associated with the scattering of electrons and holes on impurities and phonons. This term turns into zero at the Dirac point. However, far from the Dirac point, i.e., in purely electron or hole plasma, this term dominates. Meanwhile, the second term is due to the contribution of the electronhole friction. The latter results in a high resistivity of graphene at the Dirac point and its vicinity. To calculate the graphene minimal conductivity, we reasonably assume that at the Dirac point scattering between electrons and holes prevails: be ≪ beh, bh ≪ beh. Plugging Eq. (6.10) for beh into Eq. (6.21) one obtains an expression for intrinsic graphene conductivity G0 =
e2 S 02 uF2k 2 . µ beh e2
(6.22)
Strikingly, the intrinsic graphene conductivity (minimum conductivity) does not depend on temperature. This is in agreement with the experimental results [9] demonstrating a constant conductivity over a broad range of temperature from 0.3 to 300 K in which the carrier density varies by 6 orders of magnitude. Worth mentioning the Eq. (6.22) was previously obtained using the scaling theory, [10], and also via thorough description of electronhole scattering [11]. Earlier, the minimum conductivity of graphene was calculated under the assumption of strong interaction among carriers [12–14]. The strength of interaction is governed by the “finestructure constant”a = e2/kℏuF which is equal to 2.2 for intrinsic (suspended) graphene (k = 1). The stronginteraction theories bind the conductivity of graphene to the conductance quantum e2/h, regardless of the permittivity of environment. As the parameter a is about unity, both theories of weak and strong interaction give rise to close values of conductivity. However, in prospective graphene structures the screening caused by dielectrics and nearby gates
105
106
Hydrodynamic Model for ElectronHole Plasma in Graphene
make the value of a less than unity, therefore, the weakinteraction theories become more adequate to the situation. After substituting Eq. (6.11) for beh into Eq. (6.22) one can rewrite that equation in the conventional form appropriate for the estimation of the electronhole collision frequency neh:
G0 =
2S 0e2 , M0n eh
(6.23)
where M0 is the fictitious mass of electrons and holes in intrinsic graphene dependent on temperature. Comparing G0 given by Eq. (6.23) with the experimental value G0 ≃ (6 kΩ)–1, one can estimate the electronhole collision frequency as neh = 3 ¥ 1013 s–1. Such a high value justifies an employment of the hydrodynamic model. In the monopolar limit (Se ≫ Sh), the expression for the conductivity could be also simplified: G=
e2 S 2e . be
(6.24)
Equation (6.24) allows to estimate the coefficient l in the phonon collision term given by Eq. (6.12). It is widely assumed that in suspended graphene samples or twisted graphene stacks the conductivity and mobility are limited by phonon scattering only. For instance [16], the carrier mobility B, defined as B=
G , e Se  Sh
reaches the value of 120,000 cm2 V–1 s–1 at Se – Sh = 2 ¥ 1011 cm–2 and the temperature T = 240 K (when the chemical potential m ≃ 0.028 eV). Hence, in the monopolar limit, one obtains B
eS e e = . be S e lT pe2
(6.25)
Equation (6.25) yields l ≃ 2.4 ¥ 1054 cm s–1J–2. Accordingly, the characteristic collision frequency ne = 2uFbe/3·peÒ at room temperature varies from 8.6 ¥ 1011 s–1 at the Dirac point to 3.5 ¥ 1012 s–1 at VG = 10 V and d = 10 nm. Figure 6.1 demonstrates the dependence of the lowfield dc conductivity G of graphene on the gate voltage VG, plotted using Eqs.
Effect of ElectronHole Drag and DC Conductivity of Gated Graphene
(6.11), (6.12), and (6.21). The voltage dependence of the graphene resistivity and the dependence of the carrier mobility on the chemical potential m [given by Eq. (6.25)] are shown in the insets in Fig. 6.1. In the case when scattering on acoustic phonons dominates, the conductivity tends to saturation at high gate voltages and the phononlimited mobility decreases. To describe the conductivity of realistic graphene structures, one should account for other scattering objects: charged impurities, interfacial phonons, bulk phonons, etc. For example, scattering on charged impurities results in the following trends of conductivity curves in monopolar case: G(VG) µ VG if the density of impurities is constant and G(VG) µ VG if the distribution of impurity levels is uniform in an energy scale [10]. The latter fact manifests a decrease in defect scattering at low temperatures.
Figure 6.1 Conductivity of graphene G vs. gate voltage at T = 300 K, d = 10 nm, and k = 4. Insets: left panel—resistivity G–1 near the Dirac point vs. gate voltage, right panel—mobility B vs. chemical potential.
The conductivity and mobility curves in Fig. 6.1 exhibit a good agreement with the experimental works, where phononlimited mobility was investigated [16–18]. As for the theoretical approaches to the description of graphene conductivity, significant efforts have been focused on the calculation of the minimum conductivity and the conductivity far from the neutrality point [5, 7, 19]. The conductivity
107
108
Hydrodynamic Model for ElectronHole Plasma in Graphene
at an arbitrary value of carrier density was considered in Refs. [14, 15] without specifying the mechanism of scattering. Our model provides an opportunity to calculate the transport characteristics of graphene at any charge carrier density taking into account the definite scattering processes. Above all, we show that the effect of electronhole drag significantly impacts the transport properties of graphene and leads to an abrupt drop of graphene resistivity outside of the Dirac point. It is remarkable that the drag effect is crucial even at a small mismatch in the electron and hole densities [10]. The conductivity in the regime of drag almost does not depend on electronhole scattering, although it still remains the strongest one in the system. Indeed, the phonon (impurity) scattering term in the expression for conductivity (6.21) dominates under the condition Sh  Se Se
>
bh beh
.
(6.26)
m =0
For the preceding estimations, the ratio given by Eq. (6.26) is evaluated as 0.3 at room temperature. Providing Eq. (6.26) is satisfied, the difference between electron and hole velocities [Eq. (6.19)] becomes rather small: Vh  Ve
Vh + Ve
1 bh 2 beh
.
m =0
(6.27)
The difference between velocities still exists because of the opposite charges of electrons and holes and, therefore, the opposite directions of the electric forces. In principle, for the drag regime the twofluid description of graphene system might be reduced to a single electronhole fluid with renormalized charge of particles according to Eq. (6.26). However, it seems preferable to retain twofluid model to cover all possible situations. It is readily seen from above mentioned that a narrow resistivity peak in Fig. 6.1 could be explained by the drag effect. Moreover, stronger scattering leads to a wider resistivity peak. The latter is in concordance with the experimental data [17].
Plasma and ElectronHole Sound Waves in Graphene
6.4 Plasma and ElectronHole Sound Waves in Graphene 6.4.1 General Dispersion Relation for Collective Excitations Below we demonstratethe applicationofthe hydrodynamic equations for the calculation of the spectra of collective excitations in electronhole system. We use the same gradual channel approximation as in the previous section [Eq. (6.16)]. To derive the spectra, one can apply the common technique of smallsignal analysis assuming that me = me,0 + dme ei( kx wt ) ,
dVe = dVe,0ei( kx wtt ) ,
mh = mh,0 + dmh ei( kx wt ) ,
dVh = dVh,0ei(kx wt ) ,
j = j0 + djei( kx wt ) , where dme, dmh, dVe,0, dVh,0, and dj are the amplitudes of alternating variations. The nonperturbed chemical potentials me,0 and mh,0 coincide if the steady state is an equilibrium one and are determined by the doping and the gate potential. In particular, at VG = 0 and zero doping the Fermi level is located in the Dirac point. In intrinsic graphene under optical interband pumping the chemical potentials of electrons and holes can be rather different. For example, at VG = 0, me,0 = m0 > 0, and mh = –m0 < 0, where m0 is determined by the intensity of pumping. From the linearized versions of Eqs. (6.7–6.9) as well as Eq. (6.16) the following system of algebraic equations arises: ˘ È 2 2Ê 2ˆ Íiw 3 pe + ik S e Á uF + e ˜ + b + b ˙ dV e eh ˙ e Í C˜ w Á pe 1 2 uF Ë ¯ ÍÎ ˙˚ È ik 2 S e S h e2 ˘ + beh ˙ dVh = 0, Í C ÎÍ w ˚˙
(6.28)
109
110
Hydrodynamic Model for ElectronHole Plasma in Graphene
È ˘ 2 2 Ê 2ˆ Íiw 3 ph + ik S h Á uF + e ˜ + b + b ˙ dV h eh ˙ h Í 2 uF w Á ph 1 C˜ ¯ Ë ÎÍ ˚˙ ˘ È ik 2 S e S h e2 + beh ˙ dVh = 0. Í C ÍÎ w ˚˙
(6.29)
The solvability condition for Eqs. (6.28) and (6.29) results in the general dispersion relation for the collective excitations: È 2beh ik 2ue2 (1 + re ) + ve + uF Íiw + w 3 pe ÍÎ
˘ ˙ ˙˚
È 2beh ik 2uh2 (1 + rh ) + vh + uF Íiw + w 3 ph ÍÎ
˘ ˙ ˙˚
È ik 2ue2 S h b u ˘ È ik 2uh2 S e b u ˘ =Í re + eh F ˙ Í rh + eh F ˙ . ph ˚˙ pe ˙˚ ÍÎ wS h ÍÎ wS e
(6.30)
Here for brevity we have introduced the dimensionless constants re =
e2 pe1 CuF
, rh =
the squared characteristic velocities ue2 =
2S 2euF2
3 pe
and the frequencies
ne =
pe1
, uh2 =
e2 ph1 CuF
,
2S 2huF2 3 ph ph1
,
2uF be 2u b , nh = F h , 3 ph 3 pe
The quantities re and rh determine the ratio of the electrostatic energy to the kinetic energy in the wave. In the particular gated structures we have considered above (k = 4, d = 10 nm) the dimensionless constant re varies from 1.9 at VG = 0 to 45 at VG = 10 V. The electronphonon collision frequencies ne and nh, as shown below, determine the damping of the waves.
Plasma and ElectronHole Sound Waves in Graphene
6.4.2 Analytical Solutions for Symmetric Bipolar and Monopolar Systems Exact solutions of the general dispersion equation (6.30) can be acquired for symmetric bipolar plasma (optically pumped or intrinsic graphene) and monopolar plasma. In symmetric bipolar plasma all quantities characterizing the electron and hole systems coincide (e.g., ue = uh = u, Se = S– = S, ...), therefore, we shall omit the subscripts in this certain case. In symmetric systems Eq. (6.30) provides two solutions: 2
w  = i
n Ênˆ + k 2u 2  Á ˜ , Ë 2¯ 2
2
n ˆ Ên n ˆ 2 Ên w + = i Á + eh ˜ + k 2u 2 (1 + 2r )  Á + eh ˜ . Ë 2 3 ¯ Ë2 3 ¯
(6.31)
(6.32)
The second solution w+ represents the waves with opposite motion of electrons and holes leading to the strong damping. These waves correspond to the perturbations of charge density (plasma waves). The branch given by Eq. (6.31) is of the most interest. Electrons and holes in these waves move in the same direction, i.e., the electronhole plasma remains quasineutral. Due to the codirectional motion of the electron and hole components, their mutual collisions do not affect the wave damping. In the case, it originates from the collisions of electrons and holes with impurities and phonons. We can conclude that those waves are associated solely with the pressure gradient. In the following, such waves will be referred to as electronhole sound waves in analogy with electronion sound waves in classical plasma. The velocity of electronhole sound is s = u = uF
2S 2
3 p p1
.
(6.33)
It does not depend on structure parameters and does not exceed the Fermi velocity for any electron and hole densities. If the Fermi level crosses the Dirac point the analytical expression for velocity is s = uF
p2
18 ln 2z (3)
0.6uF ,
where z(x) stands for Riemann zeta function.
111
112
Hydrodynamic Model for ElectronHole Plasma in Graphene
The dispersion laws for monopolar plasma can be derived providing the inequalities Se ≫ Sh, be ≫ bh, and re ≫ 1 ≫ rh are satisfied: 2
w + = i
ne Ên ˆ + k 2ue2 (1 + re )  Á e ˜ , Ë 2¯ 2
(6.34)
2
n ˆ n ˆ Ên Ên w  = i Á h + eh ˜ + k 2uh2 (1 + 2rh )2  Á h + eh ˜ . Ë 2 Ë 2 3 ¯ 3 ¯
(6.35)
A detailed analysis of these solutions shows that the branches w+ and w– correspond to the oscillations of majority (electrons) and minority (holes) carriers, respectively. The minority carrier oscillations are strongly damped by electronhole friction and, therefore, they are omitted in the further consideration. The wave velocity of the electronic plasma oscillations s+ is s+ = ue (1 + re )
1/ 2
uF 4akF d µVG1/4d 1/4 ,
(6.36)
where a = e2/kℏuF is the coupling constant (“finestructure constant”) and kF = me/ℏuF is the Fermi momentum of electrons. This velocity markedly exceeds the Fermi one and is primarily determined by the Coulomb interaction of carriers with the gate.
Figure 6.2 Dispersion of plasma and electronhole sound waves at different gate voltages. Inset: nonlinear dispersion of the waves at small frequencies resulting from collisions.
The dispersions for electronhole sound in intrinsic graphene and plasma waves in gated graphene at high gate voltages are
Plasma and ElectronHole Sound Waves in Graphene
depicted in Fig. 6.2 in the THz range of frequencies. The curves are calculated under the assumption of equal chemical potentials me,0 = mh,0, i.e., when the nonperturbed state is an equilibrium one. The spectra exhibit nonlinear dispersion at low frequencies originating from the damping (see the inset in Fig. 6.2). Worth mentioning the dispersions are also nonlinear at short wavelengths (kd ~ 1) when the gradual channel approximation becomes inapplicable. However, this limitation can be overcome if we use the rigorous solution of Poisson equation [21] instead of Eq. (6.16). For the considered gated structure the transition to the rigorous solution can be performed by the substitution: CÆ
2k k
4p (1  e 2kd )
.
(6.37)
Equation (6.37) restrains the unlimited growth of the plasma wave velocities for large distances d between graphene sheet and metal gate.
6.4.3 Velocities and Damping Rates of the Waves
The wave velocities and damping rates can be calculated analytically in the linear domain of spectra, i.e., at (ve,h < w < s/d) at an arbitrary value of electron and hole densities. Assuming w = sk, where s is the wave velocity, and plugging this into Eq. (6.30), one obtains two solutions s– and s+:
Figure 6.3 Velocities of plasma waves vs. gate voltage calculated for different gate layer thicknesses [Eq. (6.36)]. Dashdotted line corresponds to the electronhole sound velocity in the vicinity of the neutrality point. Regions of strong damping are filled.
113
114
Hydrodynamic Model for ElectronHole Plasma in Graphene
1
s±2 = ÎÈue2 (1 + re ) + uh2 (1 + rh )˘˚ 2
±
2
1 È 2 2 ˘ + 4ue2uh2re rh , (6.38) u (1 + r ) u (1 + r ) e e h h ˚ 2 Î
consistent with Eqs. (6.33) and (6.36).
Figure 6.4 Damping rates for the two branches of spectrum: w+ (a, top) and w– (b, bottom).
In the vicinity of Dirac point the waves with the lower velocity s– correspond to the electronhole sound, while in the monopolar plasma they turn into the oscillations of minority carriers. The waves with the higher velocity s+ behave as plasma waves at any electron
Plasma and ElectronHole Sound Waves in Graphene
and hole densities. The solutions given by Eq. (6.38) are plotted in Fig. 6.3 as the functions of gate voltage with the assumption of equal steadystate chemical potentials (me,0 = mh,0). One can readily see that the velocity s– almost does not depend on the gate voltage applied, while the velocity s+ exhibits unlimited growth at high gate voltages s+µ VG1/4.. To calculate the damping rates of the waves we assume w± = s± k + ig±, where g± characterizes the damping rate of the waves. The obtained damping rates g± vs. the gate voltage are demonstrated in Fig. 6.4. It is clearly seen that in symmetric bipolar plasma the electronhole sound branch w– exhibits weak damping. In the monopolar case (Se ≫ Sh) the plasma wave, corresponding to the oscillations of the majority carriers, is weakly damped. The minimum damping rate for the waves considered is of the order of 5 ¥ 1011 s–1 and is determined by electronphonon (or holephonon) collision frequency if the only scattering mechanism is acoustic phonon scattering. At high gate voltages the damping coefficient g+ grows linearly in accordance with the expression for characteristic collision frequency ne. The maximum damping rate of the waves is of the order of electronhole collision frequency neh. In accordance with these calculations, the regions of strong damping in Fig. 6.3 are marked with filling.
6.4.4 Comparison with Other Models
Plasma waves in gated graphene were discussed in Refs. [20, 21] using the kinetic approach under assumption of collisionless transport. As expected, formally setting the collision frequency zero in Eq. (6.34), we obtain the spectrum of plasma waves, derived previously [21]. Meanwhile, in the kinetic approach the existence of the electronhole sound could not be predicted as it was assumed that the wave velocity should overcome Fermi velocity. The dispersion curves of the plasma waves obtained via the hydrodynamic and kinetic theories are compared in Fig. 6.5 for the same parameters of the gated structure (k = 4, d =10 nm), gate voltage VG = 10 V, and three different collision frequencies. The only difference between the curves is in the nonlinear part of spectra originating from collisions.
115
116
Hydrodynamic Model for ElectronHole Plasma in Graphene
Figure 6.5 Comparison of dispersions for plasma waves, calculated using kinetic model [21] (disregarding collisions with impurities and phonons, solid line) and hydrodynamic model for Vg = 10 V, d = 10 nm, k = 4, and three different collision frequencies.
Plasmons in graphene were also intensively studied within the analysis of the polarizability function ∏(q, w) in randomphase approximation [22–24]. In particular, the squareroot w µ k and linear w µ k dispersions were obtained for the nongated and gated graphene, consequently. To obtain the plasma wave dispersion for the nongated graphene in hydrodynamic model we tend d to infinity in Eq. (6.37) and plug it into Eq. (6.34). Thus, plasma waves in nongated graphene at high electron densities exhibit the following dispersion: 2
w+ =
n uF2k 2 Ên ˆ (1 + 4akF )  Á e ˜  i e . Ë 2¯ 2 2
In the low frequency limit the above equation is simplified w + uF 2a kkF ,
(6.39)
(6.40)
and the result quantitatively coincides with that predicted in Ref. [24]. What concerns the result obtained in Ref. [22] for plasmons in gated graphene, it coincides both with that obtained within kinetic approach [21] and, hence, with our result (6.34). The transition from almost linear to squareroot plasma wave dispersion at different gate dielectric thicknesses is shown in
Discussion of the Results
Fig. 6.6 for the given value of electron density Se = 5 ¥ 1012 cm–2. In the shortwave limit kd ≫ 1 (providing the applicability of the hydrodynamic model) the dispersion of plasma waves is linear again with the velocity depending only on the fundamental constants of graphene. Worth mentioning that the electronhole sound waves are insensitive to the gate and exhibit almost linear dispersion at any gated structure parameters.
Figure 6.6 Dispersions of plasma waves at a given carrier density Se = 5 ¥ 1012 cm–2 and different thicknesses of gate dielectric.
6.5 Discussion of the Results The hydrodynamic model of electron and hole transport in graphene which takes into account the linearity of carrier spectra has been developed. Strong interactions between electrons and holes result in mutual frictional forces proportional to the mismatch in electron and hole drift velocities. The interaction of carriers with acoustic phonons and impurities is also governed by a friction term in Euler equations. The estimated electronhole collision rate is greater than that between carriers and phonons (impurities) at room temperature. The model has been applied to the solution of two challenging problems: dc graphene conductivity and spectra and damping of the collective excitations in graphene structures.
117
118
Hydrodynamic Model for ElectronHole Plasma in Graphene
The hydrodynamic equations derived provide an opportunity to calculate the conductivity of graphene sheet in a wide range of gate voltages including the Dirac point, where the influence of electronhole collisions on the charge transport is dominant. However, when there is even a small difference (proportional to the ratio of external scattering rate to that of carriercarrier) between electron and hole densities the majority carriers drag the minority ones. In this case, the conductivity is governed by scattering on phonons and impurities. The effect of drag is particularly pronounced in highpurity (suspended) graphene samples. The spectra of collective excitations in electronhole system in graphene have been calculated. The existence of two types of the excitations has been revealed: quasineutral electronhole sound waves and plasma waves. In the vicinity of the Dirac point or in the optically pumped intrinsic graphene the sound waves undergo weak damping of the order of 5 ¥ 1011 s–1 in perfect structures. The damping of such waves is caused by weak scattering on acoustic phonons and is insensitive to strong electronhole scattering. The latter fact is due to codirectional motion of electrons and holes in quasineutral sound waves, which almost eliminates electronhole friction. The quasineutral electronhole sound waves under consideration are akin to those in bipolar electronhole plasma in semimetals considered by Konstantinov and Perel a long time ago [25]. Later such waves were studied in semiconductors [26], twoband metals [27], and superconducting compounds [28]. Recently the acoustic plasma waves were studied in two dimensional semimetals [30] (CdHgTe/HgTe/CdHgTe quantum wells). It was shown that those waves can contribute to the thermodynamic properties of the materials, e.g., carrier relaxation rates in bulk semiconductors [29] and critical temperatures of superconducting compounds [28]. In graphene such waves could be feasibly excited by optical spots or modulated optical radiation. In both situations quasineutral non uniform distributions of electrons and holes arise. The propagation of plasma waves in symmetric electronhole systems is strongly suppressed by electronhole collisions. Strong damping of such waves can significantly decrease the rate of electronhole recombination via plasmon emission, discussed in Ref.
Appendix
[31]. In its turn, the recombination via the emission of electronhole sound waves is prohibited as their velocity is smaller than uF [Eq. (6.38)]. In sufficiently monopolar systems (electron or hole plasma, e.g., in gated graphene at high gate voltages) the damping of plasma waves, corresponding to the oscillations of majority carriers, is associated solely with the scattering on disorder (phonons and impurities). It can be rather weak in perfect structures, particularly at low temperatures. The dispersion of plasma waves in gated graphene structures is linear in a wide range of frequencies [32]. The dependence of the plasma wave velocity on the gated structure parameters is quantitatively similar to that obtained for the twodimensional electron gas of massive electrons [33]. The hydrodynamic and kinetic models yield the same dispersions of plasma waves if one formally tends the collision frequency to zero. However, the hydrodynamic approach provides a regular way to describe the damping of the waves, associated with carrier scattering. In conclusion, the hydrodynamic equations for bipolar graphene system were derived and applied for calculation of dc conductivity and spectra of collective excitations in graphene structures. The model opens the prospects to the simulation of graphenebased transistors, THzrange detectors and generators, and light emitting devices.
Acknowledgment
The research was supported via the grants 110700464a of the Russian Foundation for Basic Research, F793/805 of Computer Company NIX ([email protected]), and by the Japan Science and Technology Agency, CREST, Japan.
Appendix A: Dissipative Terms in the Euler Equations
In this appendix we derive explicit expression for the friction forces, associated with carriercarrier, carrierimpurity, and carrierphonon scattering.
119
120
Hydrodynamic Model for ElectronHole Plasma in Graphene
A.1 Mutual ElectronHole Friction To derive the expression for electronhole friction force one should linearize the collision integral
Ú
St{ fe , f h } = 4 W (q){ fe (p  q ) fh (p1 + q )[1  fe (p)]
[1  f h (p1 )]  fe (p) fh (p1 )[1  fe (p  q )] [1  fh (p1 + q )]}
d 2p1d 2q (2p )4
(6.A1)
,
where the nonequilibrium distribution functions for electrons and holes are determined via Eqs. (6.3) and (6.4), the factor of 4 arises from 2 possible spins and valleys for particle p1. W(q) is the Coulomb scattering probability which can be written down as 2
2 È 2pe2 ˘ up1 up ¢ ˙ up up¢ Í 1 ÍÎk (q + qTF ) ˙˚ ¥ d(p + p1  p  q + p1 + q ),
2p W (q ) = uF
2
(6.A2)
where qTF = 4aT/uF ln(1 + e me /T )(1 + e mh /T ) is the Thomas– Fermi momentum describing screening in graphene [24, 34], up up¢
2
= (1 + cos q pp¢ )/ 2 is the matrix element of two Bloch
functions in honeycomb lattice. In Eq. (6.A2) the Thomas–Fermi momentum could be replaced by the reciprocal gatedielectric thickness for the qualitative description of gate screening. In case of small velocities p ◊ Ve ≪ T, p ◊ Vh ≪ T, the electronhole collision integral can be transformed using the common linearization technique for Fermisystems [35]
Ú
St{ fe , f h } = 4 W (q) fe (p) f h (p1 )[1  fe (p  q )] [1  fh (p1 + q)] ¥
q ◊(Vh  Ve ) d 2qd 2p1 , T (2p )4
(6.A3)
where the energy and momentum conservation laws were used. Equation (6.A3) timed by q/2 and integrated over dGp is electronhole friction force feh per unit area in the right hand side of the Euler equations (6.8) and (6.9). After averaging over angle between q and Vh – Ve it is presented as
Appendix
where
feh = beh (Vh – Ve),
Ú
beh = W (q)fe (p) f h (p1 )[1  fe (p  q )][1  f h (p1 + q )] ¥
4q2 d 2qd 2p1d 2p . T (2p)6
(6.A4)
In Refs. [11, 36], it was shown that almost collinear vectors p, p1, and q give the leading contribution to the collision integral. This facts originates from the linearity of the carrier spectrum, i.e., particles moving with the same velocity and the same direction interact infinitely long. Following the technique, described in Ref. [11], the quantity beh in the collinear limit is presented as beh µ
T 4e 4 ln(1 / a ) 5k 2uF6
Ú
•
dP
0
Ú
•
0
dP1
Ú
P
P1
F ( P  ze )F ( P1 + zh )
ÈÎ1  F ( P  Q  ze )˘˚ ¥ [1  F ( P1 + Q + zh )] PP1 ( P  Q )( P1 + Q )
Q 2dQ ( Q  4a ln F(ze )F (  zh ))2
,
(6.A5)
where F(x) = (1 + ex)–1, ze = me/T, zh = mh/T, and the term ln 1/a originates from the corrections to the electronic sperctrum due to electronelectron interactions. In this form the friction coefficient beh can be simply computed numerically.
A.2 Friction Caused by Charged Impurities and Phonons
Calculation of friction force caused by charged impurities can be drawn analytically in the limit of monopolar plasma. The momentum relaxation rate is given by
Ú
t p1,i = S iW (q)(1  cosq pp¢ ) up up¢
2
d 2p¢
(2p)2
,
(6.A6)
where Si is the sheet density of charged impurities. The Coulomb scattering probability W(q) is given by Eq. (6.A2) with the following deltafunction d(puF – p¢uF). Here we put into consideration only selfscreening caused by carriers in graphene.
121
122
Hydrodynamic Model for ElectronHole Plasma in Graphene
To calculate the friction force per unit area fei one should integrate the momentum relaxation rate (6.A6) timed by p with the ∂fe,0 p ◊ Ve: nonequilibrium part of distribution function d fe = ∂e ∂f (6.A7) fei = p p ◊ Vet p1,i dG p . ∂e
Ú
In monopolar case one can set ∂fe,0/∂e = –d(puF – me) and perform trivial integration fei = 
pe 4 S e S iVe uF2k 2
Ú
2p
0
sin2 q pp¢ dq pp¢
(2 sin(q pp¢ / 2) + 4a )2
,
where the dimensionless integral actually depends only on the permittivity κ of the environment. We can use the same technique to derive the expression for the friction force, caused by phonon scattering. We start from the expression t p1, ph =
D2Tp
4rs s2 3uF
,
derived in Ref. [5], and, using Eq. (6.A7), arrive at the following friction term fe ph = 
D2T pe2 Ve 4rs s2uF2 3
.
(6.A8)
References 1. A. Jungel, QuasiHydrodynamic Semiconductor Equations (Birkauser Verlag, 2001). 2. R. Bistritzer and A. H. MacDonald, Phys. Rev. B, 80, 085109 (2009).
3. V. F. Gantmacher and Y. B. Levinson, Carrier Scattering in Metals and Semiconductors (NorthHolland, Amsterdam, 1987).
4. G. E. Uhlenbeck and G. W. Ford, Lectures in Statistical Mechanics (Providence, AMS, 1963). 5. F. Vasko and V. Ryzhii, Phys. Rev. B, 76, 233404 (2007).
6. L. A. Falkovsky, Phys. Lett. A, 372, 31 (2008).
References
7. E. H. Hwang and S. Das Sarma, Phys. Rev. B, 77, 115449 (2008).
8. M. Shur, Physics of Semiconductor Devices (PenticeHall, Englewood Clifs, NJ, 1990). 9. K. S. Novoselov, et al., Nature, 438, 197–200 (2005).
10. V. Vyurkov and V. Ryzhii, JETP Lett., 88, 322–325 (2008). 11. A. Kashuba, Phys. Rev. B, 78, 085415 (2008).
12. M. I. Katsnelson, Eur. Phys. J. B, 51, 157–160 (2006).
13. K. Ziegler, Phys. Rev. B, 75, 233407 (2007).
14. L. A. Falkovsky and A. A. Varlamov, Eur. Phys. J. B, 56, 281–284 (2007).
15. K. Ziegler, Phys. Rev. Lett., 97, 266802 (2006).
16. K. I. Bolotin, et al., Phys. Rev. Lett., 101, 096802 (2008).
17. K. I. Bolotin, et al., Solid State Commun., 146, 351 (2008).
18. R. S. Shishir, et al., J. Comput. Electron., 8(2), 43–50 (2009).
19. R. S. Shishir and D. K. Ferry, J. Phys.: Condens. Matter, 21, 232204 (2009). 20. V. Ryzhii, Jpn. J. Appl. Phys., 45, L923 (2006).
21. V. Ryzhii, A. Satou, and T. Otsuji, J. Appl. Phys., 101, 024509 (2007).
22. A. Principi, R. Asgari, and M. Polini, Solid State Commun., 151, 21 (2011). 23. B. Wunsch, et al., New J. Phys., 8, 318 (2006).
24. S. D. Sarma and E. H. Hwang, Phys. Rev. Lett., 102, 206412 (2009).
25. O. V. Konstantinov and V. I. Perel, Sov. Phys.Solid State, 9, 3051 (1967). 26. A. S. Esperidiao, A. R. Vasconcellos, and R. Luzzi, Solid State Commun., 73(4), 275–279 (1990). 27. H. Gutfreunda and Y. Unnaa, J. Phys. Chem. Sol., 34, 9 (1973). 28. J. Ruvalds, Adv. Phys., 30(5), 677–695 (1981).
29. J. F. Lampin, F. X. Camescasse, A. Alexandrou, M. Bonitz, and V. ThierryMieg, Phys. Rev. B, 60, R8453–R8456 (1999). 30. A. V. Chaplik, JETP Lett., 91, 4 (2010).
31. F. Rana, Phys. Rev. B, 84, 045437 (2011).
32. A. V. Chaplik, Sov. Phys. JETP, 35, 395 (1972).
33. M. Dyakonov and M. Shur, Phys. Rev. Lett., 71, 2465–2468 (1993).
34. A. H. C. Neto, F. Guinea, N. M. R. Peres, K. S. Novoselov, and A. K. Geim, Rev. Mod. Phys., 81, 109–162 (2009).
123
124
Hydrodynamic Model for ElectronHole Plasma in Graphene
35. E. M. Lifshitz and L. P. Pitaevsky, Physical Kinetics (Pergamon Press, Oxford, 1981).
36. L. Fritz, J. Schmalian, M. Muller, and S. Sachdev, Phys. Rev. B, 78, 085416 (2008).
Chapter 7
Interplay of Intra and Interband Absorption in a Disordered Graphene*
F. T. Vasko,a V. V. Mitin,a V. Ryzhii,b and T. Otsujib aDepartment
of Electrical Engineering, University at Buffalo, Buffalo,
New York 14601920, USA
bResearch Institute of Electrical Communication, Tohoku University,
Sendai 9808577 and Japan Science and Technology Agency, CREST,
Tokyo 1070075, Japan
[email protected]
The absorption of heavily doped graphene in the terahertz (THz) and midinfrared (MIR) spectral regions is considered taking into account both the elastic scattering due to finiterange disorder and the variations of concentration due to longrange disorder. The interplay between intra and interband transitions is analyzed for the highfrequency regime of response, near the Pauli blocking threshold. The gate voltage and temperature dependencies of the *Reprinted with permission from F. T. Vasko, V. V. Mitin, V. Ryzhii, and T. Otsuji (2012). Interplay of intra and interband absorption in a disordered graphene, Phys. Rev. B, 86, 235424. Copyright © 2012 The American Physical Society. GrapheneBased Terahertz Electronics and Plasmonics: Detector and Emitter Concepts Edited by Vladimir Mitin, Taiichi Otsuji, and Victor Ryzhii
Copyright © 2021 Jenny Stanford Publishing Pte. Ltd.
ISBN 9789814800754 (Hardcover), 9780429328398 (eBook)
www.jennystanford.com
126
Interplay of Intra and Interband Absorption in a Disordered Graphene
absorption efficiency are calculated. It is demonstrated that for typical parameters, the smearing of the interband absorption edge is determined by a partly screened contribution to longrange disorder while the intraband absorption is determined by finiterange scattering. The latter yields the spectral dependencies which deviate from those following from the Drude formula. The obtained dependencies are in good agreement with recent experimental results. The comparison of the results of our calculations with the experimental data provides a possibility to extract the disorder characteristics.
7.1 Introduction
Both the gapless (massles) energy band structure and peculiarities of scattering mechanisms determine the response of graphene on the inplane polarized radiation in the terahertz (THz) and midinfrared (MIR) spectral regions. Such a response is caused by both the direct interband transitions and the intraband transitions of free carriers accompanied by scattering processes (the Drude mechanism), see the reviews in Refs. [1–3] and references therein. The contributions of these two mechanisms in heavily doped graphene are described by the inter and intraband dynamic conductivities, sinter and sintra, respectively, given by Res inter ª
sF e2 q(w  2e F ), s intra (w ) ª , 4 1 + iwt F
(7.1)
where eF and tF stand for the Fermi energy and the momentum relaxation time, s F = (e2/4ℏ)eFtF/ℏ is the static conductivity, and q(e) is a unity steplike fuction. Here we have neglected a weak imaginary contribution Ims inter [4] and the smearing of the interband absorption edge associated with the finiteness of the temperature T, and the collisional damping of the electron spectrum. When such a damping can be neglected at T = 0, the expression for Res inter describes an abrupt jump at photon energy ℏw = 2eF due to the Pauli blocking effect. The interband and intraband contributions are of the same order of magnitude at wtF ~ 4e Ft F / p  1. Therefore, the overlap of these contributions disappears if eFtF/ℏ ≥ 20 (see Fig. 7.1a). Thus, the description of interplay between both
Introduction
contributions is necessary in the THz (or MIR, depending on the doping level) spectral region for the typical samples with ℏ/eFtF ≥ 0.2. As shown below, the quasiclassical description of the intraband absorption and, therefore, the expression for s intra(w) based on the Drude formula is not valid if ℏw exceeds temperature of carriers [5, 6]. This is because of the variation of the relaxation time as a function of the electron energy over energy intervals ~ ℏw, where the intraband transitions take place (see Fig. 7.1b).
Figure 7.1 (a) Spectral dependencies of Res (ω) described by simplified Eq. (7.1) for different doping levels determined by eFtF/ℏ. (b) Intra and interband transitions between linear branches of gapless energy spectra. (c) Screening of nonuniform charge in ungated graphene with field distribution shown by dashed curves. (d) Gated graphene structure with partly screened charge and distribution of weak field shown by dotted curves.
The constant value for the interband conductivity Res inter associated with the frequencyindependent absorption was observed for undoped suspended graphene in the visible range of the spectrum [7]. By analogy with electrical transport in fieldeffect transistors, MIR spectroscopy allows for the control of the Pauli blocking effect using the electrical gating [8]. In sufficiently heavily doped graphene, the Drude mechanism of absorption was observed near the interband threshold, up to the MIR spectral region [9–11].
127
128
Interplay of Intra and Interband Absorption in a Disordered Graphene
Despite of a series of theoretical studies (see Refs. [12–14] and references therein), which have treated the problem of intra and interband absorption at different levels of approximation, there are two drawbacks in the interpretation of the abovelisted experimental data. First, the quantum description of the intraband absorption was not connected with the scattering parameters determined from the conductivity measurements and, second, an inhomogeneous smearing of the interband threshold due to longrange disorder was not considered. Thus, a reexamination of the intra and interband absorption processes in a disorded graphene is timely now. In this chapter, we present a general consideration which is based on the Kubo formula and takes into account both the scattering due to finiterange disorder and a longrange partly screened variation of concentration. The latter contribution appears to be essential because the screening of the potential spatial variations associated with the disorder with the inplane scales longer than (or comparable to) the distance to gate is suppressed. This mechanism is schematically illustrated in Figs. 7.1c and 7.1d. As a result, the inhomogeneous mechanism of smearing of the interband absorption at ℏw ~ 2eF should be taken into account, together with the thermal smearing of the Fermi distribution and broadening of the spectral density due to the elastic scattering on the finiterange disorder. The dynamic conductivity in the highfrequency range (if wtF > 1) is expressed via the Green’s function, which is averaged over the finiterange disorder, and the carrier distribution averaged over the longrange partly screened disorder. The averaged characteristics of Green’s function were obtained using the phenomenological description of the static conductivity similarly to Ref. [15]. Considering the interplay of the intra and interband contributions, we analyze the spectral, temperature, and gate voltage dependencies of the absorption efficiency. The obtained results are compared with the recent experimental data [10, 11]. The fitting procedure demonstrates that the disorder characterization, including the evaluation of the parameters of highenergy scattering and longrange inhomogeneties, can be performed using the THz and MIR spectroscopy. The chapter is organized as follows. In the next section (Section 7.2), we present the basic equations which describe the inter and intraband mechanisms of absorption and consider partly screened
Basic Equations
longrange disorder in gated graphene. In Section 7.3 we analyze the spectra of relative absorption and their dependencies on the temperature disorder and as well as on the doping conditions. The last section includes the discussion of experimental data and the approximations used, and the conclusions.
7.2 Basic Equations
We start with consideration of the dynamic conductivity based on the Kubo formula which takes into account the elastic scattering and the partly screened longrange disorder. Since the absorption is determined by the real part of conductivity, Res w, we neglect the Ims w contribution [4].
7.2.1 Dynamic Conductivity
Absorption of the THz (MIR) radiation propagating along the normal to the graphene layer is described by the real part of dynamic conductivity [6], given by Res w =
2pe2
¥
wL2
Ú dE( f
Â (a v�
�
E
 fE + w ) 2
a ¢ ) d (E  ea )d(E  ea ¢ + �w ) .
aa ¢
(7.2)
Here L2 is the normalization area, f(ea) is the equilibrium distribution 2 over the states a) with energies ea, and (a v� � a ¢) is the matrix element of the inplane velocity operator v� � between the states a and a¢ connected by the energy conservation law described by the d function. The a states are defined by the eigenvalue problem (h + Vx )y(xa ) = ea y(xa ) expressed via the singleparticle Hamiltonian h , a random potential Vx, and the twocomponent wave function y(lxa ) with l = 1, 2. The statistical averaging of Eq. (7.2) over the random potential is denoted as ·ºÒ. To perform this averaging, we introduce the spectral density function Ae (lx , l¢ x ¢ ) =
Â d (e  e a
a
)y(lxa )y(l¢ax)*¢ .
Thus, Res w given by Eq. (7.1) is transformed into
(7.3)
129
130
Interplay of Intra and Interband Absorption in a Disordered Graphene
Res w =
2p(ev )2 w L2
Ú dE( f
E
Ú Ú
 fE + w ) dx1 dx2
A E+nw (x , x )sA 1 ˘ , ¥ tr È AAE ( x1 , x2 )sA 1 A 2 1 Î ˚
(7.4)
where tr . . . means trace over the isospin variable, u = 108 cm/s is the characteristic velocity, and s� I = (s� ◊e) is written through the 2 ¥ 2 Pauli matrix s and the polarization ort e. Further, the spectral density function is expressed through the R exact retarded and advanced Green’s functions G E ( x1 , x2 ) and A A E ( x , x ) = i ÈGG ER (x , x )  GG EA ( x , x )˘ / 2p . G E ( x1 , x2 ) as follows A 1 2 1 2 1 2 ˙ ÍÎ ˚ These Green’s functions are governed by the standard equation R
[E  i0  v(s� ◊ p1 )  ux1  vx1 ]G E ( x1 , x2 )
(7.5)
= 1 d(x1  x2 ),
which is written through the potential energy with separated contributions from finite and longrange disorder, ux1 and ux1 labeled as fr and lr respectively. The averaging ·ºÒ in Eq. (7.4) should also be separated as ·ºÒlr and ·ºÒfr. It is convenient to introduce the variables (x1 + x2)/2 = x and x1 – x2= Dx in Eqs. (7.4) and (7.5). Using these variables and neglecting a weak contribution of —ux we obtain ux+Dx/2 ≃ ux . As a result, after the replacement E ⟶ E + up one can separate the averaging over fr and lrdisorder contributions and Eq. (7.4) takes the form Res w =
Ú
2p (ev )2 dE( fE + vp w
lr
 f E + vp+ w
lr
)
A ( x , x )sA A A ¥ dDx tr È A (x , x )A ˘ Î E 1 2 I E+nw 2 1 s I ˚
Ú
, fr
(7.6)
where we take into account that ·ºÒ f r depends only on Dxand use Ú dx = L 2 . We consider below the highfrequency spectral region, wtF ≫ 1, when the correlation function · º Ò f r can be factorized through
E (x , x ) the averaged spectral functions ADxE ∫ A 1 2 over fr disorder gives the contribution
Ú dDx tr[[]
sr
= L2
Â tr ( AA p
A
fr
A I ApE +nw sA I pE s
. The averaging
).
(7.7)
Basic Equations
Here the spectral densities ApE should be written through the A R+ R averaged Green’s functions, G pE = G pE and G pE , which are given by the matrix expression
R R � pE ˘ G� pE = È E  v(s� ◊ p1 )  S ÍÎ ˙˚
1
,
R = z R + (s ◊ p) h R , S pE pE pE p
(7.8)
where the selfenergy function is determined in the Born approximation through the functions R z pE
R hpE
=
dp1
Ú (2p) W 2
¥
Using
ux1 ux2
1 1 + E + i0  vp1 E + i0 + vp1 ˆ (p ◊ p1 ) Ê 1 1 Á pp1 Ë E + i0  vp1 E + i0 + vp1 ¯˜ Fourier
the
.
transformation
(7.9) of
= u exp[( x1  x2 ) / 2l fr ], one obtains in (7.9) the 2
fr
p  p1
2
Gaussian correlation function WDp expressed through the strength R of potential and correlation length u and lfr. Because G pE depends only on the matrix (s ◊ p), the averaged spectral density of Eq. (7.7)
takes the form
(+) () ApE = ApE + ApE + (s ◊ p) A ( + )  A(  ) pE pE 2 2p
(
A( ± ) = pE
ˆ 1 i Ê 1 Á ˜, 2p Ë e pE vpE p e pE ± vpE p ¯
)
(7.10)
where we introduced the renormalized dispersion law and velocity R R e pE = E  z pE and vpE = v(1 + hpE / vp), respectively. For the averaging over lr disorder in Eq. (7.6) we introduce •
the population factor
fE+v
lr
=
Ú dE¢f
•
E  E¢ f E¢
with the kernel
131
132
Interplay of Intra and Interband Absorption in a Disordered Graphene
fE–E¢ determined by the characteristics of disorder, see Section 7.2.2. Thus, based on the two assumptions employed (smoothness of lrpotential —u ⟶ 0 and highfrequency approach wtF ≫ 1) we obtain Res w written through the triple integral Res w =
p (ev )2 w L2
¥
Ú dE Ú dE ¢f
Â( A
(+) pE
() + ApE
p
E  E ¢ ( fE ¢
) (A
(+) pE+w
 fE ¢+w )
)
) + Ap( E+ w ,
(7.11)
(±) (±) (±) () ApE and ApE ApE correspond to where the contributions µ ApE the intra and interband absorption processes, respectively. Similar expressions for the homogeneous case, without lr contribution, were considered in Ref. [13].
7.2.2 Partly Screened LongRange Disorder
Here we evaluate the squareaveraged potential of lr disorder which is caused by a builtin random potential wx. We take into account the screening effect in the gated structure with the graphene sheet placed at z = 0 on the substrate of the width d and the static dielectric permittivity Œ, see Fig. 7.1d. The electrostatic potential Vxz is defined by the Poisson equation with the induced charge at z = 0 determined by the concentration of electrons in the heavily doped graphene 2 nx = (4 / L4 )S pq (e F  e xp ) = ÎÈ(e F  vx )/ p v ˘˚ . The dispersion law epx = up + ux is written here through the screened potential ux = wx + Vxz=0. Performing the Fourier transformation over x plane one obtains < > the secondorder equations for Vqz and Vqz which correspond to the substrate 0 > z > – d and to the upper halfspace z > 0 > Ê d2 ˆ Vqz z >0 2 q Á 2 ˜ < = 0, 0 > z > d . Ë dz ¯ Vqz
(7.12)
The jump of electric field at z = 0 is defined by the charge distribution over graphene (z ⟶ 0) > dVqz
dz
Œ
z=0
dVq 100, the relation v / w (1+ Œ)/ gF appears to be valid for the interval of d/llr > 0.1.
7.3 Relative Absorption
In this section we consider the absorption of radiation propagated along the normal to graphene sheet placed on semiinfinite substrate with the highfrequency dielectric permittivity k. Here we analyze the relative absorption coefficient xw
16p Res w
k (1 + k )2 c
(7.20)
neglecting the secondorder corrections with respect to the parameter 4p s w / c k . Note that the reflection and transmission coefficients Rw and Tw (these values are connected by the energy conservation requrement Rw + Tw + xw = 1), involve the firstorder correction µ 4p s w / c k and the Resw contributions should be involved for description of Rw and Tw .
7.3.1 Spectral Dependencies
First, we consider xw given by Eq. (7.20) after substituting the dynamic conductivity determined by Eqs. (7.9)–(7.11). Performing the multiple integrations in Resw, one obtains the spectral, gate voltage, and temperature dependencies of relative absorption. For calculations of the renormalized energy spectra and velocity defined by Eq. (7.9) we use here the typical parameters of fr disorder corresponding to the sample with the maximal sheet resistance ~3.5 kW and the correlation length lfr ~ 7.5 nm, see Ref. [15] for details. Level of longrange disorder v , corresponding to llr ≫ l F , is determined by the ratio d/llr, see Fig. 7.2; here we consider heavily doped graphene because a more complicated analysis is necessary for the case when electronhole puddles are formed [16]. The spectral dependencies of xw normalized to the highfrequency interband contribution xinter are plotted in Fig. 7.3 for the homogeneous graphene case v = 0 at concentrations 5 ¥ 1011 cm–2
135
136
Interplay of Intra and Interband Absorption in a Disordered Graphene
and 1012 cm–2 for temperatures T = 77 and 300 K. Similarly to the schematic spectra in Fig. 7.1a, one can separate contributions from intra and interband transitions at ℏw ~ 100 meV and ~150 meV for lower and higherdoped samples with the minimal value of xw/xinter ~0.15 and ~0.08, respectively. A visible deviation from the Drude spectral dependence (µ w–2 ) takes place due to quantum character of intraband transitions if ℏw ≥ T. Different signs of these deviations, which depend on ℏw, T, and n F , appear due to complicated energy and momentum dependencies in Eqs. (7.9) and (10). The smearing of interband absorption around the Fermi energies (2eF are marked by arrows) is defined by both the scatteringinduced broadening of the spectral density (7.10) and thermal effect (c.f. solid and dashed curves in Fig. 7.3).
Figure 7.3 Spectral dependencies of relative absorption in homogeneous graphene (normalized to xinter = xw⟶•) at temperatures 77 and 300 K (solid and dashed curves, respectively) for concentrations (1) 5 ¥ 1011 cm–2 and (2) 1012 cm–2. Arrows correspond to the doubled Fermi energies and dotted curves are µ w–2 asymptotics for Drude absorption.
In addition, the inhomogeneous smearing of the interband absorption threshold due to partly screened longrange variations of concentration is essential, as it is shown in Fig. 7.4 for T = 77 K. Here we considered a strong lrdisorder case with v 30 meV for nF = 5 ¥ 1011 cm–2 and v 20 meV for nF = 1012 cm–2 (we used the dependencies of Fig. 7.2 with w 50 meV and d/llr £ 0.1). Similarly to the thermally induced effect, the partly screened disorder effect results both in smearing of the interband absorption threshold and in enhancement of the minimal absorption in the region between intra and interband contributions.
Relative Absorption
Figure 7.4 The same as in Fig. 7.3 at T = 77 K taking into account inhomogeneous smearing of threshold due to partly screened variations of concentrations around (1) 5 ¥ 1011 cm–2 and (2) 1012 cm–2. Dashed curves are plotted for the homogeneous case v 0.
7.3.2 Comparison with Experiment We turn now to comparison of our calculations with the recent experimental data [10, 11] where both the spectral dependencies of relative absorption in largearea samples and the static conductivity s versus gate voltage Vg were measured. Using the phenomenological momentum relaxation rate vp suggested in Ref. [15] and the experimental data for hole conductivity from Refs. [10, 11], one can fit the dependency s(Vg) as it is shown in Fig. 7.5. This approach gives us the frdisorder scattering parameters for energies up £ 200 meV and we can extrapolate these data up to ~400 meV energies, which are necessary for description of the MIR response measured in Refs. [10, 11]. In Fig. 7.6 we plot the spectral dependencies of relative absorption measured in Ref. [12] for graphene with hole concentrations ~2.2, ~ 4.3, and ~5.8 ¥ 1012 cm–2 at T = 100 K. Solid curves are plotted for the case of homogeneous sample with the scattering parameters determined from the transport data shown in Fig. 7.5. These dependencies are in agreement with experiment both in the intraband absorption region (at ℏw £ 150 meV) and above threshold of interband absorption, at ℏw > 2eF. But the absorption in the intermediate region ℏw ~200–300 meV appears to be suppressed in comparison to the experimental data. The minimal absorption increases if we take into account the partly screened lrdisorder
137
138
Interplay of Intra and Interband Absorption in a Disordered Graphene
contribution with v ~ 80 , 75, and 60 meV for curves 1, 2, and 3, respectively. Such values of v are realized if w is comparable to eF and d/llr £ 0.1, i.e., micrometer scale of inhomogeneities takes place, see Fig. 7.2. Thus, we have obtained a reasonable agreement with the experimental data. But the smearing of the interband threshold is stronger in comparison to experimental data because the Gaussian model does not describe a real lr distribution. A more accurate description is possible with the use of lrdisorder parameters taken from additional structure measurements.
Figure 7.5 Fitting of experimental data from Refs. [10, 11] marked as 1 and 2: (a) momentum relaxation rate vp versus energy up and (b) sheet conductivity versus gate voltage. Squares and triangles are experimental points from Refs. (1) [10] and (2) [11], respectively.
Figure 7.6 Fitting of relative absorption spectra (normalized to xinter) to conditions of Ref. [10] at gate voltages (1) –30, (2) –60, and (3) –80 V. Solid and dotted curves correspond to homogeneous and inhomogeneous (with w ~ 150 meV) samples. Squares, triangles, and diamonds are experimental points for the cases 1, 2, and 3, respectively. Arrows correspond to the doubled Fermi energies.
A similar fitting of xw/xinter measured in Ref. [11] for hole concentrations ~4.3, ~6.5, and ~8.6, and 11 ¥ 1012 cm–2 at T = 300
e
Relative Absorption
K is presented in Fig. 7.7. We plot the spectral dependencies both for the homogeneous sample (solid curves) and for the inhomogeneous sample taking into account the strong lr disorder (dotted curves) with v ~ 120 , 105, 90, and 75 meV for curves 1, 2, 3, and 4, respectively. Now, reasonable agreement with experimental data for interband absorption takes place (see the above discussion of Fig. 7.6 about the lrdisorder contribution) while the intraband absorption appears to be 2–3 times stronger in comparison to the disorderinduced contributions calculated. An additional contribution may appear due to relaxation via emission of optical phonons of energy ℏw0. Such a channel of intraband absorption is allowed if eF > ℏw0 and the rate of transitions is proportional to the density of states at eF – ℏw0. As a result, this process may be essential for the conditions of Ref. [11], where eF ≥ 250 meV, while this mechanism should be negligible at the lower concentrations and temperatures used in Ref. [10]. Recent calculations of the phononinduced intraband contribution [17] gives an additional absorption ∼0.2ξinter for the conditions of Ref. [11]. This contribution is of the order of the disagreement between calculations and experimental data presented in Fig. 7.7. More detailed experimental data, for the spectral range 200–400 meV at temperatures £ 300 K, are necessary in order to verify this contribution.
Figure 7.7 The same as in Fig. 7.6 for conditions of Ref. [11] at gate voltages (1) –30, (2) –60, (3) –90, and (4) –120 V. Squares, triangles, diamonds, and inverse triangles are experimental points for the cases 1, 2, 3, and 4, respectively.
Overall, the comparison performed here demonstrates reasonable agreement with the experimental data, which opens a way for the verification of scattering mechanisms and longrange disorder parameters. The Drude spectral dependencies (for the region £
139
140
Interplay of Intra and Interband Absorption in a Disordered Graphene
100 meV) were fitted to the experimental data in Refs. [10, 11]; our calculations are in good agreement with these data because we used the scattering parameters taken from the transport measurements. A complete verification can be performed under complex analysis which should include comparisons of spectroscopic data with (i) steadystate transport measurements of conductivity and Hall effect versus Vg and T, (ii) a structural (e.g., scanning tunneling microscopy) characterization of longrange disorder, and (iii) effect of largearea inhomogeneties (ripples, wrinkles, holes, etc.) in centimetersized samples.
7.4 Conclusions
We have examined the spectral, concentration (gate voltage), and temperature dependencies of the relative absorption due to intraand interband transitions in graphene taking into account both elastic scattering and partly screened longrange variations of concentration. The smearing of the interband absorption edge, deviation from the Drude spectral dependence due to quantum regime of intraband transitions, and interplay of these two contributions are demonstrated. The results are in agreement with the recent experimental data obtained for heavily doped graphene [10, 11]. This analysis allows to extract disorder parameters in the highenergy region (up to ℏw above the Fermi energy). Let us discuss the assumptions used in the calculations performed. The main restriction of the results is due to consideration of the highfrequency spectral region, when Resw can be written through the matrix product of the averaged spectral density function (7.10). A more complicate description, based on the Bethe–Salpeter equation, is necessary for the lowfrequency region ωτF £ 1, which is beyond the scope of our consideration. This case is realized if ℏω < 20 meV, where the Drude dispertsion takes place, see Figs. 7.3 and 7.4. We also restrict ourselves by the phenomenological models for the finiterange disorder scattering [15] and for the partly screened longrange variations of concentration. It is enough for a description of spectral, gate voltage, and temperature dependencies of ξω because they are expressed through simple correlation functions which are similar for any microscopic nature of disorder. In addition,
References
a longrange random strain [18] may have affect on the interband transitions in largearea samples. The scattering processes caused by phonons and carriercarrier collisions should be analyzed under calculations of the intra and interband absorption in clean samples. A possible contribution of optical phonons at room temperature [11] is discussed in Section 7.3.2 (more detailed analysis is beyond of the scope of this chapter) while the interaction with acoustic phonons is negligible. The Coulomb interaction changes the interband absorption in the UV spectral region due to the excitonic effect [19]. The comparison with the experiment was performed here for the hole doping case and electronhole asymmetry reported in Refs. [10, 11] is unclear. According to Ref. [20], the Coulombinduced renormalization of the response and scattering processes give a weak contribution for typical disorder levels. This disagreement requires an additional investigation. To conclude, we believe that our results open a way for characterization of scattering processes and longrange inhomogeneities using THz and MIR spectroscopy. More important, that effect of disorder on THz and MIR response is the main factor which determines characteristics of different devices (e.g., lasers [21] and photodetectors [22]) in this spectral region. We believe that our study will stimulate a further investigation of these device applications.
Acknowledgment
This research is supported by the NSFPIRETeraNano grant (USA), by the JSPS Grant in Aid for Specially Promoting Research (No. 23000008, Japan), and by the JSPS CoretoCore Program (No. 23004, Japan).
References
1. N. M. R. Peres, Rev. Mod. Phys., 82, 2673 (2010).
2. M. Orlita and M. Potemski, Semicond. Sci. Technol., 25, 063001 (2010); F. Bonaccorso, Z. Sun, T. Hasan, and A. C. Ferrari, Nat. Photonics, 4, 611 (2010). 3. L. A. Falkovsky, Phys. Usp., 51, 887 (2008); K. F. Mak, L. Ju, F. Wangb, and T. F. Heinz, Solid State Commun., 152, 1341 (2012).
141
142
Interplay of Intra and Interband Absorption in a Disordered Graphene
4. The imaginary contribution Imσω is expressed through Resinter with the use of the KramersKronig relation. Using a cutoff frequency correspondent to the width of valence band em one obtains a weak contribution Imsw ~ (ℏw/2pem)e2/ℏ. 5. K. Zeeger, Semiconductor Physics (Springer, New York, 1973).
6. G. D. Mahan, ManyParticle Physics (Plenum Press, New York, 1990); F. T. Vasko and O. E. Raichev, Quantum Kinetic Theory and Applications (Springer, New York, 2005).
7. R. R. Nair, P. Blake, A. N. Grigorenko, K. S. Novoselov, T. J. Booth, T. Stauber, N. M. R. Peres, and A. K. Geim, Science, 320, 1308 (2008); K. F. Mak, M. Y. Sfeir, Y. Wu, C. H. Lui, J. A. Misewich, and T. F. Heinz, Phys. Rev. Lett., 101, 196405 (2008).
8. F. Wang, Y. Zhang, C. Tian, C. Girit, A. Zettl, M. Crommie, and Y. R. Shen, Science, 320, 206 (2008); Z. Q. Li, E. A. Henriksen, Z. Jiang, Z. Hao, M. C. Martin, P. Kim, H. L. Stormer, and D. N. Basov, Nat. Phys., 4, 532 (2008).
9. J. M. Dawlaty, S. Shivaraman, J. Strait, P. George, Mvs. Chandrashekhar, F. Rana, M. G. Spencer, D. Veksler, and Y. Chen, Appl. Phys. Lett., 93, 131905 (2008).
10. J. Horng, C.F. Chen, B. Geng, C. Girit, Y. Zhang, Z. Hao, H. A. Bechtel, M. Martin, A. Zettl, M. F. Crommie, Y. R. Shen, and F. Wang, Phys. Rev. B, 83, 165113 (2011).
11. L. Ren, Q. Zhang, J. Yao, Z. Sun, R. Kaneko, Z. Yan, S. Nanot, Z. Jin, I. Kawayama, M. Tonouchi, J. M. Tour, and J. Kono, Nano Lett., 12, 3711 (2012).
12. T. Ando, Y. Zheng, and H. Suzuura, J. Phys. Soc. Jpn., 71, 1318 (2002); T. G. Pedersen, Phys. Rev. B, 67, 113106 (2003); A. Gruneis, R. Saito, G. G. Samsonidze, T. Kimura, M. A. Pimenta, A. Jorio, A. G. Souza Filho, G. Dresselhaus, and M. S. Dresselhaus, ibid., 67, 165402 (2003); L. A. Falkovsky and A. A Varlamov, Eur. Phys. J. B, 56, 281 (2007). 13. V. P. Gusynin, S. G. Sharapov, and J. P. Carbotte, Phys. Rev. Lett., 96, 256802 (2006); T. Stauber, N. M. R. Peres, and A. H. Castro Neto, Phys. Rev. B, 78, 085418 (2008).
14. N. M. R. Peres, F. Guinea, and A. H. Castro Neto, Phys. Rev. B, 73, 125411 (2006); S. Yuan, R. Roldan, H. D. Raedt, and M. I. Katsnelson, Phys. Rev. B, 84, 195418 (2011). 15. P. N. Romanets and F. T. Vasko, Phys. Rev. B, 83, 205427 (2011); F. T. Vasko and V. Ryzhii, Phys. Rev. B, 76, 233404 (2007).
16. J. Martin, N. Akerman, G. Ulbricht, T. Lohmann, J. H. Smet, K. von Klitzing, and A. Yacoby, Nat. Phys., 4, 144 (2007); Y. Zhang, V. W. Brar, C. Girit, A. Zettl, and M. F. Crommie, Nat. Phys., 6, 722 (2009).
References
17. B. Scharf, V. Perebeinos, J. Fabian, and P. Avouris, arXiv:1211.3329.
18. V. M. Pereira, R. M. Ribeiro, N. M. R. Peres, and A. H. Castro Neto, Europhys. Lett., 92, 67001 (2010); V. K. Dugaev and M. I. Katsnelson, Phys. Rev. B, 86, 115405 (2012).
19. L. Yang, J. Deslippe, C.H. Park, M. L. Cohen, and S. G. Louie, Phys. Rev. Lett., 103, 186802 (2009); K. F. Mak, J. Shan, and T. F. Heinz, ibid., 106, 046401 (2011).
20. A. G. Grushin, B. Valenzuela, and M. A. H. Vozmediano, Phys. Rev. B, 80, 155417 (2009); N. M. R. Peres, R. M. Ribeiro, and A. H. Castro Neto, Phys. Rev. Lett., 105, 055501 (2010); S. H. Abedinpour, G. Vignale, A. Principi, M. Polini, W.K. Tse, and A. H. MacDonald, Phys. Rev. B, 84, 045429 (2011). 21. V. Ryzhii, M. Ryzhii, and T. Otsuji, J. Appl. Phys., 101, 083114 (2007); B. Dora, E. V. Castro, and R. Moessner, Phys. Rev. B, 82, 125441 (2010).
22. A. Urich, K. Unterrainer, T. Mueller, Nano Lett., 11, 2804 (2011); V. Ryzhii, M. Ryzhii, V. Mitin, and T. Otsuji, J. Appl. Phys., 107, 054512 (2010).
143
Chapter 8
VoltageControlled surface plasmonpolaritons in double graphene layer structures*
D. Svintsov,a,b V. Vyurkov,a,b V. Ryzhii,c,d and T. Otsujic,d aInstitute
of Physics and Technology, Russian Academy of Sciences, Moscow 117218, Russia bDepartment of Physical and Quantum Electronics, Moscow Institute of Physics and Technology, Dolgoprudny 141700, Russia cResearch Institute for Electrical Communication, Tohoku University, Sendai 9808577, Japan dJapan Science and Technology Agency, CREST, Tokyo 1070075, Japan [email protected]
The spectra and damping of surface plasmonpolaritons (SPPs) in double graphene layer structures are studied. It is proved that SPPs in those structures exhibit an outstanding voltage tunability of velocity and damping, inherent to gated graphene, and a pronounced low
*Reprinted with permission from D. Svintsov, V. Vyurkov, V. Ryzhii, and T. Otsuji (2013). Voltagecontrolled surface plasmonpolaritons in double graphene layer structures, J. Appl. Phys., 113, 053701. Copyright © 2013 American Institute of Physics. GrapheneBased Terahertz Electronics and Plasmonics: Detector and Emitter Concepts Edited by Vladimir Mitin, Taiichi Otsuji, and Victor Ryzhii
Copyright © 2021 Jenny Stanford Publishing Pte. Ltd.
ISBN 9789814800754 (Hardcover), 9780429328398 (eBook)
www.jennystanford.com
146
Voltagecontrolled surface plasmonpolaritons
frequency coupling with photons inherent to nongated structures. It is also shown that the spatial dispersion of conductivity significantly augments the free path and cutoff frequency of SPPs, which is of great importance for practical applications.
8.1 Introduction
Recently the fabrication of double graphene layer (GL) structures was reported [1]. These structures consist of two GLs separated by a dielectric. If a bias voltage Vb is applied between GLs, the layers serve as a gate for each other. Such a possibility of tuning electronic properties of graphene without any metal gates has already found its application for tunnel fieldeffect transistors [2] and optical modulators [3]. Moreover, the devices based on 2GL seem promising for resonant THz detectors [4] and nearfield amplifiers [5]. Plasmonic properties of 2GL structures are of particular interest too. Firstly, they can operate as modulators of plasma waves (recently proposed for gated graphene in Ref. [6]). Secondly, plasma resonances can affect the characteristics of optical modulators, resulting in greater modulation depth near the plasmon peak [7]. Apart from the plasmons in GLbased structures [8–12], the surface plasmonpolaritons (SPPs) in GLs are of considerable practical interest too [13–15]. The spectra of plasmons in adjacent GLs were previously considered in Ref. [9]. In the present communication, we obtain the spectra of SPPs in doubleGL structures. Those spectra exhibit a pronounced coupling with photons at low frequencies in contrast to gated GLs [8]. Moreover, just like in the gated structures, the velocity and damping of SPPs can be tuned by the voltage applied between layers. In particular, at low bias voltages the SPPs are strongly damped due to interband transitions of electrons. At high bias voltages those transitions are forbidden by the Pauli blocking and the propagation length of SPPs is limited only by the Drude absorption. This opens the prospects of using 2GL structures as efficient SPP modulators. In contrast to many previous works on plasma waves in GLbased structures [9, 12, 16], in our calculations the spatial dispersion of conductivity is rigorously taken into account. It shows up in a major alteration of SPP spectra at the Fermi energies m comparable with the temperature T or higher. For instance, the spectra k(w) (k is the
Device Model
wave vector and w is the frequency) are no longer scalable with the Fermi energy, and the edge of SPP absorption associated with the interband transitions is significantly shifted from w = 2m/ℏ, expected from the analysis of the Pauli blocking, to higher values.
Figure 8.1 Schematic view of the 2GL structure and directions of vectors E, H, and k in the TM SPP.
8.2 device Model The doubleGL structure under consideration is sketched in Fig. 8.1. The two GLs are separated by a thin insulating layer of width d and permittivity em, the permittivities of the media under and over the GLs can be generally different, they are denoted by eb and et, respectively. One side of each GL is connected to the contact while the other side is isolated. A bias voltage Vb can be applied between contacts, thus, one GL can serve as a gate for another. The xaxis coincides with the direction of the SPP propagation parallel to the metal contacts, the zaxis is orthogonal to the GL plane. The applied bias voltage Vb between GLs (as shown in Fig. 8.1) induces an excess electron density in the top layer and hole density in the bottom one. If the residual doping of GLs is weak, the excess electron and hole densities in layers are equal. Meanwhile, the Fermi energies m in GLs coincide in absolute values but have the opposite sign. The band diagram of the structure under the bias voltage is shown in Fig. 8.2. The potential difference between GLs is equal to Vb – 2m/e. The distinction of this value from Vb is attributed to the effect of quantum capacitance. The Gauss theorem binds the bias voltage Vb and the charge density ±eS in GLs as follows:
em m (Vb  2 ) = eS. 4p d e
(8.1)
147
148
Voltagecontrolled surface plasmonpolaritons
+m eVb –m
Figure 8.2 Band diagram of the double graphene layer structure at bias voltage Vb.
Provided the Fermi energy m substantially exceeds the temperature T (measured in energy units), the charge density can be explicitly written, eS =
em 2
p 2vF2
.
(8.2)
Equations (8.1) and (8.2) allow to obtain the value of Fermi energy at given bias voltage and, thus, derive the kinetic characteristics of GLs, in particular, the conductivity necessary for the dispersion of SPPs.
8.3 spp dispersion in double graphene layer
Hereafter the spectrum (or dispersion law) will be regarded as the dependence of complex wave vector k on real frequency ω. Such statement of problem is consistent with the description of wave modulator. To obtain the dispersion law of SPP one has to solve the complete set of Maxwell equations in free space and then match the solutions on conducting graphene layers. As the imaginary part of graphene conductivity is positive in a wide range of frequencies, the propagation of transverse electric (TE) SPP modes along its surface is prohibited [17]. Thus, we focus only on transverse magnetic (TM)
SPP Dispersion in Double Graphene Layer
modes with the ac electric and magnetic fields E = {Ex, 0, Ez}, H = {0, Hy, 0}. The field of SPP is localized near the graphene layers, and, therefore, is searched in the form, Et = E0 t ei( kx wt )k t z ,
Em = (E0 m≠ ek m z + E0mØ e k m z ) ei( kx wt ) , Eb = E0 bei( kx wt )+k b z ,
(8.3)
(8.4) (8.5)
where the indices t, m, and b refer to the top, middle, and bottom
media, respectively, k i = k 2  e i w 2 / c 2 , and c is the speed of light. Matching the vectors E and H on the graphene layers (top and bottom layer conductivities are st and sb, respectively), one arrives at the dispersion law, ˘ È iw Ê et e m ˆ  st ˙ Í Á + ˜ ÍÎ 4p Ë k t k m ¯ ˚˙
˘ È iw Ê e b e m ˆ +  s b ˙ e2k md Í Á ˜ ˙˚ ÎÍ 4p Ë k b k m ¯
˘ È iw Ê e ˘ È iw Ê e e ˆ e ˆ = Í Á b  m ˜  s b ˙ Í Á t  m ˜  st ˙. ˙˚ ÎÍ 4p Ë k t k m ¯ ÎÍ 4p Ë k b k m ¯ ˚˙
(8.6)
As pointed out above, the Fermi energies in GLs are equal in modulus, hence, due to electronhole symmetry the layer conductivities are equal st = sb = s. If, therewith, the top and bottom media are identical (i.e., et = eb = e), the general dispersion relation decouples into two independent modes, Ê k md ˆ Ê iwe ˆ iwe m ÁË k  4ps ˜¯ + k tanh ÁË 2 ˜¯ = 0, m Ê k d ˆ iwe m Ê iwe ˆ  4ps ˜ tanh Á m ˜ + = 0. ËÁ k ¯ Ë 2 ¯ km
(8.7)
(8.8)
Equation (8.7) corresponds to a symmetric (optical) mode when the current oscillates in phase in both layers, while Eq. (8.8) represents an antisymmetric (acoustic) mode. We are especially interested in symmetric oscillations, because the antisymmetric ones are strongly damped [9]. For small separation between layers (κmd 1), the dispersion of symmetric mode depends only on the total conductivity of two layers [16],
149
150
Voltagecontrolled surface plasmonpolaritons
et e b 4pi =◊ 2s . + w kt kb
(8.9)
To perform a numerical analysis of SPP spectra using Eq. (8.7), one needs to know the conductivity of GLs. The latter itself is a function of frequency and wave vector. A number of models of the GL conductivity has been developed so far [18], each being valid in a certain range of frequencies and carrier densities. For highfrequency SPPs (from THz to infrared range), we use the relation for the GL conductivity derived from the Kubo formula [19], s kw = +
ie2
ÂÚ
p 2 a =1,2
2ie2 w p 2
Ú
d 2pv2x { f [Œa (p )]  f [Œa ( p+ )]} [Œa (p+ )  Œa (p )][w  Œa (p ( + )+ Œa (p )]
d 2pv21v12 { f ÈŒ Î 1 (p )˘˚  f [Œ2 (p+ )]} . [Œ2 (p+ )  Œ1 (p )][(( w )2  [Œ2 (p+ ) Œ1 (p )]2 ]
(8.10)
Here the indices 1 and 2 refer to conductance and valence bands, in particular, Œ1(p) = pvF and Œ2(p) = –pvF, vF ≃ 106 m/s, p± = p ± ћk/2, f(Œ) is the electron distribution function (the equilibrium Fermi function f(Œ) = [1 + e(Œ–m)/T]–1 is assumed), vx = vF cos qp and v12 = ivF sin qp are the matrix elements of velocity operator. The upper line in Eq. (8.10) corresponds to the intraband transitions, while the lower one accounts for the interband transitions. To allow for the momentum relaxation one should treat the frequency as w Æ w + it–1. The definite expressions for t–1 for different scattering processes can be found in Ref. [18]. Here, we restrict our consideration with perfect samples when electronphonon scattering is the dominating mechanism. The corresponding relaxation time is given by the following formula [20]: t 1 = t 01
m , T
(8.11)
where the parameter t0–1 ≃ 3 ¥ 1011 s–1 at room temperature T = 26 meV. It turns out that in the case under consideration, the spatial dispersion of the conductivity is significant. It can be neither omitted [16] nor treated as a perturbation [12]. As shown in the following, at fairly high Fermi energies the condition kvF w is broken because the electron transitions in momentum space become substantially indirect. In the situation, it is the most convenient to calculate the
Results and Discussion
conductivity (Eq. (8.10)) in elliptic coordinates: 2px = k cosh u cos v, 2py = k sinh u sin v. It should be noted that the wave vector is complex and the functions p ± ћk/2 should be regarded as absolute values of complex vectors. Extracting the real part from Eq. (8.10) with the help of the Sokhotski theorem in the limit t–1 Æ 0, one can arrive at the following expressions for the dissipation parts of the GL conductivity associated with the interband (Resinter) and intraband (Resintra) transitions, respectively, p
Re s inter =
Ï È w
e 2 ˘ 1  q 2 Ì f Í (1 + q cos v )˙ 2p Î 2
˚ 0 Ó
Ú
È w ˘ ¸ 1  q2 cos 2 v 2 sin vdv ,
 f Í (1  qcos v )˙ ˝ Î 2 ˚ ˛ 1  q 2 sin 2 v
(8.12)
•
Re s intra
e 2 È 2 ˘ 1/2 Ï È w ˘ =
q  1˚ Ì f Í (q cosh u  1)˙ 2p Î 2
Î ˚ 0 Ó
Ú
È w
˘ ¸ q2 cosh 2 u  1
(q q cosh u + 1)˙ ˝ 2 cosh 2 udu ,
 f Í 2 2 Î ˚ ˛ q sinh u + 1
(8.13)
where the dimensionless parameter of spatial dispersion q = kvF/w is introduced. The reduction of interband absorption with rising q obvious from Eq. (8.12) results in lower damping of SPPs.
8.4 Results and discussion
The spectra Rek(w) and Imk(w) of SPPs calculated numerically with Eqs. (8.7) and (8.10) are presented in Figs. 8.3 and 8.4. The structure parameters are as follows et = em = eb = 5 (boron nitride [21]), d = 2 nm. The following three characteristic ranges can be singled out in the SPP spectra. Small wave vectors and frequencies k 8am/(ћc), where a = e2/ (ћc) is the fine structure constant. In this range of wave vectors, the dispersion is purely “photonic” (see the inset in Fig. 8.3), i.e., the dispersion law reads k =
w e . c
(8.14)
151
152
Voltagecontrolled surface plasmonpolaritons
This region of spectra is specific to SPPs in nongated twodimensional electron gas, while in the gated structures the velocity of plasma waves at low frequencies is much lower than speed of light [8, 22], and the coupling with photons is impossible. w
m
c
e w/
m m
Figure 8.3 Dispersions Rek(w) of SPPs in double GL at different Fermi energies. Inset: lowenergy “photonic” behavior of spectra.
m m
m
Figure 8.4 Damping Imk(w) of SPPs in double GL at different Fermi energies. Inset: quality factor of SPPs defined as Rek/Imk at the same Fermi energies.
Intermediate wave vectors and frequencies 8am/(ћc) k ω/vF, w 2m/ћ. In this situation the coupling with photons is negligible and the spatial dispersion of conductivity could be omitted as well. For this reason, we can accept that κ ª k and simplify the expression for the SPP dispersion, k=
iwe , 8ps k =0,w
where the longwavelength conductivity at μ ≫ T is
(8.15)
Results and Discussion
s k =0,w = +
mt ie2 2m  w + ln p 1  iwt 2p 2m + w e2
2
e2 È Ê w ˆ Íf 4 Î ÁË 2 ˜¯
Ê w ˆ ˘ fÁ . Ë 2 ˜¯ ˙˚
(8.16)
Equations (8.15) and (8.16) yield a wellknown squarelaw dependence [22] Re k µ w2 until the interband transitions become significant (w ≃ 2m/ћ) or until the spatial dispersion of conductivity starts playing role (k ≃ w/vF). High frequencies w ~ 2m/ћ or high wave vectors k ~ w/vF. A simple analysis based on the Pauli exclusion principle states that the direct interband transitions are allowed at frequencies w > 2m/ћ. At such frequencies, the light incident on GLs is effectively absorbed. This lies in the basis of graphene optical modulators [3]. One could expect that SPPs, just like photons, could also be strongly absorbed in the frequency range w > 2m/ћ. However, this is not true. The situation is different for SPPs as their wave vectors can be large and the interband transitions are markedly indirect. From Eq. (8.12), it is readily seen that the interband absorption at finite k is not as strong as it is at k = 0. In the threshold case k > w/vF, the interband transitions are forbidden at all due to the nonconservation of the energy and momentum. On the contrary, the intraband transitions at k > w/vF are extremely strong because the quantity Resintra exhibits a singularity Resintra µ [(kvF/w)2 – 1]–1/2. The imaginary parts of SPP spectra obtained with and without accounting for the spatial dispersion of conductivity are compared in Fig. 8.5, upper panel. The models disregarding the spatial dispersion were widely used before [9, 12, 16]; though, they can overestimate the damping of SPPs by an order of magnitude. The difference in damping rates obtained with these two approaches is especially pronounced at high Fermi energies and frequencies w ~ 2m/ћ. The real part of dependence k(w) is also altered by indirect transitions, which is shown in Fig. 8.5, lower panel. The dispersions obtained without accounting for spatial dispersion cross the threshold line k = w/vF and penetrate in the region of strong intraband damping k > w/vF; but in point of fact, the spatial dispersion of conductivity keeps the spectrum under the threshold.
153
154
Voltagecontrolled surface plasmonpolaritons
w
m
w
Figure 8.5 Comparison of SPP dispersions obtained with and without taking into account the spatial dispersion of conductivity. Upper panel: Imk(w), lower panel: Rek(w).
For practical applications, it is important to study the dependence of SPP propagation length lp = (Imk)–1 on the bias voltage Vb. A high sensitivity of propagation length to the bias voltage near the threshold is required for efficient plasmonic modulators. The dependence lp(Vb) obtained from Eqs. (8.1) and (8.7) is plotted in Fig. 8.6. At high voltages (such that 2m > ћw), the propagation length of SPPs is limited by the Drude absorption. If the only scattering mechanism is acoustic phonon scattering, the propagation length at m ≫ T, 2m > ћw is voltageindependent and given by lp = 4
e2 T . we t 01
(8.17)
Worth noting the propagation length of SPP in double graphene layer is twice higher than in a single layer.
Conclusions
Providing the bias voltage decreases the interband transitions go in, resulting in strong damping. Near the threshold voltage the dependence lp(Vb) is nearly exponential with the slope dlglp/dVb ≃ 20 dB/V for the interlayer thickness d = 2 nm. At almost zero bias, the SPP damping might be even greater than that predicted by our present consideration because the electronhole scattering plays a significant role in the vicinity of the Dirac point [23].
Figure 8.6 SPP propagation length vs. bias voltage Vb between layers at different frequencies.
8.5 Conclusions The spectra of surface plasmonpolaritons in double graphene layer structures are obtained. Those excitations combine the voltage control inherent to gated structures and pronounced lowfrequency coupling with photons intrinsic to nongated graphene. The bias voltage applied between graphene layers shifts their Fermi energies and, hence, changes the rate of interband plasmon absorption. At low bias voltages, the SPPs are strongly damped, while at high voltages their propagation length is large since it is limited only by Drude absorption. This effect can be used in doubleGL plasmonic modulators. The substantial influence of the spatial dispersion of the GL conductivity (i.e., the indirect electron transitions) on the SPP spectra in doubleGL structures is revealed. In particular, the interband
155
156
Voltagecontrolled surface plasmonpolaritons
cutoff frequency of SPPs is shifted to much higher values. The propagation length of SPPs turns out to be by an order of magnitude higher than that obtained from previous models neglecting the spatial dispersion.
Acknowledgement
The work of D. Svintsov was supported by the Grant 14.132.21.1687 of the Russian Ministry of Education and Science. The work of V. Vyurkov was supported by the Grant 110700464 of the Russian Foundation for Basic Research. The work at RIEC was supported by the Japan Science and Technology Agency, CREST and by the Japan Society for Promotion of Science.
References
1. K. Kim, J. Choi, T. Kim, S. Cho, and H. Chung, Nature, 479, 338–344 (2011). 2. L. Britnell, R. Gorbachev, R. Jalil, B. Belle, F. Schedin, A. Mishchenko, T. Georgiou, M. Katsnelson, L. Eaves, S. Morozov, N. Peres, J. Leist, A. Geim, K. Novoselov, and L. Ponomarenko, Science, 335, 947 (2012). 3. M. Liu, X. Yin, and X. Zhang, Nano Lett., 12(3), 1482–1485 (2012).
4. V. Ryzhii, T. Otsuji, M. Ryzhii, and M. S. Shur, J. Phys. D: Appl. Phys., 45, 302001 (2012). 5. T. Stauber and G. GomezSantos, Phys. Rev. B, 85, 075410 (2012). 6. D. R. Andersen, J. Opt. Soc. Am. B, 27(4), 818–823 (2010).
7. V. Ryzhii, T. Otsuji, M. Ryzhii, V. G. Leiman, S. O. Yurchenko, V. Mitin, and M. S. Shur, J. Appl. Phys., 112, 104507 (2012).
8. V. Ryzhii, A. Satou, and T. Otsuji, J. Appl. Phys., 101, 024509 (2007). 9. E. H. Hwang and S. Das Sarma, Phys. Rev. B, 80, 205405 (2009).
10. F. Koppens, D. Chang, and F. Javier Garcia de Abajo, Nano Lett., 11(8), 3370–3377 (2011).
11. L. Ju, B. Geng, J. Horng, C. Girit, M. Martin, Z. Hao, H. A. Bechtel, X. Liang, A. Zettl, Y. Ron Shen, and F. Wang, Nat. Nanotechnol., 6, 630–634 (2011). 12. M. Jablan, H. Buljan, and M. Soljacic, Phys. Rev. B, 80, 245435 (2009).
13. Yu. Bludov, N. M. R. Peres, and M. I. Vasilevskiy, Phys. Rev. B, 85, 245409 (2012).
References
14. A. Ferreira and N. M. R. Peres, Phys. Rev. B, 86, 205401 (2012).
15. Yu. V. Bludov, M. I. Vasilevskiy, and N. M. R. Peres, Europhys. Lett., 92, 68001 (2010).
16. A. A. Dubinov, V. Ya. Aleshkin, V. Mitin, T. Otsuji, and V. Ryzhii, J. Phys.: Condens. Matter, 23, 145302 (2011). 17. G. W. Hanson, J. Appl. Phys., 103, 064302 (2008).
18. S. Das Sarma, S. Adam, E. H. Hwang, and E. Rossi, Rev. Mod. Phys., 83, 407–470 (2011). 19. L. A. Falkovsky and A. A. Varlamov, Eur. Phys. J. B, 56, 281–284 (2007).
20. F. Vasko and V. Ryzhii, Phys. Rev. B, 76, 233404 (2007).
21. R. Geick, C. H. Perry, and G. Rupprecht, Phys. Rev., 146, 543–547 (1966). 22. S. Das Sarma and E. H. Hwang, Phys. Rev. Lett., 102, 206412 (2009).
23. D. Svintsov, V. Vyurkov, S. Yurchenko, V. Ryzhii, T. Otsuji, J. Appl. Phys., 111(8), 08371508371510 (2012).
157
Chapter 9
Hydrodynamic Electron Transport and Nonlinear Waves in Graphene*
D. Svintsov,a V. Vyurkov,a V. Ryzhii,b and T. Otsujib aInstitute
of Physics and Technology, Russian Academy of Science,
Moscow 117218 and Moscow Institute of Physics and Technology,
Dolgoprudny 141 700, Russia
bResearch Institute for Electrical Communication, Tohoku University,
Sendai 9808577, Japan
[email protected]
We derive the system of hydrodynamic equations governing the collective motion of massless fermions in graphene. The obtained equations demonstrate the lack of Galilean and Lorentz invariance, and contain a variety of nonlinear terms due to quasirelativistic nature of carriers. Using those equations, we show the possibility of soliton formation in electron plasma of gated graphene. The quasirelativistic effects set an upper limit for soliton amplitude, which marks graphene out of conventional semiconductors. The *Reprinted with permission from D. Svintsov, V. Vyurkov, V. Ryzhii, and T. Otsuji (2013). Hydrodynamic electron transport and nonlinear waves in graphene, Phys. Rev. B, 88, 245444. Copyright © 2013 The American Physical Society. GrapheneBased Terahertz Electronics and Plasmonics: Detector and Emitter Concepts Edited by Vladimir Mitin, Taiichi Otsuji, and Victor Ryzhii
Copyright © 2021 Jenny Stanford Publishing Pte. Ltd.
ISBN 9789814800754 (Hardcover), 9780429328398 (eBook)
www.jennystanford.com
160
Hydrodynamic Electron Transport and Nonlinear Waves in Graphene
mentioned noninvariance of equations is revealed in spectra of plasmawaves in the presence of steady flow, which no longer obey the Doppler shift. The feasibility of plasmawave excitation by direct current in graphene channels is also discussed.
9.1 Introduction
The models of carrier transport in graphene should account for strong carriercarrier interaction [1, 2], which is governed by a large ‘finestructure constant’ e2/(ℏuF) ~ 1 and logarithmically divergent collision integral for collinear scattering [3, 4]. The relative strength of carriercarrier scattering compared to other relaxation mechanisms was also proved in the transparency measurements of optically pumped graphene [5, 6]. The corresponding relaxation time is estimated to be less than 100 fs. The most natural way to account for carriercarrier interactions in transport models is to use local equilibrium (hydrodynamic) distribution functions as a first approximation to the solution of kinetic equation [7]. Several approaches for description of hydrodynamic transport in graphene were presented in Refs. [8–15]. Within hydrodynamic models, it is possible to explain the temperatureindependent dc conductivity of graphene in charge neutrality point [8] and the strong Coulomb drag between electrons and holes [8, 15, 16]. The other predictions of hydrodynamic transport, such as preturbulent current flow due to low viscosity [11], existence of electronhole sound [8], and current saturation at high electric fields due to heating of electrons [10], still expect their experimental verification. In recent works on graphene hydrodynamics [9, 11 ,14], the equations were obtained under assumption of low drift velocity u of electron plasma (u ≪ uF). Several nonlinear terms were inevitably lost under such assumption. In several other works [12, 13], the hydrodynamics of massless quasiparticles in graphene was obtained from hydrodynamics of ultrarelativistic plasma by a simple replacement of the speed of light, c, by the Fermi velocity uF. Such a spurious analogy is misleading in this particular case as electrons in graphene are neither Galilean [17] nor truly Lorentzinvariant system (in general, this refers to any electrons in solids).
Introduction
The reason is that for velocities less and of the order of uF ≃ c/300, the distortion of spacetime metrics is negligible. Hence, dealing with quasirelativistic particles in Galilean spacetime, one will obtain hydrodynamic equations that are neither Galilean nor Lorentz invariant. In this chapter, we present an explicit derivation of hydrodynamic equations for massless electrons in graphene, following the general strategy put forward by Achiezer et al. [18]. In addition, we eliminate the restriction on the flow velocity requiring it to be much less than the Fermi velocity. This opens up an opportunity to study a wide variety of nonlinear phenomena, such as propagation of largeamplitude waves [19, 20], photovoltaic response [21], transport at high current flows [22], and acoustoelectronic interactions [23]. The peculiarities of electron interactions with impurities and phonons along with electronhole interactions have already been studied within a hydrodynamic approach in Refs. [8, 10, 13]. For this reason, in the present work we focus mainly on nondissipative nonlinear hydrodynamic transport. In graphene it is impossible to introduce a constant electron effective mass m as a proportionality coefficient binding the momentum to the velocity. Consequently, the Euler equation can be no longer presented in canonical form ∂tu + (u—)u + (—P)/r = 0, where u is the drift velocity, r is the mass density of electrons, and P is the pressure. However, a fictitious (hydrodynamic) mass M depending on the particle density n and the drift velocity naturally arises in the Euler equation. One more unusual feature of Euler equation is an appearance of density and velocitydependent factor before the convection term (u—)u. We show that in the degenerate electron system this term vanishes, giving way to a weaker fourthorder nonlinearity proportional to u2(u—)u. Using the derived equations, we study the nonlinear effects in plasmawave propagation in graphene. Hydrodynamics proved to be an extremely efficient tool for the study of electron plasma in twodimensional (2D) electron systems [24–27]. Collective dynamics of electrons in two dimensions has a rich analogy with the hydrodynamics of liquids, including the phenomena of electron flow choking [27] and formation of shallow and deepwater plasma waves in gated and nongated systems, respectively [26]. Despite huge efforts in the field of graphene plasmonics [28–32], the problem of
161
162
Hydrodynamic Electron Transport and Nonlinear Waves in Graphene
nonlinear plasma waves stayed beyond the scope of recent works. We show that the balance between nonlinearities and dispersion allows the formation of solitary plasma waves in gated graphene. We find that ‘relativistic’ terms in Euler equation set an upper limit for the soliton amplitude and broaden its profile. This much differs from the solitons in systems of massive 2D electrons [25, 33], which behave similarly to the solitary waves in water. The features of electron hydrodynamics are also pronouncedly revealed in the spectra of collective (plasma) excitations in graphene in the presence of stationary electron flow with velocity u0. It is natural to expect that velocities of forward and backward plasma waves are u0 ± s0, where s0 is the wave velocity in electron fluid at rest. We demonstrate, however, that in graphene the dependence of the wave velocities on the flow velocity is more complicated due to the lack of Galilean and Lorentz invariance. In particular case of 1 strongly degenerate electron system, these velocities are u0 ± s0. 2 We also revealed the potentiality of plasma instability in gated graphene in the presence of steady current. We prove that this effect (predicted for highmobility 2D electron systems based on the conventional semiconductors by Dyakonov and Shur [25]) persists for graphene with its unusual hydrodynamics. We find the ultimate increment of plasma waves and show that this instability could be realized in graphene channels of submicron length. The work is organized as follows. In Section 9.2 we derive the set of hydrodynamic equations and discuss the terms arising due to the massless nature of Dirac fermions. In Section 9.3 we demonstrate several solutions of those equations revealing the features of electrons in graphene. In particular, we obtain the profiles of solitary waves in gated graphene, find the spectra of plasma waves in the presence of steady flow, and show the possibility of plasmawave selfexcitation under certain boundary conditions. The main results are discussed in Section 9.4. Some mathematical details concerning the derivation of equations are singled out into Appendix.
9.2 Derivation of Hydrodynamic Equations
We consider 2D plasma of massless electrons in graphene with a linear dispersion law Œp = puF. We assume the Fermi level to be
Derivation of Hydrodynamic Equations
above the Dirac point and neglect the contribution of holes. The starting point for derivation of hydrodynamic equations lies in the construction of the distribution function of carriers which turns the collision integral to zero. Regardless of the energy spectrum Œp this function is 1
È Ê Œp pu  m ˆ ˘ f (p ) = Í1 + exp Á (9.1) ˜˙ , T Ë ¯ ˙˚ ÍÎ where the quantities defined from the hydrodynamic equations are the chemical potential m, the drift velocity u, and the temperature T (measured in the energy units). The set of hydrodynamic equations is obtained by integrating the kinetic equation timed by 1, pi, and Œp over the phase space. The kinetic equation for massless electrons reads ∂f p ∂f ∂f +F = St e i { f } + St e e { f }. + uF ∂t p ∂r ∂p
(9.2)
Here Ste–i{f} includes the electronimpurity and electronphonon collision integrals, Ste–e{f} is the electronelectron collision integral, F = e∂j/∂r is the force acting on electron, e = e. The dissipative terms in hydrodynamic equations due to the electronimpurity and electronphonon collisions were discussed in previous works [8, 10], and further will be omitted. It is instructive that all statistical average values like the electron density n = 4Sp fP, flux j = 4Sp vpfp, and internal energy density e = 4Sp Œp fp can be calculated exactly with the distribution function (9.1) when the spectrum Œp is linear (see the derivation in Appendix); namely, n=
n0
È1  u2 / uF2 ˘ Î ˚
j = nu, e=
e0
3/2
,
(9.3)
(9.4)
(9.5) . 5/2 È1  u / uF2 ˘ Î ˚ Here n0 and e0 are the steadystate particle density and energy density, respectively, given by 2
163
164
Hydrodynamic Electron Transport and Nonlinear Waves in Graphene
n0 =
e0 =
2T 2
•
tdt
Ú 1+e
p 2uF2 0 2T 2
•
t m/T
t 2dt
Ú 1+e
p 2uF2 0
t m /T
,
(9.6)
.
(9.7)
For brevity, we introduce the pressure of electron plasma
e , 2 and an analogue of the electron mass density P=
r=
3e
2uF2
.
(9.8) (9.9)
In these notations, the set of hydrodynamic equations takes on the form ∂n ∂(nui ) = 0, + ∂t ∂x i
∂(rui ) ∂’ij ∂j +  en = 0. ∂t ∂xj ∂x i
(9.10)
(9.11)
Equations (9.10) and (9.11) represent the continuity and the Euler equation, respectively. The elements of stress tensor are (the velocity u is directed along x axis) ’ xx = P ÎÈ1 + 2(u / uF )2 ˘˚ ,
’ yy = P ÎÈ1  2(u / uF )2 ˚˘ .
(9.12)
(9.13)
The heat transfer equation (which will not be discussed here in detail) reads ∂(rui ) ∂e ∂j + uF2 + enui = 0. ∂x i ∂t ∂x i
(9.14)
It is important that the electron sheet density n arises in the continuity equation, while the mass density r arises in the Euler equation. Those quantities are not directly proportional to each other as it is impossible to introduce a constant electron effective mass m. In other words, the fictitious particle mass M = r/n is
Derivation of Hydrodynamic Equations
density and velocitydependent and cannot be factored out of the differential operator. In the degenerate electron system (m ≫ T) the expression for mass reads M=
m / uF2
1  u2 / uF2
.
(9.15)
To recognize the peculiarities of the Euler equation obtained and analyze the emerging nonlinearities, it would be convenient to present it in the canonical form (hereafter we restrict ourselves to onedimensional motion). Excluding the time derivatives of density r with the use of Eqs. (9.3) and (9.5) [see also Eqs. (9.A5) and (9.A6)], we arrive at the following equation: ∂u È b 2 (5  6x) ˘ ∂u È b 2 (5  6x) ˘ ˙ Í1 + ˙ + u Í(3  4x) 2 ∂t ÎÍ ∂x ÍÎ 1 b 1  b 2 ˙˚ ˙˚ 2xuF2 ∂n n ∂(ej ) + (1  b 2 ) = 0. 3n ∂x r ∂x
(9.16)
Here we have introduced the relativistic factor b = u/uF and the dimensionless function x characterizing the thermodynamic state of the electron system, x=
n2
e e 1
,
(9.17)
where ·e–1Ò π e–1 is the density of inverse energy [see Eq. (9.A4)]. The function x varies from 1/2 at m/T Æ – • to 3/4 at m/T Æ + •. At m ≫ T it is given by the following asymptotic relation: xmT =
n ˆ 3Ê 12 T ˜. 4 ÁË n¯
(9.18)
Here nT is the density of thermally activated electrons at m = 0. In hydrodynamic equations for massive particles, two sources of nonlinearities exist: the currentdensity term in continuity equation, ∂x (nu), and the nonlinearconvection term in Euler equation, u∂xu. Much greater variety of nonlinearities is involved in the Euler equation for electrons in graphene (9.16). They can be classified as relativistic nonlinearities due to high drift velocities and nonlinearities due to density dependence of hydrodynamic mass
165
166
Hydrodynamic Electron Transport and Nonlinear Waves in Graphene
M. To compare their ‘strength,’ we consider small perturbations of density, velocity, and electric potential: n = n0 + dn(x, t), u = du(x, t), j = j0 + dj(x, t). It is easy to see that the relativistic nonlinearities are, at least, the thirdorder terms. Dropping them, we can rewrite the Euler equation as ∂u ∂u 1 È 1 ∂P ∂(ej ) ˘ + u ( 3  4x) + = 0. ∂t ∂x ∂x ˙˚ M ÍÎ n ∂x
(9.19)
The nonlinear convection term in Euler equation is weakened due to the factor 3 – 4x < 1. In degenerate electron system this term can be estimated as 6
nT n s2 ∂dn ∂du du ª 6 T 02 dn . n0 n0 n0 dx dx
(9.20)
Here s0 is the velocity of collective excitations (plasma waves) in graphene. At low temperatures and elevated Fermi energies this term becomes infinitesimal and surrenders to the higherorder nonlinearity u3dxu. In comparison with the convective term, the nonlinearity due to the density dependent mass (M µ n1/2) is much stronger. The corresponding term could be evaluated as 
s02 1 dn È 1 ∂P ∂(ej ) ˘ ∂dn dÍ dn . ª ˙ ∂x ˚ 2M n0 Î n0 ∂x ∂x 2n02
(9.21)
It is readily seen from the above considerations that nonlinear transport phenomena in graphene are rather governed by the density dependence of mass M than by nonlinear convection, which used to occur in common semiconductors.
9.3 Nonlinear Effects in PlasmaWave Propagation
9.3.1 Formation of Solitons in Gated Graphene In gated structures the electron density n is related to the local electric field –∂j/∂x in graphene via a weak nonlocality approximation (see derivation in Appendix B, and also Ref. [25])
Nonlinear Effects in PlasmaWave Propagation
4pe2d1d2 ∂n 4pe2d12d22 ∂3n ∂(ej ) =. k(d1 + d2 ) ∂x 3k(d1 + d2 ) ∂x 3 ∂x
(9.22)
Here d1 and d2 are distances from the graphene layer to the top and bottom gates, respectively, and k is the gate dielectric permittivity. The first term on the righthand side simply follows from Gauss’s theorem for uniform electron density. The third derivative term is associated with a weak nonuniformity of charge in 2D layer; it accounts for a weak dispersion of plasma waves in gated structures. A subtle balance between dispersion and nonlinearity results in the formation of solitary waves. We search for the solutions of hydrodynamic equations in the form n = n0 + dn(z), u = du(z), where z = x – u0t is the running coordinate, and u0 is the soliton velocity being slightly different from the plasmawave velocity s0 due to the dispersion. Within the hydrodynamic model, the expression for plasmawave velocity can be represented as [8] s02 = uF2
ˆ 2x Ê 4pe2 d1d2 1+ e 1 ˜ . Á 3Ë k d1 + d2 ¯
(9.23)
Integration of the continuity equation (9.10) provides the relation between u and n: u = u0
n  n0 . n
(9.24)
Eliminating the drift velocity u and the electric potential j from the Euler equation (9.16) with the help of Eqs. (9.22) and (9.24), we arrive at the dynamic equation for a solitary wave. The latter is concisely represented in the limit m ≫ T using the dimensionless variables V = z 3 /(d1d2 ), v = dn / n0 , b = u / uF , b0 = u0 / uF , s0 = s0 / uF as follows: F (v )
∂v Ê 2 1 ˆ ∂3v + s0  ˜ 3 = 0, ∂z ËÁ 2 ¯ ∂z
F (v ) = s02 
b 0 b 2 ( b + b0 ) 1 2 2(v + 1)3/2 (1  b 2 )
(9.25)
167
168
Hydrodynamic Electron Transport and Nonlinear Waves in Graphene
+
1  b2 2 v +1

b02 (v + 1)3/2
(9.26)
.
Upon expanding F(v) in series over v, one arrives at the wellknown Korteweg–de Vries [34] (KdV) equation
(s
2 0
 b02
) ∂z∂v + ËÁÊ s
2 0
1ˆ ∂3 v Ê 3 1 ˆ ∂v  ˜ 3 + Á b02  ˜ v = 0. Ë2 2 ¯ ∂z 4 ¯ ∂z
(9.27)
The solutions of this equation correspond to the socalled bright solitons; their shape is given by [35] Èz s02 dnmax 3 dn(z) = dnmax cosh–2 Í 2 2 Í 2 d1d2 2s0  uF n0 Î
˘ ˙. ˙ ˚
(9.28)
The maximum soliton height dnmax is bound to its velocity u0 via dnmax =
The soliton width W is
W =2
n0 u02  s02 . 2 s02
d1d2 2s02  uF2 dnmax . 3 n0 s02
(9.29)
(9.30)
Because dnmax ≪ n0, and s02 > uF2 / 2 , the soliton width can be much greater than the distance to the gates, which justifies the applicability of weak nonlocality approximation. Besides, the soliton width should markedly exceed the inelastic (electronelectron) free path to justify the validity of hydrodynamic approach. The free path is less than 100 nm, which follows from the experimental [5, 6] and theoretical [8] estimates of collision frequencies. Apart from the numerical coefficients, the obtained parameters of solitons coincide with those in 2D plasma of massive electrons in Ref. [25]. To reveal the unique features of graphene electron hydrodynamics, one should go beyond the condition dn ≪ n0 and analyze the general expression for F(v ). The necessity of rigorous treatment arises when the velocity u approaches the Fermi velocity, i.e., already at dnmax/n0 ª uF/s0. The numerical solution of Eq. (9.25) shows that solitons exist when the maximum particle density dnmax lies below a certain critical
Nonlinear Effects in PlasmaWave Propagation
density. The higher is the plasmawave velocity s0, the lower is the critical density. The relation between dnmax and soliton velocity u0 – s0 is plotted in Fig. 9.1, the termination of the curves corresponds to the critical density and velocity. It is seen from Eq. (9.28) that the soliton width shrinks as its amplitude increases. The numerical results of solving the rigorous KdV equation (9.25) plotted inside the insets in Fig. 9.1 indicate that the width of soliton decreases only slightly as its amplitude grows. Given the value of dnmax, the profile of real soliton is broader than that obtained from ‘nonrelativistic’ approximation (9.27).
Figure 9.1 Dependence of soliton amplitude dnmax/n0 on its velocity (u0 – s0)/ uF at different velocities of plasma waves, s0. The dashed black line indicates the boundary of soliton existence. The profiles of solitary waves obtained from numerical integration of Eq. (9.25) are plotted in the insets.
9.3.2 ‘ShallowWater’ Plasma Waves in the Presence of Steady Electron Flow To obtain the spectra of plasma waves in the presence of steady flow with velocity u0 we linearize the hydrodynamic equations assuming a harmonic time dependence of perturbations n = n0 + dn( x )e iwt ,
u = u0 + du( x )e iwt .
(9.31)
(9.32)
This procedure leads to the ‘equations of motion’ for plasma oscillations,
169
170
Hydrodynamic Electron Transport and Nonlinear Waves in Graphene
∂du ∂dn + u0 = 0, ∂x ∂x
iwdn + n0 iw[1 + g ]d u + u0
(9.33)
s2 ∂dn ∂du [3  4x0  g ]+ 0 = 0, ∂x n0 ∂x
where we have introduced another relativistic factor g : g =
b02
1  b02
(5  6x0 ).
A weak dispersion of plasma waves was neglected here.
(9.34) (9.35)
m
m m
m m m
Figure 9.2 Dependencies of plasmawave velocities s± in the presence of steady flow on the flow velocity u0.
Assuming a harmonic dependence of all quantities on the coordinate, that is µeikx, we obtain the linear law of plasmawave dispersion w± = s±k. The velocities of forward (s+) and backward (s–) waves are given by s± =
2u0 (1  x ) ± s02 (1 + g ) + u02 (2x  1 + g )2
1+g
.
(9.36)
Nonlinear Effects in PlasmaWave Propagation
This relation distinctly manifests the lack of Galilean invariance in the graphene hydrodynamic equations. On the contrary, in 2D plasma of massive electrons, the velocities sm± are given by sm ± = u0 ± s0 .
(9.37)
In graphene, the presence of steady flow modifies the properties of electron system; therefore, the plasmawave velocity s± depends on the flow velocity in a quite complicated manner described by Eq. (9.36). Particularly, when the flow velocity is small (b0 ≪ 1), we obtain s± = 2u0 (1  x ) ± s0 .
(9.38)
In a limit of strongly degenerate electrons (x = 3/4), the velocity of plasma waves is reduced to 1 s± = u 0 ± s0 . 2
(9.39)
The factor 1 /2 formally originates due to the vanishing nonlinear convective term in the Euler equation. In case of large drift velocities u0, the sign of convective term in Eq. (9.16) can switch from positive to negative. This, in its turn, leads to a decrease in wave velocity s+ with rising flow velocity. An increase in fictitious mass M also contributes to this process. The wave velocities s± obtained from Eq. (9.36) are plotted in Fig. 9.2 for different values of chemical potential, and for flow velocities ranging from zero up to uF. An unusual ‘halved’ drag by the flow at small velocities turns to a decrease in wave velocity at large u0. Formally, at u0 = uF the velocities of both branches converge to s± = ±uF. However, this case is of purely academic interest as such fast flows are unattainable owing to velocity saturation [36].
9.3.3 Excitation of Electron PlasmaWaves by Direct Current
A special kind of plasmawave instability (Dyakonov–Shur instability) occurs in highmobility fieldeffect transistors under the condition of constant drain current [26]. An amplification of plasmawave amplitude occurs after the reflection from the drain end. The corresponding increment w’’m (for 2D plasma of massive electrons)
171
172
Hydrodynamic Electron Transport and Nonlinear Waves in Graphene
was shown to be governed by the ratio of forward and backwardwave velocities: w m¢¢ =
s02  u02 È s0 + u0 ˘ ln Í ˙. 2Ls0 Î s0  u0 ˚
(9.40)
This plasmawave instability leads to radiation of electromagnetic waves due to oscillations of image charges in metal electrodes [37]. To find out whether such instability persists for the unusual electron dynamics in graphene, we solve Eqs. (9.33) and (9.34) with the boundary conditions dn x =0 = 0, ÈÎn0d u + u0d n˚˘ = 0. x =L
(9.41)
The latter condition corresponds to a constant drain current. This can be realized either for transistors operating in the currentsaturation mode [36], or with the help of an external circuit sustaining the constant current. It is easy to show that the complex eigenfrequencies wn = w’n + iw’’n of Eqs. (9.33) and (9.34) with boundary conditions (9.41) are w n¢ =
s02  u02 (3  4x  g ) pn , 2L s2 (1 + g ) + u2 (2x  1 + g )2 0 0 ¢¢ w n=1 =
ª
¢ s w n=1 ln + sp
s02  u02 (3  4x  g ) 2u0 (1  x ) . L s02 (1 + g ) + u02 (1  2x  g )2
(9.42)
(9.43)
The imaginary part of the complex frequency is positive, which means an amplification of the waves. We also see that for the existence of instability it does not matter whether the spectrum of electrons is parabolic or linear. The instability persists if only the velocities of forward and backward plasma waves are different. At the same time, compared with massive particles, the wave increment (9.43) is smaller due to a smaller difference in wave velocities [s+ – s– ª u0 for degenerate massless electrons instead of 2u0 for massive electrons]. As the flow velocity u0 increases (b0 ≳ 1/2), the wave increment begins to fall down because the velocity difference decreases.
Discussion of the Results
The ultimate wave increment in such kind of instability is estimated as uF/(4L), which is attained at u0 ≃ uF/2 (see Fig. 9.3). For the selfexcitation to arise, it should exceed (2tp)–1, where tp is the momentum relaxation time. Considering the highquality samples, where scattering from acoustic phonons dominates, we can estimate tp–1 ª 3 ¥ 1011 s–1 at room temperature [38]. The selfexcitation turns out to be possible for channel lengths L ≲ 1.5 mm. This optimistic anticipation could be hampered by the presence of impurity scattering, velocity saturation, and dependence of relaxation time on electron density. Nevertheless, even for shorter channels the hydrodynamic approach is valid and the selfexcitation seems plausible. m m m
Figure 9.3 Dependence of wave increment w1¢¢ on flow velocity u0 at different values of Fermi energy.
9.4 Discussion of the Results We have derived hydrodynamic equations describing the transport of massless electrons in graphene. A linear energy spectrum of carriers should be taken into account from the very beginning of derivation. It cannot be introduced as a small correction to the parabolic dispersion (like p4 terms in Si, Ge, A3B5 [39]). On the other hand, the hydrodynamic equations for ultrarelativistic plasmas cannot be also directly applied to graphene as the Fermi velocity is much smaller compared to that of light.
173
174
Hydrodynamic Electron Transport and Nonlinear Waves in Graphene
The dependence of particle density n on drift velocity u [(Eq. (9.3)] may look confusing. However, it is the immediate consequence of the particular choice of distribution function (9.1). At the same time, one can choose the distribution function in the form 1
È Ê puF  pu mˆ˘ f (p) = Í1 + exp Á  ˜˙ . 2 2 3/ 4 T ¯˙ Ë T (1  u / uF ) ˚ ÎÍ
(9.44)
This function turns collision integral to zero, reduces to the equilibrium Fermi function at u Æ 0, and the corresponding particle density does not depend on u (but the internal energy still does). It is easy to show that Euler and continuity equations derived with this function and written in terms of n and u coincide with Eqs. (9.11) and (9.10). The equation of state also holds its view. The boundary conditions for hydrodynamic equations are imposed on measurable quantities n and u. Hence, the solutions of hydrodynamic equations do not depend on the choice between distribution functions (9.1) and (9.44). In the obtained hydrodynamic equations for electrons in graphene, the effect of linear spectrum is clearly visible. First, the drift velocity u cannot overcome the Fermi velocity uF . Secondly, a
varying fictitious hydrodynamic mass M ª ( m / uF2 )/ 1  u2 / uF2 originates in the Euler equation. The obtained equations are neither Lorentz nor Galilean invaraint, which is directly revealed in the spectra of plasma waves in the presence of steady electron flow [Eq. (9.36)]. Our main conclusions concerning the spectra can be verified experimentally using the techniques of plasmon nanoimaging [30] in gated graphene under applied bias. As we became aware recently, the spectra of plasma waves in the presence of steady flow and Dyakonov–Shur instability in graphene were analyzed in Ref. [9]. The form of Euler equation used was different from our Eq. (9.16) even in the limit u ≪ uF; particularly, in Ref. [9] the gradient term u∂xu did not vanish for degenerate electron systems. This led to different expression for plasmawave velocities (3u0/4 ± u0 instead of our s±), and to higher estimate of the plasmawave instability increment. One possible reason for the distinction of the Euler equations lies in dissimilar expressions for the electron plasma pressure P, which is substantially velocity dependent [see Eqs. (9.A2) and (9.A3): P = e/2 µ m3/(1 – b 2)5/2].
Conclusions
The set of problems which could be solved via nonlinear hydrodynamic equations is not restricted within plasma waves. It would be also interesting to study the effects of velocity saturation associated with the upper limit of drift velocity u equal to uF. Those effects could be pronounced in graphene samples on substrates with high optical phonon energy. If it is the case, the velocity saturation caused by emission of optical phonons [36] seems as irrelevant. For rigorous simulation of emerging graphenebased devices for THz generation and detection [21] one can as well employ the derived nonlinear equations. In the case, however, an Euler equation for holes and electronhole friction terms should be supplied [8]. With large electron mobility and new hydrodynamic nonlinearities, graphenebased THz devices could outperform those based on conventional semiconductors.
9.5 Conclusions
The hydrodynamic equations governing the collective motion of massless electrons in graphene were derived. The validity of those equations is not restricted to small drift velocities. A variable fictitious mass depending on density and velocity arises in the hydrodynamic equations. It results in several nonlinear terms specific to graphene. The possibility of soliton formation in electron plasma of the gated graphene was shown. The quasirelativistic terms in the dynamic equations set an upper limit of the soliton amplitude and stabilize its shape. The obtained hydrodynamic equations demonstrate a lack of Galilean and true Lorentz invariance. This noninvariance is pronouncedly revealed in the spectra of plasma waves in the presence of steady flow with velocity u0. The difference in velocities of forward and backward waves turns out to be u0 instead of 2u0, expected for massive electrons in conventional semiconductors. The possibility of plasmawave selfexcitation in highmobility graphene samples under certain boundary conditions (Dyakonov– Shur instability) was demonstrated. The increment of such instability in graphene is less than that in common semiconductors due to smaller difference in velocities of forward and backward waves. However, the high mobility of electrons in graphene allows plasmawave selfexcitation for micronlength and shorter channels.
175
176
Hydrodynamic Electron Transport and Nonlinear Waves in Graphene
Acknowledgement The work of D.S. and V.V. was supported by the Russian Ministry of Education and Science (Grant No. 14.132.21.1687), the Russian Foundation for Basic Research (Grant No. 110700464), and Russian Academy of Science. The work at RIEC was supported by the Japan Science and Technology Agency, CREST and by the Japan Society for Promotion of Science. The authors are grateful to S.O. Yurchenko for helpful discussions, and to Prof. M. Polini for valuable comments.
Appendix A: Calculation of Average Values
The statistical average values can be exactly calculated with the distribution function (9.1) for linear energy spectrum. The particle density is given by n=
=
4
(2p )
2
Ú
pdpdq
p(uF ucosq )m T 1+e
Ï • 2ptdt Ô Ì (p uF )2 Ô 0 1 + et m /T Ó T2
Ú
2p ¸Ï dq ÔÔ 1 Ô¸ . ˝Ì 2˝ Ô˛ ÔÓ 2p 0 [1  b cosq ] Ô˛
Ú
(9.A1)
The last term could be evaluated as [1 – b2] –3/2, while the remainder is nothing more but the particle density in the absence of flow n0. Similarly, the energy density reads as follows: e=
• 2 ÔÏ 2pt dt Ì (p uF )2 Ô 0 1 + et m/T Ó
T3
Ú
=
The stress tensor is
’ xx =
¸Ï 1 2p dq Ô¸ ÔÔ ˝ÌÌ ˝ 2p [1  b cosq ]3 Ô ÔÔ 0 ˛Ó ˛
Ú
e0 [1  b 2]5/2
4 (2p )2
Ú
.
uF p2 cos2 qdpdq 1+e
p(uF ucosq )m T
(9.A2)
Appendix B
=
2 Ï• Ô 2p t dt 2 Ì t m/T (p uF ) Ô 0 1 + e Ó
T3
Ú
¸Ï 2p cos2 q dq ¸ ÔÔ 1 Ô ˝Ì 3˝ 2p [1 ] b cosq ÔÔ Ô˛ 0 ˛Ó
Ú
e = (1 + 2b 2 ). 2
(9.A3)
The density of inverse energy ·e–1Ò can be expressed in terms of elementary functions e 1 =
2T ln [1 + e m/T ]
p 2uF2 1  u2 / uF2
.
(9.A4)
The following relations for the derivatives of average values are required to represent the Euler equation in the canonical form: dn =
1
1  b2
de =
( e 1 dm + 3nb db ),
1 1  b2
(2nd m + 5eb db ).
(9.A5)
(9.A6)
Appendix B: Weak Nonlocality Approximation for Poisson Equation One solves the Poisson equation for the gated 2D electron gas (2DEG). The 2DEG plane is z = 0, the grounded top and bottom gates are placed at z = d1 and z = –d2, respectively, and the top and bottom dielectric permittivities are k1 and k2. We assume that electron density in 2DEG varies only in the x direction and write the Poisson equation as ∂2j ∂x 2
+
∂2j ∂z 2
= 0,
with boundary conditions
j z = d1 = j z = d2 = 0, j z =+0 = j z =0 ,
k 1 ∂j/∂z z =+0 k 2∂j/∂z z=0 = 4ps .
(9.B1)
(9.B2)
(9.B3) (9.B4)
177
178
Hydrodynamic Electron Transport and Nonlinear Waves in Graphene
Here s = –en is the 2D charge density, and n is the electron density.
After the Fourier transform j k = equation becomes k 2j k +
∂2j k
∂z 2
Ú
+•
•
j( x , z)e ikx dx the Poisson
= 0 .
(9.B5)
Solving Eq. (9.B5) with boundary conditions (9.B2)–(9.B4), which apply to the Fourier components as well, we obtain j kz=0 =
4ps k . k[k 1 coth( kd1 ) +k 2 coth( kd2 )]
(9.B6)
Assuming that the 2D electron density varies slowly (kd1 1, kd2 1), we expand Eq. (9.B6) in series over k and arrive at the final solution after inverse Fourier transform: jz=0 =
4ps 4p d1k 1 + d2k 2 ∂2s + . k 2/d2 +k 1 /d1 3 (k 2/d2 + k 1 /d1 )2 ∂x 2
(9.B7)
Equation (9.B7) is further simplified to Eq. (9.22) for equal permittivities of top and bottom gate dielectrics k 1 = k 2 = k.
References
1. V. N. Kotov, B. Uchoa, V. M. Pereira, F. Guinea, and A. H. Castro Neto, Rev. Mod. Phys., 84, 1067 (2012). 2. M. Schutt, P. M. Ostrovsky, I. V. Gornyi, and A. D. Mirlin, Phys. Rev. B, 83, 155441 (2011). 3. A. B. Kashuba, Phys. Rev. B, 78, 085415 (2008).
4. L. Fritz, J. Schmalian, M. Müller, and S. Sachdev, Phys. Rev. B, 78, 085416 (2008). 5. J. M. Dawlaty, S. Shivaraman, M. Chandrashekhar, F. Rana, and M. G. Spencer, Appl. Phys. Lett., 92, 042116 (2008).
6. S. BoubangaTombet, S. Chan, T. Watanabe, A. Satou, V. Ryzhii, and T. Otsuji, Phys. Rev. B, 85, 035443 (2012). 7. G. E. Uhlenbeck and G. W. Ford, Lectures in Statistical Mechanics (Providence, AMS, 1963).
8. D. Svintsov, V. Vyurkov, S. Yurchenko, V. Ryzhii, and T. Otsuji, J. Appl. Phys., 111(8), 083715 (2012).
9. A. Tomadin and M. Polini, Phys. Rev. B, 88, 205426 (2013).
References
10. R. Bistritzer and A. H. MacDonald, Phys. Rev. B, 80, 085109 (2009).
11. M. Müller, J. Schmalian, and L. Fritz, Phys. Rev. Lett., 103, 025301 (2009). 12. M. Mendoza, H. J. Herrmann, and S. Succi, Sci. Rep., 3, 1052 (2013).
13. M. Müller, L. Fritz, and S. Sachdev, Phys. Rev. B, 78, 115406 (2008).
14. R. Roldan, J. N. Fuchs, and M. O. Goerbig, Solid State Commun., (2013).
15. M. Schütt, P. M. Ostrovsky, M. Titov, I. V. Gornyi, B. N. Narozhny, and A. D. Mirlin, Phys. Rev. Lett., 110, 026601 (2013).
16. J. C. W. Song, D. A. Abanin, and L. S. Levitov, Nano Lett., 13(8), 3631 (2013). 17. S. H. Abedinpour, G. Vignale, A. Principi, M. Polini, W.K. Tse, and A. H. MacDonald, Phys. Rev. B, 84, 045429 (2011).
18. A. I. Akhiezer, V. F. Aleksin, and V. D. Khodusov, Low Temp. Phys., 20, 939 (1994). 19. E. Vostrikova, A. Ivanov, I. Semenikhin, and V. Ryzhii, Phys. Rev. B, 76, 035401 (2007).
20. S. Rudin, G. Samsonidze, and F. Crowne, J. Appl. Phys., 86, 2083 (1999). 21. L. Vicarelli, M. S. Vitiello, D. Coquillat, A. Lombardo, A. C. Ferrari, W. Knap, M. Polini, V. Pellegrini, and A. Tredicucci, Nat. Mater., 11, 865 (2012).
22. A. Barreiro, M. Lazzeri, J. Moser, F. Mauri, and A. Bachtold, Phys. Rev. Lett., 103, 076601 (2009).
23. C. X. Zhao, W. Xu, and F. M. Peeters, Appl. Phys. Lett., 102, 222101 (2013).
24. A. V. Chaplik, Zh. Eksp. Teor. Fiz., 62, 746 (1972) [Sov. Phys. JETP, 35, 395 (1972)]. 25. A. O. Govorov, V. M. Kovalev, and A. V. Chaplik, JETP Lett., 70, 488 (1999).
26. M. I. Dyakonov and M. S. Shur, Phys. Rev. Lett., 71, 2465 (1993). 27. M. I. Dyakonov and M. S. Shur, Phys. Rev. B, 51, 14341 (1995).
28. A. N. Grigorenko, M. Polini, and K. S. Novoselov, Nat. Photonics, 6, 749 (2012). 29. L. Ju, B. Geng, J. Horng, C. Girit, M. Martin, Z. Hao, H. A. Bechtel, X. Liang, A. Zettl, Y. Ron Shen, and F. Wang, Nat. Nanotechnol., 6, 630 (2011).
30. Z. Fei, A. S. Rodin, G. O. Andreev, W. Bao, A. S. McLeod, M. Wagner, L. M. Zhang, Z. Zhao, M. Thiemens, G. Dominguez, M. M. Fogler, A. H. Castro Neto, C. N. Lau, F. Keilmann, and D. N. Basov, Nature, 487, 82 (2012).
179
180
Hydrodynamic Electron Transport and Nonlinear Waves in Graphene
31. S. Das Sarma and E. H. Hwang, Phys. Rev. Lett., 102, 206412 (2009).
32. V. Ryzhii, A. Satou, and T. Otsuji, J. Appl. Phys., 101, 024509 (2007).
33. A. Nerses, and E. E. Kunhardt, J. Math. Phys., 39, 6392 (1998). 34. D. J. Korteweg and G. de Vries, Philos. Mag., 5, 422 (1895).
35. E. M. Lifshitz and L. P. Pitaevsky, Physical Kinetics (Pergamon Press, Oxford, 1981). 36. I. Meric, M. Y. Han, F. A. Young, B. Ozyilmaz, P. Kim, and K. L. Shepard, Nat. Nanotechnol., 3, 654 (2008). 37. W. Knap, J. Lusakowskia, T. Parenty, S. Bollaert, A. Cappy, V. V. Popov, and M. S. Shur, Appl. Phys. Lett., 84, 2331 (2004).
38. F. T. Vasko and V. Ryzhii, Phys. Rev. B, 76, 233404 (2007).
39. D. L. Woolard, H. Tian, R. J. Trew, M. A. Littlejohn, and K. W. Kim, Phys. Rev. B, 44, 11119 (1991).
Chapter 10
Effect of SelfConsistent Electric Field on Characteristics of Graphene pin Tunneling TransitTime Diodes*
V. L. Semenenko,a V. G. Leiman,a A. V. Arsenin,a V. Mitin,b M. Ryzhii,c,d T. Otsuji,d,e and V. Ryzhiid,e aDepartment
of General Physics, Moscow Institute of Physics and Technology, Dolgoprudny, Moscow Region 141700, Russia bDepartment of Electrical Engineering, University at Buffalo, Buffalo, New York 14601920, USA cComputational Nanoelectronics Laboratory, University of Aizu, AizuWakamatsu 9658580, Japan dJapan Science and Technology Agency, CREST, Tokyo 1070075, Japan eResearch Institute for Electrical Communication, Tohoku University, Sendai 9808577, Japan [email protected].
*Reprinted with permission from V. L. Semenenko, V. G. Leiman, A. V. Arsenin, V. Mitin, M. Ryzhii, T. Otsuji, and V. Ryzhii (2013). Effect of selfconsistent electric field on characteristics of graphene pin tunneling transittime diodes, J. Appl. Phys., 113, 024503. Copyright © 2013 American Institute of Physics. GrapheneBased Terahertz Electronics and Plasmonics: Detector and Emitter Concepts Edited by Vladimir Mitin, Taiichi Otsuji, and Victor Ryzhii
Copyright © 2021 Jenny Stanford Publishing Pte. Ltd.
ISBN 9789814800754 (Hardcover), 9780429328398 (eBook)
www.jennystanford.com
182
Effect of SelfConsistent Electric Field on Characteristics of Graphene
We develop a device model for pin tunneling transittime diodes based on single and multiple graphene layer structures operating at the reverse bias voltages. The model of the graphene tunneling transittime diode (GTUNNETT) accounts for the features of the interband tunneling generation of electrons and holes and their ballistic transport in the device isection, as well as the effect of the selfconsistent electric field associated with the charges of propagating electrons and holes. Using the developed model, we calculate the dc currentvoltage characteristics and the smallsignal ac frequencydependent admittance as functions of the GTUNNETT structural parameters, in particular, the number of graphene layers and the dielectric constant of the surrounding media. It is shown that the admittance real part can be negative in a certain frequency range. As revealed, if the isection somewhat shorter than one micrometer, this range corresponds to the terahertz frequencies. Due to the effect of the selfconsistent electric field, the behavior of the GTUNNETT admittance in the range of its negativity of its real part is rather sensitive to the relation between the number of graphene layers and dielectric constant. The obtained results demonstrate that GTUNNETTs with optimized structure can be used in efficient terahertz oscillators.
10.1 Introduction
Pioneering papers by Shur and Eastman [1, 2] have stimulated extensive studies (which continue already for the fourth decade) of ballistic electron and hole transport (BET and BHT, respectively), i.e., collision free transport in short semiconductor structures. The main incentive is the realization of fastest velocities of electrons/holes and, hence, achievement of the operation of diodes and transistors in terahertz range (THz) of frequencies and low power consumption. Even at the initial stage of the ballistic transport research, several concepts of ballistic THz sources have been put forward (see, for instance, an early review [3]). However, the realization THz generation in different semiconductor devices associated with BET/BHT, in particular, analogous to vacuum devices, meets the problems associated with electron scattering in real semiconductor structures. Creation of heterostructures with selective doping with
Introduction
a twodimensional electron gas (2DEG) spatially separated from the donors has resulted in achievement of very long mean free path of electrons, at least at low temperatures. Recent discoveries of unique properties of graphene [4, 5], in particular, the demonstration of possibility of very long electron and hole mean free path in graphene layers (GLs) and what is even more interesting in multiple graphene layers (MGLs) [6, 7] add optimism in building graphene based THz devices using BET. The concept of graphene tunneling transittime (GTUNNETT) pin diode, which exhibits a negative dynamic conductivity in the THz range, was proposed and substantiated in Refs. [8, 9]. This concept based not only on BET or quasiBET (as well as BHT or quasiBHT) in GLs and MGLs but also on a strong interband tunneling under the electric field with a pronounced anisotropy [10, 11] due to the gapless energy spectrum, and constant absolute value of electrons and holes velocities [4]. Due to this, the electrons in the conduction band and the holes in the valence band generated owing to the interband tunneling in the electric field propogate primarily in the electric field direction with the velocity (in this direction) virtually equal to the characteristic velocity uW 108cm/s. A large value of the directed velocity in GLs and MGLs promotes the device operation at elevated frequencies. As shown (Refs. [8, 9]), for the selfexcitation of THz oscillations in a circuit with GTUNNETT diode, this circuit should serve as a resonator. However, at elevated tunneling currents in GTUNNETTs considered previously [8, 9] the selfconsistent charge associated with propagating electron and hole streams can affect the spatial distribution of the selfconsistent electric field and the electric potential in the isection. As a result, the selfconsistent electric field near the pi and injuctions can be substantially reinforced. This, in turn, influences the tunneling generation of electrons and holes and their transit conditions and, hence, the GTUNNETT dc and ac characteristics. In this chapter, in contrast to the previous treatment [8, 9], we account for the selfconsistent electric field associated with the variations of the electron and hole lateral charges in the isection and their effect on the injection and the dc and ac characteristics. The effects of the space charge in planar TUNNETTs with the propagation of carriers perpendicular to the structure plane were considered by Gribnikov et al. [12]. The problems of calculation of the dc and ac
183
184
Effect of SelfConsistent Electric Field on Characteristics of Graphene
characteristics of devices based on lateral structures accounting for the selfconsistent electric field are substantially complicated by the features of the structure geometry (2D electron and hole channels and bladelike contact regions). In particular, as shown in the following, the related mathematical problems are reduced to a system of rather complex nonlinear integraldifferential equations. Using the GTUNNETT device model, we derive these equations, solve them numerically, and find the characteristics.
10.2 Equations of the Model
The device under consideration is based on a GL or MGL structures with p and nside sections with the contacts and an undoped transit isection. For definiteness, we assume that p and nsections in a GL or in an MGL are created by chemical doping [13], although in similar devices but with extra gates, these sections can be formed electrically [10, 11]. Under the reverse bias voltage V0, the potential drops primarily across the isection A schematic view of the structures in question and their banddiagram under sufficiently strong reverse bias (V0 > 0) corresponding to the potential distribution in the isection with a markedly nonuniform electric field are shown in Fig. 10.1. The electrons and holes injected into the isection of one GL are characterized by the electron and hole sheet concentrations, S– = S–(t, x) and S+ = S+(t, x), respectively, and the potential j = j (t, x, y). Here, the axis x is directed along the GL (or MGL) plane, i.e., in the direction of the current, the axis y is directed perpendicular to this plane, and t is the time. In the general case when the isection is based on MGL, S– = S–(t, x) and S+ = S+(t, x) are the electron and hole densities in each GLs. In the case of BET and BHT, on which we focus mainly, the electron and hole sheet densities in each GL obey the continuity equations ∂Â ∂S ± vw = g, ∂t dx
and the Poisson equation ∂2F ∂x
2
+
∂2F ∂y
2
=
4p eK ( S  S + ) ◊d ( y ), æ
(10.1)
(10.2)
Equations of the Model
respectively. Here, e =e  is the electron charge, æ is the dielectric constant of the media surrounding GL (or MGL structure), K is the number of GLs in the GTUNNETT structure, and d(y) is the delta function reflecting a narrowiness of GL and MGL structures even with rather large number of GLs in the ydirection. Equation (10.1) corresponds to the situation when the electrons and holes generated due to the interband tunneling in the isection obtain the directed velocities ux = uW and ux = –uW and preserve them
(a)
(b)
(c)
Figure 10.1 Schematic views of GTUNNETT pin diodes (a) with a single GL, (b) with an MGL structure, and (c) their band diagram at reverse bias. Arrows show the propagation directions of electrons and holes generated due to interband tunneling (mainly in those regions, where the electric field is relatively strong).
during the propagation. The boundary conditions correspond to the assumption that the electrons and holes appear in the isection only due to the interband tunneling (the injection of electrons from the psection and holes from the nsection is negligible) and that the
185
186
Effect of SelfConsistent Electric Field on Characteristics of Graphene
highly conducting side contacts to the p and nsections are of blade type (the thicknesses of GL and MGL and the contacts to them are much smaller than the spacing between the contacts) S
x = l
= 0, S +
F x£l , y=0 = V /2,
x =+ l
= 0,
F x≥ +l , y=0 = V /2,
(10.3)
(10.4)
where 2l is the length of the isection and V = V0 + dVw exp(–iwt) is the net voltage, which comprises the bias voltage V0 and the signal component with the amplitude dV and the frequency w. The interband tunneling generation rate of electrons and holes in each GL (per unit of its area) is given by [8–11] Ê 2l ∂j / ∂x ˆ g = g0 Á ˜ V0 Ë ¯
3/2
,
where j(x) = F(x, y)y=0, ћ is the Planck constant v Ê eV0 ˆ g0 = W2 Á ˜ 2p Ë 2l vW ¯
(10.5)
3/2
,
so that the characteristic tunneling dc current (per unit length in the transverse zdirection) and the characteristic electron and hole sheet density can be presented as S0 = 2lg0/uW.
J00 = 4elg0,
From Eq. (10.2) with boundary condition (10.4), for the potential j(x) in the GL (or MGL structure) plane, we obtain j( x ) =
where
V Ê x ˆ Ke sin 1 Á ˜ + Ë l¯ æ p
Ú
l
l
Ê x x¢ ˆ [ S + ( x¢ ) S  ( x¢ )]G Á , ˜ dx¢¢ , (10.6) Ël l¯
Ê x x ¢ ˆ 1 sin[(cos 1 x + cos 1 x¢) / 2] GÁ , ˜ = . Ë l l ¯ 2p sin[(cos 1 x  cos 1 x ¢) / 2]
(10.7)
Introducing the dimensionless quantities: n∓ = S∓/S0, x = x/l, x¢ = x¢/l, and t = uWt/l, Eqs. (10.1) and (10.6) can be reduced to the following system of nonlinear integrodifferential equations:
Equations of the Model
∂n ∂n ÈÍ V / V0 ± = +g ∂t ∂x Í p 1  x 2 Î ¥ Here,
g =
Ú
1
[n+ (x¢ ,t )  n (x¢ ,t )]
1
˘ ∂ G(x , x¢)dx¢ ˙ ∂x ˚
3/2
2Kel S 0 Ke2 = 2 æV0 4p ævW
.
2leV0 , vW
1  x ¢2 1 ∂ G(x , x ¢) = . ∂x p (x ¢  x) 1  x 2
(10.8) (10.9) (10.10)
The term with the factor g in the righthand side of Eq. (10.8) is associated with the contributions of the electron and hole charges to the selfconsistent electric field in the isection. The dc and ac components of the terminal dc and ac currents, J0 and dJw, are expressed via the dc and ac components n0 and dnw as follows: J0 = evW K S 0 (n0+ + n0 ),
d Jw = evW K S 0
Ú
1
1
r(x )(d nw+ + dnw ) dx  iw CdVw .
(10.11)
(10.12)
Here, r(x ) = 1 / p 1  x 2 is the form factor and C ~ æ/2p2 is the geometrical capacitance [14, 15]. The explicit coordinate dependence of the form factor is a consequence of the Shocley–Ramo theorem [16, 17] for the device geometry under consideration. Hence the GTUNNETT smallsignal admittance Yw = dJw/dVw is presented in the form Yw = evW K S 0
Ú
1
1
r(x )
d (d nw+ + d nw )dx  iwC . ddVw
(10.13)
As follows from Eq. (10.8), the problem under consideration is characterized by the parameter g. If æ = 1.0, K = 1, and 2l = 0.7 mm, in the voltage range V0 = 100 – 200 mV, one obtains S0 (0.6 – 1.7) ¥ 1010 cm–2 and g 0.61 – 0.87.
187
188
Effect of SelfConsistent Electric Field on Characteristics of Graphene
10.3 Spatial Potential Distributions and CurrentVoltage Characteristics If the charges created by the propagating electrons and holes in the isection are insignificant, that corresponds to g 1. In this case, the potential distribution is given by V0 Ê xˆ sin 1 Á ˜ , Ë l¯ p
j0 ( x )
(10.14)
and Eqs. (10.8), neglecting the term with g, can be solved analytically. Taking into account boundary conditions Eq. (10.3), from Eqs. (10.8), we obtain n0+ + n0 =
1
p
3/2
Ú
dx
1
1 (1  x 2 )3/ 4
= const.
(10.15)
After that, using Eq. (10.11) and considering Eq. (10.15), one can find the following formula for the dc currentvoltage characteristic: J0 =
=K
KJ00
p
3/2
1
dx
0
(1  x 2 )3/4
Ú
G(1 / 4)G(1 / 2) evW Ê eV0 ˆ Á ˜ G(3 / 4) p 7/2 2 2l Ë vW ¯
3/2
,
(10.16)
where G(x) is the Gammafunction. A distinction between J0 and J00 is due to the nonuniformity of the electric field in the isection associated with the feature of the device geometry taken into account calculating J0. At K = 1, 2l = 0.7 mm, and V0 = 100 – 200 mV, Eq. (10.16) yields J0 0.18 – 0.51 A/cm. To take the effect of the selfconsistent electric field on the tunneling, one needs to solve system of Eqs. (10.8). Due to a complexity of the nonlinear integrodifferential equations in question, a numerical approach is indispensable. Equations (10.8) were solved numerically using successive approximation method, which is valid when g < gc = 5. In the cases g > 5, the method of the parameter evolution was implemented. Using Eqs. (10.8) and (10.11) and setting V = V0, we calculated numerically the GTUNNETT dc characteristics: spatial distributions of the dc electric potential and the dc components of the electron and hole densities, as well as the dc currentvoltage characteristics. The pertinent results are shown in Figs. 10.2–10.5.
Spatial Potential Distributions and CurrentVoltage Characteristics
Figure 10.2 Spatial distributions of electron and hole concentrations (upper panel) and of electric potential (lower panel) in the GTUNNETT isection.
Figure 10.3 Currentvoltage characteristics for GTUNNETTs with different number of GLs K.
189
190
Effect of SelfConsistent Electric Field on Characteristics of Graphene
Upper panel in Fig. 10.2 shows examples of the spatial distributions of the electron and hole sheet concentrations in the isection. The spatial distributions of the dc electric potential calculated for GTUNNETTs with different numbers of GLs K at fixed voltage are shown in Fig. 10.2 (lower panel). One can see that an increase in K results in a marked concentration of the electric field near the doped sections. This is because at larger K, the net tunneling generation rate becomes stronger. This, in turn, results in higher charges of propagating electron and hole components, particularly, near the pi and injunctions, respectively.
Figure 10.4 Dependences of dc current on dielectric constant for different numbers of GLs K: net current—upper panel and current per one GL—lower panel.
Spatial Potential Distributions and CurrentVoltage Characteristics
Figure 10.3 demonstrates a difference in the dc currentvoltage characteristics in GTUNNETTs with different numbers of GLs K. As can be seen in Fig. 10.3, the dc current becomes larger with increasing K at more than Kfold rate. In paricular, Fig. 10.4 (upper panel) shows the threefold increase in K leads to more than threefold increase in the dc current particularly at relatively small dielectric constants. This is confirmed by plots in Fig. 10.4 (lower panel), from which it follows that the dc current in each GL is larger in the devices with larger number of GLs. Such a behavior of the dc currentvoltage characteristics is attributed to the following. An increase in K leads to an increase in the dc current not only because of the increase in the number of current channels (this would provide just the Kfold rise in the dc current) but because of the reinforcement of the selfconsistent electric field near the edges of the isection (as mentioned above) and, hence, strengthening of the tunneling injection.
Figure 10.5 Dependences of dc current on number of GLs K at different voltages.
It is worth noting that when the dielectric constant is sufficiently large (about 15–20), the dc current in one GL is virtually the same in the devices with different number of GLs, because in this case, the charge effect is suppressed. In this case, the value of the dc current (per one GL) is approximately the same as that obtained in the above numerical estimate using analytical formula given by Eq. (10.16). In
191
192
Effect of SelfConsistent Electric Field on Characteristics of Graphene
GTUNNETTs with a moderate value of a, the charge effect leads to superlinear dependences of the net dc current vs number of GLs as seen in Fig. 10.5.
10.4
GTunnETT Admittance
Disregarding the term in Eq. (10.8) associated with the electron and hole charges in the isection, and using Eq. (10.12), one can obtain analytically the following formulas for the ac potential distribution in the isection, and the imaginary and real parts of the GTUNNETT admittance [9] dj( x )w =
dVw Ê xˆ sin 1 Á ˜ , Ë l¯ p
ImYw = Y0 sin(wt t ) ◊J 0 (wt t )  wC , ReYw = Y0 cos(wt t ) ◊J 0 (wt t ),
(10.17)
(10.18)
(10.19)
where Y0 = dJ0 / dV0 = 3 J0 / 2V0 µ V0 is the dc differential conductivity, C is the geometrical capacitance, tt = l/uW is the characteristic transit time of electrons and holes across the isection, and J0(wt) is the Bessel function. As follows from Eqs. (10.18) and (10.19), the admittance imaginary and real parts oscillate as functions of the transit angle wtt with Re Yw < 0 at wtt near the transit time resonances wtt = (2n – 1/2)p, where n = 1, 2, 3 . . . is the resonance index. The numerical solution of Eqs. (10.8), accounting for the ac components of the applied voltage dVw and the selfconsistent charges and electric field, shows that the oscillatory frequency dependences are preserved in this more realistic case although they are be quantitatively modified. In particular, these dependences vary with varying such parameters as the number of GLs K and dielectric constant æ. The results of numerical calculations using Eq. (10.8) are demonstrated in Figs. 10.6–10.9. Figure 10.6 shows the dependence of the imaginary and real parts, Im Yw and Re Yw, of the admittance on the signal frequency calculated for GTUNNETTs with 2l = 0.7 mm and K = 1 at V0 = 200 mV at different values of dielectric constant æ. As follows from Fig. 10.6, the imaginary and real parts of the GTUNNETT admittance
GTUNNETT Admittance
Figure 10.6 Frequency dependences of imaginary part, Im Yw, and real part, Re Yw, of GTUNNETT admittance (upper and lower panels, respectively) at different values of dielectric constant æ (K = 1 and 2l = 0.7 mm).
are oscillatory functions of the signal frequency [see also Eqs. (10.18) and (10.19)]. The oscillatory behavior is due to the transittime resonances. At sufficiently high frequencies, the admittance imaginary part is negative because it is determined primarily by the geometrical capacitance, so that Im Yw –wC. In the certain frequency ranges, the admittance real part is negative as shown in Fig. 10.6 (lower panel). These ranges correspond to the transittime resonances. As seen from Fig. 10.7, the minima of the admittance real
193
194
Effect of SelfConsistent Electric Field on Characteristics of Graphene
part (where the latter is negative) become deeper and the minima shift toward smaller frequencies with increasing dielectric constant æ. This is because an increase in æ leads to weakening of the effect of the electron and hole charges on the injection and propagation processes. The dashed line corresponds to the case when the role of these charges is diminished (very large æ) considered previously [9].
Figure 10.7 Frequency dependences of real part, Re Yw, of GTUNNETT admittance in the frequency range, where Re Yw < 0 at different values of dielectric constant æ (K = 1 and 2l = 0.7 mm) calculated accounting for electron and hole charges (solid lines) and neglecting them (dashed line) [9].
Figure 10.8 Frequency dependences of real part of admittance Re Yw for GTUNNETTs with different number of GLs K (æ = 10.0 and 2l = 0.7 mm).
Discussion
Figure 10.8 shows the admittance real part vs signal frequency calculated for GTUNNETTs with different number of GLs K. One can see that GTUNNETTs with larger number of GLs K exhibit much more deep minima (compare the curves which correspond to K = 1 and æ = 10.0 in Fig. 10.7 and that for K = 10 and æ = 10.0 in Fig. 10.8.). As follows from this comparison, the tenfold increase in K leads to about fourfold increase in the minimum depth. Figure 10.9 shows the dependence of the minimum value of the real part of the GTUNNETT admittance min {ReYw} on the number of GLs K calculated for different dielectric constants æ. The nonmonotonic character of these dependences is associated with the interplay of the factors determined by the influence of electron and hole charges: an increase in æ leads to a suppression of these charges role, while an increase in K results in proportional reinforcement of the effect of these charges accompanied by proportional increase in the current.
Figure 10.9 Minimum value of real part of GTUNNETT admittance as a function of number of GLs K for GTUNNETTs with different dielectric constant æ.
10.5 Discussion Calculating the dc current, we disregarded the contributions of the thermogeneration of electronhole pairs in the isection and the
195
196
Effect of SelfConsistent Electric Field on Characteristics of Graphene
injection of minority carriers from the n and psections. The thermogeneration dc current is given by J0therm = 4Kelg0therm .
(10.20)
The thermogeneration rate g0therm at the temperature T = 300 K is estimated as [18] g0therm 1020 – 1021 cm–2s–1. As a result, at K = 1 and 2l = 0.7 mm from Eq. (10.20), one obtains J0therm 2(10–3 – 10–2) A/cm. The injection dc current can be estimated as J0inj =
Ê mˆ exp Á  ˜ , Ë T¯ p vw 2KeT 2 2 2
(10.21)
where m is the Fermi energy of electrons in the nsection and holes in the psection. Setting m = 50 meV, from Eq. (10.21) for K = 1, we find J0inj 0.077 A/cm. Thus, J0therm, J0inj J0, at least in the voltage range considered above. The typical values of the real part of the GTUNNETT smallsignal admittance in the vicinity of the first transittime resonance (wtt ~ 3/2) is in the range Re Yw –5 to –20 mS/mm depending on K and æ. This implies that the ac resistance, Rw = H/Yw of optimized GTUNNETTs with Re Yw = –20 mS/mm (K = 10, æ = 10, and V0 = 200 mV) and the width H = (0.5 – 1) mm, is Rw 50 – 100 W. Assuming that in this case J0 0.6 – 0.8 A/mm at V0 = 200 mV, the dc power, P0, generated by the propagating electrons and holes in the contact n and pregions of the device can be estimated as P0 150 mW. When Re Yw = –5 mS/mm (K = 1 and æ = 10), the same resistance is provided if H = 2 – 4 mm with the dc power P0 20 – 40 mW. The depth of the minimum of the real part of the GTUNNETT admittance can be increased by applying higher bias voltage. This is because the admittance is proportional to the dc differential conductivity which, in turn, is approximately proportional to V0 . However, an increase in V0 results in the pertinent rise of P0. If eV0 exceeds the energy of optical phonons in GLs ℏw 200 meV, their fast emission disrupts BET and BHT in the isection. The emission of acoustic and, particularly, optical phonons leads to some isotropization of the angular distribution of the electron and hole velocities of electrons and holes. This results in some decrease in their mean directed velocities (they become somewhat smaller than ±uW) and, hence, in some increase in the electron and hole charges
Conclusions
and the transit time. Such factors promote more steep dc currentvoltage characteristics and modify the frequency dependence of the admittance. Although they should not change the GTUNNETT performance qualitatively. The depth of the first resonance minimum of the real part of the GTUNNETT admittance with the parameters used in the above estimate is of the same order of magnitude as that of the small area (about 2 mm2) THz resonanttunneling diodes considered by Asada et al. [19]. It is worth noting that the frequency at which Im Yw turns zero can fall into the frequency range, where Re Yw < 0. In such a case, GTUNNETTs can exhibit the selfexcitation of THz oscillations even without the external resonant circuit. Moreover, the contact nand psections (both ungated as in the case of their chemical doping or gated in the case of the electrical “doping”) can serve as plasma resonant cavities [9, 15]. The combination of the transittime and the plasma resonances can substantially liberalize the selfexcitation conditions and enhance the THz emission efficiency. The matching of the transittime and plasma resonant frequencies requires a proper choice of the length of the n and psections (from several micrometers in the ungated structures to about one micrometer in the gated ones). The plasmons and related resonances in the gated GLs were predicted and analyzed several years ago [20, 21] (see also Ref. [22]). Recently, the plasmons in gated GLs were detected experimentally [23, 24]. It is interesting that as a gate for the GL plasmon cavity, another GL can be used [25] when the contact regions constitute doubleGL structures [26, 27].
10.6 Conclusions
We have developed a selfconsistent device model for pin GTUNNETTs with different number of GLs, which enables the calculation of their realistic dc and ac characteristics. Our calculations have shown that (i) The charges of electrons and holes propagating in the isection and their effect on the spatial distribution of the selfconsistent electric field increase the steepness of the dc currentvoltage characteristics. This effect is stronger in GTUNNETTs with larger number of GLs and can be weak
197
198
Effect of SelfConsistent Electric Field on Characteristics of Graphene
ened by using the media surrounding GL or MGL structure (substrates and top dielectric layers) with elevated values of the dielectric constant; (ii) The imaginary and real parts of the GTUNNETT admittance are oscillatory functions of the signal frequency due to the transittime resonances. In the certain frequency ranges, which correspond to the THz frequencies, the admittance real part can be negative that enables the use of GTUNNETTs in the sources of THz radiation; (iii) The charges of electrons and holes influence on the spatial distribution of the selfconsistent electric field and the interband tunneling and can substantially affect the GTUNNETT admittance, particularly, its frequency dependence near the transittime resonances. The role of this effect enhances with increasing number of GLs in the device structure and can be markedly weakened in the devices with relatively large dielectric constant; (iv) The sensitivity of the GTUNNETT characteristics to t he structural parameters (number of GLs, dielectric constant, and length of the isection) and the bias voltage opens up wide opportunity for the optimization of GTUNNETTs for THz oscillators.
Acknowledgments
This work was partially supported by the Russian Foundation for Basic Research (Grants 110712072, 110700505, and 1207 00710), by grants from the President of the Russian Federation (Russia), the Japan Science and Technology Agency, CREST, the Japan Society for Promotion of Science (Japan), and the TERANO NSF Grant (USA).
References
1. M. S. Shur and L. F. Eastman, IEEE Trans. Electron Devices, ED26, 1677 (1979).
2. M. S. Shur, IEEE Trans. Electron Devices, ED28, 1120 (1981).
3. V. I. Ryzhii, N. A. Bannov, and V. A. Fedirko, Sov. Phys. Semicond., 18, 481 (1984).
References
4. A. K. Geim and K. S. Novoselov, Nat. Mater., 6, 183 (2007).
5. A. H. Castro Neto, F. Guinea, N. M. R. Peres, K. S. Novoselov, and A. K. Geim, Rev. Mod. Phys., 81, 109 (2009).
6. M. Sprinkle, D. Suegel, Y. Hu, Hicks, J. A. Tejeda, A. TalebIbrahimi, P. Le Fevre, F. Bertran, S. Vizzini, H. Enriquez, S. Chiang, P. Soukiassian, C. Berger, W. A. de Heer, A. Lanzara, and E. H. Conrad, Phys. Rev. Lett., 103, 226803 (2009). 7. M. Orlita and M. Potemski, Semicond. Sci. Technol., 25, 063001 (2010).
8. V. Ryzhii, M. Ryzhii, V. Mitin, and M. S. Shur, Appl. Phys. Express, 2, 034503 (2009). 9. V. Ryzhii, M. Ryzhii, M. S. Shur, and V. Mitin, Physica E, 42, 719 (2010).
10. V. V. Cheianov and V. I. Fal’ko, Phys. Rev. B, 74, 041403(R) (2006).
11. A. Ossipov, M. Titov, and C. V. J. Beenakker, Phys. Rev. B, 75, 241401(R) (2007).
12. Z. S. Gribnikov, N. Z. Vagidov, V. V. Mitin, and G. I. Haddad, J. Appl. Phys., 93, 5435 (2003). 13. D. Farmer, Y.M. Lin, A. AfzaliArdakani, and P. Avouris, Appl. Phys. Lett., 94, 213106 (2009).
14. G. Khrenov and V. Ryzhii, IEEE Trans. Electron Devices, 42, 166 (1995). 15. V. Ryzhii, A. Satou, I. Khmyrova, M. Ryzhii, T. Otsuji, V. Mitin, and M. S. Shur, J. Phys.: Conf. Ser., 38, 228 (2006).
16. W. Shocley, J. Appl. Phys., 9, 635 (1938). 17. S. Ramo, Proc. IRE, 27, 584 (1939).
18. F. Rana, P. A. George, J. H. Strait, S. Shivaraman, M. Chandrashekar, and M. G. Spencer, Phys. Rev. B, 79, 115477 (2009).
19. M. Asada, S. Suzuki, and N. Kishimoto, Jpn. J. Appl. Phys., Part 1, 47, 4375 (2008). 20. V. Ryzhii, Jpn. J. Appl. Phys., Part 2, 45, L923 (2006).
21. V. Ryzhii, A. Satou, and T. Otsuji, J. Appl. Phys., 101, 024509 (2007).
22. D. Svintsov, V. Vyurkov, S. O. Yurchenko, T. Otsuji, and V. Ryzhii, J. Appl. Phys., 111, 083715 (2012). 23. Z. Fei, A. S. Rodin, G. O. Andreev, W. Bao, et al., Nature, 487, 82 (2012).
24. J. Chen, M. Badioli, P. AloncoGonzales, S. Thongrattanasari, et al., Nature, 487, 77 (2012).
25. V. Ryzhii, T. Otsuji, M. Ryzhii, and M. S. Shur, J. Phys. D: Appl. Phys., 45, 302001 (2012).
199
200
Effect of SelfConsistent Electric Field on Characteristics of Graphene
26. M. Liu, X. Yin, and X. Zhang, Nano Lett., 12, 482 (2012).
27. L. Britnel, R. V. Gorbachev, R. Jalil, B. D. Belle, F. Shedin, A. Mishenko, T. Georgiou, M. I. Katsnelson, L. Eaves, S. V. Morozov, N. M. R. Peres, J. Leist, A. K. Geim, K. S. Novoselov, and L. A. Ponomarenko, Science, 335, 947 (2012).
Chapter 11
Damping Mechanism of Terahertz Plasmons in Graphene on Heavily Doped Substrate*
A. Satou,a,b Y. Koseki,a V. Ryzhii,a,b V. Vyurkov,c and T. Otsujia,b aResearch
Institute of Electrical Communication, Tohoku University, Sendai 9808577, Japan bCREST, Japan Science and Technology Agency, Tokyo 1070075, Japan cInstitute of Physics and Technology, Russian Academy of Sciences, Moscow 117218, Russia [email protected]
Coupling of plasmons in graphene at terahertz frequencies with surface plasmons in a heavily doped substrate is studied theoretically. We reveal that a huge scattering rate may completely damp out the plasmons, so that proper choices of material and geometrical parameters are essential to suppress the coupling effect and to
*Reprinted with permission from A. Satou, Y. Koseki, V. Ryzhii, V. Vyurkov, and T. Otsuji (2014). Damping mechanism of terahertz plasmons in graphene on heavily doped substrate, J. Appl. Phys., 115, 104501. Copyright © 2014 AIP Publishing LLC. GrapheneBased Terahertz Electronics and Plasmonics: Detector and Emitter Concepts Edited by Vladimir Mitin, Taiichi Otsuji, and Victor Ryzhii
Copyright © 2021 Jenny Stanford Publishing Pte. Ltd.
ISBN 9789814800754 (Hardcover), 9780429328398 (eBook)
www.jennystanford.com
202
Damping Mechanism of Terahertz Plasmons
obtain the minimum damping rate in graphene. Even with the doping concentration 1019 – 1020 cm–3 and the thickness of the dielectric layer between graphene and the substrate 100 nm, which are typical values in real graphene samples with a heavily doped substrate, the increase in the damping rate is not negligible in comparison with the acousticphononlimited damping rate. Dependence of the damping rate on wavenumber, thicknesses of graphenetosubstrate and gatetographene separation, substrate doping concentration, and dielectric constants of surrounding materials are investigated. It is shown that the damping rate can be much reduced by the gate screening, which suppresses the field spread of the graphene plasmons into the substrate.
11.1 Introduction
Plasmons in twodimensional electron gases (2DEGs) can be utilized for terahertz (THz) devices. THz sources and detectors based on compound semiconductor heterostructures have been extensively investigated both experimentally and theoretically [1–8]. The twodimensionality, which gives rise to the wavenumberdependent frequency dispersion, and the high electron concentration on the order of 1012 cm–2 allow us to have their frequency in the THz range with submicron channel length. Most recently, a very high detector responsivity of the socalled asymmetric doublegratinggate structure based on an InPbased highelectronmobility transistor was demonstrated [9]. However, resonant detection as well as singlefrequency coherent emission have not been accomplished so far at room temperature, mainly owning to the damping rate more than 1012 s–1 in compound semiconductors. Plasmons in graphene have potential to surpass those in the heterostructures with 2DEGs based on the standard semiconductors, due to its exceptional electronic properties [10]. Massive experimental and theoretical works have been done very recently on graphene plasmons in the THz and infrared regions (see review papers Refs. [11, 12] and references therein). One of the most important advantages of plasmons in graphene over those in heterostructure 2DEGs is much weaker damping rate close to 1011 s–1 at room temperature in disorderfree graphene suffered only
Introduction
from acousticphonon scattering [13]. That is very promising for the realization of the resonant THz detection [14] and also of plasma instabilities, which can be utilized for the emission. In addition, interband population inversion in the THz range was predicted [15, 16], and it has been investigated for the utilization not only in THz lasers in the usual sense but also in THz active plasmonic devices [17, 18] and metamaterials [19]. Many experimental demonstrations of graphenebased devices have been performed on graphene samples with heavily doped substrates, in order to tune the carrier concentration in graphene by the substrate as a back gate. Typically, either peeling or CVD graphene transferred onto a heavily doped p+ Si substrate, with a SiO2 dielectric layer in between, is used (some experiments on graphene plasmons have adapted undoped Si/SiO2 substrates [20, 21]). Grapheneonsilicon, which is epitaxial graphene on doped Si substrates [22], is also used. For realization of THz plasmonic devices, properties of plasmons in such structures must be fully understood. Although the coupling of graphene plasmons to surface plasmons in perfectly conducting metallic substrates with/without dielectric layers in between have been theoretically studied [23, 24], the influence of the carrier scattering in a heavily doped semiconductor substrate (with finite complex conductivity) has not been taken into account so far. Since the scattering rate in the substrate increases as the doping concentration increases, it is anticipated that the coupling of graphene plasmons to surface plasmons in the heavily doped substrate causes undesired increase in the damping rate. The purpose of this chapter is to study theoretically the coupling between graphene plasmons and substrate surface plasmons in a structure with a heavily doped substrate and with/without a metallic top gate. The chapter is organized as follows. In the Section 11.2, we derive a dispersion equation of the coupled modes of graphene plasmons and substrate surface plasmons. In Section 11.3, we study coupling effect in the ungated structure, especially the increase in the plasmon damping rate due to the coupling and its dependences on the doping concentration, the thickness of graphenetosubstrate separation, and the plasmon wavenumber. In Section 11.4, we show that the coupling in the gated structures can be less effective due to the gate screening. We also compare the effect in structures having different dielectric layers between the top gate, graphene layer,
203
204
Damping Mechanism of Terahertz Plasmons
and substrate, and reveal the impact of values of their dielectric constants. In Section 11.5, we discuss and summarize the main results of this chapter.
11.2 Equations of the Model
We investigate plasmons in an ungated graphene structure with a heavilydoped p+Si substrate, where the graphene layer is exposed on the air, as well as a gated graphene structure with the substrate and a metallic top gate, which are schematically shown in Figs. 11.1a and b, respectively. The thickness of the substrate is assumed to be sufficiently larger than the skin depth of the substrate surface plasmons. The top gate can be considered as perfectly conducting metal, whereas the heavily doped Si substrate is characterized by its complex dielectric constant.
Figure 11.1 Schematic views of (a) an ungated graphene structure with a heavily doped Si substrate where the top surface is exposed on the air and (b) a gated graphene structure with a heavily doped Si substrate and a metallic top gate.
Here, we use the hydrodynamic equations to describe the electron motion in graphene [26], while using the simple Drude model for the hole motion in the substrate (due to virtual independence of the effective mass in the substrate on the electron density, in contrast to graphene). In addition, these are accompanied by the selfconsistent
Equations of the Model
2D Poisson equation (the formulation used here almost follows that for compound semiconductor highelectronmobility transistors, see Ref. [25]). Differences are the hydrodynamic equations accounting for the linear dispersion of graphene and material parameters of the substrate and dielectric layers. In general, the existence of both electrons and holes in graphene results in various modes such as electrically passive electronhole sound waves in intrinsic graphene as well as in huge damping of electrically active modes due to the electronhole friction, as discussed in Ref. [26]. Here, we focus on the case where the electron concentration is much higher than the hole concentration and therefore the damping associated with the friction can be negligibly small. Besides, for the generalization purpose, we formulate the plasmon dispersion equation for the gated structure; that for the ungated structure can be readily found by taking the limit Wt Æ • (see Fig. 11.1). Then, assuming the solutions of the form exp(ikx – iwt), where k = 2p/l and w are the plasmon wavenumber and frequency (l denotes the wavelength), the 2D Poisson equation coupled with the linearized hydrodynamic equations can be expressed as follows: ∂2jw ∂z 2
 k 2jw = 
8pe2 S e 3meŒ
k2
1 w 2 + ivew  (vF k)2 2
jw d ( z ),
(11.1)
where jw is the ac (signal) component of the potential, Se, me, and ve are the steadystate electron concentration, the hydrodynamic “fictitious mass,” and the collision frequency in graphene, respectively, and Œ is the dielectric constant which is different in different layers. The electron concentration and fictitious mass are related to each other through the electron Fermi level, me, and electron temperature, Te: Se =
me =
Ú
•
0
1 vF2 S e
1
È Ê e  me ˆ ˘ 1 + exp Á ˙ de , 2 2 Í Ë kBTe ˜¯ ˙˚ p vF ÍÎ 2e
Ú
•
0
1
Ê e  me ˆ ˘ 2e 2 È 1 + exp Á ˜ ˙ de . 2 2 Í Ë kBTe ¯ ˙˚ p vF ÍÎ
(11.2)
(11.3)
In the following we fix Te and treat the fictitious mass as a function of Se. The dielectric constant can be represented as
205
206
Damping Mechanism of Terahertz Plasmons
Ï Œt 0 < z < Wt , Ô Œ= Ì Œb Wb < z < 0, Ô 2 z < Wb , ÓŒs [1  Ws / w (w + ivs )],
(11.4)
where Œt, Œb, and Œs are the static dielectric constants of the top and bottom dielectric layers and the substrate, respectively, Ws =
4pe2 Ns / mhŒs is the bulk plasma frequency in the substrate with Ns and mh being the doping concentration and hole effective mass, and vs is the collision frequency in the substrate, which depends on the doping concentration. The dielectric constant in the substrate is a sum of the static dielectric constant of Si, Œs = 11.7 and the contribution from the Drude conductivity. The dependence of the collision frequency, vs, on the doping concentration, Ns , is calculated from the experimental data for the hole mobility at room temperature in Ref. [27]. We use the following boundary conditions: vanishing potential at the gate and far below the substrate, jwz = Wt = 0 and jwz = – • = 0; continuity conditions of the potential at interfaces between different layers, jwz = +0 = jwz = –0 and jwz = –Wb +0 = jwz = –Wb –0; a continuity condition of the electric flux density at the interface between the bottom dielectric layer and the substrate in the zdirection, Œb∂jw/∂zz = –Wb +0 = Œs∂jw/∂zz = –Wb –0; and a jump of the electric flux density at the graphene layer, which can be derived from Eq. (11.1). Equation (11.1) together with these boundary conditions yield the following dispersion equation where
Fgr (w)Fsub (w)= Ac,
(11.5)
1 Fgr (w ) = w 2 + ivew  (vF k )2  W2gr , 2
(11.6)
Fsub (w ) = w(w + ivs )  W2sub , Ac =
Wgr =
Œb2 ( Hb2  1) W2gr W2sub , (ŒbHb + Œt H t ) (Œs + ŒbHb)
8p e2 S e k Œ + Œs Hb , Œgr (k ) = Œt Ht + Œb b , Œs + Œb Hb 3meŒgr ( k)
(11.7)
(11.8) (11.9)
Ungated Plasmons
Wsub =
Œ + Œt H t Hb 4pe2 Ns , Œsub(k ) = Œs + Œb b , (11.10) mhŒsub ( k) ŒbHb + Œt H t
and Hb,t = cothkWb,t. In Eq. (11.5), the term Ac on the righthand side represents the coupling between graphene plasmons and substrate surface plasmons. If Ac were zero, the equations Fgr(w) = 0 and Fsub(w) = 0 would give independent dispersion relations for the former and latter, respectively. Qualitatively, Eq. (11.8) indicates that the coupling occurs unless kWb 1 or kWt 1, i.e., unless the separation of the graphene channel and the substrate is sufficiently large or the gate screening of graphene plasmons is effective. Note that the nonconstant frequency dispersion of the substrate surface plasmon in Eq. (11.10) is due to the gate screening, which is similar to that in the structure with two parallel metal electrodes [28]. Equation (11.5) yields two modes which have dominant potential distributions near the graphene channel and inside the substrate, respectively. Hereafter, we focus on the oscillating mode primarily in the graphene channel; we call it “channel mode,” whereas we call the other mode “substrate mode.”
11.3 Ungated Plasmons
First, we study plasmons in the ungated structure. Here, the temperature, electron concentration, and collision frequency in graphene are fixed to Te = 300 K, Se = 1012 cm–2, and ve = 3 ¥ 1011 s–1. With these values of the temperature and concentration the fictitious mass is equal to 0.0427 m0 , where m0 is the electron rest mass. The value of the collision frequency is typical to the acousticphonon scattering at room temperature [13]. As for the structural parameters, we set Œt = 1 and Wt Æ •, and we assume an SiO2 bottom dielectric layer with Œb = 4.5. Then Eq. (11.5) is solved numerically. Figures 11.2a and b show the dependences of the plasmon damping rate and frequency on the substrate doping concentration with the plasmon wavenumber k = 14 ¥ 103 cm–1 (i.e., the wavelength l = 4.5 mm) and with different thicknesses of the bottom dielectric layer, Wb . The value of the plasmon wavelength is chosen so that it gives the frequency around 1 THz in the limit Ns Æ 0. They clearly demonstrate that there is a huge resonant increase in the damping
207
Damping Mechanism of Terahertz Plasmons
rate at around Ns = 3 ¥ 1017 cm–3 as well as a drop of the frequency. This is the manifestation of the resonant coupling of the graphene plasmon and the substrate surface plasmon. The resonance corresponds to the situation where the frequencies of graphene plasmons and substrate surface plasmons coincide, in other words, where the exponentially decaying tail of electric field of graphene plasmons resonantly excite the substrate surface plasmons.
(a)
Damping rate, 1012 s1
7
0.30
6
0.25
5
0.20
4
0.15
3
1019
2
1020
1 0 17 10
(b) 1.2 Frequency, THz
208
18
10
10
19
3
Doping concentration, cm
1
10
20
Wb = 50, 100, 200, 300, 400 nm
0.8 0.6 0.4 0.2 0 17 10
18
10
10
19
3
Doping concentration, cm
20
10
Figure 11.2 Dependences of (a) the plasmon damping rate and (b) frequency on the substrate doping concentration, Ns, with the plasmon wavenumber k = 14 ¥ 103 cm–1 (the wavelength l = 4.5 mm) and with different thicknesses of the bottom dielectric layer, Wb, in the ungated graphene structure. The inset in (a) shows the damping rate in the range Ns = 1019 – 1020 cm–3 (in linear scale).
At the resonance, the damping rate becomes larger than 1012 s–1, over 10 times larger than the contribution from the acousticphonon scattering in graphene, ve/2 = 1.5 ¥ 1011 s–1. For structures with Wb =
Ungated Plasmons
50 and 100 nm, even the damping rate is so large that the frequency is dropped down to zero; this corresponds to an overdamped mode. It is seen in Figs. 11.2a and b that the coupling effect becomes weak as the thickness of the bottom dielectric layer increases. The coupling strength at the resonance is determined by the ratio of the electric fields at the graphene layer and at the interface between the bottom dielectric layer and substrate. In the case of the ungated structure with a relatively low doping concentration, it is roughly equal to exp(–kWb ) . Since l = 4. 5 mm is much larger than the thicknesses of the bottom dielectric layer in the structures under consideration, i.e., kWb 1, the damping rate and frequency in Figs. 11.2a and b exhibit the rather slow dependences on the thickness. Away from the resonance, we have several nontrivial features in the concentration dependence of the damping rate. On the lower side of the doping concentration, the damping rate increase does not vanish until Ns = 1014 – 1015 cm–3. This comes from the wider field spread of the channel mode into the substrate due to the ineffective screening by the lowconcentration holes. On the higher side, one can also see a rather broad linewidth of the resonance with respect to the doping concentration, owning to the large, concentrationdependent damping rate of the substrate surface plasmons, and a contribution to the damping rate is not negligible even when the doping concentration is increased twoordersofmagnitude higher. In fact, with Ns = 1019 cm–3, the damping rate is still twice larger than the contribution from the acousticphonon scattering. The inset in Fig. 11.2a indicates that the doping concentration must be at least larger than Ns = 1020 cm–3 for the coupling effect to be smaller than the contribution from the acousticphonon scattering, although the latter is still nonnegligible. It is also seen from the inset that, with very high doping concentration, the damping rate is almost insensitive to Wb . This originates from the screening by the substrate that strongly expands the field spread into the bottom dielectric layer. As for the dependence of the frequency, it tends to a lower value in the limit Ns Æ • than that in the limit Ns Æ 0, as seen in Fig. 11.2b, along with the larger dependence on the thickness Wb . This corresponds to the transition of the channel mode from an ungated plasmon mode to a gated plasmon mode, where the substrate effectively acts as a back gate.
209
210
Damping Mechanism of Terahertz Plasmons
(a)
1.4
1.2
1
0.6
cm
18
cm
5 x 10
0.4
0.2
18
Ns = 2 x 10
0.8
3
19
5
3 3
1 x 10 cm 10 15 20 25 30 35
(b)
Figure 11.3 Dependences of (a) the plasmon damping rate and (b) frequency on the substrate doping concentration, Ns, and the plasmon wavenumber, k, with different the thickness of the bottom dielectric layer Wb = 300 nm in the ungated graphene structure. The inset of (a) shows the wavenumber dependence of the damping rate with certain doping concentrations. The region with the damping rate below 0.2 ¥ 1012 s–1 is filled with white in (a).
To illustrate the coupling effect with various frequencies in the THz range, dependences of the plasmon damping rate and frequency on the substrate doping concentration and plasmon wavenumber with Wb = 300 nm are plotted in Figs. 11.3a and b. In Fig. 11.3a, the peak of the damping rate shifts to the higher doping concentration as the wavenumber increases, whereas its value decreases. The first feature can be understood from the matching condition of the wavenumberdependent frequency of the ungated graphene
Gated Plasmons
plasmons and the dopingconcentrationdependent frequency of the substrate surface plasmons, i.e., Wgr µ k1/2, roughlly speaking, and Wsub µ Ns1/2. The second feature originates from the exponential decay factor, exp(–kWb ) , of the electric field of the channel mode at the interface between the bottom dielectric layer and the substrate; since the doping concentration is ≲ 1018 cm–3 at the resonance for any wavevector in Fig. 11.3, the exponential decay is valid. Also, with a fixed doping concentration, say Na > 1019 cm–3, the damping rate has a maximum at a certain wavenumber, resulting from the first feature (see the inset in Fig. 11.3a).
11.4 Gated Plasmons
Next, we study plasmons in the gated structures. We consider the same electron concentration, ficticious mass, and collision frequency, Se = 1012 cm–2, me = 0.0427 m0, and ve = 3 ¥ 1011 s–1, as Section 11.3. As examples of materials for top/bottom dielectric layers, we examine Al2 O3 /SiO2 and diamondlike carbon (DLC)/3CSiC. These materials choices not only reflect the realistic combination of dielectric materials available today but also demonstrate two distinct situations for the coupling effect under consideration, where Œt > Œb for the former and Œt < Œb for the latter. Figures 11.4a and b show the dependences of the plasmon damping rate and frequency on the substrate doping concentration with the wavenumber k = 37 ¥ 103 cm–1 (the plasmon wavelength l =1.7 mm), with thicknesses of the Al2O3 top dielectric layer Wt = 20 and 40 nm, and with different thicknesses of the SiO2 bottom dielectric layer, Wb. As seen, the resonant peaks in the damping rate as well as the frequency drop due to the coupling effect appear, although the peak values are substantially smaller than those in the ungated structure (cf. Fig. 11.2). The peak value decreases rapidly as the thickness of the bottom dielectric layer increases; it almost vanishes when Wb ≥ 300 nm. These reflect the fact that in the gated structure the electric field of the channel mode is confined dominantly in the top dielectric layer due to the gate screening effect. The field only weakly spreads into the bottom dielectric layer, where its characteristic length is roughtly proportional to Wt, rather than the wavelength λ as in the ungated structure. Thus, the coupling
211
Damping Mechanism of Terahertz Plasmons
0.35
0.65
0.20
0.30 0.15 19 10
0.25
1020
0.20
0.15 17 10
(b)
18
10
Damping rate, 1012 s1
Damping rate, 1012 s1
(a)
20
19
10
3
Doping concentration, cm
10
0.30 0.25 0.20 0.15 19 10
0.55
0.45
1020
0.35
0.25
0.15 17 10
18
19
10
20
10
Doping concentration, cm3
10
1.10
0.85
0.83
0.82
0.81 Wb = 50, 100, 200, 300, 400 nm
0.80
0.79
0.78 1017
1018
1019
3
Doping concentration, cm
Frequency, THz
0.84
Frequency, THz
212
1020
1.05 Wb = 50, 100, 200, 300, 400 nm
1.00
0.95 17
10
18
19
10 10 3 Doping concentration, cm
20
10
Figure 11.4 Dependences of (a) the plasmon damping rate and (b) frequency on the substrate doping concentration, Ns, with the plasmon wavelength l = 1.7 mrn (the wavenumber k = 37 ¥ 103 cm–1), with thicknesses of the Al2O3 top dielectric layer Wt = 20 and 40 nm (left and right panels, respectively), and with different thicknesses of the SiO2 bottom dielectric layer, Wb, in the gated graphene structure. The insets in (a) show the damping rate in the range Ns = 1019 – 1020 cm–3 (in linear scale).
effect on the damping rate together with on the frequency vanishes quickly as Wb increases, even when the wavenumber is small and kWb 1. More quantitatively, the effect is negligible when the first factor of Ac given in Eq. (11.8) in the limit kWb 1 and kWt 1, Œb2 ( Hb2  1) 1 (Œb Hb + Œt H t )(Œs + Œb Hb ) 1 + (Wb /Œb )/(Wt /Œt )
(11.11)
is small, i.e., when the factor (Wb/Œb)/(Wt/Œt) is much larger than unity. A rather strong dependence of the damping rate on Wb can be also seen with high doping concentration, in the insets of Fig. 11.4a. Figure 11.5 shows the dependence of the plasmon damping rate on the substrate doping concentration and plasmon wavenumber,
Gated Plasmons
with dielectric layer thicknesses Wt = 20 and Wb = 50 nm. As compared with the case of the ungated structure (Fig. 11.3a), the peak of the damping rate exhibits a different wavenumber dependence; it shows a broad maximum at a certain wavenumber (around 150 ¥ 103 cm–1 in Fig. 11.5) unlike the case of the ungated structure, where the resonant peak decreases monotonically as increasing the wavenumber. This can be explained by the screening effect of the substrate against that of the top gate. When the wavenumber is small and the doping concentration corresponding to the resonance is low, the field created by the channel mode is mainly screened by the gate and the field is weakly spread into the bottom direction. As the doping concentration increases (with increase in the wavevector which gives the resonance), the substrate begins to act as a back gate and the field spreads more into the bottom dielectric layer, so that the coupling effect becomes stronger. When the wavenumber becomes so large that kWb 1 does not hold, the field spread is no longer governed dominantly by the substrate or gate screening, i.e., the channel mode begins to be “ungated” by the substrate. Eventually, the coupling effect on the damping rate again becomes weak, with the decay of the field being proportional to exp(–kWb).
Figure 11.5 Dependence of the plasmon damping rate on the substrate doping concentration, Ns, and the plasmon wavenumber, k, with different the thicknesses of the Al2O3 top dielectric layer Wt = 20 nm and the SiO2 bottom dielectric layer Wb = 50 nm in the gated graphene structure. The region with the damping rate below 0.2 ¥ 1012 s–1 is filled with white.
213
Damping Mechanism of Terahertz Plasmons
(a)
2.5
0.8
0.15 19 10
0.6
20
10
0.4
0.2
0.0 1017
(b)
18
10
1019
Damping rate, 1012 s
1
0.20
1.0
3
Doping concentration, cm
1020
1.5
0.0 1017
1.00
0.60
Wb = 50, 100, 200, 300, 400 nm 0.55 0.50 1017
10
18
19
10
Doping concentration, cm
3
20
0.5
0.75
0.65
10
1.0
1.10
0.70
0.30 0.25 0.20 0.15 19 10
2.0
0.80
Frequency, THz
Damping rate, 1012 1
1.2
Frequency, THz
214
1018
1019
3
Doping concentration, cm
1020
0.90 0.80 0.70
Wb = 50, 100, 200, 300, 400 nm
0.60 17 20 10 10
18
10
19
10
Doping concentration, cm
20
3
10
Figure 11.6 The same as Figs. 11.4a and b but with the DLC top and 3CSiC bottom dielectric layer.
Figure 11.7 The same as Fig. 11.5 but with the DLC top and 3CSiC bottom dielectric layer.
As illustrated in Eq. (11.11), the coupling effect in the gated strcture is characterized by the factor (Wb/Œb)/(Wt /Œt) when
Conclusions
the conditions kWb 1 and kWt 1 are met. This means that not only the thicknesses of the dielectric layers but also their dielectric constants are very important parameters to determine the coupling strength. For example, if we adapt the highk material, e.g., HfO2 in the top dielectric layer, it results in the more effective gate screening than in the gated structure with the Al2 O3 top dielectric layer, so that the coupling effect can be suppressed even with the same layer thicknesses. The structure with the DLC top and 3CSiC bottom dielectric layers (with Œt = 3.1 (Refs. [29, 30]) and Œb = 9.7) corresponds to the quite opposite situation, where the gate screening becomes weak and the substrate screening becomes more effective, so that stronger coupling effect is anticipated. Figures 11.6a, b, and 11.7 show the same dependences as in Figs. 11.4a, b, and 11.5, respectively, for the structure with the DLC top and 3CSiC bottom dielectric layers. Comparing with those for the structure with the Al2 O3 top and SiO2 bottom dielectric layers, the damping rate as well as the frequency are more influenced by the coupling effect in the entire ranges of the doping concentration and wavevector. In particular, the increase in the damping rate with high doping concentration Ns = 1019 – 1020 cm–3 and the thickness of the bottom layer Wb = 50 – 100 nm, which are typical values in real graphene samples, is much larger. However, this increase can be avoided by adapting thicker bottom layer, say, Wb ≳ 200 nm or by increasing the doping concentration.
11.5 Conclusions
In summary, we studied theoretically the coupling of plasmons in graphene at THz frequencies with surface plasmons in a heavily doped substrate. We demonstrated that in the ungated graphene structure there is a huge resonant increase in the damping rate of the “channel mode” at a certain doping concentration of the substrate (~1017 cm–2) and the increase can be more than 1012 s–1, due to the resonant coupling of the graphene plasmon and the substrate surface plasmon. The dependences of the damping rate on the doping concentration, the thickness of the bottom dielectric layer, and the plasmon wavenumber are associated with the field spread of the channel mode into the bottom dielectric layer and
215
216
Damping Mechanism of Terahertz Plasmons
into the substrate. We revealed that even with very high doping concentration (1019 – 1020 cm–2), away from the resonance, the coupling effect causes nonnegligible increase in the damping rate compared with the acousticphononlimited damping rate. In the gated graphene structure, the coupling effect can be much reduced compared with that in the ungated structure, reflecting the fact that the field is confined dominantly in the top dielectric layer due to the gate screening. However, with very high doping concentration, it was shown that the screening by the substrate effectively spreads the field into the bottom dielectric layer and the increase in the damping rate can be nonnegligible. These results suggest that the structural parameters such as the thicknesses and dielectric constants of the top and bottom dielectric layers must be properly chosen for the THz plasmonic devices in order to maximize the active plasmonic effect onto real device implementations.
Acknowledgments
Authors thank M. Suemitsu and S. Sanbonsuge for providing information about the grapheneonsilicon structure and Y. Takakuwa, M. Yang, H. Hayashi, and T. Eto for providing information about the diamondlikecarbon dielectric layer. This work was supported by JSPS GrantinAid for Young Scientists (B) (#23760300), by JSPS GrantinAid for Specially Promoted Research (#23000008), and by JSTCREST.
References
1. M. Dyakonov and M. Shur, Phys. Rev. Lett., 71, 2465 (1993).
2. M. Dyakonov and M. Shur, IEEE Trans. Electron Devices, 43, 380 (1996). 3. M. S. Shur and J.Q. Lu, IEEE Trans. Micro. Theory Tech., 48, 750 (2000).
4. M. S. Shur and V. Ryzhii, Int. J. High Speed Electron. Syst., 13, 575 (2003).
5. F. Teppe, D. Veksler, A. P. Dmitriev, X. Xie, S. Rumyantsev, W. Knap, and M. S. Shur, Appl. Phys. Lett., 87, 022102 (2005).
6. T. Otsuji, Y. M. Meziani, T. Nishimura, T. Suemitsu, W. Knap, E. Sano, T. Asano, V. V. and Popov, J. Phys.: Condens. Matter, 20, 384206 (2008). 7. V. Ryzhii, A. Satou, M. Ryzhii, T. Otsuji, and M. S. Shur, J. Phys.: Condens. Matter, 20, 384207 (2008).
References
8. V. V. Popov, D. V. Fateev, T. Otsuji, Y. M. Meziani, D. Coquillat, and W. Knap, Appl. Phys. Lett., 99, 243504 (2011).
9. T. Watanabe, S. Boubanga Tombet, Y. Tanimoto, Y. Wang, H. Minamide, H. Ito, D. Fateev, V. Popov, D. Coquillat, W. Knap, Y. Meziani, and T. Otsuji, SolidState Electron., 78, 109 (2012).
10. V. Ryzhii, Jpn. J. Appl. Phys., Part 2, 45, L923 (2006); V. Ryzhii, A. Satou, and T. Otsuji, J. Appl. Phys., 101, 024509 (2007).
11. T. Otsuji, S. A. Boubanga Tombet, A. Satou, H. Fukidome, M. Suemitsu, E. Sano, V. Popov, M. Ryzhii, and V. Ryzhii, J. Phys. D: Appl. Phys., 45, 303001 (2012). 12. A. N. Grigorenko, M. Polini, and K. S. Novoselov, Nat. Photonics, 6, 749 (2012).
13. E. Hwang and S. Das Sarma, Phys. Rev. B, 77, 115449 (2008).
14. V. Ryzhii, T. Otsuji, M. Ryzhii, and M. S. Shur, J. Phys. D: Appl. Phys., 45, 302001 (2012). 15. V. Ryzhii, M. Ryzhii, and T. Otsuji, J. Appl. Phys., 101, 083114 (2007). 16. M. Ryzhii and V. Ryzhii, Jpn. J. Appl. Phys., Part 2, 46, L151 (2007).
17. A. A. Dubinov, V. Ya. Aleshkin, V. Mitin, T. Otsuji, and V. Ryzhii, J. Phys.: Condens. Matter, 23, 145302 (2011). 18. V. Popov, O. Polischuk, A. Davoyan, V. Ryzhii, T. Otsuji, and M. Shur, Phys. Rev. B, 86, 195437 (2012).
19. Y. Takatsuka, K. Takahagi, E. Sano, V. Ryzhii, and T. Otsuji, J. Appl. Phys., 112, 033103 (2012). 20. L. Ju, B. Geng, J. Horng, C. Girit, M. Martin, Z. Hao, H. Bechtel, X. Liang, A. Zettl, Y. R. Shen, and F. Wang, Nat. Nanotechnol., 6, 630 (2011).
21. J. H. Strait, P. Nene, W.M. Chan, C. Manolatou, S. Tiwari, F. Rana, J. W. Kevek, and P. L. McEuen, Phys. Rev. B, 87, 241410 (2013). 22. M. Suemitsu, Y. Miyamoto, H. Handa, and A. Konno, eJ. Surf. Sci. Nanotechnol., 7, 311 (2009).
23. N. J. M. Horing, Phys. Rev. B, 80, 193401 (2009).
24. J. Yan, K. Thygesen, and K. Jacobsen, Phys. Rev. Lett., 106, 146803 (2011).
25. A. Satou, V. Vyurkov, and I. Khmyrova, Jpn. J. Appl. Phys., Part 1, 43, L566 (2004).
26. D. Svintsov, V. Vyurkov, S. Yurchenko, T. Otsuji, and V. Ryzhii, J. Appl. Phys., 111, 083715 (2012). 27. C. Bulucea, SolidState Electron., 36, 489 (1993).
217
218
Damping Mechanism of Terahertz Plasmons
28. S. A. Maier, Plasmonics: Fundamentals and Applications (Springer Science, NY, 2007).
29. The dielectric constant of DLC varies in the range between 3.1 and 7.8, depending on its growth condition (Ref. [30]). Here, we choose the lowest value for demonstration of the case where Œt Œb.
30. H. Hayashi, S. Takabayashi, M. Yang, R. Jesko, S. Ogawa, T. Otsuji, and Y. Takakuwa, “Tuning of the dielectric constant of diamondlike carbon films synthesized by photoemissionassisted plasmaenhanced CVD,” in 2013 International Workshop on Dielectric Thin Films for Future Electron Devices Science and Technology (2013 IWDTF), Tokyo, Japan, November 7–9, 2013.
Chapter 12
Active Guiding of Dirac Plasmons in Graphene*
M. Yu. Morozov,a A. R. Davoyan,b I. M. Moiseenko,c A. Satou,d T. Otsuji,d and V. V. Popova,c,e aKotelnikov
Institute of Radio Engineering and Electronics (Saratov Branch), Russian Academy of Sciences, Saratov 410019, Russia bDepartment of Electrical and Systems Engineering, University of Pennsylvania, Philadelphia, Pennsylvania 19104, USA cPhysics Department, Saratov State University, Saratov 410012, Russia dResearch Institute of Electrical Communication, Tohoku University, 211 Katahira, Aobaku, Sendai 9808577, Japan eSaratov Scientific Center of the Russian Academy of Sciences, Saratov 410028, Russia [email protected]
The Dirac plasmon propagation in active pristine graphene with the carrier population inversion created by the diffusion of the photoexcited carriers from a semiconductor substrate is studied *Reprinted with permission from M. Y. Morozov, A. R. Davoyan, I. M. Moiseenko, A. Satou, T. Otsuji, and V. V. Popov (2015). Active guiding of Dirac plasmons in graphene, Appl. Phys. Lett., 106, 061105. Copyright © 2015 AIP Publishing LLC. GrapheneBased Terahertz Electronics and Plasmonics: Detector and Emitter Concepts Edited by Vladimir Mitin, Taiichi Otsuji, and Victor Ryzhii
Copyright © 2021 Jenny Stanford Publishing Pte. Ltd.
ISBN 9789814800754 (Hardcover), 9780429328398 (eBook)
www.jennystanford.com
220
Active Guiding of Dirac Plasmons in Graphene
theoretically. It is shown that an order of magnitude smaller pump power can be used for the diffusion pumping as compared to direct optical pumping of graphene for obtaining the same plasmon gain in graphene. We find that the field of the amplified plasmons remains strongly confined in the vicinity of graphene similarly to the case of the attenuated plasmons. Remarkably, the diffusion pumping is characterized by low insertion losses due to small photoexcited carrier concentration in the carriersupplying semiconductor substrate in the region of the plasmon field confined near graphene. Recent advances in the areas of nanophotonics, plasmonics, and metamaterials open promising possibilities for highspeed, broadband, and powersaving electromagnetic signal processing. Further progress in these directions could be based on merging and unifying principles of electronics and integrated optics, and employing recently emerging electronic technologies. Terahertz (THz) plasmonics that incorporates the advantages of both highspeed electronic semiconductor technology and subwavelength nanophotonics may bring optics and electronics together for designing highly functional THz devices. Recently, ideas of graphene plasmonics have been actively discussed, and a number of important graphenebased THz integrated optoelectronic devices have been proposed theoretically and demonstrated experimentally (see, e.g., review papers, Refs. [1, 2], and references therein). Excitation of highly confined plasmons in graphene allows for the guiding and manipulation of THz radiation in a deep subwavelength regime [3–6]. Such a strong THz field localization may be utilized for the design of highspeed plasmonic interconnects and electrically controllable graphene plasmonic devices on a single chip. However, the plasmon damping due to the Drude absorption by free carriers in graphene and semiconductor substrate might hinder their application in THz integrated nanocircuits [7]. Previously, the plasmons in graphene charged by the doping or electrostatic gating have been mostly considered while the thermoactivated Dirac plasmons in pristine (neutral) graphene [8, 9] have not received much of the experimental attention due to small carrier density in pristine graphene at the thermal equilibrium. On the other hand, the gapless linear energy spectrum and high carrier mobility make pristine graphene a promising medium for
Active Guiding of Dirac Plasmons in Graphene
THz amplification and lasing. Optical pumping of pristine graphene may lead to an effective carrier population inversion and THz gain in graphene caused by the dominance of the interband carrier transitions with THz photon emission over the intraband (Drude like) carrier absorption [10]. Various designs of graphene based THz lasers and THz plasmonic amplifiers with the optical pumping were proposed recently (see review paper Ref. [11] and references therein). Under optical pumping, the carrier density in pristine graphene enhances considerably so that the plasmon frequency can reach THz range. Amplification of the Dirac plasmons in optically pumped pristine graphene was theoretically considered in Ref. [12] and experimentally observed in Ref. [13]. However, because graphene absorbs below 2.3% of the incident optical pump power [14], the efficiency of optically pumped graphene laser is questionable. A concept of the diffusion pumping that allows for much weaker pump power as compared with direct optical pumping of graphene was proposed recently [15]. In this chapter, we employ the diffusion pumping concept for suppressing plasmon losses and amplification of Dirac plasmons in graphene. We study the plasmon propagation in pristine graphene deposited on a widegap semiconductor substrate and demonstrate that graphene pumping by diffusion of the electronhole pairs photoexcited in the semiconductor substrate by incoming light suppresses the plasmonic losses and can lead to the plasmonic gain in graphene at THz frequencies. This phenomenon may be used as a tool for controlling plasmon propagation and creating the “lossfree” and active graphenebased THz nanocircuits. The proposed concept of diffusionpumping amplification of the plasmons in graphene is schematically shown in Fig. 12.1. A monolayer of pristine graphene is deposited on the top surface (y = d in Fig. 12.1) of widegap semiconductor (GaAs in our particular case) substrate of thickness d. An incident optical pump beam illuminates the bottom surface (y = 0 in Fig. 12.1) of the semiconductor substrate generating the electronhole pairs inside semiconductor. The photoexcited carriers diffuse across the semiconductor slab and, approaching the top surface of the substrate slab, are captured into graphene creating the carrier population inversion in graphene. It is shown below that the plasmonic gain in the population inverted graphene can totally suppress the plasmon losses and can lead to
221
222
Active Guiding of Dirac Plasmons in Graphene
strong amplification of the plasmons guided along the graphene layer at practically achievable input optical pump power.
Figure 12.1 Diffusion pumping of THz plasmons in graphene. The electronhole pairs in GaAs are generated by illuminating the bottom surface of GaAs substrate with optical beam. The photoexcited carriers diffuse towards the top surface of the substrate and, being captured into graphene, create the carrier population inversion that leads to the plasmon gain in graphene.
In order to get a deeper insight into the physical processes in such a system, we use a system of coupled equations describing (i) the plasmon propagation in graphene and (ii) diffusionpumping of graphene. We consider the plasmon propagation in pristine (neutral) graphene with the carrier population inversion. Because the plasmon wavelength is two or even three orders of magnitude shorter than the freespace electromagnetic radiation wavelength at the same frequency [3–5], we utilize the quasielectrostatic approach and, representing the spatiotemporal dependence of the plasmon field as exp (–iwt + ikxx + ikyy), write the plasmon dispersion relation as [16] kx = i
e0 (e air + e s )w , s (w )
(12.1)
where kx and w are the xcomponent of the plasmon wavevector and angular frequency, respectively, eair and es are the dielectric constants of the ambient medium (air) and semiconductor material of the substrate, respectively, e0 is the electric constant, and s(w) is the dynamic conductivity of the population inverted graphene. Equation (12.1) allows us to determine the plasmon wavelength, 2p/Re kx, and power decrement for the attenuated plasmons,
Active Guiding of Dirac Plasmons in Graphene
2 Im kx > 0, (or power increment for the amplified plasmons, 2 Im kx < 0). Equation (12.1) describes the plasmon propagation in graphene on the substrate of infinite thickness. This is a justified assumption because, as shown below, the plasmon wavelength is much shorter than the substrate thickness so that the plasmons “do not feel” the bottom surface of the substrate. General equation for the plasmon dispersion, Eq. (12.1), is valid for either charged or pristine (neutral) graphene. For the population inverted pristine graphene, the dynamic conductivity is given by [12] s (w ) =
È Ê E ˆ˘ e2 ÏÔ 8kBTt ln Í1 + exp Á F ˜ ˙ Ì 4 Ô p(1  iwt ) ÍÎ Ë kBT ¯ ˚˙ Ó Ê w  2EF ˆ + tanh Á Ë 4kBT ˜¯

4w ip
Ú
• G(e , E
¸
Ô F )  G( w/2, E F ) de ˝ , 2 2
(w )  4e
0
Ô˛
(12.2)
where e is the electron charge, ℏ is the reduced Planck constant, kB is the Boltzmann constant, t and T are the mean free time and temperature of the carriers in graphene, respectively, EF is the quasiFermi energy in graphene (+EF and –EF for electrons and holes, respectively), and G(e, e¢) = sinh(e/kBT)/[cosh(e/kBT) + cosh(e¢/ kBT)]. It is assumed in Eq. (12.2) that the diffusively populated carriers in graphene are in the thermal equilibrium within the carrier gas described by the FermiDirac distribution function with the carrier temperature T. At the thermal equilibrium within the ensemble of carriers, the density of the electronhole pairs in graphene ngr can be related to the quasiFermi energy as [17] ngr =
2
p2VF2
Ú
•
0
e de , Ê e  EF ˆ 1 + exp Á Ë kBT ˜¯
(12.3)
where VF ª 108 cm/s is the characteristic velocity of electrons and holes in graphene. Thus, upon knowing the carrier density ngr, we can calculate the quasiFermi energy in graphene, EF, by the numerical reversion of integral in Eq. (12.3).
223
224
Active Guiding of Dirac Plasmons in Graphene
We find the density of the electronhole pairs in graphene, ngr, created by their diffusion from the semiconductor substrate by solving the equation for the ambipolar diffusion of the photoexcited electronhole pairs in the substrate [18] Da
d 2ns dy
2

ns a + Ppe a y = 0, t R w p
(12.4)
where ns is the bulk concentration of electronhole pairs in the semiconductor, Da is the ambipolar diffusion coefficient, tR is the electronhole pair recombination time in semiconductor, Pp and wp are the input optical pump power and frequency, respectively, and a is the light absorption coefficient in semiconductor. We solve Eq. (12.4) with the boundary conditions dns/dy = 0 for y = 0 and ns = 0 for y = d. The first condition implies the absence of carrier flux through the bottom (graphenefree) surface of the substrate, whereas the second one describes the infinitely fast capture of carriers reaching the top semiconductorsubstrate surface into graphene. This assumption is reasonable as a first approximation due to a significant energy gap offset between semiconductor and graphene. Populated carrier density in graphene ngr is related to the diffusion carrier flux density from the semiconductor substrate, Jin = –Da(dns/dy)y=d, by the rate equation ngr/tgr – Jin = 0, where tgr is the carrier spontaneous recombination time in graphene. (In principle, the populated carrier density in graphene also changes (decreases) due to the stimulated emission of plasmons. However, within the linear problem of calculating plasmon dispersion and plasmon gain in this chapter, this effect is neglected.) Moving further, we calculate the plasmon propagation and amplification in a diffusionpumped graphene. We solved Eq. (12.1) assuming the following characteristic parameters: es = 12.8 (GaAs) and eair = 1, T = 300 K, the mean free time of carriers in graphene is t = 1 ps [19], and tgr = 5 ps [20]. The diffusion equation Eq. (12.4) was solved for ℏwp = 2.5 ¥ 10–19 J (which corresponds to the wavelength 808 nm of commercially available laser diodes), Da = 20 cm2/s, tR = 5 ns, and a = 104 cm–1 [18]. First, we calculate the dispersion of THz plasmons for different pump power values (see Fig. 12.2a) neglecting the losses in the substrate. One can see that the THz plasmon wavelength is from
Active Guiding of Dirac Plasmons in Graphene
two to three orders of magnitude shorter than the freespace THz radiation wavelength (at the same frequency). This justifies the use of the quasielectrostatic approach for describing the dispersion of graphene plasmons. We also note that with the increase of the pump power, the plasmon wavelength also increases for a given frequency due to the enhancement of carrier concentration in graphene with increasing the pump power. We plot in Fig. 12.2b the power gain per the plasmon wavelength, G = exp (–4p Im kx/Re kx), versus the pump power for different substrate thicknesses (G > 1 and G < 1 correspond to the amplification and damping of plasmons, respectively) at frequency 5 THz. It is seen from Fig. 12.2b that the same maximal plasmon gain (about 2.2) is reached for any substrate thickness but at different pump power values for different substrate thicknesses. That can be explained as the following. For each substrate thickness, the quasiFermi energy steadily grows with increasing the pump power. At small quasiFermi energy values, the Drude absorption in graphene surpasses the stimulated emission of the plasmons that corresponds to the plasmon absorption G < 1. For greater values of EF, the stimulated emission of the plasmons starts prevailing over the Drude absorption, which results in the plasmon gain G > 1. For further increasing the quasiFermi energy level, the Drude losses in graphene (described by the real part of the first term in the curly brackets of the conductivity expression Eq. (12.2)) grow roughly proportional to the quasiFermi energy value (for EF kBT) while the second term in the curly brackets of Eq. (12.2) responsible for the stimulated emission of plasmons in graphene saturates for high values of EF. Therefore, sooner or later, the Drude absorption again prevails over the stimulated emission which results in diminishing the plasmon gain for large EF. In the process of increasing the pump power, the quasiFermi energy passes through the same value corresponding to the maximal power released from graphene due to the carrier population inversion, which results in the same maximal plasmon gain for any substrate thickness. One can notice the existence of optimal substrate thickness (see curve 2 in Fig. 12.2b) corresponding to the smallest optical pump power value yielding a maximum plasmon gain in graphene. The optimal value of the substrate thickness is determined by the interplay of carrier generation and recombination in the substrate.
225
226
Active Guiding of Dirac Plasmons in Graphene
For the substrate thickness much smaller than the opticalpump power attenuation length in semiconductor, 1/a, which is about 1 mm for GaAs, only a small part of the optical pump power is absorbed in the semiconductor substrate generating small number of the electronhole pairs which results in a weak population inversion (see Fig. 12.2c) and hence small plasmon gain in graphene. When the thickness of the substrate by far exceeds the ambipolar carrier diffusion length La = Dat R (La ª 3 mm for GaAs), only a small number of the photoexcited carriers reach graphene due to their recombination in the substrate which also leads to a weak population inversion and hence small plasmon gain in graphene. Therefore, the optimal substrate thickness (2 mm in Fig. 12.2b) yielding the maximum population inversion and greatest plasmon gain in graphene is in between 1/a and La.
Figure 12.2 (a) Plasmon wavelength versus plasmon frequency for different pump power values 1000 W/mm2 (curve 1), 500 W/mm2 (curve 2), and 100 W/mm2 (curve 3) for the substrate thickness d = 2 mm. (b) Power gain per the plasmon wavelength versus input optical pump power for different substrate thicknesses 0.1 mm (curve 1), 2 mm (curve 2), and 7 mm (curve 3) at frequency 5 THz. Curve 4 corresponds to direct optical pumping of suspended graphene (with no substrate). (c) Carrier density in graphene as a function of the substrate thickness. The optical pump power attenuation length, 1/a, and diffusion lengths, La, are shown by the vertical dashed straight lines.
The main finding of this work is that, with using the diffusion pumping mechanism, the maximal plasmon gain can be reached for rather small optical pump power. This value of the pump power is by an order of magnitude smaller than that for direct optical pumping of suspended (with no substrate) graphene (cf. curves 2 and 4 in Fig. 12.2b). (The generation rate of the photoexcited carriers in suspended graphene for direct optical pumping was estimated as κPp/ℏwp, where the light absorption coefficient in graphene was
Active Guiding of Dirac Plasmons in Graphene
put at κ = 2.3%. It is worth mentioning that the optical absorption in graphene on the semiconductor substrate illuminated from the graphene side is even smaller than that in suspended graphene due to partial optical reflection from the substrate surface [21]. Therefore, the direct optical pumping of graphene layer on the semiconductor substrate from the graphene side is even less efficient than the direct optical pumping of suspended graphene.)
Figure 12.3 Amplitudephase patterns of the plasmon field for (a) attenuated and (b) amplified plasmons. The equiamplitude and equiphase lines of the plasmon field are shown by solid and dashed straight lines, respectively. The equiamplitude line density corresponds to the plasmon field amplitude at a given point of space. The energyflux vectors of the plasmon field are shown by blue arrows. The plane of graphene is shown by the thick dashed line. (c) Normalized photoexcited electronhole pair concentration (left ordinate axis) and the plasmon electric field amplitude at frequency 5 THz (right ordinate axis) versus the substrate thickness. The bottom surface of the substrate is at y = 0 and graphene is located on the top surface of the substrate at y = 2 mm.
The last important question to be answered is whether the plasmon amplification affects the plasmon confinement in the vicinity of the graphene layer. The amplitudephase patterns of the plasmon field for attenuated and amplified plasmons are shown in Figs. 12.3a and b, respectively. The equiamplitude and equiphase lines of the plasmon field (shown by solid and dashed straight lines, respectively, in Figs. 12.3a and b) are perpendicular to each other in the media above and below graphene. The equiamplitude line density corresponds to the plasmon field amplitude at a given point of space. The energyflux vectors of the plasmon field (shown by arrows in Figs. 12.3a and b) are directed at the normal to the equiphase lines. For attenuated plasmons (Fig. 12.3a), the energyflux vectors have the normaltographene components directed towards graphene in both media above and below graphene, which corresponds to the
227
228
Active Guiding of Dirac Plasmons in Graphene
absorption of the plasmon energy in graphene. On the contrary, for the amplified plasmons (Fig. 12.3b), the energyflux vectors have the normaltographene components directed outwards graphene in both media above and below graphene, which corresponds to the plasmon gain due to the energy flux effused from the population inverted graphene. Surprisingly, in spite of the fact that the energy leaks from graphene in this case, the amplified plasmon field still decays away from the graphene layer. This happens because the plasmon field farther away from graphene is created by the energy flux effused from graphene at earlier moments of time when the plasmon energy in graphene was much smaller. It is known that the plasmon field of attenuated (lossless in the limiting case) plasmons rapidly decays away from graphene [3, 16]. Actually, the same decay length (of the order the plasmon wavelength shown in Fig. 12.2a) is also characteristic of the amplified plasmons, which means that the amplified plasmons are strongly confined in the vicinity of graphene (Fig. 12.3c). The photoexcited carrier distribution across the substrate thickness is also shown in Fig. 12.3c. One can see from Fig. 12.3c that the bulk free carrier density in semiconductor ns is very small in the vicinity of the graphene layer due to fast capture of the carriers into graphene. At the same time, the plasmon field rapidly decays in the substrate away from graphene. Therefore, the Drude losses in the substrate have a marginal effect on the plasmon damping in graphene. (This validates the assumption of a lossless substrate while calculating the plasmon dispersion and damping (gain) in graphene.) In conclusion, we have developed a concept of the plasmonic graphene amplifier employing the carrier diffusion pumping from a semiconductor substrate. It is shown that an order of magnitude smaller pump power can be used with the diffusion pumping as compared to direct optical pumping of graphene. We find that the field of the amplified plasmons remains strongly confined in the vicinity of graphene similarly to the case of the attenuated plasmons. Diffusion pumping mechanism combines an effective pumping of graphene with low insertion losses due to small photoexcited carrier concentration in the carriersupplying semiconductor substrate in the region of the plasmon field confined near graphene. Amplified plasmons can be used as lowloss interconnects and active elements in the plasmonic graphene THz nanocircuits.
References
The work was supported by the Russian Foundation for Basic Research through Grant No. 130212070 and by JSPS GrantinAid for Specially Promoting Research (No. 23000008), Japan.
References
1. A. N. Grigorenko, M. Polini, and K. S. Novoselov, Nat. Photonics, 6, 749 (2012). 2. X. Luo, T. Qiu, W. Lu, and Z. Ni, Mater. Sci. Eng. R, 74, 351 (2013).
3. F. H. L. Koppens, D. E. Chang, and F. J. García de Abajo, Nano Lett., 11, 3370 (2011). 4. J. Chen, M. Badioli, P. AlonsoGonzález, S. Thongrattanasiri, F. Huth, J. Osmond, M. Spasenović, A. Centeno, A. Pesquera, P. Godignon, A. Z. Elorza, N. Camara, F. J. García de Abajo, R. Hillenbrand, and F. H. Koppens, Nature, 487, 77 (2012).
5. Z. Fei, A. S. Rodin, G. O. Andreev, W. Bao, A. S. McLeod, M. Wagner, L. M. Zhang, Z. Zhao, M. Thiemens, G. Dominguez, M. M. Fogler, A. H. Castro Neto, C. N. Lau, F. Keilmann, and D. N. Basov, Nature, 487, 82 (2012).
6. J. T. Kim and S.Y. Choi, Opt. Express, 19(24), 24557 (2011).
7. A. Satou, Y. Koseki, V. Ryzhii, V. Vyurkov, and T. Otsuji, J. Appl. Phys., 115, 104501 (2014).
8. O. Vafek, Phys. Rev. Lett., 97, 266406 (2006).
9. S. Das Sarma and Q. Li, Phys. Rev. B, 87, 235418 (2013).
10. V. Ryzhii, M. Ryzhii, and T. Otsuji, J. Appl. Phys., 101, 083114 (2007).
11. T. Otsuji, S. A. Boubanga Tombet, A. Satou, H. Fukidome, M. Suemitsu, E. Sano, V. Popov, M. Ryzhii, and V. Ryzhii, MRS Bull., 37, 1235 (2012). 12. A. A. Dubinov, V. Ya. Aleshkin, V. Mitin, T. Otsuji, and V. Ryzhii, J. Phys.: Condens. Matter, 23, 145302 (2011).
13. T. Watanabe, T. Fukushima, Y. Yabe, S. A. Boubanga Tombet, A. Satou, A. A. Dubinov, V. Ya. Aleshkin, V. Mitin, V. Ryzhii, and T. Otsuji, New J. Phys., 15, 075003 (2013). 14. R. R. Nair, P. Blake, A. N. Grigorenko, K. S. Novoselov, T. J. Booth, T. Stauber, N. M. R. Peres, and A. K. Geim, Science, 320, 1308 (2008).
15. A. R. Davoyan, M. Yu. Morozov, V. V. Popov, A. Satou, and T. Otsuji, Appl. Phys. Lett., 103, 251102 (2013).
16. M. Jablan, H. Buljan, and M. Soljacic, Phys. Rev. B, 80, 245435 (2009).
17. V. Ya. Aleshkin, A. A. Dubinov, and V. Ryzhii, JETP Lett., 89, 63 (2009).
229
230
Active Guiding of Dirac Plasmons in Graphene
18. Y. Morozov, T. Leinonen, M. Morozov, S. Ranta, M. Saarinen, V. Popov, and M. Pessa, New J. Phys., 10, 063028 (2008).
19. T. Otsuji, S. A. BoubangaTombet, A. Satou, H. Fukidome, M. Suemitsu, E. Sano, V. Popov, M. Ryzhii, and V. Ryzhii, J. Phys. D: Appl. Phys., 45, 303001 (2012). 20. P. A. George, J. Strait, J. Dawlaty, S. Shivaraman, M. Chandrashekhar, F. Rana, and M. G. Spencer, Nano Lett., 8, 4248 (2008).
21. J. M. Dawlaty, S. Shivaraman, J. Strait, P. George, M. Chandrashekhar, F. Rana, M. G. Spencer, D. Veksler, and Y. Chen, Appl. Phys. Lett., 93, 131905 (2008).
Chapter 13
Vertical Electron Transport in van der Waals Heterostructures with Graphene Layers*
V. Ryzhii,a,b T. Otsuji,a M. Ryzhii,c V. Ya. Aleshkin,d A. A. Dubinov,d V. Mitin,a,e and M. S. Shurf aResearch
Institute for Electrical Communication, Tohoku University, Sendai 9808577, Japan bCenter for Photonics and Infrared Engineering, Bauman Moscow State Technical University and Institute of Ultra High Frequency Semiconductor Electronics of RAS, Moscow 111005, Russia cDepartment of Computer Science and Engineering, University of Aizu, AizuWakamatsu 9658580, Japan dInstitute for Physics of Microstructures of RAS and Lobachevsky State University of Nizhny Novgorod, Nizhny Novgorod 603950, Russia eDepartment of Electrical Engineering, University at Buffalo, Buffalo, New York 14601920, USA fDepartment of Electrical, Electronics, and Systems Engineering and Department of Physics, Applied Physics, and Astronomy, Rensselaer Polytechnic Institute, Troy, New York 12180, USA [email protected]
*Reprinted with permission from V. Ryzhii, T. Otsuji, M. Ryzhii, V. Ya. Aleshkin, A. A. Dubinov, V. Mitin, and M. S. Shur (2015). Vertical electron transport in van der Waals heterostructures with graphene layers, J. Appl. Phys., 117, 154504. Copyright © 2015 AIP Publishing LLC. GrapheneBased Terahertz Electronics and Plasmonics: Detector and Emitter Concepts Edited by Vladimir Mitin, Taiichi Otsuji, and Victor Ryzhii
Copyright © 2021 Jenny Stanford Publishing Pte. Ltd.
ISBN 9789814800754 (Hardcover), 9780429328398 (eBook)
www.jennystanford.com
232
Vertical Electron Transport in van der Waals Heterostructures
We propose and analyze an analytical model for the selfconsistent description of the vertical electron transport in van der Waals graphenelayer (GL) heterostructures with the GLs separated by the barriers layers. The top and bottom GLs serve as the structure emitter and collector. The vertical electron transport in such structures is associated with the propagation of the electrons thermionically emitted from GLs above the interGL barriers. The model under consideration describes the processes of the electron thermionic emission from and the electron capture to GLs. It accounts for the nonuniformity of the selfconsistent electric field governed by the Poisson equation which accounts for the variation of the electron population in GLs. The model takes also under consideration the cooling of electrons in the emitter layer due to the Peltier effect. We find the spatial distributions of the electric field and potential with the highelectricfield domain near the emitter GL in the GL heterostructures with different numbers of GLs. Using the obtained spatial distributions of the electric field, we calculate the currentvoltage characteristics. We demonstrate that the Peltier cooling of the twodimensional electron gas in the emitter GL can strongly affect the currentvoltage characteristics resulting in their saturation. The obtained results can be important for the optimization of the hotelectron bolometric terahertz detectors and different devices based on GL heterostructures.
13.1 Introduction
Van der Waals heterostructures based on graphenelayers (GLs) separated by the barrier layers made of hBN, MoS2,WS2, and others have recently attracted a considerable interest (see, for example, the review paper [1]). These heterostructures can be used in novel electron and optoelectron devices. Several devices using these structures (among other GLstructures) have been proposed and realized [2–16]. In particular, we proposed and evaluated the hotelectron bolometric GLbased detectors of terahertz (THz) radiation consisting of multipleGL structures with the interGL barrier layers [1]. In these devices (see Fig. 13.1), the extreme (top and bottom) GLs serve as the emitter and collector, respectively. In our previous work [17], considering the vertical electron transport in the multipleGL
General Equations of the Model
heterostructures, we used a simplified model in which the spatial distribution of the electric field across the main portion of the GL detector structure was assumed virtually uniform. However, the features of the electron injection from the emitter GL and the electron capture into the inner GLs in the multipleGL heterostructures, leading to a charging of the GLs adjacent to the emitter and deviation of the selfconsistent electricfield distributions from uniform ones, can affect the characteristics of the vertical electron transport in such heterostructures. The cooling of the twodimensional electron gas (2DEG) in the emitter GL due to the Peltier effect can add complexity to the characteristics. In this chapter, we develop a model for the vertical electron transport in van der Waals GLbased heterostructures accounting for the thermionic electron emission from and the electron capture into GLs, selfconsistent electricfield distributions, and the electron cooling in the emitter GL. The developed model and obtained results might be useful for the optimization of the performance of the hotelectron bolometric THz detectors, particularly, their dark current characteristics and, hence, the detector detectivity, as well as the optimization of other devices based multipleGL heterostructures.
Figure 13.1 Schematic structure of the multipleGL heterostructure under consideration. The horizontal arrows correspond to the electrons injected and absorbed by contacts, whereas the vertical arrows correspond to the electrons crossing and captured into GLs.
13.2 General Equations of the Model We consider multipleGL heterostructures with the ndoped GLs and the sufficiently thick interGL barrier layers (tunneling nontransparent), made, for example, of WS2. Figure 13.1 shows the
233
234
Vertical Electron Transport in van der Waals Heterostructures
GLstructure under consideration. The top and bottom GLs are connected to the pertinent electrodes. These GLs serve as the emitter and collector of electrons. The bias voltage V is applied between the latter. The inner GLs are disconnected from any contacts, so that their potentials are floating. The bottom electrode serves as the collector of the electrons passed through all GLs (not captures into the inner GLs) and as the heat sink. The heterostructure can be supplied by the back electrode (not shown in Fig. 13.1), can provide the collection of the electrons passed through all GL, and plays the role of the extra heat sink. The terminal current is due to the electrons thermionically emitted from GLs and propagating above the tops of the barriers. Since the thickness of the interGL barriers d and the net thickness of the GLheterostructure dN, where N is the number of the barriers in the heterostructure under consideration, is relatively large [the number of GLs is equal to (N + 1)], the geometrical interGL capacitance is much smaller than the quantum capacitance, so that the effect of quantum capacitance [18] can be disregarded. The Poison equation governing the electric potential distribution j = j(z) in the direction perpendicular to the GL plane (the zdirection) and the equation governing the electron balance in each GL are presented in the following form: d 2j dz 2
N
=
Â
4pe (S n  S D )◊d ( z  nd ), k n=0
Ê m  DC ˆ jpn = Q n , Q n = QD exp Á n . e Ë Tn ¯˜
(13.1)
(13.2)
Here, e = e is the electron charge, Sn , SD, and mn, are the 2D densities of electrons and donors (assumed to be the same in all GLs) and the electron Fermi energy in the GL with the index n = 1, 2, . . ., N, d(z) is the Dirac delta function, k and d are the barrier dielectric constant and thickness, j is the density of the electron current across GLs, p n and Q n are the capture parameter [19–21] (proportional to the probability of the electron capture into GLs), and the rate of the electron thermoemission from the nth GL (p0 = 1, p1, p 2 , . . ., p N £ 1), respectively, DC is the band offset between the GL and the barrier material, and T n is the electron temperature (in the energy unit) in the nth GL. In Eq. (13.2), we put
General Equations of the Model
QD =
2Tl2 2 pt �2u W
Ê DC ˆ SD ÁË T + 1¯˜ � t , esc l
(13.3)
where T l is the lattice temperature, t is the characteristic time of the momentum relaxation of electrons with the energy exceeding DC in GLs, ℏ is the Plank constant, u W 108 cm/s is the characteristic electron velocity in GLs, and tesc is the characteristic escape time from GLs. We disregard small variations of the electron density and the temperature in the preexponential factors. Equation (13.2) is valid if the density of electrons above the barriers substantially exceeds its value in equilibrium. The boundary conditions for the potential governed by Eq. (13.1) can be set as j
z=0 = 0,
j
z= Nd = V .
(13.4)
As follows from Eq. (13.1), the electric field in the nth barrier (dj/dx)n = En (n = 1, 2, 3, . . ., N), i.e., at (n – 1)d < z < nd, is equal to: 4p e (S n  S D ). k According to Eq. (13.4), we obtain E n+1 = E n +
(13.5)
n= N
d
ÂE
n
=V.
n=1
(13.6)
Assuming that the 2DEG in all GLs, except those fully depleted, is degenerate due to sufficiently high donor density (mn kBT), one can use the following equation which relates the Fermi energy mn and the electron density S n : mn = uW pS n .
(13.7)
It is commonly believed that the probability of the electron capture to quantum wells (QWs) in the customary heterostructures is determined by the emission of optical phonons [22–25]. The scattering of the electrons propagating over the barriers on the electrons located in GLs can also be rather effective mechanism of the capture of the former. Generally, the capture parameter p n , which relates the current density j and the rate of the capture and is proportional to the probability of the capture of electrons [23–25], depends on the electricfield distribution across the GLstructure.
235
236
Vertical Electron Transport in van der Waals Heterostructures
In the case of ballistic or near ballistic transport of electrons above the barriers, p n depends mainly on E n . In the GLstructures with the collisiondominated electron transport, one can assume that p n is determined by the electric field around the n th GL, in particular, by the electric fields E n and En+1. For the definiteness, we use the following approximation for the electricfield dependence (see the Appendix): pn = EC/En.
(13.8)
Here, E C = · W C Òu t /b is the characteristic capture field, which is determined by the barrier layer and GL structural parameters: the average (averaged over the electron Maxwellian distribution in the barrier layer) probability of the capture of electrons crossing a GL, ·W C Ò , the electron mobility across the barrier, b = b ( E ), and the electron thermal velocity and the electron effective mass in the
barrier layer, uT = Tb / 2mb and mb, respectively. Using Eqs. (13.2) and (13.6), we obtain equations which relates S 0 and S n and the current density j Ê mD S 0 / S D  D C ˆ j , exp Á ˜= T j 0 D Ë ¯
for the emitter GL, and
Ê mD S n / S 0  D C ˆ jp n exp Á , ˜= Tn jD Ë ¯
for the inner GLs. Here, mD = u W pS D jD
eS D const. t esc
and
(13.9)
(13.10)
(13.11)
Generally, the electron temperature in the emitter GL T 0 can differ from the electron temperatures in the inner GLs T n and the lattice temperature T l , in particular, due to the Peltier effect (see below). Neglecting for simplicity the electron heating in the barrier layers (see below), we put the electron temperatures in all inner GLs to be equal to the lattice temperature: T n = T l . Due to the smallness of the ratio E C/E D, where E D = 4 p e S D /k , monotonic electricfield distributions can be partitioned into a smooth quasineutral (S n = S D ) portion with relatively small
General Equations of the Model
electric field in a wide range adjacent to the collector and a narrow highfield portion (highelectricfield domain) near the emitter GL. At S D = 1.8 ¥ 1012 cm–2 and k = 4, one obtains E D = 270 kV/cm and mD = 150 meV. Due to relatively strong doping of GLs, the highelectric field is concentrated primarily in the emitter barrier layer (similar to that in the multiplequantum well structures based on the standard semiconductors [26–30]). Considering this and using Eqs. (13.8) and (13.10), for the electric field in the quasineutral region E Bulk (in the barrier layers with n > M, where M is the number of charged, i.e., fully and partially depleted GLs), we find EBulk = EC
Ê D  mD ˆ j exp Á C . jD Ë Tl ˜¯
(13.12)
Taking into account that E Emitter = E1 = E d (S 0 /S d – 1), from Eq. (13.10), we obtain EEmitter
2 ÈÊ ˘ j ˆ Í DC + T0 ln ˙ Á jD ˜ ˙ Í = ED ÍÁ ˜  1˙ . mD ˜ Á ÍÁ ˙ ˜¯ Ë ÎÍ ˚˙
(13.13)
Thus, the spatial distribution of the electric field is given by E n = EEmitter  (n  1)ED , 1 £ n £ M , E n = EBulk , M < n £ N . Using Eq. (13.6), we arrive at the following equation: MEEmitter  (M  1)ED + (N  M )EBulk =
V , d
with M is determined by the following inequalities:
(EEmitter  EBulk ) (E  EBulk ) < M < Emitter + 1. ED ED
(13.14)
(13.15)
(13.16) (13.17)
The first two terms in the lefthand side of Eq. (13.16) correspond to the potential drop at the depleted region, whereas the third term is equal to the potential drop across the bulk of the heterostructure (across all other barrier layers). Equation (13.16) with Eqs. (13.12) and (13.13) yields the following current voltage characteristics (with the electron temperature in the emitter GL T 0 as a parameter):
237
238
Vertical Electron Transport in van der Waals Heterostructures
È Ê m  DC Í D C + T0 D + ln ÁË T Í l Í mD Í Í Î =
2 ˆ ˘ J˜ ˙ ¯ ˙ ( N  M ) EC J ˙+ M ED ˙ ˙ ˚
V / VD + 2M  1 , M
where J =(j/j D ) exp[(DC – mD )/T l ] .
(13.18)
13.3 The Peltier Cooling
The electrons leaving the emitter GL extract some energy from 2DEG in this GL. This can lead to the 2DEG cooling (the Peltier effect) and affect the electron thermionic emission from the emitter GL, the spatial distributions of the electric field and electron population in GLs, and the current density. The density of the energy flux from the emitter GL is equal to Q = j(DC – 2m0/3)/e. We assume that the main mechanism transferring the energy from the emitter GL lattice to 2DEG in this GL is associated with the GL’s optical phonons. In this case, the electron effective temperature T 0 in the emitter GL is governed by the following equation describing the balance between the energy taken away by the emitted electrons from the emitter GL and the energy which the 2DEG in this GL receives from the lattice: �w 0 t0
È Ê �w 0 ˆ Ê �w ˆ ˘ ( D  2mD / 3) j . (13.19)  exp Á  0 ˜ ˙ �  C Íexp Á ˜ jD t essc Ë Tl ¯ ˙˚ Ë T0 ¯ ÍÎ
Here, ℏw0 and t0 are the optical phonon energy in GL and their characteristic spontaneous emission time, respectively. Equation (13.19) leads to Ê 1 1 1 Jˆ = ln Á 1  ˜ , T0 Tl w 0 Ë JS ¯
with
JS =
ˆ Ê D  mD  w 0 ˆ w 0 t esc Ê exp Á C Á ˜ ˜¯ . Tl t 0 Ë D C  2mD / 3 ¯ Ë
(13.20)
(13.21)
Electric Fields versus Current and CurrentVoltage Characteristics
Figure 13.2 shows the dependences of the normalized electron temperature in the emitter GL T 0 /T l on the normalized current J calculated using Eq. (13.20). It is assumed that tesc ~ t0 ~ 10–12 s, DC = 400 meV, ℏw0 = 200 meV, mD = 150 meV (S D = 1.8 ¥ 1012 cm–2), and T l = 25 meV (Tl 300 K). At the above parameters, J S 5, j D exp[(mD – DC )/T l] 14.5 A/cm2 and j S = J S j D exp[(mD – DC )/T l] 72.6 A/ cm2. As follows from Eq. (13.20) andseen from Fig. 13.2, the electron temperature in the emitter GL is lower than the lattice temperature due to the effect of thermoelectric (Peltier) cooling. When the current J approaches to J S (the saturation current), T 0 drastically decreases.
Figure 13.2 Current dependences of electron temperature in the emitter GL and difference between the emitter and bulk electric field.
13.4 Electric Fields versus Current and CurrentVoltage Characteristics Equation (13.12) yields the following expression for E Bulk as a function of the normalized current J: EBulk = EC J.
(13.22)
Using Eqs. (13.13) and (13.20), we find the following E Emitter – J relation:
239
240
Vertical Electron Transport in van der Waals Heterostructures
2 ¸ ÏÈ (m D  D C + Tl ln J )
˘
Ô Í D C +
Ô 1  (Tl / w 0 ) ln (1  J / JS ) ˙
Ô ˙  1Ô˝ . (13.23)
E Emitter = E D Ì Í Í ˙ m D Ô Ô ˙ Ô Ô ÍÎ
˚
˛
Ó
Apart from the T 0 – J relation, Fig. 13.2 shows also the dependence of (E Emitter – E Bulk )/E D on the normalized current J correspond calculated using Eqs. (13.19), (13.22), and (13.23) (for E D = 270 kV/cm and E C = 1.5 kV/cm). As seen, the difference E Emitter – E Bulk steeply increases when J becomes close to the normalized saturation current J S . Using the value of the difference (E Emitter – E Bulk) and inequalities (13.17), one can find the intervals of the normalized current corresponding to different numbers, M , of the charged inner GLs. Considering the above, we arrive at the following currentvoltage characteristic: 2
(m D  D C + Tl ln J )
˘
È
Í D C + 1  (T / w ) ln (1  J / J ) ˙ l 0 S ˙ Í Í ˙ mD Í ˙ Î
˚
V /VD + 2M  1
(N  M) EC +
.
J =
M M ED
(13.24)
Figure 13.3 shows the currentvoltage characteristics of the heterostructures with the numbers of the interGL barriers equal to N = 6 and N = 11 (the numbers of GLs are five and ten, respectively) for different values of E C . Other parameters are the same as for Fig. 13.2. The obtained characteristics clearly demonstrate the tendency to saturation with increasing voltage. At a relatively small E C , the currentvoltage characteristics of the heterostructures with different N are rather close to each other. This is because at such values of E C and N , the potential drop across the quasineutral region is small in comparison with that across the depleted region, so that E Emitter V/d +(M – 1 )E D and, hence, the current is virtually independent on N . However, when E C is not so small, the potential drop across the quasineutral region becomes essential and dependent on N . In this case, the currentvoltage characteristics at different N can be markedly different (see curves for E C = 7. 5 kV/ cm in Fig. 13.3).
Potential Profiles
Figure 13.3 Currentvoltage characteristics in GL structures with different numbers of interGL barrier layers N [with ( N – 1 ) inner GLs] and different characteristic capture field ec.
13.5 Potential Profiles Considering the obtained currentvoltage characteristics, one can find the voltage dependences of E Emitter and E Bulk corresponding to their current dependences shown in Fig. 13.2. Figure 13.4 shows these voltage dependences for the heterostructures with different E C . One can see that in both cases EEmitter E Bulk, the difference between this fields at E C = 7. 5 kV/cm is markedly smaller. Using Eqs. (13.14) and (13.15) and accounting for the calculated data for the E Emitter – V and E Bulk – V relations (see Fig. 13.4), one can find the spatial distributions of the electric potential (potential profiles) between the emitter and collector GLs. Figures 13.5 and 13.6 show examples of the potential profiles found for heterostructures with N = 11, E D = 270 kV/cm, and d = 5 ¥ 10–6 cm with E C = 1.5 kV/cm and E C = 7.5 kV/cm, respectively, at different voltages. One can see that the potential spatial distributions are substantially nonuniform: they steeply vary near the emitter GL (in the depleted, i.e., charged region) and are fairly smooth in the heterostructure bulk. It is also seen that an increase in the voltage leads to a change of the number of the charged GLs M (from M = 1 to M = 3 at the parameters used for Fig. 13.5 and in the chosen voltage range). The transition from the
241
242
Vertical Electron Transport in van der Waals Heterostructures
voltage corresponding a certain M to M + 1 results in the occurrence of jogs (actually rather weak) on the characteristics shown in Figs. 13.3 and 13.4. It is also seen that in a heterostructure with relatively large E C and moderate voltages, the potential distribution is rather smooth except the immediate vicinity of the emitter GLs, where the electric field is only slighter higher (see the line for V = 1 V in Fig. 13.6). This can justify the simplified model [15] at not too small pn.
Figure 13.4 Electric fields in the emitter GL and in the heterostructure bulk versus voltage for GL structures with different values of the characteristic capture field ec.
Figure 13.5 Potential profiles at different voltages. Markers correspond to positions of charged GLs.
Discussions
Figure 13.6 The same as in Fig. 13.5, but for EC = 7.5 kV/cm and with dashed line corresponding to EC = 1.5 kV and V = 3 V (from Fig. 13.5).
13.6 Discussions 13.6.1 Limiting Cases In the voltages range not so close to the saturation, the Peltier cooling can be disregarded. In this range, the currentvoltage characteristics can be expressed by simple equations. Taking into account that at moderate voltages only one GL is charged and the potential drops primarily across the barrier layer closest to the emitter GL (see Fig. 13.5), we obtain EEmitter V / d ,
Èm Ê ˆ˘ Êm V ˆ V ,  1˜ ˙ exp Á D J exp Í D Á 1 + VD Ë 2Tl VD ˜¯ ¯ ˙˚ ÎÍ Tl Ë i.e.,
Èm Ê ˆ˘ Ê m  DC ˆ V exp Í D Á 1 +  1˜ ˙ , j jD exp Á D ˜ VD Ë Tl ¯ ÍÎ 2Tl Ë ¯ ˙˚ Êm V ˆ Ê m  DC ˆ jD exp Á D exp Á D , ˜ Ë 2Tl VD ˜¯ Ë Tl ¯
(13.25)
(13.26)
243
244
Vertical Electron Transport in van der Waals Heterostructures
Ê m  DC ˆ 1 = jD exp Á D . Ë Tl ˜¯ pCeff pCeff = exp( mDV / 2TlVD ).
Here,
(13.27)
In the heterostructures with not too small E C and sufficiently large N, one has E Emitter < (N – 1)E C , i.e., the potential drops predominantly across the quasineutral region (bulk), and the following relation is true: EEmitter > EBulk
V . Nd
(13.28)
In this limiting cases, the current density can be presented as J�
Hence,
V > 1. NdEC �
(13.29)
Ê m  DC ˆ V j jD exp Á D , Ë Tl ˜¯ NdEC Ê m  DC ˆ 1 = jD exp Á D , Ë Tl ˜¯ pCeff
(13.30)
where pC is the effective capture parameter, which, in this case, is determined by the electric field in the main portion of the eff heterostructure, namely, by EBulk : pC = EC / EBulk [see Eq. (13.8)]. It is instructive that in the latter limit, the current density can be presented in the Ohmic form eff
j enb bV / Nd ,
(13.31)
with the electron density in the barrier layers n b µ S D / ·W C Ò) exp[( mD – DC )/T l )]. Equations (13.27) and (13.29) coincide in form with those obtained previously using a simplified model [17]. However, pCeff in these equations is determined by the electricfield spatial distribution and the number of GLs (instead of p C = const or pC) determined by the average electric field in Ref. [17]. Moreover, pCeff can explicitly depend on the capture probability W C and
Discussions
characteristic capture field E C (see the Appendix) as in the case of Eq. (13.30), or be independent of these parameters as in the case of Eq. (13.27).
13.6.2 Role of the pn–E n Relation
Above, we used the p n – E n relation given by Eq. (13.8). The deviation from this relation does not lead to qualitative change in the obtained result. To demonstrate this, let us assume now that (see, for example, Refs. [27, 28]) pn = exp(E n / EC* ),
(13.32)
where the characteristic field EC* generally differs from EC. In this case, Eq. (13.12) should be replaced by the following equation: Ê D  mD jˆ E bulk = EC* Á C + ln ˜ . jD ¯ Ë Tl
(13.33)
The second term in the lefthand side of Eq. (13.18) (and the only this term) should also be modified accordingly. Such a replacement does not affect the saturation of the current voltage characteristics and the value Js (and jS) and again leads to Eqs. (13.27) and (13.30). In eff * the latter equation, there should be now pC exp( V / NdEC ) 1.
The current across the GLheterostructures under consideration eff essentially depends on the effective capture parameter pC [see, Eqs. (13.27) and (13.28)], which, in turn, depends on the electricfield distribution and the number of GLs in the heterostructure. Hence, the voltage dependence of the dark current, i.e., the current in the absence of irradiation in the hotelectron bolometric THz detectors on the base of these heterostructures proposed in Ref. [17], is more complex than that follows from the simplified model of such photodetectors. In particular, the dark currentvoltage characteristics calculated using the present model explicitly depend on the number of GLs (see Fig. 13.3) in contrast to more simple model [17]. The photocurrent caused by the THz radiation in the photodetectors in question and their responsivity also depend on pCeff . Qualitative reasonings show that since the photodetector detectivity is determined by the responsivity, dark current, and eff the photoelectric gain g µ 1 / pC , the effects of the electricfield nonuniformity (as well as the Peltier cooling effect) can
245
246
Vertical Electron Transport in van der Waals Heterostructures
pronouncedly influence the detectivity as a function of the voltage and number of GLs. Therefore, such effects should be taken into account considering the photodetector quantitative optimization. One of the parameter which should be optimized is the number of GLs in the photodetector. The quantitative study of the impact of the nonuniformity effects and the effect of the Peltier cooling on the photodetector responsivity and detectivity require a separate detailed treatment.
13.6.3 Electron Heating in the Barrier Layers
In contrast to the cooling of the 2DEG in the emitter GL, the electron heating in the inner GLs, associated with the capture of relatively hot electrons heated in the barrier layers and cooled due the electron emission from these GLs, is relatively weak. This is because the energy brought to a GL by a captured electron and the energy swept away by an emitted electron are close to each other (these energies are close to DC unless the electron temperature in the barrier layers Tb DC). Due to this, Tn – Tl Tl – T0. The effect of heating of the electrons propagating in the barrier layers is also should not be too marked. Indeed, assuming the relaxation of the electron energy obtained from the electric field (Joule heating power in the whole heterostructure is equal to jV) in the barrier layers is mainly due to the interaction of the electrons with the optical phonons in the barrier layers, for the estimate of the electron effective temperature, Tb, in these barriers, one can use the following equation: 2 Ê w 0( b ) ˆ ˘ Ê w 0( b ) ˆ w 0( b ) È Ê V ˆ ˙ Íexp = exp eb ˜ ˜ Á Á ÁË Nd ¯˜ . t 0( b ) ÍÎ Ë kBTl ¯ ˙˚ Ë kBTb ¯
(13.34)
Here, w 0( b ) and t 0( b ) are the optical phonon energy in the barrier layers and the characteristic time of their spontaneous emission. Equation (13.31) yields È Ê w 0( b ) ˆ ˘ 1 1 1 Í = + ln 1 B exp ˜˙, Á N Tl ¯ ˙ Tb Tl w 0( b ) Í Ë Î ˚
(13.35)
Discussions
where
2
BN =
t 0( b)eb Ê V ˆ Á ˜ . w 0( b) Ë Nd ¯
Assuming w 0( b ) = 50 meV, t 0( b ) 10–2s, b = (10 – 15) cm2/V ◊ s, d = 10 – 50 nm, T l = 300 K, N = 11, and V = 1 V, we obtain BN exp( �w 0( b ) / Tl ) � 0.4885  0.7328. As a result, from Eq. (13.35), we get the following estimate: T b/ T l 1.248 – 1.378 (or Tb 374 – 413 K). Since the average capture probability and the characteristic capture electric field slowly vary with the temperature (see Fig. 13.8), the pertinent effect should not essentially change the obtained characteristics. In principle, the effect of electron heating in the barrier layers can be accounted for by the inclusion of the dependence of E C on V (because T b increases with increasing voltage). This might lead to somewhat more complex characteristics at elevated voltages.
Figure 13.7 Energy dependence of the net capture probability as well as the contributions of different capture mechanisms.
13.6.4 Quantum Capacitance Above, we disregarded the effect of quantum capacitance [16]. The ratio of the interGL capacitance C and the GL quantum capacitance C Q is equal to
247
248
Vertical Electron Transport in van der Waals Heterostructures
2 C k 2uW . = CQ 8 mDd
(13.36)
Assuming that κ = 4, mD = 150 meV, and d = 10 – 50 nm, we obtain C / C Q 0.09 – 0.018, i.e., C/ C Q 1 and, hence the quantum capacitance plays an insignificant role in comparison with the geometrical capacitance.
Figure 13.8 Temperature dependence of average capture probability for different barrier electric fields.
13.6.5 Contact Effects The voltage drop across the contacts, V c , to the GL heterostructures under consideration can be fairly small. Indeed, setting j D exp[(mD – DC )/T l ] = 14.5 A/cm2 (as above), considering the voltage range V = 1–2 V in Fig. 13.3 , for a device with the length (spacing between the side contacts) L = 100 mm2, for the current I = jL , we obtain I 0.3 – 0.6 A/cm. According to the experimental data [31–34] for contacts to GLs, the contact resistance can be estimated as R C = (100 – 500) W mm. As a result, we find V C (1 – 15) ¥ 10–3 V. These values are much smaller than the applied voltage (voltage drop between the emitter and collector GLs). Hence, the contact effects can be neglected. The necessity to apply voltages about few volts is due to a relatively high emittercollector resistance, which is associated with current created by relatively small fraction of electrons overcoming the interGL barriers.
Conclusions
13.7 Conclusions Using an analytical model for the selfconsistent description of the vertical electron transport in the van der Waals GL heterostructures with the GLs separated by the barrier layers, we calculated currentvoltage characteristics and potential distribution in those heterostructures. The thermionic current over the barriers is controlled by the electron thermionic emission from the GLs and by the capture of electrons into GLs. At small applied voltages, the electric field is practically homogeneous through the structure with equal potential drop on each barrier. As the voltage increases, the probability of electrons capture into GLs decreases and the potential distributions (see Figs. 13.5 and 13.6) turn to be substantially inhomogeneous with well pronounced two regions: with high electric field near the emitter and low electric field region in the heterostructure bulk (highfield domain and quasineutral lowfield quasineutral domains, respectively). An increase in the applied voltage gives rise to an increase of the number of charged, fully or partially depleted GLs and, therefore, to an increase in the width of the highelectric field (charged) region. The electric field in the bulk is practically homogeneous. We demonstrated that the thermionic emission from the emitter GL can lead to a substantial cooling of the 2DEG in this GL (the Peltier effect). This effect results in the saturation of the currentvoltage characteristics with increasing voltage. The high and low field domains were observed in conventional semiconductor heterostructures with quantum wells, but the current saturation in the van der Waals GL heterostructures under consideration is new phenomenon associated with the specifics of the emitter with 2DEG. The obtained results, which reveal the origin of the currentvoltage characteristics nonlinearity in the van der Waals GL heterostructures, can be important for the optimization of the dark current characteristics of the THz hotelectron bolometers based on those heterostructures. An extended version of the developed model can also be applied for the consideration of the GL heterostructures response to incoming THz radiation and strict calculations of the responsivity and detectivity of such bolometric detectors.
249
250
Vertical Electron Transport in van der Waals Heterostructures
Acknowledgments This work was supported by the Japan Society for promotion of Science (GrantinAid for Specially Promoting Research 23000008), Japan and by the Russian Scientific Fund Foundation (Project #14 29 00277). The works at UB and RPI were supported by the U.S. Air Force Award No. FA9550101391 and the U.S. Army Research Laboratory Cooperative Research Agreement, respectively.
Appendix: Capture Parameter
Let us introduce the probability W c( e) of the capture of an electron crossing a GL. Considering the interaction of the electrons crossing the GL with the optical phonons in GL, optical phonons in the barrier layer material (WS2 [35]), and with the electrons located in the GLs, one can obtain the dependence of W ( e ) on the electron energy e . Figure 13.7 shows an example of the energy dependence of the capture probability w C( e , E ) for the electron density in GLs equal to 1012 cm–2 and the electric field of 104 V/cm. At not too low voltages when the electron system in the barrier layers is sufficiently far from equilibrium, the rate of the capture C GL into a GL of electrons incident from left and right is
Ú
C GL µ
•
0
dpz u zWC (e z )
ÏÔ È (pz + mbub )2 ˘ ¸Ô È ( p  mbub )2 ˘
¥ Ìexp Í z ˙˝ ˙ + exp Í
2mbTb 2mbTb ˙˚ ˛Ô
ÍÎ
˙˚
ÓÔ ÍÎ
Ú
2
•
0
Ê e ˆ deWC (e , E ) exp Á  ˜ .
Ë Tb ¯
(13.A1)
The current through the GL (assuming that the capture probability W C( e ) is small) is given
Ú
j µ
•
0
dpz u z
ÏÔ È (pz + mbub )2 ˘ ¸Ô È (p  mbub )2 ˘
¥ Ìexp Í z ˙  exp Í
˙˝ 2mbTb 2mbTb ÍÎ
˙˚ Ô˛
ÔÓ ÍÎ
˚˙
Appendix
Ú
2
•
0
Ê e ˆ Ê 2mbe ub ˆ de exp Á  ˜ Á ˜. Tb Ë Tb ¯ Ë ¯
(13.A2)
Here, T b , m b , and b ( E ) are the effective electron temperature, the effective mass, and mobility in the material of the barrier layers, respectively, and u b = b(E)E is the drift velocity across the barrier. Thus introducing the capture parameter p C as C = p C j/e, we obtain
Ú
0
pC =
Ú
•
0
=
•
Ê eˆ deWC (e )exp Á  ˜ Ë Tb ¯
Ê e ˆ Ê 2mbe ub ˆ de exp Á  ˜ Á ˜ Tb Ë Tb ¯ Ë ¯
2uT p ub
Ú
• deW (e ) C
0
Tl
Ê eˆ exp Á  ˜ . Ë Tb ¯
As it should follow from Eq. (13.A3): pC
WC uT b(E )E
,
,
(13.A3) (13.A4)
where ·W C Ò is the average capture probability, uT = Tb / 2mb is the thermal velocity (in the barrier layer), and b (E) is the electron mobility in the barrier layers. Figure 13.8 shows the average capture probability as function of the electron temperature in the barrier T b . As seen, the average capture probability is weakly dependent on the electric field (affecting the electron wave functions in the barrier layers) in a wide range of the latter (at least up to 105 V/cm). If the electric field E is smaller than that corresponding to the electron velocity saturation in the material of the barriers E S , Eq. (13. A4) yields p C = E C/E, i.e., Eq. (13.8), where E C ·W C Òut / b . Setting the lowfield mobility perpendicular to the layers equal to b = 10 – 15 cm2/V ◊ s, i.e., somewhat lower than the achieved values of lateral mobility of WS2 [36–39], and uT = 107 cm/s, for T b = 300–400 K, we obtain W C ( e ) ~ 1.5 ¥ 10–3 (see Fig. 13.8). This leads to the following estimate: E C (1.0–1.5) kV/cm. Lower transverse mobility, higher doping of GLs, and the inclusion of other mechanisms (say, the capture associated with the plasmon emission) can result in some increase in ·W C Ò and EC. In the main text, we assume that E C = 1.5 and 7.5 kV/cm. Note that Eq. (13.8) is valid at E n EC.
251
252
Vertical Electron Transport in van der Waals Heterostructures
References 1. A. K. Geim and I. V. Grigorieva, Nature, 499, 419 (2013).
2. M. Liu, X. Yin, and X. Zhang, Nano Lett., 12, 1482 (2012).
3. L. Britnell, R. V. Gorbachev, R. Jalil, B. D. Belle, F. Shedin, A. Mishenko, T. Georgiou, M. I. Katsnelson, L. Eaves, S. V. Morozov, N. M. R. Peres, J. Leist, A. K. Geim, K. S. Novoselov, and L. A. Ponomarenko, Science, 335, 947 (2012). 4. L. Britnell, R. V. Gorbachev, R. Jalil, B. D. Belle, F. Schedin, M. I. Katsnelson, L. Eaves, S. V. Morozov, A. S. Mayorov, N. M. R. Peres, A. H. Castro Neto, J. Leist, A. K. Geim, L. A. Ponomarenko, and K. S. Novoselov, Nano Lett., 12, 1707 (2012).
5. T. Georgiou, R. Jalil, B. D. Bellee, L. Britnell, R. V. Gorbachev, S. V. Morozov, Y.J. Kim, A. Cholinia, S. J. Haigh, O. Makarovsky, L. Eaves, L. A. Ponomarenko, A. K. Geim, K. S. Nonoselov, and A. Mishchenko, Nat. Nanotechnol., 8, 100 (2013).
6. L. Britnell, R. V. Gorbachev, A. K. Geim, L. A. Ponomarenko, A. Mishchenko, M. T. Greenaway, T. M. Fromhold, K. S. Novoselov, and L. Eaves, Nat. Commun., 4, 1794 (2013).
7. V. Ryzhii, T. Otsuji, M. Ryzhii, V. G. Leiman, S. O. Yurchenko, V. Mitin, and M. S. Shur, J. Appl. Phys., 112, 104507 (2012). 8. V. Ryzhii, T. Otsuji, M. Ryzhii, and M. S. Shur, J. Phys. D: Appl. Phys., 45, 302001 (2012). 9. V. Ryzhii, A. Satou, T. Otsuji, M. Ryzhii, V. Mitin, and M. S. Shur, J. Phys. D: Appl. Phys., 46, 315107 (2013).
10. V. Ryzhii, M. Ryzhii, V. Mitin, M. S. Shur, A. Satou, and T. Otsuji, J. Appl. Phys., 113, 174506 (2013).
11. V. Ryzhii, A. A. Dubinov, V. Ya. Aleshkin, M. Ryzhii, and T. Otsuji, Appl. Phys. Lett., 103, 163507 (2013).
12. V. Ryzhii, A. A. Dubinov, T. Otsuji, V. Ya. Aleshkin, M. Ryzhii, and M. S. Shur, Opt. Express, 21, 31567 (2013).
13. V. Ryzhii, T. Otsuji, V. Ya. Aleshkin, A. A. Dubinov, M. Ryzhii, V. Mitin, and M. S. Shur, Appl. Phys. Lett., 104, 163505 (2014).
14. C. Oh Kim, S. Kim, D. H. Shin, S. S. Kang, J. M. Kim, C. W. Jang, S. S. Joo, J. S. Lee, J. H. Kim, S.H. Choi, and E. Hwang, Nat. Commun., 5, 3249 (2014).
15. A. Mishchenko, J. S. Tu, Y. Cao, R. V. Gorbachev, J. R. Wallbank, M. T. Greenaway, V. E. Morozov, S. V. Morozov, M. J. Zhu, S. L. Wong, F. Withers, C. R. Woods, Y.J. Kim, K. Watanabe, T. Taniguchi, E. E. Vdovin,
References
O. Makarovsky, T. M. Fromhold, V. I. Fal’ko, A. K. Geim, L. Eaves, and K. S. Novoselov, Nat. Nanotechnol., 9, 808 (2014).
16. C.H. Liu, Y.C. Chang, T. B. Norris, and Z. Zhong, Nat. Nanotechnol., 9, 273 (2014).
17. V. Ryzhii, A. Satou, T. Otsuji, M. Ryzhii, V. Mitin, and M. S. Shur, J. Appl. Phys., 116, 114504 (2014). 18. S. Luryi, Appl. Phys. Lett., 52, 501 (1988).
19. H. C. Liu, Appl. Phys. Lett., 60, 1507 (1992).
20. E. Rosencher, B. Vinter, F. Luc, L. Thibaudeau, P. Bois, and J. Nagle, IEEE J. Quantum Electron., 30, 2875 (1994).
21. V. Ryzhii, J. Appl. Phys., 81, 6442 (1997).
22. J. A. Brum and G. Bastard, Phys. Rev. B, 33, 1420 (1986).
23. L. Thibaudeau and B. Vinter, Appl. Phys. Lett., 65, 2039 (1994).
24. D. Bradt, Y. M. Sirenko, and V. Mitin, Semicond. Sci. Technol., 10, 260 (1995). 25. M. Ryzhii and V. Ryzhii, Jpn. J. Appl. Phys., Part 1, 38, 5922 (1999).
26. M. Ershov, V. Ryzhii, and C. Hamaguchi, Appl. Phys. Lett., 67, 3147 (1995).
27. L. Thibaudeau, P. Bois, and J. Y. Duboz, J. Appl. Phys., 79, 446 (1996).
28. M. Ershov, H. C. Liu, M. Buchanan, Z. R. Wasilewski, and V. Ryzhii, Appl. Phys. Lett., 70, 414 (1997).
29. V. Ryzhii and H. C. Liu, Contact and spacecharge effects in quantum well infrared photodetectors, Jpn. J. Appl. Phys., Part 1, 38, 5815 (1999). 30. V. Ryzhii, M. Ryzhii, and H. C. Liu, J. Appl. Phys., 92, 207 (2002).
31. E. Watanabe, A. Conwill, D. Tsuya, and Y. Koide, Diamond Relat. Mater., 24, 171 (2012).
32. J. S. Moon, M. Antcliffe, H. C. Seo, D. Curtis, S. Lin, A. Schmitz, I. Milosavljevic, A. A. Kiselev, R. S. Ross, D. K. Gaskill, P. M. Campbell, R. C. Fitch, K.M. Lee, and P. Asbeck, Appl. Phys. Lett., 100, 203512 (2012). 33. A. Hsu, H. Wang, K. K. Kim, J. Kong, and T. Palacios, IEEE Electron Device Lett., 32, 1008 (2011).
34. L. Wang, I. Meric, P. Y. Huang, Q. Gao, Y. Gao, H. Tran, T. Taniguchi, K. Watanabe, L. M. Campos, D. A. Muller, J. Guo, P. Kim, J. Hone, K. L. Shepard, and C. R. Dean, Science, 342, 614 (2013).
35. H. Shi, H. Pan, Y.W. Zhang, and B. Yakobson, Phys. Rev. B, 87, 155304 (2013). 36. D. Braga, I. Gutiérrez Lezama, H. Berger, and A. F. Morpurgo, Nano Lett., 12, 5218 (2012).
253
254
Vertical Electron Transport in van der Waals Heterostructures
37. N. Huo, Sh. Yang, Zh. Wei, S.S. Li, J.B. Xia, and J. Li, Sci. Rep., 4, 5209 (2014).
38. S. Jo, N. Ubrig, H. Berger, A. B. Kuzmenko, and A. F. Morpurgo, Nano Lett., 14, 2019 (2014).
39. D. Ovchinnikov, A. Allain, Y.S. Huang, D. Dumcenco, and A. Kis, ACS Nano, 8, 8174 (2014).
Chapter 14
Giant Plasmon Instability in DualGratingGate Graphene FieldEffect Transistor*
Y. Koseki,a V. Ryzhii,a T. Otsuji,a V. V. Popov,b,c,d and A. Satoua aResearch
Institute of Electrical Communication, Tohoku University, Sendai 9808577, Japan bKotelnikov Institute of Radio Engineering and Electronics (Saratov Branch), 410019 Saratov, Russia cSaratov State University, Saratov 410012, Russia dSaratov Scientific Center of the Russian Academy of Sciences, Saratov 410028, Russia [email protected]
We study instability of plasmons in a dualgratinggate graphene fieldeffect transistor induced by dc current injection using selfconsistent simulations with the Boltzmann equation. With only the acousticphononlimited electron scattering, it is demonstrated that
*Reprinted with permission from Y. Koseki, V. Ryzhii, T. Otsuji, V. V. Popov, and A. Satou (2016). Giant plasmon instability in a dualgratinggate graphene fieldeffect transistor, Phys. Rev. B, 93, 245408. Copyright © 2016 The American Physical Society. GrapheneBased Terahertz Electronics and Plasmonics: Detector and Emitter Concepts Edited by Vladimir Mitin, Taiichi Otsuji, and Victor Ryzhii
Copyright © 2021 Jenny Stanford Publishing Pte. Ltd.
ISBN 9789814800754 (Hardcover), 9780429328398 (eBook)
www.jennystanford.com
256
Giant Plasmon Instability in DualGratingGate Graphene FieldEffect Transistor
a total growth rate of the plasmon instability, with the terahertz/ midinfrared range of the frequency, can exceed 4 ¥ 1012 s–1 at room temperature, which is an order of magnitude larger than in twodimensional electron gases based on usual semiconductors. By comparing the simulation results with existing theory, it is revealed that the giant total growth rate originates from simultaneous occurrence of the socalled Dyakonov–Shur and Ryzhii–Satou–Shur instabilities.
14.1 Introduction
Electronic, hydrodynamic, and electromagnetic properties of twodimensional (2D) plasmons in channels of fieldeffect transistors (FETs) have been investigated extensively for their utilization to terahertz (THz) devices [1–6] (see also review papers [7–10] and references therein). Especially, plasmon instability is one of the most important properties to realize compact, roomtemperature operating THz sources. Selfexcitation of plasmons due to instability induces ac voltages in the gate electrodes and, in turn, leads to the emission of THz waves. The socalled Dyakonov–Shur (DS) instability [2, 11–13] and Ryzhii–Satou–Shur (RSS) instability [14–16] in singlegate FETs were proposed theoretically as mechanisms of plasmon instability by dc current injection through the transistor channel. The DS instability originates from the Doppler shift effect at asymmetric boundaries in the channel, i.e., zero time variation of potential at the source contact and zero time variation of electron velocity near the drain contact, which are naturally realized by operating the FET in the saturation regime. In the same saturation regime, the RSS instability takes place due to the transittime effect of fastmoving electrons in the highfield region in the drain side. Alternatively, the socalled dualgratinggate structure (see Fig. 14.1a), in which two types of interdigitately placed gates form a very efficient grating coupler between THz waves and 2D plasmons [17, 18], has been proposed for direct THz emission without antenna integration [17, 19]. The RSS instability in this structure has been investigated analytically [16]. In addition, asymmetry of the gate placement expects to lead to partial realization of the asymmetric boundary conditions and, in turn, of the DS instability [9, 10].
Introduction
However, in FETs or highelectronmobility transistors (HEMTs) based on usual semiconductors (Si and compound semiconductors such as InGaAs and GaN), growth rates of the instabilities are of the order of 1011 s–1, which are limited by electron saturation velocities (2 ¥ 107 cm/s in the GaAs channel). With such low growth rates the plasmons are easily damped out at room temperature by a large damping rate (1012 s–1) associated with electron scattering. Plasmons in graphene have then attracted much attention owning to its gapless energy spectrum and massless carriers [20–29]. The most straightforward yet striking advantage of graphene plasmons over those in usual semiconductors is its ultimately low scattering rate at room temperature, if external scattering sources in graphene such as impurities and defects and those induced by the substrate and gate insulator are excluded and the electron scattering is limited only by the acousticphonon scattering [30] in graphene. Then, the plasmon damping rate can be down to 1011 s–1 [31], together with the electron drift velocity up to 108 cm/s. These lead to an expectation that the plasmon instabilities in graphene are very strong and can take place at room temperature. Although the technology of graphene fabrication with ulitimately high quality still needs to be progressed, a recent experimental report on graphene encapsulated into hexagonal boron nitride layers [32], which demonstrated the electron mobility at room temperature comparable to the acousticphononlimited value, supports its feasibility. In this chapter, we conduct simulations of the plasmon instabilities in the dualgratinggate graphene FET with dc current injection, assuming the acousticphononlimited scattering rate at room temperature, and demonstrate occurrence of giant instabilities with their total growth rate (which we define as the growth rate subtracting the damping rate) exceeding 4 ¥ 1012 s–1 and with the plasmon frequency ranging in the THz/midinfrared range. We show the gatelength dependence of the plasmon frequency and the total growth rate extracted from the simulations, and we found distinct dependences of growth rates specific to the DS and RSS instabilities [2, 14], thus identifying the giant total growth rate as simultaneous occurrence, or more specifically, a linear superposition of those instabilities.
257
258
Giant Plasmon Instability in DualGratingGate Graphene FieldEffect Transistor
,m Figure 14.1 Schematic views of (a) a dualgratinggate graphene FET and (b) a profile of steadystate electron concentration under consideration.
14.2 Mechanisms of Dyakonov–Shur and Ryzhii–Satou–Shur Instabilities The mechanisms of the DS and RSS instabilities and their features are summarized as follows. The DS instability originates from the Doppler shift effect at asymmetric boundaries. In case of FETs in the saturation regime, the potential is fixed at the source side (the short boundary), while the current, i.e., the electron velocity is fixed at the drain side (the open boundary). Between these asymmetric boundaries, a resonant cavity for plasmons is formed. Then, the open boundary reflects traveling plasmons towards it with the current amplitude preserved, whereas the short boundary reflects them with amplification. The resonant frequency of the excited plasmons is determined by geometrical factors (gate length, gate dielectric thickness, and lengths of ungated regions in the channel) and gate voltage through the electron concentration. The latter enables the tuning of the frequency. On the other hand, the RSS instability takes place in the same saturation regime due to the transittime effect of fastmoving electrons in the highfield region (i.e., the lowconcentration region) in the drain side. The electric field created by those electrons modulates the concentration at the edge of the highconcentration region and results in the bunching of electrons in the lowconcentration region. Depending on the length of the lowconcentration region and the electron velocity, it interferes with plasmons in the highconcentration region either constructively or destructively. The constructive interference corresponds to
Simulation Model
the instability. The plasmon frequency is again determined by the geometrical factors in the highconcentration region and the gate voltage. In case of dualgratinggate structures, both instabilities can be realized by following configurations. First, the resonant plasmon cavity can be formed by modulating the concentration profile through gate voltages in such a way that high and lowconcentration regions are created. This also enables the occurrence of the RSS instability. Second, asymmetry of the gate placement leads to partial realization of the asymmetric boundary conditions and, in turn, of the DS instability.
14.3 Simulation Model
Figure 14.1a shows a dualgratinggate graphene FET under consideration. In our simulation model, we assume that the number of periods of the grating gates is sufficiently large, i.e., the total channel length is longer than the THz/midinfrared wavelength, so that we can ignore effects of nonperiodicity, such as the presence of the source and drain contacts and we can consider one period as a unit cell. In addition, we assume that the channel width in the y direction is so long compared with the length of a period that the electron concentration in the channel, together with the geometry, can be treated as uniform in the y direction. We fix the thickness of the gate dielectric, Wg = 50 nm, the left spacings of the gates 1 and 2, sg1 = 200 nm, sg2 = 300 nm, whereas we vary the lengths of the gate 1 and 2, Lg1 and Lg2, in the range between 100 and 400 nm in order to reveal characteristics of the instabilities obtained in this work by comparison with existing theory. The values of those parameters were chosen such a way that frequencies of selfexcited plasmons fall into the THz/midinfrared range. The dielectric constant of media surrounding the graphene channel is set to Œ = 4. Figure 14.1b is a profile of the steadystate electron concentration without current flow, and it was calculated selfconsistently with a uniform electron doping Se = 5 ¥ 1011 cm–2, together with certain gate voltages. The slight electron doping is introduced to avoid plasmon damping due to the electronhole friction [27]; even at the point with the lowest electron concentration, the hole concentration is negligibly low,
259
260
Giant Plasmon Instability in DualGratingGate Graphene FieldEffect Transistor
Sh = 6.8 ¥ 109 cm–2. On the other hand, the highest electron concentration is set not so high that the difference between maximum and minimum Fermi energies (166 and 68.5 meV, respectively) does not exceed opticalphonon energies in graphene and thus electrons injected quasiballistically from the region with high electron concentration do not experience opticalphonon emission, which would critically hinder the RSS instability. We use the quasiclassical Boltzmann equation to describe the electron transport in the channel: p ∂f ∂f ∂f + uF x  eE x = J LA ( f  p), ∂t  p ∂x ∂px
(14.1)
where u = 108 cm/s is the Fermi velocity in graphene, Ex is the selfconsistent electric field in graphene, and p = (px, py) is the momentum. The boundary condition for Eq. (14.1) is periodic, i.e., fx=0 = fx=L. On the righthand side of Eq. (14.1), we take into account collision integrals for the acousticphonon scattering JLA, where JLA ( f  p) =
1
(2p )2
Ú dp¢ W
LA (p¢  p)[ f ( p¢ ) 
f ( p)],
(14.2)
and an explicit expression of the transition probability WLA can be found in Ref. [30]. We use the socalled weighted essentially nonoscillatory finitedifference scheme [33, 34] to solve Eq. (14.1), which is demonstrated to be applicable for graphene transport simulation [35]. The time step of the simulation was set to Dt = 0.05 fs to avoid numerical instabilities. Equation (14.1) is accompanied by the selfconsistent 2D Poisson equation ∇
· [Œ∇φ(t,x,z)] = 4πe[Σ(t,x) − Σe]δ(z),
(14.3)
where ∇ = (∂/∂x, ∂/∂z), φ is the electric potential, Σ = ∫dpf/π2ℏ2 is the electron concentration in the channel, and Σe is the electron doping concentration. The electric field in the channel can be found by Ex = −(∂φ/∂x)z=0. The boundary condition at x = 0 and L = 0 is periodic, while we set the natural boundary conditions, ∂φ/∂z = 0, at z = Wt and z = −Wb, where Wt and Wb are sufficiently large so that they do not affect the numerical results. Besides, the electron concentration in the channel expressed as a delta function in Eq. (14.3) is accounted for as a boundary condition at z = 0:
Simulation Model
∂j ∂z
z=+0
∂j ∂z
= z =0
4pe ( S  S e ). Œ
(14.4)
We use a finiteelement library called LIBMESH [36] to solve Eq. (14.3) with those boundary conditions. More details of the simulation model are given elsewhere [31].
Figure 14.2 Time evolution of the electric field at the middle of a channel region under the gate 2 with (a) Lg1 = 160 nm and (b) 110 nm. In both cases, the external electric field is set to Eext = 0.8 kV/cm. The insets show corresponding absolute value of the Fourier transform.
A simulation starts by applying a uniform external dc electric field in the channel direction Eext to inject positive sourcedrain dc current. To avoid unwanted plasmon excitation associated with an abrupt turnon of the dc electric field, an artificially large damping factor is set in front of the collision integral in Eq. (14.1), and it is gradually decreased to unity within 6 ps, which is much longer than the inverse of plasmon frequency obtained in the simulation. Then, the electron concentration, electric field, etc., begin to oscillate and their amplitudes increase with time, as shown in Fig. 14.2a. This is identified as occurrence of plasmon instability. In general, simulated oscillations contain several modes. Distinct fundamental modes can be obtained with certain sets of parameters, and the frequency and total growth rate can be easily extracted. However, with other sets they contain fundamental and second modes with very close frequencies and/or higher harmonics which have comparable amplitudes with the fundamental modes, resulting in the beating (see Fig. 14.2b) and/or the distortion of wave forms.
261
262
Giant Plasmon Instability in DualGratingGate Graphene FieldEffect Transistor
To extract the frequency and total growth rate of the fundamental mode, we perform the Fourier transform of the oscillation with respect to time, pick up the first peak and another close peak, if any, and perform a curve fitting to them with the following function: F(w ) =
g i 
Ei
Â 4p
i =1 ,2
g i2
+ (w  w i )2
.
(14.5)
Equation (14.5) is equal to the absolute value of the Fourier transform of the summation of two exponentially growing harmonic functions Si=1,2 Ei exp(git)cos(wit + qi) around its peak(s). As seen in the insets of Figs. 14.2a and b, the fundamental and adjacent second modes can be well separated by this method.
Figure 14.3 (a) Total growth rate and (b) frequency of the fundamental plasmon mode as functions of the length of the gate 1 (circles with solid lines) and theoretical fitting curves (dashed lines).
14.4 Results and Discussion Figures 14.3a and b show the total growth rate and frequency of the fundamental mode as a function of the length of the gate 1 with Eext = 0.8 kV/cm and with Lg2 = 300 nm. They clearly demonstrates the
Results and Discussion
total growth rate of the instability exceeding 4 ¥ 1012 s–1 with the frequency in the THz/midinfrared range. This value is an order of magnitude larger than achievable in FETs or HEMTs based on usual semiconductors at room temperature. This giant total growth rate of the plasmon instability in the dualgratinggate graphene FET is attributed to the lower plasmon damping and also to the larger drift velocity, both originating from the lower scattering rate limited only by acoustic phonons. This point shall be discussed in more detail shortly later. The gatelength dependence of the total growth rate exhibits an oscillatory behavior; the oscillation period becomes shorter and the amplitude becomes larger as the gate length becomes shorter. It is specific to the RSS instability, and it corresponds to the constructive/destructive interference between plasmons in the highconcentration region (under gate 1) and the bunched electrons in the lowconcentration region (under gate 2). This effect is illustrated in Fig. 14.4, where an oscillation of the electron velocity is built up at the left edge of the highconcentration region (near x = 150 nm), where the electrons are injected to the lowconcentration region. Besides, there is a monotonically increasing portion of the total growth rate with decreasing Lg1 in Fig. 14.3a. This can be attributed to the DS instability, in which the growth rate is inversely proportional to the traveling time of plasmons in the gated region and therefore to the gate length [2]. Those characteristics signify the simultaneous occurrence of the DS and RSS instabilities. In fact, the overall characteristics of the growth rate can be described qualitatively well by the formula according to Ref. [15], which is a linear superposition of the growth rates of those instabilities: g =
uDS uRSS Ê Lg ˆ J0 Á ˜, Lg1 Lg1 Ë Lg1 ¯
(14.6)
where uDS = 4 ¥ 107 cm/s, uRSS = 7.5 ¥ 107 cm/s, and Lg = 5800 nm are fitting parameters (see the fitting curve in Fig. 14.3a). As seen in Fig. 14.3b, the frequency is almost inversely proportional to Lg1, and it obeys the wellknown dispersion of gated 2D plasmons, f =
sg1
Lg1
,
(14.7)
263
Giant Plasmon Instability in DualGratingGate Graphene FieldEffect Transistor
ime, ps Velocity, ×107cm/s
where sg1 = 1.15 ¥ 108 cm/s is the plasmon phase velocity which is extracted as a fitting parameter and which is quantitatively consistent with the value calculated analytically [20] for the region under gate 1. −4 −3 −2 −1 0 11
10.8
T Elapsed
264
10.6 10.4 0
200 400 600 800 1,000
Position, nm
Figure 14.4 Time evolution of the electron velocity distribution after the onset of plasmon instability, in the case with Lg1 = 160 nm and Lg2 = 300 nm.
The giant instability found here at room temperature originates from the ultimately weak electron scattering rate in graphene, and there are two factors for this: (1) the weak damping of plasmons and (2) the large drift velocity in both high and lowconcentration regions that leads to large DS and RSS instabilities, respectively. First, the estimated damping rate was around 1.2 ¥ 1011 s–1 in the lowconcentration region and 2.5 ¥ 1011 s–1 in the highconcentration region; note that the electron scattering rate, and thus the plasmon damping rate, for the acousticphonon scattering is proportional to the square root of the electron concentration [30, 31]. Such low values of the plasmon damping rate can be achieved only at nitrogen temperature or lower in other materials. It is worth mentioning that the lowconcentration region with adjacent ungated regions acts as a better (passive) plasmon resonant cavity, while the instabilities take place primarily for plasmons in the highconcentration region, as is evident from the dependence of the frequency on Lg1 and its consistency with Eq. (14.7), and the frequency is insensitive to the length of the gate 2, as shown in Fig. 14.5 (in contrast, the total growth rate can vary with it). This is similar to the situation discussed in
Conclusion
4
12 1
5 4 3 2 1 0 200
3 2 Eext = 0.8 kV/cm Lg1 = 200 nm
250
300
Lg2, nm
350
1 0 400
Growth rate, ×10 s
Frequency, THz
Ref. [37], where the ungated plasmon resonance can be effectively tuned by the gated region of the channel. In fact, it can be seen in Fig. 14.4 that a higher harmonic oscillation with more than one node is excited in the lowconcentration region. This, together with the oscillation in the highconcentration region, form the fundamental mode of the whole period.
Figure 14.5 Total growth rate and frequency of the fundamental mode as functions of the length of gate 2.
In addition, values of drift velocities obtained in the simulation, 4 ¥ 107 cm/s in the lowconcentration region and 107 cm/s in the highconcentration region, confirm the factor (2) for the giant growth rate. Especially the former is more than twice larger than the saturation velocity in Si and InGaAs channels. However, the velocities extracted by Eq. (14.6) as fitting parameters differ from these values by several factors. A reasonable explanation to this discrepancy is that the DS instability also takes place not only in the highconcentration region but also in the lowconcentration region. Figure 14.4 exhibits waves propagating in opposite directions in the latter, suggesting the occurrence of the DS instability there. This should add a constant term in Eq. (14.6), and then the fitting velocities should become closer to the simulated values.
14.5 Conclusion
In conclusion, we have conducted simulations of plasmon instability driven by dc current injection in the dualgratinggate graphene FET. We have obtained a giant total growth rate of the instability at room temperature exceeding 4 ¥ 1012 s–1. Through the dependences of the
265
266
Giant Plasmon Instability in DualGratingGate Graphene FieldEffect Transistor
total growth rate and frequency on the gate lengths, we have revealed that the giant total growth rate originates from simultaneous occurrence of the DS and RSS instabilities. The obtained result strongly suggests that a graphene FET with the dualgratinggate structure is very promising for the realization of a highpower, compact, roomtemperature operating THz source.
Acknowledgments
This work was financially supported by Japan Society for the Promotion of Science (JSPS) GrantinAid for Young Researcher (No. 26820122), by JSPS GrantinAid for Specially Promoted Research (No. 23000008), and by JSPS and Russian Foundation for Basic Research under JapanRussia Research Cooperative Program. The simulation was carried out using the computational resources provided by Research Institute for Information Technology Center, Nagoya University, through the HPCI System Research Project (No. hp140086), by the Information Technology Center, the University of Tokyo, and by Research Institute for Information Technology, Kyushu University.
References
1. S. J. Allen, D. C. Tsui, and R. A. Logan, Phys. Rev. Lett., 38, 980 (1977). 2. M. Dyakonov and M. Shur, Phys. Rev. Lett., 71, 2465 (1993).
3. M. Dyakonov and M. Shur, IEEE Trans. Electron Devices, 43, 380 (1996). 4. D. Veksler, F. Teppe, A. P. Dmitriev, V. Y. Kachorovskii, W. Knap, and M. S. Shur, Phys. Rev. B, 73, 125328 1 (2006).
5. G. C. Dyer, G. R. Aizin, S. J. Allen, A. D. Grine, D. Bethke, J. L. Reno, and E. A. Shaner, Nat. Photonics, 7, 925 (2013).
6. I. V. Rozhansky, V. Y. Kachorovskii, and M. S. Shur, Phys. Rev. Lett., 114, 246601 (2015).
7. M. S. Shur and V. Ryzhii, Int. J. High Speed Electron. Syst., 13, 575 (2003). 8. W. Knap, M. Dyakonov, D. Coquillat, F. Teppe, N. Dyakonova, J. Lusakowski, K. Karpierz, M. Sakowicz, G. Valusis, D. Seliuta, I. Kasalynas, A. Fatimy, Y. M. Meziani, and T. Otsuji, J. Infrared, Millimeter, Terahertz Waves, 30, 1319 (2009). 9. T. Otsuji and M. Shur, IEEE Microwave Mag., 15, 43 (2014).
References
10. T. Otsuji, IEEE Trans. Terahertz Sci. Technol., 5, 1110 (2015).
11. A. P. Dmitriev, A. S. Furman, V. Y. Kachorovskii, G. G. Samsonidze, and G. G. Samsonidze, Phys. Rev. B, 55, 10319 (1997).
12. M. Dyakonov and M. S. Shur, Appl. Phys. Lett., 87, 111501 (2005).
13. V. V. Popov, G. M. Tsymbalov, and M. S. Shur, J. Phys.: Condens. Matter, 20, 384208 (2008).
14. V. Ryzhii, A. Satou, and M. S. Shur, Phys. Status Solidi A, 202, 113 (2005).
15. V. Ryzhii, A. Satou, and M. S. Shur, IEICE Trans. Electron. E89C, 1012 (2006). 16. V. Ryzhii, A. Satou, M. Ryzhii, T. Otsuji, and M. S. Shur, J. Phys.: Condens. Matter, 20, 384207 (2008).
17. T. Otsuji, M. Hanabe, T. Nishimura, and E. Sano, Opt. Express, 14, 4815 (2006). 18. V. V. Popov, D. V. Fateev, T. Otsuji, Y. M. Meziani, D. Coquillat, and W. Knap, Appl. Phys. Lett., 99, 243504 (2011).
19. T. Otsuji, Y. M. Meziani, T. Nishimura, T. Suemitsu, W. Knap, E. Sano, T. Asano, and V. V. Popov, J. Phys.: Condens. Matter, 20, 384206 (2008). 20. V. Ryzhii, Jpn. J. Appl. Phys., 45, L923 (2006).
21. V. Ryzhii, A. Satou, and T. Otsuji, J. Appl. Phys., 101, 24509 (2007). 22. S. A. Mikhailov, Phys. Rev. B, 84, 045432 (2011).
23. A. A. Dubinov, V. Y. Aleshkin, V. Mitin, T. Otsuji, and V. Ryzhii, J. Phys.: Condens. Matter, 23, 145302 (2011). 24. L. Ju, B. Geng, J. Horng, C. Girit, M. Martin, Z. Hao, H. a. Bechtel, X. Liang, A. Zettl, Y. R. Shen, and F. Wang, Nat. Nanotechnol., 6, 630 (2011).
25. L. Vicarelli, M. S. Vitiello, D. Coquillat, A. Lombardo, A. C. Ferrari, W. Knap, M. Polini, V. Pellegrini, and A. Tredicucci, Nat. Mater., 11, 865 (2012). 26. B. Wang, X. Zhang, F. J. GarcíaVidal, X. Yuan, and J. Teng, Phys. Rev. Lett., 109, 073901 (2012). 27. D. Svintsov, V. Vyurkov, S. Yurchenko, T. Otsuji, and V. Ryzhii, J. Appl. Phys., 111, 083715 (2012).
28. A. N. Grigorenko, M. Polini, and K. S. Novoselov, Nat. Photonics, 6, 749 (2012).
29. V. V. Popov, O. V. Polischuk, S. A. Nikitov, V. Ryzhii, T. Otsuji, and M. S. Shur, J. Opt., 15, 114009 (2013).
267
268
Giant Plasmon Instability in DualGratingGate Graphene FieldEffect Transistor
30. E. H. Hwang and S. Das Sarma, Phys. Rev. B, 77, 115449 (2008).
31. A. Satou, V. Ryzhii, F. T. Vasko, V. V. Mitin, and T. Otsuji, Proc. SPIE, 8624, 862412 (2013).
32. L. Wang, I. Meric, P. Y. Huang, Q. Gao, Y. Gao, H. Tran, T. Taniguchi, K. Watanabe, L. M. Campos, D. A. Muller, J. Guo, P. Kim, J. Hone, K. L. Shepard, and C. R. Dean, Science, 342, 614 (2013).
33. J. A. Carrillo, I. M. Gamba, A. Majorana, and C.w. Shu, J. Comput. Phys., 184, 498 (2003).
34. M. Galler and F. Schürrer, J. Comput. Phys., 212, 778 (2006).
35. P. Lichtenberger, O. Morandi, and F. Schürrer, Phys. Rev. B, 84, 045406 (2011). 36. B. S. Kirk, J. W. Peterson, R. H. Stogner, and G. F. Carey, Eng. Comput., 22, 237 (2006). 37. V. V. Popov, A. N. Koudymov, M. Shur, and O. V. Polischuk, J. Appl. Phys., 104, 024508 (2008).
Part 2
Detectors Based on Lateral
Transport in Graphene and
Graphene Structures
Chapter 15
Plasma Mechanisms of Resonant Terahertz Detection in a TwoDimensional Electron Channel with Split Gates*
V. Ryzhii,a A. Satou,a T. Otsuji,b and M. S. Shurc aComputer
Solid State Physics Laboratory, University of Aizu,
AizuWakamatsu 9658580, Japan
bResearch Institute of Electrical Communication, Tohoku University,
Sendai 9808577, Japan
cDepartment of Electrical, Computer, and Systems Engineering,
Rensselaer Polytechnic Institute, Troy, New York 12180, USA
[email protected]
We analyze the operation of a resonant detector of terahertz (THz) radiation based on a twodimensional electron gas (2DEG) channel with split gates. The side gates are used for the excitation of plasma oscillations by incoming THz radiation and control of the resonant plasma frequencies. The central gate provides the potential barrier
*Reprinted with permission from V. Ryzhii, A. Satou, T. Otsuji, and M. S. Shur (2008). Plasma mechanisms of resonant terahertz detection in a twodimensional electron channel with split gates, J. Appl. Phys., 103, 014504. Copyright © 2008 American Institute of Physics. GrapheneBased Terahertz Electronics and Plasmonics: Detector and Emitter Concepts Edited by Vladimir Mitin, Taiichi Otsuji, and Victor Ryzhii
Copyright © 2021 Jenny Stanford Publishing Pte. Ltd.
ISBN 9789814800754 (Hardcover), 9780429328398 (eBook)
www.jennystanford.com
272
Plasma Mechanisms of Resonant Terahertz Detection
separating the source and drain portions of the 2DEG channel. Two possible mechanisms of the detection are considered: (1) modulation of the ac potential drop across the barrier and (2) heating of the 2DEG due to the resonant plasmaassisted absorption of THz radiation followed by an increase in thermionic dc current through the barrier. Using the device model we calculate the frequency and temperature dependences of the detector responsivity associated with both dynamic and heating (bolometric) mechanisms. It is shown that the dynamic mechanisms dominates at elevated temperatures, whereas the heating mechanism provides larger contribution at low temperatures, T ≲ 35–40 K.
15.1 Introduction
Plasma oscillations in heterostructures with a twodimensional electron gas (2DEG) and some devices using the excitation of these oscillations have been experimentally studied over decades (see, for instance, Refs. [1–17]). There are also many theoretical papers on different aspects of these plasma waves and their potential applications. The gated and ungated 2DEG channels in heterostructures can serve as resonant cavities for terahertz (THz) electron plasma waves [18]. The resonant properties of such channels can be utilized in different THz devices, in particular, resonant detectors [3–5, 9, 10, 12–17]. The mechanism of the THz detection observed in transistor structures [3, 4, 6, 7, 9, 10, 15–17] might be attributed to the nonlinearity of the plasma oscillations as suggested previously [18]. The variation of the conductivity of 2DEG with periodic gate system can be possibly explained by the heating of 2DEG by absorbed THz radiation (heating or bolometric mechanism) [5, 13]. Recently, a concept of resonant detectors in which a plasma resonant cavity is integrated with a Schottky junction has been proposed and substantiated [19, 20]. As shown, when the frequency of incoming THz radiation is close to one of the plasma resonant frequencies, the ac potential drop across the barrier at the Schottky junction becomes resonantly large. This leads to rather large values of the rectified component of the current through the junction, which is used as output signal of the detector. Since the resonant excitation of the plasma oscillations by absorbed THz radiation
Introduction
Vg
Vd+Vω cos ω t Vcg Lcg
W
Vg
2l 2DEG channels Cgg Cg
Source L c
Depletion region Gates
Ccg Rc
Cgg Ccg
Cdr
Rc
Cg L c Drain
R dr
Figure 15.1 Schematic view of the THz detector under consideration and its simplified equivalent circuit.
leads to the heating of 2DEG, the heating (bolometric) mechanism can also contribute to the rectified current over the Schottky barrier. Thus, two mechanisms can be responsible for the operation of this detector: the dynamic mechanism considered previously [19] and the heating mechanism. Similar mechanisms can work in the detectors utilizing the excitation of plasma oscillations but having the barrier of another origin. In particular, the barrier formed by an additional gate which results in an essential depletion under it was used in recent experiments [14]. In this chapter, we develop a device model for a THz resonant detector based on a heterostructure with the 2DEG channel and the barrier region utilizing the plasma oscillations excitation. We consider a device with three gates (see Fig. 15.1): the 2DEG under two extreme gates forms the plasma resonant cavities, while the central gate, to which a sufficiently large negative bias voltage is applied, forms the barrier. The excitation of the plasma oscillations by the incident THz radiation is assumed to be associated with an antenna connected with the source and drain contacts to the 2DEG channel. In the following, we demonstrate that each of the mechanisms in question can dominate in different temperature ranges (the dynamic mechanism is predominant at elevated temperatures, whereas the heating mechanism provides a
273
274
Plasma Mechanisms of Resonant Terahertz Detection
larger contribution at low temperatures, T ≲ 35–40 K). The device structure under consideration differs from that studied in Ref. [14], in which the THz radiation input was realized by a periodic grating. However, the physical mechanisms of detection are the same.
15.2 Equations of the Model
We assume that the net drainsource voltage V includes both the dc bias voltage Vd and the ac component Vw cos wt induced by incoming THz radiation via an antenna connected with the source and drain contacts. Thus, V = Vd + Vw cos wt, where w is the THz radiation frequency. The bias voltage Vg is applied between the side gates and the pertinent contacts. This voltage affects the electron density in the quasineutral portions of the 2DEG channel, so that the dc electron density is given by Â0 = Â d +
æVg
4p eW
,
(15.1)
where e is the electron charge, W is the gate layer thickness, and æ is the dielectric constant. It is also taken to be that the potential drop, Vcg, between the central gate and the source contact is negative and its absolute value is sufficiently large to deplete some portion of the 2DEG channel underneath this gate and create a potential barrier. This implies that Vcg < –4peW/æSd = Vth, where Vth is the 2DEG threshold voltage. The ac component of the electric potential in the channel dj satisfies the boundary conditions which follow from the fact that at the source and drain contacts its values coincide with the ac components of the incoming signal voltage: dj
x =L = dj x =+L
1 = Vw cos wt . 2
(15.2)
Assuming that at the conductivity of the quasineutral sections is much larger than that of depletion region (including the thermionic current over the barrier and the displacement current associated with the capacitances shown in the equivalent circuit of Fig. 15.1), one may use the following additional conditions: ∂ dj 0. ∂x x =±l
(15.3)
Equations of the Model
Here 2L is the length of the 2DEG channel between the source and drain contacts, 2l > Lcg is the length of the depletion region under the central gate, and Lcg is the length of the latter (see Fig. 15.1). The quantity l is determined by the potential of the central gate Vcg. Definitely, the conductivity of the quasineutral sections markedly exceeds the real part of the depleted region admittance. The role of the displacement current across the depleted region is discussed in Section 15.8. The electron transport in the channel is governed by the hydrodynamic equations coupled with the Poisson equation for the selfconsistent electric potential [18]. At sufficiently small intensities of THz radiation, this system of equations can be linearized and reduced to the following equation [21, 22] valid in the quasineutral regions of the channel (–L £ x < –l and l < x £ L): ∂Ê ∂ ∂2 ˆ + v˜ dj = s2 2 dj , Á ¯ ∂t Ë ∂t ∂x
(15.4)
where v is the frequency of electron collisions with impurities and
phonons, s = 4p e2 S 0W / mæ is the plasma wave velocity, and m is the electron effective mass. The effect of electron pressure results in some renormalization of the plasma wave velocity [23–25]:
s = (4p e2 S 0W / mæ) + s02 , where s0 is the velocity of the electron “sound” (usually s0 s). Assuming that the central gate length is comparable with the gate layer thickness, the shape of the barrier under the central gate can be considered as parabolic: Db(x) = Db[1 – (x/l)2] – e(Vd + dVb)(l + x)/2l, where Db is the barrier height in equilibrium (it depends on potential, Vcg, of the central gate), and Vd + dVb is the lateral potential drop across the depletion (barrier) region associated with the dc bias voltage Vd and the ac voltage dVb. The variation of the barrier height dDb due to the lateral potential drop is given by dD b = 
e(Vd + dV b ) È e(Vd + dV b ) ˘ e(Vd + dV b ) . Í1 ˙2 8D b 2 ÍÎ ˙˚
(15.5)
Hence, at eVd + dVb Db, the net sourcedrain current can be calculated using the following formula: È e(V + dV b ) ˘ ¸Ô Ê D ˆ ÏÔ J = J m exp Á  b ˜ Ìexp Í d ˙  1˝ , Ë kBT ¯ ÓÔ ˚˙ Ô˛ ÎÍ 2kBT
(15.6)
275
276
Plasma Mechanisms of Resonant Terahertz Detection
where Jm is the maximum current (for a 2DEG Jm µ T3/2), the ac potential drop, dVb, across the depletion (barrier) region is given by
dV b = dj x =+ l  dj x = l = 2dj x =+l ,
(15.7)
and T = T0 + dT is the electron temperature, T0 is the lattice temperature, and dT is the variation of the electron temperature due to THz irradiation. In this case, at edVb < kBT < Db, Eq. (15.6) yields the following equation for the dc sourcedrain current J0: Ê D ˆ Ê eVd ˆ DJ0 = J0  J00 = J m exp Á  b ˜ exp Á Ë kBT0 ¯ Ë 2kBT0 ˜¯ È e2 (dV b )2 + 8( D  eV / 2)k dT ˘ b d B ˙ ¥Í 2 ˙ Í 8(kBT0 ) Î ˚ at eVd > kBT0 and
(15.8)
Ê D ˆ Ê eVd ˆ DJ0 = J0  J00 = J m exp Á  b ˜ Á Ë kBT0 ¯ Ë 2kBT0 ¯˜ È e2 (dV b )2 + 8( D  eV ˘ b e d / 2)kB dT ˙ ¥Í Í ˙ 8(kBT0 )2 Î ˚
at eVd kBT0. Here,
˘ Ê eVd ˆ Ê D ˆÈ J00 = J m exp Á  b ˜ Íexp Á  1˙ ˜ Ë kBT0 ¯ ÎÍ Ë 2kBT0 ¯ ˙˚
(15.9) (15.10)
is the dc sourcedrain current without THz irradiation (dark current).
15.3 Plasma Resonances
Solving Eq. (15.4) with boundary conditions (15.2) and (15.3) and taking into account Eq. (15.7), we obtain dV b =
Vw 2
¸Ô eiwt e iwt ÔÏ + Ì ˝. ÔÓ cos ÈÎqw ( L  l )˘˚ cos ÈÎqw ( L  l)˘˚ ˛Ô
(15.11)
Resonant Electron Heating
Here
q±w =
mæw (w iv ) 4pe2 S 0W
(15.12)
.
Equation (15.11) yields (dV b )2 =
Vw2 2
where
È 2 Ê pw ˆ Ê pv ˆ ˘ + sinh2 Á Ícos ËÁ ˜ Ë 4W ˜¯ ˙˚ 2W ¯ Î
W=
p 3e2 S 0W
1
,
(15.13) (15.14)
æ m( L  l )2
is the characteristic plasma frequency. Due to the dependence (given by Eq. (15.1)) of the dc electron density on the gate voltage Vg, the characteristic plasma frequency W can be tuned by this voltage. Because of the dependence of W on the length, L – l, of the quasineutral sections of the getated 2DEG channel (serving as the resonant plasma cavities) and, hence, on the potential of the central gate Vcg, W is somewhat varied with varying Vcg.
15.4 Resonant Electron Heating
The power absorbed by the channel can be calculated using the following equation: d Pw =
2e2 S 0v
m(w 2 + v2 )
Ú
l
L
2
dx
∂dj . ∂x
(15.15)
Considering Eq. (15.15), the energy balance equation governing the averaged electron temperature can be presented as 2
Ê dV b ˆ kB d T e 2v = Á ˜ K, te m(v2 + w 2 ) Ë L  l ¯
(15.16)
where te is the electron energy relaxation time. The factor K is associated with the nonuniformity of the ac electric field under the side gates. This factor is given by
277
278
Plasma Mechanisms of Resonant Terahertz Detection
2
Ê p ˆ w w 2 + v2 K =Á ˜ Ë 8¯ W2 ÈÊ 2W ˆ Ê pw ˆ ˘ Ê pv ˆ Ê W ˆ sinh Á sin Á . Á ÍÁË ˜ ˜ ˜ Ë W ˜¯ ˙˚ Ë 2W ¯ Ë pw ¯ Î pv ¯
(15.17)
At v w, W, Eq. (15.17) yields 2
2
Êpˆ Êwˆ È Ê W ˆ Ê pw ˆ ˘ K = Á ˜ Á ˜ Í1  Á sin Á , Ë 8 ¯ Ë W ¯ Î Ë pw ˜¯ Ë W ˜¯ ˙˚
(15.18)
so that one can use the following simplified formula: 2
2 Ê p ˆ e vt e kB d T Á ˜ (dV b )2 . Ë 8 ¯ mL2W2
(15.19)
15.5 Rectified Current and Detector Responsivity Using Eqs. (15.8) and (15.15), we obtain
Ê V  2D b ˆ (1 + H )e2 (dV b )2 , DJ0 = Jm exp Á d ˜◊ Ë 2kBT0 ¯ 8(kBT0 )2
where the term
H=
4(2D b  eVd )vt e m(v2 + w 2 )( L  l )2
(15.20)
K
(15.21)
is associated with the contribution of the electron heating to the rectified current. Combining Eqs. (15.13) and (15.20), we arrive at Ê V  2D b ˆ exp Á d (1 + H) Ë 2kBT0 ¯˜
2
Ê eVw ˆ DJ0 = Jm ◊ Á ˜ . È Ê pw ˆ 2 Ê pv ˆ ˘ Ë 2kBT0 ¯ + sinh 4 Ícos2 Á ÁË 4W ˜¯ ˙ Ë 2W ˜¯ Î ˚
(15.22)
Since Vw2 is proportional to the incoming THz power, the detector responsivity as a function of the signal frequency and the structural
Comparison of Dynamic and Heating Mechanisms
parameters (except the antenna parameters) can be in the following form: Rµ
Ê V  2D b ˆ exp Á d Ë 2kBT0 ˜¯
È 2 Ê pw ˆ 2 Ê pv ˆ ˘ Ícos ËÁ 2W ¯˜ + sinh ÁË 4W ¯˜ ˙ Î ˚
(1 + H ) kBT0
.
(15.23)
As follows from Eq. (15.23), the responsivity as a function of the frequency of incoming THz radiation exhibits sharp peaks at the plasma resonant frequencies w = W(2n – 1), where n = 1, 2, 3, . . . is the resonance index, provided that the quality factor of resonances W/v 1.
15.6 Comparison of Dynamic and Heating Mechanisms
As seen from Eq. (15.22), the ratio of the heating and dynamic components of the rectified dc sourcedrain current is given by the quantity H (heating parameter). At v w, W, considering Eqs. (15.18) and (15.19), the quantity H can be estimated as D bvt e p 2 (2D b  eVb )vt e p 2 H = � . 2 2 8 mW2 (L  l )2 16 mW (L  l)
(15.24)
Considering that W = ps/2(L – l), Eq. (15.24) can be presented in the following form: H
Ê D ˆ 1 Ê 2D b  eVd ˆ vt e Á b 2 ˜ vt e . Á ˜ 2 ¯ Ë 2ms ¯ 4 Ë ms
(15.25)
The first factor in Eq. (15.25) is usually small, while the second one can be large, so that H can markedly exceed unity, particularly, at low temperatures. In line with the above assumptions, Eqs. (15.24) and (15.25) are valid at moderate drain voltages when Db−eVd/2 is positive and, moreover, not too small in comparison with Δb. It is natural to assume that in a wide range of the temperature (from liquid helium to room temperatures), the electron collision frequency (the inverse momentum relaxation time) is determined by the electron interaction with acoustic phonons and charged impurities, while the electron energy relaxation is due to the
279
280
Plasma Mechanisms of Resonant Terahertz Detection
interaction with both acoustic and polar optical phonons. Hence, v = v(ac) + v(i) and t e = t e(ac )t e(op) /[t e(ac ) + t e(op) ], where v(ac) and v(i) are related to the electron scattering on acoustic phonons and impurities (charged), respectively, whereas t e(ac ) and t e(op) are the electron energy relaxation times associated with the acoustic and optical phonons. As a result, the product vtε can be presented as Èv(ac ) + v( i ) ˘ t e(ac )t e(op) ˚ (15.26) . vt e = Î Èt e(ac ) + t e(op) ˘ Î ˚ We shall use the following formulas for the temperature dependences of the parameters in this equation: v
1 t e(ac )
( ac )
=
1 Êk T ˆ = (ac ) Á B 0 ˜ t PA Ë w 0 ¯
2msa2 w 0 1
t e(op)
1/ 2
1 Êk T ˆ + (ac ) Á B 0 ˜ t DA Ë w 0 ¯
3/2
,
1/2 1/ 2 È Ê kBT0 ˆ 1 Ê kBT0 ˆ ˘˙ Í 1 , + ( ac ) Á w ˜ ( ac ) Á w ˜ Í t PA ˙ Ë Ë t DA 0¯ 0¯ ˚ Î 2
Ê w 0 ˆ 1 2 Ê w 0 ˆ = (op) Á exp Á ˜ ˜, 3 Ë kBT0 ¯ Ë kBT0 ¯ t
(15.27)
(15.28) (15.29)
( ac ) ( ac ) where t PA = 8 ps, t DA = 4 ps, and t (op) = 0.14 ps (Ref. [26]) are the characteristic scattering times for the acoustic phonon scattering (polar and deformation mechanisms, respectively) and for the optical phonon scattering, and ℏw0 is the optical phonon energy. The temperature dependence of the collision frequency of 2D electrons with charged impurities is assumed to be as follows:
Ê w 0 ˆ v( i ) = v ( i ) Á ˜ ◊ S ( zi , kBT0 / w 0 ). Ë kBT0 ¯
Here the function [27]
S ( zi , x) =
Ú
1
0
exp(a  zi  x x )
(15.30)
dx 1  x2
characterizes a decrease in the collision frequency with increasing thickness of the spacer, zi, between the 2DEG channel and the charged donor sheet, and a = 4 2mw 0 / ≃ 107 cm–1. The
Comparison of Dynamic and Heating Mechanisms
characteristic frequency vi is proportional to the donor sheet density. We set v ( i ) = (108 – 109) s–1. At T0 = 4.2 K, these values correspond to v(i) = 1010 – 1011 s–1 and the electron mobilities m ≃ (105 – 106) cm2/V s. When zi= 0, Eq. (15.30) yields vi µ T01 , while at sufficiently thick spacers, one obtains vi µ T03/2 . In the case of relatively thick electron channels, in which the quantization is insignificant, vi µ T03/2 . Figure 15.2 shows the temperature dependence of the “heating” parameter H, which determines the relative contribution of the heating mechanism to the detector responsivity, calculated for different values of parameter v ( i ) , i.e., different doping levels. It is assumed that for a GaAs channel ℏw0/kB = 421 K [26]. We set s = 1 ¥ 108 cm/s, sa = 5 ¥ 105 cm/s, the barrier height Db = 110 meV, and the bias voltage Vd = 20 mV, so that the effective barrier height ) = Db – eVb/2 = 100 meV. As seen from Fig. 15.2, the heating D(eff b mechanism can provide significantly larger contribution to the detector responsivity at low temperatures (T0 ≲ 35–40 K). However at elevated temperatures, this mechanism becomes relatively inefficient. This is attributed to weak electron heating due to strong energy relaxation on optical phonons at elevated temperature. 30
zi = 3 nm
25
ν
(i)
9 1
= 10 s 8 1 = 10 s
11
10
15
10
1
,s (ac)
9
10
�
10
zi = 3, 5, 10 nm
10
ν
(i)
ν ,s
1
H
�
20
5 0 0
8
10 0
20
40
20
60
40
60
Temperature, K
80 100
80
100
Figure 15.2 Temperature dependences of heating parameter H. The inset shows the temperature dependences of the electron collision frequencies associated with impurity and acoustic scattering mechanism.
281
Plasma Mechanisms of Resonant Terahertz Detection
15.7 Temperature Dependences of the Detector Responsivity and Detectivity As mentioned in Section 15.5, the detector resonsivity exhibits sharp peaks at the plasma resonant frequencies w = W(2n – 1). The sharpness of these peaks depends on the electron collision frequency v, which in turn depends on the temperature. As follow from Eq. (15.23), the maximum values of the detector responsivity at the fundamental resonance (n = 1) are given by Ê V  2D b ˆ exp Á d Ë 2kBT0 ˜¯ (1 + H ) max R µ . kBT0 2 Ê pv ˆ sinh Á Ë 4W ˜¯
(15.31)
As a result, for the value of the ratio of the detector responsivity at the resonance and the dark current one obtains
10
10
1 1+ H . Ê p v ˆ (kBT )2 sinh2 Á Ë 4W ˜¯ max R/J00, a.u.
max R µ J00
max R/J00, a.u.
282
4
2
1
2
10 0
ν
(i)
9 1
= 10 s 8 1 = 10 s
20
10
4 2
10 1
2
10 0 20 40 60 80 100
Dynamic
Heating
40
(15.32)
60
Temperature, K
80
100
Figure 15.3 Temperature dependences of dynamic and heating contributions to max R/J00, of the detector responsivity maximum (resonant) value and the dark current. The inset shows the net value max R/J00 as a function of temperature.
Temperature Dependences of the Detector Responsivity and Detectivity
Figure 15.3 shows the temperature dependences of the maximum (resonant) values of the dynamic and heating contributions to the detector responsivity devided by the dark current value calculated using Eq. (15.32) for the barrier height D(eff) = 100 meV, the b fundamental plasma frequencies W/2p = 1 THz, and different values of the parameter v ( i ) . The inset shows the temperature dependence of max R/J00, which accounts for both mechanisms. Taking into account that the detector detectivity D* µ R / J00 , we arrive at the following formula: Ê V  2D b ˆ exp Á d Ë 4kBT0 ˜¯ (1 + H ) . max D* µ 5/ 4 È 2 Ê pv ˆ ˘ ( kBT0 ) Ísinh ÁË 4W ˜¯ ˙ Î ˚
(15.33)
Figure 15.4 shows the temperature dependences of the detector detectivity calculated for different values of the effective barrier ) height D(eff = D b  eVd / 2. b
Dectectivity, a.u.
10
10
8
(eff)
Δb
6
= 10 meV (eff)
Δb
= 50 meV (eff)
Δb 10
4
10
2
1
0
50
100
150
200
Temperature, K
= 100 meV
250
300
Figure 15.4 Temperature dependences of the detector responsivity D* for (eff ) different values of the effective barrier height Db .
As follows from the above formulas, the detector responsivity and detectivity increase with decreasing effective barrier height. However, this quantity cannot be set too small (at a given temperature
283
284
Plasma Mechanisms of Resonant Terahertz Detection
T0) in the frame of our model, which is valid if D(beff ) kBT0, and when the 2DEG channel can be partitioned into the quasineutral and deleted sections.
15.8 Discussion
The displacement current across the depleted region can be, in principle, essential. To take this current into consideration, one needs to modify Eq. (15.3) [28]. Introducing the admittance, Yw, of the barrier region, we can use the following boundary conditions at the edge of the quasineutral sections of the 2DEG channel (for the asymmetrical plasma modes for which djw x =1 = djw x =l ): s w
djw dx
x =± l
= 2Yw djw
x =± l
(15.34)
.
Here, s w = i[e2 S 0 / m(w + iv )] is the ac conductivity of the quasineutral sections of the channel accounting for the electron collisions and inertia. Since the real part of the conductivity of the depleted (barrier) region is definitely small in comparison with the conductivity of the quasineutral sections, one can take into account only the capacitive component of the current across the depleted region. In this case, Yw = –iwC, where C is the pertinent capacitance, which is determined by the capacitances Ccg and Cdr: C = Cdr + Cgs/2 (see the equivalent circuit in Fig. 15.1). This equivalent circuit accounts for the inductance of the quasineutral sections Lc, due to the inertia of the electron transport along the channel, the channel resistance due to the electron scattering, the resistance of the barrier region Rdr, and different capacitances. Equation (15.34) can be presented in the form: W2 (L  l) ddjw w (w + iv) dx
where
c=
= cdjw
x =± l
2p 2CW 2p 2CW . æ(L  l) æL
x =± l
,
(15.35)
(15.36)
Conclusions
If the parameter c 1, Eqs. (15.3) and (15.35) practically coincide (except the case w W). According to Ref. [28], Cdr = (æ/2p2)Ldr and Ccg = (æ/2p2)Lcg, where Ldr and Ldr are logarithmic factors which are determined by the geometry of the planar conducting areas (the gates and quasineutral sections of the channel). These factors can be estimated as [28] Ldr ~ Lcg ~ ln(2L/l). Hence, c ≃ (W/L)L, where L = Ldr + Lcg/2. The factor L somewhat exceeds unity, although it is not too large. Thus, taking into account that W L, one can conclude that for real device structures, c 1. The condition of the smallness of c can be also presented in the form Cg C, where Cg = æ4p W ≃ L/W is the capacitance of the side gates (see Fig. 15.1). Relatively small capacitances Cdr and Ccg can, to some extent, affect the plasma oscillations. However, their role reduces mainly to a small modification in the resonant plasma frequencies [28]. If c would be large, the ac potential near the edges of the quasineutral regions is small as well as the ac potential drop across the depleted region. This implies that the boundary condition (15.34) could be djw x =±l 0. In such a case, the fundamental plasma frequency is doubled and dynamic mechanism is weakened. However, the details of the ac potential distribution near the edges of the quasineutral regions are not crucial for the heating mechanism. Actually, there is some delay in the electron transit across the barrier. The delay time can be estimated as tb ≃ 2l/uT, where uT kBT0 / m is the thermal electron velocity. The delay in the electron transit and, therefore, the electron transit time effects can be disregarded if wtb ~ Wtb < 1 [29]. Assuming W/2p = 1 THz and uT = 107 cm/s, from the last inequality we obtain 2l < 0.6 mm.
15.9 Conclusions
We developed a device model for a resonant detector of THz radiation based on the gated 2DEG channel with an electrically induced barrier. The model accounts for the resonant excitation of the plasma oscillations in the gated 2DEG channel as well as the rectified dc current through the barrier. As shown, this current comprises two components: the dynamic component associated with the ac potential drop across the barrier and the heating (bolometric) component due to a change in the electron temperature, which stems
285
286
Plasma Mechanisms of Resonant Terahertz Detection
from the resonant plasmaassisted absorption of THz radiation. Using our model, we calculated the frequency and temperature dependences of the detector responsivity. The detector responsivity exhibits sharp resonant peaks at the frequencies of incoming THz radiation corresponding to the plasma resonances in the gated 2DEG channel. The plasma resonances can tuned by the gate voltage Vcg and, to some extent, by the potential of the central gate Vcg. It is demonstrated that the dynamic mechanism dominates at elevated temperatures, whereas at low lattice temperatures (T0 ≲ 35–40 K for AlGaAs/GaAsbased detectors), the heating mechanism prevails. This can be attributed to a marked increase in the electron energy relaxation time te with decreasing lattice temperature. ) At rather low temperatures when the ratio D(eff / kBT0 is large, b the thermionic electron current over the barrier can be surpassed by the tunneling current. The rectified portion of this current can be associated with both dynamic and heating mechanisms (the thermoassisted tunneling current in the case of the latter mechanism). This, however, requires a separate detailed study. In the case of detection of THz radiation modulated at some frequency wm w, the relative contributions of the dynamic and heating mechanisms to the responsivity, Rm, characterizing the detector response at the frequency wm can be different than those considered above. This is due to different inertia of these mechanisms. In particular, if w m > t e1 (but w m w ), the variation of the electron effective temperature averaged over the THz oscillations dTm dT / w mt e , i.e., dTm dT . As a result, Rm/R ≃ (wmte)–1. This implies that even at low temperatures, the heating mechanism can be inefficient if w m > t e1 . Both dynamic and heating mechanisms might be responsible for the THz detection in the plasmonic resonant detectors utilizing another barrier structure (for instance, with the lateral Schottky barrier [19, 20] or with electron transport through the gate barrier [30–32]) and another types of the plasma resonant cavity (with ungated quasineutral regions as in highelectron mobility transistors with relatively long ungated sourcegate and gatedrain regions), as well as in those with other methods of the excitation of plasma oscillations (utilizing periodic gate structures [14]).
References
Acknowledgments This work was supported by the GrantinAid for Scientific Research (S) from the Japan Society for Promotion of Science, Japan. The work at RPI was partially supported by the Office of Naval Research, USA.
References
1. S. J. Allen, Jr., D. C. Tsui, and R. A. Logan, Phys. Rev. Lett., 38, 980 (1977).
2. D. C. Tsui, E. Gornik, and R. A. Logan, Solid State Commun., 35, 875 (1980).
3. W. Knap, Y. Deng, S. Rumyantsev, J.Q. Lu, M. S. Shur, C. A. Saylor, and L. C. Brunel, Appl. Phys. Lett., 80, 3433 (2002). 4. W. Knap, Y. Deng, S. Rumyantsev, and M. S. Shur, Appl. Phys. Lett., 81, 4637 (2002).
5. X. G. Peralta, S. J. Allen, M. C. Wanke, N. E. Harff, J. A. Simmons, M. P. Lilly, J. L. Reno, P. J. Burke, and J. P. Eisenstein, Appl. Phys. Lett., 81, 1627 (2002).
6. W. Knap, J. Lusakowski, T. Parently, S. Bollaert, A. Cappy, V. V. Popov, and M. S. Shur, Appl. Phys. Lett., 84, 2331 (2004). 7. J. Lusakowski, W. Knap, N. Dyakonova, L. Varani, J. Mateos, T. Gonzales, Y. Roelens, S. Bullaert, A. Cappy, and K. Karpierz, J. Appl. Phys., 97, 064307 (2005).
8. T. Otsuji, M. Hanabe, and O. Ogawara, Appl. Phys. Lett., 85, 2119 (2004). 9. F. Teppe, D. Veksler, V. Yu. Kacharovskii, A. P. Dmitriev, X. Xie, X.C. Zhang, S. Rumyantsev, W. Knap, and M. S. Shur, Appl. Phys. Lett., 87, 022102 (2005).
10. F. Teppe, W. Knap, D. Veksler, M. S. Shur, A. P. Dmitriev, V. Yu. Kacharovskii, and S. Rumyantsev, Appl. Phys. Lett., 87, 052105 (2005). 11. M. Hanabe, T. Otsuji, T. Ishibashi, T. Uno, and V. Ryzhii, Jpn. J. Appl. Phys., Part 1, 44, 3842 (2005).
12. M. Lee, M. C. Wanke, and J. L. Reno, Appl. Phys. Lett., 86, 033501 (2005). 13. E. A. Shaner, M. Lee, M. C. Wanke, A. D. Grine, J. L. Reno, and S. J. Allen, Appl. Phys. Lett., 87, 193507 (2005). 14. E. A. Shaner, A. D. Grine, M. C. Wanke, M. Lee, J. L. Reno, and S. J. Allen, IEEE Photonics Technol. Lett., 18, 1925 (2006).
15. D. Veksler, F. Teppe, A. P. Dmitriev, V. Yu. Kacharovskii, W. Knap, and M. S. Shur, Phys. Rev. B, 73, 125328 (2006).
287
288
Plasma Mechanisms of Resonant Terahertz Detection
16. A. El Fatimy, F. Teppe, N. Dyakonova, W. Knap, D. Seliuta, G. Valusis, A. Shcherepetov, Y. Roelens, S. Bollaert, A. Cappy, and S. Rumyantsev, Appl. Phys. Lett., 89, 131926 (2006).
17. J. Torres, P. Nouvel, A. AkwaoueOndo, L. Chusseau, F. Teppe, A. Shcherepetov, and S. Bollaert, Appl. Phys. Lett., 89, 201101 (2006).
18. M. Dyakonov and M. Shur, IEEE Trans. Electron Devices, 43, 1640 (1996).
19. V. Ryzhii and M. S. Shur, Jpn. J. Appl. Phys., Part 2, 45, L1118 (2006).
20. A. Satou, N. Vagidov, and V. Ryzhii, IEICE Techn. Rep., ED2006197, p. 77 (2006).
21. A. Satou, V. Ryzhii, I. Khmyrova, M. Ryzhii, and M. S. Shur, J. Appl. Phys., 95, 2084 (2004).
22. V. Ryzhii, A. Satou, W. Knap, and M. S. Shur, J. Appl. Phys., 99 (2006) 084507. 23. S. Rudin and T. L. Reinecke, Phys. Rev. B, 54, 2791 (1996).
24. F. J. Crowne, J. Appl. Phys., 82, 1242 (1997).
25. S. Rudin and G. Samsonidze, Phys. Rev. B, 58, 16369 (1998).
26. V. F. Gantmakher and Y. B. Levinson, Carrier Scattering in Metals and Semoconductors (NorthHolland, Amsterdam, 1987). 27. A. Shik, Quantum Wells (World Scientific, Singapore, 1997).
28. V. Ryzhii, A. Satou, I. Khmyrova, M. Ryzhii, T. Otsuji, V. Mitin, and M. S. Shur, J. Phys.: Conf. Ser., 38, 228 (2006). 29. V. Ryzhii and M. S. Shur, Phys. Status Solidi A, 202, R113 (2005).
30. V. Ryzhii, I. Khmyrova, and M. Shur, J. Appl. Phys., 88, 2868 (2000).
31. I. Khmyrova and V. Ryzhii, Jpn. J. Appl. Phys., Part 1, 39, 4727 (2000).
32. A. Satou, V. Ryzhii, I. Khmyrova, and M. S. Shur, Semicond. Sci. Technol., 18, 460 (2003).
Chapter 16
Terahertz and Infrared Photodetection Using pin MultipleGrapheneLayer Structures*
V. Ryzhii,a,b M. Ryzhii,a,b V. Mitin,c and T. Otsujib,d aComputational
Nanoelectronics Laboratory, University of Aizu, AizuWakamatsu 9658580, Japan bJapan Science and Technology Agency, CREST, Tokyo 1070075, Japan cDepartment of Electrical Engineering, University at Buffalo, State University of New York, New York 14260, USA dResearch Institute for Electrical Communication, Tohoku University, Sendai 9808577, apan [email protected]
We propose to utilize multiplegraphenelayer structures with lateral pin junctions for terahertz and infrared (IR) photodetection and substantiate the operation of photodetectors based on these structures. Using the developed device model, we calculate the *Reprinted with permission from V. Ryzhii, M. Ryzhii, V. Mitin, and T. Otsuji (2010). Terahertz and infrared photodetection using pin multiplegraphenelayer structures, J. Appl. Phys., 107, 054512. Copyright © 2010 American Institute of Physics. GrapheneBased Terahertz Electronics and Plasmonics: Detector and Emitter Concepts Edited by Vladimir Mitin, Taiichi Otsuji, and Victor Ryzhii
Copyright © 2021 Jenny Stanford Publishing Pte. Ltd.
ISBN 9789814800754 (Hardcover), 9780429328398 (eBook)
www.jennystanford.com
290
Terahertz and Infrared Photodetection
detector dc responsivity and detectivity as functions of the number of graphene layers and geometrical parameters and show that the dc responsivity and detectivity can be fairly large, particularly, at the lower end of the terahertz range at room temperatures. Due to relatively high quantum efficiency and low thermogeneration rate, the photodetectors under consideration can substantially surpass other terahertz and IR detectors. Calculations of the detector responsivity as a function of modulation frequency of THz and IR radiation demonstrate that the proposed photodetectors are very fast and can operate at the modulation frequency of several tens of gigahertz.
16.1 Introduction
Unique properties of graphene layers (GLs) [1–3] make them promising for different nanoelectronic device applications. The gapless energy spectrum of GLs, which is an obstacle for creating transistorbased digital circuits, opens up prospects to use GLs in terahertz and infrared (IR) devices. Novel optoelectronic terahertz and IR devices were proposed and evaluated, in particular, in Refs. [4–11]. Recent success in fabricating multipleGL structures with long momentum relaxation time of electrons and holes [12] promises a significant enhancement of the performance of future graphene optoelectronic devices [13]. In this chapter, we study the operation of terahertz and IR photodetectors based on multipleGL structures with reverse biased pin junctions. We refer to the photodetectors in question as to GLphotodetectors (GLPDs). We focus on GLPDs (a) with p and ndoped sections in GLs near the side contacts [14, 15], p+ and n+ contacts (for example, made of doped polySi) [16], and multiple GLstructures with the Ohmic side contacts and (b) with split gates which provide the formation of the electrically induced p and nsections [17– 22]. These gates are separated from a multipleGL structure by a insulating layer (gate layer) made of, for instance, SiO2 or HfO2. Its thickness Wg should be chosen (sufficiently small) to provide an effective formation of the electron and hole regions under the gates in sufficiently large number of GLs under the applied gate voltages. The device structures under considerations are shown in Figs. 16.1a
Introduction
and b. It is assumed that the highly conducting GL(s) between the SiC substrate and the top GLs is removed. Multiple GLstructures without this highly conducting GL can be fabricated using chemical/ mechanical reactions and transferred substrate techniques (chemically etching the substrate and the highly conducting bottom GL (Ref. [23]) or mechanically peeling the upper GLs, then transferring the upper portion of the multipleGL structure on a Si substrate). The operation of GLPDs is associated with the interband photogeneration of the electrons and holes in the isections of GLs by incoming THz or IR radiation. The photogenerated electrons and holes propagate under the electric field created by the bias voltage (which provides the pin junction reverse bias) in the directions toward the nsection and psection, respectively. This results in the dc or ac photocurrent induced in the circuit. The GLPD operation principle is actually similar to that in the standard pin photodiodes based on bulk semiconductor materials.
Figure 16.1 Device structures of GLPDs with (a) doped and (b) electrically induced pin junctions.
Using the developed device model, we calculate the GLPD responsivity and detectivity as terahertz or IR photodetector (Sections 16.2 and 16.3), evaluate its dynamic response (Section 16.4), and compare GLPDs with some other terahertz and IR photodetectors (Section 16.5), in particular, with quantumwell
291
292
Terahertz and Infrared Photodetection
IR photodetectors (QWIPs) and quantumdot IR photodetectors (QDIPs). In Section 16.6, we discuss possible role of the Pauli blocking in the spectral characteristics of GLPDs and draw main conclusions. The calculations related to the effect of screening of the vertical electric field on the formation of the electrically induced p and nsections in multipleGL structures are singled out in the Appendix.
16.2 Responsivity and Detectivity
We assume that the intensity of the incident terahertz or IR radiation with the frequency W apart from the dc component I0 includes the ac component: I(t) = I0 + dIw exp(–iw)t, where dIw and w are the amplitude of the latter component and its modulation frequency, respectively. In such a situation, the net dc current (per unit width of the device in the direction perpendicular to the current) can be presented in the following form: with and
J0 = J0dark + J0photo ,
(16.1)
J0dark = 4Kel( gth + gtunn )
(16.2)
K
J0photo = 4el
bW I0( k ) . W k =1
Â
(16.3)
Here e is the electron charge, K is the number of GLs, 2l is the 2/3 3/2 length of the GL isection, gth and gtunn = (eV / 2lu W ) / 8p 2 are the rates of thermal and tunneling generation of the electronhole pairs (per unit area) [22], V is the reverse bias voltage, uW ≃ 108 cm/s is the characteristic velocity of electrons and holes in graphene (see, for instance, Ref. [3]), bW = b[1  2 f (W / 2)] is the absorption coefficient of radiation in a GL due to the interband transitions [24], where bW = (p e2 / c� ) � 0.023, f(e) is the distribution function of electrons and holes in the isection, ℏ is the Planck constant, and c is the speed of light. The term gtunn in Eq. (16.2) is associated with the interband tunneling in the electric field in the isection. The quantity I0( k ) = I0 (1  bW )K  k is the intensity of terahertz or IR radiation at the kth GL (1 £ k £ K).
Responsivity and Detectivity
At a sufficiently strong reverse bias, electrons and holes are effectively swept out from the isection to the contacts and heated. Due to this, one can assume that under the GLPD operation conditions, f(ℏW/2) 1, so that the distinction between bW and b can be disregarded (see below). Using Eqs. (16.1) and (16.3), we arrive at the following formula for the GLPD dc responsivity: R0 =
J0photo 2ebW =K* , W 2lI0
(16.4)
where K * = S Kk =1 (1  bW )K k = [1  (1  bW )K ]/ bW . Equation (16.4) can also be rewritten as R0 = [1  (1  bW )K ]
2e e 1 =h µ , W W W
(16.5)
where h = 2[1–(1–bW)k] is the GLPD quantum efficiency and the factor 2 appears because each photon absorbed due to the interband transition generates two carriers, an electron and a hole. As a result, h can exceed unity. However, h < 2 because there is no multiplication of the photoelectrons and photoholes propagating in the isection, so that the photoelectric gain G in the photodetectors under consideration is equal (or, at least, close) to unity. If K = 1, Eq. (16.5) at W/2p = 1 THz, yields, R0 ≃ 12 A/W. For K = 50–100 (K* ≃ 30–39), setting K = 50, in the frequency range W/2p = 1–10 THz, from Eq. (16.4) we obtain R0 ≃ 35–350 A/W. As follows from Eqs. (16.4) and (16.5), the GLPD responsivity is virtually independent of the temperature. This results from the temperatureindependent absorption coefficient and G ≃ 1. The darkcurrent limited detectivity, D*, defined as D* = = ( J photo / NP ) A ◊ Df , where N is the noise (in Amperes), P is the power received by the photodetector (in watts), A is the area of the photodetector (in cm2) (see, for instance, Refs. [25, 26]), and Df is the bandwidth, can be expressed via the responsivity R0 and the dark current J0dark H , where H is the device width in the direction perpendicular to the current, and be presented as D* = R0
A
4eJ0dark H
Using Eqs. (16.2)–(16.6), we arrive at
.
(16.6)
293
Terahertz and Infrared Photodetection
D* = =
K * bW 1 K W 2( gth + gtunn ) [1  (1  bW )K ]
1 2( gth + gtunn )
K W
µ
1 . W
(16.7)
Assuming that K = 1 and gth = 1021 cm–2 s–1 [27], at T = 300 K for W/2p = 1–2 THz we obtain D* ≃ (4.1–8.2) ¥ 108 cm Hz1/2/W. Setting K = 50, we arrive at D* ≃ (1.7–3.4) ¥ 109 cm Hz1/2/W. Due to a significant decrease in the thermogeneration rate at lower temperatures, the detectivity markedly increases with decreasing temperature. Indeed, at T = 77 K, setting gth = 1013 cm–2 s–1 [27], we obtain D* ≃ (1.7–3.4) ¥ 1013 cm Hz1/2/W. 2.0
300
T = 300 K
250
1.5
9
200
1.0
150 100
0.5 0 0
Responsivity, R0 (A/W)
1/2
Detectivity, D* (x10 cm·Hz /W)
294
Ω/2π = 2 THz 3 THz 20
40 80 60 Number of GLs , K
50 0 100
Figure 16.2 Responsivity R0 and detectivity D* vs. number of GLs K for W/2p = 2 and 3 THz.
Figure 16.2 shows the dependences of the dc responsivity and detectivity on the number of GLs K calculated for W/2p = 2 and 3 THz using Eqs. (16.5) and (16.7) for GLPDs with sufficiently large l in which the tunneling is weak (see below). Equation (16.7) shows that the GLPD detectivity decreases with increasing photon frequency. This is because the spectral dependence of the GLPD detectivity is determined by that of the responsivity. As follows from Eqs. (16.6) and (16.7), the detectivity drops at elevated bias voltages when the interband tunneling prevails over the thermogeneration of the electron and hole pairs. According to Eqs. (16.4) and (16.7), the GLPD responsivity is independent of the length of the isection 2l and the bias voltage V (at least if the latter is not too small), whereas the detectivity increases with increasing l and decreases with V. This
Responsivity and Detectivity
is because the component of the dark current associated with the thermogeneration rate increases linearly with increasing l. At the same time, the tunneling component is proportional to V 3/2/ l . As a result, from Eq. (16.7) one can arrive at D* µ
1
1 + b(V / l)3/2
(16.8)
,
where b µ 1/gth. Thus, at elevated bias voltages when the tunneling generation surpassed the thermal generation, D* µ V–3/4. * Figure 16.3 shows the voltagedependence of the detectivity Dtunn with the interband tunneling normalized by the detectivity D* without tunneling calculated for different values of the isection length 2l.
1.0
T = 300 K
D*tunn/D*
0.8 0.6
l = 10 µm
0.4 0.2 0 0
l = 0.1 µm
l = 1 µm
1.0 0.5 1.5 Bias voltage, V (V)
2.0
Figure 16.3 Normalized detectivity vs. reverse bias voltage for GLDPs with different length of the isection 2l.
Since the value of D* is determined by both l and V, the latter values should be properly chosen. There is also a limitation associated with the necessity to satisfy the condition 2l ≲ lR, where lR is the recombination length. Otherwise, the recombination in the isection can become essential resulting in degrading of the GLPD performance. The recombination length can be defined as lR = LV, where Lv u t R , tr is the recombination time, and u is the average drift velocity in the iregion. Assuming that for the electron and hole densities close to that in the intrinsic graphene at T = 300
295
296
Terahertz and Infrared Photodetection
K, one can put tr = 5 ¥ 10–10 s. Setting for sufficiently large bias u = 5 ¥ 107 cm/s [28], one can find LV ≃ 250 mm.
16.3 Features of GLPD with Electrically Induced Junction
The main distinctions of the detectors with doped and electrically induced pin junction are that the Fermi energies of electrons and holes in the latter depend on the gate voltages Vp < 0 in the psection and Vn > 0 in the nsection [see Fig. 16.1b] and that these energies and, hence, the heights of the barriers confining electrons and holes in the pertinent section are different in different GLs. This is due to the screening of the transverse electric field created by the gate voltages by the GL charges. This screening results in a marked decrease in the barrier heights of the GLs located in the MGLstructure depth (with large indices k) in comparison with the GLs near the top. In the following, we set Vn = –Vp = Vg. The barriers in question effectively prevent the electron and hole injection from the contacts under the reverse bias if the barrier heights are sufficiently large. However, the electron and hole injection into the GLs with large k leads to a significant increase in the dark current (in addition to the current of the electrons and hole generated in the isection). This can substantially deteriorate the GLPD detectivity. As for the responsivity, it can still be calculated using Eq. (16.4) or Eq. (16.5). To preserve sufficiently high detectivity, the number of GLs should not be too large. Indeed, taking into account the contributions of the current injected from the p and nregions to the net dark current, the detectivity of a GLPD with the electrically induced pin junction can be presented as K * bW D* = � , W 2[ S Kk =1 ji( k ) / el + K ( gth + gtunn )]
(16.9)
where ji( k ) µ exp( e F( k ) / kBT ) is the electron current injected from the pregion and the hole current injected from the nregion, and e F( k ) is the Fermi energy of holes (electrons) in the pregion (nregion) of the kth GL (1 £ k £ K). The injected currents are small in comparison with the current of the electrons and holes thermogenerated in the iregion if
Dynamical Response
Ê e (k ) ˆ uw S0 exp Á  F ˜ < 2lg th . p Ë kBT ¯
(16.10)
Here S0 is the electron and hole density in the intrinsic graphene (at given temperature). Considering Eqs. (16.A5) and (16.A6) from the Appendix, the latter imposes the following limitation on the number of GLs in GLDs with the electrically induced pin junctions and the gate voltage Vg: K < K max =
e FT 1 µVg1/12 . g kBT ln(u W S 0 /2plg th )
(16.11)
The quantity g is defined in the Appendix. For g = 0.12, assuming that the Fermi energy in the topmost GL e F(1) = e FT = 100 meV , T = 300 K, S0 ≃ 8 ¥ 1010 cm–2, l =10 mm, and gth ≃ 1021 cm–2 s–1, we obtain Kmax ≃ 34, i.e., fairly large. A decrease in l results in smaller Kmax due to a substantial increase in the tunneling current. For instance, if l = 0.1 mm [11], we obtain Kmax ≃ 7. Thus, by applying gate voltages one can form the p and nsections with sufficiently high densities and large Fermi energies of holes and electrons in GLstructures with a large number of GLs.
16.4 Dynamical Response
To describe the dynamic response to the signals modulated with the frequency w W, one needs to find the ac components of the net density of photogenerated electron and holes, dSw and dSw+ , respectively. These components are governed by the following equation: iwdSw� ± u
K
ddSw� bWd Iwk = . �W dx k =1
Â
As in above, d Iw( k ) = d Iw (1  b )K k , so that
(16.12)
K
bWd Iw( k ) b dI = K* W w . W W k =1
Â
In the case of ballistic transport of electrons and holes across the isection, u u W . If the electron and hole transport is substantially affected by quasielastic scattering, so that the momentum
297
298
Terahertz and Infrared Photodetection
distributions of electrons and holes are virtually semiisotropic, one can put u u W / 2 (see also Ref. [28]). Solving Eq. (16.12) with the = 0, we obtain boundary conditions dSw x =±l
dSw� = K *
bW exp[iw(l ± x)/ u ] 1 d Iw . ◊ �W iw
(16.13)
Using Eq. (16.13) and considering the Ramo–Shockley theorem [28, 29] applied to the case of specific contact geometry [30] the ac current induced in the side contacts (terminal current) can be presented as d Jwphoto elbW =K* d Iw pW
Ú
1
1
[eiwt t cos(wt t x)  1] . 2 iwt t 1x dx
(16.14)
Here we introduced the characteristic transit time t t = l / u . The feature of the contact geometry (the bladelike contacts) was accounted for by using the form factor g(x ) = 1 / p 1  x 2 [31]. This is valid because the thickness of the side contacts and multipleGL structure under consideration Kd l even at rather large numbers of GLs K, where d is the spacing between GLs. Similar approach was used previously to analyze the dynamic response of the lateral pn junction photodiodes made of the standard semiconductors [32] and the graphene tunneling transittime terahertz oscillator [22]. Integrating in Eq. (16.14), we arrive at the following: 4elbW È sin(wt t ) 0 (wt t ) d Jwphoto = K* Í W Î wt t d Iw +i
1  cos(wt t ) 0 (wtt t ) ˘ ˙, wt t ˚
where 0 (x ) is the Bessel function. Equation (16.15) yields d J wphoto d Iw
=K*
4elbW W
1  2cos(wt t ) 0 (wt t ) + 02 (wt t ) wt t
.
(16.15)
(16.16)
Using Eq. (16.16), for the frequency dependent responsivity Rw = d Jwphoto / 2ld Iw , we obtain Rw = K *
2 2eb 1  2cos(wt t ) 0 (wt t ) + 0 (wt t ) W wt t
Comparison with QWIPs and QDIPs
= R0
1  2cos(wt t ) 0 (wt t ) + 02 (wt t ) wt t
.
(16.17)
Figure 16.4 shows the responsivity Rw normalized by its dc value versus the modulation frequency w calculated using Eq. (16.17) for 7 different values of the transit time t t µ l. At u = vW / 2 5 ¥ 10 cm/s, the range tt = 10–30 ps corresponds to the length of the isection 2l = 10–30 mm. As seen from Fig. 16.4, Rw / R0 = 1 / 2 when the modulation cutoff frequency ft = wt/2p ≃ 8.3–24.39 GHz. Naturally, in GLPDs with shorter isections, ft can be markedly larger (although, at the expense of a substantial increase in the tunneling current). Due to this, GLPDs can be used as ultrafast terahertz and IR photodetectors (Fig. 16.4). 1.0
R ω/R 0
0.8 0.6 0.4
τt =10 ps 15 ps 20 ps 30 ps
0.2 0 0
100 200 50 150 Modulation frequency, ω/2π (GHz)
Figure 16.4 Dependence of responsivity (normalized) on modulation frequency w/2p for different tt.
16.5 Comparison with QWIPs and QDIPs Now we compare the responsivity and detectivity of GLPDs with K GLs calculated above and those of QWIPs (properly coupled with the incident terahertz or IR radiation) and QDIPs with the same number of QWs. The fraction of the absorbed photon flux in one (QW ) (QW ) (QW ) sW S 0 , where s(QW) is the cross section of the QW bW photon absorption due to the intersubband transitions and Sd the (QW) ≃ 2 ¥ 10–15 cm2 donor sheet density. Setting the usual values s W
299
300
Terahertz and Infrared Photodetection
(QW ) and S(0QW) ≃ 1012 cm–2, one obtains bW ≃ 0.002. This value is one order of magnitude smaller that bW. Hence, one can neglect the attenuation of radiation in QWIPs with K ≲ 100 (whereas in GLPDs it can be essential). In such a case, the responsivity of QWIPs is independent of the number of QWs K in the QWIP structure [33] and given by
R0(QW) =
(QW) eb W , Wpc
(16.18)
where pc is the socalled capture probability which relates to the QWIP gain G(QW) as G(QW) = (1  pc )/ Kpc 1 / Kpc [33]. Using Eqs. (16.4) and (16.18), we obtain R0 (QW) R0
2bW pc (QW) RW
K *.
(16.19)
Assuming that K = 50–100, (K* ≃ 30–39), R0(QW) = 0.002, and pc = 0.1, we obtain R0 /R0(QW) 70  90. The ratio of the detectivities can be presented as D*
D*(QW)
2bW pc K * (QW ) K bW
g(QW) th gth
(16.20)
As can be extracted from Ref. [26], gth µ exp( w 0 / kBT ), where ℏw0 ≃ 0.02 eV is the energy of optical phonon in GLs, whereas ) µ exp( e (QW) / kBT ), where e(QW) is the QW ionization energy g(QW th (ℏW ≳ e(QW)), Eq. (16.17) yields D*
D*(QW)
µ
2bW pc K * È (w 0  W) ˘ exp Í ˙. (QW) K bW Î 2kBT ˚
(16.21)
Different dependences of the responsivities and detectivities of GLDs and QWIPs on K are due different directions of the dark current and photocurrent: parallel to the GL plane in the former case and perpendicular to the QW plane in the latter case. The product of the factors in the righthand side of Eq. (16.21 ) except the last one can (QW) be on the order of unity. This is because a large ratio 2bW / bW can be compensated by relatively small capture parameter pc. However, the exponential factor in Eq. (16.21) is large in the terahertz range: W ≲ w0, i.e., at W/2p ≲ 50 THz. In particular, at T = 300 K and W/2p = 5–10 THz, the exponential factor in question is about 24–36.
Comparison with QWIPs and QDIPs
The GLPD responsivity and detectivity can also markedly exceed those of QDIPs [for which formulas similar to Eqs. (16.21) can be used] despite lower capture probability and thermoexcitation rate in QDIPs in comparison with QWIPs (see, for instance, Refs. [34– 36]). The ratios D*/D*(QW) and D*/D*(QD) dramatically increases with decreasing ℏW and T. This is attributed to the fact that the spectral dependence of the GLPDs detectivity is similar to the spectral dependence of the responsivity (D* µ bW/ℏW), whereas the GLPDs intended for the photodetection in different spectral ranges exhibit the same dark current (due to the gapless energy spectrum). In contrast, in QWIPs, QDIPs, and some other photodetectors (see, for example, Refs. [9, 10]) the transition to lower photon frequency requires to utilize the structures with lower ionization energy and, hence, exponentially higher dark current. The latter leads to quite different spectral dependencies of the GLPD detectivity and the detectivity of QWIPs and QDIPs (which drops with creasing photon frequency). GLPDs can surpass QWIPs and QDIPs in responsivity even at relatively high photon frequencies. For example, for a GLPD with K =25 at W/2p = 75 THz (wavelength l about 4 mm), we arrive at R0 ≃ 3 A/W. This value is three times larger than R0(QD) obtained experimentally for a QDIP with 25 InAs QD layers [37]. As for the detectivity, comparing a GLPD with K = 70 operating at T = 300 K and W/2p ≃ 15 THz (l ≃ 20 mm) and a QDIP with 70 QD layers [38], we obtain D* ~ 2 ¥ 108 cm Hz1/2/W and D*(QD) ~ 107 cm Hz1/2/W, respectively. GLPDs can surpass also photodetectors on narrowgap and gapless bulk semiconductors like HgCdTe (BSPDs). Apart from advantages associated with potentially simpler fabrication, GLPDs might exhibit higher detectivity (compare the data above and those from Ref. [39]). This can be attributed to relatively low thermogeneration rate in GLPDs compared to BSPDs with very narrow or zeroth gap. The point is that thermogeneration rate in GLPDs at room temperatures is primarily due absorption of optical phonons [27] which have fairly large energy ℏw0 (the Auger processes in GLs are forbidden) [40], whereas this rate in BSPDs is essentially determined by the Auger processes which are strong [39].
301
302
Terahertz and Infrared Photodetection
16.6 Discussion and Conclusions Analyzing Eqs. (164)–(16.7), we accepted that f(ℏW) 1 and, therefore, disregarded the frequency dependence of the absorption coefficient bW associated with the population of the low energy states by electrons and holes. For a rough estimate, the value of distribution function f(0) can be presented as f(0) ≲ f0(0)S/S0, where S is the electron and hole density in the isection under the reverse bias. This density, in turn, can be estimated as S = 2gthtt = gth2l/ v . Using the same parameters as above, for l =10 mm and T = 30 K, we obtain S/S0 = 0.25, so that f(0) ≲ 0.125 and bW WÆ0 ≳ 0.75b. It implies that the numerical data obtained above for the frequencies at the lower end of the terahertz range might be slightly overestimated. However, since the electronhole system in the isection can be pronouncedly heated by the electric field, the actual values of f(ℏW/2) can be smaller than in the latter estimate and, hence, bW can be rather close to b. The electron and hole heating in intrinsic GLs under the electric field was studied recently [28, 41]. As shown in Ref. [41] solving the kinetic equations, the electron and hole distribution functions in a GL in the range of low energies becomes f(0) become small at fairly small electric fields. Indeed, at T =300 K, f(0) varies from f(0) ≃ 0.2 to f(0) ≃ 0.05 when the electric field E increases from E = 3 V/cm to E =30 V/cm. For a GLPD with the length of the isection 2l = 10–30 mm (as in the estimates in Sections 16.3 and 16.4), these values of the electric field correspond to the reverse bias voltage V ≃ 3 ¥ 10–3–9 ¥ 10–2 V. Hence, the electron and hole populations in the isection should not lead to a marked deviation of the GL absorption bW from b = const. In contrast with the cases considered in Refs. [28, 41]. The finiteness of the transit time of electrons and holes in the isection of the GLstructures under consideration might affect the electron and hole heating resulting in minor modification of the absorption coefficient. Therefore, more careful calculation of bW at relatively low W can, in principle, be useful. In summary, we proposed and evaluated GLPDs based multipleGL pin structures. It was shown that GLPDs can exhibit high responsivity and detectivity in the terahertz and IR ranges at room temperatures. Due to relatively high quantum efficiency and low
Appendix
thermogeneration rate, the GLPD responsivity and detectivity can substantially exceed those of other photodetectors.
Acknowledgments
The authors are grateful to M. S. Shur, A. A. Dubinov, V. V. Popov, A. Satou, M. Suemitsu, and F. T. Vasko for fruitful discussions and comments. This work was supported by the Japan Science and Technology Agency, CREST, Japan.
Appendix: Effect of Vertical Screening in Multiple GLStructures
As was pointed out above, the thickness of multiple GLstructures even with rather large number of GLs K is in reality small in comparison with the lateral sizes of the device, namely, the lengths of all the section and, hence, the gates. Owing to this, the distribution of the dc electric potential y = 2j0/Vg normalized by Vg/2 (where Vg = Vn = –Vp) in the direction perpendicular to the GL plane (corresponding to the axis z) can be found from the onedimensional Poisson equation: d 2y dz 2
=
8p e æVg
K
ÂS
(k )
d(z  kd + d ).
k =1
(16.A1)
Here S(0k ) is the electron (hole) density in the kth GL in the nsection (psection), d is the spacing between GLs, and d(z) is the Dirac delta function. Considering that , where e Fk is the S(0k ) = (e Fk )2 / p2uF2 = (e2Vg2 / 4p 2uF2 )y 2 z = kd Fermi energy in the nsection (psection) of the kth GL, and replacing the summation in Eq. (16.A1 ) by integration (that is valid if K is not too small), we reduce Eq. (16.A1 ) to the following: d 2y dz
2
=
y2 L2s
,
(16.A2)
with the characteristic screening length Ls = uF æd / 2e3Vg µVg1/2 . One can assume that y z =0 = 2 + Wg (dy / dz) z=0 and y z =• = 0 [as
well as (dy / dz ) z=• = 0 ], where Wg is the thickness of the layer
303
304
Terahertz and Infrared Photodetection
separating the multiple GLstructure and the gates. Solving Eq. (16. A2) with the latter boundary conditions, we arrive at y=
1
(C + z / 6Ls )2
(16.A3)
,
where C satisfies the following equation:
C 3  C / 2 = (Wg / 6 Ls ).
(16.A4)
Since in reality Wg 6Ls , one obtains C (Wg / 6 Ls ) µVg1/6 . Setting d = 0.35 nm, Wg = 10 nm, æ = 4, and Vg = 2 V, one can obtain Ls ≃ 0.31 nm, and C ≃ 2.4. Equation (16.A3) yields 1/3
e F( k )
eVg
2[C + (k  1)d / 6Ls ]2
= e FT a( k ) .
(16.A5)
Here e FT = e F(1) = eVg / 2C 2 µ(Vg / Wg )2/3 is the Fermi energy of electrons in the topmost GL in the nsection (holes in the psection) and a(k) = [1 + (k –1)g]–2,
(16.A6)
where g = d / 6LsC µ Vg1/3 . At the above parameters (in particular, Wg = 10–50 nm and Vg = 2 V) g = d / 6LsC 0.12  0.20.
References
1. C. Berger, Z. Song, T. Li, X. Li, A. Y. Ogbazhi, R. Feng, Z. Dai, A. N. Marchenkov, E. H. Conrad, P. N. First, and W. A. de Heer, J. Phys. Chem., 108, 19912 (2004).
2. K. S. Novoselov, A. K. Geim, S. V. Morozov, D. Jiang, M. I. Katsnelson, I. V. Grigorieva, S. V. Dubonos, and A. A. Firsov, Nature (London), 438, 197 (2005).
3. A. H. Castro Neto, F. Guinea, N. M. R. Peres, K. S. Novoselov, and A. K. Geim, Rev. Mod. Phys., 81, 109 (2009).
4. F. T. Vasko and V. Ryzhii, Phys. Rev. B, 77, 195433 (2008).
5. V. Ryzhii, M. Ryzhii, and T. Otsuji, J. Appl. Phys., 101, 083114 (2007). 6. F. Rana, IEEE Trans. Nanotechnol., 7, 91 (2008).
7. A. Satou, F. T. Vasko, and V. Ryzhii, Phys. Rev. B, 78, 115431 (2008).
References
8. A. A. Dubinov, V. Ya. Aleshkin, M. Ryzhii, T. Otsuji, and V. Ryzhii, Appl. Phys. Express, 2, 092301 (2009).
9. V. Ryzhii, V. Mitin, M. Ryzhii, N. Ryabova, and T. Otsuji, Appl. Phys. Express, 1, 063002 (2008).
10. V. Ryzhii and M. Ryzhii, Phys. Rev. B, 79, 245311 (2009).
11. F. Xia, T. Murller, Y.M. Lin, A. ValdesGarsia, and F. Avouris, Nat. Nanotechnol., 4, 839 (2009).
12. P. Neugebauer, M. Orlita, C. Faugeras, A.L. Barra, and M. Potemski, Phys. Rev. Lett., 103, 136403 (2009).
13. V. Ryzhii, M. Ryzhii, A. Satou, T. Otsuji, A. A. Dubinov, and V. Ya. Aleshkin, J. Appl. Phys., 106, 084507 (2009).
14. Yu.M. Lin, D. B. Farmer, G. S. Tulevski, S. Xu, R. G. Gordon, and P. Avouris, Device Research Conf., Tech. Dig., p. 27 (2008).
15. D. Wei, Y. Liu, Y. Wang, H. Zhang, L. Huang, and G. Yu, Nano Lett., 9, 1752 (2009).
16. J. Zhu and J. C. S. Woo, Ext. Abstracts of the 2009 Int. Conf. on Solid State Devices and Materials, Sendai, 2009 (unpublished), pp. G9–G2. 17. V. V. Cheianov and V. I. Fal’ko, Phys. Rev. B, 74, 041403(R) (2006).
18. L. M. Zhang and M. M. Fogler, Phys. Rev. Lett., 100, 116804 (2008).
19. B. Huard, J. A. Sulpizio, N. Stander, K. Todd, B. Yang, and D. GoldhaberGordon, Phys. Rev. Lett., 98, 236803 (2007). 20. B. Ozyilmaz, P. JarilloHerrero, D. Efetov, D. Abanin, L. S. Levitov, and P. Kim, Phys. Rev. Lett., 99, 166804 (2007).
21. M. Ryzhii and V. Ryzhii, Jpn. J. Appl. Phys., Part 2, 46, L151 (2007).
22. V. Ryzhii, M. Ryzhii, V. Mitin, and M. S. Shur, Appl. Phys. Express, 2, 034503 (2009). 23. A. Bostwick, T. Ohta, T. Seyller, K. Horn, and E. Rotenberg, Nat. Phys., 3, 36 (2007). 24. L. A. Falkovsky and A. A. Varlamov, Eur. Phys. J. B, 56, 281 (2007).
25. A. Rose, Concepts in Photoconductivity and Allied Problems (Wiley, New York, 1963). 26. Long Wavelength Infrared Detectors, edited by M. Razeghi (Gordon and Breach, Amsterdam, 1996).
27. F. Rana, P. A. George, J. H. Strait, S. Shivaraman, M. Chanrashekhar, and M. G. Spencer, Phys. Rev. B, 79, 115447 (2009).
28. R. S. Shishir, D. K. Ferry, and S. M. Goodnick, J. Phys.: Conf. Ser., 193, 012118 (2009).
305
306
Terahertz and Infrared Photodetection
29. S. Ramo, Proc. IRE, 27, 584 (1 3 ).
30. C. K. Jen, Proc. IRE, 29, 345 (1941).
31. V. Ryzhii and G. Khrenov, IEEE Trans. Electron Devices, 42, 166 (1995).
32. N. Tsutsui, V. Ryzhii, I. Khmyrova, P. O. Vaccaro, H. Taniyama, and T. Aida, IEEE J. Quantum Electron., 37, 830 (2001). 33. H. Schneider and H. C. Liu, Quantum Well Infrared Photodetectors (Springer, Berlin, 2007). 34. V. Ryzhii, Semicond. Sci. Technol., 11, 759(1996).
35. V. Ryzhii, I. Khmyrova, M. Ryzhii, and V. Mitin, Semicond. Sci. Technol., 19, 8 (2004).
36. A. Rogalski, J. Antoszewski, and L. Faraone, J. Appl. Phys., 105, 091101 (2009).
37. H. Lim, S. Tsao, W. Zhang, and M. Razeghi, Appl. Phys. Lett., 90, 131112 (2007). 38. S. Chakrabarti, A. D. SiffRoberts, X. H. Su, P. Bhattacharya, G. Ariyawansa, and A. G. U. Perera, J. Phys. D, 38, 2135 (2005).
39. P. Martyniuk, S. Krishna, and A. Rogalski, J. Appl. Phys., 104, 034314 (2008). 40. M. S. Foster and I. L. Aleiner, Phys. Rev. B, 79, 085415 (2009).
41. O. G. Balev, F. T. Vasko, and V. Ryzhii, Phys. Rev. B, 79, 165432 (2009).
Chapter 17
Negative and Positive Terahertz and Infrared Photoconductivity in Uncooled Graphene*
V. Ryzhii,a,b,c,d D. S. Ponomarev,b,c M. Ryzhii,e V. Mitin,a,f M. S. Shur,g,h and T. Otsujia aResearch
Institute of Electrical Communication, Tohoku University, Sendai 9808577, Japan bInstitute of Ultra High Frequency Semiconductor Electronics of RAS, Moscow 117105, Russia cCenter of Photonics and TwoDimensional Materials, Moscow Institute of Physics and Technology, Dolgoprudny 141700, Russia dCenter for Photonics and Infrared Engineering, Bauman Moscow State Technical University, Moscow 111005, Russia eDepartment of Computer Science and Engineering, University of Aizu, AizuWakamatsu 9658580, Japan fDepartment of Electrical Engineering, University at Buffalo, Buffalo, NY 1460192, USA gDepartment of Electrical, Computer, and Systems Engineering and Department of Physics, Applied Physics, and Astronomy, Rensselaer Polytechnic Institute, Troy, NY 12180, USA hElectronics of the Future, Inc., Vienna, VA22181, USA vryzhii@ riec.tohoku.ac.jp *Reprinted with permission from V. Ryzhii, D. S. Ponomarev, M. Ryzhii, V. Mitin, M. S. Shur, and T. Otsuji (2019). Negative and positive terahertz and infrared photoconductivity in uncooled graphene, Opt. Mater. Express, 9(2), 585–597. Copyright © 2019 Optical Society of America. GrapheneBased Terahertz Electronics and Plasmonics: Detector and Emitter Concepts Edited by Vladimir Mitin, Taiichi Otsuji, and Victor Ryzhii
Copyright © 2021 Jenny Stanford Publishing Pte. Ltd.
ISBN 9789814800754 (Hardcover), 9780429328398 (eBook)
www.jennystanford.com
308
Negative and Positive Terahertz and Infrared Photoconductivity
We develop the model for the terahertz (THz) and infrared (IR) photoconductivity of graphene layers (GLs) at room temperature. The model accounts for the linear GL energy spectrum and the features of the energy relaxation and generationrecombination mechanisms inherent at room temperature, namely, the optical phonon absorption and emission and the Auger interband processes. Using the developed model, we calculate the spectral dependences of the THz and IR photoconductivity of the GLs. We show that the GL photoconductivity can change sign depending on the photon frequency, the GL doping and the dominant mechanism of the carrier momentum relaxation. We also evaluate the responsivity of the THz and IR photodetectors using the GL photoconductivity. The obtained results along with the relevant experimental data might reveal the microscopic processes in GLs, and the developed model could be used for the optimization of the GLbased photodetectors.
17.1 Introduction
The gapless energy carrier spectrum and high carrier mobility in graphene layers (GLs) [1] enable unique optical and transport properties. The GL conductivity dependence on the carrier effective temperature has been analyzed and reported in a number of publications (for example, [2–9]). Due to the specifics of the carrier scattering in the GLs, the variation of the GL DC conductivity under the terahertz (THz) and infrared (IR) irradiation (THz and IR photoconductivity) can exhibit interesting behavior [6, 10]. The response of the carrier system in the GLs caused by the THz and IR radiation enables their utilization in the bolometric photodetectors [11–15]. Extensive studies of the carrier dynamics in the GLs in the response to ultrashort optical pulses (for example, [16–24]) stimulate the creation of novel ultrafast optoelectronic devices. The GL ac (dynamic) conductivity under the optical pumping can become negative in the THz range due to the population inversion [25–28] (see also [16, 19]). The THz and IR photoconductivity in GLs is associated with the interplay of the variations of the carrier effective temperature and density (the quasiFermi energy). Depending on the dominating scattering mechanisms and the photon energies, the effective
Introduction
temperature can either exceed or be smaller than the lattice temperature. This can be accompanied by a splitting of the quasiFermi levels [25, 29]. The interplay of the intra and interband absorption of the incident THz and IR radiation [30] adds complexity to the processes governing the GL conductivity. The GL photoconductivity was experimentally studied in a number of works demonstrating the effect of negative photoconductivity [10, 31, 32]. However, it was also shown that the sign of the THz photoconductivity of the GLs changes with the radiation frequency depending on the environment [32]. Despite a variety of the works aimed to describe and explain the features of the THz and IR photoconductivity, there is still no transparent model of the phenomena. The previous studies mainly were focused on the deeply cooled GLs and related bolometric photodetectors. Due to this, the main energy relaxation and generationrecombination mechanisms were associated with the carrier interaction with acoustic phonons and ambient thermal radiation. However, in the uncooled GLs, the carrier intraband and interband transitions due to the recombination and emission of the optical phonons [33] (see also [10]) and the carriercarrier interaction (Auger processes) [34, 35] can dominate. The inclusion of these mechanisms is necessary for the explanation of the nontrivial spectral characteristics of the GL photoconductivity. Namely, the observed inversion of the photoconductivity sign requires an adequate but transparent model. In this chapter, we develop such a model, which accounts not only for the variations of the carrier temperature but also for the possible splitting of the quasiFermi levels associated with the THz and IR radiation absorption. This approach allows us to consider the effect of the THz and IR photoconductivity at room temperatures in more details. We also evaluate the application of this effect for uncooled THz and IR photodetectors. The obtained results can be used for the optimization of these photodetectors and promote a deeper insight into the GL microscopic properties. We focus on both the intrinsic (or compensated) and pdoped GLs at relatively elevated temperatures (such as room temperature). We assume that the carrier momentum relaxation is associated with impurity scattering, scattering on defects, and and on the acoustic phonons. The carrier scattering on the clustered impurities
309
310
Negative and Positive Terahertz and Infrared Photoconductivity
inside the GLs and the substrate inclusions in the decorated GLs is accounted for as well. The intraband and interband transitions of the carriers due to the emission and absorption of the optical phonons are considered as the crucial mechanism of the energy relaxation and the generationrecombination. Despite the specifics of the Auger generationrecombination in the GLs associated with the carrier dispersion law [34] and the carrier collinear scattering (see [35] and references therein), these generationrecombination mechanisms are also included into the model under consideration.
17.2 GL Conductivity Dependence on the Carrier Temperature
Due to relatively high carrier densities in GLs at the room temperature, their pair collisions lead to the establishment of the quasiFermi energy distributions, f e(e) and f h(e), with the same effective temperature T. Therefore, we use the following formula for the real part of the intraband conductivity of the GL channel sW at the frequency W (see [2–4]): e2 T t Ê T ˆ s W =  02 0 Á ˜ p Ë T0 ¯
l +1
Ú
•
dxx l+1
0 (1 + W2t 2 (T 0
d e [ f (x ) + f h (x )]. / T0 ) x ) dx (17.1) 2l 2l
Here it is assumed that the momentum relaxation time as a function of the momentum p is equal to t p = t 0 ( pvW / T0 )l = t 0 (T / T0 )l x l , where t 0 is its characteristric value, x = pvW/T0 is the normalized carrier energy in the GL, vW ≃ 108 cm/s is the characteristic velocity in GLs, and ℏ is the Planck constant. If the scattering on the weakly screened charged objects (weakly screened Coulomb, longscale scattering) prevails, tp µ p. This case corresponds to the superscript l in Eq. (17.1) equal to unity (l = 1). In the case of scattering on the neutral impurities and defects, the strongly screened charged impurities, and the acoustic phonons, t µ p–1 (i.e., l = –1). If several mechanisms contribute to the carrier scattering, tp can be described by a combination the linear and the inverse dependences. For a simplified description, in some papers tp = const is used.
GL Conductivity Dependence on the Carrier Temperature
The scattering processes can depend on the presence of largescale charged defects, clustered impurities [36, 37], and various particles in the GL or near the GL interface with the substrate. The latter can be important in the socalled decorated GLs [38, 39]. When the carrier momentum relaxation is determined by the short–range scattering, Eq. (17.1) yields for the pertinent conductivity sW is given by sW =
È ˘ 1 1 + ˙ . (17.2) Í e h (1 + W t ) ÍÎ exp(  m / T ) + 1 exp( m / T ) + 1 ˙˚ s 00
2 2
Here s00 = (e2T0t0/pℏ2) is the characteristic intraband conductivity (it is equal to the low electricfield conductivity in the case of shortrange scatterers). In the intrinsic (or compensated) GLs, the electronhole symmetry leads to the equality of the pertinent quasiFermi energies me = mh = m (this does not generally imply that the positions of the quasiFermi levels e Fe = m e /T and e Fh = m h / T coincide; such a coincidence only occurs if m = 0). In this case, Eq. (17.2) transforms to the following: sW =
2s 00
1 . (1 + W t ) [exp(m /T ) + 1] 2 2
(17.3)
In the case of the short–range scattering, one can find for the characteristic time t from Eq. (17.1) t t 0 3 / p . If the longscale momentum relaxation is the dominant (l = 1), we obtain from Eq. (17.1) 2
ÊTˆ Ê mˆ sW = F1 Á ˜ , 2 2 ÁT ˜ Ë T¯ (1 + W t ) Ë 0 ¯ 4s 00
where
F1 (h ) =
Ú
•
0
(17.4)
dxx exp(x  h ) + 1
is the FermiDirac integral. Equations (17.3) and (17.4) show that the variations of both the quasiFermi energy m and the effective temperature T caused by the radiation absorption determine the variation of the conductivity, i.e., the effect of photoconductivity. As demonstrated in the following, the quasiFermi energy changes not only due to the carrier density change but due to the heating.
311
312
Negative and Positive Terahertz and Infrared Photoconductivity
17.3 GenerationRecombination and Energy Balance Equations The equation governing the interband balance of the carriers can be generally presented as GAuger + GOpt + GAc + GRad = 0.
(17.5)
The terms in Eq. (17.5) correspond to the interband Auger generationrecombination processes and the processes associated with opticalphonon, acousticphonon, and radiative transitions (in particular, indirect transitions, for which some selection restrictions are lifted). In the situations under consideration (in particular in the temperature range in question), the characteristic times of the processes associated with acoustic phonons and radiative transitions (as was mentioned in Section 17.1) are much longer than those related to the opticalphonon and Auger mechanisms [6, 9, 33, 35]. Due to this, we disregard the terms GAc and GRad in Eq. (17.5). Due to the fast processes of the optical phonon decay into acoustic phonons and their effective removal, confirmed by high values of the Glayer thermal conductivity [40–42], the optical phonon system in the GLs is assumed to be in equilibrium with the lattice having the temperature T0. For the rate, GOpt, of the interband and intraband transitions assisted by the optical phonons emission and absorption one can use rather general equations accounting for the transitions matrix elements, the features of carrier energy spectrum in the GLs, and the conservation of the carrier momentum and energy [33]. As shown [29] (see also [11, 43]), at ℏw0 m, T, T0, where ℏw0 ≃ 200 meV is the energy of optical phonons in the GL, the general equations for GOpt [33] can be simplified by separating of the exponential factors and relatively slow varying factors depending on m and T0. Similar procedure leads to a simplified formula for GAuger. As the result, in the situation under consideration, we present Eq. (17.5) describing the carrier balance in the conduction and valence bands of the GL in the following form: È 2m Ê 1 1 ˆ ˘ ¸Ô 1 ÏÔ 1 + w 0 Á  ˜ ˙  1˝ + Ìexp Í t Opt Ô T T T t ¯ Ë ˙˚ Ô˛ Auger 0 ÎÍ Ó
˘ È Ê 2m ˆ int er IW Íexp ÁË ˜¯  1˙ = b T Â0 Î ˚
(17.6)
GenerationRecombination and Energy Balance Equations
The equation governing the energy electron and hole balance is given by: 1 t Opt
ÏÔ È 2m � Ê 1 1 ˆ ˘ ¸Ô 1
+ w 0 Á  ˜ ˙  1 ˝ + intra Ìexp Í Ë T0 T ¯ ˙˚ ˛
Í T
Ô t � Opt Î
ÓÔ W
I
intra W . = b � + b inter w 0 S 0
(
)
ÏÔ È Ê 1 1 ˆ ˘ ¸Ô e Í w 0 Á  ˜ ˙  1˝ Ìexp Ë T0 T ¯ ˙˚ Ô˛
ÍÎ
ÓÔ (17.7)
intra are the characteristic recombination and Here tOpt and t Opt intraband relaxation times associated with the carrier interaction with the optical phonons, tAuger is the Auger recombination time, b inter = (pa / k ) tanh(ℏW/4T) [2] (for a small m) and b intra = (4ps W / k c ) are the GL interband and intraband absorption coefficients (determined by the interband and intraband ac conductivities), respectively, S0 is the characteristic carrier density, a = (e2/cℏ) ≃ 1/137 is the fine structure constant, c is the speed of light in vacuum, and k is the background dielectric constant. The inter factors Â0 /t Opt , Â 0 /t � Opt , and S0/tAuger are weak functions of m and T (mentioned above, see, for example, [29]). These factor can be considered as phenomenological parameters of the model. The exponential terms in the lefthand sides of Eqs. (17.6) and (17.7) are proportional to the rate of the generationrecombination and the rate of the energy transfer into the lattice, respectively. The terms in the righthand sides of these equations correspond to the carrier photogeneration and to the power obtained by the electronhole system due to the radiation absorption. The latter is proportional to (bintra + binter )ℏW IW. Limiting our consideration by low radiation intensities IW, Eqs. (17.6) and (17.7) are presented as
1 2m �Ê 1
1 ˆ �w 0 (T  T0 ) intra in nter WIW + Á + intra ˜ )
.
+ b � � ( b � 0 0 2 ˜ ÁË t � w 0 Â 0 t � T0 t � Opt T
Opt Opt ¯ (17.8)
Ê 1 I 1 ˆ 2m 1 w 0 (T  T0 ) + + = b 0inter W ,
Á ˜ 2 t T t t � Â
T0 Ë Opt Opt Auger ¯
0
(17.9)
313
314
Negative and Positive Terahertz and Infrared Photoconductivity
where, due to a smallness of we put IW, 2 ÂG = Â0 = pT02 / 32vW and b inter b0inter = (pa / k ) tanh(ℏW/4T0)
and b intra b0intra = paD0 / k (1 + 3W2t 02/p 2 ). Here D0 = (4T0t0/pℏ) is the Drude factor. At T0 = 25 meV and t0 = (10–12 – 10–13) s, one obtains D0 ≃ 5.3 – 52.7.
17.4 GL Photoconductivity
Using Eqs. (17.8) and (17.9), we express the normalized carrier quasiFermi energy m/T and temperature variation (T – T0)/T0 via the radiation intensity IW, its frequency W, and the characteristic intra times t Opt ,t Opt , and tAuger as ˘t I È Ê Wˆ m  Í( b0inter + b0intra )Á ˜  b0inter (1 + a)˙ R W . T Ë w0 ¯ ÎÍ ˚˙ 2 Â0
˘ T t I Ê Wˆ T  T0 È inter � Í( b0 + b0intra )Á ˜ (1 + b)  b0inter ˙ 0 R W . T0 Ë w0 ¯ ÍÎ ˚˙ �w 0 Â0 Here
(17.10)
(17.11)
1 (1 + a) a = + , t R t Auger t Opt
is the characteristic relaxationrecombination time, which accounts for the interband transitions associated with the optical phonons and the Auger generation recombination processes, as well as the intraband energy relaxation on the optical phonons, intra and b = t Opt /t Auger . The parameters a and b can be a = t Opt /t Opt estimated using the data found previously [29, 33] and [33, 35], respectively. Equations (17.10) and (17.11) can be rewritten as Ê �W ˆ Ê W ˆ T0 È T  T0 1 � (1 + b)  1˜ Ítanh Á ˜ Á T0 (a + b + ab) �w 0 ÎÍ ¯ Ë 4T0 ¯ Ë w 0 +
˘
Ê W ˆ IW ˙ 2 2 2 Áw ˜ (1 + 3W t 0 /p ) Ë 0 ¯ ˚˙ IW D0 (1 + b)
,
(17.12)
È Ê W ˆ ˘ IW Ê �W ˆ Ê W ˆ D0 m 1 � 1  a˜ + Ítanh Á Á ˜˙ , ˜ Á 2 2 2 T 2(a + b + ab) ÎÍ Ë 4T0 ¯ Ë w 0 ¯ (1 + 3W t 0 /p ) Ë w 0 ¯ ˙˚ IW
(17.13)
GL Photoconductivity
where
IW =
k Â0 . pat Opt
The first term in the square brackets of Eq. (17.12) is negative when W < w0/(1 + b). In this case, the interband transitions promote a decrease in the carrier temperature. The point is that every act of the photon absorption brings the energy ℏW to the carrier system, while the interband emission of optical phonon decreases the carrier system energy by the value ℏw0, which is a smaller value. If b 1, these processes lead to the carrier heating. The Auger recombination (in the gapless GLs) does not directly change the carrier energy, but decreases the cooling role of the optical photon emission. In the limit of very strong Auger processes (tAuger tOpt, i.e., b 1), Eq. (17.12) yields
˘I Ê �W ˆ D0 T  T0 T0 Ê W ˆ È 1 � + Ítanh Á ˙ W ≥ 0. Á ˜ ˜ 2 2 2 T0 (1 + a) �w 0 Ë w 0 ¯ ÎÍ Ë 4T0 ¯ (1 + 3W t 0 /p ) ˙˚ IW (17.14)
In the latter case, the radiative interband processes supply the energy, while the interband optical phonon emission does not work (only the intraband optical phonon processes contribute to the carrier energy relaxation). In this limit, we obtain from Eq. (17.13) m = 0. The latter implies that the electron and hole quasiFermi levels coincide (e Fe = e Fh = 0) .
Figure 17.1 shows the carrier temperature variation (T – T0)/ T0 and the quasiFermi energy m/T normalized by IW /IW (i.e., the quantities [(T  T0 )/T0 ]( I W /I W) and ( m/T )(IW /IW )) , versus the photon energy ℏW in the GLs with dominating shortrange scattering calculated using Eqs. (17.12) and (17.13) for different b (i.e., different tAuger) and different t0. We set ℏw0 = 200 meV, T0 = 25 meV, a ≃ p2(T0/ ℏw0)2(1 + 2.19T0/ ℏw0) ≃ 0.2 [24]. As seen from Fig. 17.1 that the photon energies where m and (T – T0) change their signs do not coincide. Using Eqs. (17.3) and (17.13) when m 2T, for the difference Ds W = s WÆ0  s 00 between the dc conductivity under irradiation and the dc dark conductivity we obtain Ds W m , s 00 2T
(17.15)
315
316
Negative and Positive Terahertz and Infrared Photoconductivity
so that
È Ê �W ˆ Ê W Ê W ˆ ˘ IW ˆ D0 Ds W 1 � 1  a˜ + Ítanh Á ˙ . ˜ Á 2 2 2 Áw ˜ 4T 4(a + b + ab) ÍÎ w s 00 Ë 0¯Ë 0 ¯ (1 + 3W t 0 /p ) Ë 0 ¯ ˚˙ IW
(17.16)
1
0.2
10
100 0.8
0.1
0.4
0.0
0.0 0
0.1 0.2 1
=1 ps b=5.0 b=1.0 b=0.1
0.4
10
10
1
0.2
ħ
b=0.1 100
0.8
100 0.8
0.1
0
=1 ps
0
1
0.0
0.0 0.1 0.2 1
0.4
b=0.1
0.4
=1.0 ps 0 =0.5 ps 0 =0.1 ps 0
10
0.8 ħ
100
Figure 17.1 Upper panel: the normalized carrier temperature variation (T – T0)/T0 (dashed lines) for different values of the parameter b (upper panel) and t0 = 1 ps and the quasiFermi energy m/T (solid line) for b = 0.1 and t0 = 1 ps. Lower panel: the normalized carrier temperature variation (T – T0)/T0 (dashed line) for b = 0.1 and t0 = 1 ps and the quasiFermi energy m/T (solid lines) for b = 1 and different t0.
GL Photoconductivity
Figure 17.2 shows the GL photoconductivity (DsW/s00) normalized by a factor ( IW /IW ) ) calculated using Eq. (17.16) for different parameters. The GL photoconductivity as a function of the photon energy changes its sign twice at ℏW = ℏW0 and ℏW = ℏW1 which correspond to the points, where m/T = ee = eh = 0. One can see that the absolute value of the GL photoconductivity steeply decreases with increasing b, i.e., with the decreasing Auger recombination time tAuger (and, hence, decreasing tr). If tAuger tends to zero, the quantities m/T and Ds0 also tend to zero, despite (T – T0) π 0, as follows from Eqs. (17.13) and (17.16). All this is because at very intensive Auger processes the splitting of the quasiFermi levels vanishes, and the factor in the square brackets in the rightside of Eq. (17.2) is equal to unity. Hence, the conductivity becomes independent of the carrier temperature. 1
10
100
0.4
10
1
100
0.4
0.2
0.0
0.0 0.2
0
0.4 1
10
=1 ps b=5.0 b=1.0 b=0.1
100
0.4
b=0.1 =1.0 ps =0.5 ps 0 =0.1 ps
0
0.8
0
1 ħ
10
100
Figure 17.2 The normalized GL photoconductivity DsW/s00 as functions of the photon energy ℏW (dominant shortrange scattering) for different b = tOpt/tAuger and t0 = 1 ps (left panel) and different t0 and b = 0.1 (right panel).
As seen from Fig. 17.2, the GL photoconductivity is negative DsW < 0 in the photon energy ranges 0 < ℏW < ℏW0 and ℏW1 > ℏW. In the intermediate range ℏW0 < ℏW < ℏW1, the GL photoconductivity is positive. Taking into account that in reality D0 > 4T0(1 + a)/ ℏw0, i.e., w0t0 > p(1 + a), from Eq. (17.16) we obtain W0 �
p
3t 0
T0 D0 4T0 16p 1 � µ t 01/2 (17.17) (1 + a) w 0 3(1 + a)w 0t 0 �
317
318
Negative and Positive Terahertz and Infrared Photoconductivity
and
È T0 ˘ 4p 2 W1 : (1 + a)w 0 Í1  ˙ : (1 + a)w 0 . 2 ÍÎ 3(1 + a) w 0t 0 nw 0 ˚˙
(17.18)
For t0 = (10–12 – 10–13) s–1 and a ≃ 0.2, from Eqs. (17.17) and (17.18) one obtains W0/2p ≃ (1.35 – 3.16) THz and W1/2p ≃ (59.29 – 60.92) THz. Thus, the frequencies, at which the GL photoconductivity changes sign, correspond to the THz range (W0/2p) and to the MidIR range (W1/2p). It should be noted that if the momentum relaxation time tp is independent of the momentum p (as was assumed in some GL conductivity models [10, 44, 45]), the conductivty variation Ds0/s00 ≃ m/4T [46] (compare with Eq. (17.15). Therefore, the results for the case of tp = const are qualitatively close to those obtained in this section.
17.5 Clustered Impurities and Decorated GLs: LongRange Scattering
In this case, using Eq. (17.4), at relatively low intensities of the incident radiation IΩ when the deviation of m from zero is small, we obtain ÊTˆ sW = 2 2 ÁT ˜ (1 + W t 0 ) Ë 0 ¯ s 00
2
Hence,
2 2 È p 2 4m ÊTˆ s 00 Ê m ˆ ˘ p2 Í + ln2 + Á ˜ ˙ . Ë T ¯ ˙ 3 (1 + W2t 02 ) ËÁ T0 ¯˜ T ÍÎ 3 ˚ (17.19)
Ds W 2p 2 (T  T0 ) . T0 s 00 3
(17.20)
The latter is quite different from Eq. (17.15), which is valid in the case of shortrange momentum relaxation. Equation (17.19) with an equation similar to Eq. (17.11) results in (compare with Eq. (17.14)) T0 Ds W 2p 2 " s 00 3(a + b + ab) tw 0
È Ê tW ˆ Ê W ˆ D (1 + b) Ê W ˆ ˘ I (1 + b  1)˜ + 0 2 2 Á ˜ ˙ W . Ítanh Á ˜ Á Ë 4T0 ¯ Ë w 0 ¯ (1 + W t 0 ) Ë w 0 ¯ ˚˙ IW ÎÍ
(17.21)
Clustered Impurities and Decorated GLs: LongRange Scattering
Figure 17.3 shows the normalized responsivity of the photodetectors based on the GLs with the dominant longrange scattering calculated using Eq. (17.21). 1
5 4 3
0
10
100
10
1
=1 ps b=5.0 b=1.0 b=0.1
100
b=0.1 =1.0 ps =0.5 ps 0 =0.1 ps
0
0
2 1 0 1 1
10
100
1 ħ
10
100
Figure 17.3 The same as in Fig. 17.2 but in the case of dominant longrange scattering: for b = tOpt/tAuger and t0 = 1 ps (left panel) and for t0 and b = 0.1 (right panel).
As follows from the comparison of Eqs. (17.16) and (17.21) (see also Figs. 17.2 and 17.3), the photoconductivities involving the short and longrange scattering mechanisms exhibit fairly different spectral dependences: the photoconductivity at longrange scattering is positive at low and high photon energy and negative in the range of the intermediate photon energies. This is because in the case of the dominant shortrange scattering, the variation of the dc conductivity stimulated by the interband and intraband radiative transitions is associated primarily with the variation of m (more exactly with the variation of m/T), i.e., with the shifts of the electron and hole quasiFermi levels. The latter is in contrast with the case of the dominant longscale scattering in which the variation of the dc conductivity is due to the variation of the carrier effective temperature. This can be seen from the comparison of Eqs. (17.3) and (17.19) describing a decrease in the conductivity with increasing –m/T and an increase with increasing T, respectively.
319
320
Negative and Positive Terahertz and Infrared Photoconductivity
17.6 Responsivity of the GLBased Photodetectors Using the obtained values of the photoconductivity, DsW, of the GLs one can find the responsivity RW = DsWE/ℏWIW of the photodetectors based on undoped GL. Using Eqs. (17.16) and (17.21), for the cases of the dominant short and longscale scattering we arrive at Ê �W ˆ Ê W Ê Wˆ ˆ D0 D0 RW Ê T0 ˆ � tanh Á  1  a)˜ + Á ˜, R (a + b + ab) ÁË �W ˜¯ Ë 4T0 ¯˜ ËÁ w 0 ¯ (1 + 3W2t 02/p 2 ) Ë w 0 ¯
(17.22)
Ê �W ˆ Ê W ˆ D0 (1 + b) Ê W ˆ 2p 2 D0 Ê T02 ˆ RW � , (1 + b)  1˜ + ˜ tanh Á Á R 3(a + b + ab) Ë �2w 0 W ¯ Ë 4T0 ¯˜ ËÁ w 0 ¯ (1 + 3W2t 02/p 2 ) ÁË w 0 ˜¯
respectively, where
(17.23) R=
2 2 3a �e t Opt v W E
16 k
T03 L
(17.24)
Here E is the electric field along the GL plane and L is the spacing between the contacts. For example, setting t0 = 10–12 s, tOpt = 10–12 s, k = 4, L = 10–4 cm, and E = 100 V/cm, from Eq. (17.24) we obtain R ≃ 2.47 ¥ 10–4 A/W. One needs to note that the expression for RW includes a large parameter D0. In particular, for the responsivity of the photodetector using high quality GLs (t0 = 10–11 s) at ℏW = 10 meV (i.e., W/2p ≃ 2.5 THz) Eq. (17.21) yields RW ≃ 1.8 A/W. Figures 17.4 and 17.5 show the RW/R versus ℏW dependences calculated using Eqs. (17.12) and (17.22) for the GLphotodetectors with different t0 and b at a = 0.2. As the GL photoconductivity, the detector responsivity RW also turns to zero at certain frequencies. The responsivity of the GLbased photodetectors is proportional to the fundamental constant pa ≃ 0.023, which determines the coupling of the carriers and the incident radiation. The inclusion of the plasmonic effects associated with the excitation of the plasmons in the optical couplers (metal gratings and so on) and in the GLs can lead to a substantial reinforcement of the carrierradiation coupling (see, for example [47] and references therein). As a result, the GLdetector responsivity can be markedly enhanced. The responsivity spectral characteristic can exhibit pronounced plasmonic resonances superimposed on the spectral dependences obtained above.
Heavily Doped GLs
10 40
100 0
30
10
100 b=0.1 0 =1.0 ps 0 =0.5 ps 0 =0.1 ps
=1 ps b=5.0 b=1.0 b=0.1
20 10 10
100
100
10 ħ
Figure 17.4 The spectral characteristics of the responsivity, RW/R, of the GLbased photodetectors with dominant shortrange scattering at different b and t0 = 1 ps (left panel) and different t0 and b = 0.1 (right panel).
10
100 0
20
10
=1 ps b=5.0 b=1.0 b=0.1
100 b=0.1 0 =1.0 ps 0 =0.5 ps 0 =0.1 ps
10
10
100
10
100
ħ
Figure 17.5 The same as in Fig. 17.4 but for the photodetectors with the dominant longrange scattering.
17.7 Heavily Doped GLs Since the pristine GLs are usually ptype, we will consider the GLs with sufficiently high acceptor and hole densities SA. In the limit of short Auger recombination time, me = –mh and the variations of the carrier temperature do not lead to the variations of the GL conductivity and the effect of the photoconductivity vanishes. In a more realistic situation one can to assume the long recombination
321
322
Negative and Positive Terahertz and Infrared Photoconductivity
time tAuger, therefore, the term with tAuger can be omitted. In this case, we can use Eqs. (17.6) and (17.7) but with 2m replaced by (me + mh). Apart from this, the quantities b0inter and b0intra should be replaced by b Ai nter =
and
Ê W/2 + m0 ˆ ˘ Ê W/2  m0 ˆ pa È + tanh Á Ítanh Á ˜ ˜¯ ˙ 2T0 2T0 Ë ¯ Ë 2 k ÎÍ ˚˙ b Ai ntra =
4paD0 k (1 + W2t 02T02/m02 )
,
respectively, and instead of S0 one needs to put S = SA S0. As a result, we arrive at the following equations:
È È Ê 1 1ˆ˘ Ê W ˆ˘ I Ê Wˆ i ntra exp Íw 0 Á  ˜ ˙ = 1 + Íb Aintra Á ˜ + b Ainter Á .  1˜ ˙ W t Opt w T T w Â Ë ¯ Ë ¯ Ë ¯ ÍÎ ÍÎ 0 0 0 ˚˙ A ˚˙ (17.25) È me + mh Ê 1 1ˆ˘ I + w 0 Á  ˜ ˙ = 1 + b Ainter W t Opt . exp Í SA Ë T0 T ¯ ˙˚ ÍÎ T
From Eqs. (17.25) and (17.26), we obtain
(17.26)
Ê Wˆ Ê W ˆ˘ I T  T0 T È intra , (17.27) � 0 Íb Aintra Á ˜ + b Ainter Á  1˜ ˙ W t Opt �w 0 ÍÎ T0 Ë w0 ¯ Ë w0 ¯ ˙˚ S A I m e + m h w 0 (T  T0 ) = b Ainter W t Opt . + SA T T0T
(17.28)
The hole Fermi energies me and mh are related to the effective temperature T as 2 Ê me ˆ ˘ Ê T ˆ È Ê mh ˆ F U = Á ˜ ÍF1 Á 1Á ˜ ˜ ˙. Ë T0 ¯ ÍÎ Ë T ¯ Ë T ¯ ˙˚
(17.29)
Here U µ SA = const. Taking into account that at m T, F1(x) ≃ (x2/2 + p2/6) + x ln(1 + exp(–x), at T ~ T0 from Eq. (17.28) for mh = m we obtain m m0 È Ê p 2 T02 ˆ (T  T0 ) ˘ m0 È (T  T0 ) ˘ Í1  Á 1 + ˙ Í1 ˙ . (17.30) ˜ T0 ˚ T T0 Í Ë 3 m02 ¯ T0 ˙ T0 Î Î ˚
Conclusions
The screening length of the charged scatterers in the doped GLs with m T, is much shorter than that in the intrinsic GLs. Therefore, it is natural to assume that in the former GLs the shortrange scattering dominates. Considering Eq. (17.2) with the carrier temperature and the quasiFermi energies given by Eqs. (17.27), (17.28), and (17.30), we get Ê m ˆ ÏÔ È Ê �W/2  m0 ˆ Ê �W/2 + m0 ˆ ˘ S Ds W �  0 exp Á  0 ˜ Ì Ítanh Á + tanh Á ˜ ˜˙ s 00 2T0 2T0 aS A Ë T0 ¯ ÔÓ ÍÎ Ë ¯ Ë ¯ ˙˚ Ê W ˆ Ô¸ IW Ê W ˆ D0 ¥Á  1  a˜ + Á ˜˝ , 2 2 2 2 Ë w0 ¯ (1 + W t 0T0 /m0 ) Ë w 0 ¯ Ô˛ IW
(17.31)
If m0 > ℏW1/2 ≃ (1 + a) ℏw0/2, Eq. (17.15) yields DsW < 0 at all the photon energies. This is in line with the experimental results for the pGLs with SA = (2 – 11) ¥ 1012 cm–2, i.e., with m0 = 192 – 367 meV [10]. Equation (17.31) resembles Eq. (17.16). However, the latter includes a small factor [exp(–m0/T0)/SA], different frequencydependent factor of the interband absorption coefficient, and much shorter t = t 0T0 /m0 3t 0 /p . Due to the former, the responsivity of the photodetectors based on doped GLs is smaller than that of the intrinsic GLs. The factor [exp(–m0/T0)/SA] reflects the facts that the GL conductivity is a rather weak function of the carrier temperature at m0 T0 and that heat received by the carrier system from the absorbed radiation is distributed among a larger number of the carriers (SA S0).
17.8 Conclusions
We developed an analytical model describing the THz and IR photoconductivity in the GLs at room temperature. Using this model we showed that the energy relaxation and the generationrecombination associated with the optical phonons and the Auger processes are crucial for determining the behavior of GL photoconductivity. We found that in the GLs with dominating shortrange scattering mechanism of the carrier momentum relaxation the photoconductivity of the intrinsic GLs changes sign at a certain photon frequency W0 in the THz range. Depending on
323
324
Negative and Positive Terahertz and Infrared Photoconductivity
the GL parameters (the transition from the negative to positive photoconductivity) occurs at a certain photon frequency W1 in the midIR range (the photoconductivity is negative at W < W0 and W > W1, while it is positive in the range W0 < W < W1. In contrast, in the case of the longrange scattering dominances, the photoconductivity is positive at W < W0 and W > W1 and negative at W0 < W1. The change in the GL environment might result in the change from the shortrange to longrange scattering. The evaluated responsivity of the GLbased THz and IR photodetectors indicates their prospects for different applications.
Funding
Japan Society for Promotion of Science (16H06361); Russian Science Foundation (142900277); Russian Foundation for Basic Research (163760110, 180701379); RIEC NationWide Collaborative Research Project, Japan; Office of Naval Research (Project Monitor Dr. Paul Maki).
Acknowledgments
The authors are grateful to A. Arsenin, V. E. Karasik, V. G. Leiman, and P. P. Maltsev for useful discussions.
Disclosures
The authors declare that there are no conflicts of interest related to this article.
References
1. A. H. Castro Neto, F. Guinea, N. M. R. Peres, K. S. Novoselov, and A. K. Geim, The electronic properties of graphene, Rev. Mod. Phys., 81(1), 109–162 (2009).
2. L. A. Falkovsky and A. A. Varlamov, Spacetime dispersion of graphene conductivity, Eur. Phys. J. B, 56(4), 281–284 (2007).
3. V. T. Vasko and V. Ryzhii, Voltage and temperature dependence of conductivity in gated graphene, Phys. Rev. B, 76(23), 233404 (2007).
References
4. E. H. Hwang, S. Adam, and S. D. Sarma, Carrier transport in twodimensional graphene layers, Phys. Rev. Lett., 98(18), 186806 (2007).
5. V. Vyurkov and V. Ryzhii, Effect of Coulomb scattering on graphene conductivity, JETP Lett., 88(5), 370–373 (2008).
6. V. T. Vasko and V. Ryzhii, Photoconductivity of intrinsic graphene, Phys. Rev. B, 77(19), 195433 (2008).
7. E. H. Hwang and S. das Sarma, Acoustic phonon scattering limited carrier mobility in twodimensional extrinsic graphene, Phys. Rev. B, 77(11), 115449 (2008).
8. E. H. Hwang and S. das Sarma, Screening induced temperature dependent transport in 2D graphene, Phys. Rev. B, 79(16), 165404 (2009). 9. O. G. Balev, V. T. Vasko, and V. Ryzhii, Carrier heating in intrinsic graphene by a strong dc electric field, Phys. Rev. B, 79(16), 165432 (2009).
10. J. N. Heyman, J. D. Stein, Z. S. Kaminski, A. R. Banman, A. M. Massari, and J. T. Robinson, Carrier heating and negative photoconductivity in graphene, J. Appl. Phys., 117(1), 015101 (2015).
11. V. Ryzhii, T. Otsuji, M. Ryzhii, N. Ryabova, S. O. Yurchenko, V. Mitin, and M. S. Shur, Graphene terahertzuncooled bolometers, J. Phys. D: Appl. Phys., 46, 065102 (2013).
12. Xu Du, D. E. Prober, H. Vora, and C. Mckitterick, Graphenebased bolometers, 2D Mater., 1(1), 1–22 (2014). 13. Qi Han, T. Gao, R. Zhang, Yi Chen, J. Chen, G. Liu, Y. Zhang, Z. Liu, X. Wu, and D. Yu, Highly sensitive hot electron bolometer based on disordered graphene, Sci Rep., 3, 3533 (2013).
14. G. Skoblin, J. Sun, and A. Yurgens, Graphene bolometer with thermoelectric readout and capacitive coupling to an antenna, Appl. Phys. Lett., 112(6), 063501 (2018).
15. Y. Wang, W. Yin, Q. Han, X. Yang, H. Ye, Q. Lv, and D. Yin, Bolometric effect in a waveguideintegrated graphene photodetector, Chin. Phys. B, 25(11), 118103 (2016).
16. T. Li, L. Luo, M. Hupalo, J. Zhang, M. C. Tringides, J. Schmalian, and J. Wang, Femtosecond population inversion and stimulated emission of dense Dirac fermions in graphene, Phys. Rev. Lett., 108(16), 167401 (2012). 17. S. BoubangaTombet, S. Chan, T. Watanabe, A. Satou, V. Ryzhii, and T. Otsuji, Ultrafast carrier dynamics and terahertz emission in optically pumped graphene at room temperature, Phys. Rev. B, 85(3), 035443 (2012).
325
326
Negative and Positive Terahertz and Infrared Photoconductivity
18. I. Gierz, J. C. Petersen, M. Mitrano, C. Cacho, I. E. Turcu, E. Springate, A. Stohr, A. Kohler, U. Starke, and A. Cavalleri, Snapshots of nonequilibrium Dirac carrier distributions in graphene, Nat. Mater., 12(12), 1119– 1124 (2013).
19. T. Watanabe, T. Fukushima, Y. Yabe, S. A. BoubangaTombet, A. Satou, A. A. Dubinov, V. Ya. Aleshkin, V. Mitin, V. Ryzhii, and T. Otsuji, The gain enhancement effect of surface plasmonpolaritons on terahertz stimulated emission in optically pumped monolayer graphene, New J. Phys., 15(7), 07503 (2013). 20. K. J. Tielrooij, J. C. W. Song, S. A. Jensen, A. Centeno, A. Pesquera, A. Z. Elorza, M. Bonn, L. S. Levitov, and F. H. L. Koppens, Photoexcitation cascade and multiple hotcarrier generation in graphene, Nat. Phys., 9(4), 248–252 (2013).
21. E. Gruber, R. A. Wilhelm, R. Petuya, V. Smejkal, R. Kozubek, A. Hierzenberger, B. C. Bayer, I. Aldazabal, A. K. Kazansky, F. Libish, A. V. Krasheninnikov, M. Schleberger, S. Facsko, A. G. Borisov, A. Arnau, and F. Aumayr, Ultrafast electronic response of graphene to a strong and localized electric field, Nat. Commun., 7, 13948 (2016).
22. G. X. Ni, L. Wang, M. D. Goldflam, M. Wagner, Z. Fei, A. S. McLeod, M. K. Liu, F. Keilmann, B. Ozyilmaz, A. H. Castro Neto, J. Hone, M. M. Fogler, and D. N. Basov, Ultrafast optical switching of infrared plasmon polaritons in highmobility graphene, Nat. Photonics, 10, 244–247 (2016).
23. A. Mousavian, B. Lee, A. D. Stickel, and Y.S. Lee, Ultrafast photocarrier dynamics in singlelayer graphene driven by strong terahertz pulses, J. Opt. Soc. Am. B, 35(6), 1255–1259 (2018).
24. M. Baudisch, A. Marini, J. D. Cox, T. Zhu, F. Silva, S. Teichmann, M. Massicotte, F. Koppens, L. S. Levitov, F. J. G. de Abajo, and J. Biegert, Ultrafast nonlinear optical response of Dirac fermions in graphene, Nat. Commun., 9, 1018 (2018).
25. V. Ryzhii, M. Ryzhii, and T. Otsuji, Negative dynamic conductivity of graphene with optical pumping, J. Appl. Phys., 101(8), 083114(2007).
26. V. Ryzhii, M. Ryzhii, A. Satou, T. Otsuji, A. A. Dubinov, and V. Y. Aleshkin, Feasibility of terahertz lasing in optically pumped epitaxial multiple graphene layer structures, J. Appl. Phys., 106(8), 084507 (2009). 27. D. Svintsov, V. Ryzhii, A. Satou, T. Otsuji, and V. Vyurkov, Carriercarrier scattering and negative dynamic conductivity in pumped graphene, Opt. Express, 22(17), 19873–19686 (2014). 28. D. Svintsov, V. Ryzhii, and T. Otsuji, Negative dynamic Drude conductivity in pumped graphene, Appl. Phys. Express, 7, 115101 (2014).
References
29. V. Ryzhii, M. Ryzhii, V. Mitin, A. Satou, and T. Otsuji, Effect of heating and cooling of photogenerated electronhole plasma in optically pumped graphene on population inversion, Jpn. J. Appl. Phys., 50(9), 094001 (2011).
30. F. T. Vasko, V. V. Mitin, V. Ryzhii, and T. Otsuji, Interplay of intra and interband absorption in disordered graphene, Phys. Rev. B, 86(23), 235424 (2012).
31. S. Zhuang, Y. Chen, Y. Xia, N. Tang, X. Xu, J. Hu, and Z. Chen, Coexistence of negative photoconductivity and hysteresis in semiconducting graphene, AIP Adv., 6(4), 045214 (2016). 32. C. J. Docherty, C. T. Lin, H. J. Joyce, R. J. Nicholas, L. M. Hertz, L. J. Li, and M. B. Johnston, Extreme sensitivity of graphene photoconductivity to environmental gases, Nat. Commun., 3, 1228 (2012). 33. F. Rana, P. A. George , J. H. Strait, S. Sharavaraman, M. Charasheyhar, and M. G. Spencer, Carrier recombination and generation rates for intravalley and intervalley phonon scattering in graphene, Phys. Rev. B, 79(11), 115447 (2009).
34. M. S. Foster and I. L. Aleiner, Slow imbalance relaxation and thermoelectric transport in graphene, Phys. Rev. B, 79(8), 085415 (2009).
35. G. Alymov, V. Vyurkov, V. Ryzhii, A. Satou, and D. Svintsov, Auger recombination in Dirac materials: a tangle of manybody effects, Phys. Rev. B, 97(20), 205411 (2018).
36. K. M. McCreary, K. Pi, A. G. Swartz, Wei Han, W. Bao, C. N. Lau, F. Guinea, M. I. Katsnelson, and R. K. Kawakami, Effect of cluster formation on graphene mobility, Phys. Rev. B, 81(11), 115453 (2010).
37. N. Sule, S. C. Hagness, and I. Knezevic, Clustered impurities and carrier transport in supported graphene, Phys. Rev. B, 89(16), 165402 (2014).
38. T. Stauber, G. GomezSantos, and F. Javier Garcia de Abajo, Extraordinary absorption of decorated undoped graphene, Phys. Rev. Lett., 112(7), 077401 (2014),
39. V. Ryzhii, T. Otsuji, M. Ryzhii, V. Mitin, and M. S. Shur, Effect of indirect interband transitions on terahertz conductivity in “decorated” graphene bilayer heterostructures, Lithuanian J. Phys., 55(4), 243–248 (2015). 40. A. A. Balandin, S. Ghosh, W. Bao, I. Calizo, D. Teweldebrhan, F. Miao, and C. N. Lau, Superior thermal conductivity of singlelayer graphene, Nano Lett., 8(3), 902–907 (2008).
327
328
Negative and Positive Terahertz and Infrared Photoconductivity
41. S. Ghosh, I. Calizo, D. Teweldebrhan, E. P. Pokatilov, D. L Nika, A. A. Balandin, W. Bao, F. Miao, and C. N. Lau, Extremely high thermal conductivity of graphene: prospects for thermal management applications in nanoelectronic circuits, Appl. Phys. Lett., 92(15), 151911 (2008). 42. A. A. Balandin, Thermal properties of graphene and nanostructured carbon materials, Nat. Mater., 10, 569–581 (2011).
43. V. Ryzhii, M. Ryzhii, V. Mitin, and T. Otsuji, Toward the creation of terahertz graphene injection laser, J. Appl. Phys., 110(9), 094503 (2011). 44. K. F. Mak, M. Y. Sfeir, Y. Wu, Ch. H. Lui, J. A. Misewich, and T. F. Heinz, Measurement of the optical conductivity of graphene, Phys. Rev. Lett., 101(19), 196405 (2008).
45. H. M. Dong, W. Xu, and F. M. Peters, Electrical generation of terahertz blackbody radiation from graphene, Opt. Express, 26(19), 24621– 24626 (2018). 46. V. Ryzhii, M. Ryzhii, D. S. Ponomarev, V. G. Leiman, V. Mitin, M. S. Shur, and T. Otsuji, Negative photoconductivity and hotcarrier bolometric detection of terahertz radiation in graphenephosphorene hybrid structures, J. Appl. Phys., 125(15), 151608 (2019).
47. B. Zhao, J. M. Zhao, and Z. M. Zhang, Resonance enhanced absorption in a graphene monolayer using deep metal gratings, J. Opt. Soc. Am. B, 32(6), 1176–1185 (2018).
Part 3
Population Inversion and Negative
Conductivity in Graphene and
Graphene Structures
Chapter 18
Negative Dynamic Conductivity of Graphene with Optical Pumping*
V. Ryzhii,a M. Ryzhii,a and T. Otsujib aComputer
Solid State Physics Laboratory, University of Aizu,
AizuWakamatsu 9658580, Japan
bResearch Institute of Electrical Communication, Tohoku University,
Sendai 9808577, Japan
[email protected]
We study the dynamic ac conductivity of a nonequilibrium twodimensional electronhole system in optically pumped graphene. Considering the contribution of both interband and intraband transitions, we demonstrate that at sufficiently strong pumping the population inversion in graphene can lead to the negative net ac conductivity in the terahertz range of frequencies. This effect might be used in graphenebased coherent sources of terahertz radiation. *Reprinted with permission from V. Ryzhii, M. Ryzhii, and T. Otsuji (2007). Negative dynamic conductivity of graphene with optical pumping, J. Appl. Phys., 101, 083114. Copyright © 2007 American Institute of Physics. GrapheneBased Terahertz Electronics and Plasmonics: Detector and Emitter Concepts Edited by Vladimir Mitin, Taiichi Otsuji, and Victor Ryzhii
Copyright © 2021 Jenny Stanford Publishing Pte. Ltd.
ISBN 9789814800754 (Hardcover), 9780429328398 (eBook)
www.jennystanford.com
332
Negative Dynamic Conductivity of Graphene with Optical Pumping
18.1 Introduction A significant progress in the fabrication of graphene, demonstration of its exceptional electronic properties, and the possibility of creating electronic and optoelectronic devices on the basis of graphene heterostructures have attracted widespread attention [1] (see also, Refs. [2–16]). The gapless energy spectrum of electrons and holes in graphene can lead to specific features of its transport, plasma, and optical properties. One might expect that under optical pumping resulting in photogeneration of electronhole pairs, the population inversion can be achieved. In such a case, lasing of rather longwave (terahertz) radiation in graphene may be possible. In this work, using the developed model, we calculate the dynamic ac conductivity of a nonequilibrium twodimensional electronhole system in graphene under interband optical excitation. Both interband and intraband transitions are taken into account in the model. It is assumed that the energy of the photogenerated electrons and holes is close to the energy of several optical phonons, so that the photogeneration of electrons and holes followed by the emission of the cascade of optical phonons leads to an essential population of the bottom of the conduction band (by electrons) and the top of the valence band (by holes). We demonstrate that sufficiently strong optical excitation may result in the population inversion in graphene, so that the real part of the net ac conductivity (which is proportional to the absorption coefficient of radiation) can be negative. Due to the gapless energy spectrum, the ac conductivity is negative in the range of terahertz frequencies.
18.2 Equations of the Model
Under optical excitation, electrons and holes are photogenerated with the energy e0 = hW/2. Here hW is the energy of the incident photons. Due to rather short characteristic time, t0, of the optical phonon emission, the photogenerated electrons and holes emit a cascade of optical phonons populating the states with the energies eN = hW/2–Nhw0, where hw0 is the optical phonons, and N = 1, 2, 3, . . . (N £ Nmax). Upon emitting the cascade of optical phonons, the photogenerated electrons and holes are thermalized. The band
Equations of the Model
diagram (corresponding to linear gapless dispersion relations for electrons and holes), the processes under consideration, and the energy distributions of the photogenerated electrons and holes are shown schematically in Fig. 18.1. If the characteristic times of the electronelectron, electronhole, and holehole interactions tee = thh are small compared to the recombination time tR, these interactions result in the Fermi distributions of both electrons and holes. In the optically pumped ungated graphene in which the equilibrium electron and hole concentrations are equal to each other, the Fermi distributions of electrons and holes are characterized by the same Fermi energy eF and the effective temperature T, i.e., fe(e) = fh(e) = f(e), where 1
È Ê e  eF ˆ ˘ f (e ) Í1 + exp Á
˙ .
Ë kBT ˜¯ ˙˚ � ÍÎ
(18.1)
Here e = uFp and eF are the electron (hole) kinetic energy and the Fermi energy, uF is the characteristic velocity of the electron and hole energy spectra (uF ≃ 108 cm/s), p is the absolute value of the electron (hole) momentum, and kB is the Boltzmann constant. In the ungated graphene heterostructures (and gated heterostructures with the gate potential Vg = 0) in the absence of irradiation, eF = 0 and T = T0, where T0 is the lattice temperature. Assuming that W/2–Nmaxw0 w0, where Nmax ≃ W/2w0, i.e., assuming that the energy transferring by the optical radiation to the twodimensional (2D) electronhole system is small, we may disregard the difference between T and T0.
Figure 18.1 Schematic view of graphene band structure and energy distributions of photogenerated electrons and holes. Arrows show the transitions corresponding to optical excitation by photons with energy hW, cascade emission of optical phonons with energy hw0, and radiative recombination with emission of photons with energy hw.
333
334
Negative Dynamic Conductivity of Graphene with Optical Pumping
We shall calculate the real part of the ac conductivity Re sw of a nonequilibrium electronhole system in graphene. The quantity Re sw is proportional to the absorption coefficient of photons with the frequency w. It comprises the contributions of both interband and intraband transitions accompanied by the absorption and emission of photons: Res w = Res w(inter) + Res w(intra) .
(18.2)
Here the contributions of the interband and intraband (the Drudemechanism) transitions into the real part of the ac conductivity of the electronhole system are given, respectively, by (see, for instance, Refs. [12, 16]) Res w(inter) =
= and
e2 È Ê hw ˆ Ê hw ˆ ˘  fh Á Í1  fe ÁË Ë 2 ˜¯ ˙˚ 4h Î 2 ˜¯
Ê hw  2e F ˆ e2 È Ê hw ˆ ˘ e2 tanh Á Í1  2 f ÁË ˙= ˜ ¯ 4h Î 2 ˚ 4h Ë 4kBT ¯˜
Res w(intra) = =
where
e2uFt p h (1 + w t 2
2 2
)Ú
•
0
Ê df ˆ dpp Á  0 ˜ Ë dp ¯
Ê e ˆ FÁ F ˜ , ph (1 + w t ) Ë kBT ¯
F(hF ) =
e2kBTt
2
Ú
•
0
(18.3)
2 2
dxx exp(x  hF ) [1 + exp(x  hF )]2
,
(18.4) (18.5)
and t is the momentum relaxation time of electrons and holes associated with their scattering on impurities and acoustic phonons. In the case of generation of the electronhole pairs by normally incident optical radiation, the normalized electron and hole Fermi energy hF = eF/kBT obeys the following balance equations: R(hF) – R(0) = aWIW,
(18.6)
where R(hF) is the rate of electronhole recombination, aW and IW are the efficiency of the photogeneration of the electronhole pairs and the intensity of incident optical radiation with the photon energies hW. The term in the righthand side of Eq. (18.6) is the rate of the electronhole pair photogeneration
Weak Pumping
(inter) 4p Res W , c hW
aW =
(18.7)
where c is the speed of light and sW is the conductivity of graphene associated with the interband transitions induced by the photons with the frequency W. Considering that for optical photons hW KBT, eF, the real part of the conductivity can be set as [12] (inter) = Res W
Ê �W  2e F ˆ e2 e2 tanh Á � , 4� Ë 4kBT ¯˜ 4�
so that
æW =
pa , hW
(18.8) (18.9)
where a = (e2/ch) ≃ 1 /137.
18.3 Weak Pumping When optical pumping is not strong, one might assume that hF < 1. In this case, introducing the characteristic recombination time tr, determined by the dominant recombination mechanism, the recombination term in the lefthand side of Eq. (18.2) can be presented as R(hF )  R(0)
where
S0 =
1 ph
1Êk Tˆ = Á B ˜ p Ë huF ¯
2
2
Ú
Ú
•
0
•
0
Â0 hF , tR
(18.10)
dpp [1 + exp(vF p / T )] 2
dxx p Êk Tˆ = Á B ˜ , (exp x + 1) 12 Ë huF ¯
(18.11)
is the electron (hole) concentration in the absence of the pumping (i.e., when eF = 0). In this particular case, the electron (hole) concentration S = S0 + DS, where DS ≃ (ln 2/p)(kBT/huF)2hF, so that the term in the righthand side of Eq. (18.10) S0hF/tR ≃ (12 ln 2/p2) DS0/tR. Using Eqs. (18.5) and (18.9), we obtain
335
336
Negative Dynamic Conductivity of Graphene with Optical Pumping
2
hF =
Ê hu ˆ t I t R æW IW = 12a Á F ˜ R W . Â0 Ë kBT ¯ hW
(18.12)
If eF π 0, Eq. (18.8) for hw/2, eF < kBT can be presented in the following form: Res w(inter) �
ˆ e 2 Ê �w  hF ˜ . Á 8� Ë 2kBT ¯
(18.13)
Taking into account that at hF< 1, F(hF) ≃ ln 2 + hF/2, the contribution of the intraband transitions can be estimated as Res w(intra) �
(ln2 + hF /2)e2 p�
(
kBTt
� 1 + w 2t 2
)
.
(18.14)
Considering Eqs. (18.2), (18.13), and (18.14), we arrive at the following equation for the net ac conductivity of the electronhole system under consideration: Res w �
8 ln 2 Ê kBTt /� ˆ e2 ÔÏ �w + Ì 8� ÓÔ 2kBT p ÁË 1 + w 2t 2 ˜¯
È 4 Ê k Tt/� ˆ ˘ ¸Ô  Í1  Á B 2 2 ˜ ˙ hF ˝ , Î p Ë 1 + w t ¯ ˚ ˛Ô
(18.15)
Using Eq. (18.12) in the case kBTt/h < w2t2, Eq. (18.15) can be presented as Res w �
where
gw =
2 Ê �u ˆ t I ˘ e2 ÈÍ gw  12a Á F ˜ R W ˙ , 8� Í Ë kBT ¯ �W ˙ Î ˚
(18.16)
hw 8 ln 2 Ê kBTt/h ˆ . + 2kBT p ËÁ 1+ w 2t 2 ¯˜
(18.17)
Accounting for that function gw exhibits a minimum at w = w , where Ê 32ln 2 ˆ w =Á Ë p ˜¯
1/3
Ê kBTt ˆ ÁË � ˜¯
2/3
1 Ê kBTt ˆ � t ÁË � ˜¯
2/3
1.5 , t
(18.18)
the net ac conductivity near the threshold at which it changes sign can be presented as Res w �
2 I ˘ e2 g È 3 Ê w  w ˆ Í1 + Á  W ˙, ˜ 8� Í 2 Ë w ¯ IW ˙˚ Î
(18.19)
Weak Pumping
where
and
Ê 4 ln 2 ˆ g=Á Ë p ˜¯
IW
1/3
Ê h ˆ ÁË k Tt ¯˜
Ê � ˆ � 11 Á Ë k Tt ¯˜
� ˆ ÁË k Tt ˜¯ B
B
1/3
(18.20)
B
1/3 4 ln 2 / p ) Ê ( =
12a
1/3
1/3
2
Ê kBT ˆ �W ÁË �u ˜¯ t F R
2
Ê kBT ˆ �W ÁË �u ¯˜ t , F R
(18.21)
is the threshold intensity of optical radiation. As follows from Eq. (18.19), Re sw < 0 in the frequency range wmin< w < wmax, where È w max = w Í1 ÍÎ È w max = w Í1 + ÍÎ
˘ 2 IW  1˙ , 3 IW ˙˚ ˘ 2 IW 1˙. 3 IW ˙˚
(18.22)
Figure 18.2 Frequency dependence of normalized ac conductivity at different intensities of optical radiation.
At uF = 108 cm/s, T = 77 K, t = 1 ¥ 10–12 s, hW ≃ 0.8 eV (hW = 4hw0, where the optical phonon energy in graphene is assumed
337
338
Negative Dynamic Conductivity of Graphene with Optical Pumping
to be hw0 = 0.2 eV), and tr =10–7–10–9 s, we obtain w 1.5 THz, g 0.4 , and IW 0.07 ¥ (1–100) W/cm2. If t = 3 ¥ 10–12 s and the same as above other parameters, w 1THz , g 0.3 , and IW 0.05 ¥ (1  100) W/cm2 . Figure 18.2 shows the frequency dependence of the ac conductivity normalized by the characteristic conductivity e2/4h at different intensities of optical radiation. It is assumed that T = 77 K and t = 1 ¥ 10–12 s. One can see that the range of frequencies in which Re sw £ 0 widens when the intensity of incident optical radiation increases beyond its threshold value. Figure 18.3 shows the variation of this range (confined by the frequencies wmax and wmin) with increasing optical intensity calculated for different values of the electron and hole momentum relaxation time t (at T = 77 K). As follows from Fig. 18.3, the graphenebased structures with longer momentum relaxation time exhibit smaller threshold frequency w but slower expansion of the interval (wmax – wmin). This is due to the dependence of both w and IW on t.
Figure 18.3 Maximum (upper branch) and minimum (lower branch) frequency as functions of optical radiation intensity for different values of momentum relaxation time.
Combining Eqs. (18.8) and (18.18), one can obtain Ê 4 ln 2 ˆ hF = Á Ë p ˜¯
1/3
Ê h ˆ ÁË k Tt ¯˜ B
1/3
IW
IW
=g
IW
IW
,
(18.23)
where g = (4 ln 2/p)1/3(h/kBTt)1/3. As follows from Eq. (18.23), the condition when Eqs. (18.10)–(18.22) are valid (hF < 1) can be
Strong Pumping
presented as IW < IW /g. At T = 77 K and t = (1–3) ¥ 10–12 s, g–1 ≃ 2.3 – 3.3. Hence, at elevated intensities of incident optical radiation when IW >IW /g , Eq. (18.10) should be replaced by the more general equation that is valid at hF >1.
18.4 Strong Pumping
Under strong illumination, the electron and hole Fermi energy eF can be relatively large. If W/2–Nmaxw0 w0, the optical radiation absorbed by the electronhole system should not, nevertheless, result in a significant heating of the latter. In this case, hF 1 and Eq. (18.10) is replaced by 2
R(hF )  R(0) =
2
Â 1 Ê kBT ˆ 2 1 Ê eF ˆ � hF = . (18.24) ˜ Á t R 2pt R Ë �uF ¯ 2pt R ËÁ �uF ˜¯
Equations (18.6), (18.9), and (18.24) lead to
2p 2at R IW (18.25) . hW Since at strong optical pumping one may expect that in the terahertz range of frequencies hw < eF, the interband contribution to the ac conductivity in the case under consideration is e F = huF
Res w( inter) =
Ê �w  2e F ˆ e2 e2 tanh Á � . ˜ 4� 4� Ë 4kBT ¯
(18.26)
Simultaneously, taking into account that at hF 1 Eq. (18.5) yields F(hF) ≃ hF, the contribution of the intraband transitions accompanied with the electron and hole scattering on impurities and acoustic phonons can be presented in the following form [compare with Eq. (18.14)]: Res w(intra ) �
te F e2 Ê kBTt/� ˆ e2 = . h F Á ˜ 2 p� Ë 1 + w 2t 2 ¯ p� 1 + w 2t 2
As a result, we arrive at Res w �
(
È tuF e2 Í 1 + Í 4� 1+ w 2t 2 Î
(
)
˘ 32at R IW ˙ . ˙ �W ˚
)
(18.27)
(18.28)
339
340
Negative Dynamic Conductivity of Graphene with Optical Pumping
For w ,w t 1 , Eq. (18.28) can be presented as Res w �
e2 È Ê wˆ Í 1 + x Á ˜ Ë w¯ 4� Í Î
2
IW ˘ ˙, IW ˚˙
(18.29)
where x = p/24 ln2 0.43. Equation (18.29) implies that when the intensity becomes too large, the ac conductivity changes its sign from negative to positive. It occurs when IW > IW /x . This is associated with the saturation of the contribution of the interband transitions [see Eq. (18.24)], while the contribution of the intraband transitions increases with increasing intensity (due to an increase in the electron and hole concentration). This effect is weaker for relatively high frequencies (w w ) . Assuming, for instance, w = w we find that Re sw < 0 when Iw < Iomega < 5IW .
18.5 Conclusions
We developed a model of a nonequilibrium twodimensional electronhole system in optically pumped graphene. The model accounts for the feature of the energy spectrum of electrons and holes and the processes determining the ac conductivity. Using the developed model, we calculated the ac conductivity of graphene under optical excitation followed by emission of a cascade of optical phonons. We demonstrated that at sufficiently strong pumping the population inversion in graphene can lead to the negative net ac conductivity in the terahertz range of frequencies. The main effect determining the low end of the frequency range where the ac conductivity is negative is associated with the intraband transitions electrons and holes due to their scattering on impurities and acoustic phonons (free carrier intraband absorption). The effect of population inversion and negative ac conductivity might be used in graphenebased coherent sources of terahertz electromagnetic radiation utilizing stimulated photon emission. A similar effect can occur in gated graphene structures, for example, in the structures with graphene separated from a highly conducting substrate playing the role of the gate. In these structures, varying the gate voltage one can control the equilibrium concentrations of electrons and holes and, hence, control the ac conductivity and output terahertz radiation. Since a twodimensional electronhole system can serve as a resonant plasma
References
cavity [17, 18], the negative ac conductivity in the terahertz range can also lead to the selfexcitation of plasma waves [12–15] followed by their conversion into electromagnetic radiation. We considered the case of normally incident optical radiation photogenerating electrons and holes. The lateral (waveguide) optical input can also be used for the pumping of graphenebased structures.
Acknowledgment
This work was supported by the GrantinAid for Scientific Research (S) from the JSPS, Japan.
References
1. K. S. Novoselov, A. K. Geim, S. V. Morozov, D. Jiang, M. I. Katsnelson, I. V. Grigorieva, S. V. Dubonos, and A. A. Firsov, Nature, 438, 197 (2005).
2. C. Berger, Z. Song, T. Li, X. Li, A. Y. Ogbazhi, R. Feng, Z. Dai, A. N. Marchenkov, E. H. Conrad, P. N. First, and W. A. de Heer, J. Phys. Chem., 108, 19912 (2004). 3. B. Obradovic, R. Kotlyar, F. Heinz, P. Matagne, T. Rakshit, M. S. Giles, M. A. Stettler, and D. E. Nikonov, Appl. Phys. Lett., 88, 142102 (2006).
4. K. Nomura and A. H. MacDonald, condmat/0606589 (2006). 5. I. L. Aleiner and K. B. Efetov, condmat/0607200 (2006).
6. B. Trauzettel, Ya. M. Blanter, and A. F. Morpurgo, condmat/0606505 (2006). 7. V. P. Gusynin and S. G. Sharapov, Phys. Rev. Lett., 95, 146801 (2005).
8. Y. Zhang, Y.W. Tan, H. Stormer, and P. Kim, Nature, 438, 201 (2005).
9. D. Abanin, P. A. Lee, and L. S. Levitov, Phys. Rev. Lett., 96, 176803 (2006).
10. V. P. Gusynin, S. G. Sharapov, and J. P. Carbotte, Phys. Rev. Lett., 96, 256802 (2006). 11. V. P. Gusynin and S. G. Sharapov, Phys. Rev. B, 73, 245411 (2006).
12. L. A. Falkovsky and A. A. Varlamov, condmat/0606800 (2006). 13. V. Ryzhii, Jpn. J. Appl. Phys., Part 2, 45, L923 (2006).
14. O. Vafek, Phys. Rev. Lett., 97, 266406 (2006).
15. V. Ryzhii, A. Satou, and T. Otsuji, J. Appl. Phys., 101, 024509 (2007). 16. L. A. Falkovsky, Phys. Rev. B, 75, 033409 (2007).
341
342
Negative Dynamic Conductivity of Graphene with Optical Pumping
17. M. Dyakonov and M. Shur, IEEE Trans. Electron. Devices, 43, 1640 (1996).
18. M. S. Shur and V. Ryzhii, Int. J. High Speed Electron. Syst., 13, 575 (2003).
Chapter 19
Population Inversion of Photoexcited Electrons and Holes in Graphene and Its Negative Terahertz Conductivity*
V. Ryzhii,a M. Ryzhii,a and T. Otsujib aComputer Solid State Physics Laboratory, University of Aizu, AizuWakamatsu 9658580, Japan
bResearch Institute of Electrical Communication, Tohoku University,
Sendai 9809577, Japan [email protected]
We demonstrate that sufficiently strong optical excitation may result in the population inversion in graphene, so that the real part of the ac conductivity can be negative in the terahertz range of frequencies. We study also how the heating of the electronhole system influences the effect of negative ac conductivity. The effect of population inversion and negative ac conductivity might be used in graphenebased coherent sources of terahertz electromagnetic radiation.
*Reprinted with permission from V. Ryzhii, M. Ryzhii, and T. Otsuji (2008). Population inversion of photoexcited electrons and holes in graphene and its negative terahertz conductivity, Phys. Status Solidi C, 5(1), 261–264. Copyright © 2008 WILEYVCH Verlag GmbH & Co. KGaA. GrapheneBased Terahertz Electronics and Plasmonics: Detector and Emitter Concepts Edited by Vladimir Mitin, Taiichi Otsuji, and Victor Ryzhii
Copyright © 2021 Jenny Stanford Publishing Pte. Ltd.
ISBN 9789814800754 (Hardcover), 9780429328398 (eBook)
www.jennystanford.com
344
Population Inversion of Photoexcited Electrons and Holes
19.1 Introduction A significant progress in fabrication of graphene, demonstration of its exceptional electronic properties and possibility of creating novel electronic and optoelectronic devices on the basis of graphene heterostructures have attracted widespread attention [1]. The gapless energy spectrum of electrons and holes in graphene (e = ±uF p, where uF ≃ 108 cm/s is the characteristic velocity and p is the momentum) can lead to specific features of its transport, plasma, and optical properties. Due to the gapless energy spectrum of graphene, the Fermi energy eF in equilibrium is equal to zero. Hence, the electron and hole distribution functions at the bottom of the conduction band and the top of the valence band fe(0) = fh(0) = 1/2. This implies that at even weak photoexcitation, the values of the distribution functions at low energies can be fe(e) = fh(e) > 1/2, that corresponds to the population inversion [2]. Such a population inversion might lead to the negative ac conductivity at relatively small frequencies associated with the interband transitions. However, the intraband processes determined the Drude conductivity provide the positive contribution to the ac conductivity. Nevertheless, one might expect that under sufficiently strong optical excitation resulting in photogeneration of electronhole pairs, the population inversion can be achieved. In such a case, lasing of rather longwave (terahertz) radiation in graphene may be possible. In this work, which generalizes our previous paper [2], using the developed model, we study the ac conductivity of a nonequilibrium twodimensional electronhole system in graphene under interband optical excitation. Both interband and intraband transitions are taken into account in the model. It is assumed that the energy of the photogenerated electrons and holes is close to the energy of several optical phonons, so that the photogeneration of electrons and holes followed by emission of the cascade of optical phonons leads to an essential population of the bottom of the conduction band (by electrons) and the top of the valence band (by holes). We show that the ac conductivity can be negative in certain (terahertz) range of frequencies. The heating of the electronhole system by absorbed optical radiation is also considered. It is demonstrated that the role of this heating essentially depends on the ratio of the photon energy and the energy of optical phonons.
Qualitative Pattern
19.2 Qualitative Pattern We consider a graphenebased heterostructure illuminated by light with the photon energy hW, where h is the reduced Planck constant and W is the photon frequency. The illumination results in the photogeneration in graphene of electrons and holes with kinetic energy e0 = hW/2. Due to a very short time of the optical phonon emission t0, the photogeneration of electrons and holes leads to the emission of a cascade of optical phonons, so that the photogenerated electrons and holes occupy the states with the energies close to eN = h(W/2 – Nw0). Here hw0 is the optical phonon energy and N is the number of emitted optical phonons (N £ Nm, where Nm is determined by the integer part of W/2w0). When eNm = h(W/2 – Nmw0) ≃ 0, the photogenerated electrons and holes after the cascade emission of optical phonons are concentrated near the bottom of the graphene conduction band and the top of the graphene valence band, respectively. In this case, the energy distribution of electrons and holes corresponds to that shown schematically in Fig. 19.1. In such a
Figure 19.1 Schematic view of graphene band structure (leftside figure). The arrows show different interband and intraband transitions: transitions associated with absorption of photons with energy hW, emission of terahertz photons with energy hw, interaction with optical and acoustic phonons (with energies hw0 and hwq). Rightside figure shows energy distributions of photogenerated electrons and holes.
case, the processes of the electron and hole photogeneration do hot heat the electronhole system, and one can assume that the effective temperature of the latter T ≃ T0, where T0 is the lattice temperature. However, if eNm is not small, the processes in question can result in a marked heating of the electronhole system (T > T0). Taking into account that in graphene hw0 ≃ 0.2 eV, the first case can occur when
345
346
Population Inversion of Photoexcited Electrons and Holes
the graphene structure is illuminated by a semiconductor laser with the photon energy hW = 0.8 eV (Nm = 2). If the graphene structure is photoexcited by a CO2 laser with the photon energy hW = 0.1 eV (Nm = 0), a significant part of the absorbed optical energy goes to the heating of the electronhole system because the electron and hole energy relaxation on optical phonons is “switched off.”
19.3 Frequency Dependence of the Conductivity
We shall analyze the real part of the ac conductivity Re sw of a nonequilibrium electronhole system in graphene. For this purpose, the general formulae for the ac conductivity of graphene obtained previously are used [2, 3]. The quantity Re sw is proportional to the absorption coefficient of photons with the frequency w. It comprises the contributions of both interband and intraband transitions accompanied by the absorption and emission of photons: Res w = Res winter + Res wintra .
(19.1)
Here the first and the second terms represents the contributions of the interband and intraband (the Drudemechanism) transitions into the real part of the ac conductivity of the electronhole system [2, 3, 5]. The interband contribution can be expressed via the normalized Fermi quasienergy hF = eF/kBT, of the nonequilibrium electron (hole) system, where kB is the Boltzmann constant. In equilibrium, i.e., without optical excitation, hF µ eF = 0. At relatively weak optical excitation when the concentration of photogenerated electrons and holes is small in comparison with their thermal concentration, one may assume that eF < kBT, i.e., hF < 1. In this case, for the frequencies w < 2kBT/h, the interband contribution to the real part of the ac conductivity can be presented in the following form: inter )
Res w(
�
ˆ e2 Ê �w  hF ˜ , Á 8� Ë 2kBT ¯
(19.2)
where e is the electron charge. In equilibrium, when hF = 0, and Eq. (19.2) reduces to that obtained previously [3]. At hF < 1, the contribution of the intraband transitions can be estimated as [4]
Frequency Dependence of the Conductivity
( ln2+ hF /2) e Tt intra ) Res w( . = ph h 1+ w 2t 2 2
(
)
(19.3)
Here t is the momentum relaxation time of electrons and holes. As shown previously [2], at weak optical excitation, 2
hF =
Ê hu ˆ t I t R æW IW = 12a Á F ˜ R W . Â0 Ë kBT ¯ hW
(19.4)
Here æW = pa/ hW is the interband absorption coefficient, S0 = (p/12) (kBT/huF)2 is the equilibrium density of electrons and holes, tr is the recombination time (the lifetime of nonequilibrium electrons and holes), and a = (e2/hc) ≃ 1/137, where c is the speed of light. Using Eqs. (19.1)–(19.4) at kBTt/h w2t2, we arrive at the following equation for the ac conductivity of the electronhole system under consideration: 2 Ê huF ˆ t R IW ˘ e2 ÍÈ ˙. gw  12a Á Res w = 8h Í Ë kBT ¯˜ hW ˙ Î ˚
Here
gw =
hw 8 ln 2 Ê kBTt /h ˆ + . p ÁË 1 + w 2t 2 ¯˜ 2kBT
(19.5)
(19.6)
One can see that gw as a function of w exhibits a minimum at w = w , where Ê 32ln2 ˆ w =Á Ë p ˜¯
1/3
Ê kBTt ˆ ÁË h ˜¯
2/3
1 . t
(19.7)
Considering this, the ac conductivity near the threshold, at which the ac conductivity changes its sign, can be presented as Res w "
where
2 I ˘ e2 g È 3 Ê w  w ˆ Í1 + Á  W ˙, ˜ 8/ Í 2 Ë w ¯ IW ˚˙ Î
Ê 4 ln 2ˆ g=Á Ë p ˜¯ IW
1/3 4 ln 2/p ) Ê ( =
12a
1/3
Ê h ˆ ÁË k Tt ¯˜
1/3
,
B
h ˆ ÁË k Tt ¯˜ B
1/3
(19.8)
2
Ê kBT ˆ hW ÁË hu ˜¯ t F R
(19.9) (19.10)
347
Population Inversion of Photoexcited Electrons and Holes
is the threshold intensity of optical radiation, and
È ˘ 2 IW  1˙, w min = w Í1 3 IW ÍÎ ˙˚
(19.11)
È ˘ 2 IW  1˙, w max = w Í1 + 3 IW ˙˚ ÍÎ
(19.12)
As follows from Eq. (19.8) and seen in Fig. 19.2, Re sw < 0 in the frequency range wmin < w < wmax. Let us set uF = 108 cm/s, T = 77 K, t = 1 ¥ 10–12 s, hW ≃ 0.8 eV (hW = 4hw0, where the optical phonon energy in graphene is assumed to be hw0 = 0.2 eV). The recombination time associated with the emission of acoustic phonons can be roughly estimated as tr ≃ t(uF/s) where s is the speed of sound. Hence, tr ≃ 103 t ≃ 10–9 s. As a result, we 1/3 obtain ( �/kBTt ) � 0.45, w � 1.5 THz, and IW 7 W/cm2 . If t = 3 ¥ 10–12 s, assuming the same as above other parameters, w 1 THz, g 0.3 and IW 1.7 W/cm2 . Figure 19.2 shows the frequency dependence of the ac conductivity normalized by the characteristic conductivity e2/2h at different intensities of optical radiation. It is assumed that T = 77 K and t =1 × 10–12 s. One can see that the range of frequencies in which Resw £ 0 widens when the intensity of incident optical radiation increases beyond its threshold value. 0.15
Real part of ac conductivity
348
0.10
0.05
0.0
ω
ω_
ω+ IΩ / IΩ= 0.5 1.0 1.5
0.05
0.10
0
1
2
3
Frequency, THz
4
5
6
Figure 19.2 Normalized ac conductivity versus frequency for different intensities of optical excitation.
Heating of Electrons and Holes
19.4 Heating of Electrons and Holes As follows from Eqs. (19.7) and (19.10), w and IW depend on the effective temperature of the electronhole system. This leads also to the temperature dependences of wmin and wmax. Let assume that t (T) µ Ts and tR(T) µ Tr, where s and q are some numbers. Therefore w µT (2s)/3 , IW µT (5s)/3r .
(19.13)
Considering the impurity and acoustic phonon scattering mechanisms at kBT hw0, one may set [4] s = 1. The effective temperature of the electronhole system is governed the energy balance equation kB (T  T0 ) Â0 te
=
= h(W/2  Nmw 0 )æW IW
pa Ê W  2Nmw 0 ˆ ˜¯ IW . 2 ÁË W
(19.14)
Here te is the energy relaxation time. If the electron and hole momentum and energy relaxation is associated with acoustic phonons, one can use the following estimate te ≃ t(uF/s) t. At moderate intensities of optical excitation, the effective temperature is close to T0, so that T = T0 + DT, where È pa Ê W  2Nmw 0 ˆ t e IW ˘ DT = Í ˜¯ Â ˙ . Á W 0 ˚ Î 2kB Ë
(19.15)
Considering Eqs. (19.13) and (19.15), one obtains the following formula, which replaces Eq. (19.8): Res w � Here
e2 g È 3 Ê w  w *ˆ Í1 + 8� Í 2 ÁË w * ¯˜ Î
2
Ê W  2Nmw 0 ˆ IW2 ˘ ˙. +Á ¯˜ I I * ˙ W IW Ë W W˚ IW
w* Ê 2  s ˆ Ê W  2Nmw 0 ˆ IW 1+Á ˜¯ * Ë 5  s  3r ¯˜ ÁË w W IW
(19.16) (19.17)
349
350
Population Inversion of Photoexcited Electrons and Holes
and
IW* =
kBT Â0 6 . 5 s pa te 3r ( )
(19.18)
The ratio of the characteristic intensities IW and IW* , as follows from Eqs. (19.10) and (19.18), is given by Ê Wˆ = bÁ ˜ , Ë w0 ¯ IW*
IW
where
Ê � ˆ b ∼Á Ë kBTt ¯˜
1/3
Ê t e ˆ Ê �w 0 ˆ . ËÁ t R ¯˜ ËÁ kBT ¯˜
(19.19)
(19.20)
Thus, the heating of the electronhole system due to optical excitation results in a shift of the frequency corresponding to the minimum of Re sw and in a nonlinear dependence of the latter quantity on the intensity. The first and second factors in the righthand side of Eq. (19.19) are of the order unity. In contrast, the
second factor is rather large. Hence generally b 1, i.e., IW I W* . This implies that if W is sufficiently close to 2Nmw0, the terms associated with the heating can be disregarded. However, when W markedly deviates from 2Nmw0, the role of the nonlinear term in Eq. (19.16) rises drastically. In such a case, the frequency range where Re sw < 0 shrinks and can disappear.
19.5 Discussion
The effect of negative ac conductivity can also occur in gated graphene structures [1, 5], for example, in the structures with graphene separated from a highly conducting substrate playing the role of the gate. In these structures, varying the gate voltage one can control the equilibrium concentrations of electrons and holes and, hence, control the ac conductivity not only in equilibrium but under optical excitation as well. However, an increase in the equilibrium density of electrons (or holes) might lead to a significant increase in the intraband contribution to the ac conductivity, which can prevail the contribution of the interband transitions. If the real part of ac
References
conductivity is negative, it can be used for generating of terahertz radiation. One option is associated with the utilization of the optically pumped graphene as an active region for a terahertz laser provided that the pertinent conditions for effective reflection of the generated terahertz photons are satisfied by proper design of the graphene heterostructure edges. Another option is associated with the selfexcitation of plasma oscillations. This is because a twodimensional electronhole system, in particular in the graphene, can serve as a resonant plasma cavity [5, 6]. The selfexcitation of plasma waves due to the negative ac conductivity in the terahertz range followed by their conversion into electromagnetic radiation can also be used in sources of terahertz radiation.
Acknowledgements
The authors are grateful to Professor F. T. Vas’ko for stimulating comments. One of the authors (V. R.) thanks Professor A. A. Varlamov for numerous discussions. This work was supported by the GrantinAid for Scientific Research (S) from the Japan Society for Promotion of Science, Japan.
References
1. K. S. Novoselov, A. K. Geim, S. V. Morozov, et al., Nature, 438, 197 (2005).
2. V. Ryzhii, M. Ryzhii, and T. Otsuji, J. Appl. Phys., 101, 083114(2007). 3. L. A. Falkovski and A. A. Varlamov, Eur. Phys. J., 56, 281 (2007). 4. L. A. Falkovski, Phys. Rev. B, 75, 033409 (2007).
5. V. Ryzhii, A. Satou, and T. Otsuji, J. Appl. Phys., 101, 024509 (2007).
6. M. S. Shur and V. Ryzhii, Int. J. High Speed Electron. Syst., 13, 575 (2003).
351
Chapter 20
Negative Terahertz Dynamic Conductivity in Electrically Induced Lateral pin Junction in Graphene*
V. Ryzhii,a M. Ryzhii,a M. S. Shur,b and V. Mitinc aComputational
Nanoelectronics Laboratory, University of Aizu,
AizuWakamatsu 9658580, and Japan Science and Technology Agency,
CREST, Tokyo 1070075, Japan
bDepartment of Electrical, Electronics, and Systems Engineering,
Rensselaer Polytechnic Institute, Troy 12180, USA
cDepartment of Electrical Engineering, University at Buffalo,
Buffalo 14260, USA
[email protected]
We analyze a graphene tunneling transittime device based on a heterostructure with a lateral pin junction electrically induced in the graphene layer and calculate its ac characteristics. Using the developed device model, it is shown that the ballistic transit *Reprinted with permission from V. Ryzhii, M. Ryzhii, M. S. Shur, and V. Mitin (2010). Negative terahertz dynamic conductivity in electrically induced lateral pin junction in graphene, Physica E, 42, 719–721. Copyright © 2009 Elsevier B.V. GrapheneBased Terahertz Electronics and Plasmonics: Detector and Emitter Concepts Edited by Vladimir Mitin, Taiichi Otsuji, and Victor Ryzhii
Copyright © 2021 Jenny Stanford Publishing Pte. Ltd.
ISBN 9789814800754 (Hardcover), 9780429328398 (eBook)
www.jennystanford.com
354
Negative Terahertz Dynamic Conductivity in Electrically
of electrons and holes generated due to interband tunneling in the isection results in the negative ac conductance in the terahertz frequency range. The device can serve as an active element of terahertz oscillators.
20.1 Introduction
Theoretical predictions and experimental observations of unique properties of graphenebased structures, in particular, the possibility of ballistic electron and hole transport in fairly large samples at room temperatures (see, for instance, Refs. [1–3]) stimulate proposals of novel graphene electron and optoelectron devices. In this chapter, we consider a tunneling transittime device based on a gated graphene with electrically induced lateral pin junction and present the device dynamic characteristics, the frequency dependences of the real and imaginary parts of the ac conductance, calculated using the developed device model. In the graphene tunneling transittime (GTUNNETT) device under consideration, the depleted isection of the graphene layer play the role of both the tunneling injector and the transit region at the same time. Extending the device model used by us recently [4] (mainly by the inclusion into the consideration of the nonuniformity of the electric field in the isection and the possibility of the selfexcitation of plasma oscillations in the gated p and nsections), we show that the GTUNNETT can exhibit negative ac conductance in the terahertz (THz) range of frequencies and, hence, serve as an active element in THz oscillators.
20.2 Device Model and Terminal AC Conductance
The GTUNNETT structure under consideration is shown schematically in Fig. 20.1a. It is assumed that the gatesource voltage (Vp < 0) and the draingate voltage (Vn > 0) are applied. This results in creating the hole and electron twodimensional systems (with the Fermi energy eF), i.e., the p and nregions in the channel sections under the pertinent gates. Under the reverse sourcedrain voltage
Device Model and Terminal AC Conductance
(V > 0), a lateral pin junction is formed, which corresponds to the band diagram shown in Fig. 20.1b. It is assumed that apart from a dc component V0 > 0 which corresponds to a reverse bias, the net sourcedrain voltage V comprises also an ac component dVexp(–iwt): V = V0 + dVwexp(–iwt), where dVw and w are the signal amplitude and frequency, respectively.
Figure 20.1 Structure of a GTUNNETT device (a) and its band diagram under the reverse bias (b). Arrows with wavy tail indicate the directions of propagation of the generated electrons and holes generated due to interband tunneling.
The probability of interband tunneling in graphene is a fairly sharp function of the angle between the direction of the electron (hole) motion and the xdirection (from the source to the drain) [5]. Taking this into account, we disregard some spread in the xcomponent of the velocity of the injected electrons and assume that all the generated electrons and holes propagate in the xdirection with the velocity vx ≃ vW, where vW ≃ 108 cm/s is the characteristic velocity of the electron and hole spectra in graphene. Considering the formula for the interband tunneling probability [5], we assume that the rate of the local tunneling generation of electron hole pairs G/2l µ E3/2, where 2l is the length of the depleted isection and E is the electric field in the isection. In the structures with the spacing between the top gates D Wt, ls, where Wt is the thickness of the
355
356
Negative Terahertz Dynamic Conductivity in Electrically
layers separating the graphene layer and the gates and ls is the characteristic screening lengths, one can assume 2l ≃ D (as for the problem of screening in twodimensional electron and hole systems, see, for instance, Refs. [6, 7]). One can expect that this is valid when the dc conductivity of the p and nsections is much higher than the dc conductivity of the intrinsic graphene. Actually, the length of the depleted highelectric field isection 2l depends also on V0. However, we disregard this effect. In the case of ballistic electron and hole transport in the isection when the generated electrons and holes do not change the directions of their propagation, the continuity equations governing the ac components of the electrons and holes densities d Âw and d Âw+ can be presented as iwd Âw ±vW
dd Âw 3G0 dVw = . dx 4l V0
(20.1)
Here G0 = G0(x) and dGw are the dc and ac components of the local tunneling rate, respectively. The boundary conditions are as follows: d Âw x= l = 0. We shall consider Eq. (20.1) in the following two limiting cases: (a) the nonuniformity of the electric field in the isection is insignificant, so that the components of the latter can be estimated as E0 ≃ V0/2l and dEw ≃ dVw/2l, and (b) the electric field exhibits strong maxima near the edges of the n and psections. In the former case, the tunneling generation of electrons and holes takes place in the whole isection, whereas in the latter case, the electrons and holes are primarily generated at the points x ≲ l. Solving Eq. (20.1) in the case “a” and using the Shockley–Ramo theorem for the induced current, the real and imaginary parts of the ac (dynamic) component of the sourcedrain (terminal) conductance s wsd = d Jwsd /d Vw can be presented as Res wsd =
Ims wsd =
3s 0 sin( wt ) J 0 (wt ), 2 wt
˘ 3s 0 È 1 cos( wt ) J 0 ( wt )  cwt ˙ . Í 2 ÎÍ wt ˚˙
(20.2)
(20.3)
Here s0 = J0/V0 is the dc conductance, J0 is the dc current, c = 2C/3s0t, C is the lateral pin junction capacitance, J0(x) is the Bessel function, and t = l/vW is the characteristic transit time of electrons and holes
Device Model and Terminal AC Conductance
across the isection. In the case “b,” instead of Eq. (20.3), we arrive at Res wsd =
Ims wsd =
3s 0 cos( wt ) J 0 ( wt ) , 2
(20.4)
3s 0 [sin(wt )J 0 (wt )  cwt ]. 2
(20.5)
Re σωsd/σ0
0.75 0.5 0.25 0 1
2
3
4
1
2
3
4
Re σωsd/σ0
0.75 0.5 0.25 0 0.25 Signal frequency, THz
Figure 20.2 Real part of the ac conductance s wsd versus the signal frequency f = w/2p calculated for uniform (a) and strongly nonuniform (b) electricfield spatial distributions in the isection for different lengths of isection: solid lines correspond to 2l = 0.5 mm (t = 0.25 ps) and dashed lines correspond to 2l = 0.7 mm (t = 0.35 ps).
Figure 20.2 shows the real part of the ac conductance s wsd (normalized by its ac value) as a function of the signal frequency f = w/2p calculated for GTUNNETTs with 2l = 0.5 and 0.7 mm (this corresponds to t = 0.25 and 0.35 ps, respectively) and using Eqs. (20.2) and (20.4). As seen, the real part of the ac conductance exhibits a pronounced oscillatory behavior with the frequency ranges where it has different signs. The real part of the ac conductance can be negative in the THz range of frequencies in the GTUNNETT structures with the isection length only moderately smaller than 1 mm. As follows from Eq. (20.2) and Fig. 20.2 in the case “a,” the relative value of the real part of the ac conductance, corresponding
357
358
Negative Terahertz Dynamic Conductivity in Electrically
to the first minima, for l = 0.25 mm is Res wsd=2p f1 /s 0 0.034 at the
frequency w/2p = f1 ≃ 1.75 THz and Res wsd=2p f1 /s 0 0.141 at the frequency w/2p = f1 ≃ 1.25 THz in the case “b,” respectively. At V0 = 0.2 V, one can obtain s0 ≃ 3 ¥ 1012 s–1 and Res wsd=2p f1 1 ¥ 1011 s1 . In the case “b,” Eq. (20.4) (see also Fig. 20.2) for the same parameters and the same dc current yields f1 ≃ 1.25 THz, Res wsd=2p f1 /s 0 0.141, and Res wsd=2p f1 4 ¥ 1011 s1 . A significant difference in the absolute
values of Res wsd=2p f1 /s 0 in the limiting cases under consideration is associated with the following. In the case “a,” there is a marked spread Dttr in the transit times of electrons and holes generated at a different points of the isection: Dt tr( ) t . However, in the case “b,” b Dt tr( ) t , so that the oscillations of Re sw are more pronounced. Smaller value of f1 in the case “b” is due a longer average transit time: b a t ( ) 2t , while t ( ) t . tr
tr
20.3 SelfExcitation of Plasma Oscillations
The fundamental plasma frequency in the gated p and nsections, in which the spectrum of the plasma waves is a soundlike with the characteristic velocity s and the characteristic plasma frequency W = ps/2(L–l). At sufficiently high gate voltages when the electron (hole) Fermi energy in the nsection (psection)
e F = (�vw /2 2) æVt /eWt � kBT , one obtains s � 2e2 Wt e F /æ�2 > vW [8], where 2L is the spacing between the source and drain contacts, T is the temperature, and kB is the Boltzmann constant. Since the plasma frequency in graphene can be rather large (owing to a large s), the condition w < W assumed above can be easily fulfilled for the signal frequencies in the THz range (as well as the condition w ≃ W) by a proper choice of the device structure length 2L and the gate voltage Vt. Indeed, setting, for example, s = 8 ¥ 108 cm/s, and L–l = 1 mm, one can obtain W/2p = 4 THz. If the frequencies f1, f2, . . ., which corresp6ond to the pertinent minimum in the Re sw versus w dependence, are far from the resonant plasma frequency W/2p, the quasineutral p and nsections serve as the highly conducting contacts. However, when f1 ~ W/2p (or f2 ~ W/2p), i.e., when the frequency of the plasma oscillations falls into
SelfExcitation of Plasma Oscillations
the range where Res wsd < 0 , the hole and electron systems in the gated p and nsections, respectively, can play the role of the plasma resonators [9]. In this situation, the selfexcitation of the plasma oscillations (plasma instability) can be possible [10]. Indeed, taking into account that the Drude conductance of the gated p and nsections is equal to s wD = s 0D [i/(w + in )t ], where s 0D = (e2 pF /p h2 )[l/( L  l )] is the characteristic Drude dc conductance of the gated graphene section with the Fermi momentum pF and n is the frequency of hole and electron collisions with defects and acoustic phonons, one can arrive at the following dispersion equation for the plasma oscillations in the gated p and nsections with the frequency w: È p w (w + in ) ˘ w ˙ = iRF(wt), cot Í Í ˙ w + in 2W Î ˚
(20.6)
where R = s 0 /s 0D =(6h2s0/e2pF)[(L–l)/l], F(wt) = sin(wt)J0(wt), and F(wt) = (wt)cos(wt)J0(wt) in the cases “a” and “b,” respectively. Using the expression for the dc tunneling current [4], R can be expressed via the dc sourcedrain voltage V0 and the electron and hole density in the gated sections S0 as R = (3/2)3/2 p 3 (eV0 /vW lÂ0 h )[( L  l )/l ] (since it is assumed that the dc voltage drops primarily across the depleted isection, the R 1). Assuming that S0 = 5 ¥ 1011 cm–2, l = 0.25 mm, L–l = 2.35 mm, (for s = 6 ¥ 108 cm/s, this corresponds to f = 1.25 THz) and V0 = 0.2–0.8 V, one obtains R ≃ 0.16–0.32. Here we have neglected the contribution of electrons and holes in the isection to its capacitance as well as the geometrical capacitance of this section, which are small in comparison with the gated p and nsections capacitance. When W n (i.e., Q = 4W/pn 1), Eq. (20.7) yields Re w ≃ (2n–1)W, where n = 1, 2, 3, . . . is the plasma mode index. Simultaneously, from Eq. (20.6) we obtain the following expressions for the damping/growth rate g = Im w of plasma oscillations (with n = 1): g = –n/2RWF(Wt)p for the oscillations with the asymmetrical distribution of the ac potential djw corresponding to the upper curve in Fig. 20.3 with the inplane ac electric field in the isection (–l < x < l) dEw 0 (the phases of oscillation in the p and nsections are opposite), and g ≃ –n/2 for the oscillations (damped) with the symmetrical distributions of the ac potential (see the lower curve in Fig. 20.3) and dEw = 0. Using this, we arrive at the following condition
359
360
Negative Terahertz Dynamic Conductivity in Electrically
of the plasma oscillations selfexcitation: Q > 2[RminF(Wt)]–1. As follows from the latter inequality, the selfexcitation of plasma oscillations (plasma instability) can occur if their quality factor Q is sufficiently large. Setting minF(Wt) = 0.28, and R = 0.16–0.32, we obtain that Q should be fairly large: Q > 25–50. The latter requires n ≲ (1–2) ¥ 1011 s–1. As a result, the selfexcitation of the plasma oscillations in the GTUNNETTs under consideration is possible only in sufficiently perfect graphene layers.
Figure 20.3 Qualitative view of spatial distributions of the ac potential for asymmetrical and symmetrical modes.
20.4 Conclusions We demonstrated that the GTUNNETT under consideration can exhibit the negative terminal dynamic conductivity in the THz range of frequencies due to the tunneling and transittime effects in its isection. Owing to this, GTUNNETTs can be used in THz oscillators with a complementary resonant cavity. The generation of THz radiation is also possible due to the selfexcitation of the plasma oscillations in the device p and nsections.
Acknowledgments
The authors are grateful to Professors T. Otsuji and M. Asada for stimulating discussions. The work was supported by the Japan Science and Technology Agency, CREST and the Japan Society for Promotion of Science, Japan, as well by the Airforce Office of Scientific Research, USA.
References
References 1. C. Berger, Z. Song, T. Li, X. Li, A. Y. Ogbazhi, R. Feng, Z. Dai, A. N. Marchenkov, E. H. Conrad, P. N. First, and W. A. de Heer, J. Phys. Chem., 108, 19912 (2004).
2. S. V. Morozov, K. S. Novoselov, M. I. Katsnelson, F. Schedin, D. C. Elias, J. A. Jaszczak, and A. K. Geim, Phys. Rev. Lett., 100, 016602 (2008).
3. X. Du, I. Skachko, A. Barker, and E. Y. Andrei, Nat. Nanotechnol., 3, 491 (2008). 4. V. Ryzhii, M. Ryzhii, V. Mitin, and M. S. Shur, Appl. Phys. Express, 2, 034503 (2009).
5. V. V. Cheianov and V. I. Fal’ko, Phys. Rev. B, 74, 041403 (R) (2006).
6. V. Ryzhii, M. Ryzhii, and T. Otsuji, Phys. Status Solidi A, 205, 1527 (2008).
7. L. M. Zhang and M. M. Fogler, Phys. Rev. Lett., 100, 116804 (2008).
8. V. Ryzhii, A. Satou, and T. Otsuji, J. Appl. Phys., 101, 024509 (2007).
9. M. Dyakonov and M. Shur, IEEE Trans. Electron. Devices, 43, 1640 (1996).
10. V. Ryzhii, A. Satou, and M. Shur, Phys. Status Solidi A, 202, R113 (2005).
361
Chapter 21
Threshold of Terahertz Population Inversion and Negative Dynamic Conductivity in Graphene Under Pulse Photoexcitation*
A. Satou, V. Ryzhii, Y. Kurita, and T. Otsuji Research Institute of Electrical Communication, Tohoku University, 211 Katahira, Aobaku, Sendai 9808577, Japan [email protected]
We present a theoretical study of population inversion and negative dynamic conductivity in intrinsic graphene in the terahertz (THz) frequency range upon pulse photoexcitation at near/midinfrared wavelengths. The threshold pulse fluence required for population inversion and negative dynamic conductivity can be orders of magnitude lower when the pulse photon energy is lower, because of *Reprinted with permission from A. Satou, V. Ryzhii, Y. Kurita, and T. Otsuji (2013). Threshold of terahertz population inversion and negative dynamic conductivity in graphene under pulse photoexcitation, J. Appl. Phys., 113, 143108. Copyright © 2013 AIP Publishing LLC. GrapheneBased Terahertz Electronics and Plasmonics: Detector and Emitter Concepts Edited by Vladimir Mitin, Taiichi Otsuji, and Victor Ryzhii
Copyright © 2021 Jenny Stanford Publishing Pte. Ltd.
ISBN 9789814800754 (Hardcover), 9780429328398 (eBook)
www.jennystanford.com
364
Threshold of Terahertz Population Inversion
the inverse proportionality of the photoexcited carrier concentration to the pulse photon energy and because of the weaker carrier heating. We also investigate the dependence of dynamic conductivity on momentum relaxation time. Negative dynamic conductivity takes place either in high or lowquality graphene, where Drude absorption by carriers in the THz frequency is weak.
21.1 Introduction
Graphene has attracted much attention for a wide variety of devices, owning to its exceptional electronic and optical properties [1–3]. In particular, THz devices such as lasers [4–9] and photodetectors [10–12] which take advantage of the high carrier mobility and gapless dispersion of graphene have been investigated [13]. We have demonstrated that population inversion can occur in optically pumped graphene in the THz/farinfrared range of frequencies; hence lasing in this range is possible, utilizing the gapless linear energy spectrum and relatively high optical phonon (OP) energy in graphene [4–8]. Due to the energy spectrum e = ±uFhk, where uF ≃ 108 cm/s is the Fermi velocity and k is the wavenumber, the Fermi energy eF at equilibrium in intrinsic graphene is equal to zero. Hence, the electron and hole distribution functions at the bottom of the conduction band and the top of the valence band have values of fe(0) = fh(0) = 1/2. This implies that upon photoexcitation, the values of the distribution functions at low energies can be greater than one half, fe(e) = fh(e) > 1/2, corresponding to the population inversion. This type of population inversion means that the total dynamic conductivity in graphene at THz/farinfrared frequencies is negative, and that lasing in graphene at these frequencies is possible. Recently, we measured the carrier relaxation and recombination dynamics in optically pumped epitaxial graphene on silicon [14] and in exfoliated graphene [15] by THz timedomain spectroscopy based on an optical pump/THz & optical probe technique, and we observed the amplification of THz radiation by stimulated emission from graphene under pulse excitation. To our knowledge, those are the first observation of THz amplification using optically pumped graphene, and they demonstrate the possibility of realizing THz lasers based on graphene.
Formulation of the Model
The carrier dynamics in optically pumped graphene strongly depend on the initial temperature of carriers and the intensity of the optical pumping. For sufficiently low carrier concentrations, that is, at low temperatures under weak pumping, photoexcited carriers accumulate effectively near the Dirac point via the cascade emission of OPs. It is predicted that population inversion can be achieved efficiently under these conditions [4, 5, 8]. In contrast, at room temperature or under stronger pumping, where the carrier concentration is high (~1012 cm–2), carriercarrier (CC) scattering plays a crucial role in the dynamics after pulse excitation, because of the fast quasiequilibration of the carriers. Ultrafast optical pumpprobe spectroscopy on graphene has indicated that the quasiequilibration by CC scattering occurs on a time scale of 10 – 100 fs [16–19], which is much faster than a single OP emission. In this case, the pulse excitation makes carriers initially very hot initially, and the energy relaxation and recombination via OP emission follow. The short time scale for the quasiequilibration is partly caused by the ineffective dielectric screening of the Coulomb potential by relatively low dielectric layers surrounding graphene, which is typically supported by a SiC or SiO2 substrate and exposed to air. We have previously shown that population inversion and negative dynamic conductivity in intrinsic graphene at room temperature under pulse excitation with a photon energy of 0.8 eV, which corresponds to a wavelength of 1.55 mm, can be achieved with a pulse energy fluence above a certain threshold [7, 20]. In the present chapter, we investigate the dependence on the pulse photon energy of the threshold pulse fluence for THz negative dynamic conductivity, by extending our previous model to take into account the effect of the Pauli blocking [7, 20]. We also examine the dependence of dynamic conductivity on momentum relaxation time, t. We consider the two limiting cases where wt ≥ 1, which correspond to highquality graphene, and where wt 1, which corresponds to lowquality graphene.
21.2 Formulation of the Model
Assuming a quasiFermi distribution of carriers due to quasiequilibration through CC scattering, such that fe = {1 + exp[(e –
365
366
Threshold of Terahertz Population Inversion
eF)/kBTc]}–1, the time evolution of the distribution is represented by the quasiFermi level, eF(t), and the carrier temperature, Tc(t). In intrinsic graphene, both the electron distribution and the hole distribution can be expressed by a single carrier distribution; the symmetric dispersion of electrons and holes in the energy range under consideration, e < 1 eV, means that the distributions remain identical even under the pulse excitation. The rate equations that governs the quasiFermi level and carrier temperature can be obtained from the quasiclassical Boltzmann equation [7, 20, 21] dn 2 = dt p i = G ,K
ÂÚ
•
0
(
)
È 1  f fe f hw i e hw i  e (1  f e ) kdk Í + ) ( ( ) Í t i,inter t i,inte i r Î
(
)
(
˘ ˙, ˙ ˚
Ï È f 1 f fe 1  fe hw i e e +hw i Ô kdk Ìhw i Í ( ) (+ ) Í 0 t i,intra Ô Î t i,intra Ó È 1 f fe f hw i  e ˘ Ô¸ hw i  e (1  fe ) ˙˝ , + e Í ( ) (+ ) Í t i,inter ˙˚ Ô t i,inter Î ˛
de 2 = dt p i =G ,K
ÂÚ
(
•
)
) ˘˙
(21.1)
˙ ˚ (21.2)
where n = n(eF, Tc) and e = e(eF,, Tc) are the concentration and energy density of either type of carriers, which are obtained by integrating the distribution function multiplied by proper factors over k. The index i includes the longwavelength GOP and shortwavelength KOP, which result in intravalley and intervalley transitions, (± ) (± ) respectively; t i,intra and t i,inter , which are the intraband and interband scattering rates for OPs, where (+) indicates absorption and (–) indicates emission. All the possible transitions via OP (± ) scattering are illustrated in Fig. 21.1a. The expression for t i,intra and (± ) t i,inter have been reported by Suzuura and Ando [22]. Figure 21.1b shows that these rates are on the order of subpicoseconds for highenergy carriers. The first term (intraband transition) in Eq. (21.2) in the curly brackets contains the factor hwi, whereas the second term (interband transition) contains e. These terms describe the energy that a carrier loses or acquires during their transitions. The energy conservation for the latter transition is implicitly satisfied because the rest of the OP energy, hwi – e, is taken into account in the same equation for the
Formulation of the Model
other kind of carrier. Here, we assume the OPs are at equilibrium and neglect the nonequilibrium OP population, because of their emission via OP scattering of carriers. The effects of the nonequilibrium OP population have been discussed elsewhere [8].
Figure 21.1 (a) Schematic view of the intra/interband, intra/intervalley transitions via OP scattering and (b) their rates for OP emission. Note that the rates for OP absorption can be neglected compared with those for the emission because of the negligible OP occupation number at room temperature.
Equations (21.1) and (21.2) and the initial conditions form a nonlinear system of equations for eF(t) and Tc(t), which can be solved numerically. Equations (21.1) and (21.2) are accompanied by the initial carrier concentration and energy density from which the initial quasiFermi level and carrier temperature can be found n
t =0 = n0
+ Dn, e t =0 = e0 + De ,
(21.3)
where n0 and e0 are the intrinsic carrier concentration and energy density, and Dn and De are the contributions of photogenerated carriers. These are equal to the concentration and energy density generated by pumping Dn �
paDJ
(1  2 f Œ�W
�W/2 t =0
Dn, ) , De � �W 2
(21.4)
367
368
Threshold of Terahertz Population Inversion
where a ~ 1/137, Œ is the dielectric constant surrounding graphene, hW is the pulse photon energy, and DJ is the pulse fluence. In Eq. (21.4), the last factor 1 – 2fhW/2 roughly takes into account the Pauli blocking of photoabsorption, and its distribution function is approximated by the quasiFermi distribution after the photoabsorption by eFt=0 and Tct=0, calculated selfconsistently from Eqs. (21.3) and (21.4). This approximation underestimates the effect of Pauli blocking by the nonequilibrium photogenerated carriers when the pulse is so intense that the rate of the photogeneration is comparable to that of the quasiequilibration by the CC scattering. However, it overestimates the effect of the timedependent increase in the distribution function during pulse excitation, which partly compensates for the underestimation. In addition, we assume the pulse has sufficiently narrow such that OP scattering is not effective (+ ) (+ ) during the pulse absorption: Dt t i,inter ( hW/2) ,t i,intra ( hW/2) . To study not only the gain acquired from the population inversion but also the net gain, including the loss from Drude absorption of electromagnetic waves by carriers in graphene, we introduce the real part of dynamic conductivity [23] because it is related to the net gain Res w �
2e2uF2 e2 1  2 f �w /2 + p 4�
(
)
Ú
•
0
dkk
t
1 + (wt )
2
Ê dfe ˆ ÁË  de ˜¯ ,
(21.5)
where t is the momentum relaxation time. The first term in Eq. (21.5) corresponds to the interband contribution, which depends on only frequency through the distribution function and can be negative when the rate of stimulated emission exceeds the rate of absorption during the population inversion. Because the distribution functions the quasiFermi distribution, the condition of the population inversion for photon energy hw is represented as eF > hw/2. However, the second term corresponds to the intraband contribution (Drude conductivity) which is always positive in this system. When the real part of dynamic conductivity becomes negative at a particular frequency, the electromagnetic wave at that frequency passing through optically pumped graphene is amplified and graphene acts as a gain medium. Equation (21.5) shows that the largest achievable negative value of the conductivity is –e2/4h, which corresponds to the amplification of 2.3 / Œ % of the incoming electromagnetic wave.
(
)
Results and Discussion
21.3 Results and Discussion 21.3.1 Time Evolution of QuasiFermi Level and Carrier Temperature We use our model to investigate population inversion and timedependent dynamic conductivity in intrinsic graphene at room temperature after pulse excitation. We varied the pulse photon energy, hW, between 0.1 and 0.8 eV, corresponding to infrared wavelengths of 12.4–1.55 mm. In addition, Œ = 5. 5, which corresponds to the effective dielectric constant of the interface between the air and SiC. We use pulse fluence rather than pulse intensity as a measure of pulse strength because the former does not depend explicitly on the pulse photon energy, whereas the latter does, through the pulse width. Figure 21.2 shows the time evolution of the quasiFermi level and carrier temperature after the pulse excitation for different pulse fluences and pulse photon energies. Population inversion at THz frequencies of up to ~10 THz, which corresponds to hw/2 ~ 20 meV, is achieved at certain threshold pulse fluences, and it lasts for around 10 ps. The mechanism of population inversion in the THz range is explained as follows. Shortly after pulse excitation, the carrier temperature rapidly increases, except for excitation with lowenergy photons, and the quasiFermi level can even be negative because of the quasiequilibration of carriers at very high temperatures induced by the photogenerated carriers. After several picoseconds, the highenergy carriers relax through intraband OP emission and accumulate in the lowenergy region, which is shown by the increase in the quasiFermi level. Satou et al. reported that population inversion lasts for around 10 ps due to the imbalance between the time scales of intra and interband OP emission [20]. Figures 21.2a–d show that the threshold fluence of population inversion decreases as the pulse photon energy decreases. This is also visible in Fig. 21.3, which illustrates the dependence of the threshold fluence for population inversion on the pulse photon energy for different THz photon frequencies. There are several factors which contribute to this decrease. First, a lower fluence is required for the lower photon energy pulse to have the same carrier concentration; more precisely, Eq. (21.4) shows that DJ µ hW. Second, the less
369
370
Threshold of Terahertz Population Inversion
heating of the carriers reduces the carrier temperature, resulting in the carriers accumulating in the lowenergy region (even the cooling can occur as shown in Fig. 21.2d; see below for more details). Third, recombination which arises from interband OP emission is suppressed by the lower carrier temperature. These factors result in the nonlinear lowering of the threshold as pulse photon energy decreases; Fig. 21.3 shows an almost linear dependence of the threshold in the highenergy photon region, caused by the first factor, and the sharp drop in the region of photon energy below 0.25 eV, caused by the second and third factors.
Figure 21.2 The time evolution of the quasiFermi level and carrier temperature for different pulse fluences and pulse photon energies. (a) hW = 0.8 eV, (b) 0.4 eV, (c) 0.2 eV, (d) 0.1 eV. Room temperature (300 K) is indicated by the thin solid lines.
Results and Discussion
The effect of Pauli blocking depends strongly on the pulse photon energy. For hW = 0.8 eV, the changes in the quasiFermi level and the carrier temperature are negligible for the pulse fluences when Pauli blocking is taken into account. In contrast, for hW = 0.1 eV, the threshold fluence is 1.3 to 1.8fold larger depending on the frequency, and the quasiFermi level that can be achieved is also smaller.
Figure 21.3 Dependence of threshold fluence for population inversion on pulse photon energy for different THz photon frequencies. Inset shows the same dependence but with a linear scale.
As has been discussed in Refs. [5, 8], the cooling for low pulse photon energies occurs because the initial photoexcitation can give a lower energy to the carriers than at thermal equilibrium. In fact, the energy of the photogenerated carriers, hW/2, is lower than the average energy of the carriers in intrinsic graphene at room temperature, e/n ª 0.0567 eV, when hW < 0.13 eV. Furthermore, a small amount of cooling after the heating caused by the photoexcitation can also occur (Figs. 21.2a–c). This arises from the discrete nature of the OP emission and absorption which means the carrier temperature cannot exactly match the lattice temperature. The lattice temperature must be reached via acoustic phonon scattering or radiative generation/recombination on a substantially longer time scale.
371
372
Threshold of Terahertz Population Inversion
21.3.2 Time Evolution of Dynamic Conductivity for High and LowQuality Graphene Dynamic conductivity in Eq. (21.5) depends primarily on the carrier distribution, i.e., on the carrier concentration, and also on the momentum relaxation time, t. Because photoexcitation leads to population inversion and also to higher carrier concentration, the negative dynamic conductivity arises if the increase in the absolute value of interband conductivity overcomes the increase in Drude absorption in Eq. (21.5). To achieve a low threshold for negative dynamic conductivity in the THz range, it is necessary to suppress the Drude absorption. This can be done by using either highquality graphene, where wt ≥ 1, or lowquality graphene, where wt 1. As can be seen in Eq. (21.5), in highquality graphene, the highfrequency cutoff of the Drude conductivity occurs. In lowquality graphene, the Drude conductivity ceases over the entire frequency range. Figure 21.4 shows the time evolution of normalized dynamic conductivity, Re sw/(e2/4h), in the THz range with different pulse photon energies and momentum relaxation times. The pulse fluence for each pulse photon energy was chosen so that sufficiently large negative dynamic conductivity is obtained. It demonstrates that the negative dynamic conductivity can be achieved in the THz range with sufficiently high pulse fluence, and that the same level of negative dynamic conductivity can be achieved with a much lower pulse fluence for lower pulse photon energies. Furthermore, the magnitude, frequency range, and time duration of negative dynamic conductivity depend strongly on the momentum relaxation time. For t = 10 ps, negative dynamic conductivity occurs from 1 to greater than 10 THz, and it duration is 5–30 ps, depending on the frequency. The duration is longer for lower frequencies, as a result of the relaxation of the quasiFermi level shown in Fig. 21.2. For t = 1 ps, negative dynamic conductivity occurs between 4 and 10 THz with a smaller magnitude and a much shorter duration. This indicates that the highquality graphene with a longer momentum relaxation time is preferable. Figure 21.4 shows that the minimum frequency for negative dynamic conductivity is primarily determined by the momentum relaxation time, although it is slightly reduced for lower pulse photon energies.
Results and Discussion
Figure 21.4 Timeevolution of dynamic conductivity in the THz range normalized to e2/4h and cut off above zero. Columns from left to right correspond to hW = 0.8, 0.4, 0.2, and 0.1 eV and DJ = 9 ¥ 103, 6 ¥ 103, 1 ¥ 103, and 1 ¥ 102 nJ/cm2, respectively. Rows from top to bottom correspond to t = 10 ps, 1 ps, and 1 fs, respectively.
In contrast, for t = 1 fs, negative dynamic conductivity occurs in the low frequency region, below 6 THz. However, that the meaning of the “timedependent dynamic conductivity” is valid only if its variation is slower than the frequency under consideration, which is above several hundred GHz in this study. This means the negative dynamic conductivity can be achieved as low as several hundred GHz. The upper limit of the frequency range for this negative dynamic conductivity is lower than for the case where wt 1. This is because the Drude conductivity is almost constant in the THz range, whereas it vanishes due to the highfrequency cutoff for wt 1. Our calculation show that even for hW = 0.1 eV the threshold momentum relaxation time of negative dynamic conductivity is t = 5 fs. Above this, dynamic conductivity does not occur in the THz range, regardless of how large the pulse fluence is. This threshold roughly corresponds to the value at which the Drude term in Eq. (21.5) at the zerofrequency limit exceeds the largest negative value of the interband contribution, t ~(p/8 log2)(h/kBTl). Figure 21.5 shows the maximum negative value of dynamic conductivity over its duration as a function of frequency and pulse fluence for different pulse photon energies and momentum relaxation
373
374
Threshold of Terahertz Population Inversion
times. It shows that the threshold pulse fluence and the pulse fluence required to obtain the same negative dynamic conductivity are decreased by several orders of magnitude for any frequency as the pulse photon energy is decreased. Comparing the cases where t = 10 and 1 ps, it is seen that the decrease in the momentum relaxation time causes a large increase in the minimum frequency for the negative dynamic conductivity and an increase in the threshold pulse fluence for frequencies near the minimum. However, this is insignificant for frequencies sufficiently above the minimum because of the highfrequency cutoff of Drude conductivity. The minimum frequency for the negative dynamic conductivity is reduced for the lower pulse photon energy. The frequency can be as low as about 700 GHz for hW = 0.1 eV and t = 10 ps, whereas it is around 1.1 THz for hW = 0.8 eV and t = 10 ps, demonstrating that pumping with a lower photon energy is superior. For t = 1 fs, the threshold pulse fluence for each photon energy is on the same order of magnitude as that for t = 10 ps.
Figure 21.5 Maximum negative value of dynamic conductivity over its duration as a function of frequency and pulse fluence. Columns from left to right correspond to hW = 0. 8, 0.4, 0.2, and 0.1 eV, respectively. Rows from top to bottom correspond to t = 10 ps, 1 ps, and 1 fs, respectively.
In addition, the maximum is saturated below the fundamental limit, –e2/4h, for very high pulse fluences. For example, for t = 10 ps and hW = 0.1 eV, it is saturated with the value Re sw/(e2/4h) ª – 0.4 at f = 1 THz and ª – 0.8 at f = 2 THz. The reason is that, for very high pulse
Results and Discussion
fluences, the increase in Drude absorption caused by the increase in carrier concentration exceeds the interband contribution, even though a very high quasiFermi level is obtained, and the maximum negative value of dynamic conductivity, which corresponds to the saturation value, is reached at a later time after the relaxation of the carrier concentration. The Pauli blocking also contributes to the saturation at lower photon energies. The saturation values for t = 1 fs are smaller than those for t = 10 ps; in particular, it is about 3fold smaller for hW = 0.4 and 0.8 eV. Again, this is due to the nonzero, almost constant value of Drude conductivity in the THz range with the limit wt 1. Above, we have considered a very short momentum relaxation time, ~1 fs, to demonstrate the possibility of negative dynamic conductivity in lowquality graphene. This might be achieved with high concentration of impurities, disorders, or grain boundaries, which correspond to graphene samples with carrier mobility roughly 10–102 cm2/Vs with electron concentration ~1012 cm–2. In such a case, modification of the graphene band structure caused by these imperfections is no longer negligible, and more sophisticated discussion is necessary. However, our discussion above should be a good starting point for negative dynamic conductivity in lowquality graphene.
21.3.3 OpticalPhonon Emission versus Other Recombination Mechanisms
In this chapter, we have considered interband OP emission alone as the dominant recombination mechanism. There are other recombination mechanisms allowed in graphene, which we will briefly compare with interband OP emission. Radiative recombination in graphene takes place on a submicrosecond time scale, which is much slower than that of the interband OP emission, and can be neglected. Recombination via acousticphonon emission in disordered graphene also occurs on a submicrosecond time scale [24]. Recombination via interband plasmon emission in intrinsic graphene or optically pumped intrinsic graphene with the same amount of electrons and holes should be strongly suppressed by electronhole friction [25], which results in a very short quasiparticle lifetime of plasmons, on the order of 0.1 ps.
375
376
Threshold of Terahertz Population Inversion
The recombination via the interband tunneling between the boundaries of adjacent electronhole puddles can be effective in graphene samples with puddle sizes of ~30 nm and an average carrier concentration fluctuation of ~4 ¥ 1010 cm–2 [27]. However, it should be naturally suppressed in graphene samples with a larger puddle size and smaller carrier concentration fluctuation, such as in graphene on a very clean SiO2 substrate [15] or graphene on hBN [28]. It has been suggested that Auger processes, which are forbidden by the vanishing phase space for the case of strictly linear band dispersion with no energylevel broadening, could be allowed in heavily doped, strongly pumped graphene with an electron concentration >1013 cm–2 as a consequence of the appearance of the finite energy level broadening due to electronelectron interaction [29–31]. However, in intrinsic graphene with a moderate photocarrier concentration of ~1012 cm–2 and a dielectric constant of Œ = 5.5, the screening is inefficient and the characteristic parameter of the electronelectron interaction, a2ee = (e2/ŒhuF)2 = 0.16, is relatively small. In this case, the broadening should be small [32], at least in the energy range under consideration. Therefore, the characteristic time scale for Auger processes should be neglected compared with that for the interband OP emission. Moreover, Auger processes can be further suppressed by introducing a dielectric layer above graphene with a high dielectric constant. Other extrinsic mechanisms of energy level broadening, such as disorder, must be avoided to suppress Auger processes. Trigonal warping of the graphene band structure also allows the finite phase space for Auger processes [26], although the generation and recombination rates are expected to be negligible in the energy range under consideration. This validates our assumption that only the interband OP emission is dominant compared with other recombination mechanisms. In conjunction with the discussion in preceding subsections, this suggests that the use of highquality graphene with a long momentum relaxation time, low disorder, and few electronhole puddles is required for achieving lowthreshold negative dynamic conductivity. Even where the other recombination mechanisms cannot be neglected, the dependence of the threshold on the pulse photon energy should be unchanged. Quantitatively, the threshold pulse fluence should increase as the recombination rate increases.
References
21.4 Conclusions We have investigated population inversion and negative dynamic conductivity in intrinsic graphene under pulse photoexcitation with pulse photon energy of 0.1–0.8 eV and their dependences on pulse fluence. We showed that the threshold pulse fluence can be lowered by two orders of magnitude with a lower pulse photon energy. This was attributed to the inverse proportionality of the photogenerated carrier concentration to the photon energy, as well as to the weaker carrier heating, which results in more carriers accumulating in the lowenergy region and in the suppression of recombination via interband OP emission. We also showed that negative dynamic conductivity occurs within the long relaxation time limit, wt ≥ 1, where Drude absorption in the THz range is reduced by the highfrequency cutoff, and within the very short relaxation time limit, wt 1, where it ceases for the entire frequency range. We also demonstrated that pulse excitation with lower pulse photons has a lower threshold pulse fluence and a lower minimum frequency for negative dynamic conductivity, as low as 700 GHz with hW = 0.1eV and t = 10 ps.
Acknowledgments
This work was supported by JSPS GrantinAid for Specially Promoted Research (#23000008) and by JSPS GrantinAid for Young Scientists (B) (#23760300).
References
1. K. S. Novoselov, A. K. Geim, S. V. Morozov, D. Jiang, M. I. Katsnelson, I. V. Grigorieva, S. V. Dubonos, and A. A. Firsov, Nature, 438, 197 (2005).
2. A. K. Geim and A. H. MacDonald, Phys. Today, 60(8), 35 (2007).
3. F. Bonaccorso, Z. Sun, T. Hasan, and A. C. Ferrari, Nat. Photonics, 4, 611 (2010).
4. V. Ryzhii, M. Ryzhii, and T. Otsuji, J. Appl. Phys., 101, 083114 (2007).
5. V. Ryzhii, M. Ryzhii, and T. Otsuji, Phys. Status Solidi C, 5, 261 (2008).
6. V. Ryzhii, M. Ryzhii, A. Satou, T. Otsuji, A. A. Dubinov, and V. Ya. Aleshkin, J. Appl. Phys., 106, 084507 (2009).
377
378
Threshold of Terahertz Population Inversion
7. A. Satou, T. Otsuji, and V. Ryzhii, Jpn. J. Appl. Phys., Part 1, 50, 070116 (2011). 8. V. Ryzhii, M. Ryzhii, V. Mitin, A. Satou, and T. Otsuji, Jpn. J. Appl. Phys., Part 1, 50, 094001 (2011).
9. V. Ryzhii, M. Ryzhii, V. Mitin, and T. Otsuji, J. Appl. Phys., 110, 094503 (2011).
10. V. Ryzhii, V. Mitin, M. Ryzhii, N. Ryabova, and T. Otsuji, Appl. Phys. Express, 1, 063002 (2008).
11. V. Ryzhii, N. Ryabova, M. Ryzhii, N. V. Baryshnikov, V. E. Karasik, V. Mitin, and T. Otsuji, OptoElectron. Rev., 20, 15 (2012).
12. L. Vicarelli, M. S. Vitiello, D. Coquillat, A. Lombardo, A. C. Ferrari, W. Knap, M. Polini, V. Pellegrini, and A. Tredicucci, Nat. Mater., 11, 865 (2012).
13. T. Otsuji, S. A. Boubanga Tombet, A. Satou, H. Fukidome, M. Suemitsu, E. Sano, V. Popov, M. Ryzhii, and V. Ryzhii, J. Phys. D: Appl. Phys., 45, 303001 (2012).
14. H. Karasawa, T. Komori, T. Watanabe, H. Fukidome, M. Suemitsu, V. Ryzhii, and T. Otsuji, Int. J. Infrared Millimeter Waves, 32, 655 (2011).
15. S. BoubangaTombet, S. Chen, T. Watanabe, A. Satou, V. Ryzhii, and T. Otsuji, Phys. Rev. B, 85, 035443 (2012).
16. D. Sun, Z.K. Wu, C. Divin, X. Li, C. Berger, W. A. de Heer, P. N. First, and T. B. Norris, Phys. Rev. Lett., 101, 157402 (2008).
17. J. M. Dawlaty, S. Shivaraman, M. Chandrashekhar, F. Rana, and M. G. Spencer, Appl. Phys. Lett., 92, 042116 (2008).
18. M. Breusing, C. Ropers, and T. Elsaesser, Phys. Rev. Lett., 102, 086809 (2009).
19. K. Dani, J. Lee, R. Sharma, A. Mohite, C. Galande, P. Ajayan, A. Dattelbaum, H. Htoon, A. Taylor, and R. Prasankumar, Phys. Rev. B, 86, 125403 (2012). 20. A. Satou, T. Otsuji, V. Ryzhii, and F. T. Vasko, in Proceedings of the PIERS, Kuala Lumpur, (2012), p. 486.
21. Although a more elaborated model based on the system of the Bloch equations which takes into account quantum manyparticle effects has been developed in the literature [for instance, see E. Malic, T. Winzer, E. Bobkin, and A. Knorr, Phys. Rev. B, 84, 205406 (2011)], the quasiclassical approach used here suffices for the qualitative analysis of the threshold behavior of the population inversion and negative dynamic conductivity.
References
22. H. Suzuura and T. Ando, J. Phys. Soc. Jpn., 77, 044703 (2008).
23. L. A. Falkovsky and A. A. Varlamov, Eur. Phys. J. B, 56, 281 (2007). 24. F. Vasko and V. Mitin, Phys. Rev. B, 84, 155445 (2011).
25. D. Svintsov, V. Vyurkov, S. Yurchenko, T. Otsuji, and V. Ryzhii, J. Appl. Phys., 111, 083715 (2012).
26. L. E. Golub, S. A. Tarasenko, M. V. Entin, and L. I. Magarill, Phys. Rev. B, 84, 195408 (2011). 27. V. Ryzhii, M. Ryzhii, and T. Otsuji, Appl. Phys. Lett., 99, 173504 (2011).
28. J. Xue, J. SanchezYamagishi, D. Bulmash, P. Jacquod, A. Deshpande, K. Watanabe, T. Taniguchi, P. JarilloHerrero, and B. J. LeRoy, Nat. Mater., 10, 282 (2011). 29. T. Winzer and E. Malić, Phys. Rev. B, 85, 241404(R) (2012).
30. S. Tani, F. Blanchard, and K. Tanaka, Phys. Rev. Lett., 109, 166603 (2012).
31. D. Brida, A. Tomadin, C. Manzoni, Y. J. Kim, A. Lombardo, S. Milana, R. R. Nair, K. S. Novoselov, A. C. Ferrari, G. Cerullo, and M. Polini, eprint arXiv:1209.5729v1.
32. V. Kotov, B. Uchoa, V. Pereira, F. Guinea, and A. Castro Neto, Rev. Mod. Phys., 84, 1067 (2012).
379
Chapter 22
Double Injection in Graphene pin Structures*
V. Ryzhii,a I. Semenikhin,b M. Ryzhii,c D. Svintsov,b V. Vyurkov,b A. Satou,a and T. Otsujia aResearch
Institute for Electrical Communication, Tohoku University,
Sendai 9808577, Japan
bInstitute of Physics and Technology, Russian Academy of Sciences,
Moscow 117218, Russia
cDepartment of Computer Science and Engineering, University of Aizu,
AizuWakamatsu 965–8580, Japan
[email protected]
We study the processes of the electron and hole injection (double injection) into the iregion of graphenelayer and multiple graphenelayer pin structures at the forward bias voltages. The hydrodynamic equations governing the electron and hole transport in graphene coupled with the twodimensional Poisson equation *Reprinted with permission from V. Ryzhii, I. Semenikhin, M. Ryzhii, D. Svintsov, V. Vyurkov, A. Satou, and T. Otsuji (2013). Double injection in graphene pin structures, J. Appl. Phys., 113, 244505. Copyright © 2013 AIP Publishing LLC. GrapheneBased Terahertz Electronics and Plasmonics: Detector and Emitter Concepts Edited by Vladimir Mitin, Taiichi Otsuji, and Victor Ryzhii
Copyright © 2021 Jenny Stanford Publishing Pte. Ltd.
ISBN 9789814800754 (Hardcover), 9780429328398 (eBook)
www.jennystanford.com
382
Double Injection in Graphene pin Structures
are employed. Using analytical and numerical solutions of the equations of the model, we calculate the band edge profile, the spatial distributions of the quasiFermi energies, carrier density and velocity, and the currentvoltage characteristics. In particular, we demonstrated that the electron and hole collisions can strongly affect these distributions. The obtained results can be used for the realization and optimization of graphenebased injection terahertz and infrared lasers.
22.1 Introduction
Due to unique properties, graphenelayer (GL) and multiple graphenelayer (MGL) structures [1] with pn and pin junctions are considered as novel building blocks for a variety of electron, terahertz, and optoelectronic devices. Such junctions have been realized using both chemical doping [2–6] and “electrical” doping in the gated structures [7–10]. The formation of pn and pin junctions with the electrically induced p and nregions is possible even in MGL structures with rather large number of GLs [11]. Different devices based on pin junctions in GL and MGL structures have been proposed recently. In particular, the GL and MGL structures with reversed biased pin junctions can be used in infrared (IR) and terahertz (THz) detectors [12–19] and the tunneling transittime THz oscillators [20, 21]. The GL and MGL pin junctions under the forward bias can be the basis of IR and THz lasers exploiting the interband population inversion [22–25] (see also recent experimental results [26–28]), in which the injection of electrons and holes from the n and pregions is utilized [29, 30] instead of optical pumping. A simplified model of the GL and MGL injection lasers with the pin junctions was considered recently [30]. The model in question assumes that the recombination of electrons and holes in the iregion and the leakage thermionic and tunneling currents at the pi and in interfaces are relatively small. This situation can occur in the structures with sufficiently short iregions or at relatively low temperatures when the recombination associated with the emission of optical phonons and thermionic leakage are weakened. In such a case, different components of the current can be considered as perturbations, and the spatial distributions of the electric potential
Introduction
and the carrier density along the iregion are virtually uniform. However, in the pin structures with relatively long iregions and at the elevated voltages the spatial distribution of the potential can be rather nonuniform, particularly, near the edges of the iregion, i.e., near the pi and in interfaces. In this case, the electric field in the iregion can be sufficiently strong. Such an effect can markedly influence the density of the injected carriers, the conditions of the population inversion, and currentvoltage characteristics. In this chapter, we develop a model for the GL and MGL forward biased pin structures which accounts for relatively strong recombination and consider its effect on the characteristics which can be important for realization of IR/THz injection lasers. The problem of the electron and hole injection (double injection) in GL and MGL pin structures is complicated by the twodimensional geometry of the device and the features of the carrier transport properties. This makes necessary to use twodimensional Poisson equation for the selfconsistent electric potential around the iregion and to invoke the hydrodynamic equations for carrier transport in GL and MGLs. Thus, the present model is a substantial generalization of the model applied in the previous paper [30]. To highlight the effects of strong recombination and the nonuniformity of the potential distributions, we, in contrast to Refs. [30, 31], disregard for simplicity the effects of the carrier heating or cooling and the effects associated with the nonequilibrium optical phonons. This can be justified by the fact that the injection of electrons and holes from the pertinent contacts does not bring a large energy to the electronhole system in the iregion unless the applied bias voltage is large. The chapter is organized as follows. In Section 22.2, we present the GL and MGL pin structures under consideration and the device mathematical model. Section 22.3 deals with an analytical solutions of the equations of the model for a special case. Here the general equations are reduced to a simple equation for the quasiFermi energies of electrons and holes as functions of the applied bias voltage. In Section 22.4, the equations of the model are solved numerically for fairly general cases. The calculations in Sections 22.3 and 22.4 provide the spatial distributions of the band edges, the quasiFermi energies and densities of electrons and holes, and their average (hydrodynamic) velocities. It is shown that the obtained analytical distributions match well with those obtained numerically,
383
384
Double Injection in Graphene pin Structures
except very narrow regions near the pi and in interfaces. In Section 22.5, the obtained dependences are used for the calculation of the currentvoltage characteristics of the GL and MGL pin structures. Section 22.6 deals with the discussions of some limitations of the model and possible consequences of their lifting. In Section 22.7 we draw the main conclusions.
22.2 Model
22.2.1 The Structures Under Consideration We consider the GL or MGL pin structures with either chemically or electrically doped p and nregion (see the sketches of the structures on the upper and lower panels in Fig. 22.1). We assume that the pand nregions (called in the following p and ncontacts) in single or
Figure 22.1 Schematic view of the crosssections of MGL pin structures with chemically doped n and pcontact regions (upper panel) and with such regions electrically induced by the side gatevoltages Vp = –Vg and Vn = Vg > 0 (lower panel).
multipleGL structures are strongly doped, so that the Fermi energy in each GL in these structures eFc and hence the builtin voltage Vbi are sufficiently large
Model
e
Fc =
eVbi/2 kBT,
where T is the temperature and kB is the Boltzmann constant. In the singleGL structures with the electrically induced p and ncontact regions e Fc = eVbi /2 =
u w 2
k Vg
eWg
,
where ℏ and k are the Planck constant and the dielectric constant, respectively, uW ≃ 108 cm/s is the characteristic velocity of electrons and holes in GLs, Wg is the gate layer thickness, and Vg is the gate voltage (Vp = –Vg and Vn = Vg (see Fig. 22.1)). Figure 22.2 shows the schematic views of the band profiles of a GL pin structure at the equilibrium (see Fig. 22.2a) and at the forward bias (see Fig. 22.2b). The Fermi energies of the holes and electrons in the contact p and nregions are assumed to be eFc. It is shown that at V = 0, the densities of electron and hole (thermal) in the iregion are relatively small. However, at the forward bias these densities become
Figure 22.2 Qualitative view of band profiles of a GL pin structure (a) at V = 0 and (b) at forward bias V > 0. Opaque and open circles correspond to electrons and holes, respectively. Wavy, straight, and dashed arrows correspond to the recombination in the iregion (assisted by optical phonon emission), tunneling at the contact, and thermionic leakage to the contact, respectively.
rather large due to the injection. The injection is limited by the hole charge near the pi junction and by the electron charge near the
385
386
Double Injection in Graphene pin Structures
in junction. Due to this, the Fermi energy of the injected electrons and holes, eFi, at the pertinent barriers is generally smaller than eFc. However, at the bias voltages comparable with the buildin voltage Vbi, these Fermi energy can be close to each other. The qualitative band profiles of Fig. 22.2 are in line with the band profiles found from the selfconsistent numerical calculation shown in Section 22.4. Due to high electron and hole densities in the iregion under the injection conditions, the electron and hole energy distribution are characterized by the Fermi functions with the quasiFermi (counted from the Dirac point) eFe and eFh, respectively, and the common effective temperature T, which is equal to the lattice temperature.
22.2.2 Equations of the Model
The model under consideration is based on the twodimensional Poisson equation for the selfconsistent electric potential and the set of hydrodynamic equations describing the electron and hole transport along the GL (or GLs) in the iregion. The Poisson equation for the twodimensional electric potential y = y(x, z) is presented as ∂2y ∂x
2
+
∂2y ∂z
2
=
4pe ( Âe  Âd  Â h + Âa ) ◊d ( z ), k
(22.1)
where e = e is the electron charge, Se and Sh are the net electron and hole sheet densities in the system (generally consisting of K GLs), Sd = Sd(x) and Sa = Sa(x) are the densities of donors and acceptors in the iregion (located primarily near the contact regions), and d(z) is the delta function reflecting the fact that the GL (MGL system) are located in a narrow layer near the plane z = 0. The axis x is directed in this plane. The transport of electrons and holes is governed by the following system of hydrodynamic equations [32]: d Âe ue d Â h uh = R , = R , dx dx
1 d (ej  e Fe ) = vue + veh (ue  uh ), M dx 
1 d (ej + e Fh ) = vuh + veh (uh  ue ), M dx
(22.2)
(22.3) (22.4)
Model
Âe =
Âh =
2kB2T 2K 2 p 2u W
2kB2T 2K
Ú
•
Ú
•
0
dyy , Èexp ( y  e Fe /kBT ) + 1˘ ˚ Î dyy
(22.5)
, (22.6) ÎÈexp ( y  e Fh /kBT ) + 1˚˘ Here j = yz=0 is the potential in the GL plane, eFe, eFh, ue, and uh are the quasiFermi energies and hydrodynamic velocities of electrons and holes, respectively, v is the collision frequency of electrons and holes with impurities and acoustic phonons, veh is their collision frequency with each other, and M is the fictitious mass, which at the Fermi energies of the same order of magnitude as the temperature can be considered as a constant. The recombination rate R in the case of dominating optical phonon mechanism can be presented in the following simplified form (see, for instance, Refs. [30, 31, 33]): R= �
2 p 2u W
0
˘ Ê e + e  �w 0 ˆ K Â T È ( N 0 + 1) exp Á Fe Fh  1˙ Í ˜ t R ÎÍ N0 kBT ¯ Ë ˚˙ K ÂT tR
È ˘ Ê e Fe F + e Fh ˆ  1˙ . Íexp Á ˜ Ë kBT ¯ ˚˙ ÎÍ
(22.7)
2 Here Â T = p kB2T 2/62u W is the equilibrium density of electrons and holes in the iregion in one GL at the temperature T, tR = ST/GT is the characteristic time of electronhole recombination associated with the emission of an optical phonon, GT µN0 is the rate of thermogeneration of the electronhole pairs due to the absorption of optical phonons in GL at equilibrium, ℏw0 is the optical phonon energy, and N0 = [exp(ℏw0/kBT) – 1]–1.
22.2.3 Boundary Conditions
The boundary conditions for the electron and hole velocities and Fermi energies are taken in the following form: ue x=L = uR ,
and
uh x =L = uR ,
e Fe x = L = e Fh x =L = e Fc /2 = eVbi /2,
(22.8)
(22.9)
where 2L is the spacing between p and nregion (length of the iregion), uR is the recombination velocity of electrons and holes
387
388
Double Injection in Graphene pin Structures
in narrow spacecharge regions adjacent to the p and nregion, respectively, due to the interband tunneling and due to the leakage over the barriers (edge recombination velocity) [7, 34] and V is the applied bias voltage (see Fig. 22.1). The quantity eFc is the Fermi energy at the contact regions. The electric potential at the contact regions is determined by the applied voltage V (ey + e Fh ) x£ L ,z =0 =
eV , 2
(ey  e Fe ) x ≥ L ,z =0 = 
eV , 2
(22.10)
(22.11)
where V is the applied bias voltage. Combining Eqs. (22.9)–(22.11), one obtains y x £ L ,z = 0 = j x= L =
y x ≥ L ,z =0 = j x=L = 
e (V  Vbi ) 2
e (V  Vbi ) 2
,
(22.12)
.
(22.13)
The dependence ej = ej(x) yields the coordinate dependence of the Dirac point or the band edge profile (with respect to its value in the iregion center, x = 0).
22.2.4 Dimensionless Equations and Boundary Conditions
To single out the characteristic parameters of the problem we introduce the following dimensionless variables: Y = ey/kBT, F = ej/T, me = eFe/T, mh = eFh/kBT, mc = eFc/kBT, se = Se/ST, sh = Sh/ST, sd = Sd/ST, sa = Sa/ST, Ue = uetR/L, Uh = uhtR/L, Ur = urtr/L, x = x/L, and z = z/L. Using these variables, Eqs. (22.1) and (22.6) are presented as ∂2 Y
∂2x 2
+
∂2 Y ∂z 2
= 4p Q(s e  s d  s h + s a ) ◊ d (z ),
ds eUe = 1  exp (me + mh ), dx ds hU h = 1  exp (me + mh ), dx
(22.14)
(22.15) (22.16)
Model
d (F  me ) dx 
È Ê v ˆ ˘ = q ÍUe Á + Ue  U h ˙ , ˜ ˙˚ ÎÍ Ë veh ¯
d (F + m h ) dx se = sh =
12 p
2
12 p
2
˘ È Ê v ˆ = q ÍU h Á + U h  Ue ˙ , ˜ ÎÍ Ë veh ¯ ˚˙
Ú
•
Ú
•
0
0
dyy
˘ È Îexp ( y  me ) + 1˚ dyy
ÈÎexp ( y  mh ) + 1˘˚
(22.17) (22.18)
,
(22.19)
.
(22.20)
Here Q and q are the “electrostatic” and “diffusion” parameters given, respectively, by the following formulas: Q=K
pe2 LkBT 2 6k2u W
,q=
Mveh L2 . t R kBT
Assuming, L = 1 – 5 mm, K = 1 – 2, κ = 4, T = 300 K. eFc = 100 meV, veh = 1013 s–1, and tR = 10–9 s, we obtain Q = 12.5–125, q = 0.04–1.0. The same values of q one obtains if veh = 1012 s–1 and tR = 10–10 s. The parameters Q and q can also be presented as 4pQ L/rST and
2 /4e2T) and LD = ( Dt R ) q ~ (L2/Dtr) ≃ (L/Ld)2, where rST = (k 2u w are the characteristic screening and the diffusion lengths in the 2 iregion (in equilibrium when mi = 0), respectively, and D = u w /2veh is the diffusion coefficient. The boundary conditions for the set of the dimensionless Eqs. (22.14)–(22.20) are given by
me x =1 = mh x =1 = mc = eVbi /2kBT , Ue x =1 = UR , U h x =1 = UR ,
Y x £1,z =0 = F x =1 = eV/2kBT  mc , Y x ≥1,z =0 = F x =1 = eV /2kBT + mc .
(22.21)
(22.22)
(22.23) (22.24)
In the following we focus our consideration mainly on the structures with very abrupt pi and ip junction neglecting terms sd and sa in Eq. (22.14). The effect of smearing of these junctions resulting in sd π 0 and sa π 0 will be briefly discussed in Section 22.6.
389
390
Double Injection in Graphene pin Structures
22.3 Injection Characteristics (Analytical
Approach for a Special Case)
Consider the special case in which v/veh, UR 1. When Q 1, Eq. (22.14) is actually a partial differential equation with a small parameter (Q–1 1) at highest derivatives. Usually the net solution of such equations can be combined from their solutions disregarding the left side (valid in a wide range of independent variables) and the solution near the edges (which are affected by the boundary conditions) in the regions of width h ∼ Q 1 ∼ rST /L � 1, where the derivatives are large, provided a proper matching of these solutions [35]. Hence, since parameter Q 1, for a wide portion of the iregion one can assume that se ≃ sh ≃ si = const and, consequently, me ≃ mh = mi. In this case, Eqs. (22.15) and (22.16) yield 2mi
Ue
(e =
2mi
Uh
(e =
) (x + 1),
1
si
(22.25)
) (x  1).
1
si
(22.26)
It is instructive that the condition me = mh = mi ≃ const, assumed above, is fulfilled only if the collisions with impurities and acoustic phonons are disregarded. Therefore, in this section we assume that v veh. Considering this, we find
(e F = 2q
) x.
1
2mi
si
(22.27)
At the points x = ±(1 – h) ≃ ±1, one can use the simplified matching conditions (see Fig. 22.2b) and obtain the following equation for mi:
(e m + 2q i
or
mi +
(
2mi
)=
1
si
eV 2kBT
)
2qp 2 e2mi  1
Ú
•
12
0
dyy
ÈÎexp ( y  mi ) + 1˘˚
=
(22.28)
eV . 2kBT
(22.29)
Injection Characteristics (Analytical Approach for a Special Case)
If eV < 2kBT, one can expect that 2mi < 1, so that si ≃ 1, and Eq. (22.29) yields mi
eV . 2kBT (1 + 4q )
(22.30)
At eV > 2T, 2mi > 1 (the electron and hole components are degenerate), from Eq. (22.29) mi +
p 2q
3mi2
e2mi =
eV . 2kBT
(22.31)
If formally q Æ 0 (very long diffusion length or near ballistic transport of electrons and holes in the iregion), one can see from Eqs. (22.29)–(22.31) that mi tends to eV/2T, i.e., the Fermi energies of electrons and holes tend to eV/2 (as in the previous paper [30]).
Figure 22.3 Fermi energy in the iregion eF as a function of the bias voltage V for different values of parameter q. Opaque squares correspond to electron (hole) Fermi energies at x = 0 calculated numerically in Section 22.4.
Figure 22.3 shows the voltage dependences of the Fermi energy, eFe = Tmi ≃ eFh, of electrons and holes in the main part of the iregion calculated using Eq. (22.29) for different values of parameter q µ(L/LD)2. The dependences shown in Fig. 22.3 imply that the recombination leads to the natural decrease in the Fermi energies and the densities of electrons and holes in the iregion. These quantities increase with increasing applied voltage V, but such an
391
392
Double Injection in Graphene pin Structures
increase is a slower function of V (logarithmic) than the linear one. The results of the calculations based on Eq. (22.29) (i.e., based on a simplified model valid for weak electron and hole collisions with impurities and acoustic phonons and the edge recombination) practically coincide with the results of numerical calculations involving a rigorous model (shown by the markers in Fig. 22.3). The results of these calculations are considered in Section 22.4.
22.4 Numerical Results
Finding of analytical solutions of Eq. (22.14) coupled with Eqs. (22.15)–(22.20) in the nearedge region and their matching with the smooth solutions in the main portion of the iregion is a difficult problem due to the nonlinearity of these systems of equations and its integrodifferential nature. In principle, what could such solutions provide is an information on the width of the nearedge regions. The latter is not so important, because the main characteristics of the structures under consideration are determined by the electronhole system in the structure bulk (in the main portion of the iregion). However, the net solution is particularly interesting to verify the results of the analytical model considered in Section 22.3. For this purpose, we solved Eqs. (22.14)–(22.20) numerically by iterations. Due to large values of parameter Q, one could expect very sharp behavior of Y and F near the edges of the iregion, so that strongly nonuniform mesh was used. The potential F was found by reducing the Poisson Eq. (22.14) to the following: V /T  2mc sin 1 x p 4pQ 1 + dx ¢G(x ,x ¢)[s h (x ¢)  s e (x¢ )], k 1
F(x ) = 
Ú
where
(22.32)
1 Ï ˘¸ È 1 1 Ô 1 + cos Îsin (x ) + sin (x¢ )˚ Ô G(x , x ¢) = ln Ì ˝ 4p Ô 1  cos Èsin 1 (x )  sin 11 (x¢ )˘ Ô Î ˚˛ Ó is the Green function, which corresponds to the geometry and the boundary conditions under consideration.
Numerical Results
Figure 22.4 Conduction band bottom (valence band top) profiles in the iregion calculated for different bias voltages V at q = 0.1 (upper panel) and q = 1.0 (lower panel) at Q = 100. The extreme left and right markers (at x/L = ∓ 1) show the positions of the Dirac point at pi and in junctions. Insets show detailed behavior in close vicinities near the iregion edges.
Figure 22.4 shows the profiles of the band edges, i.e., the conduction band bottom (valence band top) in the iregion (–L £ x £ L) obtained from numerical solutions of Eqs. (22.14)–(22.20) for different values of the bias voltage V and parameter q at Q = 100 (and v/veh, UR 1 as in Section 22.3). As follows from Fig. 22.4, an increase in the bias voltage V leads to the rise of the barrier for
393
394
Double Injection in Graphene pin Structures
the electrons injected from the nregion and the holes from the pregion. These barriers are formed due to the electron and hole selfconsistent surface charges localized in very narrow region (of the normalized width h ~ Q–1 = 0.01) in the iregion near its edges. The electric field near the edges changes the sign. In the main portion of the iregion, the electric field is almost constant. Its value increases with increasing parameter q, i.e., with reinforcement of the recombination. Figures 22.5 and 22.6 demonstrate the spatial distributions of the electron Fermi energy eFe(x) and the electron density Se(x) in the iregion for q = 1.0 at different bias voltages. The hole Fermi energy and the hole density are equal, respectively, to eFh(x) = eFe(–x) and Sh(x) = Se(–x).
Figure 22.5 Spatial distributions of the electron Fermi energy eFe at q = 1 and Q = 100 calculated for different values of bias voltage V at Ur = 0. Inset shows dependences near the ncontact. Opaque circles correspond to data obtained using analytical model.
One can see from Figs. 22.5 and 22.6 that the electron Fermi energy and the electron density steeply drop in fairly narrow region adjacent to the pregion. However, they remain virtually constant in the main portion of the iregion if the ratio of the collisions frequency of electrons and holes with impurities and acoustic phonons and the frequency of electronhole collisions v/veh 1. In the latter case, the values of these quantities across almost the whole iregion coincide with those obtained analytically above with a high accuracy (see
Numerical Results
Figure 22.6 Spatial distributions of electron density Se at different bias voltages V (v/veh = 0 and Ur = 0).
Figure 22.7 Spatial distributions of the electron Fermi energy eFe at q = 1 and
Q = 100 calculated for different values of ratio v/veh and V = 250 mV at Ur = 0.
the markers in Figs. 22.3 and 22.5). This justifies the simplified approach used in the analytical model for the case v/veh, Ur 1 developed in Section 22.3. Nevertheless, at not too small values of parameter v/veh, the coordinate dependences of the electron (and hole) Fermi energy exhibit a pronounced sag (see Fig. 22.7). Similar
395
396
Double Injection in Graphene pin Structures
sag was observed in the coordinate dependences of the electron and hole densities (not shown). As seen from Fig. 22.8, an increase in the ratio v/veh leads also to a pronounced modification of the coordinate dependences of the electron (hole) velocity: the absolute value of the electron velocity markedly decreases with increasing v/ veh. However, the changes in the band edge profiles and hence the electric field in the main portion of the iregion are insignificant. Above, we have considered the cases of the pin structures with sufficiently long iregion, so that the normalized edge recombination velocity Ur 1. In such cases, in accordance with the boundary conditions Ue (and Uh) tends to zero at the pertinent contact region (see Fig. 22.8).
Figure 22.8 Coordinate dependences of normalized electron velocity Ue calculated for q = 1.0 and V = 250 mV at different values of v/veh.
The calculations of the spatial distributions of the band edge profiles, Fermi energies, and carrier concentrations showed that the variation of the edge recombination velocity Ur (at least in the range from zero to ten) does not lead to any pronounced distinction even in the nearedge regions. In all cases considered, as seen from Fig. 22.9, the absolute value of Ue steeply increases in a narrow region near the ncontact and the gradually drops (virtually linearly) across the main portion of the iregion. However, Ue (and, hence, the electron hydrodynamic velocity ue), being virtually independent of Ur from
CurrentVoltage Characteristics
the nregion to the nearedge region adjacent to the pi interface, strongly depends on UR in the latter region (see Fig. 22.9 (both left and right panels)). The hole velocity exhibits the same behavior with Uh(x) = – Ue(–x).
Figure 22.9 The normalized electron velocity Ue versus coordinate x for q = 1.0 and V = 250 mV at different values of normalized edge recombination velocity UR (left panel). Right panel shows details of the same dependences in close vicinity of the pi interface.
Due to rather short nearcontact regions, the edge recombination does not affect substantially the integral characteristics of the pin structures under consideration, in particular total number of the injected electrons and holes and their net recombination rate at least in the practical pin structures with Q 1 and not too large UR (i.e., not too short iregions).
22.5 CurrentVoltage Characteristics
The current (associated with the recombination in the iregion) can be calculated as J =e
Ú
L
L
dxR =
eKLS T tR
Ú
1
1
dx[e(me + mh )  1].
(22.33)
Using the obtained analytical formulas derived above, in which me(x) ≃ mh(x) = mi ≃ const, we find J=
2eKLS T 2mi (e  1) tR
(22.34)
397
398
Double Injection in Graphene pin Structures
or where
J = K J0 (e2mi  1),
J0 =
p eLkB2T 2 2 32u w tR
.
(22.35) (22.36)
Setting L = 1 – 5 mm and tR = 10–10 – 10–9 s at T = 300 K, from Eq. (22.34) one obtains J0 ≃ (3 – 150) ¥ 10–3 A/cm. The currentvoltage characteristics obtained for different parameters q (using Eqs. (22.29) and (22.35) at v/veh 1) are shown in Fig. 22.10. As follows from Fig. 22.10, the injection current superlinearly increases with increasing bias voltage V. The steepness of such currentvoltage characteristics decreases with increasing parameters q. This is because a larger q corresponds in part to larger veh, i.e., to a larger resistance. In the limit q Æ 0, the currentvoltage dependence approaches to J µ exp(eV/2T). Thus, at the transition from near ballistic electron (q 1) and hole transport to collision dominated transport (q ~ 1), the currentvoltage characteristics transform from exponential to superlinear ones.
Figure 22.10 Currentvoltage characteristics for different values of parameter q. Inset shows the current as a function of parameter v/veh calculated at V = 250 mV for q = 1.0.
Discussion
However, at finite values of parameter v/veh, mi can be a pronounced function of the coordinate as seen from Fig. 22.7. This results in a dependence of the current on the parameter in question. Inset in Fig. 22.10 shows the dependence of the current on parameter v/veh at fixed bias voltage. A decrease in the current with increasing parameter v/veh is associated with a sag in the spatial dependence of the Fermi energy (see Fig. 22.7), which gives rise to weaker recombination in an essential portion of the iregion and, therefore, lower recombination (injection) current.
22.6 Discussion
The rigorous calculation of the edge recombination current, particularly, its tunneling component and parameter UR requires special consideration. Here we restrict ourselves to rough estimates based of a phenomenological treatment. The characteristic velocity, uRtunn , of the edge recombination due to tunneling of electrons through the barrier at the piinterface (and holes through the barrier at the ininterface) can be estimated as uRtunn = D tunnu W /p . Here Dtunn is the effective barrier tunneling transparency, determined, first of all, by the shape of the barrier. The appearance of factor 1/p is associated with the spread in the directions of electron velocities in the GL plane. In the case of very sharp barrier, Dtunn ≃ 1. However, practically Dtunn is less than unity, although due to the gapless energy spectrum of carriers in GLs and MGLs one can not expect that it is very small. The edge recombination velocity associated with the thermionic current of electrons (holes) over the pertinent barrier is proportional to Dth µ exp(–mc), so that uRth µ (u W /p )exp( mc ). The factor exp (–mc) is very small when the contact n and pregions are sufficiently doped (mc 1), hence, URth URtunn . In the case of the electrically induced p and nregions in MGL structures, the condition mc 1 can impose certain limitation on the number of GL K [11]. As a result, parameter UR can be estimated as UR ≃ uRtunn tR/L = DtunnuWtR/pL. At tR = 10–10 s, L = 5 mm, and Dtunn = 0.5 we find that UR ≃ 3. As shown above, the edge recombination even at relatively large parameter UR markedly influences the carrier densities and their Fermi energies only in immediate vicinity of the pi and in interfaces (see Fig. 22.9). To find conditions when the surface (tunneling) recombination can be
399
400
Double Injection in Graphene pin Structures
disregarded in comparison to the recombination assisted by optical phonons, we compare the contributions of this recombination to the net current. Taking into account Eq. (22.35) and considering that the edge recombination tunneling current Jtunn ≃ evWDtunnST, we obtain J
J
tunn
2pL 2 (e2mi  1) � tunn e2mi . > tunn � D uWt R UR
(22.37)
Equation (22.37) yields the following condition when the edge recombination is provides relatively small contribution to the injection current: L>
D tunnu W t R 2mi e . 2p
(22.38)
Assuming that tR = 10–10 s, Dtunn = 0.5, and mi = 1.0 – 1.4 (eFi = 25 – 35 meV), from inequality (22.36) we obtain 2L > (1 – 2) mm. As follows from Eq. (22.38), the role of the edge recombination steeply drops when mi, i.e., the bias voltage V increase. This is because the recombination rate R, associated with optical phonons, rapidly rises with increasing mi. If tR = (10–10 – 10–9) s and mi = 2.5 (eFi = 62.5 meV), one can arrive at the following condition: 2L > 0.1 – 1 mm. As demonstrated in Section 22.4, the spatial variations of the band edge profile, density of carriers and their Fermi energies are very sharp near the pi and in interfaces. This is owing to large values of parameter Q and the assumption of abrupt doping profiles. In this case, the normalized width of the transition region is h ~ Q–1 ~ rST /L 1. In real GL and MGL pin structures, the boundaries between p, i, and nregion are somewhat smeared (with the characteristic length l L). This can be associated with the specifics of chemical doping or with the fringing effects. In the latter case, the length of the intermediate region is about the thickness of the gate layer l ~ Wg (see Fig. 22.1). In both cases, this can result in a smoothing of the dependences in nearcontact regions in comparison with those shown in Figs. 22.4–22.9 and in a marked decrease in the electric field in the pi and ip junctions and in the edge tunneling current. Figure 22.11 demonstrates examples of the band edge profiles calculated for the abrupt pi and in junctions and for that with smeared junction. In the latter case, it was assumed that the acceptor and donor densities varied exponentially with the characteristic length l = 0.03L: sd µ exp[–(x – 1)2/h2] and sd µ exp[–(x + 1)2/h2],
Discussion
with h = l/L = 0.03, Sc = 5.6 ¥ 1012cm–2 (sc = 62.8, mc ≃ 10). As seen from Fig. 22.11, an increase in smearing of the dopant distributions leads to a natural increase in the widths of the transition regions and a decrease (relatively small) in the electrical field in the iregion.
Figure 22.11 Comparison of band edge profiles in structures with abrupt (solid line with markers, the same as in Fig. 22.4) and with smeared pi and ni junctions (without markers) at V = 500 mV for q = 1.0.
At moderate number of GLs K in the pin structures under consideration, the net thickness of the latter Kd, where d ~ 0.35 nm is the spacing between GLs, is smaller than all other sizes. In such a case, the localization of the space charges of electrons and holes in the iregion in the zdirection can be described by the delta function d(z) as in Eq. (22.1). In the case of large K, the delta function should be replaced by a function with a finite localization width. This also should give rise to an extra smearing of the spatial distributions in the xdirection. The pertinent limitation on the value K can be presented as follows: Kd rs, l L, where rs = [rST /ln(1 + e mi )] is the screening length. At rs ≲ l L, assuming that k = 4 and mi ≳ 1 one can obtain rs ≃ 10 nm and arrive at the following condition K 30. An increase in K results in an increase in parameters Q and, hence, in some modification of the spatial distributions in near contact region, although the latter weakly affects these distributions in the main portion of the iregion. As a result, the injection current increases proportionally to K (see Eq. (22.35)).
401
402
Double Injection in Graphene pin Structures
We disregarded possible heating (cooling) of the electronhole system in the iregion. Under large bias voltages the electric field in this region can be fairly strong. In this case, the dependence of the drift electron and hole velocities on the electric field might be essential. However, relatively strong interaction of electrons and holes with optical phonons having fairly large energy prevents substantial heating [36] in the situations considered in Sections 22.4 and 22.5. Moreover, in the essentially bipolar system the recombination processes with the emission of large energy optical phonons provide a marked cooling of the system, so that its effective temperature can become even lower than the lattice temperature [30, 31]. The above consideration was focused on the double injection in GL and MGL pin structures at the room temperatures. The obtained results are also applicable at somewhat lower temperatures if the recombination is primarily associated with optical phonons. However, at lower temperatures, other recombination mechanisms can become more crucial, for instance, the Auger recombination mediated by scattering mechanisms on impurities and acoustic phonons and due to trigonal warping of the GL band structure, which provide additional momentum and enables transitions to a broader range of final states [37–39], i.e., the indirect Auger recombination [40] (see also Refs. [41, 42]), acoustic phonon recombination, invoking the momentum transfer due to disorder [43], radiative recombination [44], tunneling recombination in the electronhole puddles [45], and edge tunneling recombination (see Ref. [34] and Section 22.4). Relatively weak role of the optical phonon assisted processes at low temperatures can result in pronounced hot carrier effects (see, for instance, Refs. [46, 47). However, these effects are beyond the scope of our chapter and require special consideration.
22.7 Conclusions
We studied theoretically the double electronhole injection in GL and MGL pin structures at the forward bias voltages using the developed device model. The mathematical part of the model
Conclusions
was based on a system of hydrodynamic equations governing the electron and hole transport in GLs coupled with the twodimensional Poisson equation. The model is characterized primarily by the following two parameters: the electrostatic parameter Q and the diffusion parameter q. Large value of parameter Q in practical structures results in the formation of very narrow edge regions near pi and in interfaces, in which all physical quantities vary sharply, and the formation of a wide region, which is stretched across the main portion of the iregion, where all spatial dependences are rather smooth. Using analytical and numerical solutions of the equations of the model, we calculated the band edge profiles, the spatial distributions of the quasiFermi energies, carrier density and velocity, and the currentvoltage characteristics. It was demonstrated that the electronhole collisions and the collisions of electrons and holes with impurities and acoustic phonons can strongly affect the characteristics of the pin structures. In particular, such collisions result in a pronounced lowering of the injection efficiency (weaker dependences of the electron and hole Fermi energies and their densities on the bias voltage) and the modification of the currentvoltage characteristics from an exponential to superlinear characteristics (at collisiondominated transport). It is also shown that for the case of relatively perfect GL and MGL structures, the developed analytical model provides sufficient accuracy in the calculations of spatial distributions in the main portion of the iregion and of the pin structure overall characteristics. The effects associated with the edge recombination and smearing of the pi and in junctions are evaluated. The obtained results appear to be useful for the realization and optimization of GL and MGLbased injection terahertz and infrared lasers.
Acknowledgments
The authors are grateful to M. S. Shur and V. Mitin for numerous fruitful discussions. The work was financially supported in part by the Japan Science and Technology Agency, CREST and by the Japan Society for Promotion of Science.
403
404
Double Injection in Graphene pin Structures
References 1. A. H. C. Neto, F. Guinea, N. M. R. Peres, K. S. Novoselov, and A. K. Geim, Rev. Mod. Phys., 81, 109 (2009). 2. D. Farmer, Y.M. Lin, A. AfzaliArdakani, and P. Avouris, Appl. Phys. Lett., 94, 213106 (2009).
3. E. C. Peters, E. J. H. Lee, M. Burghard, and K. Kern, Appl. Phys. Lett., 97, 193102 (2010). 4. K. Yan, Di Wu, H. Peng, L. Jin, Q. Fu, X. Bao, and Zh. Liu, Nat. Commun., 3, 1280 (2012).
5. H. C. Cheng, R. J. Shiue, C. C. Tsai, W. H. Wang, and Y. T. Chen, ACS Nano, 5, 2051 (2011).
6. Yu Tianhua, C. Kim, C.W. Liang, and Yu Bin, Electron Device Lett., 32, 1050 (2011). 7. V. V. Cheianov and V. I. Falko, Phys. Rev. B, 74, 041403 (2006).
8. B. Huard, J. A. Silpizio, N. Stander, K. Todd, B. Yang, and D. GoldhaberGordon, Phys. Rev. Lett., 98, 236803 (2007). 9. J. R. Williams, L. DiCarlo, and C. M. Marcus, Science, 317, 638 (2007).
10. H.Y. Chiu, V. Perebeinos, Y.M. Lin, and P. Avouris, Nano Lett., 10, 4634 (2010). 11. M. Ryzhii, V. Ryzhii, T. Otsuji, V. Mitin, and M. S. Shur, Phys. Rev. B, 82, 075419 (2010).
12. F. Xia, T. Mueller, Y.M. Lin, A. ValdesGarcia, and P. Avoris, Nat. Nanotechnol., 4, 839 (2009).
13. V. Ryzhii, M. Ryzhii, V. Mitin, and T. Otsuji, J. Appl. Phys., 107, 054512 (2010). 14. T. Mueler, F. Xia, and P. Avouris, Nat. Photonics, 4, 297 (2010).
15. M. Ryzhii, T. Otsuji, V. Mitin, and V. Ryzhii, Jpn. J. Appl. Phys., 50, 070117(2011).
16. N. M. Gabor, J. C. W. Song, Q. Ma, N. L. Nair, T. Taychatanapat, K. Watanabe, T. Taniguchi, L. S. Levitov, and P. JarilloHerrero, Science, 334, 648 (2011). 17. V. Ryzhii, N. Ryabova, M. Ryzhii, N. V. Baryshnikov, V. E. Karasik, V. Mitin, and T. Otsuji, Optoelectron. Rev., 20, 15 (2012).
18. D. Sun, G. Aivazian, A. M. Jones, J. Ross, W. Yao, D. Cobden, and X. Xu, Nat. Nanotechnol., 7, 114 (2012). 19. M. Freitag, T. Low, and P. Avouris, Nano Lett., 13, 1644 (2013).
References
20. V. Ryzhii, M. Ryzhii, M. S. Shur, and V. Mitin, Appl. Phys. Express, 2, 034503 (2009).
21. V. L. Semenenko, V. G. Leiman, A. V. Arsenin, V. Mitin, M. Ryzhii, T. Otsuji, and V. Ryzhii, J. Appl. Phys., 113, 024503 (2013). 22. V. Ryzhii, M. Ryzhii, and T. Otsuji, J. Appl. Phys., 101, 083114 (2007).
23. V. Ryzhii, M. Ryzhii, A. Satou, T. Otsuji, A. A. Dubinov, and V. Ya. Aleshkin, J. Appl. Phys., 106, 084507 (2009). 24. V. Ryzhii, A. A. Dubinov, T. Otsuji, V. Mitin, and M. S. Shur, J. Appl. Phys., 107, 054505 (2010).
25. A. A. Dubinov, V. Ya. Aleshkin, V. Mitin, T. Otsuji, and V. Ryzhii, J. Phys.: Condens. Matter, 23, 145302 (2011).
26. S. BoubangaTombet, S. Chan, A. Satou, T. Otsuji, and V. Ryzhii, Phys. Rev. B, 85, 035443 (2012).
27. T. Otsuji, S. BoubangaTombet, A. Satou, M. Ryzhii, and V. Ryzhii, J. Phys. D, 45, 303001 (2012).
28. T. Li, L. Luo, M. Hupalo, J. Zhang, M. C. Tringides, J. Schmalian, and J. Wang, Phys. Rev. Lett., 108, 167401 (2012).
29. M. Ryzhii and V. Ryzhii, Jpn. J. Appl. Phys., 46, L151 (2007).
30. V. Ryzhii, M. Ryzhii, V. Mitin, and T. Otsuji, J. Appl. Phys., 110, 094503 (2011). 31. V. Ryzhii, M. Ryzhii, V. Mitin, A. Satou, and T. Otsuji, Jpn. J. Appl. Phys., 50, 094001 (2011).
32. D. Svintsov, V. Vyurkov, S. O. Yurchenko, T. Otsuji, and V. Ryzhii, J. Appl. Phys., 111, 083715 (2012). 33. F. Rana, P. A. George, J. H. Strait, J. Dawlaty, S. Shivaraman, M. Chandrashekhar, and M. G. Spencer, Phys. Rev. B, 79, 115447 (2009).
34. V. Ryzhii, M. Ryzhii, and T. Otsuji, Phys. Status Solid A, 205, 1527 (2008). 35. A. H. Nayfeh Perturbation Methods (WileyVCH, Weinheim, 2004).
36. R. S. Shishir and D. K. Ferry, J. Phys.: Condens. Matter, 21, 344201 (2009).
37. M. S. Foster and I. Aleiner, Phys. Rev. B, 79, 085415 (2009).
38. L. E. Golub, S. A. Tarasenko, M. V. Entin, and L. I. Magarill, Phys. Rev. B, 84, 195408 (2011).
39. A. Satou, V. Ryzhii, Y. Kurita, and T. Otsuji, J. Appl. Phys., 113, 143108 (2013). 40. E. Kioupakis, P. Rinke, K. T. Delaney, and C. G. Van de Walle, Appl. Phys. Lett., 98, 161107 (2011).
405
406
Double Injection in Graphene pin Structures
41. P. A. George, J. Strait, J. Davlaty, S. Shivaraman, M. Chandrashekhar, F. Rana, and M. G. Spencer, Nano Lett., 8, 4248 (2008). 42. T. Winzer and E. Malic, Phys. Rev. B, 85, 241404 (2012).
43. F. Vasko and V. Mitin, Phys. Rev. B, 84, 155445 (2011).
44. V. Vasko and V. Ryzhii, Phys. Rev. B, 77, 195433 (2008).
45. V. Ryzhii, M. Ryzhii, and T. Otsuji, Appl. Phys. Lett., 99, 173504 (2011).
46. O. G. Balev, F. T. Vasko, and V. Ryzhii, Phys. Rev. B, 79, 165432 (2009). 47. O. G. Balev and F. T. Vasko, J. Appl. Phys., 107, 124312 (2010).
Chapter 23
CarrierCarrier Scattering and Negative Dynamic Conductivity in Pumped Graphene*
D. Svintsov,a,b,c V. Ryzhii,a,d A. Satou,a T. Otsuji,a and V. Vyurkovb aResearch
Institute for Electrical Communication, Tohoku University, Sendai 9808577, Japan bInstitute of Physics and Technology, Russian Academy of Sciences, Moscow 117218, Russia cDepartment of General Physics, Moscow Institute of Physics and Technology, Dolgoprudny 141700, Russia dCenter for Photonics and Infrared Engineering, Bauman Moscow State Technical University, Moscow 105005, Russia [email protected]
We theoretically examine the effect of carriercarrier scattering processes on the intraband radiation absorption and their contribution to the net dynamic conductivity in optically or electrically pumped *Reprinted with permission from D. Svintsov, V. Ryzhii, A. Satou, T. Otsuji, and V. Vyurkov (2014). Carriercarrier scattering and negative dynamic conductivity in pumped graphene, Opt. Express, 22(17), 19873–19886. Copyright © 2014 Optical Society of America. GrapheneBased Terahertz Electronics and Plasmonics: Detector and Emitter Concepts Edited by Vladimir Mitin, Taiichi Otsuji, and Victor Ryzhii
Copyright © 2021 Jenny Stanford Publishing Pte. Ltd.
ISBN 9789814800754 (Hardcover), 9780429328398 (eBook)
www.jennystanford.com
408
CarrierCarrier Scattering and Negative Dynamic Conductivity
graphene. We demonstrate that the radiation absorption assisted by the carriercarrier scattering is comparable with Drude absorption due to impurity scattering and is even stronger in sufficiently clean samples. Since the intraband absorption of radiation effectively competes with its interband amplification, this can substantially affect the conditions of the negative dynamic conductivity in the pumped graphene and, hence, the interband terahertz and infrared lasing. We find the threshold values of the frequency and quasiFermi energy of nonequilibrium carriers corresponding to the onset of negative dynamic conductivity. The obtained results show that the effect of carriercarrier scattering shifts the threshold frequency of the radiation amplification in pumped graphene to higher values. In particular, the negative dynamic conductivity is attainable at the frequencies above 6 THz in graphene on SiO2 substrates at room temperature. The threshold frequency can be decreased to markedly lower values in graphene structures with highk substrates due to screening of the carriercarrier scattering, particularly at lower temperatures.
23.1 Introduction
Graphene, a twodimensional carbon crystal, possesses no energy band gap and, hence, is promising for detection and generation of farinfrared and terahertz (THz) radiation [1–3]. Several concepts of graphenebased THz lasers with optical pumping [4] or electrical (injection) pumping [5, 6] have been proposed and analyzed. Recently, the possibility of THzwave amplification by optically pumped graphene was shown experimentally [7]. Generally, one of the main reasons for low efficiency of THz semiconductor laser is the intraband (Drude) radiation absorption [8], which grows rapidly with decreasing the radiation frequency. This absorption process aggressively competes with the radiation amplification due to the stimulated interband electron transitions under the conditions of population inversion. This problem is crucial for graphenebased lasers as well. The optical conductivity of clean undoped graphene is equal to the universal value sq = e2/4ℏ, where e is the elementary charge and ℏ is the Planck’s constant. This value corresponds to the interband
Introduction
radiation absorption coefficient pa = 2.3% [10], where a = e2/ℏc is the finestructure constant (c is the speed of light in vacuum). The optical conductivity of pumped graphene can be negative due to prevailing stimulated electron transitions from the conduction to the valence band associated with the interband population inversion [11]. The interband dynamic conductivity appears to be negative at frequencies w < 2eF/ℏ, where eF is the quasiFermi energy of pumped carriers (see Fig. 23.1a and b). However, the coefficient of radiation amplification in pumped graphene is still limited by 2.3%. Hence, for the operation of graphenebased lasers the Drude absorption coefficient [12] should lie below 2.3%. In the previous models of negative dynamic conductivity in pumped graphene, it was usually assumed that the Drude absorption originates from electron and hole scattering on impurities, lattice defects, and phonons (Fig. 23.1d), which can, in principle, be removed almost completely in highquality graphene samples and at low temperatures (see, for example, [3, 13]). However, there is an unavoidable mechanism leading to the intraband absorption, namely, the radiation absorption assisted by the carriercarrier scattering (Fig. 23.1c). The carriercarrier scattering (for brevity denoted as cc scattering) was shown to be a key factor in the relaxation kinetics of photoexcited electrons and holes in graphene [7, 9, 14, 15]. It can also be responsible for weakly temperaturedependent minimal dc conductivity of graphene [16–20]. The strength of cc scattering in graphene is governed by the relatively large coupling constant, ac = e2/(k0ℏvF) ~ 1, where vF = 106 m/s is the velocity of massless electrons and holes (Fermi velocity) and k0 is the background dielectric constant. Among a variety of phenomena originating from the carriercarrier scattering in graphenebased structures, there are modifications of quasiparticle spectra [20], relaxation [14, 15], thermalization, and recombination [9]. In this chapter, we focus on the scatteringassisted intraband radiation absorption. The latter appears to be a quite strong absorption mechanism, especially in the pumped graphene with population inversion. We derive the expression for the real part of the intraband dynamic conductivity Rescc (which is proportional to the intraband contribution to the radiation absorption) arising due to carriercarrier collisions in clean pumped graphene. The probability of corresponding intraband radiation absorption process
409
410
CarrierCarrier Scattering and Negative Dynamic Conductivity
is evaluated using the secondorder perturbation theory and the Fermi golden rule. Comparing Rescc with the interband conductivity Resinter, we find the threshold values of the quasiFermi energies of pumped carriers, required to attain the net negative dynamic conductivity (negative absorption coefficient) at given frequency, and calculate the pertinent threshold frequencies. We also show that screening of the Coulomb potential by the carriers in graphene plays the significant role in the cc scattering. Because of screening, the intraband conductivity due to the cc collisions grows slowly (almost linearly) with increasing the quasiFermi energy of pumped carriers. We find that in the pumped graphene, the main contribution to the intraband conductivity arises from electronhole (eh) scattering, while the electronelectron (ee) and holehole (hh) collisions yield less than one tenth of its total value. The rate of cc scattering and the corresponding radiation absorption can be reduced in graphene clad between materials with high dielectric constants.
Figure 23.1 Schematic views of band diagrams of (A) ntype graphene in equilibrium and (B) pumped graphene. Wavy arrows indicate photon absorption and emission processes. Diagram of photon absorption by an electron (e) associated with (C) electronelectron (electronhole) and (D) impurity (i) scattering.
In the present chapter, we shall restrict our consideration of dynamic conductivity within terahertz range (1–15 THz). At higher frequencies, the optical response is governed mainly by interband transitions [21] which lead to the absorption of radiation at ℏw > 2eF, while the Drude absorption drops proportionally to w–2. At lower frequencies, one can readily use the static limit of Boltzmann/ hydrodynamic theory to obtain the conductivity.
Intraband Dynamic Conductivity General Equations
The chapter is organized as follows. In Section 23.2, we derive the general equations for the radiation power absorbed due to cc scatteringassisted intraband transitions, and find the pertinent contribution to the dynamic conductivity. In Section 23.3, we obtain the dependences of the intraband, interband, and net dynamic conductivity on the radiation frequency, the quasiFermi energy, the background dielectric constant; and find the frequency threshold of the radiation amplification. Section 23.4 deals with discussion of the obtained results and their validity. In Section 23.5, we draw the main conclusions. Some mathematical details are singled out in Appendix.
23.2 Intraband Dynamic Conductivity General Equations
There are two mechanisms through which the cc scattering affects the optical conductivity, and, hence, absorption of radiation. First, the finite lifetime of carriers leads simply to the smearing of the interband absorption/amplification edge [22]. Second, a free electron can absorb a photon and transfer the excess energy and momentum to the other carrier (Fig. 23.1c). The latter mechanism is quite similar to the conventional Drude absorption, where the excess momentum is transferred to an impurity or phonon (Fig. 23.1d). However, in the case of graphene, the radiation absorption due to cc scattering exhibits a number of unusual features. In semiconductors with parabolic bands, ee scattering cannot directly affect the conductivity and absorption of radiation. The reason is that the total current carried by two electrons is not changed in the scattering process due to momentum conservation. In graphene, however, electron velocity and momentum are not directly proportional to each other (sometimes referred to as “momentumvelocity decoupling” [19]). Hence, the momentum conservation does not imply the current conservation, and ee scattering can contribute to relaxation of current [23] and optical absorption. Such effects were studied in III–V semiconductors in the light of p4corrections to the parabolic bands [24]. In graphene, the carrier dispersion law is not parabolic “from the very beginning.” Hence, those effects can play a more considerable role.
411
412
CarrierCarrier Scattering and Negative Dynamic Conductivity
Electronhole (eh) scattering processes do not conserve the total current and can contribute to radiation absorption independent of the carrier spectrum. Apart from graphene with Fermi energy close to Dirac point, eh scattering plays a minor role in conductivity due to vanishing number of holes. This is not the case of the pumped graphene, where eh scattering is intensified due to the great number of carriers in both bands. We consider a twostep quantummechanical process: the quasiparticle (electron or hole) absorbs light quantum passing to the virtual state, then it collides with other quasiparticle and transfers the excess energy (and momentum) to it. If the frequency of electromagnetic wave w substantially exceeds the electron (or hole) collision frequency v, one can use the Fermi golden rule to calculate the absorption probability in unit time. We will first consider the radiation absorption due to ee collisions, and then generalize the result to account for eh processes. The initial momenta of incoming quasiparticles are denoted by p1 and p2, while the final momenta are p3 and p4. To work out the matrix elements appearing in the Fermi golden rule we apply the second order perturbation theory considering the two perturbations. The first one, V F (t) , is the interaction of electron with external electromagnetic field � F (t) = e (A , v� 1 + v� 2 )(e iw t + e iw t ), V 0 2c
(23.1)
where v 1 and v 2 are the velocity operators of the two electrons, A0 is the amplitude of field vector potential, and w is the frequency of the electromagnetic wave. The vector A0 and the corresponding electric field E0 = iwA0/c lie in the plane of graphene layer. The second perturbation, V C , is the Coulomb interaction between carriers. It has nonzero matrix elements connecting the twoparticle states p1, p2Ò and p3, p4Ò = p1 + q, p2 – qÒ, where q is the transferred momentum. We denote these matrix elements by V (q) ∫ p , p  V C p , p , C
3
4
1
VC (q ) = where
2
2pe2 (e ) (e ) u u qk 0k (q ) p1 p3
(e ) (e ) up up , 2
4
(23.2)
(e) u(e) = cos(q ij /2) are overlap factors of the electron p up i
j
Intraband Dynamic Conductivity General Equations
envelope functions in graphene, qij is the angle between momenta pi and pj, k0 is the background dielectric constant, and k(q) is the dielectric function of graphene itself. For our purposes, it can be taken in the static limit k
(q) = 1 + qTF/q,
(23.3)
qTF is the ThomasFermi (screening) momentum [25]. A wellknown relation for the secondorder matrix element connecting initial iÒ = p1, p2Ò and final  f Ò = p3, p4Ò states reads [26] f  V�i =
Â (e m
f V� Fw m m V� C i
P1
) (
+ e P2  e P1m + e P2m
f V� C m m V� Fw i
+
) (e
P1
) (
+ e P2 + �w  e P1m + e P2m
)
,
(23.4)
where the index m counts the intermediate states, ep = pvF is the electron dispersion law in graphene, and V� Fw = (e/2c)( A0 , v� 1 + v� 2 ) is the Fouriercomponent of electronfield interaction. The summation over intermediate momenta pm is easily performed as photon momentum is negligible compared to electron momentum. Using also the energy conservation law e p1 + e p2 + w = e p3 + e p4 ,
we obtain a very simple relation for matrix element fVi =
(23.5)
e VC (q ) (A0 , v p1 + v p2  v p3  v p4 )cos(q13/2)cos(q24 /2). 2c w (23.6)
Equation (23.6) clearly demonstrates that for parabolic bands no absorption due to ee scattering can occur as vp + vp – vp – vp 1 2 3 4 turns to zero as a result of momentum conservation. The power, P, absorbed by an electron system is calculated using the Fermi golden rule, taking into account the occupation numbers of the initial and final states: P=
w 2p g2 2 p
Â
fVi
2
d (e p1 + e p2 + w  e p3  e p4 )
1 , p2 ,q
¥ fe (p1 ) fe (p2 )[1  fe (p3 )][1  fe (p4 )][1  exp( w/kBT )]. (23.7)
Here g = 4 stands for the spinvalley degeneracy factor in graphene. The prefactor 1/2 cuts off the equivalent scattering processes;
413
414
CarrierCarrier Scattering and Negative Dynamic Conductivity
without it the indistinguishable collisions p1 + p2 and p2 + p1 are treated separately, which would be incorrect. The function fe(p) in Eq. (23.7) is the electron distribution function, which is assumed to be the quasiequilibrium Fermi function: 1
È Ê e p  me ˆ ˘ fe (p ) = Í1 + exp Á (23.8) ˜˙ . Ë kBT ¯ ˙˚ ÍÎ To treat the radiation absorption in pumped graphene, we introduce the different quasiFermi energies of electrons and holes, me and mh. In symmetrically pumped systems me = –mh = eF > 0. In what follows, if otherwise not stated, we will consider symmetrically pumped graphene. In such system, the occupation numbers of electrons and holes with energies ep > 0 are equal, hence, the subscripts e and h of the distribution functions can be omitted. In deriving Eq. (23.7) we have also neglected the exchangetype scattering, which occurs only between electrons with same spin and from the same valley. This assumption does not significantly affect the final numerical values. Finally, to obtain the real part of the intraband dynamic conductivity due to ee collisions Resee, we express the vectorpotential in Eq. (23.6) through electric field and equate (23.7) with Res ee E02/2. As a result, this conductivity is expressed via the universal optical conductivity of clean graphene sq, the coupling constant ac = e2/(k0ℏvF), and the dimensionless ‘collision integral’ Iee,w: Res ee = s q
Iee,w =
Ú
dQdk 1 dk 2 Q2k 2 (Q )
3 Ê w ˆ ˘ a c2 Ê kBT ˆ È Í1  exp Á ˙ Iee,w , ˜ 3 Á Ë kBT ¯˜ ˚˙ p Ë w ¯ ÎÍ
(23.9)
( Dnee )2 cos2 (q1± /2)cos2 (q2± /2)
¥d [k1+ + k2 + w/(kBT )  k1  k2+ ]F (k1+ )F (k2 )[1  F (k1 )][1  F (k2+ )].
(23.10)
Here, for the simplicity of further analysis, we have introduced the dimensionless momenta k1± = (p1 ± q/2)vF/(kBT), k2± = (p2 ± q/2) vF/(kBT), Q = qvF/(kBT), as well as the dimensionless change in the electron current Dnee = (k1+/k1+ + k2–/k2–) – (k1–/k1– + k2+/k2+); q1± and q2± are the angles between k1+ and k1– and between k2+ and k2–,
Intraband Dynamic Conductivity General Equations
respectively, F(x) = {1 + exp[x – eF/(kBT)]}–1 is the Fermi function of dimensionless argument. At the frequencies exceeding the carrier collision frequency w v, the contributions to the real part of dynamic conductivity from different scattering mechanisms are summed up. The intraband conductivity due to eh collisions is given by expression similar to (9–10), with several differences. First, the change in current carried by electron and hole is given by Dneh = (k1+/k1+ – k2–/k2–) – (k1–/k1– – k2+/k2+) as the charge of hole is opposite to that of electron. Second, along with ‘simple’ electronhole scattering, the annihilationtype interaction between electron and hole is also possible. In such process, electron and hole annihilate, emit a virtual photon, which produces again an electronhole pair. The probability of such process is the same as of scattering process, but the overlap factors u(pe)u(pe) = cos(q ij/2) should be changed to u(pe)u(ph) = sin(q ij)[17]. i
j
i
j
As a result, the electronhole scattering contribution to the optical conductivity becomes Res eh = s q
Ieh,w =
Ú
¥ d [k1+
3 Ê w ˆ ˘ 2a c2 Ê kBT ˆ È Í1  exp Á ˙ Ieh,w , ˜ 3 Á Ë kBT ˜¯ ˚˙ p Ë w ¯ ÎÍ
dQdk 1 dk 2
(23.11)
( Dneh )2[cos2 (q1± /2)cos2 (q2± /2) + sin2 (q1± /2)sin2 (q2± /2)] Q2k 2 + k2 + w/(kBT )  k1  k2+ ]F (k1+ )F (k2 )[1  F (k1 )][1  F (k2+ )].
(23.12)
Accordingly, the net intraband conductivity due to cc collisions Resintra in symmetrically pumped graphene is Res cc = s q
3 Ê w ˆ ˘ 2a c2 Ê kBT ˆ È 1 exp Í ˙ (Iee,w + Ieh,w ). Á ˜ Á Ë kBT ˜¯ ˚˙ p 3 Ë w ¯ ÎÍ
(23.13)
Here we have noted that hh scattering contribution equals ee contribution. The coefficient of radiation absorption is readily obtained from Eq. (23.13) timing it by 4p/c. The dimensionless ‘collision integrals’ Iee,w and Ieh,w are given by Eqs. (23.10) and (23.12). They can be evaluated numerically passing to the elliptic coordinates [9]. In those coordinates, the deltafunction can be analytically integrated, reducing the dimensionality of integral by unity. This procedure is described in Appendix.
415
416
CarrierCarrier Scattering and Negative Dynamic Conductivity
23.3 Analysis of Intraband and Net Dynamic Conductivity It is natural that the obtained expression (23.13) for the real part of conductivity is proportional to the universal ac conductivity of clean undoped graphene sq, and the square of the coupling constant ac. The latter characterizes the strength of Coulomb interaction between carriers in graphene. The frequency behavior of Rescc follows the wellknown Drudelike dependence w–2. At frequencies ℏw kBT, the prefactor before the collision integral in Eq. (23.13) yields the w–2dependence. At large frequencies ℏw ≥ kBT, the pre factor behaves as w–3, but the “collision integrals” Iee,w and Ieh,w grow linearly due to the increasing number of final states.
Figure 23.2 Real parts of the intraband (upper panels) and interband (lower panels) contributions, Resintra and Resinter, to dynamic conductivity normalized by sq at different quasiFermi energies ef in graphene structures with different background dielectric constants k0 (T = 300 K).
In what follows, we shall study the dynamic conductivity of sufficiently clean pumped graphene. In this situation, the positive intraband conductivity is due to carriercarrier collisions only, thus Resintra = Rescc. Figure 23.2 shows the dependences of Resintra given by Eq. (23.13) (normalized by sq) on frequency w/2p for the symmetrically pumped graphene at different quasiFermi energies eF and different background dielectric constants k0 at room temperature T = 300 K. In Fig. 23.2, we also show the frequencydependent real part of the dynamic conductivity associated with the interband transitions [11]: Ê w / 2  e F ˆ Res inter = s q tanh Á . Ë 2kBT ¯˜
(23.14)
Analysis of Intraband and Net Dynamic Conductivity
From Fig. 23.2 one can see that at frequencies above ~ 6.5 THz at k0 = 1 (and above ~ 2.5 THz at k0 = 20) the Drude conductivity due to cc collisions lies below sq. Accordingly, the net conductivity Re(sintra + sinter) can be negative in this frequency range at some level of pumping. As the background dielectric constant k0 is increased, the intraband conductivity due to cc collisions drops, which is illustrated in Fig. 23.2. Ex facte, one could expect that it scales as k 02 , and increasing the dielectric constant one could reduce the radiation absorption due to cc collisions almost to zero. Such considerations are actually irrelevant due to screening. The ThomasFermi screening momentum in pumped graphene is given by qTF ª 8a c
Ê e ˆ˘ kBT È ln Í1 + exp Á F ˜ ˙ . vF Ë kBT ¯ ˙˚ ÍÎ
(23.15)
Thus, at small momenta q the Coulomb scattering matrix element is independent of k0. At large momenta q ≈ eF/vF the scattering matrix element VC2 (kF ) µ [k 02 + 8e2/(vF )]2 , which slightly depends on k0 due to large value of bare coupling constant e2/ℏvF ≈ 2.2. In Fig. 23.3 we show the net dynamic conductivity including interband and intraband cc contributions. At weak pumping (ef ≃ 20 meV) the negative dynamic conductivity is attainable only in graphene clad between highk substrates. At elevated pumping (ef ≃ 40 meV) the negative conductivity is possible at any value of k0. Further increase in the pumping level is not much efficient as the interband conductivity reaches its maximum value of sq at eF ℏw, while the intraband conductivity continues to grow with increasing eF .
Figure 23.3 Real parts of net dynamic conductivity Re(sintra + sinter) normalized by sq at different quasiFermi energies ef in graphene structures with different background dielectric constants k0 (T = 300 K).
417
418
CarrierCarrier Scattering and Negative Dynamic Conductivity
Both the interband and intraband cc conductivities are actually functions of two dimensionless combinations ℏw/kBT and eF/ kBT. Once the temperature is reduced, Resintra drops as well due to reduced phase space for collisions near Fermisurface. The dependence Resinter(w) becomes more abrupt in the vicinity of interband threshold ℏw = 2eF . Thereby, cooling of graphene sample is advantageous for achieving the negative dynamic conductivity. This is confirmed by Fig. 23.4. In Figs. 23.4a and b, we show the real part of the net dynamic conductivity versus frequency w/2p and quasiFermi energy eF (values of Res are marked by colors) at the room temperature T = 300 K (A) and at T = 200 K (B). It is worth noting that the temperature T in the above equations is in fact the effective temperature of the electronhole system. Therefore, the reduction of this temperature can be achieved not only by decreasing of the ambient temperature, but also by direct cooling of this system at a certain pumping conditions. In particular, the cooling of electronhole system in the optically and electrically pumped graphene lasing structures due to the emission of optical phonons can be substantial [5, 27].
Figure 23.4 Map of real part of net dynamic conductivity Re(sintra + sinter)/sq vs frequency and quasiFermi energy for k0 = 5: (A) at T = 300 K and (B) at T = 200 K. The area Re(sintra + sinter)/sq < – 0.75 is filled in solid color.
In Fig. 23.5a we show the threshold lines of the negative net dynamic conductivity [which are solutions of the equation Res (w, eF) = 0] at different values of background dielectric constant. The normalized threshold frequency ℏw0/kBT slowly moves to lower values as k0 increases. This is illustrated in Fig. 23.5b. At
Analysis of Intraband and Net Dynamic Conductivity
room temperature and k0 = 1, the negative conductivity could be attained only at frequencies w/2p ≥ 6.5 THz. For graphene on SiO2 substrate [k0 = (kSiO2 + 1)/2 = 2.5], the room temperature threshold lies at w0/2p ª 6 THz. As discussed before, such slow decrease in threshold frequency is owing to the ThomasFermi screening of Coulomb interaction. Note that screening can be further enhanced by placing graphene close to the metal gate. In gated graphene, the Fourier component of Coulomb scattering potential VC(q) gains an additional factor [1 – exp(–2qd)], where d is the distance to the gate.
Figure 23.5 (A) Thresholds of negative dynamic conductivity at different values of background dielectric constant k0. Solid lines correspond to Re(sintra + sinter) = 0. (B) Threshold frequencies wo/2p vs background dielectric constant at different temperatures T (eF = 3kBT).
Figure 23.6 Real parts of intraband dynamic conductivity Resintra (solid lines) and interband conductivity –Resinter (dashed line) as functions of quasiFermi energy eF at fixed frequency w/(2p) = 6 THz and different values of background dielectric constant k0.
419
420
CarrierCarrier Scattering and Negative Dynamic Conductivity
The dependences of the inter and intraband (carriercarrier) conductivities on the quasiFermi energy at fixed frequency are shown in Fig. 23.6. The interband conductivity reaches its ultimate value of sq at eF ℏw/2. Intuitively, Resintra and the corresponding radiation absorption coefficient should be proportional to the number of particleparticle collisions in unit time. This number is proportional to the carrier density squared, at least for classical carrier systems. In reality, the dependence of Resintra on the quasiFermi energy eF appears to be almost linear. This, first of all, results from the screening and also from the restricted phase space for collisions in Fermisystems in a narrow layer near the Fermisurface.
23.4 Discussion of the Results
The obtained relation for the intraband conductivity associated with the cc scattering (Eq. (23.13)) corresponds to a Drudelike dependence Resintra µ w–2. The latter tends to infinity at small frequencies. This tendency should be cut off at w ~ v, where v is the electron collision frequency. At such small frequencies, the finite lifetime of quasiparticles leads to inapplicability of the Fermi golden rule. However, one can estimate the carriercarrier collision frequency and the corresponding lowfrequency conductivity by solving the kinetic equation for the massless electrons in graphene. We have generalized the variational approach to the solution of kinetic equation [28] developed in [16, 17] for intrinsic graphene, to the case of symmetrically pumped graphene. As a result, the following lowfrequency dependence of intraband conductivity due to cc scattering was obtained: Res intra =
Ê e ˆ˘ v 2e2 kBT È ln Í1 + exp Á F ˜ ˙ 2 cc 2 , p Ë kBT ¯ ˚˙ w + vcc ÎÍ
(23.16)
where the carriercarrier collision frequency vcc includes the contributions from the ee and eh scattering vcc =
a c2 kBT 4p 2
Iee,0 + Ieh,0
È Ê e ˆ˘ ln Í1 + exp Á F ˜ ˙ Ë kBT ¯ ˚˙ ÍÎ
,
(23.17)
Discussion of the Results
and the “zero” index at dimensionless collision integrals means that they are taken at w = 0. At intermediate frequencies vcc w £ kBT/ℏ, the results obtained from the kinetic equation (Eq. (23.16)) and the Fermi golden rule (Eq. (23.13)) coincide. At room temperature, zero Fermi energy, and background dielectric constant k0 = 1, the characteristic collision frequency is equal to vcc ª 1013 s–1. Once k0 or ef are increased, the collision frequency decreases due to screening of the Coulomb potential. Hence, for the ‘target’ frequencies w/(2p) = 5 – 10 THz one can readily use the golden rule result (Eq. (23.13)) to evaluate the carriercarrier scattering contribution to the optical conductivity. Until now we considered the intraband conductivity due to the cc collisions only, as if other scattering processes were removed. In realty, the acoustic phonon contribution is unavoidable as well. The corresponding collision frequency can be presented as (t p1 )ph = v0 ( pvF /kBT), where v0 ≃ 3 ¥ 1011 s–1 at room temperature [29]. Thus, at least for not very large values of k0, the cc scattering contribution to intraband conductivity appears to be larger than the acoustic phonon contribution. The momentum relaxation time due to scattering by randomly distributed charged impurities with average density ni is
( )
t p1 i = 2pa c2
pvF 2ni 2 qTF
Ú
p
sin2 q dq
. (23.18) 2 ÈÎ1 + (2p /qTF ) sin (q / 2)˘˚ The estimates for intrinsic graphene at room temperature, k0 = 1, impurity density ni = 1011 cm–2 and electron energy equal to the thermal energy (pvF = kBT) yield the electronimpurity collision 0
frequency (t p1 )i ª 7 ¥ 1012 s1 , which is of the same order as the carriercarrier collision frequency, and scales linearly with ni. To obtain the real part of the net intraband dynamic conductivity, one should sum the collision frequencies due to various scattering mechanisms. The presented analysis shows that the carriercarrier scattering contribution cannot be neglected in the case of intrinsic or symmetrically pumped graphene. In our estimates for the Coulomb scattering probability, we have used the static (ThomasFermi) approximation for dielectric function of graphene. The use of the dynamic dielectric function can be mandatory to avoid the divergence in collision integrals for
421
422
CarrierCarrier Scattering and Negative Dynamic Conductivity
collinear scattering [9]. However, in Eqs. (23.10) and (23.12) such a divergence does not appear due to the presence of factor Dn2. The difference between Resintra obtained using static and dynamic screening is below 10%. As known, the ee and hh scattering does not lead to the finite resistivity and the absorption of radiation by the carriers with the parabolic dispersion law (in the absence of umklapp processes [28]). In graphene, such an effect is possible due to the momentumvelocity decoupling. Formally, ee collisions in pumped graphene are of the same “strength” as eh collisions (see Eqs. (23.9) and (23.11)). However, the numerical comparison of Eqs. (23.9) and (23.11) shows that the ee and hh collisions play a minor role in the radiation absorption in the pumped graphene. The major contribution to Rescc comes from the electronhole collisions, while Resee actually constitutes less than 10% of Rescc (see Fig. 23.7a). This can be understood by analyzing the change in current in a single collision act. The corresponding change is given by the terms (Dnee)2 and (Dneh)2 in Eqs. (23.10) and (23.12). Expanding in powers of q and averaging over directions, one obtains (Dnee )2 µ q2 (k11  k21 )2 and (Dneh )2 µ q2 (k11 + k21 )2 . The latter implies that collisions of electrons with sufficiently different energies only play significant role in the ee and hh scatteringassisted absorption. For electronhole collisions there is no such a restriction.
Figure 23.7 Separate contributions of eh, ee, and hh scattering processes to real part of interband conductivity: (A) for pumped graphene and (B) for electrondoped graphene in thermodynamic equilibrium (k0 = 1, w/2p = 6 THz, and T = 300 K).
For the electronhole system in equilibrium, the relative contributions of ee and eh scattering to the intraband conductivity
Conclusions
are much different (see Fig. 23.7b). The hh and eh contributions drop quickly with increasing the Fermi energy due to vanishingly small number of holes. The remaining part of intraband conductivity due to the ee collisions is of order of 0.1sq at w/(2p) = 6 THz and k0 = 1. The corresponding contribution to radiation absorption can be in principle detected for rather clean samples. Recent experiments have shown that the THz radiation gain in the pumped graphene can greatly exceed 2.3% [30]. This phenomenon is attributed to the selfexcitation of surface plasmonpolaritons in electronhole system with population inversion [31]. The threshold of plasmon selfexcitation in the pumped graphene is also governed by the ratio of the negative interband and positive intraband conductivities. The latter results mainly from the eh collisions [18]. The presented calculations show that terahertz plasmons are rather amplified than damped in the pumped graphene, at least at high pumping levels and large background dielectric constants.
23.5 Conclusions
We have shown that in graphene there exists a strong mechanism of the intraband Drudelike radiation absorption, assisted by the carriercarrier collisions. In such a process, a carrier absorbs a photon and transfers the excess energy and momentum to the other carrier, electron or hole. The radiation absorption assisted by the electronelectron and holehole collisions is possible only in semiconductors with nonparabolic bands, and graphene (with its linear energy spectrum of electrons and holes) is one of brightest representatives of such a family. We have evaluated the carriercarrier scattering contribution to the intraband conductivity using the secondorder perturbation theory and the Fermi golden rule. As demonstrated, the radiation absorption due to the carriercarrier collisions can markedly surpass the Drude absorption due to the scattering on thermal or static disorder. This is especially pronounced in the pumped graphene with a large number of carriers in both bands. We have studied the effect of carriercarrier scattering on the conditions of the negative dynamic conductivity in pumped graphene by comparing the positive intraband dynamic conductivity due to the carriercarrier collisions and the negative interband
423
424
CarrierCarrier Scattering and Negative Dynamic Conductivity
conductivity. We have shown that at room temperature, the net negative dynamic conductivity is attainable at frequencies above ~6.5 THz in suspended graphene. This frequency threshold can be shifted to lower values (~2.5 THz at room temperature) for graphene on highk substrates, as the presence of dielectric partially screens the Coulomb interaction. Cooling of the electronhole system also reduces the negative conductivity threshold. Our results show that screening of Coulomb interaction by carriers in graphene itself (ThomasFermi screening) significantly affects the real part of intraband conductivity. Due to the screening, the cc contribution to the intraband conductivity grows slowly (almost linearly) with increasing quasiFermi energy of nonequilibrium electrons and holes.
Appendix: Evaluation of Coulomb Integrals
We introduce the dimensionless energies of incident particles e1 = k1+ and e2 = k2–, and the transferred energy de = k1+ – k1– – w/2 = k2+ – k2– – w/2. Here, for brevity, w = ℏw/(kBT). The kernel of the ee Coulomb integral depends only on those energies and the transferred momentum Q:
Ú
Cee (e1, e2,de , Q ) = dk 1dk 2 (Dnee )2 cos2 (q1± /2)cos2 (q2± /2)d (e1  k1+ )d (e 2  k2 ) ¥d [de  (k2+  k2  w/2)]d [de  (k1+  k1 + w/2)].
In these notations, Iee,w is rewritten as •
Iee,w =
de max
QdQ
Ú (Q + Q ) Ú 2
w/2
TF
de min
•
dde
Ú
e1min
(23.19)
•
de1
Ú
de 2Cee (e1 , e 2 ,de , Q)F (e1 )F (e 2 )
e2min
¥[1  F(e 2 + de + w/2)][1  F(e1  de + w/2)].
(23.20)
The limits of integration will be found further. In elliptic coordinates the Coulomb kernel is evaluated analytically. The change of variables is (i = 1, 2)
Q (23.21) {coshui cos vi , sinhui sin vi } , 2 where ui > 0, and –p < vi < p. The product of four deltafunctions in Eq. (23.19) can be rewritten as ki =
Appendix
w/2  de + 2e1 ˆ Ê de + w/2ˆ Ê de  w/2 ˆ Ê d Á cosv2 d Á cos v1 d Á cosh u1 ˜¯ ˜ ˜ ¯ Ë ¯ Ë Q Q Q Q Ë 4
4
w/2 + de + 2e2 ˆ Ê ¥d Á coshu2 . ¯˜ Ë Q
(23.22)
Considering the arguments of deltafunctions in Eq. (23.22), one finds the limits of integration over energies in Eq. (23.20) from general requirements coshui > 1, cos vi < 1, i = 1, 2: e1 >
(Q + de  w/2) ;e 2
2
>
(Q  de  w/2) ,Q > w/2; Q + w/2 < de < Q  w/2. 2
(23.23)
Integration over du1, du2, dv1, and dv2 removes the deltafunctions, and the Coulomb kernel becomes 4 ( Dn )
cos2 (q1± /2) cos2 (q2± /2)
Q4
u1 sinh u2 sin v1 sin v2 sinhu
2
C(e1 , e2 ,de , Q) =
k1+ k1 k2+ k2 .
(23.24)
Here the sin and sinhterms in the denominator appear from the rule d [f(x)] = Si f¢(xi)–l d(x – xi), where the summation is performed over all zeros xi of f(x). In Eq. (23.24) k1+k1–k2+k2– is the Jacobian determinant for elliptic coordinates. The envelope function overlap factors are also concisely expressed in the elliptic coordinates: cos2 (q1± /2)cos2 (q2± /2)k1+ k1 k2+ k2
1 2e 2 + de + w/2)2  Q2]. (23.25) [(2e1  de + w/2)2  Q2][(2 16 As a result, the Coulomb kernel takes on the following form: =
Cee (e1 , e 2 ,de , Q ) =
=
( Dn )2ee 4
( Dn )2ee sinhu1 sinhu2 4
sin v1 sin v2
È(2e  de + w/2)2  Q2 ˘[(2e + de + w/2)2  Q2 ] 2 ÍÎ 1 ˚˙ . [Q2  (de + w/2) ][Q2  (de  w/2) ] 2
2
(23.26)
The expression for (Dn)2ee in elliptic coordinates is quite lengthy, here we present in only in the limit w Æ 0:
425
426
CarrierCarrier Scattering and Negative Dynamic Conductivity
(Dn)2ee =
(
2 Q2  de 2
)
e1e2 (e1  de )(de + e2 )
È de 2 (de  2e1 )(de + 2e2 ) ˘ ˙. (23.27) ¥ Íde 2 + 4de(e2  e1 ) + 2(e1  e 2 )2 Q2 ÍÎ ˙˚
Note that Eq. (23.26) contains the denominator divergent at w Æ 0, which manifests the collinear scattering anomaly for massless particles [9, 16, 17]. This divergence is removed by the similar term in the expression for (Dn)2ee , which stands in the numerator.
Acknowledgments
The authors are grateful to M. Ryzhii for useful comments. The work at RIEC was supported by the Japan Society for Promotion of Science (GrantinAid for Specially Promoting Research #23000008), Japan. The work at IPT RAS was supported by the Russian Foundation of Basic Research (grant #140700937). The work by D.S was also supported by the grant of the Russian Foundation of Basic Research #140731315 and by the JSPS Postdoctoral Fellowship For Foreign Researchers (Shortterm), Japan.
References
1. F. Bonaccorso, Z. Sun, T. Hasan, and A. C. Ferrari, Graphene photonics and optoelectronics, Nat. Photonics, 4, 611–622 (2010).
2. A. Tredicucci and M. S. Vitiello, Device concepts for graphenebased terahertz photonics, IEEE J. Sel. Top. Quantum Electron., 20, 8500109 (2014). 3. P. Weis, J. L. GarciaPomar, and M. Rahm, Towards loss compensated and lasing terahertz metamaterials based on optically pumped graphene, Opt. Express, 22(7), 8473–8489 (2014).
4. A. Dubinov, V. Ya. Aleshkin, M. Ryzhii, T. Otsuji, and V. Ryzhii, Terahertz laser with optically pumped graphene layers and FabriPerot resonator, Appl. Phys. Express, 2, 092301 (2009).
5. V. Ryzhii, M. Ryzhii, V. Mitin, and T. Otsuji, Toward the creation of terahertz graphene injection laser, J. Appl. Phys., 110, 094503 (2011).
References
6. V. Ryzhii, A. Dubinov, T. Otsuji, V. Ya. Aleshkin, M. Ryzhii, and M. Shur, Doublegraphenelayer terahertz laser: concept, characteristics, and comparison, Opt. Express, 21(25), 31567–31577 (2013).
7. S. BoubangaTombet, S. Chan, T. Watanabe, A. Satou, V. Ryzhii, and T. Otsuji, Ultrafast carrier dynamics and terahertz emission in optically pumped graphene at room temperature, Phys. Rev. B, 85, 035443 (2012).
8. M. Martl, J. Darmo, C. Deutsch, M. Brandstetter, A. M. Andrews, P. Klang, G. Strasser, and K. Unterrainer, Gain and losses in THz quantum cascade laser with metalmetal waveguide, Opt. Express, 19, 733 (2011). 9. D. Brida, A. Tomadin, C. Manzoni, Y. J. Kim, A. Lombardo, S. Milana, R. R. Nair, K. S. Novoselov, A. C. Ferrari, G. Cerullo, and M. Polini, Ultrafast collinear scattering and carrier multiplication in graphene, Nat. Commun., 4, article number: 1987 (2013).
10. K. F. Mak, M. Y. Sfeir, Y. Wu, C. H. Lui, J. A. Misewich, and T. F. Heinz, Measurement of the optical conductivity of graphene, Phys. Rev. Lett., 101, 196405 (2008).
11. V. Ryzhii, M. Ryzhii, and T. Otsuji, Negative dynamic conductivity of graphene with optical pumping, J. Appl. Phys., 101, 083114 (2007).
12. L. Ren, Q. Zhang, J. Yao, Z. Sun, R. Kaneko, Z. Yan, S. Nanot, Z. Jin, I. Kawayama, M. Tonouchi, J. M. Tour, and J. Kono, Terahertz and infrared spectroscopy of gated largearea graphene, Nano Lett., 12, 3711–3715 (2012). 13. A. Satou, V. Ryzhii, Y. Kurita, and T. Otsuji, Threshold of terahertz population inversion and negative dynamic conductivity in graphene under pulse photoexcitation, J. Appl. Phys., 113, 143108 (2013).
14. J. M. Dawlaty, S. Shivaraman, M. Chandrashekhar, F. Rana, and M. G. Spencer, Measurement of ultrafast carrier dynamics in epitaxial graphene, Appl. Phys. Lett., 92, 042116 (2008).
15. M. Mittendorff, T. Winzer, E. Malic, A. Knorr, C. Berger, W. A. de Heer, H. Schneider, M. Helm, and S. Winnerl, Anisotropy of excitation and relaxation of photogenerated charge carriers in graphene, Nano Lett., 14(3), 1504–1507 (2014).
16. A. B. Kashuba, Conductivity of defectless graphene, Phys. Rev. B, 78, 085415 (2008).
17. L. Fritz, J. Schmalian, M. Müller, and S. Sachdev, Quantum critical transport in clean graphene, Phys. Rev. B, 78, 085416 (2008).
427
428
CarrierCarrier Scattering and Negative Dynamic Conductivity
18. D. Svintsov, V. Vyurkov, S. Yurchenko, V. Ryzhii, and T. Otsuji, Hydrodynamic model for electronhole plasma in graphene, J. Appl. Phys., 111(8), 083715 (2012).
19. M. Schütt, P. M. Ostrovsky, I. V. Gornyi, and A. D. Mirlin, Coulomb interaction in graphene: relaxation rates and transport, Phys. Rev. B, 83, 155441 (2011).
20. V. N. Kotov, B. Uchoa, V. M. Pereira, F. Guinea, and A. H. Castro Neto, Electronelectron interactions in graphene: current status and perspectives, Rev. Mod. Phys., 84, 1067 (2012).
21. L. A. Falkovsky and S. S. Pershoguba, Optical farinfrared properties of a graphene monolayer and multilayer, Phys. Rev. B, 76, 153410 (2007). 22. F. T. Vasko, V. V. Mitin, V. Ryzhii, and T. Otsuji, Interplay of intra and interband absorption in a disordered graphene, Phys. Rev. B, 86, 235424 (2012).
23. D. Sun, C. Divin, M. Mihnev, T. Winzer, E. Malic, A. Knorr, J. E. Sipe, C. Berger, W. A. de Heer, and P. N. First, Current relaxation due to hot carrier scattering in graphene, New J. Phys., 14, 105012 (2012).
24. G. G. Zegrya and V. E. Perlin, Intraband absorption of light in quantum wells induced by electronelectron collisions, Semiconductors, 32, 417–422 (1998).
25. E. H. Hwang and S. Das Sarma, Dielectric function, screening, and plasmons in twodimensional graphene, Phys. Rev. B, 75, 205418 (2007). 26. L. D. Landau and E. M. Lifshitz Quantum Mechanics (Pergamon Press, 1965).
27. V. Ryzhii, M. Ryzhii, V. Mitin, A. Satou, and T. Otsuji, Effect of heating and cooling of photogenerated electronhole plasma in optically pumped graphene on population inversion, Jpn. J. Appl. Phys., 50, 094001 (2011). 28. J. M. Ziman, Electrons and Phonons (Oxford University Press, 1960).
29. F. T. Vasko and V. Ryzhii, Voltage and temperature dependencies of conductivity in gated graphene, Phys. Rev. B, 76, 233404 (2007). 30. T. Watanabe, T. Fukushima, Y. Yabe, S. A. Boubanga Tombet, A. Satou, A. Dubinov, V. Ya. Aleshkin, V. Mitin, V. Ryzhii, and T. Otsuji, The gain enhancement effect of surface plasmon polaritons on terahertz stimulated emission in optically pumped monolayer graphene, New J. Phys., 15, 075003 (2013).
31. A. Dubinov, V. Aleshkin, V. Mitin, T. Otsuji, and V. Ryzhii, Terahertz surface plasmons in optically pumped graphene structures, J. Phys.: Condens. Matter, 23, 145302 (2011).
Chapter 24
Negative Terahertz Conductivity in Disordered Graphene Bilayers with Population Inversion*
D. Svintsov,a T. Otsuji,b V. Mitin,b,c M. S. Shur,d and V. Ryzhiib aLaboratory of Nanooptics and Plasmonics, Moscow Institute of Physics and Technology, Dolgoprudny 141700, Russia bResearch Institute of Electrical Communication, Tohoku University, Sendai 9808577, Japan cDepartment of Electrical Engineering, University at Buffalo, SUNY, Buffalo, New York 1460–1920, USA dDepartments of Electrical, Electronics, and Systems Engineering and Physics, Applied Physics, and Astronomy, Rensselaer Polytechnic Institute, Troy, New York 12180, USA [email protected]
The gapless energy band spectra make the structures based on graphene and graphene bilayer with the population inversion to be promising media for the interband terahertz (THz) lasing. However,
*Reprinted with permission from D. Svintsov, T. Otsuji, V. Mitin, M. S. Shur, and V. Ryzhii (2015). Negative terahertz conductivity in disordered graphene bilayers with population inversion, Appl. Phys. Lett., 106, 113501. Copyright © 2015 AIP Publishing LLC. GrapheneBased Terahertz Electronics and Plasmonics: Detector and Emitter Concepts Edited by Vladimir Mitin, Taiichi Otsuji, and Victor Ryzhii
Copyright © 2021 Jenny Stanford Publishing Pte. Ltd.
ISBN 9789814800754 (Hardcover), 9780429328398 (eBook)
www.jennystanford.com
430
Negative Terahertz Conductivity in Disordered Graphene Bilayers
a strong intraband absorption at THz frequencies still poses a challenge for efficient THz lasing. In this chapter, we show that in the pumped graphene bilayer, the indirect interband radiative transitions accompanied by scattering of carriers by disorder can provide a substantial negative contribution to the THz conductivity (together with the direct interband transitions). In the graphene bilayer on highk substrates with point charged defects, these transitions substantially compensate the losses due to the intraband (Drude) absorption. We also demonstrate that the indirect interband contribution to the THz conductivity in a graphene bilayer with the extended defects (such as the charged impurity clusters) can surpass by several times the fundamental limit associated with the direct interband transitions, and the Drude conductivity as well. These predictions can affect the strategy of the graphenebased THz laser implementation. The absence of a band gap in the atomically thin carbon structures, such as graphene and graphene bilayer, enables their applications in different terahertz (THz) and infrared devices [1–4]. One of the most challenging and promising problems is the creation of the graphenebased THz lasers [5–8]. These lasers are expected to operate at room temperature, particularly, in the 6–10 THz range, where the operation of III–V quantum cascade lasers is hindered by the optical phonons [9]. Recent pumpprobe spectroscopy experiments confirm the possibility of the coherent radiation amplification in the optically pumped graphene [10–16], enabled by a relatively longliving interband population inversion [16]. As opposed to optically pumped graphene lasers, graphene based injection lasers are expected to operate in the continuous mode, with the interband population inversion maintained by the electron and hole injection from the nand ptype contacts [6]. A single sheet of pumped graphene as the gain medium provides the maximum radiation amplification coefficient equal to 4psq/c = pa = 2.3%, where sq = e2/4ℏ is the universal optical conductivity of a single graphene layer, e is the electron charge, ℏ is the Planck constant, and a ≃ 1/137 is the finestructure constant [16]. The THz gain in the graphene bilayer [17] or the nonBernal stacked multiple graphene layers [6] can be enhanced approximately proportional to the number of the layers. However, more crucial is the problem of competition between the interband radiation amplification and
Negative Terahertz Conductivity in Disordered Graphene Bilayers
intraband (Drude) radiation absorption [5, 15, 18]. The latter scales with frequency w approximately as 1/w2t, where t is the momentum relaxation time. Hence, the onset of THz gain is typically believed to occur only in clean samples, where wt 1 [19].
Figure 24.1 Energy band diagram of a graphene bilayer with population inversion (left) and schematic energy dependence of its density of states (right). Arrows indicate possible radiative transitions. Direct interband transitions involve only vertical photon emission (wavy arrow), while indirect emission and absorption processes are accompanied by carrier scattering (straight horizontal arrows).
In this letter, we show that the intraband radiation absorption in disordered graphene bilayer does not actually pose a problem for the THz lasing. On the contrary, the presence of a certain type of defects reinforces the negative contribution to the THz conductivity and, hence, improves the gain properties of the pumped graphene bilayer. The origin of such an effect is associated with the indirect interband radiative transitions (see Fig. 24.1), in which the electrons from the conduction band emit the photons being scattered by the defects, thus contributing to the radiation gain. The inclusion of such processes can be important in the indirectgap materials and gapless semiconductors. However, in singlelayer graphene with charged impurities, the indirect interband processes contribute to the net THz conductivity s only moderately due to a low density of states (DoS) near the band edges [20]. The situation is remarkably different is the intrinsic graphene bilayer, where the electronhole dispersion is gapless and almost parabolic [21]. With constant DoS near the
431
432
Negative Terahertz Conductivity in Disordered Graphene Bilayers
band edges, the indirect interband radiative processes significantly contribute to the net radiation gain (which is proportional to –Re s) under the population inversion conditions. We analyze the spectral dependencies of the real part of the net dynamic THz conductivity Re s in the pumped graphene bilayers for the scattering by the point charged impurities [22, 23] and by the impurity clusters [24, 25]. Our analysis shows that in the first case, the gain due to the indirect interband transitions substantially compensates the losses due to the Drude absorption. In the case of the cluster scattering, the gain due to the indirect interband transitions even exceeds the intraband losses. Depending on the cluster size and their density, the ratio Re s/sq can markedly exceed unity resulting in elevated net THz gain. The real part of the net inplane dynamic THz conductivity, Re s, comprises the contributions of the direct (vertical) interband intra electron transitions, Re sd, and the contributions, Re s ind and inter Re s ind , of two types of the indirect electron transitions (inside both the bands and between the two bands), respectively inter intra Re s = Re s d + Re s ind + Re s ind .
(24.1)
The interband conductivity of graphene bilayers due to the direct transitions is given by [19, 21] Re s d = s Q
w + 2g 1 [ fu ( w / 2)  fc ( w / 2)], w + g 1
(24.2)
where fu(e) and fc(e) are the carrier distribution functions in the valence and conduction bands, and g1 ≃ 0.4 eV is the hopping integral between carbon atoms in adjacent graphene planes [26]. Here and in the following, we assume that fu and fc are the Fermi functions characterized by the quasiFermi energies mu = –eF and mc = eF, respectively. This is justified by strong carriercarrier scattering leading to a fast thermalization of excited carriers [10, 13]. In the THz frequency range of interest, ℏw g1, and the conductivity of bilayer is simply twice as large as that of a single layer. Under the pumping conditions, mc = –mu = eF > 0, and, according to Eq. (24.2), the conductivity is negative for photon energies ℏw below the double quasiFermi energy eF of pumped carriers [17]. To evaluate the real part of the THz conductivity due to the indirect transitions, we calculate the secondorder transition amplitudes for the photon emission (absorption) accompanied
Negative Terahertz Conductivity in Disordered Graphene Bilayers
by the electron scattering and apply the Fermi’s golden rule. As a result, the general expressions for the indirect intra and interband conductivities read as follows: intra Re s in d =
8ps Q w 3
Â [f
l (e k )  f l (e k¢ )]
k ,k ¢ ,l
ll ¥ d (w + e k  e k¢ ) VS ( k  k ¢ )2 ukk¢ ( v k¢  v k )2 , (24.3)
inter Re s ind =
8ps Q w 3
Â [ f (e u
k )  f c (e k¢ )]
k ,k ¢
cu 2 ¥ d (w  e k  e k¢ ) VS ( k  k ¢ )2 ukk ¢ ( v k ¢ + v k ) . (24.4)
Here, l = ±1 is the index corresponding to the conduction and valence bands, v k = 2u02 k/g 1 is the electron velocity in the graphene bilayer, u0 ≃ 108 cm/s is the velocity characterizing the energy spectra of graphene and graphene bilayer, VS(q) is the qth Fourier component ll ¢ of the scattering potential, and ukk ¢ = (1 + ll¢ cos 2qkk¢)/2 is the overlap between the envelope wave functions in graphene bilayers. For a correct qualitative description of the lowfrequency conductivity, we replace the frequency w in the denominators of Eqs. (24.2) and (24.3) with (w2 + t–2)1/2, where t is given by t 1 =
2p
Â V (k  k ¢) (1  cos q 2
S
2 kk ¢ ) cos q kk ¢ d (e k
 e k ¢ ).
k¢
Equation (24.3) yields the wellknown result for the dynamic conductivity in the highfrequency limit w t–1. In the most practical situations, the Coulomb scattering by the substrateinduced charged impurities is the main factor determining the conductivity [27]. Considering impurities as random uncorrelated point scatterers with the average density ni, we write the scattering matrix element as [28] 2
È 2p e2 ˘  VS (q)2 = ni Í ˙ , ÎÍk (q + qs ) ˚˙
(24.5)
where k is the background dielectric constant and qs is the ThomasFermi screening wave vector [30]. Using the Lindhard type formula for the graphene bilayer polarizability [28] with the quasiequilibrium Fermi functions for the conduction and valence
433
434
Negative Terahertz Conductivity in Disordered Graphene Bilayers
bands, we obtain qs = 4acg1(1 – ln2)/ℏ u0, where ac = e2/ℏk u0 is the coupling constant. Evaluating the integral in Eq. (24.4), we find the scatteringassisted interband conductivity inter Re s ind � 8pa c2s Q
u02ni
(w + t 2 ) 2
Ê �w  2e F ˆ Ê �u0qs ˆ ¥ tanh Á FÁ ˜, Ë 4T ˜¯ Ë �w wg 1 ¯ where F(x) =
Ú
2
0
(24.6)
dy (1 – 1 – y)(1 – y/2)/(y1/2 + x)2 with the
following asymptotes: F(x) ª 2ln2 – 1/2, x 1, F(x) ª 1/(2x2), x 1. At intermediate frequencies, 1/t w ℏ(u0qs)2/g1, the conductivity due to the indirect interband transitions scales as w–1. This is substantially different from the case of a single graphene layer, where it tends to a constant. A pronounced increase in the indirect interband contribution to the dynamic conductivity in a bilayer at low frequencies is attributed to the constant density of states in the vicinity of the band edges. Figure 24.2 (upper panel) shows the spectral dependences of different contributions to the dynamic THz conductivity as well its net value for a moderatequality exfoliated graphene bilayer [23] on the SiO2 substrate with impurity density ni = 5 ¥ 1011 cm–2, at temperature T = 300 K, and for the quasiFermi energy eF = 60 meV (t = 5 ¥ 10–14 s). The bottom panel in Fig. 24.2 demonstrates the twodimensional maps of the dynamic THz conductivity versus the frequency and the quasiFermi energy for the same structure. As seen, the contribution of the indirect interband transitions in such a sample is still weaker than those of both the indirect intraband and direct interband transitions, although the former is essential for compensating, to some extent, the Drude absorption. This enables an increase in Res and some widening of the frequency range where Re s < 0. As follows from Fig. 24.2 (bottom panel), the dynamic THz conductivity is negative at eF ≳ 30 meV and w/2p ≳ 10 THz. The relative contribution of the indirect interband transitions (compared to the “normal” intraband conductivity) increases with an increasing dielectric constant. Figure 24.3 shows the same characteristics as in Fig. 24.2, for a graphene bilayer being clad by the HfO2 layers, i.e., immersed in a media with a fairly high dielectric
Negative Terahertz Conductivity in Disordered Graphene Bilayers
Figure 24.2 Contributions of different radiative transitions to the dynamic conductivity of a graphene bilayer on SiO2 (k = 2.5) and its net value (solid line) versus frequency for ni = 5 ¥ 1011 cm–2 and eF = 60 meV (upper panel) and the eF – w map of the dynamic conductivity (bottom panel). Numbers above the lines indicate the values of Re [s/sq]. The region above the white dashed line corresponds to the negative dynamic conductivity.
constant (k = 20, ni = 5 ¥ 1011 cm–2, and t = 5 ¥ 10–13 s). As seen from Fig. 24.3, the transition to the graphene bilayer structures with higher dielectric constant leads to a much stronger contribution of the indirect interband transitions and, hence, to a much larger value of Re s. It is important to note that an increase is in the relative contribution, as the absolute values of both contributions go down at larger k. The comparison of Figs. 24.2 and 24.3 shows that the ratio Re s/sq for the minimum value of Re s at k = 20 is fivesix time larger than that for k = 2.5. Moreover, in the former case Re s becomes negative starting from eF = 20 meV and w/2p ≳ 5 THz. At
435
436
Negative Terahertz Conductivity in Disordered Graphene Bilayers
higher values of eF (i.e., at a stronger pumping), Re s can be negative from the frequencies of about a few THz to a dozen THz.
Figure 24.3 Same as in Fig. 24.2 but for graphene bilayer clad by HfO2 layers (k = 20).
The reinforcement of the negative dynamic THz conductivity effect with increasing background dielectric constant demonstrated above is interpreted as follows. An increase in k results in the reduced the ThomasFermi wave vector qs. This, in turn, leads to the switching from the strongly screened to almost bare Coulomb scattering. From the energy conservation laws (see Eqs. (24.3) and (24.4)), it follows that the indirect interband electron transitions are favored by a low momentum transfer q, while for the indirect transitions within one band q should be large, namely, q > w/u0 as the electron velocity in graphene bilayer does not exceed u0. Hence, for high values of k, the scattering potential behaves approximately
Negative Terahertz Conductivity in Disordered Graphene Bilayers
as VS(q) µ 1/q, which supports the interband transitions with a low momentum transfer. As shown above, the Coulomb scattering by the screened point defects cannot lead to the dominance of the indirect interband transitions over the indirect intraband ones. However, such a dominance can be realized in the case of the carrier scattering by extended scatterers. We consider the charged cluster of size lc and charge Ze as a continuous twodimensional distribution of charge density r(r) = Ze exp (r 2/ lc2 )/ plc2 (we assume it to be Gaussian [25]). Solving the Poisson equation for this charge density and averaging over the random positions of the clusters with the average density nc, we readily find the scattering matrix elements (instead of Eq. (24.5)) 2
Ê q2lc2 ˆ
È 2p Ze 2 ˘
(24.7)
 VS (q) = n c Í ˙ exp Á 
˜ .
k ( q + qs ) ˙˚ � Ë 2 ¯ � ÍÎ � In the limit of strong screening, q qs, our model of scattering coincides with the widely accepted model of the “Gaussian correlated disorder” [29–31] with the rootmeansquare scattering potential 2
V 2 ª 2p n c /p lc2 Ze 2/kqs . Figure 24.4 shows the spectral characteristics of the dynamic THz conductivity in the pumped graphene bilayer (eF = 60 meV) with clusters of charged impurities with different size lc. If the scattering by the charged clusters is a dominating mechanism, the absolute value of the net dynamic THz conductivity, Res, can markedly exceed the fundamental “direct interband limit” of 2sQ. At reasonable values of lc ≳ 8 nm and quasiFermi energy eF = 60 meV, one obtains Re s> 4sQ. Above, we disregarded the processes of the radiative transitions accompanied by the electron and hole scattering by neutral point defects (with a shortrange scattering potential). Such processes intra inter contribute to both Re s ind and Re s ind although the relative contribution of the latter is small (≲/ℏw/4eF). Hence, the obtained results are valid when the scattering by neutral point defects is weak compared with the scattering by charges objects (as well as by neutral but largescale imperfections). In graphene bilayer with a large twist, the carrier spectrum is linear [32], and the optical conductivity is given by the expressions obtained for single layer
437
438
Negative Terahertz Conductivity in Disordered Graphene Bilayers
[20] with the renormalized band velocity u0. The crossover between the parabolic and linear energy spectra at intermediate twisting angles requires a separate study.
Figure 24.4 Net dynamic THz conductivity versus frequency calculated for graphene bilayer on SiO2 with impurity clusters of different size lc: cluster density and charge are nc = 1011 cm–2 and Z = 7, effective dielectric constant k = 2.5, and quasiFermi energy eF = 60 meV.
In conclusion, we have demonstrated that the graphene bilayer with a longrange disorder (the nanometrescale impurity clusters) can exhibit a strong negative THz conductivity with the span two times or more exceeding the fundamental limit 2sq. This effect is associated with the indirect interband transitions with the photon emission being accompanied by the disorder scattering. For the indirect interband photon emission to dominate over the “normal” Drude absorption, the longwave length Fourier components of the scattering potential should prevail. Such kind of scattering potentials can be formed also by extended surface corrugations (wrinkles), multilayer patches, grain boundaries, quantum dots on the graphene bilayer surface [33, 34], and nanohole arrays [35, 36]. The work was supported by the Japan Society for Promotion of Science (GrantinAid for Specially Promoted Research No. 23000008) and by the Russian Scientific Foundation (Project No. 142900277) and the grant of the Russian Foundation of Basic Research
References
No. 140731315. The works at UP and RPI were supported by the U.S. Air Force Award No. FA9550101391 and by the U.S. Army Research Laboratory Cooperative Research Agreement, respectively.
References
1. A. H. Castro Neto, F. Guinea, N. M. R. Peres, K. S. Novoselov, and A. K. Geim, Rev. Mod. Phys., 81, 109 (2009). 2. A. Tredicucci and M. Vitiello, IEEE J. Sel. Top. Quantum. Electron, 20, 130 (2014).
3. Q. Bao and K. P. Loh, ACS Nano, 6, 3677 (2012).
4. F. Bonaccorso, Z. Sun, T. Hasan, and A. Ferrari, Nat. Photonics, 4, 611 (2010).
5. V. Ryzhii, M. Ryzhii, and T. Otsuji, J. Appl. Phys., 101, 083114 (2007).
6. V. Ryzhii, M. Ryzhii, A. Satou, T. Otsuji, A. A. Dubinov, and V. Y. Aleshkin, J. Appl. Phys., 106, 084507 (2009). 7. V. Ryzhii, M. Ryzhii, V. Mitin, and T. Otsuji, J. Appl. Phys., 110, 094503 (2011). 8. V. Ryzhii, I. Semenikhin, M. Ryzhii, D. Svintsov, V. Vyurkov, A. Satou, and T. Otsuji, J. Appl. Phys., 113, 244505 (2013). 9. S. Kumar, IEEE J. Sel. Top. Quantum. Electron, 17, 38 (2011).
10. S. BoubangaTombet, S. Chan, T. Watanabe, A. Satou, V. Ryzhii, and T. Otsuji, Phys. Rev. B, 85, 035443 (2012). 11. T. Li, L. Luo, M. Hupalo, J. Zhang, M. C. Tringides, J. Schmalian, and J. Wang, Phys. Rev. Lett., 108, 167401 (2012).
12. S. Kar, D. R. Mohapatra, E. Freysz, and A. K. Sood, Phys. Rev. B, 90, 165420 (2014).
13. I. Gierz, J. C. Petersen, M. Mitrano, C. Cacho, I. E. Turcu, E. Springate, A. Stohr, A. Kohler, U. Starke, and A. Cavalleri, Nat. Mater., 12, 1119–1124 (2013).
14. T. Winzer, E. Malic, and A. Knorr, Phys. Rev. B, 87, 165413 (2013).
15. T. Watanabe, T. Fukushima, Y. Yabe, S. A. B. Tombet, A. Satou, A. A. Dubinov, V. Y. Aleshkin, V. Mitin, V. Ryzhii, and T. Otsuji, New J. Phys., 15, 075003 (2013).
16. I. Gierz, M. Mitrano, J. C. Petersen, C. Cacho, I. C. E. Turcu, E. Springate, A. Stöhr, A. Köhler, U. Starke, and A. Cavalleri, Population inversion in monolayer and bilayer graphene, eprint arXiv:1409.0211.
439
440
Negative Terahertz Conductivity in Disordered Graphene Bilayers
17. V. Y. Aleshkin, A. A. Dubinov, and V. Ryzhii, JETP Lett., 89, 63 (2009).
18. M. Martl, J. Darmo, C. Deutsch, M. Brandstetter, A. M. Andrews, P. Klang, G. Strasser, and K. Unterrainer, Opt. Express, 19, 733 (2011).
19. A. Satou, V. Ryzhii, Y. Kurita, and T. Otsuji, J. Appl. Phys., 113, 143108 (2013).
20. D. Svintsov, V. Ryzhii, andT. Otsuji, Appl. Phys. Express, 7, 115101 (2014).
21. E. McCann, D. S. Abergel, and V. I. Fal’ko, Eur. Phys. J.: Spec. Top., 148, 91 (2007).
22. E. H. Hwang, S. Adam, and S. D. Sarma, Phys. Rev. Lett., 98, 186806 (2007). 23. Y.W. Tan, Y. Zhang, K. Bolotin, Y. Zhao, S. Adam, E. H. Hwang, S. Das Sarma, H. L. Stormer, and P. Kim, Phys. Rev. Lett., 99, 246803 (2007).
24. K. M. McCreary, K. Pi, A. G. Swartz, W. Han, W. Bao, C. N. Lau, F. Guinea, M. I. Katsnelson, and R. K. Kawakami, Phys. Rev. B, 81, 115453 (2010).
25. N. Sule, S. C. Hagness, and I. Knezevic, Phys. Rev. B, 89, 165402 (2014).
26. L. M. Zhang, Z. Q. Li, D. N. Basov, M. M. Fogler, Z. Hao, and M. C. Martin, Phys. Rev. B, 78, 235408 (2008).
27. J.H. Chen, C. Jang, S. Adam, M. Fuhrer, E. Williams, and M. Ishigami, Nat. Phys., 4, 377 (2008).
28. E. H. Hwang and S. Das Sarma, Phys. Rev. Lett., 101, 156802 (2008).
29. F. T. Vasko and V. Ryzhii, Phys. Rev. B, 76, 233404 (2007).
30. S. Adam, P. W. Brouwer, and S. Das Sarma, Phys. Rev. B, 79, 201404 (2009). 31. C. H. Lewenkopf, E. R. Mucciolo, and A. H. Castro Neto, Phys. Rev. B, 77, 081410 (2008).
32. J. M. B. Lopes dos Santos, N. M. R. Peres, and A. H. Castro Neto, Phys. Rev. Lett., 99, 256802 (2007).
33. J. W. Klos, A. A. Shylau, I. V. Zozoulenko, H. Xu, and T. Heinzel, Phys. Rev. B, 80, 245432 (2009). 34. G. Konstantatos, M. Badioli, L. Gaudreau, J. Osmond, M. Bernechea, F. P. G. de Arquer, F. Gatti, and F. H. L. Koppens, Nat. Nanotechnol., 7, 363 (2012).
35. J. Li, G. Xu, C. Rochford, R. Li, J. Wu, C. M. Edvards, C. L. Berne, Z. Chen, and V. A. Maroni, Appl. Phys. Lett., 99, 023111 (2011).
36. Yu. I. Latyshev, A. P. Orlov, V. A. Volkov, V. V. Enaldiev, I. V. Zagorodnev, O. F. Vyvenko, Yu. V. Petrov, and P. Monceau, Sci. Rep., 4, 7578 (2014).
Chapter 25
Negative Terahertz Conductivity in Remotely Doped Graphene Bilayer Heterostructures*
V. Ryzhii,a,b M. Ryzhii,c V. Mitin,d M. S. Shur,e and T. Otsujia aResearch Institute of Electrical Communication, Tohoku University, Sendai 9808577, Japan bInstitute of Ultra High Frequency Semiconductor Electronics of RAS, and Center for Photonics and Infrared Engineering, Bauman Moscow State Technical University, Moscow 111005, Russia cDepartment of Computer Science and Engineering, University of Aizu, AizuWakamatsu 9658580, Japan dDepartment of Electrical Engineering, University at Buffalo, SUNY, Buffalo, New York 1460–1920, USA eDepartments of Electrical, Electronics, and Systems Engineering and Physics, Applied Physics, and Astronomy, Rensselaer Polytechnic Institute, Troy, New York 12180, USA [email protected]
*Reprinted with permission from V. Ryzhii, M. Ryzhii, V. Mitin, M. S. Shur, and T. Otsuji (2015). Negative terahertz conductivity in remotely doped graphene bilayer heterostructures, J. Appl. Phys., 118, 183105. Copyright © 2015 AIP Publishing LLC. GrapheneBased Terahertz Electronics and Plasmonics: Detector and Emitter Concepts Edited by Vladimir Mitin, Taiichi Otsuji, and Victor Ryzhii
Copyright © 2021 Jenny Stanford Publishing Pte. Ltd.
ISBN 9789814800754 (Hardcover), 9780429328398 (eBook)
www.jennystanford.com
442
Negative Terahertz Conductivity in Remotely Doped Graphene
Injection or optical generation of electrons and holes in graphene bilayers (GBLs) can result in the interband population inversion enabling the terahertz (THz) radiation lasing. The intraband radiative processes compete with the interband transitions. We demonstrate that remote doping enhances the indirect interband generation of photons in the proposed GBL heterostructures. Therefore, such remote doping helps to surpass the intraband (Drude) absorption, and results in large absolute values of the negative dynamic THz conductivity in a wide range of frequencies at elevated (including room) temperatures. The remotely doped GBL heterostructure THz lasers are expected to achieve higher THz gain compared with previously proposed GBLbased THz lasers.
25.1 Introduction
The population inversion created by injection or optical pumping in graphene layers (GLs) and graphene bilayers (GBLs) [1] results in the negative dynamic conductivity in the terahertz (THz) range of frequencies [2, 3] and enables the graphenebased THz lasers [2–5]. Different research groups have demonstrated the THz gain in the pumped GLs [6–17] (see also Ref. [16]). GLs and GBLs can serve as the active regions of the THz lasers with the FabryPerot resonators, dielectric waveguides, and slotlines including the plasmonic lasers [8, 18–23]. The GL and GBL heterostructure lasers can operate in a wide frequency range, including the 6–10 THz range, where using materials like A3B5 is hindered by the optical phonon effects [24– 26]. The THz lasing in the GL and GBL structures is possible if the contribution of the interband radiative transitions to the real part of the dynamic conductivity Re s in a certain range of frequencies surpasses the contribution of the intraband radiative processes associated with the Drude losses. The interband transitions include the direct (with the conservation of the electron momenta) and the indirect transitions (accompanied with the variation of the electron momentum due to scattering). The limitations imposed by the momentum and energy conservation laws allow only for the indirect intraband radiative transitions. In the GLs and GBLs with sufficiently long carrier momentum relaxation time t, the direct interband radiative transitions dominate over the indirect intraband
Introduction
transitions and Re s < 0. Recently [27, 28], we demonstrated that in GLs and GBLs with primarily longrange disorder scattering, the indirect interband transitions can prevail over the indirect intraband transitions, leading to fairly large absolute values of the negative conductivity Res. These values could exceed the fundamental limits for the direct transitions, which are sQ = e2/4ℏ for GLs and 2sQ for GBLs [1] (here e is the electron charge and ℏ is the Planck constant). As a result, in the GL and GBL structures with a longrange disorder, one can expect that the condition Re s < 0 could be fulfilled in a wider range of the THz frequencies, including the low boundary of the THz range. When the momentum relaxation is associated with longrange scattering mechanism, moderate values of t might be sufficient for achieving Re s < 0, especially in GBLs where the density of states (DoS) r(e) as a function of energy e near the band edges (r(e) ≃ const) in the latter is considerably larger than in GLs (where r(e) µ e). This chapter deals with the GBL heterostructures with a remote impurity layer (RIL) located at some distance from the GBL plane, and incorporating donors and acceptors or donor and acceptor clusters. We consider the GBLRIL heterostructure as an active region of an injection THz laser. We show that the electron and hole injection from the side n and pcontact regions into the GBLRIL heterostructures leads to the population inversion enabling the enhanced negative dynamic conductivity, which, in turn, can result in lasing in the THz range. Figure 25.1 shows the schematic view of an injection laser based on the GBLRIL heterostructure at the reverse bias voltage V. The remote (selective) doping can markedly affect the scattering of electrons and holes (see, for example, Refs. [29, 30]), hence the indirect radiative transitions. The GL and GBL heterostructures using remote doping were already fabricated and used for device applications [31, 32]. The GBLRIL heterostructures demonstrate the following distinct features. First, the net electron and hole densities determined by both the pumping and RIL and the electron and hole quasiFermi energies, eF,e and eF,h, are generally not equal. Second, relatively large scale donor and acceptor density fluctuations result in smooth (longrange) spatial variations of the potential in the GBL created by the RIL, separated by a distance d from the GBL. This could result in the electron and hole scattering with a relatively small momentum change, and consequently,
443
444
Negative Terahertz Conductivity in Remotely Doped Graphene
increase in the contribution of the indirect interband transitions in comparison with the intraband transitions. Thus, the main role of the RIL is not to induce extra carrier in the GBL (as in highelectron mobility transistors) but to provide the specific mechanism of the electron and hole scattering reinforcing the indirect interband radiative transitions. The intraband radiative transitions (leading to the Drude radiation absorption) are accompanied by a change in the electron or hole momentum. However, such transitions in the GBLs require larger variation of the momentum than the interband radiative transitions. As a result, an increase in the longrange scattering contributions results in an increase in the relative role of the indirect interband transitions and even, as shown in the following, their dominance. One needs to stress that all this takes place under the conditions of the interband population inversion and in the gapless materials. In the standard semiconductors with sufficiently wide energy gap and the lasers on the base of such semiconductors, the interband transitions (both direct and indirect) usually correspond to relatively large photon energies, at which the Drude absorption is much less important. In this regard, the situation under consideration (population inversion in gapless semiconductors) is, in some sense, unique. Although the domination of the longrange scattering and, therefore, a substantial increase in the relative contribution of the indirect interband transitions can occur in the GBL heterostructures with the clusterized charged impurities immediately in the GBL [28] (that is difficult to realize in a systematic engineering manner), the implementation of the RIL can intentionally provide a similar or stronger effect using the standard doping techniques.
Figure 25.1 Schematic view of an injection laser based on the GBLRIL heterostructure with the GBL doped with acceptors and the RIL doped with both donors and acceptors and with the chemically doped n and pinjectors.
Device Model
We calculate the spectral characteristics of the real part of the dynamic conductivity Re s in the pumped GBLRIL heterostructures as a function of the doping level and the spacer thickness d and compare the obtained characteristics with those of the undoped heterostructures. This analysis reveals the conditions for the selective doping enabling the negative dynamic conductivity in a wide frequency range, including the frequencies of a few THz. This might open new prospects of the GBL heterostructures for the efficient THz lasers.
25.2 Device Model
We study the GBLRIL heterostructures pumped via the injection from the side p and ncontacts as shown in Fig. 25.1. In the very clean pumped GBLs (or GLs) with a fairly high carrier mobility, the intraband (Drude absorption) at the radiation frequencies above 1 THz should not play a dominant role. Hence, adding the selective doping might not be needed. However, in the GBLs with a relatively low carrier mobility, caused by unavoidable (residual) charge impurities and imperfections, the RIL induced scattering could result in a substantial compensation of the Drude absorption, and therefore, enhancement of the negative dynamic conductivity. In the following, for definiteness, we consider the GBLRIL heterostructures with the GBL doped with acceptors (with the density SA) and the RIL formed by partially compensated donors (with the density SD,R) and acceptors (with the density SA,R). Hence, SD,R – SA,R ≃ SA. We further assume that in these heterostructures, the RIL might comprise the clusterized acceptors and donors (with the correlated charge defects forming the charged clusters with the charge Zce > e and the characteristic size lc, where e is the electron charge). In the latter case, we assume that the cluster density is equal to (SA,R + SD,R)/Zc. Such GBLRIL heterostructures are quasineutral even in the absence of the pumping. Pumping results in the formation of the twodimensional (2D) electron and hole gases in the GBL with the equal densities Se = Sh = S and the quasiFermi energies eF,e = eF,h = eF. Figure 25.2 shows the GBL band diagram under pumping. In Fig. 25.2, the arrows indicate different radiative transitions: vertical interband transitions, indirect intraband transitions accompanied by the electron scattering on the impurities, phonons and holes
445
446
Negative Terahertz Conductivity in Remotely Doped Graphene
(leading to the Drude absorption of radiation), and the interband indirect transitions. The transverse electric field arising in the spacer due to the features of the doping can lead to the local opening of the energy gap [1, 33]. However, as shown below, for the doping levels under consideration, the energy gap is expected to be small, and the band opening and the energy spectrum nonparabolicity will be disregarded [33–35]. The energy spectrum is assumed to be ep = 2 /g 1 = ±p2/2m [1], where g1 ≃ 0.35–0.43 eV is the intere p = ±p2uW GL overlap integral in the GBLs, uW ≃ 108 cm/s is the characteristic 2 velocity, and m = g 1 /2uW is the effective mass of electrons and holes.
Figure 25.2 Energy band diagram of a pumped GBL (left panel) and energy dependency of its DoS (right panel). Arrows correspond to the direct and indirect interband transitions with the photon emission (wavy arrow “1” and wavy + smooth arrows “2”) as well as to indirect intraband transitions with the photon absorption in the conduction and valence bands (wavy + smooth arrows “3” and “3*,” respectively).
25.3 Main Equations The real part of the net dynamic (THz) conductivity in the inplane direction, Re s, of GLs and GBLs, comprises the contributions from inter the direct (vertical), Re sd, and two types of the indirect, Res ind intra and Res ind , transitions, respectively,
(
)
inter intra Res = Re s d + s ind + s ind .
(25.1)
Main Equations
The first term in Eq. (25.1) corresponds to the transitions of type “1” in Fig. 25.2, the second term corresponds to type “2,” and the third term corresponds to types “3” and “3*” transitions, respectively. The last term in the righthand side of Eq. (25.1) corresponds to the processes responsible for the Drude absorption. Due to the high frequencies of the intercarrier scattering under sufficiently strong pumping, the energy distributions of the pumped carriers are characterized by the Fermi distribution functions fu(ep) and fc(ep), where ep is the dispersion relationship for the 2D carriers in GBLs, with the quasiFermi energy, eF ≃ pℏ2S/2m and the effective temperature T. The calculations of the GBL dynamic conductivity in the inplain direction associated with the direct interband transitions accounting for the GBL energy spectra, following the approach developed in Refs. [36, 37] (see also Ref. [5]), yield Re
s d ( �w + 2g 1 ) Ê �w  2e F ˆ = tanh Á Ë 4T ¯˜ s Q ( �w + g 1 ) Ê �w  2e F ˆ . � 2tanh Á Ë 4T ˜¯
(25.2)
Applying the Fermi golden rule for the indirect intra and interband electron radiative transitions and using the standard procedure [38], we obtain the following formulas for the respective components of the dynamic conductivity real parts (proportional to the absorption coefficients): Re
intra
s ind 4p g ll =  V (p  p¢)2 upp¢ ( v p¢  v p )2 d ( w + e p  e p¢ ) sQ w 3 p ,p¢
Â
ÏÔ ¸Ô 1 1 ¥Ì ˝, ÓÔ 1 + exp[(e p  e F )/ T ] 1 + exp[(e p¢  e F )] ˛Ô
Re
(25.3)
inter
s ind 2p g cv  V (p  p¢ )2 upp¢ (v p¢ + v p )2 d (w  e p  e p¢ ) = sQ w 3 p , p ¢
Â
ÏÔ ¸Ô 1 1 ¥Ì ˝ . (25.4) ÓÔ 1 + exp[(e p  e F )/ T ] 1 + exp[(e p¢ + e F ) / T ] ˛Ô
447
448
Negative Terahertz Conductivity in Remotely Doped Graphene
2 Here, g = 4 is the spinvalley degeneracy factor, ep, vp = 2p uW /g 1 = p/m is the velocity of electrons and holes with the momentum p in GBLs, V(q) is the qthe Fourier component of the scattering potential,
ll upp¢ = (1 + ll¢ cos 2qpp¢)/2 is the overlap between the envelope wave functions in the GBLs, and l = ±1 is the index indicating the conduction and valence bands. The extra factor of 2 in Eq. (25.3) accounts for the intraband electron and hole contributions. Equation (25.3) yields the wellknown result for the dynamic Drude conductivity in the highfrequency limit G = ℏ/t < ℏw < eF, where G is the broadening of the carrier spectra.
25.4 Scattering Mechanisms
For the GBLRIL heterostructures under consideration, we have the following formulas: 2
È 2pe2 ˘  V ( q) = Í (25.5) ˙ [S A + S RCL exp(2qd)], ÍÎk (q + qTF ) ˙˚ for the discrete acceptors in the GBL and the discrete acceptors and donors in the RIL (see, for example, Ref. [30]) and 2
2
È 2pe2 ˘ 2 2  V ( q) = Í ˙ [S A + Z c S RCL exp( 2qd q l /2)], ÍÎk(q + qTF ) ˙˚ 2
(25.6)
for the point charged defects (acceptors) in the GBL and the correlated clusterized acceptors and donors in the RIL, respectively. Here, q = p – p¢, SRCL = SA,R + SD,R is the net density of the charge impurities of both types located in the RIL (therefore, the cluster density in the “clusterized” RIL is equal to SRCL/Zc with SRCL > SA), k is the effective dielectric constant (which is the halfsum of the dielectric constants of the materials surrounding the GBL, i.e., of the spacer and the substrate), qTF = (4e2m/ℏ2k) is the ThomasFermi screening wavenumber [37, 39, 40], which is independent of the carrier density. Deriving Eq. (25.6), we have taken into account that the density of the charged clusters in the clusterized RCL is Zc times smaller than the donor and acceptor densities, but the crosssection of the carrier scattering on the clusters is proportional to Z c2e 4 . The factor exp(–2qd) in Eqs. (25.5) and (25.6) is associated with the remote position of a portion of the charged scatterers (see,
Net THz Conductivity
for example, Ref. [30]). Equation (25.6) corresponds to the Gaussian spatial distributions of the clusters that leads to the appearance of the factor exp (q2lc2/ 2) (compare with Refs. [28, 41–43]). One can see that the scattering matrix element explicitly depends on the background dielectric constant k and via the dependence of qTF on k.
25.5 Net THz Conductivity
In the following, we consider the most practical case of the temperature, frequency range, and pumping in which ℏ/t < ℏw, T < eF. For T = 300 K, the frequency range w/2p = 1–10 THz and eF ≳ 50 meV, these inequalities are satisfied when t ≳ 0.05–0.5 ps. For GBL structures without the RIL (SRIL = 0) and the totally intra intra inter screened charges in the GBL, in which Res ind = s ind and Res ind inter = s ind , invoking Eqs. (25.3)–(25.6), one obtains 2
intra Res ind 2
e2 S 1 Êw ˆ = 2s Q Á D ˜ , 2 Ë w ¯ mt w
(25.7)
where w D = 4S/mt = 8e F / p t is the Drude frequency. This quantity characterizes the relative strength of the Drude processes (absorption). As the above takes place, Eqs. (25.3) and (25.4) lead to inter Res ind
intra Res in d
�w �  4e F
(25.8)
To avoid cumbersome calculations and obtain transparent formulas suitable for a qualitative analysis, we use the mean value theorem for the integrals over dq. As a result, we arrive at the intra inter following simplified formulas for Res ind + Res in d :
(
intra inter Re s ind + s ind
)
Ï Q [1 + Dexp( 2qd  q2l 2/2)] intra Ô �max � Res ind dqq 2 Ì 2 (Qmax  Qmin )(q / qTF + 1)2 ÓÔ Qmin
Ú

�w 4e F
Ú
qma x
qmin
[1 + Dexp(2qd  q2l 2/2)] ¸Ô dqq 2 ˝. 2 (qmax  qm ) q / qTF + 1)2 ˛Ô in )(
(25.9)
449
450
Negative Terahertz Conductivity in Remotely Doped Graphene
Here, D = Zc(SRCL/SA) = Zc(SD,R + SA,R)/(SD,R – SA,R) ≃ Zc(SD,R + SA,R)/SA ≥ Zc ≥ 1 is the doping parameter (Zc = 1 and l = 0 for the RGL with the point charges (acceptors and donors) and Zc > 1 and l = lc in the case of RIL with the clusterized acceptors and donors), ℏQmax � 2 2me F (1  �w / 4e F ), �Qmin � 2 2me F ( �w/4e F ),
�qmax � 2 m�w , qmin � 0. The latter quantities follow from the conservation laws for the indirect intraband and interband radiative transitions. In particular, Eq. (25.9) gives rise to
(
intra inter Re s ind + s ind
)
intra Res ind
1
1 2
Ú
qmax
Ú
Qmax
qmin
Qmin
dqq
[1 + Dexp( 2qd  q2l 2/2)] (q/qTF + 1)2
dqq
[1 + Dexp( 2qd  q2l 2/2)] (q/qTF + 1)2
.
(25.10)
For sufficiently pure GBLs and relatively strong RIL doping (with nearly complete compensation of the donor and acceptors), the doping parameter D can be fairly large. In this case, the contribution of the carrier scattering on the remote impurities to the net scattering rate can be dominant. In such a case, the absolute value of the net THz conductivity Res can markedly exceed the contribution solely from the direct interband transitions, i.e., Res > 2sQ. Considering Eqs. (25.1), (25.2), and (25.9), we arrive at the following formula for the net THz conductivity: Res Ê �w  2e F ˆ � tanh Á Ë 4T ˜¯ 2s Q Êw ˆ +Á D ˜ Ë w ¯ 
w 4e F
Ú
2
ÏÔ Ì ÔÓ
Ú
qmax
qmin
Qmax
Qmin
dqq
dqq
[1 + Dexp(2qd  q2l 2/2)] 2 2 2 (Qmax  Qm in )(q/qTF + 1)
[1 + Dexp(2qd  q2l 2/2)] ¸Ô ˝. 2 2 (qmax  qmin )((q/qTF + 1)2 ˛Ô
(25.11)
25.6 Results and Analysis Using Eqs. (25.9) and (25.10), one can analyze the conditions when the interband radiative processes surpass the intraband ones, i.e.,
Results and Analysis
(
)
intra inter when Re s ind + s ind < 0.
For the practical GBLRIL heterostructures with the HfO2 spacer and the substrate material like Si and SiC, the effective dielectric constant (which is the halfsum of the dielectric constants of the spacer and the substrate) is in the range k = 10–20. In the calculations, we assume set m = 4 ¥ 10–29 g and eF = 60 meV (S ~ 2.5 ¥ 1012 cm–2). Equations (25.9)–(25.11) for d = 0 (no spacer) lead to approximately the same results as in Ref. [28] in both the cases l = 0 and l π 0 (clusterized charge impurities in the GBL). In particular, at d = 0 and l = 0, the indirect intraband radiative transitions can partially compensate the Drude absorption but not prevail over the latter. Because of this, we focus on the GBLRIL heterostructures (i.e., the heterostructures with d π 0 and D π 0).
(
)
intra inter Figure 25.3 Frequency dependences of Re s ind + s ind calculated for the GBLRIL heterostructures with spacer thickness d = 15 nm, different dielectric constants (k = 10, 15, and 20), and different doping parameters D: (a) D = 0, (b) D = 10, and (c) D = 20.
451
452
Negative Terahertz Conductivity in Remotely Doped Graphene
Figure 25.4 The same as in Fig. 25.3 but for doping parameter D = 20, different spacer thicknesses (d = 10, 15, and 25 nm), and different dielectric constants: (a) k = 10, (b) k = 15, and (c) k = 20.
(
)
(
)
intra inter Figures 25.3 and 25.4 show the dependences of Re s ind + s ind on the frequency f = w/2p calculated using Eq. (25.9) with l = 0 (uncorrelated impurities in the RIL) for different values of the doping parameter D, the spacer thickness d, and effective dielectric constant k. As seen from Fig. 25.3a, in the absence of the RCL (D = 0), the indirect intraband transitions prevail over the indirect interband transitions. In such a case, the indirect transitions lead to the photon absorption in the entire frequency range, although the photon emission due to the interband transitions partially compensates the Drude absorption. This compensation is enhanced in the heterostructures with the doped RIL, i.e., for D > 0 (see Figs. 25.3b and c): an increase in the doping parameter D leads to the appearance of the frequency intra inter range where Re s ind + s ind < 0 . The latter range becomes wider (it starts from lower frequency) with increasing dielectric constant intra inter k. These features of the transformation of the Re s ind + s ind
(
)
Results and Analysis
frequency dependence are attributed to reinforcing of the longrange carrier scattering (with increasing D) and smoothing of the scattering potential (due to a stronger screening at higher k). Both these effects result in an increase in the relative role of the indirect interband transitions. The scattering potential smoothing associated with an increase in the spacer thickness d also beneficial for the indirect interband transitions is seen in Fig. 25.4 as well.
( ) ) < 0 (above these
intra inter Figure 25.5 shows the Dd plane where Re s ind + s ind >0
(below the D versus d lines) and Re
(
intra s ind
inter + s ind
lines) are calculated considering Eq. (25.10) at different values of k and frequency f = w/2p. As seen, the ranges of parameters D and
(
intra inter d where the quantity Re s ind + s ind
) is negative are markedly
wider in the case of a relatively large dielectric constant k and the frequency f.
(
)
intra inter Figure 25.5 Areas in the D–d plane where Re s ind + s ind > 0 (areas below
lines corresponding to given frequencies) and Re
(
intra inter s ind + s ind
) < 0 (above
these lines) at different values of dielectric constant k: (a) k = 15 and (b) k = 20.
Figure 25.6 shows the threshold frequency w0/2p corresponding intra inter to Re s ind + s ind = 0 as a function of the spacer thickness d calculated for D = 20 and different values of k.
(
)
453
454
Negative Terahertz Conductivity in Remotely Doped Graphene
(
)
intra inter Figure 25.6 Threshold frequency w0/2p corresponding to Re s ind + s ind =0 as a function of the spacer thickness d calculated for D = 20 and different values of dielectric constant k. As in Fig. 25.5, areas above the pertinent line are intra inter related to Re s ind + s ind DS = SA + SA,R – SD,R, Eqs. (25.2), (25.9), and (25.10) are still approximately valid until ℏw/2 < min{eF,e, eF,h}. The above model disregarded the opening of the band gap in the GBL under the transverse electric field arising due to the impurity charges in the RIL and GBL. Despite a fairly complex pattern of the opening gap in the GBLs by the electric field and doping [44, 45], the pertinent energy gap Dg can roughly be estimated in the manner as it was done in Ref. [34]. In the absence of the electron and hole injection from the side contacts, the carrier density in the GBL is rather small due to the compensation of the acceptor charges in the GBL and the donor and acceptor charges in the RIL (see Section 25.2). In this case, Dg ~ eE^dGBL, where E^ = 4peSA/k is the transversal electric field created by the charged impurities and dGBL ≃ 0.36 nm is the spacing between GLs in the GBL, so that Dg ~ 4p e2SAdGBL/k. Under the pumping conditions, the 2D electron and hole gases partially screen the electric field in the GBL structure. eff eff As a result, one obtains Dg ~ eE^ dGBL with dGBL < dGBL [34]. Taking into account the screening of the transversal electric field E^ by both electron and hole components, we obtain the following estimate: Dg ~ 4p e2SAdGBL/k[1 + (8dGBL/aB)], where aB = kℏ2/me2 is the Bohr radius. Assuming ab = 10–20 nm and SA = (5–10) ¥ 1011 cm–2, we obtain Dg ~ 1.5–5 meV. These values are in line with those estimated in Ref. [34] and extracted from the experimental data [44, 45]. This estimate validates our model.
457
458
Negative Terahertz Conductivity in Remotely Doped Graphene
In the case of the clusterized charged impurities, the long range variations of the potential associated with the clusters lead to the variation of the band gap. The latter variations reinforce the electron and hole scattering on the clusters, but this effect is not really essential. In Eqs. (25.3) and (25.4), we have disregarded the indirect radiative processes associated with the electronhole scattering in the GBL. The point is that the probability of such processes is proportional to [2p e2/k(q + qTF)]2Sh, where (in the degenerated twodimensional electron and hole gases) the factors h < 1 is the fraction of electrons and holes effectively participated in the scattering processes h = T/eF at ℏw < T, so that Sh ≃ ST = 2mT/ pℏ2. The values of qTF and Sh are independent of the electron and hole densities and, hence, of the pumping conditions. This is because of the virtually constant density of state. At room temperatures, the value of ST can be of the order of or less than SA and much smaller than SRIL. In the former case, one needs to replace the quantity D in Eqs. (25.9) and (25.10) by D* = D/(1 + 2St/Sa).
25.8 Conclusions
We proposed to use the GBLRIL heterostructure with the population inversion due to the electron and hole injection as the active region of the interband THz lasers, and demonstrated that the incorporation of the RIL enables a substantial reinforcement of the effect of negative THz conductivity and the laser THz gain. This is associated with the domination of the indirect interband transitions in the GBL over the indirect intraband transitions (resulting in the Drude absorption) when the carrier scattering on a longrange potential prevails. As shown, the latter can be realized due to the remote doping and enhanced by the clusterization of impurities. Using a simplified device model, we calculated the THz conductivity of the GBLRIL heterostructures as a function of the frequency for different structural parameters (dopant densities, spacer thickness, impurity cluster size, and the injected carrier momentum relaxation time). We found that the absolute value of the THz conductivity in the GBLRIL heterostructures, with a sufficiently highly doped RIL separated from the GBL by a spacer layer of
References
properly chosen thickness, can markedly exceed the pertinent value in the GBLheterostructures without the RIL. Thus, the remotely doped GBL heterostructures can be of interest for applications as the active media in the THz lasers.
Acknowledgments
The authors are grateful to D. Svintsov and V. Vyurkov for useful discussions and information. The work was supported by the Japan Society for Promotion of Science (GrantinAid for Specially Promoted Research No. 23000008) and by the Russian Scientific Foundation (Project No. 142900277). The works at UB and RPI were supported by the U.S. Air Force Award No. FA9550101391 and by the U.S. Army Research Laboratory Cooperative Research Agreement, respectively.
References
1. A. H. Castro Neto, F. Guinea, N. M. R. Peres, K. S. Novoselov, and A. K. Geim, Rev. Mod. Phys., 81, 109 (2009).
2. V. Ryzhii, M. Ryzhii, and T. Otsuji, J. Appl. Phys., 101, 083114 (2007). 3. M. Ryzhii and V. Ryzhii, Jpn. J. Appl. Phys., Part 2, 46, L151 (2007).
4. V. Ryzhii, M. Ryzhii, V. Mitin, and T. Otsuji, J. Appl. Phys., 110, 094503 (2011).
5. V. Ya. Aleshkin, A. A. Dubinov, and V. Ryzhii, JETP Lett., 89, 63 (2009).
6. S. BoubangaTombet, S. Chan, A. Satou, T. Otsuji, and V. Ryzhii, Phys. Rev. B, 85, 035443 (2012).
7. T. Otsuji, S. BoubangaTombet, A. Satou, H. Fukidome, M. Suemitsu, E. Sano, V. Popov, M. Ryzhii, and V. Ryzhii, J. Phys. D, 45, 303001 (2012).
8. T. Li, L. Luo, M. Hupalo, J. Zhang, M. C. Tringides, J. Schmalian, and J. Wang, Phys. Rev. Lett., 108, 167401 (2012).
9. Y. Takatsuka, K. Takahagi, E. Sano, V. Ryzhii, and T. Otsuji, J. Appl. Phys., 112, 033103 (2012).
10. T. Watanabe, T. Fukushima, Y. Yabe, S. A. Boubanga Tombet, A. Satou, A. A. Dubinov, V. Ya. Aleshkin, V. Mitin, V. Ryzhii, and T. Otsuji, New J. Phys., 15, 075003 (2013). 11. T. Winzer, E. Maric, and A. Knorr, Phys. Rev. B, 87,165413 (2013).
459
460
Negative Terahertz Conductivity in Remotely Doped Graphene
12. I. Gierz, J. C. Petersen, M. Mitrano, C. Cacho, I. C. Edmond Turcu, E. Springate, A. Stohr, A. Kohler, U. Starke, and A. Cavalleri, Nat. Mater., 12, 1119 (2013).
13. S. Kar, D. R. Mohapatra, E. Freysz, and A. K. Sood, Phys. Rev. B, 90, 165420 (2014).
14. R. R. Hartmann, J. Kono, and M. E. Portnoi, Nanotechnology, 25, 322001 (2014). 15. T. Otsuji, S. BoubangaTombet, A. Satou, M. Suemitsu, V. Ryzhii, and J. Infrared, Millimeter, Terahertz Waves, 33, 825 (2012).
16. I. Gierz, M. Mitrano, J. C. Petersen, C. Cacho, I. C. E. Turcu, E. Springate, A. St0hr, A. K0hler, U. Starke, and A. Cavalleri, J. Phys.: Condens. Matter, 27, 164204 (2015). 17. A. A. Dubinov, V. Ya. Aleshkin, M. Ryzhii, T. Otsuji, and V. Ryzhii, Appl. Phys. Express, 2, 092301 (2009).
18. V. Ryzhii, M. Ryzhii, A. Satou, T. Otsuji, A. A. Dubinov, and V. Ya. Aleshkin, J. Appl. Phys., 106, 084507 (2009).
19. V. Ryzhii, A. A. Dubinov, T. Otsuji, V. Mitin, and M. S. Shur, J. Appl. Phys., 107, 054505 (2010). 20. F. Rana, IEEE Trans. Nanotechnol., 7, 91 (2008).
21. A. A. Dubinov, V. Ya. Aleshkin, V. Mitin, T. Otsuji, and V. Ryzhii, J. Phys.: Condens. Matter, 23,145302 (2011).
22. V. V. Popov, O. V. Polischuk, A. R. Davoyan, V. Ryzhii, T. Otsuji, and M. S. Shur, Phys. Rev. B, 86,195437 (2012).
23. A. Tredicucci and M. S. Vitiello, IEEE J. Sel. Top. Quantum Electron., 20, 8500109 (2014).
24. H. C. Liu, C. Y. Song, A. J. SpringThorpe, and J. C. Cao, Appl. Phys. Lett., 84, 4068 (2004). 25. B. S. Williams, Nat. Photonics, 1, 517 (2007).
26. S. Kumar, IEEE J. Sel. Top. Quantum Electron., 17, 38 (2011).
27. D. Svintsov, V. Ryzhii, and T. Otsuji, Appl. Phys. Express, 7, 115101 (2014). 28. D. Svintsov, T. Otsuji, V. Mitin, M. S. Shur, and V. Ryzhii, Appl. Phys. Lett., 106, 113501 (2015).
29. M. Shur, Physics of Semiconductor Devices (PrenticeHall, New Jersey, 1990), ISBN: 0136664962. 30. A. Shik, Quantum Wells: Physics and Electronics of TwoDimensional Systems (World Scientific, Singapore, 1997), ISBN: 9810232799.
References
31. T. Stauber, G. GomezSantos, and F. Javier Garcia de Abajo, Phys. Rev. Lett., 112, 077401 (2014).
32. G. Konstantatos, M. Badioli, L. Gaudreau, J. Osmond, M. Bernechea, F. P. Garcia de Arquer, F. Gatti, and F. H. L. Koppens, Nat. Nanotechnol., 7, 363–368 (2012). 33. E. McCann and V. Fal’ko, Phys. Rev. Lett., 96, 086805 (2006).
34. E. McCann, D. S. L. Abergel, and V. I. Fal’ko, Eur. Phys. J.: Spec. Top., 148, 91–103 (2007). 35. L. M. Zhang, Z. Q. Li, D. N. Basov, M. M. Fogler, Z. Hao, and M. C. Martin, Phys. Rev. B, 78, 235408 (2008).
36. L. A. Falkovsky and S. S. Pershoguba, Phys. Rev. B, 76, 153410 (2007).
37. S. Das Sarma, E. H. Hwang, and E. Rossi, Phys. Rev. B, 81, 161407(R) (2010).
38. F. T. Vasko and A. V. Kuznetsov, Electronic States and Optical Transitions in Semiconductor Heterostructures (Springer, New York, 1998). 39. E. McCann and M. Koshino, Rep. Prog. Phys., 76, 056503 (2013).
40. H. Min, D. S. L. Abergel, E. H. Hwang, and S. Das Sarma, Phys. Rev. B, 84, 041406(R) (2011). 41. F. T. Vasko and V. Ryzhii, Phys. Rev. B, 76, 233404 (2007).
42. C. H. Lewenkopf, E. R. Mucciolo, and A. H. Castro Neto, Phys. Rev. B, 77, 081410(R) (2008).
43. S. Adams, P. W. Brouwer, and S. Das Sarma, Phys. Rev. B, 79, 201404 (2009).
44. A. J. Samuels and J. D. Carey, ACS Nano, 7(3), 2790 (2013).
45. W. Zhang, Ch.T. Lin, K.K. Liu, T. Tite, Ch.Y. Su, Ch.H. Chang, Y.H. Lee, Ch.W. Chu, K.H. Wei, J.L. Kuo, and L.J. Li, ACS Nano, 5(9), 7517 (2011).
461
Part 4
Stimulated Emission and Lasing in
Graphene and Graphene Structures
Chapter 26
Feasibility of Terahertz Lasing in Optically Pumped Epitaxial Multiple Graphene Layer Structures*
V. Ryzhii,a,b M. Ryzhii,a,b A. Satou,a,b T. Otsuji,b,c A. A. Dubinov,d and V. Ya. Aleshkind aComputational
Nanoelectronics Laboratory, University of Aizu, AizuWakamatsu 9658580, Japan bJapan Science and Technology Agency, CREST, Tokyo 1070075, Japan cResearch Institute of Electrical Communication, Tohoku University, Sendai 9808577, Japan dInstitute for Physics of Microstructures, Russian Academy of Sciences, Nizhny Novgorod 603950, Russia [email protected], [email protected]
A multiple graphene layer (MGL) structure with a stack of GLs and a highly conducting bottom GL on SiC substrate pumped by optical radiation is considered as an active region of terahertz and far infrared
*Reprinted with permission from V. Ryzhii, M. Ryzhii, A. Satou, T. Otsuji, A. A. Dubinov, and V. Ya. Aleshkin (2009). Feasibility of terahertz lasing in optically pumped epitaxial multiple graphene layer structures, J. Appl. Phys., 106, 084507. Copyright © 2009 American Institute of Physics. GrapheneBased Terahertz Electronics and Plasmonics: Detector and Emitter Concepts Edited by Vladimir Mitin, Taiichi Otsuji, and Victor Ryzhii
Copyright © 2021 Jenny Stanford Publishing Pte. Ltd.
ISBN 9789814800754 (Hardcover), 9780429328398 (eBook)
www.jennystanford.com
466
Feasibility of Terahertz Lasing in Optically Pumped Epitaxial MGL Structures
lasers with external metal mirrors. The dynamic conductivity of the MGL structure is calculated as a function of the signal frequency, the number of GLs, and the optical pumping intensity. The utilization of optically pumped MGL structures might provide the achievement of lasing with the frequencies of about 1 THz at room temperature due to a high efficiency of pumping.
26.1 Introduction
Since the first experimental demonstrations of the nontrivial properties of graphene (see, for instance, Refs. [1, 2] and numerous subsequent publications), due to the gapless energy spectrum of graphene, the latter can be used as an active region in the terahertz and far infrared (FIR) lasers with optical or injection pumping [3, 4]. The optical pumping with the photon energy ℏW leads to the generation of electrons and holes with the energy e0 = ℏW/2. Since the interaction of electrons and holes with optical phonons is characterized by the fairly short time t0, the photogenerated electrons and holes quickly emit cascades of N optical phonons, where N = [ε0/ℏw0] and [X] means the integer part of X. Due to relatively high energy of optical phonons in graphene (ℏw0 ≃ 200 meV), the number N can vary from zero (pumping by CO2 lasers) to a few units (pumping by quantum cascade lasers or semiconductor injection diode lasers). Thus, the photogenerated electrons and holes populate the low energy regions of the conduction and valence bands of graphene (see also Refs. [5, 6]). As a result, the Fermi levels of electrons and holes are separated and shifted from the Dirac point to the conduction and valence bands, respectively. This corresponds to the population inversion for the interband transitions with absorption or emission of photons with relatively low energies ℏw < 2eF, where eF is the quasiFermi energy of the electron and hole distributions, and leads to the negative contribution of the interband transitions to the real part of the dynamic conductivity Re sw (which includes the contributions of both interband and intraband transitions). If Re sw < 0, the stimulated emission of photons with the relatively low energy ℏw (in the terahertz or FIR range) is possible. The intraband contribution is primarily associated with the Drude mechanism of the photon absorption. As shown previously, the realization of the condition of lasing is feasible [3, 6]. Some possible
Model
schemes of the graphene lasers (with metal waveguide structure or external metal mirrors) utilizing the above mechanism of optical pumping were considered recently (see, for instance, Ref. [7]). In particular, the laser structure evaluated in Ref. [7] includes two graphene layers. Relatively weak absorption of optical radiation with the efficiency per each layer b = pe2/ ℏc ≃ 0.023, where e is the electron charge, ℏ is the reduced Planck constant, and c is the speed of light, necessitates the use of rather strong optical pumping. This drawback can be eliminated in the structures with multiple graphene layers (MGLs). Such epitaxial MGL structures including up to 100 very perfect graphene layers with a high electron mobility (m ≃ 250 000 cm2/s V) preserving up to the room temperatures and, hence, with a long momentum relaxation time were recently fabricated using the thermal decomposition from a 4HSiC substrate [8, 9]. The incident optical radiation can be almost totally absorbed in these MGL structures providing enhanced pumping efficiency. A long momentum relaxation time (up to 20 ps) [10] implies that the intraband (Drude) absorption in the terahertz and FIR ranges can be weak. The optically pumped MGL structures in question with the momentum relaxation time about several picoseconds at room temperature might be ideal active media for interband terahertz lasers. The situation however is complicated by the presence of highly conducting bottom GL (and hence absorbing terahertz and FIR radiation due to the intraband processes) near the interface with SiC as a result of charge transfer from SiC. In this chapter we analyze the operation of terahertz lasers utilizing optically pumped MGL structures by calculating their characteristics as function of the number of graphene layers K and optical pumping intensity IW and demonstrate the feasibility of realization of such lasers operating at the frequencies from about 1 THz to several terahertz at room temperatures.
26.2 Model
We consider a laser structure with an MGL structure on a SiC substrate serving as its active region. Although the active media under consideration can be supplemented by different resonant cavities, for definiteness we address the MGL structure placed between the highly reflecting metal mirrors (made of Al, Au, or Ag)
467
468
Feasibility of Terahertz Lasing in Optically Pumped Epitaxial MGL Structures
as shown in Fig. 26.1a. It is assumed that the MGL structure under consideration comprises K upper GLs (to which we refer to just as GLs) and a highly conducting bottom layer with a Fermi energy of electrons e FB , which is rather large: e FB 400 meV [8]. Apart from this, we briefly compare the MGL structure in question with that in which the bottom GL is absent. The latter structure can be fabricated by an additional peeling of upper GLs and depositing them on a Si substrate. Due to the photogeneration of electrons and holes with the energy e0 = ℏW/2, followed by their cooling associated with the cascade emission of optical phonons, low energy states near the bottom of the conduction band and the top of the valence band can be essentially occupied. Taking into account that elevated electron and hole densities (at elevated temperatures and sufficiently strong optical pumping considered in the following), the electron and hole distributions in the range of energies e ℏw0 in the kth graphene layer (1 £ k £ K) can be described by the Fermi functions with the quasiFermi energies e F(k) (see Fig. 26.1b). The case of relatively weak pair collisions of the photogenerated electrons and holes (due to their low densities) in which the energy distributions deviate from the Fermi distributions was studied in Ref. [6]. Using the Falkovsky– Varlamov formula [11] for the dynamic conductivity of a MGL structure generalized for nonequilibrium electronhole systems [3], one can obtain 1 Ê w/2  e FB ˆ ˘ Ê e2 ˆ ÏÔ È = Á ˜ Ì1  Í1 + exp Á ˜˙ kBT Ë 4 ¯ Ô ÎÍ Ë ¯ ˚˙ Ó 1 È Ê w/2 + e FB ˆ ˘ ¸Ô  Í1 + exp Á ˜˙ ˝ kBT ÍÎ Ë ¯ ˚˙ Ô ˛ 2 È Ê e FB ˆ ˘ Êe ˆ 4kBTt B Í1 exp +Á ˜ ln + ˜˙ Á Ë 4 ¯ p(1 + w 2t B2 ) ÎÍ Ë kBT ¯ ˙˚
Re s wB
for the bottom GL and
Ê w  2e F( k ) ˆ Ê e2 ˆ Re s w( k ) = Á ˜ tanh Á ˜ Ë 4 ¯ Ë 4kBT ¯
(26.1)
Model
È Ê e F( k ) ˆ ˘ Ê e2 ˆ 8kBTt Í1 exp +Á ˜ ln + ˜˙ Á Ë 4 ¯ p(1 + w 2t 2 ) ÍÎ Ë kBT ¯ ˙˚
(26.2)
for the GLs with 1 £ k £ K. Here tb and t are the electron and hole momentum relaxation times in the bottom and other GLs, respectively, T is the electron and hole temperature, and kB is the Boltzmann constant. The first and second terms in the righthand sides of Eqs. (26.1) and (26.2) correspond to the interband and intraband transitions, respectively, which are schematically shown by arrows in Fig. 26.1b. For simplicity we shall disregard the variation in the electron and hole densities in the bottom GL under the optical pumping, so that the electronhole system in this GL is assumed to be close to equilibrium with the Fermi energy e FB determined by the interaction with the SiC substrate.
Figure 26.1 (a) Schematic view of a laser with a MGL structure. (b) Occupied (by electrons) and vacant states in different GLs under optical pumping. Arrows show transitions related to interband emission and intraband absorption of THz photons with energy ℏw (interband transitions related to optical pumping as well the processes of intraband relaxation of the photogenerated electrons and holes are not shown).
469
470
Feasibility of Terahertz Lasing in Optically Pumped Epitaxial MGL Structures
The quasiFermi energies in the GLs with k ≥ 1 are mainly determined by the electron (hole) density in this layer Sk, i.e., (k ) e F( k ) µ S( k ) and, therefore, by the rate of photogeneration GW by the optical radiation (incident and reflected from the mirror) at the kth GL plane. Using Eq. (26.2) for ℏw = ℏW, we obtain (k) = GW
(k ) Ê Ê W  2e F( k ) ˆ IW pe2 ˆ tanh ˜. Á W ÁË c ˜¯ Ë 4kBT ¯
(26.3)
(k ) Here, IW is the intensity (power density) of the optical pumping radiation at the kth GL. At ℏW > 2e F( k ) (for all GLs), Eq. (26.3) yields (k ) (k ) GW � bIW /�W . Considering the attenuation of the optical pumping radiation due to its absorption in each GL, one can obtain
IW b[(1  b )K  k + (1  bB )2 (1  b )K + k 1 ] . (26.4) W Here IW is the intensity of incident pumping radiation and bB = (4p/c) s WB . The latter quantity accounts for the absorption of optical pumping radiation in the bottom layer. (k ) A relationship between e F( k ) and GW is determined by the (k ) g recombination mechanisms. We assume that e F( k ) µ [GW ] , where g is a phenomenological parameter. In this case, (k ) = GW
g
e F( k )
= e FB
2 2k1 ˘ È K k 1 + (1  bB ) (1  b ) ˙ , Í(1  b ) 1 + (1  bB )2 (1  b )2K1 ˚˙ ÎÍ
where e FB = e F(K ) is the quasiFermi energy in the topmost GL.
(26.5)
26.3 MGL Structure Net Dynamic Conductivity Taking into account that the thickness of the MGL structure is small in comparison with the wavelength of terahertz/FIR radiation, the generation and absorption of the latter is determined by the real part of the net dynamic conductivity K
Re s w = Re s wB + Re
Âs k =1
(k) w .
(26.6)
Taking into account that in the frequency range under consideration ℏw e FB , so that one can neglect the first term in the righthand
MGL Structure Net Dynamic Conductivity
side of Eq. (26.1) responsible for the interband absorption in the bottom GL, and using Eqs. (26.1), (26.2), and (26.6), we arrive at Ê e2 ˆ Re s w = Á ˜ Ë 4 ¯ +
ÏÔ È Ê e FB ˆ ˘ 4kBt B Í ln exp 1 + Ì Á ˜˙ 2 2 Ë kBT ¯ ˙˚ ÔÓ p(1 + w t B ) ÍÎ
È Ê e F(k) ˆ ˘ Í + ln 1 exp Á ˜˙ p(1 + w 2t 2 ) k=1 ÍÎ Ë kBT ¯ ˙˚ 8kBTt
K
+
Â k=1
K
Â
Ê w  2e F( k ) ˆ Ô¸ tanh Á ˜˝ . Ë 4kBT ¯ ˛Ô
(26.7)
The first two terms in the righthand side of Eq. (26.7) describe the intraband (Drude) absorption of terahertz radiation in all GLs, whereas the third term is associated with the interband transitions. When the latter is negative, i.e., when the interband emission prevails the interband absorption, the quantity Re sw as a function of w exhibits a minimum. At a strong optical pumping when the quantities e F(k) are sufficiently large, Re sw < 0 in this minimum as well as in a certain range of frequencies wmin < w < wmax. Here wmin and wmax are the frequencies at which Re sw = 0; they are determined by tb, t, and e FT (i.e., by the intensity of the incident optical pumping radiation). Since in the MGL structure in question e FB kBT, considering such frequencies that w2 t B2 , w2t2 1, one can reduce Eq. (26.7) to the following: Ê e2 ˆ Re s w = Á ˜ Ë 4 ¯
B 8kBT ÔÏ 4e F + Ì 2 2 ÔÓ p w t B pw t K
+
È Ê e (k ) ˆ ˘ ln ÍÍ1 + exp Á F ˜ ˙ ÍÎ Ë kBT ¯ ˙˚ k =1 K
Â
Ê w  2e F(k) ˆ ¸Ô ˜ ˝. 4kBT ¯ Ô ˛
Â tanh ÁË k =1
(26.8)
Under sufficiently strong optical pumping when e F(k) ℏw, kBT, and, consequently, tanh[(ℏw –2 e F(k) )/4kBT] ≃ –1, setting S Kk=1 e F(k) K * e FT , where K*< K, from Eq. (26.8) one obtains 4 Ê 4� ˆ Re s w Á 2 ˜ � Ë e ¯ p �w 2
Ê e FB 2K * e FT ˆ + ˜  K. Á t ¯ Ë tB
(26.9)
471
Feasibility of Terahertz Lasing in Optically Pumped Epitaxial MGL Structures 20
Re σω /(e /4h)
15
2
10 5 K = 20
0 5
50 100
T
εF = 15 meV
10 1.0
1.5
2.0
3.0
2.5
ω/2π, THz
Figure 26.2 Frequency dependences of the real part of dynamic conductivity Re sw normalized by quantity e2/4ℏ for MGL structures with different number of GLs K at modest pumping ( eFT = 15 meV).
26.4 Frequency Characteristics of Dynamic Conductivity Figures 26.2 and 26.3 show the frequency dependences of Re sw normalized by e2/4ℏ calculated for MGL structures with different K at different values of e FT (i.e., different optical pumping intensities) 1.0
2
T (k)
εF /εF
Re σω /(e /4h)
80 40
0.8
K = 20 50
100
0.6
0
50 k
0 T
40
εF = 30 meV
2
100 K = 20 50 100
20 0 20 40
80
Re σω /(e /4h)
472
40
0
2
4 6 8 10 ω/2π, THz
0
K = 20 50
T
ε = 50 meV
40 F 0.5
1.0
1.5
2.0
ω/2π, THz
2.5
100
3.0
Figure 26.3 Frequency dependences of the real part of dynamic conductivity Re sw normalized by quantity e2/4ℏ for MGL structures with different number of GLs K at eFT = 30 and 50 meV. The inset on the upper panel shows how the GL population varies with the GL index k, whereas the inset on the lower panel demonstrates the dependences but in a wider range of frequencies.
Frequency Characteristics of Dynamic Conductivity
using Eqs. (26.1), (26.2), (26.5), and (26.6) or Eqs. (26.5) and (26.7). We set e FB = 400 meV [8], ℏW = 920 meV, T = 300 K, tb = 1 ps, t = 10 ps, and g = 1/4. As seen from Figs. 26.2 and 26.3, Re sw can be negative in the frequency range w > wmin with wmin decreasing with increasing quasiFermi energy e FT in the topmost GL, i.e., with increasing optical pumping intensity (see below). In the MGL structures with K = 50– 100 at e FT = 30–50 meV, one has wmin/2p ≳ 1 THz (see Figs. 26.3 and 26.4). As follows from the inset on upper panel in Fig. 26.3, the quantities e F(k) are not too small in comparison with e FT even in GLs with the indices k K, i.e., in GLs near the MGL structure bottom. This implies that the pumping of such near bottom GLs is effective even in the MGL structures with K ~ 100. The quantity Re sw as a function of w exhibits a minimum (see the inset on lower panel in Fig. 26.3). The sign of Re sw becomes positive at w > wmax, where wmax is rather large (more than 10 THz). The MGL structures with a larger number K of GLs at stronger pumping exhibit smaller wmin and deeper minima Re sw. This is confirmed also by Fig. 26.5. 2.5
ωmin /2π, THz
T
εF = 15 meV = 30 meV = 50 meV
2.0
1.5
1.0 0
20
40
K
80
60
100
Figure 26.4 Dependences of wmin on number of GLs. 10 T
0
ω/2π = 1 THz
2
Re σω /(e /4h)
εF = 30 meV
10 ω/2π = 2 THz
20 30 0
ω/2π = 1.5 THz
20
40
K
60
80
100
Figure 26.5 Real part of the normalized dynamic conductivity as a function of the number of GLs for different frequencies. The line with markers corresponds to a MGL structure without the bottom GL.
473
474
Feasibility of Terahertz Lasing in Optically Pumped Epitaxial MGL Structures
26.5 Role of the Bottom GL The highly conducting bottom GL, whose existence is associated with the intrinsic features of the MGL structure growth, plays the negative role. This is mainly because it results in a marked absorption (due to the Drude mechanism) of the terahertz radiation emitted by other GLs. Since such an absorption increases with decreasing frequency, the achievement of the negative dynamic conductivity in the MGL structures with shorter momentum relaxation times tb and t even at higher frequencies is significantly complicated by the Drude absorption. This is demonstrated by Fig. 26.6 (upper panel). In contrast, a decrease in the Fermi energy e FB and the electron density in the bottom GL, of course, might significantly promote the achievement of negative dynamic conductivity in a wide frequency range, particularly at relatively low frequencies (compare the frequency dependences on upper and lower panels in Fig. 26.6). In this regard, the MGL structures with GLs exhibiting a long relaxation time t (like that found in Ref. [10]) but with a lowered electron density in the bottom GL or without the bottom layer appears to be much more preferable. Such MGL structures can be fabricated using chemical/mechanical reactions and transferred substrate techniques (chemically etching the substrate and the highly conducting bottom GL (Ref. [12]) or mechanically peeling the upper GLs, then transferring the upper portion of the MGL structure on a Si or equivalent transparent substrate). The calculation of Re sw for this MGL structure can be carried out by omitting the term Re sw in Eq. (26.6). The pertinent results are shown in Fig. 26.5 (see the marked line) and Fig. 26.7. Here, as in Fig. 26.3, we assumed that ℏw = 920 meV, T = 300 K, tb = 1 ps, and t = 10 ps. The obtained frequency dependences are qualitatively similar to those shown in Figs. 26.2 and 26.3. However the dependences for the MGL structures without the bottom layer exhibit a marked shift toward lower frequencies. In particular, as follows from Figs. 26.5 and 26.7, Re sw can be negative even at w/2p ≲ 1 THz (at chosen values of e FT ).
Role of the Bottom GL
τ = 0.3 ps = 0.5 ps = 1 ps
4 T
2
Re σω /(e /4h)
8
εF = 30 meV τB = 0.1 ps K = 100
0 4
B 8 εF = 400 meV
4
2
Re σω /(e /4h)
8
0 4 B 8 εF = 200 meV
2
4
6
8
ω/2π, THz
10
Figure 26.6 Real part of the normalized dynamic conductivity vs frequency calculated for MGL structures with tb = 0.1 ps and different t and eFB .
2
Re σω /(e /4h)
80 40 0
40
K = 20 T
εF = 30 meV
50 100
2
Re σω /(e /4h)
80 40 0
K = 20 50
T 40 εF = 50 meV
0.5
1.0
100
1.5
2.0
ω/2π, THz
2.5
3.0
Figure 26.7 Real part of the normalized dynamic conductivity vs frequency calculated for MGL structures with different numbers of GLs and without bottom GL.
475
476
Feasibility of Terahertz Lasing in Optically Pumped Epitaxial MGL Structures
26.6 Condition of Lasing To achieve lasing in the MGL structures under consideration, the following condition should be satisfied [7]:
8p Re s w  E t2 > (1  r1 )E12 + (1  r2 )E22 + (a/R )2 E12 + ES2 . (26.10) c
Here, Et, E1, and E2 are maximum amplitudes of the terahertz electric field E = E(z) at the MGL structure (placed at the distance t from the bottom mirror, where t is the thickness of the substrate), and near the pertinent mirror, respectively, ES2 = (a S nS /2) Ú 0t E 2dz, aS and nS are the absorption coefficient of THz radiation in the substrate (SiC or Si) and real part of its refraction index, r1 and r2 are the reflection coefficients of THz radiation from the mirrors, and a/R is the ratio of the diameters of the output hole a and the mirror R. In deriving inequality (26.10), we neglected the finiteness of the MGL thickness (in comparison with t and the THz wavelength) and disregarded the diffraction losses. For simplicity, one can set E t ~ E 12 ~ E 22 and ES2 ~ (ta S nS /2)E22 , disregarding, in particular, partial reflection of THz radiation from the bottom GL. In this case, inequality (26.10) can be presented as 8p  Re s w  > (1  r1 ) + (1  r2 ) + (a/R)2 + ta S nS /2 = L. (26.11) c Assuming that r1 = r2 = 0.99, (a/R) = 0.1, aS ≃ 2–4 cm–1, nS ≃ 3 [13], and t = 50 mm, for L one obtains L = 0.06–0.09. However, as follows from Fig. 26.5, the quantity (8p/c)Re sw for a MGL structure with K = 100 at w/2p = 1.5 THz at e FT = 30 meV is about 12b ≃ 0.275. At w/2p = 1.0 THz but for the structure without the bottom GL (see the line with markers in Fig. 26.5), one obtains (8p/c)Re sw ≃ 0.345. These values of (8p/c)Re sw well exceed the above value of L (in contrast with the structures with two GLs [7], for which the minimization of the losses is crucial). At the elevated frequencies, the ratio (8p/c)Re sw/L can be even much larger. Considering that the electron (hole) density ST in the topmost GL S = T
•
2
p
2
dpp
Ú 1 + exp[(u p  e 0
F
T F )/kBT ]
at e FT = 30 meV at T = 300 K, we obtain ST ≃ 2 ¥ 1011 cm–2. Such a value (and higher) of the photogenerated electron and hole density
Conclusions
is achievable experimentally (see, for instance, Ref. [14]). Assuming that K = 100, ℏW = 920 meV, and the recombination time tr ≃ 20 ps at T = 300 K and ST ≃ 2 ¥ 1011 cm–2 [15], for the pertinent optical pumping power we obtain IW ≃ 6.4 ¥ 104 W/cm2. One needs to point out that this value of IW is much larger than the threshold of lasing at a certain frequency (wmin < w < wmax). At T = 100 K, the recombination time (due to optical phonon emission) is much longer [15], hence, the electron and hole densities in question can be achieved at much weaker optical pumping. In the regime sufficiently beyond the threshold of lasing, when the stimulated radiative recombination becomes dominant, the pumping efficiency is determined just by the ratio of the energy of the emitted terahertz photons ℏw and the energy of optical photons ℏW, h = w/W. However, the nonradiative recombination mechanisms can markedly decrease h. In the regime in question, the maximum output terahertz power can be estimated as max Pw ≃ pR2(w/W)IW. For example, at ℏW = 920 meV, ℏw/2p = 5.9 meV (w/2p ≃ 1.5 THz), 2R = 0.1 cm, and IW = 3 ¥ 104 W/cm2, one obtains max Pw ≃ 1.5 W.
26.7 Conclusions
We studied real part of the dynamic conductivity of a MGL structure with a stack of GLs and a highly conducting bottom GL on SiC substrate pumped by optical radiation. It was shown that the negative dynamic conductivity in the MGL structures under consideration with sufficiently large number K of perfect upper GLs can be achieved even at room temperature provided the optical pumping is sufficiently strong. Due to large K, the absolute value of Re sw in its minimum can significantly exceed the characteristic value of conductivity e2/4ℏ. Thus, the MGL structures can serve as active media of terahertz lasers. This can markedly liberate the requirement for the quality of the terahertz laser resonant cavity. An increase in tb and t promotes widening of the frequency range where Re sw < 0, particularly, at the low end of this range. This opens up the prospects of terahertz lasing with w/2p ~ 1 THz even at room temperature. The main obstacle appears to be the necessity of sufficiently long relaxation times tb and t in GLs with rather high electron and hole
477
478
Feasibility of Terahertz Lasing in Optically Pumped Epitaxial MGL Structures
densities: S >1011 cm–2. Since the electronhole recombination at the temperatures and densities under consideration might be attributed to the optical phonon emission [15], the optical pumping intensity required for terahertz lasing can be markedly lowered (by orders of magnitudes) with decreasing temperature. The conditions of lasing in the MGL structures without the bottom GL are particularly liberal.
Acknowledgments
One of the authors (V. R.) is grateful to M. Orlita and F. T. Vasko for useful discussions and information. This work was supported by the Japan Science and Technology Agency, CREST, Japan.
Appendix: Recombination
The rate of radiative recombination in the degenerate electronhole system in the topmost GL due to spontaneous emission of photons at e FT kBT can be calculated using the following formula [6, 16]: Rr �
2ur
p �3
e FT /uF
Ú
dpp2 =
0
2ur (e FT )3 3p �3uF3
µ (e FT )3 .
(26.A1)
Here ur = æ (8e2 /3c)(uF /c )2 uF and æ is the dielectric constant pF = e FT /uF . The rate of the electronhole recombination associated with emission of optical phonons can be described the following equation [14]: w0 /uF
Rph µ
Ú 0
dpp(w 0 /uF  p)
È Ê w 0  uF p  e FT ˆ ˘ Ê u p  e FT ˆ ˘ È Í1 + exp p Í1 + exp Á F ˙ Á ˜˙ ˜ kBT Ë kBT ¯ ˙˚ ÍÎ Ë ¯ ˙˚ ÎÍ Ê 2e T  w 0 ˆ µ exp Á F ˜. kBT ¯ Ë
(26.A2)
Equalizing RrT and the rate of generation of electrons and holes by the optical pumping radiation GWT and the recombination rate, and considering Eqs. (26.A1) and (26.A2), one can find that
References
e FT µ (GWT )1/3 and e FT µ ln (GWT ) , respectively. The radiative interband transitions stimulated by the thermal photons can also contribute to the recombination rate [6, 16] as well as the processes of electronhole interaction in the presence of disorder. These processes provide different dependences of the recombination rate on the quasiFermi energy. Due to this, calculating the dependence of the latter in different GLs on the optical pumping intensity, we put, for definiteness, e FT µ (GWT )g with g = 1/4. Such a dependence is less steep than that for the spontaneous radiative recombination and somewhat steeper than in the case of optical phonon recombination. The variation in parameter g leads to some change in the e F(k)  k dependence, but it should not affect the main obtained results.
References
1. C. Berger, Z. Song, T. Li, X. Li, A. Y. Ogbazhi, R. Feng, Z. Dai, A. N. Marchenkov, E. H. Conrad, P. N. First, and W. A. de Heer, J. Phys. Chem., 108, 19912 (2004). 2. K. S. Novoselov, A. K. Geim, S. V. Morozov, D. Jiang, M. I. Katsnelson, I. V. Grigorieva, S. V. Dubonos, and A. A. Firsov, Nature (London), 438, 197 (2005).
3. V. Ryzhii, M. Ryzhii, and T. Otsuji, J. Appl. Phys., 101, 083114 (2007).
4. M. Ryzhii and V. Ryzhii, Jpn. J. Appl. Phys., Part 2, 46, L151 (2007). 5. F. Rana, IEEE Trans. Nanotechnol., 7, 91 (2008).
6. A. Satou, F. T. Vasko, and V. Ryzhii, Phys. Rev. B, 78, 115431 (2008).
7. A. A. Dubinov, V. Ya. Aleshkin, M. Ryzhii, T. Otsuji, and V. Ryzhii, Appl. Phys. Express, 2, 092301 (2009).
8. F. Varchon, R. Feng, J. Hass, X. Li, B. Ngoc Nguyen, C. Naud, P. Mallet, J.Y. Veuillen, C. Berger, E. H. Conrad, and L. Magaud, Phys. Rev. Lett., 99, 126805 (2007). 9. M. Orlita, C. Faugeras, P. Plochocka, P. Neugebauer, G. Martinez, D. K. Maude, A.L. Barra, M. Sprinkle, C. Berger, W. A. de Heer, and M. Potemski, Phys. Rev. Lett., 101, 267601 (2008).
10. P. Neugebauer, M. Orlita, C. Faugeras, A.L. Barra, and M. Potemski, Phys. Rev. Lett., 103, 136403 (2009).
11. L. A. Falkovsky and A. A. Varlamov, Eur. Phys. J. B, 56, 281 (2007).
479
480
Feasibility of Terahertz Lasing in Optically Pumped Epitaxial MGL Structures
12. A. Bostwick, T. Ohta, T. Seyller, K. Horn, and E. Rotenberg, Nat. Phys., 3, 36 (2007).
13. J. H. Strait, P. A. George, J. M. Dawlaty, S. Shivaraman, M. Chanrashekhar, F. Rana, and M. G. Spencer, Appl. Phys. Lett., 95, 051912 (2009).
14. J. M. Dawlaty, S. Shivaraman, M. Chandrashekhar, F. Rana, and M. G. Spencer, Appl. Phys. Lett., 92, 042116 (2008). 15. F. Rana, P. A. George, J. H. Strait, S. Shivaraman, M. Chanrashekhar, and M. G. Spencer, Phys. Rev. B, 79, 115447 (2009). 16. F. T. Vasko and V. Ryzhii, Phys. Rev. B, 77, 195433 (2008).
Chapter 27
Terahertz Lasers Based on Optically Pumped Multiple Graphene Structures with SlotLine and Dielectric Waveguides*
V. Ryzhii,a,b A. A. Dubinov,a,c T. Otsuji,b,d V. Mitin,e and M. S. Shurf aComputational
Nanoelectronics Laboratory, University of Aizu, AizuWakamatsu 9658580, Japan bJapan Science and Technology Agency, CREST, Tokyo 1070075, Japan cInstitute for Physics of Microstructures, Russian Academy of Sciences, Nizhny Novgorod 603950, Russia dResearch Institute for Electrical Communication, Tohoku University, Sendai 9808577, Japan eDepartment of Electrical Engineering, University at Buffalo, State University of New York, New York 14260, USA fDepartment of Electrical, Electronics, and Systems Engineering, Rensselaer Polytechnic Institute, Troy, New York 12180, USA [email protected]
*Reprinted with permission from V. Ryzhii, A. A. Dubinov, T. Otsuji, V. Mitin, and M. S. Shur (2010). Terahertz lasers based on optically pumped multiple graphene structures with slotline and dielectric waveguides, J. Appl. Phys., 107, 054505. Copyright © 2010 American Institute of Physics. GrapheneBased Terahertz Electronics and Plasmonics: Detector and Emitter Concepts Edited by Vladimir Mitin, Taiichi Otsuji, and Victor Ryzhii
Copyright © 2021 Jenny Stanford Publishing Pte. Ltd.
ISBN 9789814800754 (Hardcover), 9780429328398 (eBook)
www.jennystanford.com
482
Terahertz Lasers Based on Optically Pumped Multiple Graphene Structures
Terahertz (THz) lasers on optically pumped multiplegraphene layer (MGL) structures as their active region are proposed and evaluated. The developed device model accounts for the interband and intraband transitions in the degenerate electronhole plasma generated by optical radiation in the MGL structure and the losses in the slot or dielectric waveguide. The THz laser gain and the conditions of THz lasing are found. It is shown that the lasers under consideration can operate at frequencies 1 THz at room temperatures.
27.1 Introduction
Graphene, graphene nanoribbons, and graphene bilayers (see, for instance, Ref. [1]) can be used in different terahertz (THz) devices [2–9]. Optical excitation of graphene can result in the interband population inversion and negative real part of the dynamic conductivity of a graphene layer sw in the THz range of frequencies [7–9]. The negativity of the real part of the dynamic conductivity implies that the interband emission of photons with the energy ℏw, where ℏ is the reduced Planck constant, prevail over the intraband (Drude) absorption. If the THz photon losses in the resonant cavity are sufficiently small, the THz lasing can be realized in graphenebased devices with optical pumping [10, 11]. In Refs. [10, 11], the optically pumped THz lasers with a Fabry–Pérot resonator were considered. In this chapter, we propose and evaluate the THz lasers based on multiplegraphenelayer (MGL) structures with a metal slotline waveguide (SLW) or a dielectric waveguide (DW) pumped by optical radiation. The specific features of characteristics of the MGLbased lasers under consideration are associated with the frequency dependences of the absorption in the waveguides and the gainoverlap factor, which is sensitive to the spatial distribution of the THz electric field. As shown in the following, the characteristics of the lasers with SLW and DW are fairly similar, so that we will mainly focus on the device with SLW. This is in part because the structures with SLW exhibit somewhat better confinement, and can be used not only for MGLbased lasers with optical pumping but also in MGLbased injection lasers with lateral pin junctions (both electrically induced [12–14] and formed by pertinent doping of MGL structure).
Device Model
27.2 Device Model We consider lasers (a) with a MGL structure on a SiC or Si substrate with the side highly conducting metal strips and a highly conducting back electrode at the substrate bottom and (b) with a MGL structure on the top of a SiC or Si slab serving as a DW. The crosssections (corresponding to the y–z plane) of the device structures under consideration are schematically shown in Fig. 27.1. The axis x corresponds to the direction of the electromagnetic wave propagation, whereas the y and z directions are in the MGL structure plane and perpendicular to it, respectively (see Fig. 27.1 ). The MGL plane corresponds to z = 0. The finiteness of the MGL structure thickness can be disregarded. It is assumed that the MGL structure under consideration comprises K upper GLs and a highly conducting bottom GL on a SiC substrate or K GLs (without the bottom GL) on a Si substrate. Epitaxial MGL structures with up to K = 100 GLs with very long momentum relaxation time of electrons and holes (t 20 ps) were recently fabricated using the thermal decomposition from 4HSiC substrate [15]. MGL structures without the bottom GL can be fabricated using chemical/mechanical reactions and transferred substrate techniques, which include chemically etching the substrate and the highly conducting bottom GL (Ref. [16]) (or mechanically peeling the upper GLs) and transferring the upper portion of the MGL structure on a Si or equivalent transparent substrate. Since the electron density and the Fermi energy e FB in the bottom GL is rather large ( e FB 400 meV) [17], the Drude absorption in this GL can be significant although it can be overcome by a strong emission from the upper GLs if their number is sufficiently large. The MGL structures without the bottom GL can exhibit significant advantages (see Ref. [11] and below).
(a)
(b)
Figure 27.1 Schematic views of the device structures under consideration: (a) with a SLW and (b) with a DW.
483
484
Terahertz Lasers Based on Optically Pumped Multiple Graphene Structures
It is assumed that the MGL structure is illuminated from the top by light with the energy of photons ℏW. The optical waveguide input of the pumping radiation is also possible. When ℏW is close to Nℏw0/2, where ℏw0 0.2 eV is the optical phonon energy and N is an integer, the photogeneration of electrons and holes and their cooling, associated with the cascade emission of optical phonons, result in an essentially occupation (population inversion) of low energy states near the bottom of the conduction band and the top of the valence band. At elevated electron and hole densities (i.e., at sufficiently strong optical pumping), the electron and hole distributions in the range of energies e ℏw0 in the kth GL (1 £ k £ K) can be described by the Fermi functions with the quasiFermi energies e F(k) . The quasiFermi energies in the GLs with k ≥ 1 are mainly determined by the electron (hole) density in this layer Sk, i.e., (k) by e F(k) µ S(k) and, therefore, by the rate of photogeneration GW the optical radiation at the kth GL plane. Considering the attenuation of the optical pumping radiation due to its absorption in each GL, one can obtain (k) GW =
IW b [(1  b )K  k + (1  bB )2 (1  b )K + k 1 ]. W
(27.1)
Here, IW is the intensity of incident pumping radiation, b = pe2/ ℏc 0.023, where e is the electron charge, c is the speed of light in vacuum, and bB = (4p/c)Re s WB . The latter quantity accounts for the absorption of optical pumping radiation in the bottom (k) is determined by the layer. A relationship between e F(k) and GW recombination mechanisms [11]. As a result, e F(k) can be expressed via the quasiFermi energy in the topmost GL e FT = e F(K) , which, in turn, is a function of the intensity of incident pumping radiation IW. Since the thickness of the MGL structure is small in comparison with the wavelength of THz radiation, the generation and absorption are determined by the real part of the net dynamic conductivity, which is the sum of the real parts of the dynamic conductivity of the bottom GL Re s wB and other GLs s w(k) K
Re s w = Re s wB + Re
Âs k =1
(k) w .
(27.2)
Device Model
Considering the expressions for Re s wB and Re s w(k) obtained previously [11], one can arrive at the following: È
Ê e FB ˆ ˘ Ê e 2 ˆ Ï
Ô 4kBTt B Í1 ln
ex
Re s w = Á ˜ Ì p +
Á ˜ ˙
+ w 2t B2 ) ÍÎ (1 Ë 4 ¯ ÓÔ p � ˙ Ë kBT ¯ ˚
+
8kBTt
K
(k ) ˆ ˘ È
Ê e � ln Í1 + exp Á F ˜ ˙ Ë kBT ¯ ˙˚
ÎÍ
Â
p � (1 + w 2t 2 ) k=1
Ê w  2e F(k) ˆ Ô¸ tanh Á ˜ ˝. Ë 4kBT ¯ ˛Ô k=1 K
Â
+
(27.3)
Here, tb and t are the electron and hole momentum relaxation times in the bottom and other GLs, respectively, T is the electron and hole temperature, and kB is the Boltzmann constant. The first two terms in the righthand side of Eq. (27.3) are associated with the intraband (Drude) absorption of THz radiation in all GLs, whereas the third term corresponds to the interband transitions. In the case of lasers without the bottom GL, one can use Eq. (27.3) formally setting tb = •. The electromagnetic waves propagating along the SLW was considered using the following equation, which is a consequence of the Maxwell equations: ∂2Ew ( y , z ) ∂ y 2
+
∂2Ew ( y , z ) ∂ z 2
2 È w � ˘
+ Í 2 h( y , z )  q2 ˙ Ew ( y , z ) = 0. (27.4)
˙˚
ÍÎ c
Here, Ew(y, z) the amplitude of the yth component of the THz electric field E(t, x, y, z) = Ew(y, z)exp[i(qx – wt)], h(y, z) is the complex permittivity, q is the wavenumber of the propagating mode. The quantities Ew(y, z), dEw(y, z)/dz, and h–1(y, z)d[h(y, z)Ew(y, z)]/dy are continuous at the interfaces between the layers with different refractive indices. The boundary conditions for the guided mode correspond to the condition Ew(y, z) Æ 0 at y, z Æ ±•. Equation (27.4) was solved numerically using the effective index and transfermatrix methods (see, for instance, Refs. [18, 19]). The coefficient of absorption of the propagating mode aw and the coefficient of reflection from the interfaces between the laser structure edges and vacuum R were calculated using the following formulas, respectively: aw= 2 Im q and R = (q – q0)/(q + q0)2, where q0 = w/c. The THz gain, which describes the attenuation or amplification of the propagating
485
486
Terahertz Lasers Based on Optically Pumped Multiple Graphene Structures
mode, under optical pumping can be calculated using the following formula: gw =
where
4p Re s w c hS
Gw  aw ,
(27.5)
D/2
Gw =
Ú
•
 Ew ( y , 0) 2 dy
D/2 •
Ú Ú E
• •
w ( y,
z ) dydz 2
(27.6)
is the gainoverlap factor (in the case when sw is independent of coordinate y) and hS is the permittivity of the substrate (SiC or Si).
(a)
(b)
Figure 27.2 Coefficients of (a) absorption and (b) reflection vs frequency for SLWs with different geometrical parameters.
Results and Discussion
(a)
(b)
Figure 27.3 Spatial distributions of THz electric field (a) in SLW crosssection and (b) in DW crosssection.
27.3 Results and Discussion Figure 27.2 shows the absorption coefficient aw of electromagnetic waves propagating along the SLW and the coefficient of reflection from the laser structure edges as function of frequency w/2p calculated using Eq. (27.4) for different widths of the slot D and the strips Dc and the substrate thickness W. The strips and the back electrode are assumed to be made of Al. Examples of the spatial distributions of the THz electric field in the electromagnetic wave in laser structures with D =15 mm at w/2p = 1.8 THz in question are show in Fig. 27.3. The electric field distributions with the frequency dependences of the dynamic conductivity of the MGL structures obtained by solving Eq. (27.4) were substituted to Eqs. (27.5) and (27.6) to find the gainoverlap factor and the THz gain. Figures
487
488
Terahertz Lasers Based on Optically Pumped Multiple Graphene Structures
27.4 and 27.5 show the frequency dependences of the THz gain gw calculated for the laser structures with (Fig. 27.4) and without (Fig. 27.5) bottom GL and with different structural parameters at different pumping conditions (different values of the quasiFermi energy) and at T = 300 K. It was assumed that ℏW = 920 meV, t = 10 ps, and tb = 1 ps. The chosen value of t is twice as small as that found
(a)
(b)
Figure 27.4 Frequency dependences of THz gain in laser structures with different width of the slot D and different number of GL K at different values of the quasiFermi energy e FT : (a) D = 10 mm and (b) D = 15 mm.
(a)
(b)
Figure 27.5 The same as in Fig. 27.4 but for laser structures without bottom GL.
Results and Discussion
experimentally [15] in MGL structures with different number of GLs (up to K = 100). To take into account a shortening of the momentum relaxation time with significant increasing electron density, this time in the bottom GL was chosen ten times shorter than in other GLs. As seen from comparison of the top panels of Figs. 27.4 and 27.5, the laser structures with and without the bottom GL (with K = 20) exhibit qualitatively similar frequency dependences of the THz gain gw (at chosen geometrical parameters) but with somewhat higher maxima in the latter structures. In the case of the structures with K =100, these dependences (compare lower panels of Figs. 27.4 and 27.5) are virtually identical. The frequency wmin at which gw changes its sign is wmin/2p 2 THz in the laser structures of both types.
(a)
(b)
Figure 27.6 Comparison of THz gain vs frequency dependences in laser structures (a) with and (b) without bottom GL, and with different spacing between MGL structure and back electrode W.
489
490
Terahertz Lasers Based on Optically Pumped Multiple Graphene Structures
The latter is different from the situation in the MGL lasers with the Fabry–Pérot resonator [11], in which eliminating the bottom GL can lead to a pronounced decrease in wmin. This is attributed to the effect of SLW: the variation in the frequency results in a redistribution of the spatial distribution of the THz electric field and, hence, in a change in the gainoverlap factor. Due to this, the spacing between the MGL structure W and the back electrode affects the frequency dependences of the THz gain. Figure 27.6 shows these dependences calculated for different W. One can see that the height of the THz gain maxima decreases with increasing W. Simultaneously the frequency wmin shifts toward lower values. This shift is more pronounced in the laser structures without the bottom GL (compare Figs. 27.6a and b). As seen from Fig. 27.6b, wmin/2p can reach 1 THz. In the case of larger K and e FT , as seen from Fig. 27.7, the THz gain in the range w/2p 1–2 THz can be rather large.
d
Figure 27.7 The same as in Fig. 27.6a but for K = 100 and e FT = 50 meV.
A decrease in the momentum relaxation time t (which results in an enhancement in the Drude absorption) leads to an increase in wmin and to a decrease in Re sw in the range of frequencies, where Re sw < 0. This is seen in Fig. 27.8. The above results correspond to T = 300 K. Lowering of the temperature should lead to widening of the frequency range where Re sw is negative and where gw can be positive. As a result, wmin might decrease with decreasing temperature. The latter is confirmed by the calculated temperature dependences of wmin shown in Fig. 27.9.
Results and Discussion
Figure 27.8 Frequency dependences of THz gain in laser structures (without the bottom GL) with different t.
(a)
(b)
Figure 27.9 Temperature dependences of wmin for laser structures with different t: (a) W = 12 mm and (b) W = 25 mm.
491
492
Terahertz Lasers Based on Optically Pumped Multiple Graphene Structures
Figure 27.10 shows the frequency dependences of the THz gain calculated for laser structures with SLW and DW for T = 300 K and t = 10 ps. One can see that the maximum of the THz gain in the laser with SLW is somewhat higher than that in the laser with DW. This can primarily be explained by the effect of the spatial distribution of the THz electric field on the gainoverlap factor (compare Figs. 27.3a and b). To maximize the THz gain at the desirable frequency, one needs carefully optimize the geometrical parameters.
Figure 27.10 Comparison of the frequency dependences of THz gain in laser structures with SLW and DW.
Considering the propagation of the THz electromagnetic wave in the laser structure (with the length L in the xdirection) and its reflection from edges or from the external mirrors (with the reflective coefficients R1 and R2), the condition of lasing can be presented as Lgw > ln
1 . R1 R2
(27.7)
For a laser structure with SLW with D = 15 mm, W = 12 mm, and K = 100 at e FT = 30–50 meV and w/2p = 3.0 THz, so that R1 = R2 0.05 and gw 30–60 cm–1 (see Figs. 27.2b and 27.4b, respectively), one obtains L > 0.1–0.2 cm. If D = 15 mm, W = 25 mm, and K = 100 at e FT = 50 meV and w/2p = 1.5 THz (R1 = R2 0.05 and gw 10 cm–1 as follows from Figs. 27.2b and 27.7, respectively), one obtains L > 0.6 cm. As shown above, at the quasiFermi in the topmost GL about e FT = 30–50 meV, the achievement of the THz lasing in the devices
References
under consideration at room temperatures is feasible. At T = 300 K the condition e FT 30 meV corresponds to the electron and hole densities about 2 ¥ 1011 cm–2. Such densities can be obtained at reasonable optical powers (see Ref. [12] and the references therein).
27.4 Conclusions
We proposed THz lasers with optical pumping based on MGL structures with waveguides and calculated their characteristics. The feasibility of lasing in the devices under consideration at the low end of the THz frequency range at room temperatures was demonstrated.
Acknowledgments
The authors are grateful to V. V. Popov, M. Ryzhii, A. Satou, M. Suemitsu, and F. T. Vasko for fruitful discussions. This work was supported by the Japan Science and Technology Agency, CREST, Japan.
References
1. A. H. Castro Neto, F. Guinea, N. M. R. Peres, K. S. Novoselov, and A. K. Geim, Rev. Mod. Phys., 81, 109 (2009). 2. F. T. Vasko and V. Ryzhii, Phys. Rev. B, 77, 195433 (2008).
3. V. Ryzhii, V. Mitin, M. Ryzhii, N. Ryabova, and T. Otsuji, Appl. Phys. Express, 1, 063002 (2008). 4. F. Xia, T. Mueller, R. GolizadehMojarad, M. Freitag, Y. Lin, J. Tsang, V. Perebeinos, and P. Avouris, Nano Lett., 9, 1039 (2009).
5. V. Ryzhii and M. Ryzhii, Phys. Rev. B, 79, 245311 (2009).
6. Y. Kawano and K. Ishibashi, Proceedings of the 34th International Conference on Infrared, and Terahertz Waves, Busan, Korea, 21–25 September 2009, (unpublished), W4A04.0380. 7. V. Ryzhii, M. Ryzhii, and T. Otsuji, J. Appl. Phys., 101, 083114 (2007). 8. F. Rana, IEEE Trans. Nanotechnol., 7, 91 (2008).
9. A. Satou, F. T. Vasko, and V. Ryzhii, Phys. Rev. B, 78, 115431 (2008).
10. A. A. Dubinov, V. Ya. Aleshkin, M. Ryzhii, T. Otsuji, and V. Ryzhii, Appl. Phys. Express, 2, 092301 (2009).
493
494
Terahertz Lasers Based on Optically Pumped Multiple Graphene Structures
11. V. Ryzhii, M. Ryzhii, A. Satou, T. Otsuji, A. A. Dubinov, and V. Ya. Aleshkin, J. Appl. Phys., 106, 084507 (2009).
12. V. V. Cheianov and V. I. Fal’ko, Phys. Rev. B, 74, 041403(R) (2007).
13. M. Ryzhii and V. Ryzhii, Jpn. J. Appl. Phys., Part 2, 46, L151 (2007). 14. M. Ryzhii and V. Ryzhii, Physica E (Amsterdam), 40, 317 (2007).
15. P. Neugebauer, M. Orlita, C. Faugeras, A.L. Barra, and M. Potemski, Phys. Rev. Lett., 103, 136403 (2009).
16. A. Bostwick, T. Ohta, T. Seyller, K. Horn, and E. Rotenberg, Nat. Phys., 3, 36 (2007).
17. F. Varchon, R. Feng, J. Hass, X. Li, B. Ngoc Nguyen, C. Naud, P. Mallet, J. Y. Veuillen, C. Berger, E. H. Conrad, and L. Magaud, Phys. Rev. Lett., 99, 126805 (2007). 18. K. J. Ebeling, Integrated Optoelectronics: Waveguide Optics, Photonics, Semiconductors (SpringerVerlag, Berlin, 1993).
19. M. Born and E. Wolf, Principles of Optics: Electromagnetic Theory of Propagation, Interference and Diffraction of Light (Pergamon, Oxford, 1964).
Chapter 28
Observation of Amplified Stimulated Terahertz Emission from Optically Pumped Heteroepitaxial GrapheneonSilicon Materials*
H. Karasawa,a T. Komori,a T. Watanabe,a A. Satou,a,c H. Fukidome,a,c M. Suemitsu,a,c V. Ryzhii,b,c and T. Otsujia,c aResearch Institute of Electrical Communication, Tohoku University, 211 katahira, Aobaku, Sendai, Miyagi 9808577, Japan bDepertment of Computer Science and Engineering, University of Aizu, AizuWakamatsu 9658580, Japan cJSTCREST, 35 Chiyodaku, Tokyo 1020075, Japan [email protected]
We experimentally observed the fast relaxation and relatively slow recombination dynamics of photogenerated electrons/holes in a heteroepitaxial grapheneonSi material under pumping with a
*Reprinted with permission from H. Karasawa, T. Komori, T. Watanabe, A. Satou, H. Fukidome, M. Suemitsu, V. Ryzhii, and T. Otsuji (2011). Observation of amplified stimulated terahertz emission from optically pumped heteroepitaxial grapheneon silicon materials, J. Infrared Millimeter Terahertz Waves, 32, 655–665. Copyright © 2010 Springer Science+Business Media. GrapheneBased Terahertz Electronics and Plasmonics: Detector and Emitter Concepts Edited by Vladimir Mitin, Taiichi Otsuji, and Victor Ryzhii
Copyright © 2021 Jenny Stanford Publishing Pte. Ltd.
ISBN 9789814800754 (Hardcover), 9780429328398 (eBook)
www.jennystanford.com
496
Observation of Amplified Stimulated Terahertz Emission
1550 nm, 80 fs pulsed fiber laser and probing with the corresponding terahertz beam generated by and synchronized with the pumping laser. The timeresolved electricnearfield intensity originating from the coherent terahertz photon emission is electrooptically sampled in totalreflection geometry. The Fourier spectrum fairly agrees the product of the negative dynamic conductivity and the expected THz photon spectrum reflecting the pumping photon spectrum. This phenomenon is interpreted as an amplified stimulated terahertz emission.
28.1 Introduction
Graphene is a singlelayer carbonatomic honeycomb lattice crystal. Electrons and holes in graphene hold a linear dispersion relation with zero bandgap [1–3]. Since the discovery of the singlelayer graphene by Geim et al. [4] in 2004, with their very primitive methodology of peeling the grapheite, graphene has made a great impact in academic and industry. In this situation, we have studied the dynamic ac conductivity of nonequilibrium twodimensional electronhole systems in optically pumped graphene and have expected negativedynamic conductivity in far infrared and terahertz (THz) spectral ranges in optical pumping [5] at room temperature, due to the gapless energy spectrum. And considering the negativedynamic conductivity, a very fast relaxation (£1 ps) and relatively slow recombination (>>1 ps) [6], the population inversion can be achieved. We think this effect can be used the graphenebased coherent source of THz radiation [7, 8]. It is known that photoexcited carriers in graphene are first cooled and thermalized mainly by intraband relaxation processes on femtosecond to subpicosecond time scales, and then by interband recombination processes. Recently the ultrafast carrier relaxation via emissions from optical phonons has observed by Kamprath et al. [9], Wang et al. [10] and George et al. [11]. The measured optical phonon lifetimes found were ~7 ps [9], 2–2.5 ps [10], and ~1 ps [11], respectively. More precisely, Breusing et al. [12] revealed that photoelectons and photoholes in optically pumped exfoliated graphene and graphite loose a major fraction of their energy within 200~300 fs, mainly by emission of optical phonons.
Theoretical Model
In this work, we observe amplified stimulated THz emission in optically pumped and THzprobed epitaxial graphene heterostructures. The results reflect the recombination of photoelectrons and photoholes after the intraband ultrafast carrier relaxation via optical phonon emission, and provide evidence for the occurrence of negative dynamic conductivity in the terahertz spectral range.
28.2 Theoretical Model
When graphene is optically excited with photon energy ℏW, electrons and holes are photogenerated and first establish separate quasiequilibrium distributions at around the level ef ± ℏW/2 (ef: Fermi energy) within 20–30 fs after the excitation by the carriercarrier (cc) scattering (see Fig. 28.1b). When the electronic temperature is not so high, the relaxation process is followed by cooling of these electrons and holes mainly by emission of a cascade of optical phonons (ℏw0)within 200~300 fs to occupy the states (see Fig. 28.1c) e
± en ª ef ± ℏ(W/2 – Nw0)
(28.1)
Re s w = Re s winter + Re s wintra
(28.2)
f
where en < ℏw0, N = 1, 2, 3, . . . Then, thermalization occurs via electronhole recombination as well as intraband Fermization due to cc scattering and carrierphonon (cp) scattering (as shown with energy ℏwq in Fig. 28.1a) on a few picoseconds time scale (see Fig. 28.1d), while the interband cc scattering and cp scattering are slowed by the density of states effects and Pauli blocking [12]. The real part of the net ac conductivity, Re sw, is proportional to the absorption of photons with frequency w and comprises the contributions of both interband and intraband transitions. Here the contribution of intraband transition corresponds to the Drudelike mechanism of THz photon absorption and interband transition corresponds to the generation/recombination rates [5, 6]. The real part of the conductivity corresponds to the imaginary part of the permittivity: Im e. Im e means the energy loss. Hence the negativedynamic conductivity gives energy gain.
497
498
Observation of Amplified Stimulated Terahertz Emission
Figure 28.1 Schematic view of graphene band structure (a) and energy distributions of photogenerated electrons and holes when electronic temperature is comparable to the lattice temperature (b–d). Arrows denote transitions corresponding to optical excitation by photons with energy ℏW, cascade emission of optical phonons with energy ℏw0, and radiative recombination with emission of photons with energy ℏw. (b) after ~20 fs from optical pumping, (c) after ~200 fs from optical pumping (shaded distribution is the case for high electronic temperature), (d) after a few ps from optical pumping.
Let us consider a situation under weak pumping with infrared photons: T ª T0, eF < kBT, ℏW >> kBT, trad >> t, kBTt/ℏ < w2t2,
where T is the electron temperature, T0 is the lattice temperature, eF is the Fermi level, kB is the Boltzmann constant, trad is the electronhole radiative recombination lifetime, t is the intraband momentum relaxation time of electrons/holes, ℏ is the reduced Plank constant, and w is the angular frequency. Re s winter and Re s wintra become [9]
Theoretical Model
e2 È Ê w ˆ Ê w ˆ ˘  fh Á Í1  fe ÁË ˜ Ë 2 ¯˜ ˚˙ 4 Î 2 ¯ e F ˆ e2 Ê w p e2 t rad ˆ e2 Ê w I , = ª Á 8 ÁË 2kBT kBT ¯˜ 8 Ë 2kBT W S 0 W ¯˜ (28.3)
Re s winter =
Re s wintra ª
kBTt (ln2 + e F /2kBT )e2 , p (1 + w 2t 2 )
(28.4)
where e is the elementary charge, vF is the Fermi velocity, S0 is the carrier density in the dark, f(e,h) is the FermiDirac distribution function (e: electrons, h: holes), and IW is the pumping intensity. The contribution of the intraband transition: Re s wintra takes positive, decreasing monotonically and approaching 0 with increasing w, while the interband term contributes to the linear decrease (increase) in the intraband term in the low (high) w region. The breakeven frequency depends on IW and trad. Therefore, Resw is a minimum at a specific frequency: w = w . Around w = w , Resw becomes [5] Re s w @
where
2 I ˘ e2 g È 3 Êw wˆ Í1 + Á  W˙ ˜ 8 Í 2Ë w ¯ IW ˙ ˚ Î
Ê 4 ln 2 ˆ g = 2Á Ë p ˜¯ Ê k Tt ˆ w ªÁ B ˜ Ë ¯
1/3
1/3
,
B
2/3
Ê ˆ IW ª 11 1Á Ë kBTt ˜¯
Ê ˆ ÁË k Tt ˜¯
(28.5)
1.92 , t
1/3
2
Ê kBT ˆ W ÁË v ˜¯ t , F rad
(28.6)
and vF is the Fermi velocity (~106 m/s). As seen from Eq. 28.5, Resw is a minimum at w = w . When the pumping intensity exceeds the threshold IW > I W, the dynamic conductivity becomes negative. When T = 300 K, t = 10–12 s, and trad = 10–9 ~ 10–11 s, this threshold is
499
500
Observation of Amplified Stimulated Terahertz Emission
I W ª 60 ~ 6000 W/cm2. Assuming a device size of 100 mm ¥ 100 mm, we find that the pumping intensity required for negative dynamic conductivity is I W ª 6 ~ 600 mW. The value of 6 mW is a feasible pumping intensity (see Fig. 28.2). When graphene is strongly pumped (eF > kBT), Resw becomes [5] Re s w @
2 e2 È Ê w ˆ IW ˘ Í1 + 0.43Á ˜ ˙. Ë w ¯ IW ˙ 4 Í Î ˚
(28.7)
Figure 28.2 Calculated dynamic conductivity for various pumping intensities at 300 K. The vertical scale is normalized to the characteristic conductivity e2/4ℏ.
Equation 28.7 shows that Re sw changes from negative to positive at extremely high intensity; thus, at w = w , for example, Re sw < 0 when I W < I0 < 5 I W [5]. For the electronhole recombination, radiative recombination via directtransition to emit photons ℏw ª 2en and nonradiative recombination via Auger processes, plasmon emissions, and phonon emissions [11, 14–16] are considered. However, in the case of the radiative recombination, due to the relatively small values of ℏw ª 2en < 2ℏw0, as well as the gapless energy spectrum, photon emissions over a wide THz frequency range are expected if the pumping photon energy is suitably chosen and the pumping intensity is sufficiently high. The incident photon spectra are expected to be reflected in the THz photoemission spectra as evidence that such a process occurs.
Graphene on Silicon Sample for the Experiment
28.3 Graphene on Silicon Sample for the Experiment In order to verify the proposed concept, we conduct an experimental study on the electromagnetic radiation emitted from an optically pumped graphene structure. The sample used in this experiment is heteroepitaxial graphene film grown on a 3CSiC(110) thin film heteroepitaxially grown on a 300 mm thick Si(110) substrate via thermal graphitization of the SiC surface [17–19]. In the Raman spectrum of the graphene film, the principal bands of graphene, namely, the G (1595 cm–1) and G¢ (2730 cm–1) bands, are observed, as shown in Fig. 28.3. Furthermore, transmission electron microscopy
Figure 28.3 The Raman spectrum of the graphene, the principal bands of graphene, namely, D (1365 cm–1), G (1595 cm–1) and G¢ (2730 cm–1) bands. G band shows the structure of graphite and graphene. The peak at 1595 cm–1 corresponds to an optical phonon energy of 197.8 meV at the zone center. G¢ band is expressed as a single component related to the twodimensionality of the graphene film. The presence of D band indicates inclusion of defected graphite.
images indicate that the film is stratified. It is thus concluded that epitaxial graphene with a planar structure can be produced by this fabrication method. Furthermore, the epitaxial graphene layer is inferred to have a nonBernal stacking arrangement because the G¢ band in the Raman spectrum can be expressed as a single component related to the twodimensionality of the graphene film [20, 21]. The nonBernal stacked epitaxial graphene layers grown by
501
502
Observation of Amplified Stimulated Terahertz Emission
our method can be treated as a set of isolated single graphene layers, as in the case of an epitaxial graphene layer on a Cterminated SiC bulk crystal [22]. The Gband peak at 1595 cm–1 corresponds to an optical phonon energy at the zone center of 197.8 meV.
28.4 Experimental
We measure the carrier relaxation and recombination dynamics in optically pumped epitaxial grapheneonsilicon (GOS) heterostructures using THz timedomain spectroscopy based on an optical pump/THzandopticalprobe technique. The timeresolved field emission properties are measured by an electrooptic sampling method in totalreflection geometry [23]. To obtain the THz photon emissions from the abovementioned carrier relaxation/ recombination dynamics, the pumping photon energy (wavelength) is carefully selected to be around 800 meV (1550 nm). To perform intense pumping beyond the threshold, a femtosecond pulsed fiber laser with full width at halfmaximum (FWHM) of 80 fs, pulse energy of 50 pJ/pulse, and frequency of 20 MHz was used as the pumping source. The setup is shown in Figs. 28.4a–c. The graphene sample is placed on the quartz base stage and a 80 µm thick (101)oriented CdTe crystal is placed onto the sample; the CdTe crystal acts as a THz probe pulse emitter as well as an electrooptic sensor. The single femtosecond fiber laser beam is split into two beams: one for optical pumping and generating the THz probe beam, and the other for optical probing. The pumping laser, which is linearly polarized and mechanically chopped at ~1.2 KHz, is simultaneously focused at normal incidence onto the sample and the CdTe from below, while the probing laser, which is crosspolarized to the pumping beam, is focused from above. The incident pumping beam is defocused to about 50 μm in diameter on the sample to satisfy the abovementioned pumping power requirements. The resulting photoexcited carrier density is ~8 ¥ 1010 cm–2, which is comparable to the background carrier density. Owing to nonlinear optical effects, the CdTe crystal can rectify the pumping laser pulse to emit THz envelope radiation. This THz emission irradiate the graphene sample, acting as THz probe signals to stimulate THz photon emission via electronhole recombination in the GOS.
Experimental
Figure 28.4 Measurement setup for opticalpump/THzandopticalprobe spectroscopy. (a) Schematic image of stimulated THz emission from graphene by the opticalpump/THzprobe signals. (b) Pump/probe geometry. Left: CdTe crystal on top of the graphene sample generates THz probe pulse and allows electrooptic detection of THz electric field intensity. Right: optical pump beam (red line) generates the THz pulse making double reflection to work for the THz probe (blue line). The THz pulse also propagate through the GOS sample and reflect back (dashed blue line). (c) Electrooptic sampling setup.
503
504
Observation of Amplified Stimulated Terahertz Emission
The opticalpumping/THzprobing geometry and these beam propagations are schematically shown in Fig. 28.4b. The electric field intensity of the THz radiation is electroopticaly detected at the top surface of the CdTe crystal. Along with the propagation of the optical pump pulse through the CdTe crystal the THz pulse is generated and grows up. The THz pulse being emitted from the CdTe crystal is partially reflected at the top surface of the CdTe then subject back to the graphene, working as the THz probe pulse (shown with arrowed blue line in Fig. 28.4b). The graphene responds to this THz probe pulse radiation giving rise to stimulated THz emission. The emitted THz radiation reflects again at the heterointerface of the 80 nm thick SiC epilayer and the Si substrate, and then returns back to the top surface of the CdTe crystal. The propagation times of the THz probe pulse through the CdTe and graphene/SiC epilayer are 1000 fs and 0.75 fs, respectively (assuming the refractive index of CdTe and SiC in the THz frequencies to be 3.75 and 2.8, respectively). The total roundtrip propagation time of the THz pulse through the CdTe crystal and graphene/SiC epilayer is 2001.5 fs (~2.0 ps). Therefore the original data of the temporal response that we observe in this experiment consist of the first forward propagating THz pulsation (no interaction with graphene) followed by the double reflected secondary THz pulsation (probing the graphene) just 2.0 ps after the first pulsation. The third THz pulsation comes ~6.6 ps after the second pulsation by reflecting at the bottom surface of the GOS as shown in Fig. 28.4b with dashed arrowed blue line, which is sufficiently separated in time from the second pulsation. We focus to observe the secondary THz pulsation that reflects the response of graphene. The optical pump beam also partially reflects at the top surface of the CdTe crystal so that it may weakly pump the graphene. The time delay of the THz probing with respect to the first and second optical pumping is calculated to be 2.0 ps and 560 fs (assuming the infrared refractive index of the CdTe to be 2.69), respectively. On the other hand, through the Si prism attached to the CdTe crystal, the optical probing beam is totally reflected back to the lockin detection block, and its phase information reflecting the electric field intensity is lockin amplified. By sweeping the timing of the optical probe using an optical delay line, the whole temporal profile of the field emission properties can be obtained. The system
Results and Discussion
bandwidth is estimated to be around 6 THz, which is limited mainly by the Reststrahlen band of the CdTe sensor crystal. Figure 28.5 shows the autocorrelations and spectral profiles of the pumping laser beam. The horizontal axis indicates the wavelength and frequency together with the estimated THz photon frequency to be emitted from the sample. The estimated THz photon spectrum Fℏw(=W–2N◊w0)(W – 2N ◊ w0) is the replica of the pumping photon spectrum FℏW(W). The dotted line plots the dynamic conductivity at a pumping intensity twice as high as the threshold intensity calculated for 300 K using Eqs. 28.2–28.4 with a t value of 2 ¥ 10–12 ps. The shaded area shows the negative dynamic conductivity.
Figure 28.5 Temporal (autocorrelation) and spectral profiles of pumping laser pulse used in this experiment. Dotted line denotes the dynamic conductivity normalized to the characteristic conductivity e2/2ℏ at a pumping intensity of twice the threshold intensity at 300 K calculated using Eqs. 28.2–28.4. Shaded area denotes negative dynamic conductivity.
28.5 Results and Discussion We observed THz emissions from the CdTe crystal only without the GOS sample and from the CdTe and the GOS sample. To confirm the effects of the THz probe, we replace the first CdTe crystal with another CdTe crystal having a highreflectivity coating for IR on its bottom surface, in order to eliminate generation of the THz probe signal. In this case, no distinctive response is observed with or
505
506
Observation of Amplified Stimulated Terahertz Emission
without graphene. Since the measurements are taken as an average, the observed response is undoubtedly a coherent process that cannot be obtained via spontaneous emission processes, providing clear evidence of stimulated emission.
Figure 28.6 Typical measured temporal response of THz emission. The first pulsation (marked with a dashed circle line) is the direct propagating component, while the second pulsation (marked with a shaded solid circle line) is the double reflecting component interacting with graphene.
Typical raw data of observed temporal response is shown in Fig. 28.6. As is mentioned in IV, we extracted the temporal response of the secondary THz pulsation (designated with a shaded circle) from the measured raw data to identify the frequency response of the graphene. Figure 28.7a shows the measured temporal responses, in which repetitively measured results are overlaid, showing the measurement reproducibility. Figure 28.7b shows the Fourier spectra corresponding to the typical traces plotted with thick lines in Fig. 28.7a. Owing to the secondorder nonlinear optical effects, the emission from “CdTe only” without the GOS sample exhibits a temporal response similar to optical rectification with a single peak at around 1 THz and an upper weak side lobe extending to around 5 THz as shown by the green lines in Fig. 28.7b. On the other hand, the temporal profile of the result from “CdTe and GOS” intensifies the pulsed response with higher frequency components so that its Fourier spectrum exhibits the growth of the main lobe around 2 to 4 THz and the lower side lobe around 1 THz. The main lobe fairly corresponds to the expected gain spectral region which is shown with
Results and Discussion
the dashed line in Fig. 28.7b, while the side lobe fairly corresponds to the component of THz probe signal generated from the CdTe. It is inferred that the THz emissions from graphene are stimulated by the coherent THz probe radiation from the CdTe. Furthermore, the THz emissions are amplified via photoelectron/hole recombination in the range of the negative dynamic conductivity.
Figure 28.7 (a) Measured temporal profiles and (b) their Fourier spectra when the THz probe beam is generated by the optical rectification in the CdTe crystal. Dashed line in (b) is the photoemission spectrum predicted from the pumping laser spectrum and the negative dynamic conductivity.
The dashed line in Fig. 28.7b is the expected gain spectrum. The THz gain: gw is proportional to the negative dynamic conductivity Resw(< 0) and is given by gw = 4pResw/ (c e ) ◊ Gw, where Gw is the gain overlap factor [24]. Therefore, the gain spectrum: G(w) for the radiation of THz photon ℏw from graphene stimulated by the THz probe signal is calculated as the product of gw and the estimated THz photon spectrum Fℏ(W–2N◊w0)(w), the replica of the pumping photon
507
508
Observation of Amplified Stimulated Terahertz Emission
spectrum: G(w) = g(w) ◊ Fℏ(W–2N◊w0)(w). The transfer function of the GOS response is obtained by the calculation of the “CdTe and GOS” spectrum divided by the “CdTe only” spectrum. If the calculated GOS transfer function corresponds to G(w), the experimental results support the above mentioned assumption. The comparison between them is shown in Fig. 28.8. As is seen in Fig. 28.8, the experimental result fairly agrees with the calculated G(w).
Figure 28.8 The gain profile of the GOS sample (plotted with the thicker line) which is calculated by the ratio of the emission spectrum of the “CdTe + GOS” to the spectrum of the “CdTe only”. The expected spectrum (dashed line) and the emission spectrum from “CdTe only” (thinner line) are also plotted for comparison.
To see the Fourier spectrum shown in Figs. 28.7b and 28.8 in detail, its highfrequency part of the main lobe is weakened and lowered by ~0.5 THz with respect to the expected spectra. This result reflects the timedependent energy relaxation of photoelectrons and photoholes in graphene as shown in Fig. 28.1b–d. As is mentioned in IV, the time duration from the optical pumping to the THz probing is 2.0 ps for the first pumping and 560 fs for the second weak pumping. Thus, it is considered that the photoelectrons/holes are stimulated when they start thermalization after losing their energy via the cascade of optical phonon emissions, but still stay in the nonequilibrium state with population inversion corresponding to Fig. 28.1b and d.
References
The THz probe timing with respect to the optical pump timing could be changed by using various CdTe crystals having different thickness. This will help further detail observation of the carrier relaxation/recombination dynamics. We should put a halfreflective coating at the surface (attached to the CdTe) of the Si prism like ITO to increase the S/N. These will be the future subject.
28.6 Conclusion
We measured the carrier relaxation and recombination dynamics in optically pumped epitaxial grapheneonsilicon (GOS) heterostructures using THz timedomain spectroscopy based on an optical pump/THzandopticalprobe technique. We successfully observed coherent amplified stimulated THz emissions arising from the fast relaxation and relatively slow recombination dynamics of photogenerated electrons/holes in an epitaxial graphene heterostructures. The results provide evidence of the occurrence of negative dynamic conductivity, which can potentially be applied to a new type of THz laser.
Acknowledgments
The authors thank Yu Miyamoto and Hiroyuki Handa at RIEC, Tohoku University, Japan for their providing grapheneonsilicon samples, and also Maxim Ryzhii at University of Aizu for his valuable discussion. This work was financially supported in part by the JSTCREST program, Japan, and a GrantinAid for Basic Research (S) from the Japan Society for the Promotion of Science.
References
1. A. K. Geim and K. S. Novoselov, Nat. Mater., 6, 183 (2007).
2. K. S. Novoselov, A. K. Geim, S. V. Morozov, D. Jiang, M. I. Katsnelson, I. V. Grigorieva, S. V. Dubonos, and A. Firsov, Nature, 438, 197 (2005). 3. P. Kim, Y. Zhang, Y.W. Tan, and H. L. Stormer, Nature, 438, 201 (2005).
4. K. S. Novoselov, A. K. Geim, S. V. Morozov, D. Jiang, Y. Zhang, S. V. Dubonos, I. V. Grigorieva, and A. A. Frisov, Science, 306, 666 (2004).
509
510
Observation of Amplified Stimulated Terahertz Emission
5. V. Ryzhii, M. Ryzhii, and T. Otsuji, J. Appl. Phys., 101, 083114 (2007).
6. L. A. Falkovsky and A. A. Varlamov, Eur. Phys. J. B, 56, 281 (2007).
7. A. A. Dubinov, V. Y. Aleshkin, M. Ryzhii, T. Otsuji, and V. Ryzhii, Appl. Phys. Express, 2, 092301 (2009).
8. V. Ryzhii, M. Ryzhii, A. Satou, T. Otsuji, A. A. Dubinov, and V. Y. Aleshkin, J. Appl. Phys., 106, 084507 (2009).
9. T. Kampfrath, L. Perfetti, F. Schapper, C. Frischkorn, and M. Wolf, Phys. Rev. Lett., 95, 187403 (2005).
10. H. Wang, J. H. Strait, P. A. George, S. Shivaraman, V. B. Shields, M. Chandrashekhar, J. Hwang, F. Rana, M. G. Spencer, C. S. RuizVargas, and J. Park, Arxiv 0909.4912 (2009).
11. P. A. George, J. Strait, J. Dawlaty, S. Shivaraman, M. Chandrashekhar, F. Rana, and M. G. Spencer, Nano Lett., 8, 4248 (2008).
12. M. Breusing, C. Ropers, and T. Elsaesser, Phys. Rev. Lett., 102, 086809 (2009).
13. By substituding Eqs. (9) and (12) and a = e2/cℏ (appearing just after Eq. (9)) into Eq. (13), all in [5], one can obtain the righthand side of Eq. (28.3) in this chapter. Equation (14) in [5] corresponds to Eq. (28.4) in this chapter. 14. F. Rana, P. A. George, J. H. Strait, J. Dawlaty, S. Shivaraman, M. Chandrashekhar, and M. G. Spencer, Phys. Rev. B, 79, 115447 (2009).
15. N. Bonini, M. Lazzeri, N. Marzari, and F. Mauri, Phys. Rev. Lett., 99, 176802 (2007).
16. F. Rana, Phys. Rev. B, 76, 155431 (2007).
17. M. Suemitsu, Y. Miyamoto, H. Handa, and A. Konno, eJ. Surf. Sci. Nanotechnol., 7, 311 (2009).
18. Y. Miyamoto, H. Handa, E. Saito, A. Konno, Y. Narita, M. Suemitsu, H. Fukidome, T. Ito, K. Yasui, H. Nakazawa, and T. Endoh, eJ. Surf. Sci. Nanotechnol., 7, 107 (2009).
19. H. Fukidome, Y. Miyamoto, H. Handa, E. Saito, and M. Suemitsu, Jpn. J. Appl. Phys., 49, 01A1103 (2010).
20. L. G. Cançadoa, K. Takaia, T. Enokia, M. Endob, Y. A. Kimb, H. Mizusakib, N. L. Spezialic, A. Jorioc, and M. A. Pimentac, Carbon, 46, 272 (2008).
21. C. Faugeras, A. Nerrière, M. Potemski, A. Mahmood, E. Dujardin, C. Berger, and W. A. de Heer, Appl. Phys. Lett., 92, 011914 (2008).
References
22. J. Hass, F. Varchon, J. E. MillánOtoya, M. Sprinkle, N. Sharma, W. A. de Heer, C. Berger, P. N. First, L. Magaud, and E. H. Conrad, Phys. Rev. Lett., 100, 125504 (2008).
23. L. Min and R. J. D. Miller, Appl. Phys. Lett., 56, 524 (1999).
24. V. Ryzhii, A. A. Dubinov, T. Otsuji, V. Mitin, and M. S. Shur, J. Appl. Phys., 107, 054505 (2010).
511
Chapter 29
Toward the Creation of Terahertz Graphene Injection Laser*
V. Ryzhii,a M. Ryzhii,a V. Mitin,b and T. Otsujic aComputational Nanoelectronics Laboratory, University of Aizu,
AizuWakamatsu 9658580, Japan
bDepartment of Electrical Engineering, University at Buffalo, Buffalo,
New York 142601920, USA
cResearch Institute for Electrical Communication, Tohoku University,
Sendai 9808577, Japan
[email protected]
We study the effect of population inversion associated with the electron and hole injection in graphene pin structures at the room and slightly lower temperatures. It is assumed that the recombination and energy relaxation of electrons and holes are associated primarily with the interband and intraband processes assisted by optical phonons. The dependences of the electronhole and optical phonon *Reprinted with permission from V. Ryzhii, M. Ryzhii, V. Mitin, and T. Otsuji (2011). Toward the creation of terahertz graphene injection laser, J. Appl. Phys., 110, 094503. Copyright © 2011 American Institute of Physics. GrapheneBased Terahertz Electronics and Plasmonics: Detector and Emitter Concepts Edited by Vladimir Mitin, Taiichi Otsuji, and Victor Ryzhii
Copyright © 2021 Jenny Stanford Publishing Pte. Ltd.
ISBN 9789814800754 (Hardcover), 9780429328398 (eBook)
www.jennystanford.com
514
Toward the Creation of Terahertz Graphene Injection Laser
effective temperatures on the applied voltage, the currentvoltage characteristics, and the frequencydependent dynamic conductivity are calculated. In particular, we demonstrate that at low and moderate voltages, the injection can lead to a pronounced cooling of the electronhole plasma in the device isection to the temperatures below the lattice temperature. However at higher voltages, the voltage dependences can be ambiguous exhibiting the Sshape. It is shown that the frequencydependent dynamic conductivity can be negative in the terahertz (THz) range of frequencies at certain values of the applied voltage. The electronhole plasma cooling substantially reinforces the effect of negative dynamic conductivity and promotes the realization of terahertz lasing. On the other hand, the heating of optical phonon system can also be crucial affecting the realization of negative dynamic conductivity and terahertz lasing at the room temperatures.
29.1 Introduction
The gapless energy spectrum of electrons and holes in graphene layers (GLs), graphene bilayers (GBLs), and nonBernal stacked multiple graphene layers (MGLs) [1–3] opens up prospects of creating terahertz (THz) lasers based on these graphene structures. In such structures, GLs and MGLs with optical [4–10] and injection [11] pumping can exhibit the interband population inversion and negative dynamic conductivity in the THz range of frequencies and, hence, can serve as active media in THz lasers. The most direct way to create the interband population in GLs and MGLs is to use optical pumping [4] with the photon energy ℏW0 corresponding to middleand nearinfrared (IR) ranges. In this case, the electrons and holes, photogenerated with the kinetic energy ℏQ0/2, transfer their energy to optical phonons and concentrate in the states near the Dirac point [4, 12, 13]. The amplification of THz radiation from optically pumped GL structures observed recently [14, 15] is attributed to the interband stimulated emission. However, the optical pumping with relatively high photon energies exhibits drawbacks. First of all, the optical pumping, which requires complex setups, might be inconvenient method in different applications of the prospective graphene THz lasers. Second, the excessive energy being received by the photogenerated electrohole plasma from pumping source
Introduction
can lead to its marked heating because of the redistribution of the initial electron and hole energy ℏW0/2 among all carries due to rather effective intercarrier collisions. The latter results in a decrease of the ratio of the quasiFermi energies me and mh to the electronhole effective temperature T that, in turn, complicate achieving of sufficiently large values of the dynamic conductivity. As demonstrated recently [16, 17], the negative conductivity at the THz frequencies is very sensitive to the ratio of the photon energy ℏW and the optical phonon energy ℏw0, as well as to the relative efficiency of the intercarrier scattering and the carrier scattering on optical phonons. The decay of nonequilibrium optical phonons also plays an important role. The abovementioned complications can be eliminated in the case of pumping resulting in the generation in GLs electrons and holes with relatively low initial energies. This in part can be realized in the case of optical pumping with ℏW0/2 < ℏw0 [16]. Taking into account that in GLs ℏw0 0.2 eV, in the case of CO2 laser as a pumping source, W0/w0 0.5. As shown [16], in such a case, the electronhole plasma can even be cooled, so that T < T0, where T0 is the lattice (thermostat) temperature. Another weakly heating or even cooling pumping method which can provide low effective temperature T (including T < T0) is the injection pumping of electrons from nsection and holes from psection in GL and MGL structures with pin junctions. In this chapter, we study the injection phenomena in GL and MGL pin structures and calculate their characteristics important for THz lasers. The idea to use pn junctions in GLs was put forward and briefly discussed by us previously [11]. Here, we consider more optimal designs of the structures (with a sufficiently long isection) and account for realistic mechanisms of recombination at elevated temperatures (at the room temperature and slightly below). This chapter is organized as follows. In Section 29.2, we describe the device structures under consideration and principles of their operation. The pertinent equations of the model governing the balance of electrons, holes, and optical phonons (rate equations) are presented in Section 29.3. These equations are reduced to an equation governing the electronhole effective temperature. The solution of this equation in Sections 29.4 and 29.5 (both analytically in limiting cases and numerically) allows us to find the effective temperature of optical phonons and the current as functions of the applied
515
516
Toward the Creation of Terahertz Graphene Injection Laser
voltage, the structural parameters, and the lattice temperature. In Section 29.6, the obtained characteristics of the injected electronhole plasma are used to calculate the dependence of the dynamic conductivity of the latter as a function of the signal THz frequency and other quantities. Section 29.7 deals with the model limitations and discussion. In Section 29.8, we draw the main conclusions.
29.2 Device Model
We consider devices which comprise a GL or a MGL structure with several nonBernal stacked GLs. It is assumed that the sections of GLs adjacent to the side contacts are doped (p and nsections). The device structure under consideration is shown in Fig. 29.1a. The dc voltage V is applied between the side contacts to provide the forward bias of the pin junction. Due to doping of the side sections with the acceptor and donor sheet concentration Σi, the electron and hole Fermi energies counted from the Dirac point are me = mi and mh = –mi, where mi � �uF pS i , ℏ is the reduced Planck constant and uF 108 cm/s is the characteristic velocity of the carrier spectrum in GLs. Instead of doping of the side sections, the p and nsections can be created using highly conducting gates over these sections to which the gate voltages Vp = –Vg < 0 and Vn = Vg > 0 are applied [11]. In this case, the chemically doped p and nsections are replaced by the electrically induced sections (see, for instance [18, 19]), as shown in Fig. 292b. In singleGL structures, mi µ Vg /Wg , where Wg is the spacing between the GL and the gate. In the case of MGL structures, the situation becomes more complex due to the screening of the transverse electric field in GLs (Ref. [19]) although the effective electric doping can be achieved in MGL structures with about dozen GLs. For definiteness, in the following, we shall consider primarily the devices with chemically doped pin junctions. As shown below, under certain conditions, the frequencydependent dynamic conductivity of the GL or MGL structures can be negative in a certain range of the signal frequencies. In this case, the selfexcitation of THz modes propagating in the substrate serving as a dielectric waveguide (in the direction perpendicular to the injection current) and lasing is possible. The metal gates in the devices with electrically induced pi and in junctions can also serve as the slotline waveguides for
Device Model
THz waves. Apart from this, the selfexcitation of surface plasmons (plasmonpolaritons) is possible as well (see, for instance, Refs. [4, 6, 8–10]).
Figure 29.1 Schematic view of the crosssections of MGL laser structures (a) with chemically doped n and psections and (b) with such section electrically induced by the side gatevoltages Vp = –Vg and Vn = Vg > 0.
Figure 29.2 Band profiles of a GL in pin junctions (a) at V = 0 and (b) at forward bias V > 0. Opaque and open circles correspond to electrons and holes, respectively. Wavy arrows show some interband (recombination) and intraband transitions assisted by optical phonons. Smooth arrows indicate tunneling and thermionic leakage processes.
517
518
Toward the Creation of Terahertz Graphene Injection Laser
When the pin junction under consideration is forward biased by the applied voltage V, the electrons and holes are injected to the isection from the pertinent doped side sections. The injected electrons and holes reaching the opposite doped section can recombine at it due to the interband tunneling or escape the isection due to the thermionic processes. The band profiles in the structures under consideration at V = 0 and at the forward bias V > 0 are shown in Fig. 29.2. Since the probability of such tunneling is a very sharp function of angle of incidence, the leakage flux due to the tunneling electrons (holes) is much smaller that the flux of injected electrons (holes). The currents associated with the tunneling and thermionic leakage of electrons at the pijunction and holes at the injunction depend on the electric field at the pertinent barriers and the applied voltage V. Because the relative role of the leakage currents diminishes with increasing length of the isection 2L, width of the pi and in junctions l, and the barrier height at these junctions mi, we shall neglect it. The pertinent conditions will be discussed in the following. Thus, it is assumed that the main fractions of the injected electrons and holes recombine inside the isection. The recombination of electrons and holes in GLs at not too low temperatures is mainly determined by the emission of optical photons [20]. Considering the subthreshold characteristics (i.e., the states below the threshold of lasing) and focusing on the relatively hightemperature operation, we shall account for this recombination mechanism and disregard others [21–24] including the mechanism [25] associated with the tunneling between the electronhole puddles (if any) [26–29]. Due to high net electron and hole densities in MGL structures with sufficient number of GLs, the latter mechanism can be effectively suppressed [25]. We also assume that the net recombination rate in the whole isection is much smaller than the fluxes of injected electrons and holes.
29.3 Equations of the Model
Due to rather effective intercarrier scattering, the electron and hole distribution functions (at least at not too high energies) can be very close to the Fermi distribution functions with quasiFermi energies me and mh and the electronhole effective temperature T. The latter
Equations of the Model
quantities are generally different from those in equilibrium (without pumping) at which me = mh = 0 and T = T0. At the pumping of an intrinsic GL structure, me = –mh = m, where generally m > 0. Under these conditions, the quasiFermi energy m in the isection (neglecting the leakage and recombination in the lowest approximation), is given by (see Fig. 29.2b) m
= eV/2,
(29.1)
where e is the electron charge. The terminal current between the side contacts (per unit length in the lateral direction perpendicular to the current), which coincides with the recombination current, is given by J = 2eLR0inter
(29.2)
The rate of the optical phononassisted interband transitions (recombination rate) R0inter and the rate of the intraband energy relaxation associated with optical phonons R0intra can be calculated using the following simplified formulas [9, 16] (see, also Ref. [20]): R0inter =
˘ S0 È Ê 2m  w 0 ˆ  N0 ˙ ( N 0 + 1) exp Á ˜ inter Í Ë ¯ T t0 Î ˚
=
˘ S0 È Ê eV  w 0 ˆ ( 0 + 1) exp Á (N  N0 ˙ , ˜ inter Í Ë ¯ T t0 Î ˚
R0intra =
˘ S0 È Ê w ˆ (N 0 + 1) exp Á  0 ˜  N 0 ˙ . intra Í Ë T ¯ t0 Î ˚
(29.3) (29.4)
Here, t 0inter and t 0intra are the pertinent characteristic times (relatively slow dependent on m and T), S0 is the equilibrium electron and hole density, and N0 is the number of optical phonons. Here and in all equations in the following, T and T0 are in the energy units. When the optical phonon system is close to equilibrium, one can put N0 = [exp(ℏw0/T0) – 1]–1 = N 0eq . For numerical estimates, we set
R0inter = S 0 /t 0inter 1023 cm–2s–1 [20]. Equations (29.2) and (29.3) yield the following general formula for the structure currentvoltage characteristic: J=
˘ 2eLS 0 È Ê eV  w 0 ˆ  N0 ˙ . ( N 0 + 1) exp Á ˜ inter Í Ë ¯ T t0 Î ˚
(29.5)
519
520
Toward the Creation of Terahertz Graphene Injection Laser
Naturally, at V = 0, T = T0, so that N0 = [exp(ℏw0/T0)–1]–1 and J = 0. At V > 0, due to contributions of the recombination and injection to the energy balance of the electrohole plasma in the isection, the electronhole effective temperature T can deviate from the lattice temperature T0. The number of optical phonons N0 can also be different from its equilibrium value N 0eq . Since ℏw0 is large, in a wide range of temperatures (including the room temperatures), ℏw0 T0. The electronhole plasma gives up the energy ℏw0 in each act of the optical phonon emission (interband and intraband) and receives the same energy absorbing an optical phonon. Hence, the net rate of the energy transfer from and to the electron holeplasma due to the interaction with optical phonons is equal to 2Lw 0 (R0inter + R0intra ) . Considering Eqs. (29.3) and (29.4) and taking into account that the Joule power associated with the injection current is equal to Q = JV = 2eLR0interV , an equation governing the energy balance in the electronhole plasma in the isection can be presented as ˘ Ê eV  w 0 ˆ eV È ( N 0 + 1) exp Á ˜  N0 ˙ inter Í ¯ Ë T t0 Î ˚
=
˘ w 0 È Ê eV  w 0 ˆ ( N 0 + 1) exp Á  N0 ˙ ˜ inter Í Ë ¯ T t0 Î ˚ +
˘ w 0 È Ê w ˆ ( N0 + 1) exp Á  0 ˜  N0 ˙ . intra Í Ë T ¯ t0 Î ˚
(29.6)
Here, the lefthand side corresponds to the power received by the electronhole plasma in the isection from the pumping source, whereas the righthand side corresponds to the power transferred to or received from the optical phonon system. The number of optical phonons is governed by an equation which describes the balance between their generation in the interband and intraband transitions and decay due to the anharmonic contributions to the interatomic potential, leading to the phononphonon scattering and in the decay of optical phonons into acoustic phonons. This equation can be presented in the form
Equations of the Model
(N 0  N 0eq ) t 0decay
1
=
t 0inter
+
1 t 0intra
˘ È Ê eV  w 0 ˆ  N0 ˙ Í( N 0 + 1) exp Á ˜ ¯ Ë T Î ˚ È ˘ Ê w 0 ˆ  N0 ˙ , Í( N 0 + 1) exp Á ˜ Ë T ¯ Î ˚
(29.7)
where t 0decay is the optical phonon decay time. This time can be markedly longer than t 0inter and t 0intra , particularly in suspended GLs, so that parameter h0decay = t 0decay /t 0inter can exceed or substantially exceed unity. As shown [30–34], t 0decay in GLs is in the range of 1–10 ps. As calculated recently [17], the characteristic times t 0inter and t 0intra can be longer than 1 ps. If so, the situation when h0decay < 1 appears also to be feasible. The optical phonon decay time might be fairly short depending on the type of the substrate. Instead of Eq. (29.7), one can use the following equation which explicitly reflexes the fact that the energy received by the electronhole plasma from the external voltage source goes eventually to the optical phonon system h0decay
È ˘ Ê eV  w 0 ˆ  N0 ˙ = N0  N0eq . (29.8) Í( N0 + 1) exp Á ˜ Ë ¯ T Î ˚
eV w 0
Using Eqs. (29.6) and (29.7) or Eqs. (29.6) and (29.8), one can find T and N0 as functions of V and then calculate the currentvoltage characteristic invoking Eq. (29.5), as well as the dynamic characteristics. Equation (29.8) yields N 0eq + h0decay
N0 = 1 + h0decay
eV w 0
Ê eV  w 0 ˆ eV exp Á ˜¯ Ë w 0 T
È Ê eV  w 0 ˆ ˘ Í1  exp Á ˜¯ ˙ Ë T Î ˚
.
(29.9)
Substituting N0 given by Eqs. (29.9) to (29.6), we arrive at the following equation for T: Ê eV  w 0 ˆ ˘ eV È Í1  exp Á ˜¯ ˙ Ë T w 0 Î ˚ e  w 0 ˆ Ê eV decay eV exp Á + h0 ˜¯ Ë T w 0
1 + h0dexay N 0eq
521
522
Toward the Creation of Terahertz Graphene Injection Laser
˘ È (w 0  eV ) Ê eV ˆ ¥ Íh0 exp Á ˜ + 1˙ Ë T ¯ w 0 Î ˚ + h0
˘ (w 0  eV ) È Ê w ˆ Ê eV  w 0 ˆ  1˙ exp Á 0 ˜ Íexp Á ˜ ¯ Ë T ¯ w 0 T Î Ë ˚ Ê w ˆ  exp Á 0 ˜ + 1 = 0. Ë T ¯
(29.10)
The ratio h0 = t 0intra /t 0inter is actually a function of m and T. The h0 – m and h0 – T dependences are associated with the linearity of the density of states in GLs as a function of energy. To a good approximation, these dependences can be described [16] by function h0 = 2w 02 /(6m 2 + p 2T 2 ) with h0 µ (ℏw0/T)2 at m T and h0 µ (ℏw0/m)2 at ℏw0 > m T. Thus, considering Eq. (29.1), h0 in Eq. (29.10) is given by h0 =
22w 02
(3e2V 2 + 2p 2T 2 )
.
(29.11)
Introducing the effective temperature of the optical phonon system Q such that N0 = [exp(ℏw0/Q) – 1]–1, i.e., Q=
w 0
ln (1 + N 01 )
,
(29.12)
and substituting N0 from Eq. (29.9) to Eq. (29.11), one can relate Q and T. Then, calculating the T–V dependences using Eq. (29.10), one can find the pertinent Q – V dependences.
29.4 Effective Temperatures and CurrentVoltage Characteristics (Analytical Analysis) 29.4.1 Low Voltages
In particular, at V = 0, Eqs. (29.8) and (29.10) naturally yield N0 = N 0eq and T = T0. At sufficiently low voltages when (h0decay eV /w 0 ) T0 or even T T0. However, it is intriguing that in a rather narrow voltage range where V is about some value Vd, the T–V dependences are ambiguous, so that these dependences as a whole are of the Sshape. The appearance of the Sshape characteristics can be attributed to a decrease in parameter h0 with increasing T [see Eq. (29.11)]. This corresponds to a decrease in t 0intra and, hence, to an essential intensification of the intraband
525
526
Toward the Creation of Terahertz Graphene Injection Laser
transitions, particularly, those associated with the reabsorption of nonequilibrium optical phonons when T increases. This is because at high electronhole effective temperatures, the intraband transitions assisted by optical phonons take place between relatively high energy states with their elevated density. When V exceeds some “disruption” voltage Vd, the net power acquired by the electronhole plasma can be compensated by the intraband energy relaxation on optical phonons only at sufficiently high T. As a result, in this case, the electronhole temperature jumps to the values corresponding to higher branch of the T–V dependence. Thus, the “observable” T–V dependences and their consequences can as usual exhibit hysteresis instead of the Sbehavior. One needs to point out that if the above temperaturedependent parameter h0 is replaced in calculations by a constant, the calculated T–V dependences become unambiguous, although they exhibit a steep increase in the range V ~ Vd. The behavior of T as a function of V markedly depends on parameters h0decay and h0. The width of the voltage range where T < T0 increases when parameter h0decay becomes smaller with increasing voltage. Simultaneously, the depth of the T–V sag dependent with T < T0 increases with decreasing h0decay as well as with decreasing T0. At small h0decay , the electronhole cooling can be rather strong, particularly when T0 = 200 K. This is natural because faster decay of optical phonons prevents their accumulation (heating) and promotes the electronhole plasma cooling when the Joule power is smaller than the power transferred from electrons and holes to optical phonons. It worth noting that the voltage range where the T–V dependence is ambiguous widens with increasing h0decay . As seen from Fig. 29.4, the optical phonon effective temperature also exhibits a Sshape voltage dependence. However, contrary to the electronhole effective temperature, Q ≥ T0 at all the voltages is under consideration. The values of Q at relatively high voltages steeply increase with increasing parameter h0decay . Comparing the T–V dependences calculated for different lattice temperatures, one can find that at moderate and large values of h0decay , these dependences are virtually independent of T0. This is because in such a case, the number of optical phonons N 0 N 0eq and, hence, Q T0 even at not too high voltages, so that the role of equilibrium optical phonons is weak.
Effective Temperatures and CurrentVoltage Characteristics
Figure 29.4 Optical phonon effective temperature Q as function of applied decay voltage V for different values of h0 . Dashed line corresponds to Q = 300 K.
Figure 29.5 Normalized currentvoltage characteristics for different values of h0decay .
Invoking Eq. (29.5), the T–V dependences obtained above can be used to find the currentvoltage characteristics. Figure 29.5 shows the J–V characteristics calculated using Eq. (29.5) and the T–V and Q–V dependences obtained numerically. As a consequence of the Sshape T–V and 0–V dependences, the J–V characteristics (as well as the voltage dependences of the dynamic conductivity considered
527
528
Toward the Creation of Terahertz Graphene Injection Laser
in the following) are also of the Sshape. According to Figs. 29.3 and 29.5, the T–V and J–V characteristics in the range of low and moderate voltages are independent of parameter h0decay . This is in line with the results of the previous analytical analysis [see Eqs. (29.13) and (29.14)]. However, at relatively high voltages, distinctions in the J–V characteristics for different h0decay is significant although all of them tend to J0 when V approaches to ℏw0/e.
29.6 Dynamic Conductivity
Knowing the T–V dependences, one can calculate the dynamic conductivity, sw, of a GL under the injection pumping as a function of the signal frequency w and the applied voltage V. To achieve lasing at the frequency w, the real part of the complex dynamic conductivity at this frequency should be negative: Resw < 0. As shown previously (see, for instance, Refs. [4, 35]), the interband contribution of the nonequilibrium electronhole plasma with the quasiFermi energy m and the effective temperature T is proportional to tanh[(ℏw – 2m)/4T]. The intraband contribution to Resw, which corresponds to the Drude absorption, depends on w, m, and T as well. It also depends on the time of electron and hole momentum relaxation on impurities and phonons s. The latter is a function of the energy of electrons and holes e. The main reason for the t – e dependence is a linear increase in the density of state in GLs with increasing e. In this case, t–1 = ν0(e/T0), where ν0 is the collision frequency of electrons and holes in equilibrium at T = T0. Considering this and taking into account Eq. (29.1), we can arrive at the following formula [16] approximately valid in the frequency range w ν0: Res w (e2V 2 + 2p 2T 2 /3) Ê w  eV ˆ C . = tanh Á + Ë 4T ˜¯ s0 2w 2
(29.22)
Here, s0 = e2/4ℏ and C = 2ℏν0/pT0. In high quality MGLs (with n01 20 ps at T0 = 50 K (Refs. [2, 3]), assuming that ν0 µ T0 (Ref. [36]) for T0 = 300 K, one can set ν0 3 ¥ 1011 s–1 and hence, C 0.005. For substantially less perfect GLs with ν0 15 ¥ 1011 s–1, one obtains C 0.025. These data are used for the calculations of Resw. Figure 29.6 demonstrates the frequency dependences of Resw/s0 calculated using Eq. (29.22) for different values of parameter h0decay
Dynamic Conductivity
Figure 29.6 Dependence of normalized dynamic conductivity Resw/s0 on signal frequency w/2p for different values of h0decay and ν0 3 ¥ 1011 s–1 (upper panel) and ν0 15 ¥ 1011 s–1 (lower panel).
at different voltages V for ν0 3 ¥ 1011 s–1 and ν0 15 ¥ 1011 s–1. As seen from Fig. 29.6 at the injection conditions under consideration, the characteristic conductivity s0 is much smaller than the dc conductivity in the isection sww = 0 = s00. It is also seen that even at relatively large values of parameter h0decay , the dynamic conductivity can be negative in the THz range of frequencies provided the applied voltage is not so strong to cause the electronhole plasma and optical phonon system overheating and the ambiguity of the voltage
529
530
Toward the Creation of Terahertz Graphene Injection Laser
characteristics. This is confirmed by Fig. 29.7. Figure 29.7 shows Resw/s0 as a function of the applied voltage. As demonstrated, the range of the signal frequencies where Resw < 0 markedly shrinks and the quatity Resw decreases when either h0decay or ν0 increase. In particular, at large values of h0decay , the achievement of the negative dynamic conductivity and THz lasing can be complicated (at the temperatures T0 ~ 300 K when the optical phonon recombination mechanism dominates). This is because when h0decay increases, the quantity Vd becomes small. As a result, the optical phonon system is overheated starting from relatively low voltages that leads to an “early” overheating of the electronhole plasma (see Figs. 29.3 and 29.4). If the value of Resw is insufficient to overcome the losses of the THz modes propagating along the GL structure, the structures with MGL can be used. In this case, the net dynamic conductivity of the MGL structure is given by Resw ¥ K, where K is the number of GLs [8–10].
29.7 Limitations of the Model and Discussion
High density of the electronhole plasma in the isection under the injection conditions promotes the quasineutrality of this section. The recombination does not significantly affect the uniform distribution of the electron and hole densities in the isection (assumed above) if the recombination current J is much smaller than the maximum injection current Jm which can be provided by the p and nsections. This imposes the condition J 2Jm. The latter inequality is equivalent to the condition that the recombination length is longer than the isection length 2L. Considering a strong degeneracy of the electron and hole components in the p and nsections, respectively, the quantity Jm can be estimated as Jm �
euF
p 2 �2
[mi2  (mi  eV )2 ].
(29.23)
At T0 = 300 K, 2L = 20 mm, mi = 0.3 eV, and V = 0.1 V, one obtains J0 32 A/cm and 2Jm 65 A/cm. As seen from Fig. 29.5, J J0 at least in the most interesting voltage range, where Resw < 0 (see Fig. 29.7), the condition J Jm is satisfied.
Limitations of the Model and Discussion
Figure 29.7 Normalized dynamic conductivity Resw/s0 vs applied voltage V for different values of h0decay and ν0 3 ¥ 1011 s–1, w/2p = 4 THz (upper panel) and ν0 15 ¥ 1011 s–1, w/2p = 6 THz (lower panel).
In the above consideration, we disregarded the leakage current from the isection to the p and nsections. This current includes the tunneling and thermionic components. Both these components depend on the height, mi, of the barriers between the p and isections and i and nsections and the applied voltage V (see Fig. 29.2). As shown previously [37], the tunneling current decreases with increasing width of the pi or in junction l (see Fig. 29.2a), because it is sensitive to the electric field at the junction [18]. The width in
531